Please copy and paste this embed script to where you want to embed

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

Hans G. Vælz

Industrial Color Testing

Kinh Tang Nguyen Quoc Thiet

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

Hans G. Vælz

Industrial Color Testing Fundamentals and Techniques

Second, Completely Revised Edition

Translated by Ben Teague

Weinheim 7 New York 7 Chichester 7 Brisbane 7 Singapore 7Toronto

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

Dr. Hans G. Vælz Deswatines-Straûe 78 D-47800 Krefeld (formerly: Bayer AG, Krefeld-Uerdingen, Germany)

This book was carefully produced. Nevertheless, author, translator and publisher do not warrant the information contained therein to be free of errors. Readers are advised to keep in mind that statements, data, illustrations, procedural details or other items may inadvertently be inaccurate.

First Edition 1995 Second, Completely Revised Edition 2001

Library of Congress Card No.: Applied for. British Library Cataloguing-in-Publication Data: A catalogue record for this book is available from the British Library. Die Deutsche Bibliothek ± CIP-Cataloguing-in-Publication Data: A catalogue record for this publication is available from Die Deutsche Bibliothek.

WILEY-VCH Verlag GmbH, D-69469 Weinheim (Federal Republic of Germany), 2001 Printed on acid-free paper. All rights reserved (including those of translation into other languages). No part of this book may be reproduced in any form ± by photoprinting, microfilm, or any other means ± nor transmitted or translated into a machine language without written permission from the publishers. Registered names, trademarks, etc. used in this book, even when not specifically marked as such, are not to be considered unprotected by law. Composition: ProSatz Unger, D-69469 Weinheim Printing: Strauss Offsetdruck GmbH, D-69509 Mærlenbach Bookbinding: Wilhelm Osswald & Co., D-67433 Neustadt/Weinstraûe Printed in the Federal Republic of Germany

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

Preface to the Second Edition

The first English edition having sold out in just a few years, the publisher has decided to bring out a new one. In the meantime, changes in the field have necessitated many alterations in text and content, as well as the revision of some sections of the book. Chapter 2 contains a new Section 2.3.4 titled ªNew Systems: CIE94 and CMC.º The analysis of errors of measurement in Section 2.4.4 has been expanded. A greatly improved method for determining the change in tinting strength is now set forth in Section 4.7.3. In Section 6.1.2, a table has been added to the discussion of evaluation conditions. New methods for determining the tinting strength of inorganic and organic pigments are now discussed in Chapter 8, and the tables for the calculation of the depth of color have been updated. The example (Section 8.2.4) for the calculation of the change in tinting strength has been modified to take advantage of the new technique described in Chapter 4. Finally, the listing of standards at the end of the book has been expanded; the author expresses his gratitude to Dipl.-Chem. B. Reinmçller of DIN, Deutsches Institut fçr Normung, Berlin, and his colleagues for their exemplary work in updating the list. Mrs. K. Sora of Wiley-VCH has provided intelligent help in creating this new edition. The new text material has been translated into English by Mr. B. Teague. The contributions of both are gratefully acknowledged. Krefeld, March 2000

Hans G. Vælz

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

Preface to the English Edition

The English version of my book is appearing just four years after the successful German edition entitled Industrielle Farbprçfung. It is closely based on the German text. Revisions have been necessary in only a few passages to correct errors and update (and sometimes expand) the literature citations. Furthermore, equations that are essential for theoretical understanding and practical application have been enclosed in boxes for emphasis. New material in the colorimetric part includes the CIELAB 92 color-difference system (Section 2.3.3) and the RAL Design color-order system (Section 2.3.4). A greatly simplified and clearer description has been given for the proposition (important in the determination of tinting strength) that equality of the CIE tristimulus values Y in lightness matching implies equality of the Kubelka-Munk functions, that is, that DY = DFY = 0 (Section 4.6.4 and 4.7.1). In connection with tests of significance, it is shown how the error of preparation can be separated into specific error components (Section 6.3.3). To aid the understanding of confidence levels in relation to acceptability, an explanatory paragraph has been inserted in Section 6.5.3, and the same chapter has been expanded by the new Section 6.5.4, ªAcceptability and Test Errors.º The index of standards (Appendix 1) is completely new. Organized through keyword, it lists standards of the International Organization for Standardization (ISO), the European Committee for Standardization (CEN), and several national standards bodies: the American Society for Testing and Materials (ASTM), the British Standards Institution (BSI), the Association Franaise de Normalisation (AFNOR), the Japanese Industrial Standards (JIS), and the Deutsches Institut fçr Normung (DIN). An important role in the preparation of this table was again performed by Mr. E. Fritzsche of DIN, Berlin, to whom I would like to express my gratitude. I am also grateful to my colleague and successor, Dr. H. Heine, Krefeld, for his generous assistance, to Mr. Ben Teague for a sympathetic translation, and to Mrs. Karin Sora of VCH Publishers for her helpful collaboration. Krefeld, July 1994

Hans G. Vælz

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

Preface

This book is directed chiefly to all technical personnel who are involved with pigments and dyes, whether as manufacturers, converters, or consumers. It is often not enough to be familiar with the procedure used in a test; more must be known about the quantity being measured and the way in which it varies as a function of other parameters ± in brief, about its physicochemical habit, which is embedded in the well-known fields of chemistry and physics. This is especially important when test methods are to be rationalized; rationalization requires computers, and all computer use is based on applied mathematics. Effective rationalization is possible only when the mathematical and physical background of the quantities being measured is kept fully in view. The lack of suitable worked-out examples to illustrate test methods often creates difficulties in practice as well. This book should help close the gap by providing at least one practical example for each of the test methods described. The book should, however, also offer some utility to the scientist engaged in research and development work on pigments and dyes. Discussion of principles makes up a substantial part of the text, and many suggestions and hints are included to further the scientist's work. On the other hand, anyone working in research or development but lacking a knowledge of both the principles and the state of the art will scarcely be in a position to advance the colorimentric properties of these substances. A third audience ± so the author hopes ± will find the book beneficial: university lecturers and students in the natural sciences. The study of colorimetry in the testing of coloring material is a perfect example of the interdisciplinary effect of chemistry, physical chemistry, physics, theoretical physics, mathematics, and cybernetics (informatics). It goes without saying that one must understand the principles of each discipline before one can understand their interaction. There is, however, another point: The integrative components of the knowledge assembled in this book are hardly taught (if at all) in our universities and colleges of technology ± colorimetry and Kubelka-Munk theory being just two examples. Even beyond the field of coloring materials, both these bodies of knowledge have significant roles to play in many other technical areas, and it is hard to comprehend that people with university-level diplomas even today are entering the colorant manufacturing and converting industries without ever having come in contact with either topic. In choosing the contents of this book from the disciplines named, the author has adopted a standard that he considers trustworthy, one that has continually aided him

VIII

Preface

in distinguishing key topics from less important ones: He wanted to write the book he wishes had been available when he entered the field of pigment testing. Naturally, such a wish is a bit of a fantasy, for it is only now that this book could be written in its present form. Some three-quarters of the test methods described there did not even exist then. The same holds, in modified form, for the principles; while certain branches of knowledge had already been developed 30 years ago, they were not yet relevant for our field ± the statistical analysis of color coordinates is one of many topics that might be mentioned. Finally, the introduction of the computer in colorimetric testing has led to major changes in recent years. To avert misunderstandings, some special points relating to text selection should be stated in advance. The title of the book should be read as referring to the colorimetric examination of pigments and dyes in media; thus, all tests not carried out in mixtures with a lacquer, paint, plastic, or other coating are excluded (e. g., on textile fibers or in printing inks). The chapter on ªColorimetryº has been kept short even though it threatened to grow into another whole volume. In other words, this book does not wish to be mistaken for a textbook on colorimetry. The only aspects of that field that are covered are topics essential for the context of the book. Similarly, one will search in vain for instructions on color formulation and correction calculations. These operations do not come under the heading of pigment and dye testing, even if they must be preceded by testing. Similarly, the application of Mie theory in the determination of particle-size distributions is not covered, for it is based not on colorimetric methods but on general spectroscopic methods. In Chapter 2, on the other hand, a comparatively large proportion has been devoted to the statistical analysis of color coordinates. The reasons for this are that these applications are relatively novel in practice and that key topics such as acceptability (tolerances) are related to them. New in Chapter 3 are the fourflux equations for specular substrates, which may prove to be of interest in the future. Chapter 4 offers ± for the first time, as far as the author is aware ± a theoretical mathematical justification for the universal practice of treating wideband measurements (e. g., reflectometer values) or color coordinates (e. g., CIE tristimulus values) as spectral values in Kubelka-Munk analysis and of matching not the tristimulus values but their Kubelka-Munk functions. In Chapter 5, instructions are given for extending Mie calculations to the particle-size distribution of anisometric (i. e., bladed or rodshaped) pigments. While the text was in preparation, a number of colleagues expressed willingness to read it and offer vital suggestions and corrections. The entire text was read by Dr. H. Heine (Krefeld-Uerdingen), Dr. S. Keifer (Krefeld-Uerdingen), and A. van Leendert (Krefeld). The following experts made themselves available to read portions of the text: Dr. L. Gall (Ludwigshafen), Dr. W. Herbst (FrankfurtHæchst), Prof. G. Kåmpf (Leverkusen), Prof. J. Krochmann (Berlin), Dr. H. Pauli (Basel), Dr. K. Sommer (Krefeld-Uerdingen), Dr. J. Spille (Leverkusen), Dr. J. Thiemann (Leverkusen), Dr. J. Wiese (Krefeld-Uerdingen), and Dr. K. Witt (Berlin). Mrs. E. Lechner and Mr. E. Fritzsche of DIN, Berlin, have prepared the exemplary listing of the standards cited. The author would like to take this oppor-

Preface

IX

tunity to thank all these colleagues for their helpfulness and their valuable advice and suggestions. I am grateful to Bayer AG for its continuing interest and assistance in the writing of this book, and to VCH Publishers for its intelligent collaboration and valuable advice. Krefeld, November 1989

Hans G. Vælz

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

Contents

Part I Principles 1 Introduction 1.1 1.2 1.3 1.4

1 3

Coloring Materials 3 Color Properties 9 Summary 12 Historical and Bibliographical Notes

12

2 How Colors Depend on Spectra (Colorimetry)

15

2.1 Introduction 15 2.1.1 Concerns and Significance of Colorimetry 15 2.1.2 Reflection and Transmission 17 2.2 CIE Standard Colorimetric System 20 2.2.1 Spectral Distribution and Color Stimulus 20 2.2.2 Trichromatic Principle 21 2.2.3 CIE System 23 2.3 Sensation-Based Systems 26 2.3.1 Lightness, Hue, Saturation 26 2.3.2 Physiologically Equidistant Systems 27 2.3.3 CIELAB System 28 2.3.4 New Systems: CIE94 and CMC 36 2.3.5 Color Order Systems 39 2.4 Mathematical Statistics of Color Coordinates 42 2.4.1 Normal Distribution in Three Dimensions 42 2.4.2 Standard Deviation Ellipsoid 46 2.4.3 Standard Deviations 51 2.4.4 Color Measurement Errors and Significance 55 2.4.5 Acceptability 59 2.5 List of Symbols Used in Formulas 62 2.6 Summary 64 2.7 Historical and Bibliographical Notes 66

XII

Contents

3 How Spectra Depend on the Scattering and Absorption of Light (Phenomenological Theory) 71 3.1 Introduction 71 3.1.1 Phenomenological Theory and Its Significance 71 3.1.2 Many-Flux Theory 72 3.1.3 Surface Phenomena 75 3.2 Four-Flux Theory 78 3.2.1 The Differential Equations and Their Integration 78 3.2.2 Transmittance and Transmission Factor 83 3.2.3 Reflectance and Reflection Factor 86 3.2.4 Limiting Cases of Reflection 90 3.2.5 Determination of the Coefficients 93 3.3 Kubelka-Munk Theory 96 3.3.1 Significance and Formalism 96 3.3.2 Limiting Cases of Reflection 98 3.3.3 Determination of the Absorption and Scattering Coefficients 102 3.4 Hiding Power 104 3.4.1 General 104 3.4.2 Achromatic Coatings 105 3.4.3 Scattering and Absorption Components 108 3.5 Transparency 110 3.5.1 Description and Definition 110 3.5.2 Coloring Power 111 3.5.3 Achromatic Coatings 113 3.6 Principle of Spectral Evaluation 115 3.6.1 Description and Significance 115 3.6.2 Application to Hiding Power 116 3.6.3 Application to Transparency and Coloring Power 121 3.7 List of Symbols Used in Formulas 123 3.8 Summary 125 3.9 Historical and Bibliographical Notes 126 4 How Light Scattering and Absorption Depend on the Content of Coloring Material (Beer's Law, Scattering Interaction) 131 4.1 Introduction 131 4.1.1 Description and Significance of the Concentration Dependence 131 4.1.2 Pigment Particle Size 132 4.1.3 Dispersing of Pigments 133 4.1.4 Measures of Pigment Content 135

Contents

XIII

4.2 Absorption and Content of Coloring Material 138 4.2.1 Dyes 138 4.2.2 Pigments 139 4.3 Scattering and Pigment Content 141 4.3.1 Scattering Interaction 141 4.3.2 Experimental Test of an Empirical Formula 144 4.4 Systematic Treatment of Pigment/ Achromatic Paste Mixing 146 4.4.1 Standard Methods of Pigment/Paste Mixing 146 4.4.2 Importance of the Methods 148 4.5 Kubelka-Munk Functions of Pigment/ Paste Mixture 150 4.5.1 General Formula 150 4.5.2 Black Pigments Mixed with White Paste 151 4.5.3 White Pigments Mixed with Black Paste 156 4.5.4 Colored Pigments Mixed with White Paste 158 4.6 Tinting Strength 165 4.6.1 Significance and Definition 165 4.6.2 Coloristic Matching Criteria for Pigments 167 4.6.3 Color Matching Studies 172 4.6.4 Lightness Matching 178 4.6.5 Color Depth Matching 184 4.7 Special Problems 186 4.7.1 Lightening Power 186 4.7.2 Color Differences after Matching 188 4.7.3 Change in Tinting Strength 191 4.8 List of Symbols Used in Formulas 197 4.9 Summary 201 4.10 Historical and Bibliographical Notes 204 5 How Light Scattering and Absorption Depend on the Physics of the Pigment Particle (Corpuscular Theory) 207 5.1 Introduction 207 5.1.1 Description and Significance of the Corpuscular Theory 5.1.2 Particle-Size Distribution 208 5.1.3 The Optical Constants: Refractive Index and Absorption Index 213 5.2 Mie Theory 217 5.2.1 Integration of the Wave Equation 217 5.2.2 Absorption and Scattering of the Particle Ensemble 219 5.2.3 Scattering Behavior of Pigments 222 5.2.4 Absorption Behavior of Pigments 224

207

XIV

Contents

5.3 List of Symbols used in Formulas 226 5.4 Summary 227 5.5 Historical and Bibliographical Notes 229 Part II Test Methods

232

6 Measurement and Evaluation of Object Colors

233

6.1 Reflection and Transmission Measurement 233 6.1.1 Gloss Measurement and Assessment 233 6.1.2 Measurement and Evaluation Conditions 237 6.2 Practical Evaluation of Color Differences 243 6.2.1 Preparation of Specimens 243 6.2.2 Color Measuring 243 6.2.3 Full Shade 248 6.2.4 Special Problems 252 6.3 Test Errors 255 6.3.1 Calculation of the Standard Deviation Ellipsoid 255 6.3.2 Visualization of the Ellipsoid 257 6.3.3 Total Error and Its Components 259 6.4 Significance 263 6.4.1 Calculation of Standard Deviations 263 6.4.2 Test of Significance 265 6.5 Acceptability 268 6.5.1 Specimen Preparation 268 6.5.2 Matching and Color Measurement 270 6.5.3 Evaluation and Example 271 6.5.4 Acceptability and Test Errors 275 7 Determination of Hiding Power and Transparency

277

7.1 Measurement of Film Thickness 277 7.1.1 Selection of Method 277 7.1.2 Gravimetric,Wedge Cut, and Dial-Gauge/ Micrometer Methods 279 7.1.3 Pneumatic Method 281 7.2 Scattering and Absorption Coefficients 283 7.2.1 Kubelka-Munk Coefficients S and K of White Pigments 283 7.2.2 Kubelka-Munk Coefficients S and K of Black and Colored Pigments 288 7.2.3 Four-Flux Coefficients s+, s±, k' 293

Contents

7.3 Transparency 296 7.3.1 Single-Point and Multi-Point Methods 296 7.3.2 Method Based on Principle of Spectral Evaluation 7.4 Hiding Power 303 7.4.1 General (Graphical Method) 303 7.4.2 Achromatic Case 305 7.4.3 Based of Principle of Spectral Evaluation 310 7.4.4 Economic Aspects 318 8 Determination of Tinting Strength and Lightening Power

XV

298

323

8.1 Content of Coloring Material 323 8.1.1 Dyes 323 8.1.2 Pigments 324 8.2 Relative Tinting Strength 325 8.2.1 Dyes 325 8.2.2 Inorganic Black and Colored Pigments (Lightness Matching) 327 8.2.3 Organic Pigments (ªFIAFº Method Based on Principle of Spectral Evaluation) 332 8.2.4 Change in Tinting Strength 340 8.3 Lightening Power 345 8.3.1 Graphical Method 345 8.3.2 Rationalized Method 348 8.3.3 PVC Dependence from One Gray Mixture 351 Appendix: List of DIN, DIN ISO, and ISO Standards Cited Subject Index Name Index

363 371

357

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

Part I Principles

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

1

Introduction

1.1

Coloring Materials

This book deals with color-imparting substances and the color phenomena which they produce. The general term for all coloring substances is ªcoloring materialsº;* and includes, in particular, pigments and dyes. Pigments are substances consisting of particles that are practically insoluble in the application medium. They are used chiefly as coloring materials but can also be employed for other properties in special applications (e. g., anti-corrosion or magnetic pigments). The demarcation between pigments and fillers was formerly somewhat problematic as it cannot be stated in terms of a limiting refractive index. However they can be differentiated according to their application. In contrast to pigments, a filler is not employed to impart color but to impart certain technical properties to the coating or to increase the volume of the coating material. Such a convention does not rule out the possibility that certain substances can find use as both pigments and fillers. However, there is a large group of substances that act as pigments in the great majority of cases (e. g., TiO2 is never used as a filler). When we speak of pigments, we are referring to this group. This statement also applies to the present book. Pigments can be classified according to a variety of criteria; here we generally follow the standard scheme and speak of two classes: ± Inorganic pigments ± Organic pigments The next step in classification is according to their origin: ± Natural pigments ± Synthetic pigments Economically, synthetic pigments are very much more significant than natural pigments, and they will therefore be our exclusive focus in the following classification.

* For standards see ªColoring Materials, Termsº in Appendix 1.

4

1 Introduction

According to standards*, inorganic and organic pigments are broken down as follows: ± White pigments. Their optical effect depends on the nonselective scattering of light. Examples, inorganic: titanium dioxide pigments, zinc sulfide pigments, lithopone, lead white, zinc white; organic: white resin powders. ± Black pigments. The optical effect of black pigments is based on the nonselective absorption of light. Examples, inorganic: carbon black, black iron oxide; organic: aniline black. ± Colored pigments. Colored pigments act by selective absorption of light, often combined with selective scattering. Examples, inorganic: iron oxide pigments, cadmium pigments, ultramarine pigments, chrome yellow, molybdate red, nickel rutile yellow, cobalt blue; organic: azo pigments, quinacridone pigments, dioxazine pigments, perylene pigments, phthalocyanine pigments, lake colors based on azo dyes and triphenylmethane dyes. ± Luster pigments. These are metallic particles or particles with high refractive indices. They are predominantly planar in structure and orientation, which produces gloss effects (see below for further classification). ± Luminescent pigments. These pigments fluoresce or phosphoresce (see below for further classification). The last two groups require additional explanation. Luster (gloss) pigments include: ± Metal-effect pigments. These consist of lamellar metal particles (in contrast, powdered zinc and lead are referred to as anticorrosive ªmetallic pigmentsº and do not belong to this group). Examples, inorganic only: gold bronze, aluminum bronze. ± Nacreous pigments. These pigments consist of transparent lamellar particles, which produce a pearl-like (nacreous) gloss by multiple reflection when in a parallel orientation. Examples, inorganic: specially prepared basic lead carbonate, bismuth oxychloride, titanium dioxide precipitated on mica; organic: fish scale. ± Interference pigments. If the lamellae have the appropriate thickness, iridescence effects are produced by interference. Example, inorganic: iron oxide on mica. Luminescent pigments include the following types: ± Fluorescent pigments. Their optical effect is based on selective absorption of light with simultaneous luminescence. Excitation is achieved by high-energy radiation such as ultraviolet or short-wavelength visible light. * For standards see ªColoring Materials, Classificationº in Appendix 1.

1.1 Coloring Materials

5

Examples, inorganic: pigments for display tubes and fluorescent lamps, radioactive luminescent pigments; organic: 2-hydroxy-1-naphthaldazine. ± Phosphorescent pigments. The optical effect of phosphorescent pigments is based on selective absorption and scattering of light plus delayed luminescence. Excitation is achieved by high-energy radiation such as ultraviolet or short-wavelength visible light. Examples, inorganic only: zinc sulfide/alkaline-earth sulfides doped with heavy-metal ions. The chemical makeup of pigments will only be dealt with briefly to discuss the hues which are obtainable. Inorganic pigments, with a few exceptions, are oxides, sulfides, oxide hydroxides, silicates, sulfates, and carbonates. In general, they consist of individual particles which are uniform in chemical composition (e. g., iron oxide red is a-Fe2O3). Organic pigments, in principle, are also powders of uniform composition; the two major groups are azo pigments and polycyclic pigments. The colors associated with individual pigments are listed in four tables: ± ± ± ±

White and black pigments: Table 1-1 Inorganic colored pigments: Table 1-2 Organic colored pigments, azo pigments: Table 1-3 Organic colored pigments, polycyclic pigments: Table 1-4

Table 1-1. White and black pigments.

Inorganic pigments

Organic pigments

Chemical class

White pigments

Black pigments

Oxides

Titanium dioxide Zinc white

Black iron oxide Iron-manganese black Spinel black

Sulfides

Zinc sulfide Lithopone

Carbon and carbonates

White lead

Perylene pigments Others

Carbon black Perylene black

White resin powders

Aniline black Anthraquinone black

6

1 Introduction

Table 1-2. Inorganic colored pigments. Chemical class

Green

Blue-green

Blue

Violet

Oxides and hydrated oxides Iron oxide pigments

Chromium oxide pigments

Mixed phase oxides

Red

Orange, brown

Yellow

Yellowgreen

Red iron Brown iron Yellow iron oxide oxide oxide Mixed brown (spinel and corundum phases) Chromium oxide green

Hydrated chromium oxide green

Cobalt green

Cobalt blue

Nickel rutile yellow Chromium rutile yellow Cadmium sulfoselenide

Sulfides and sulfoselenides

Cadmium sulfide

Cadmium mercury sulfide Chromate pigments

Chrome green

Molybdate red

Ultramarine pigments

Ultramarine green, Ultramarine blue, Ultramarine violet Ultramarine red

Iron blue pigments

Iron blue

Others

Manganese blue

Cobalt and manganese violet

Chrome orange

Chrome yellow Zinc yellow Alkalineearth chromates

Cadmium zinc sulfide

1.1 Coloring Materials

7

Table 1-3. Organic colored pigments: azo pigments. Blue Monoazo pigments

Disazo pigments

Others

Violet

Red

Orange, brown

Yellow

Monoazo orange pigments (also as lakes*)

Monoazo yellow pigments (also as lakes**)

Yellow- Green green

Diaryl yellow pigments Disazopyrazolone pigments

b-Naphthol pigments (also as lakes*)

Bisacetoacetic acid arylide pigments Metal complex pigments**

Naphthol AS pigments (also as lakes*) Naphthalenesulfonic acid pigments in lake form Benzimidazolone pigments Disazo condensation pigments Isoindoline pigments Isoindolinone pigments * Pigments in lake form are Me salts between sulfonic acid and/or carboxylic acid groups of dyes and metal salts (Me = alkaline earth, Na, Mn). ** Me complexes with azo or azomethine groups (Me = Ni, Co, Fe, Cu, Zn).

8

1 Introduction

Table 1-4. Organic colored pigments: polycyclic pigments. Yellow- Green Bluegreen green Aromatic and heterocyclic pigments

Blue

Violet

Phthalocyanine pigments

Red

Orange, brown

Yellow

Quinacridone pigments Perylene pigments Perinone pigments Thioindigo pigments

Anthraquinone pigments

Flavanthrone yellow pigments

Triarylcarbonium pigments

Pyranthrone pigments Dioxazine Anthpigments anthrone pigments

Anthrapyrimidine pigments Quinophthalone pigments

Dyes are coloring materials which are soluble in the application medium. Dyes used to be exclusively natural products, but these are of virtually no commercial importance today. It is not difficult to classify all dyes in a similar way to pigments. However, the main area of application for dyes is in textile coloring as although their ease of dispersion makes them advantageous for use in coatings and plastics, dyes are often less lightfast than pigments in these media. Special types are, however, significant in the plastics industry. We do not need to classify dyes as in Tables 1-3 and 1-4 because it would look the same. Along with the classifications already mentioned, other ways of breaking down the classes of pigments and dyes are possible. For example, they might be listed by application. The industrial synthesis of coloring materials is now subject to rigorous monitoring by qualitative and quantitative chemical analysis performed in plant laboratories, quality control laboratories and special research laboratories. The chemical analysis of raw materials, intermediates, end products, by-products, and waste products serves not only to meet quality requirements, but also to satisfy environmental protection standards. Final inspection, which also considers physical properties and application qualities, takes place in properly equipped testing laboratories; this process can no longer even be thought of without the aid of computers. The principles and methods of testing, as specifically applicable to coloristic pigment and dye properties, are the subject of this book.

1.2 Color Properties

9

The creation of international standards by the ISO (International Organization for Standardization) and of national standards by AFNOR, ASTM, BSI, DIN, JIS*, and other bodies has not only made it possible to state unambiguously what requirements pigments have to meet, but has also led to greater progress towards universally accepted test methods (see Appendix 1).

1.2

Color Properties

All color phenomena that we can observe in coatings have their origin in the interaction between the coating material and visible light, i. e., the electromagnetic radiation in the wavelength range of 400 to 700 nm. Special importance is attached to the fact that such coatings need not be homogeneous but can exhibit typical inhomogeneities due to the presence of discrete pigment particles. The physical processes that result from this interaction can be broken down into a few elementary processes. When a photon enters into a dyed or pigmented coating, three processes can determine its subsequent fate (Fig. 1-1): ± The photon collides with a dye molecule or a pigment particle and is absorbed. ± The photon collides with a pigment particle and is scattered. ± The photon passes through the coating without collision (assuming that the surrounding medium does not absorb) and is scattered and/or absorbed by the substrate. The fundamental physical and optical properties of coloring materials are thus their absorbing and scattering powers. Inhomogeneity of the coating is not a necessary condition for absorption; even homogeneous coatings can absorb if they contain light-absorbing substances, such as dissolved dyes. The case is different for light scattering, which can occur only in a coating that has the following properties: ± The coating is heterogeneous in composition.** ± Its individual components differ in refractive index.

* AFNOR = Association Franaise de Normalisation ASTM = American Society for Testing and Materials BSI = British Standards Institution DIN = Deutsches Institut fçr Normung JIS = Japanese Industry Standard ** Light scattering on molecules can be ignored here because it is orders of magnitude less than scattering on multimolecular pigment particles.

10

1 Introduction

Fig. 1-1.Absorption and scattering of light in a coating with colored pigment particles. a: Directionally incident white light b: Gray substrate c: Directly reflected light d: Diffusely reflected light

In a somewhat simplified scheme, forward and backward scattering are distinguished by whether the light is scattered in the direction of incidence (into the front half-space) or in the opposite direction (into the back half-space). White pigments have very little absorbing power in comparison to their scattering power. Black pigments, on the other hand, have very little scattering power relative to their absorbing power. Colored pigments, as a rule, feature selectivity in both absorbing and scattering power, i. e., they show wavelength-dependent behavior. This explains how the two elementary processes of absorption and scattering give rise to what we can measure: the reflection spectrum, the spectral reflectance R (l) between wavelengths 400 and 700 nm.* Pigmented coatings, and thus indirectly pigments themselves, can be unambiguously characterized by their reflection spectra. But the human eye cannot see reflection spectra; it merely communicates color stimuli to the brain. The missing link in the chain is the conversion of reflection spectra to color stimuli; this is accomplished by colorimetry. Modern testing of coloring materials is able to establish an almost perfect connection between the color stimulus (and hence the optical properties of the pigments) and fundamental physical quantities. The point of making such a connection is to be able to operate under well-known rules of physics. The schematic diagram shown in Figure 1-2 will aid in unterstanding these relationships. Key physical quantities are listed at the bottom left, while application properties of importance in practice are shown at the top left of the diagram. Particularly important are the boxed entries in between, which represent theoretical ideas that link the technical properties with the physical ones. The following relationships exist: ± Colorimetry relates the perceived color quality to the color stimulus F and this, in turn, to the reflection spectrum R (l). ± Kubelka-Munk theory relates R (l) to the scattering coefficient S (l), absorption coefficient K (l), and coating thickness h. * The symbols employed in each subsequent chapter are listed at the end of that chapter. See also ªSymbols for use in formulasº in Appendix 1.

1.2 Color Properties

11

Fig. 1-2. Schematic diagram showing relationships between color properties and theoretical fundamentals.

± Multiple scattering theory relates S to the scattering cross section QS (D, l) of the individual particle and the pigment concentration s. (The absorption coefficient K is directly proportional to the absorption cross section QA (D, l) and s.) ± Mie theory, finally, relates QS (D, l) and QA (D, l) to the particle size D, the wavelength l, the refractive index n, and the absorption index k; the last two optical properties are constants of the material. In practice, either downward or upward motion is possible. For instance, to determine the hiding power it is first necessary to obtain the Kubelka-Munk coefficients by color measurements (moving downward) so that the expected color stimulus of the hiding layer can then be calculated (moving upward). A separate chapter in this book is devoted to each of the four theoretical complexes listed above. The ideas behind modern test methods are rather difficult, since they are based on the light source/sample/eye/brain configuration and the methods must reproduce it. The need to simulate this very complicated system leads to the insight that further progress is possible only if new problems with an even greater degree of difficulty can be handled. ªSimpleº test methods such as appear in the specialist literature from time to time cannot be expected to solve these problems. The only promising approach is to enhance our knowledge and understanding of the cybernetic and physico-chemical principles involved in the perception of optical stimuli by the eye and associated organs. The objection sometimes heard, that new and complicated methods entail excessive calculation effort, long ago lost its justification when powerful and economical computers became available, which meant that calculations could be done in quite a short time. This is one of the key conditions that have led to advances in this field, i. e., the remarkably fast development in computer technology. Only by virtue of this development have present-day colorimetric and testing laboratories been able to formulate such complex testing programs in a objective fashion and to perform tests such as those described in this book in a prompt and efficient manner.

12

1 Introduction

1.3

Summary

The terms ªcoloring materialsº, ªpigmentº, and ªdyeº are defined and explained in this chapter. The usual classification of pigments is according to chemical nature (inorganic, organic) and genesis (natural, synthetic). The subclasses of white, black, colored, luster, and luminescent pigments are also characterized. Inorganic pigments consist of oxides, oxide hydroxides, silicates, sulfates, sulfides, and carbonates; organic pigments are divided into two major groups, the azo pigments and polycyclic pigments. Dyes can be classified under criteria similar to those of organic pigments. The industrial synthesis of pigments and dyes today is subject to monitoring by analytical and physical-chemical methods, which would be inconceivable without the aid of computers. The existing international and national standards are of great importance for both specifications and test methods. This book is concerned with colorimetric methods used for testing coloring materials in media. The starting point is therefore the interaction of light with a coating. Typical phenomena are described: the light can be scattered and/or absorbed. While absorption of light is apparent in the case of dyes and pigments, scattering is expected only when pigments are present. White pigments are characterized by a high scattering power with very little absorption; black pigments by a high absorbing power. Colored pigments feature selective absorption, and frequently selective scattering as well. For pigment and dye testing, the color can be related to fundamental physical quantities from color stimulus to the spectrum, to scattering and absorption, to refractive and absorption indices, and to wavelength and particle size. These relationships are used in an appropriate sequence when establishing test methods. The current state of the art in color test is chiefly due to advances in computer technology, which have offered ways to perform many testing jobs in an economical way.

1.4

Historical and Bibliographical Notes

It can be presumed that the use of coloring materials for coloring by human beings goes back to the origins of cultural history. The oldest artifacts that have come down to us are the well-known cave paintings, made with natural inorganic pigments. It must not be overlooked that the materials and the fundamental knowledge available at that time were limited even though artistic expressiveness and craft knowledge were already highly advanced. It was a long historical path [1], [2], [3] that led to the present high level of scientific and technological development in the areas of inorganic pigments [4], [5], [6], organic pigments [2], and dyes [3]. An important factor in this progress was the elucidation of the principles underlying the optical and colorimetric properties of dyes and pigments, together with the result-

1.4 Historical and Bibliographical Notes

13

ing advances in objective testing and evaluation methods. The methods in use today are the subject of this book. Stages of development that have occurred mainly in recent decades can be researched in survey articles [1], [7], [8]. The development of standardization in parallel with testing techniques is covered in [9]. Standards for the specifications of inorganic pigments see [5]. Each chapter in Part I of this book contains a section of historical and bibliographical notes together with a list of references.

References [1] H. Heine, H. G. Vælz, Pigments, Inorganic, Introduction, in Ullmann's Encyclopedia of Industrial Chemistry, 5. edit.,VCH Weinheim 1992,Vol. A 20, 245. [2] W. Herbst, K. Hunger, Industrial Organic Pigments,VCH Weinheim 1993. [3] G. Booth, H. Zollinger, K. McLaren, W. G. Sharples, A. Westwell, Dyes, General Survey, in Ullmann's Encyclopedia of Industrial Chemistry, 5. edit.,VCH Weinheim 1987,Vol. A 9, 73. [4] G. Buxbaum (Ed.), Industrial Inorganic Pigments,VCH Weinheim 1993. [5] G. Buxbaum, H. Heine, P. Kæhler, P. Panek, P. Woditsch, Anorganische Pigmente, in Winnacker/ Kçchler, Chemische Technologie 4. edit., Vol. 3, Anorganische Technologie II, Hanser, Mçnchen 1983, 349. [6] W. Bçchner, R. Schliebs, G. Winter, K. H. Bçchel, Industrial Inorganic Chemistry, VCH Weinheim 1988. [7] H. G. Vælz, Progr. Org. Coat 1 (1973). [8] H. G. Vælz, Angew. Chem. Internat. edit. 14 (1975) 655. [9] E. Fritzsche, farbe + lack, 80 (1974) 731.

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

2

How Colors Depend on Spectra (Colorimetry)

2.1

Introduction

2.1.1 Concerns and Significance of Colorimetry Colorimetry, the techniques based on it, and the colorimetric way of thinking have become the norm in all fields of technology that deal with colors in any way. The special uses of colorimetry can be summed up under the following headings: ± Color identification codes. Color names are verbal descriptions; they offer little help in the unique identification or labeling of colors. Scientists, however, are accustomed to describing a phenomenon objectively in terms of a measuring unit and number. ± Systematic description of color phenomena. Colorimetric concepts make it possible to construct logical and meaningful color systems based on easily understood principles. ± Evaluation of color differences. The quantification of color differences is one of the principal tasks of colorimetry. It is vital, for example, in production control of coloring materials, varnishes, paints, etc. ± Color rendering. Color rendering involves the evaluation of color differences between the object and the reproduction, as in color television or color photography. ± Colorimetric color formulation. Colorimetry makes it possible to fulfil an ancient wish, to calculate in advance the components and the proportions needed to obtain a desired color. The color properties of coatings, which are the subject of this book, involve all of these points to a greater or lesser degree. We will return to the meaning of color difference in this context. The testing of coloring materials involves measuring them between a given specimen (ªreference sampleº) and a specimen to be evaluated (ªtest sampleº). The objective determination of color differences is essential for the following areas: ± Development of new products. Key factors in technical progress are the continuous improvement of products which are already being produced and the creation of new coloring materials. Indispensable to both, however, is a fundamental

16

2 How Colors Depend on Spectra (Colorimetry)

knowledge of colorimetric relationships and the testing and inspection methods derived from them. Analysis of optical performance can no longer be done without colorimetric testing methods based on exact scientific principles. ± Production control. Human beings use their visual apparatus, consisting of eye, nervous system, and brain, to match and assess coloring substances. This represents an information-processing system in the cybernetic sense, with the special feature that the output of this system gives rise to both physiological and physiological effects. It follows that assessment is generally not free of human prejudices, and so there is a pressing need for objective measurement techniques. ± Understanding between manufacturer and purchaser. Objective measurements are crucial so that the parties to a transaction understand each other clearly, and especially so in an area as emotionally charged as color. Thus it is easier to agree on acceptable deviations from rated values by referring to unimpeachable measuring methods than it would be to agree on how great a color difference can ªjust be seenº. When we raise the question of color deviations and measurement errors, we are in the domain of statistical analysis of color measurements. Such analysis is important for the following: ± Significance. The questioner wishes to know how precisely colors are being measured, that is, whether there is a significant difference between the measured color values for the two specimens being compared. A color comparison demands a knowledge of the significance level, which has to be tested in each case. Only when the significance level is known can one decide whether it is low enough for color comparisons to be made in a specific situation. This knowledge is needed even when color values for the same collection of samples, as measured with different types of instruments, are to be compared. What is called for in this situation is not a measure of the quality of color measurement, but a measure of the quality of the colorimeter. Given a suitable set of color samples covering the entire color space, it should be possible to compare the precisions of the colorimeters. ± Acceptability. This term refers to the limits within which measured color values must lie in order for the purchaser to classify them as ªconforming to a standard.º Acceptability must not be confused with the perceptibility of color differences, which is a threshold forming the upper limit of the region in which colors cannot be distinguished. Acceptability, in contrast, is based on a convention and on the experience of colorists. It has to do with the region within which specimens are assessed to ªconformº, that is, conform to a specified type or reference specimen. This means that some perceptible color differences may well still be acceptable. Both the criteria of significance and acceptability are built up on the same mathematical principles and require the same mathematical apparatus, namely the extension of the Gaussian normal distribution from one to three dimensions. Because

2.1 Introduction

17

these applications of well-known mathematical principles are fairly new and unusual in everyday colorimetric practice, a section is devoted to them alone. Colorimetry is discussed only as much as is necessary and sufficient in light of the theme and context of this book. Monographs and other literature on colorimetry are listed in Section 2.7.

2.1.2 Reflection and Transmission The reflection spectrum mentioned in Section 1.1 is the spectral distribution typical of object colors, and it forms the starting point for any measurement of them. It seems necessary to look more closely at the widely-used terms ªreflectanceº and ªreflection factorº. First, what are ªobject colorsº ? The standards* give the following answer: They are ªnon-luminous perceived colorsº i. e. colors of ªnon-self-radiatingº media that require illumination for their visibility. Color perception thus only takes place with light which illuminates the non-self-radiating medium. Certain standard sources have been defined as illuminants for colorimetry*; those of interest here are ± Standard Illuminant A for incandescent light ± Standard Illuminant C for artificial daylight ± Standard Illuminant D65 for natural daylight at a color temperature of 6504 K Reflection and transmission are purely physical phenomena; the related measurable quantities describe properties of how materials interact with radiation. These quantities are defined in the standards**. Of the many factors that influence them, the ones of interest here are those directly related to radiation: the direction of incidence, the direction of observation, and the aperture angles of the incident and observed beams (Fig. 2-1). Three configurations of the observed radiation are consistent with good technical realization: ± Directional (the beam consists of quasi-parallel rays) ± Conical (the beam has the shape of a narrow cone) ± Hemispherical (the beam is uniformly distributed over the half-space) In reflection measurements, the name of the result depends on the following measuring conditions: ± Reflectance R (hemispherical observation) ± Reflection factor R (conical observation) ± Radiance factor b (directional observation) If the illumination condition is included in the classification, nine geometries must be listed since there are three possibilities for illumination and three for viewing * For standards see ªColorimetryº in Appendix 1. ** For standards see ªPhotometric Properties of Materialsº in Appendix 1.

18

2 How Colors Depend on Spectra (Colorimetry)

Fig. 2-1. Nomenclature of the parameters. e1, e2, angles of incidence and reflection; j, azimuth angle.

(each can be parallel or rather quasi-parallel, conical, or hemispherical). Each of the illumination configurations is represented by a subscript on the symbol R, R, or b (Table 2-1): dif, diffuse (hemispherical case); g, directional; c, conical. Of the nine combinations, however, only three are common in colorimetry and realized in colorimeters. In the list below, the illumination geometry comes first and is followed by the observation geometry: ± Conical/hemispherical ± Hemispherical/conical ± Conical/conical

Reflectance Rc Reflectance factor Rdif Reflection factor Rc

Table 2-1. The nine types of reflectance measurement (after DIN 5036-3). Geometry

Quantity

Symbol

Illumination

Viewing

hemispherical hemispherical hemispherical

hemispherical conical directional

reflectance reflection factor radiance factor

Rdif Rdif bdif

conical conical conical

hemispherical conical directional

reflectance reflection factor radiance factor

Rc Rc bc

directional directional directional

hemispherical conical directional

reflectance reflection factor radiance factor

Rg Rg bg

The preferred measuring conditions are as follows (Fig. 2-2): ± For Rc, 08/diffuse and 88/diffuse (abbreviated 0/d and 8/d respectively) ± For Rdif , diffuse/08 and diffuse/88 (d/0 and d/8) ± For Rc, 458/08 and 08/458 (45/0 and 0/45) All measurements of surface colors in reflected light are referred to the ideal matte white surface, which reflects the incident radiation with a reflectance R = 1 inde-

2.1 Introduction

19

Fig. 2-2. Measuring conditions for colorimetry.

pendent of the angle. Because this perfect white standard is not technically realizable, a real reflection standard (secondary standard) must be adopted for colorimetry. The standard features a set of fixed values and deviates as little as possible from the ideal. It consists of a circular tablet pressed from pulverized barium sulfate*. The rated values for tested commercial barium sulfate powder are specified in Germany by the Physikalisch-Technische Bundesanstalt PTB (Federal PhysicalTechnical Institute); a tablet pressed from such powder can be employed for instrument calibration, either directly or by means of a working standard. A special point to note is that the surface of the specimen whose surface color is to be determined may exhibit peculiar reflectance behavior typical of the surface itself. If this point is not considered, measured color values may be falsified (see Section 6.1.2 for further detail). Object colors can also be evaluated in transmitted light, as in the case of plastic films, dye solutions, and the like. The property sought in such cases is the transmission. There are again three configurations for measuring the transmission** of object colors, and the terminology is analogous to that used in reflection measurement (with the following preferred measuring conditions): ± Transmittance tc, 0/d ± Transmission factor Tdif, d/0 ± Transmission factor Tc, 0/e2 (e2 is an arbitrary observation angle) If both incidence and observation angles are 08 (geometry 0/0), the transmission factor is symbolized by Tr .

* For standards see ªColorimetryº in Appendix 1. ** For standards see ªTransmission of optical radiationº in Appendix 1.

20

2 How Colors Depend on Spectra (Colorimetry)

2.2

CIE Standard Colorimetric System

2.2.1 Spectral Distribution and Color Stimulus In the context of physiological processes of color vision, colors are sensory impressions. If the psychological reactions associated with color vision are also considered, they are experiences. For this reason, it first appears contradictory to apply the term ªmetricº, meaning measurement, to colors. It will be shown that the discussion is actually about a metrical arrangement of equality judgments, in which the human eye functions solely as a null indicator. The starting point for the development is the well-known fact that any color stimulus can be prepared from the spectral colors by mixing. Thus a spectral distribution j (l) can be measured with a spectrograph. The product j (l) dl is the intensity corresponding to the narrow wavelength interval between l and l + dl in the spectrum. If we use the term ªcolor stimulusº and the symbol F for the color sensation registered by the eye, then there must be a correlation between the spectral distribution j (l) and F. Determining how these quantities are related involves knowing not only the purely physical circumstances but also the laws describing the physiology of colors, which can be summarized roughly as follows: If three suitable spectral distributions are selected, other color stimuli can be perfectly reproduced through additive mixing of these three ªreference stimuliº (also called ªprimariesº). The desired result is always achieved with a unique mixing ratio. It must be added that these mixtures are always prepared by the mixing of lights (ªadditiveº color mixing), as distinct from the use of successive optical filters each having its own transmission behavior (ªsubtractiveº color mixing). The physiological behavior just described is a summary of the rules called ªGrassmann's lawsº. If the addition of color stimuli is now defined as their mixing, the multiplication of a color stimulus by a number is also defined. For example, multiplication by the factor 2 corresponds to the addition of two identical color stimuli, etc. Now Grassmann's laws can be written out as follows: F = X7X + Y7Y + Z7Z or F = m (x 7 X + y 7 Y + z 7 Z)

(2.1)

where m = X + Y + Z, x = X/m, y = Y/m, and z = Z/m. Here X, Y and Z are called ªtristimulus valuesº; x, y, and z are called ªchromaticity coordinatesº; m is a physical measure of intensity; and X, Y, and Z are the reference stimuli. From the above definition of addition, it also follows that changing from reference stimuli X, Y, Z to different reference stimuli X',Y', Z' involves a linear (ªaffineº) transformation.

21

2.2 CIE Standard Colorimetric System

2.2.2 Trichromatic Principle The task of colorimetry is now to determine m, x, and y; the determination of z is redundant, since x + y + z = 1. The chromaticity coordinates form a 3-manifold, and this fact suggests analogy with the three dimensions of solid geometry. Indeed, in view of the addition rule, X,Y, and Z can be thought of as three-dimensional vectors forming a trihedral in which the color stimulus is a vector F = {X, Y, Z}. The above equations also show that the wavelength dependence of F is wholly contained in X,Y, Z (or x, y, z), since the reference stimuli are fixed color stimuli. The spectral colors therefore constitute a one-dimensional manifold and lie on a three-dimensional curve (ªspectral locusº) whose points can be labeled with the associated wavelengths l. Any color stimulus F = {X,Y, Z}, by virtue of the intensity distribution j (l), can be reproduced from the spectral colors by mixing, hence the sums taken over the spectral loci must give the tristimulus values exactly. This result can now be briefly derived: A color equation as in eq. (2.1) can be written for the spectral color having the wavelength 400 nm: F400 = x400 7 X + y400 7 Y + z400 7 Z where xl , yl , zl are the tristimulus values of the spectral colors. Now it must be remembered that this spectral color, in the color stimulus F being analyzed, is represented solely by the contribution j400 given by the distribution function j (l). The contributions of the spectral colors at 10 nm intervals are then j400 7 F400 j400 x400 7 X j400 y400 7 Y + j400 z400 7 Z + j410 7 F410 j410 x410 7 X j410 y410 7 Y + j410 z410 7 Z .. . + j700 7 F700 j700 x700 7 X j700 y700 7 Y + j700 z700 7 Z F

7P 00 l400

jl Fl

7P 00 l400

jl xl X

700 P l400

7P 00

jl yl Y

X7X

l400

Y7Y

jl zl Z (sum) Z7Z

Taking the sum of the components gives the initial color stimulus; comparison of coefficients then yields the tristimulus values of the color stimulus: X

700 P l400

jl xl ;

Y

700 P l400

jl yl ;

Z

700 P l400

jl zl

(2.2)

22

2 How Colors Depend on Spectra (Colorimetry)

If the intervals are sufficiently small, the sums go over to integrals, so that

X Y Z

700 R 400 700 R 400 700 R 400

j l x l dl j l y l dl j l z l dl

(2.3)

These formulae give the sought relation between F and j (l). For object colors, j (l) is the spectral distribution of the reflectance R (l) or of the reflection factor R (l) as measured under illumination with white* (ªequal-energyº) light (see Fig. 2-3 for examples). If light with a different spectral distribution S (l) is used for illumination, the reflected light will have a distribution R (l) 7 S (l), and j (l) in the integrals above must be replaced by this product. The ªcolor matching functionsº x (l), y (l), z (l) can be determined experimentally by the following procedure: On a trichromatic matching colorimeter, observers reproduce the individual spectral colors, each with an intensity of m = 1, from the primaries X, Y, Z by mixing. The relative mixing proportions are then determined for every l.

Fig. 2-3. Reflection spectra of some pigments in lacquer binders. * Or of the transmittance t (l) or the transmission factor T (l), in the case of light passing through a medium.

2.2 CIE Standard Colorimetric System

23

It should not be forgotten that this Young-Helmholtz theory of trichromatic color matching has been brilliantly confirmed by physiological research. Three and only three different visual receptors with photosensitive pigments are found in the human eye, their chemical constitutions have been determined (rhodopsins), and their spectral sensitivities have been measured. For color vision there are three types of receptors (cones), each of which contains one and only one such visual pigment. Thus a color stimulus can be defined by three tristimulus values, which are of the nature of integrals. Two color stimuli are then alike if the respective values of their integrals are equal. But the integrals change if either of the factors R (l) or S (l) is replaced by a different function. In general, this occurs if the same sample is illuminated with a different type of light: The two colored surfaces are then no longer alike but have a different appearance. If two colors appear alike only under certain conditions (e. g., under a certain type of illumination), they are, logically, said to be ªlooking alikeº or, in Ostwald's term, ªmetamericº; the phenomenon is called ªmetamerismº.

2.2.3 CIE System The colorimetric system currently in use all over the world is suggested and introduced by the CIE (Commission Internationale de l'Eclairage, International Commission on Illumination). The system includes fixed definitions of the reference stimuli X,Y, Z and the color matching functions x (l), y (l), z (l). In order that all actual colors can be described, color stimuli lying outside of the spectral locus were introduced (ªvirtual stimuliº); these three primary stimuli are obtained from three spectral colors by an affine transformation. The CIE principles are reflected in ISO Standard 7724*. The quantities X, Y, Z are called ªCIE tristimulus valuesº; x, y, z, ªCIE chromaticity coordinatesº; and x (l), y (l), z (l), ªCIE color matching functionsº. There are two sets of color matching functions, for 28 and 108 fields of view, which have been found experimentally to differ somewhat (Fig. 2-4). The CIE tristimulus values** are calculated with equations (2.3): R X = x (l) R (l) dl R Y = y (l) R (l) dl R Z = z (l) R (l) dl If light other than pure white light is used for illumination, R (l) must be replaced by the product R (l) 7 S (l), as shown previously. A number of ªCIE standard illu* For further standards see ªColorimetryº and ªColoring materialsº in Appendix 1. ** Because no limits of integration other than 400 and 700 nm are used, these are omitted from here on.

24

2 How Colors Depend on Spectra (Colorimetry)

Fig. 2-4. CIE color matching functions for 28 and 108 fields of view. (The circles at top right, viewed from a distance of ca. 8±9 cm, show the size ratio of the two fields of view.)

minantsº S (l) have been defined (see Section 2.1.2 and standards*). Table 2-2 presents some values. From the tristimulus values, the CIE chromaticity coordinates are calculated as x

X Y ; y X Y Z X Y Z

(2.4)

These are treated as coordinates in the color plane and define the CIE chromaticity diagram. Table 2-2. CIE tristimulus values and CIE chromaticity coordinates of some illuminants. (Yn = 100.00 for all standard illuminants and observers.) CIE illuminant A C D 65

Xn

28-standard observer Zn xn

109.85 98.07 95.05

35.58 118.22 108.90

0.4476 0.3001 0.3127

108-standard observer Zn xn

yn

Xn

0.4074 0.3162 0.3290

111.14 97.28 94.81

35.20 116.14 107.34

0.4512 0.3104 0.3138

yn 0.4059 0.3191 0.3310

The system exhibits the following properties (see Fig. 2-5): ± In the x, y chromaticity diagram, the additive mixture of two color stimuli lies on the straight line connecting the components, at a position determined by the center of gravity principle. * For standards see ªColorimetryº in Appendix 1.

2.2 CIE Standard Colorimetric System

25

± The shoe-sole-shaped locus of spectrum colors (ªspectral locusº) in the x, y plane is cut off below by the purple line. Colors lying on this line do not occur in the spectrum but are obtained as mixtures of red and violet. ± In the case of equal-energy illumination*, the ªequi-energy stimulusº or white locus lies at xw = yw = zw = 1/3. ± The CIE color matching function y (l) coincides with the spectral luminosity curve V (l) of the human eye. In place of m, the luminance Y = m 7 y is cited as a third color coordinate (along with x and y).

Fig. 2-5. CIE chromaticity diagram.

* Otherwise, the equi-energy stimulus is the color locus of the illuminant (standard illuminant); see Table 2-1.

26

2 How Colors Depend on Spectra (Colorimetry)

Another interesting fact of physiology should also be mentioned here. From the discussion it follows that there may be a very great number of spectral distributions R (l) that belong to one and the same color stimulus F (metameric colors). Because the human eye can distinguish of the order of 100 spectral colors and a roughly similar number of brightness levels, it should be possible to prepare the respectable number of 100100 distinguishable spectral distributions by mixing. In practice, however, by virtue of the trichromatic principle, the eye can only distinguish 1003 colors. The eye and the organs responding to it in the perceptual system thus perform a tremendous reduction in the quantity of information offered. In cybernetic terms, the huge amount of information contained in a single color stimulus (600± 700 bits), which would be nearly impossible to process in a reasonably short time, is reduced in a consistent way to some 20 bits, a quantity of information that the consciousness is well able to process in one second, as we know from a comparison with other sensory organs.

2.3

Sensation-Based Systems

2.3.1 Lightness, Hue, Saturation The CIE system offers a worldwide understanding of colors. Using the three numerical values x, y, and Y (and some few additional pieces of information*), the recipient of a communication can localize the color locus under consideration without having seen the color. Since this system came into existence, it has proved suitable for many different technical applications of color, including color television. In order to assess colored systems and pigments, however, there are additional demands. The two most important shortcomings are that it is hard to visualize information in the CIE system and that it is not suitable for direct determination of physiologically equidistant color differences. A few explanatory words follow: ± Difficulty of visualization: The values of x, y, and Y make it possible to put colors in a systematic order. It is hard, however, to visualize the nature of a color with only the coordinate values. As a way of coping with this problem, colors are classified and ordered according to another three properties so that one may come to an understanding with other parties. These are brightness (one can rank colors as ªbrighterº and ªdarkerº), hue (corresponding, in a way yet to be defined, to the spectral colors), and saturation (every color is regarded as a mixture of the ªsaturatedº hue and white; the color is more saturated the smaller the content of white). * For example, information on the geometry of the colorimeter, the standard illuminant used, and exclusion of surface reflection (all of which can be established once and for all).

2.3 Sensation-Based Systems

27

± Physiologically equidistant color differences: The introduction of the concepts of brightness, hue, and saturation has made it easier to visualize information in the system. The second difficulty, that of determining color differences, still remains. A glance at Figure 2-5 shows that the CIE chromaticity diagram cannot represent physiologically equidistant differences: The greens (from blue-green to yellow-green) occupy more than half the area enclosed by the spectral locus, while all other colors must make do with what remains. The determination of color differences is so important in practice that it must be deemed one of the principal tasks of colorimetry. One can also understand directly that the CIE diagram cannot correctly reproduce all color differences at once. The chromaticity diagram is based on the equality of color stimuli, since the mixing experiment (Section 2.2.2), in which the color matching functions are determined from the primary stimuli on the trichromatic matching colorimeter, involves using the eye solely as a kind of ªnull indicatorº for the equality of the reference and matched colors. The chromaticity diagram represents only a suitable (but arbitrary) metrical arrangement of equality judgments. In color difference measurements, however, the distinction between two color stimuli is of importance. Distinctions can be determined only through new color matching tests performed in a different way. The next section will go into more detail on this point.

2.3.2 Physiologically Equidistant Systems To determine color differences objectively, one needs to start with a notion that plays an idealized role in the physiology of colors. This is the concept of ªabsolute color spaceº, which can be thought of as a three-dimensional arrangement of color stimuli such that the distance between two color stimuli in an arbitrary spatial direction corresponds to the perceived difference. A color space with these properties cannot, however, be derived on a purely theoretical basis; its structure must be determined experimentally through color matching tests on samples having small color differences. As discussed in the previous section, such a space can be constructed with the color qualities of brightness, hue, and saturation. A configuration like that shown in Figure 2-6 results. The material needed for this purpose comprise a large number of color samples arranged by steps of hue, saturation, and finally brightness, and having physiologically equidistant differences. The derived solid is an onion-shaped body with an irregular boundary (for example, more hues can be distinguished in the dark blue than in the light red). The vertical axis is the gray scale. A horizontal cut yields a color plane like that shown in Figure 2-6; the ªringsº of the onion are loci of equal saturation. There are a number of systems built up in this way which vary in the type of color samples employed, the illumination, etc. Probably the most widely used system of this type is the Munsell system, which is available in

28

2 How Colors Depend on Spectra (Colorimetry)

Fig. 2-6. Color order based on qualities; hue, saturation, and brightness.

the form of an atlas. Brightness, hue, and saturation are termed value, hue, and chroma respectively in the Munsell system. When calculating color differences, one looks for conversion relations between the CIE system (in which color measurement must be done) and the sensationbased color system. Once these relations are known, the color differences can be calculated. Many color-difference systems have been developed, largely as a result of industrial color examination requirements. The acceptance of the CIELAB system, however, has pushed these into the background, and they need not be discussed further.

2.3.3 CIELAB System The CIELAB system has been adopted worldwide for the examination of pigmented coatings. This system, derived from the Munsell system, uses the three spatial coordinates a* (red-green axis), b* (yellow-blue axis), and L* (lightness axis) for brightness. In Figure 2-6, the a* axis is approximately the line connecting red and blue-green, while the b* axis is approximately the line connecting yellow and violet; the L* axis is the vertical lightness axis. The name ªCIELABº is a contraction from CIE and L*a*b*. In order to calculate the CIELAB coordinates, X, Y, and Z are first converted to the ªvalue functionsº X*, Y*, and Z*. The functional relation used is similar to the logarithm function and preserves physiologically equidistant (uniform) brightness steps (in a similar way to the Weber-Fechner law): r r r X 3 Y 3 Z ; Y ; Z X Xn Yn Zn

3

(2.5)

(here Xn, Yn, and Zn are the CIE tristimulus values for the illuminant used, with Yn = 100 for all standard illuminants). For X / Xn, Y /100, and Z / Zn ^ 0.008 856, however,

2.3 Sensation-Based Systems

X 7:787

X 0:138 Xn

Y 7:787

Y 0:138 100

Z 7:787

Z 0:138 Zn

29

(2.6)

With these X*,Y*, and Z* values, the a*, b*, and L* are then obtained as follows:

a* 500 (X* ± Y*) b* 200 (Y* ± Z*) L* 116 Y* ± 16

(2.7)

The color locus in the color plane (a*,b* plane) can also be described in polar coordinates: C ab

p a2 b2

(chroma, as radius vector); b hab Arctan a (hue angle, as polar angle).

(2.8) (2.9)

The expression for L* in equation (2.7) calls for some explanation. Why was the simpler form L* = 100 (Y /100)1/3, which is also similar to the logarithm function, not chosen? The answer is that the equation was based on color matching tests with gray color samples differing in brightness, which the matching colorists had to arrange on an equidistant gray scale from dark to light. The points in the diagram (Fig. 2-7) show the result for which approximation was made. It turned out that the simpler curve was too steep in the middle range, so it was ªstretchedº with a factor of 116 (instead of 100), then shifted downward by subtracting 16 so that it passed through the data points, and the condition L*(100) = 100 was restored. After this shifting, however, the curve no longer cut the Y axis at the origin but rather at a Y 4 0, so that L*5 0 below this value. Negative lightness values are meaningless, so the convention was adopted that this portion of the

30

2 How Colors Depend on Spectra (Colorimetry)

Fig. 2-7. Derivation of the L* curve (see text for explanation).

Fig. 2-8. Derivation of the L* curve (see text for explanation).

curve be replaced by the tangent to the curve that also passes through the origin* (Fig. 2-8). For the point of tangency (Yt, L*t ), we have dL*/dY)Yt = L*t /Yt, so that according to equations (2.5) and (2.7) ! r Lt 1 Y t 16 and 116 3 Yt 100 Yt dL dY

Yt

116 Y t 2=3 3 100 100

* Unfortunately, a logarithmic formulation was not immediately chosen when the CIELAB system was established; for example, L* = 100 Y* = 100 7 log (1 + 13 Y /100)/log 14 or a similar formula.

2.3 Sensation-Based Systems

31

Setting the right-hand sides equal gives solutions for the coordinates of the point of tangency: Yt 3 16 3 0:008856 ; 100 2 116 Lt

3 16 2

1 8

so that the equation of the tangent line becomes L*(Y) = (L*t /Yt ) 7 Y. Using equation (2.7),Y* is then given by Y

L Y 16 100 Lt Y 16 Y 7:787 0:138 ; 116 Y t 100 116 116 100

which is just equation (2.6) within the range from Y0 = 0 to Yt = 0.8856. Note that Y*(0) 4 0; for X*(X) and Z*(Z), equality of this equation must nonetheless be preserved so that the additive term 0.138 disappears when differences are taken for a* and b* in equation (2.7). Although the formation of differences for a* and b* in equations (2.7) seems strange at first, it has a physiological justification. In the retina, the primary excitation of the cones is processed in six types of nerve cells, four of which function in a ªspectrally opponentº antagonistic manner while the other two act in a ªspectrally nonopponentº alinear manner. The spectrally nonopponent processors form the black/white system, the spectrally opponent ones the color system. If one imagines two colors measured on pigmented coatings as radius vectors in the CIELAB color space, namely VT = {a*T, b*T, L*T } for the test sample (T) and VR = {a*R , b*R , L*R } for the reference sample (R), then DE*ab = |VT ±VR| is the color difference in the CIELAB space, measured in ªCIELAB unitsº: DEab

p Da2 Db2 DL2

(2.10)

with the components Da* = a*T ± a*R Db* = b*T ± b*R DL* = L*T ± L*R

(2.11)

In the following presentation, all differences notated as D will be defined in this sense, namely as test sample minus reference sample. A significant advantage of the CIELAB system is that the color difference can be broken down into components in another way: into brightness, ªchromaº (corre-

32

2 How Colors Depend on Spectra (Colorimetry)

sponding to saturation), and ªhueº (corresponding to the hue component used earlier), in analogy to the way the color space was constructed (Fig. 2-9): DL LT

LR

DC ab C ab;T

(lightness difference as above) 2 1=2 2 1=2 C ab;R a2 a2 T bT R bR

(2.12)

(chroma difference) DH ab DE2 ab

DL2

DC 2 ab

1=2

(2.13)

(hue difference)

Fig. 2-9. CIELAB system: breaking down of color differences into components.

DH*ab is positive if a*R b*T ± a*T b*R > 0 and negative if not. It represents the L* component of the vector product VR 6 VT and characterizes the sense of rotation in the associated vector plane. If the coincidence of the vector VR of the reference sample with the vector VT of the test sample involves a counterclockwise rotation of VR, then DH*ab is positive, and vice versa. The hue angle component is finally given by

33

2.3 Sensation-Based Systems

hab;R Arctan bT =aT

Dhab hab;T

Arctan bR =aR :

(2.14)

The sign convention for DH*ab ensures that DH*ab and Dhab will have the same sign. When these are compared with the other differences, it must not be neglected that Dhab is measured in degrees rather than CIELAB units, and thus has a different metric from these other differences. A note on the geometric meaning of DH*ab : From Figure 2-10 and equation (2.10), it follows that the line segment RT is the projection of DE*ab on the a*, b* color plane and has a length given by 2

RT Da2 Db2 DE2 ab

DL2

while, on the other hand, it can be calculated from the chromas of the test sample and reference sample and the angle between them (CR = C*ab,R , CT = C*ab,T, DC = C*ab , Dh = Dhab): 2

RT C 2R C 2T

2 C R C T cos Dh

Fig. 2-10. Geometric meaning of DH* ab (see text for explanation).

From equations (2.13) and (2.12), it follows that DH*ab2 is then: 2 DH 2 ab DEab

DL2

2

DC 2 RT

C T

C R 2 2 C R C T 1

cos Dh

In terms of the half-angle, 2 2 2 C C 1 cos Dh=2 sin Dh=2 4 C R C T sin2 Dh=2 DH 2 R T ab The right-hand side is simply the product of the two chords (Fig. 2-10) associated with CR and CT respectively, sR = 2CR sin (Dh /2) and sT = 2CT sin (Dh /2), so that the hue difference p (2.15) DH*ab sR sT

34

2 How Colors Depend on Spectra (Colorimetry)

is the geometric mean of the two chords associated with the hues of the reference sample and the test sample. For nearly achromatic, (i. e., nearly white, black, or gray) samples*, it is usually advantageous to break DE*ab down in a different way, because the usual breakdown as in equations (2.11) to (2.14) can lead to poor agreement with the observed color qualities. For example, suppose the color locus of the reference sample lies at or close to the zero point of the CIELAB system (a*R & b*R & 0) while the color locus of the test sample lies at an arbitrary distance from the zero point (a*T = 0, b*T = 0). Since Da* = a*T and Db* = b*T, the hue difference is then given by equation (2.13) as 2 DH 2 ab DE ab

DL2

2 2 C 2 ab Da Db

2 a2 T bT 0 :

This, however, does not agree with the shade actually observed in the direction of the test sample. For this reason it is better to calculate this direction and the reference sample-totest sample distance in the a*, b* color plane, as corresponding to segment RT in Figure 2-10. Its length Ds can be found for example, using equation (2.10) with DL* = 0; the direction angle of the shade Dj is obtained as tangent from the fraction Db* / Da*: Ds

p Da2 Db2 ;

Dj Arctan

Db Da

(2.16)

To simplify the evaluation, the color plane is divided into octants beginning at h = 22.58, and a color name is assigned to each of the resulting sectors (see Fig. 2-11). Table 2-3 then offers a very simple method of evaluation (with tan 22.58 & 0.4 and tan 67.58 & 2.5). For the example worked out above (a*R & 0, b*R & 0), the formula p q 2 Ds Da2 Db2 a2 T bT 6 0 correctly gives the strength while the nature of the shade follow from Db*/ Da* = b*T /a*T. The definitions and equations of the CIELAB system** are set forth in standards***. Accompanying the system when it was introduced was a recommendation * For standards see ªHue of near white specimensº and ªHue relative of near white specimensº in Appendix 1. ** On the notation: the * was selected to avoid confusion with the similarly named quantities in the earlier Adams-Nickerson system. The subscript ªabº is necessary because there is also a CIE color system with coordinates L*, u*, and u* (the ªCIELUVº system). Because CIELUV is not used for pigmented coatings, it will not be discussed here. *** For standards see ªColor Differencesº in Appendix 1.

2.3 Sensation-Based Systems

35

Fig. 2-11. Subdivision of the CIELAB color plane for calculation of the shade of achromatic samples.

Tab. 2-3. Color names Sign of Db*

+

±

±

Sign of Da*

+

yellow (Y)

|Db*/Da*| > 2.5

yellow-green (YG)

yellow-red (orange) (YR)

0.4 to 2.5

green (G)

red (R)

< 0.4

blue-green (BG)

blue-red (violet) (BR)

0.4 to 2.5

blue (B)

> 2.5

for its preferential use and testing. This proved to be justified, for the system has now gained widespread acceptance. A model of the CIELAB color space appears in Figure 2-12. The crossed cords indicate where the a* and b* axes cross; the cord running from the left foreground to the right background lies in the plane of the a* axis (left foreground is red, a* 4 0), while the cord running from right to left lies in the plane of the b* axis (right is yellow, b* 4 0). The circles marked on the plates are spaced 10 CIELAB units apart. As in the Munsell system, it is significant that there are a large number of distinguishable dark violet and light yellow hues. The formalism of the CIELAB system can easily be programmed into a desktop computer, which can also be linked on-line with a colorimeter.

36

2 How Colors Depend on Spectra (Colorimetry)

Fig. 2-12. Model of the CIELAB color space.

2.3.4 New Systems: CIE94 and CMC Despite the initial success of the CIELAB system, it should be noted that there is still room for improvement. For instance, the differences obtained by breaking down color differences are not always correctly reproduced when the system is applied to pigmented coatings. The following discrepancies are regularly established: ± Perceived brightness differences are undervalued by the CIELAB lightness difference DL*. ± Perceived saturation differences are overvalued by the CIELAB chroma difference DC*ab. Details on these points will be presented further on, in the practical section. The only remedies at this point comprise changes in the system which would eliminate these problems while preserving the differential-geometric properties. For these reasons, the CIE has proposed a new color difference formula based on CIELAB. The new ªCIE94º formula is:

DE94

s 2 DC ab 2 DH ab 2 DL kC SC kH SH kL SL

(2.17)

2.3 Sensation-Based Systems

37

where SL = 1, SC = 1 + 0.045 C*ab,R , SH = 1 + 0.015 C*ab,R (C*ab,R is the chroma of the reference). Here the ki are the parameters of externally imposed conditions, such as conditions specific to a certain application or conditions differing from the standard conditions. The standard conditions are as follows: Illuminant D65, ca. 1000 lx, surroundings gray L* = 50, ca. 100 cd/m2, sample size over 48, sample pair without gap between, homogeneous texture, 0 5 DE*94 5 5. Under these conditions, kL = kC = kH = 1. If neither of the two samples has been defined as the reference, C*ab should be taken equal to the geometric mean of C*ab,1 and C*ab,2. For coating color testing, the weaknesses of the CIE system can be compensated by a suitable choice of parametric factors, for example kH/kC = 1 and 3^ kH /kL^ 4. The formula is based on the CMC (l : c) formula but the correction terms are restricted to the chroma effect only. This is a drawback, since it must result in uncorrected color differences in the unsaturated and achromatic region. Another disadvantage is that color differences are no longer Euclidean, and spanning of a color space is therefore not possible. Two later publications have shown that the non-Euclidean CIE94 space can be transformed to an Euclidean color space so that even large color differences (ªcolor distancesº) can be calculated. Equation (2.17) was found to have two defects that must be corrected: ± The formula is not invariant to reference/sample exchange; contrary to CIE claims, the difference is not negligible. ± It is not normalized; that is, it does not use the just-accepted color difference as unit and thus is not commensurable with other color differences (e. g. with CIELAB). The first problem is remedied by the introduction of the mean C ab (see eq. 2.22 below), which is appropriate to the system as the geometric mean is not. The second is dealt with by multiplying the right-hand side of eq. (2.17) by kH . The CIE is expected to change these points. New Euclidean coordinates a94, b94, L94, C94, h94 are introduced for the transformation. It is necessary to take hab,1 and hab,2 such that their difference satisfies 08^ hab,2 ± hab,1 ^ 1808 (by interchanging the color loci if appropriate). The color difference E94 is then obtained by integrating the line element (2.17) according to the following scheme:

L94

kH L kL

(2.18)

C 94

kH ln 1 0:045 C ab 0:045 k C

(2.19)

h94 Ghab

with

G

C ab C 94 1 0:015 C ab

(2.20)

38

2 How Colors Depend on Spectra (Colorimetry)

Here 1 C 94;1 C 94;2 2 q 1 0:045 C ab;1 1 0:045 C ab;2 C 94

C ab

1 0:045

1

(2.21) (2.22)

(This formula is derived from eq. (2.21) by substituting all three C94 values with eq. (2.19).) a94 C94 cos h94 ;

b94 C94 sin h94

and finally E94

q 2 2 2 L L a a b b 94;2 94;1 94;2 94;1 94;2 94;1

(2.23)

A special case arises if h94,2 ± h94,1 4 1808: q 2 E94 L94;2 L94;1 2 C 94;2 C 94;1 These formulas hold for arbitrarily large color differences in the CIE94 space. A number of color laboratories have recently had good experience with another color-difference system, the CMC* system, and so the CMC (l : c) formulas are stated here:

DECMC

s 2 2 DL DC ab DH ab 2 lSL cSC SH

(2.24)

Here 0:040975 L ; if L* 616, 1 0:01765 L or SL 0.511, if L* < 16 0:0638 C ab SC 0:638 1 0:0131 C ab SH (FT + 1 ± F) SC SL

* CMC: Colour Measurement Committee of the Society of Dyers and Colourists in the British Standards Institution (BSI). For standards see ªColor differences: CMCº in Appendix 1.

2.3 Sensation-Based Systems

39

C 2 ab with F q 4 C ab 1900 and T 0.36 + |0.4 cos (358 + hab)| , if ±158^ hab ^ 1648, or T 0.56 + |0.2 cos (1688 + hab)| , if 1648 < hab < 3458 If there is not reference, L*, C*ab and hab must be replaced by the arithmetic means of the values at the two color loci. The factors used in the textile industry are c = l = 1; suitable values are anticipated for other industries. A later publication has shown how to transform this relation into a Euclidean color space and also revealed that it shares the shortcomings of the CIE94 equation. They are corrected by ± Allways using the arithmetic means for L*, C*ab and hab to preserve invariance to interchanging the reference and sample ± Dividing the Si functions by 0.638 to make the results commensurable with other color systems The BSI is expected to modify the CMC formulas accordingly. The transformation to a Euclidean space (ªEuclideanizationº) makes the formulas somewhat more complicated; the reader is referred to the original publication (see Section 2.7). The most recent development can only be sketched here. The German standard DIN 6176 embodies a new Euclidean color system called DIN99. Because it does not appear to have achieved its final form and because, moreover, it has little hope of international acceptance, it will not be discussed here. The CIE, too, has recently stated a new color-difference formula, CIE2000, although it has not yet been officially promulgated. Once again, a description must wait.

2.3.5 Color Order Systems Color order systems arose from the practical requirement that manufacturer and purchaser should have a common vocabulary for the manufacture of colored objects. The origins of such systems go back a long way, and from the very beginning there has been an effort to verify all orderings visually on the basis of a suitable collection of color samples. This means, however, that the difficulty inherent in any color order system was programmed into it from the start, i. e., color samples are subject to the restrictions of whether the coloring materials (pigments or dyes) are available. The controversy therefore exists already: of whether available coloring materials (or their mixtures) should be systematized, or whether a new system should be developed for color appearance. This dilemma has not yet been resolved by any color order system; it is apparent, and a problem, more or less in all systems to be discussed.

40

2 How Colors Depend on Spectra (Colorimetry)

What distinguishes such color order systems from the physiologically equidistant systems discussed earlier? This justifiable question has no easy answer, for if both systems were perfect from the physiological standpoint then they would have to be identical. In other words, the ªabsolute color spaceº (to the extent that it is Euclidean for color differences as well) would offer the ideal metric for both requirements. This fact provides the best starting point for describing the distinction. A physiologically equidistant system imposes more stringent requirements: In general, it must satisfy the postulate that the geometry of the color space is Euclidean, since otherwise it would be difficult to give an unambiguous definition of color differences (i. e., distances between color loci). Color order systems do not require this postulate, since they generally involve merely some ordering (often a naive one) of color samples. Although the samples possess some systematic features, these are not always immediately obvious. Most of these systems employ the qualities of brightness, hue, and saturation for ordering. Color order systems are still important for the classification of pigments and dyes, but play no role at all in the colorimetric inspection of colorants. This book could thus meet its objectives without taking these systems into account; the bestknown representatives will, however, be discussed briefly, because a description of them lay lead to a deeper understanding of the problems encountered in colorimetry. We have chosen the following classification in the knowledge that it is not free of arbitrariness: ± Empirical color order systems ± Colorimetry-based color order systems 1) Empirical Systems Of all the empirical systems, the Munsell system is the most important; we introduced this system in Section 2.3.2. The system approximately satisfies the postulates of a physiologically equidistant system; otherwise it would not have been such a simple matter to make it the basis for the CIELAB system. New editions of the color samples and color atlases for the Munsell system are available. The Natural Color System (NCS) was developed in Sweden and is in use there. It takes the form of a color atlas. The three variables are blackness s, chroma c, and hue f. Certain limitations became apparent after the introduction of the system: it does not span the full color space occupied by coloring materials, and it does not always give reproducible color identification codes for glossy samples. Like any empirical system, NCS is not tied to colorimetry, and so it cannot be directly converted to other color systems. A set of tristimulus values is, however, defined for one set of measuring conditions. ªRAL-Farbregister 840 HRº (RAL Color Register) is not a color order system in the narrow sense. It imposes a numbered order, with color names, on industrially manufactured coloring materials required by public authorities (railways, postal service, etc.) and by makers of consumer goods. The ordering is not highly systematic

2.3 Sensation-Based Systems

41

and features only a rough orientation to color relationships (e. g., 3 = red). Colors can be obtained as samples (paint chips); one example is RAL 3013 ªTomato Redº. The RAL Register has recently been linked to the DIN Color System through colorimetry (see below). The Color Index is also not strictly a color order system, since it lacks consistency. It includes names based on origin (ªgeneric namesº) and numbers based on chemical makeup (ªconstitution numbersº) for individual pigments. Adequate differentiation is possible only for organic pigments. 2) Colorimetry-Based Systems Among schemes based on colorimetry, the DIN Color System* should be mentioned first because it features the most complete systematization and offers many advantages. It employs the measures blackness value D, hue T, and saturation S; these are linked to the CIE system. The available color samples include only matte colors. The division of the color circle into 24 parts makes the system somewhat unclear. Because it is not widely used except in Germany, this system is not likely to become an international standard. The Optical Society of America Uniform Color Scales System (OSA-UCS) should also be mentioned. It offers a set of formulae (link to CIE) and a collection of color samples. This system is virtually restricted to the U.S.A. The Ostwald system is really only of historical interest, especially as no sample collections are available. All the color order systems mentioned up to now share the problem that they do not permit direct determination of color differences between the test sample and the reference sample or between two specimens. To make such a determination, it is necessary to use a color difference system, most commonly the CIELAB system. This in turn is possible only for the colorimetry-based order systems. The best way to avoid having to work with two fundamentally different coordinate systems (the selected color order system and the CIELAB system) would be to employ CIELAB (which spans a color space) as an order system. This is the approach taken in the new RAL Design System (RAL-DS) (a successor to the Eurocolor system, which is no longer available). The notation is directly derived from the CIELAB coordinates: hue H = hab , lightness L = L*, and chroma C = C*ab. Thus 090. 80. 70 would denote a yellow color (hab = 908) with lightness 80 and chroma 70. The RAL-DS color atlas serves as the collection of color samples. Given the stated reservations about the CIELAB system, this color order system unites all the advantages that such a system can at present. First, it offers a simple connection to colorimetry; second, it permits direct color difference determination in the same system; and since CIELAB has become accepted for color difference measurement anyway, RAL-DS should lead to an international consensus. Along with national reservations, it appears that the main obstacle to agreement on a binding color order system is conservativism. * See ªDIN Color Systemº in Appendix 1.

42

2 How Colors Depend on Spectra (Colorimetry)

2.4

Mathematical Statistics of Color Coordinates

2.4.1 Normal Distribution in Three Dimensions The values obtained from a color measurement are generally the coordinates of a color locus in color space; that is, they are components of three-dimensional vectors. This is why it is more complicated to determine, for example, a measurement error in three dimensions than in one. The components of three dimensional vectors can no longer be treated as independent variables; it must be taken into account that correlations exist between the components, and statistical analysis must allow for these correlations. For example, a* and b* are formed from the same tristimulus value Y; furthermore, the color matching functions x (l), y (l) and z (l), which lead to the tristimulus values X, Y, and Z used in calculating a*, b*, and L*, have significant overlaps (see Fig. 2-4). Mathematical treatment must therefore be oriented to extending the normal distribution from one to three dimensions. For one-dimensional variables, the probability that a measured value will lie between x and x + dx is 1 2

w dx A e where A

sx and V

n 1 P xi n i1

(2.26)

x

x

(2.25)

(2.27)

sx

(mean)

(2.28)

p V (standard deviation) 1

n

dx

1 p sx 2 p

ds

x

ds2

n P

1 i1

xi

2 x

(variance)

(2.29)

If ds2 = 1, then from equation (2.27) the limiting value xe is xe x sx

(2.30)

2.4 Mathematical Statistics of Color Coordinates

43

and, from equation (2.25), the frequency is pden

w

e

wmax

1 2

0:6

(2.31)

(wmax A) This means that the probability of encountering a measured value at xe = x + sx is 60 % as great as that of encountering the mean value. In the case of two-dimensional vectors r = {x, y}, the probability that the measured value lies between r and r + dr is given by 1 2

w dx dy B e where

ds2

dx dy

p det G B 2p g11 g12 and G g12 g22 det G g 11 g 22

g212

(2.32)

(2.33)

(determinant)

(2.34)

ds2 g11 dx2 + 2 g12 dx dy + g22 dy2

(2.35)

y ± y} dr {dx, dy} r ± r = {x ± x,

(2.36)

x

n 1P x; n i1

y

n 1P y (means) n i1

(2.37)

The expression ds2 is thus replaced by the quadratic expression in equation (2.35). If ds2 is set equal to a constant, the function dy (dx) describes an ellipse in the dx, dy plane. For ds2 = 1, this ellipse is called a ªstandard deviation ellipseº. It represents the two-dimensional analog of the standard deviation sx which is the measure of deviations in the one-dimensional case. G is the matrix formed from the coefficients of the ellipse, and det G is its determinant. The step to the third dimension now presents no difficulty. Because the quantities whose deviation is of interest here are always color differences, the remainder of the development can be stated in terms of the CIELAB color space. The formula for the probability that a triple of measured values lies between V = {a*, b*, L*} and V + dV = {a* + da*, b* + db*, L* + dL*} is now w da* db* dL* C e

1 2

ds2

da* db* dL*

(2.38)

44

2 How Colors Depend on Spectra (Colorimetry)

where

p det G C 2 p3=2 0 1 g11 g12 g13 G @ g12 g22 g23 A g13 g23 g33

(2.39) (2.40)

(symmetric matrix of ellipsoid coefficients) det G g11 g22 g33 + 2 g12 g23 g13 ± g11 g223 ± g22 g213 ± g33 g212

(2.41)

(determinant of G) ds2 g11 da*2 + g22 db*2 + g33 dL*2 + 2g12 da* db* + 2g23 db* dL* + + 2g13 da* dL*

(2.42)

dV {da , db , dL } V ± V {a ± a , b ± b , L ± L } a

n n n 1 P 1 P 1 P a ; b b ; L L n i1 n i1 n i1

(means)

(2.43) (2.44)

The exponent in the normal distribution is dominated by a quadratic form, which for ds2 = const describes an ellipsoid in the color space. The normal form ds2 = 1 now represents the ªstandard deviation ellipsoidº. The probability of encountering a measured value on the ellipsoid is, once again, ca. 60 % of the probability of the mean, since equation (2.31) holds here as well. The following statistic applies to frequency information based on the probability density: (2.45) pden exp 1=2 ds2den and ds2den 2 ln 1=pden Here, as we already know from equation (2.42), ds2den signifies a certain ellipsoid. The collection of concentric ellipsoid with parameter pden, for example with pden in 10 % steps as listed in Table 2-4, forms an image of the three dimensional normal distribution w (a*, b*, L*). To be distinguished from this is statistical information based on the cumulative probability. The cumulative probability is found by summing the probability densities between certain limits of integration, for example from zero (i. e., the mean itself) up to an ellipsoid ds2cum specified as the limit of integration. The values answer the following question: How many measured values are located inside the ellipsoid ds2cum ? If one refers to the set of all measured values, the cumulative frequency pcum is obtained; this again yields a family of concentric ellipsoids, but

2.4 Mathematical Statistics of Color Coordinates

45

Table 2-4. ds2 values for the three-dimensinal normal distribution versus frequency p, for the probability density (subscript den) and the cumulative probability (subscript cum). p

ds2den

ds2cum

0% 10 % 20 % 30 % 40 % 50 % 60 % 70 % 75 % 80 % 90 % 95 % 99 % 99.5 % 100 %

? 4.61 3.219 2.408 1.833 1.386 1.022 0.713 0.575 0.446 0.2016 0.1026 0.02010 0.01025 0

0 0.584 1.005 1.424 1.869 2.366 2.946 3.665 4.11 4.64 6.25 7.81 11.35 12.84 ?

now these image the cumulative distribution. This family of bounding ellipsoids obeys another well-known statistic, the chi-square distribution with three degrees of freedom: dsR2cum 1 x1=2 e x=2 dx (2.46) pcum 2 p1=2 0 which can also be tabulated. Table 2-4 includes recently re-calculated values of the cumulative frequency of the three-dimensional normal distribution for pcum at 10 % intervals, plus some further values in the range beyond 90 %. In the one-dimensional case, probability density and cumulative probability can also be represented in terms of simple graphs (Gaussian bell-shaped curve or Sshaped cumulative curve). In the three-dimensional case, distributions can be visualized only through families of ellipsoids, as shown here; furthermore, this is a representation suitable to the problem under consideration. The next section will discuss how the spatial position of ellipsoids can be visualized by projection into the three principal planes of the color space. The determination of the typical coefficients gik for the standard deviation ellipsoid is presented in Sections 2.4.4 and 2.4.5.

46

2 How Colors Depend on Spectra (Colorimetry)

2.4.2 Standard Deviation Ellipsoid The equation of an ellipsoid (2.42) is a special case of the equation for the general surface of order two. The necessary and sufficient conditions for the coefficients gik to describe an ellipsoid are as follows: 3 P gii > 0 g ii > 0 i 1; 2; 3; i: e:; tr G ^ i > 0 i 1; 2; 3; i: e:; det G

3 P i1

i1

^i >0 det G

det G > 0

(2.47)

^i Here tr (G) is the trace and det G the determinant of matrix G (eq. 2.40); the G are the cofactors (the 2 6 2 matrices left after the i-th row and the i-th column are deleted). Explicitly, tr (G) g11 + g22 + g33 3 P i1

^ i det G ^ 1 det G ^ 2 det G ^ 3 (g11 g22 ± g212) + (g22 g33 ± g223) + det G + (g11 g33 ± g213)

det G = g11 g22 g33 + 2g12 g23 g13 ± g11 g223 ± g22 g213 ± g33 g212

(2.48)

In order to judge the spatial orientation of the ellipsoid, it is important to know the positions of its principal axes. The partial derivatives of normal form in equation (2.42) are calculated for this purpose; the three partial derivatives are simultaneously the components of the gradient on the surface E = ds2 : 8 9 g 11 a g12 b g 13 L ; = < uE uE uE grad E ; ; 2 g 12 a g22 b g 23 L ; 2 G V (2.49) : ; ua ub uL g 13 a g23 b g 33 L ; The gradient is normal to the ellipsoid surface (Fig. 2-13). The axes of the ellipsoid (i. e., the vectors a, b, and c) have the property that the gradient is parallel to each axis; mathematically: 1 grad E G 7 V {la*, lb*, lL*} l 7 V 2 (l = scalar factor)

(2.50)

The second and last expressions lead to three equations for the three unknown coordinates, each for one principal axis of the ellipsoid.

2.4 Mathematical Statistics of Color Coordinates

47

Fig. 2-13. Gradients on the ellipsoid surface (see text for explanation).

For the system of equations to have solutions for a*, b*, and L*, the functional determinant (ªcharacteristic polynomialº of matrix G) must vanish. This requirement gives the ªcharacteristic equationº of G, also called the ªsecular equationº: 0 1 g12 g 13 g 11 l g22 l g 23 A det G l E det @ g 12 g 13 g23 g33 l l3

a2 l2 a1 l

where a0 det G ;

a1

3 P i1

a0 0

^i; det G

(2.51)

a2 tr G

(see eq. 2.48) (E = identity matrix) This is a third-degree equation in l and can be solved by well-known methods. Its ªcharacteristicº roots or eigenvalues la, lb, and lc are all real; each is associated with one of the ellipsoid axes a, b, c. The coordinate system spanned by the three ellipsoid axes is called the ªprincipal axis systemº. If the gradients in the three directions a, b, c are formed with equation (2.50), each gradient, expressed in the principal axis system, has just one component in one of the three axis directions. In this way, G from equation (2.40) becomes a diagonal matrix in which only the three diagonal components are nonzero; these positions are occupied by la, lb, and lc. From equation (2.42) this corresponds to a normal form reduced to the coefficients of the quadratic terms gii, with g11 = la, g22 = lb, and g33 = lc. From the principal axis equation of the ellipsoid a2 b2 L2 2 2 1 a2 c b

(2.52)

48

2 How Colors Depend on Spectra (Colorimetry)

it follows that the lengths of the principal axes are 1 a j aj p la 1 b j bj p lb 1 c jc j p lc

(2.53)

If we have one root l, two of equations (2.50) give the ratios u = a* / L* and u = b* / L*, that is, the directions of the principal axes: u

a g 12 g 33 L g 23 g 11

l l

g 13 g 23 g 12 g 13

u

b g12 g 33 L g13 g 22

l l

g 13 g 23 g 12 g 23

(2.54)

Then, for the principal axis a, the system of equations (2.53) and (2.54) yields a2a a2b a2L

1 la

aa ua ; aL

ab ua aL

(2.55)

and with a = {aa*, ab*, aL*} 1 aL q la 1 u2a u2a aa ua aL ab ua aL

(2.56)

and similar solutions for b and c. The axis directions can also be characterized in terms of the polar coordinate angles j and W (Fig. 2-14):

49

2.4 Mathematical Statistics of Color Coordinates

tan ja tan Wa

ab ua ; aa ua q a2a a2b aL

q u2a u2a

(2.57)

and similarly for jb, Wb and jc, Wc.

Fig. 2-14. Three-dimensional polar coordinates.

To arrive at a three-dimensional picture of the position and orientation of the ellipsoid in color space, it is useful to calculate the projections of the ellipsoid on the coordinate planes and plot these, using a plotter connected to the computer if possible. The projection on the a*, b* plane is defined by the condition that the gradient has no L* component (Fig. 2-15):

Fig. 2-15. Projections of the ellipsoid (see text for explanation).

50

2 How Colors Depend on Spectra (Colorimetry)

1 uE g13 a g23 b g33 L 0 2 uL

(2.58)

from which it follows that 1 g13 a g23 b g33

L

(2.59)

Now the normal form of the ellipsoid equation (2.42) becomes Ea*b* = g'11 a*2 + g'22 b*2 + 2 g'12 a* b* = 1 where g'11 g11

g213 g33

g'22 g22

g223 g33

g'12 g12

g13 g23 g33

(2.60)

Equation (2.60) is the desired ellipse in the a*, b* plane (horizontal projection).The two axes of this ellipse are obtained from the ªsmallº secular equation det

g011 l0 g012

g012

g022

l0

0

(2.61)

which is quadratic. By analogy to equation (2.54), its two solutions l0a ; l0b imply two linear equations for the axes: b

1 l0 g012

g011 a

(2.62)

The three projections of the ellipsoid can so be calculated and then drawn as a horizontal and two vertical projections. To do this, it is desirable to connect pairs of exterior points by ªsection linesº. These are determined as follows: The gradient of equation (2.60) also has no b* component: 1 uEa b g012 a g022 b 0 2 u b Then b

g012 a g022

(2.63)

(2.64)

2.4 Mathematical Statistics of Color Coordinates

51

From equation (2.60) it now follows that the lines are tangent to the ellipse at +a*sec : 1/2 asec g022 = g011 g022 g02 (2.65) 12 2 by virtue of the ellipse conditions). (g'11 g'22 > g'12 The projections, axes, and section lines for the other two coordinates are calculated in a similar fashion, using appropriately modified equations.

2.4.3 Standard Deviations We refer to the discussion in Section 2.4.1; given the coefficients of the standard deviation ellipsoid, we now wish to calculate the standard deviations of the color measurements. In color space, the standard deviation is a vector s, defined as the point on the ellipsoid to which s points. Because the components of a vector can be expressed as a direction and a magnitude, the vectorial standard deviation of direction n is described by sn {asn , bsn , gsn} where

(2.66)

sn | sn |

Here n = {a, b, g} is a unit vector, which accordingly has to characterize only the direction of sn. Its components are the direction cosines, that is, the cosines of the angles between sn and the three coordinate axes. Substitution in the normal form of the standard deviation ellipsoid, equation (2.42), yields ds2 (g11 a2 + g22 b2 + g33 g2 + 2 g12 ab + 2 g23 bg + 2 g13 ag) 7 s2n = 1 so that for sn 1 sn q g11 a2 g22 b2 g33 g2 2 g12 a b 2 g23 bg 2 g13 a g

(2.67)

Here sn gives the length of the ellipsoid radius in spatial direction n. Thus, if a specified spatial direction is substituted in Equation (2.67), the radius for this direction is obtained. For a color coordinate or a color difference (or a difference obtained by breaking down the color difference) having the direction of n, the radius found is the desired standard deviation sn. The task thus consists of determining only the directions of the color coordinates or color difference and its differences obtained by breaking down the color difference, then substituting these in equation (2.67).

52

2 How Colors Depend on Spectra (Colorimetry)

We begin with the color coordinates*. The calculation is particularly simple for the standard deviations of a*, b*, and L*. For a*, aa = 1 and ba = ga = 0. Substitution in equation (2.67) gives the following for sa (similarly for sb and sL ): 1 sa p ; g11

1 sb p ; g22

1 sL p g33

(2.68)

The standard deviations of C*ab and hab also follow from the coefficients of the ellipsoid. For C*ab, aC

a cos h ; C

bC

b sin h ; C

gC 0

Hence it follows that 1 sC p g11 cos2 h 2 g12 sin h cos h g22 sin2 h C p 2 g11 a 2 g12 ab g22 b2

(2.69)

The direction in which hab can vary is given by the chord perpendicular to C*ab, s = 2sH. The magnitude is + (s /2) = + sH (Fig. 2-16): aH = ± sin h ;

bH = cos h ; gH = 0

1 sH p 2 g11 sin h 2 g12 sin h cos h g22 cos2 h

(2.70)

To calculate sh, half the chord must be divided by C = C*ab and converted back to an angle by taking the arctangent: sh Arctan

1 p 2 C g11 sin h 2 g12 sin h cos h g22 cos2 h

1 Arctan p g11 b2 2 g12 ab g22 a2

(2.71)

* To simplify the notation, the subscript ab and the * are dropped from the color coordinates and color differences; thus C = C*ab, DE = DE* ab, etc.

2.4 Mathematical Statistics of Color Coordinates

53

Fig. 2-16. Calculation of sh (see text for explanation).

Now on to the standard deviations of the color differences. Here the standard deviation ellispoid GD, of the color differences must be known. It is defined as in equation (2.40) except that the gik are now replaced by gDik ; da*, db*, and dL* by the differences dDa* = Da* ± Da*, dDb* = Db* ± Db*, and dDL* = DL* ± DL*, where Da*, Db*, DL* are the arithmetic means. We use arguments presented in the next section (Section 2.4.4), where it is shown that the difference ellipsoid GD is linked to the coordinate ellipsoid GR of the reference by the relation GD gDik 1=2 gRik 1=2 GR

(2.72)

Thus, if GD has not been determined separately, i. e., if only the reference ellipsoid GR is available, then the coefficients of GD can be calculated with equation (2.72). If, on the other hand, only GD is known, then GR can be obtained from equation (2.72). Proceeding in the same way as before, we substitute the direction cosines of the respective color differences in equation (2.67), thus obtaining the following relationships. For the differences Da*, Db*, DL*: 1 1 1 sDa q ; sDb q ; sDL q gD11 gD22 gD33

(2.73)

For the hue difference DH*ab : The hue difference is perpendicular (see Fig. 2-10) to the bisector of the angle h0 = (1/2)(hR + hT).

54

2 How Colors Depend on Spectra (Colorimetry)

Therefore,

aDH ± sin h0 ; bDH cos h0 ;

gDH 0

so that by equations (2.67) and (2.70) sDH sH (gDik , h0)

(2.74)

For the hue angle Dhab : Its standard deviation is the angle associated with sDH, that is, tan sDh = sDH /OW (Fig. 2-10). The length OW can be expressed in either of two ways, in terms of DH or OH, or in terms of both. From Figure 2-10 and equation (2.15), it is also easy to show that OH2 = CRCT. Accordingly, sDh Arctan 2 sDh =DH tan Dh=2 n o Arctan sDh = CR CT 1=2 cos Dh=2 n 1=2 o Arctan sDh = CR CT DH=22

(2.75)

For the chroma difference DC*ab : Because, in general, the chromas of reference sample and test sample differ in direction (Fig. 2-10), their standard deviations sC,R and sC,T must be calculated separately using equation (2.69). This must be done with the ellipsoid GR of the reference sample; if it is not available, equation (2.72) is employed to calculate it from GD. Then, by the additive rule for variances, 1=2 sDC s2C;R s2C;T

(2.76)

For the color difference DE*ab : The direction cosines are aDE

Da Db DL ; bDE ; gDE DE DE DE

The magnitude of the standard deviation is then DE sDE q gD11 Da2 gD22 Db2 gD33 DL2 2 gD12 Da Db 2 gD23 Db DL 2 gD13 Da DL (2.77)

2.4 Mathematical Statistics of Color Coordinates

55

The equations fulfill the objective: The standard deviations of the three color coordinates, the chroma, and the hue angle, as well as the standard deviations of the color difference and of all its composant differences, can now be calculated. All that is necessary to know are the six coefficients gDik of the standard deviation ellipsoid of the differences (or gRik of the reference) for a specified threshold confidence level.

2.4.4 Color Measurement Errors and Significance The ellipsoid coefficients gik needed for all the calculations in the preceding section can be determined by known methods. Firstly, from the number of measurements n, the arithmetic means are formed in accordance with equation (2.44), then the variances of a*, b*, and L* are formed: Var a Var b Var L

1 n

1 i1 1

n

n P

1 i1 1

n

n P

n P

1 i1

ai

a 2 ;

bi

b 2 ;

Li

L 2 ;

(2.78)

In the case of vector quantities, the variances alone are not enough to characterize the deviations in space. Correlations between the individual components must also be taken into account and can strongly influence their standard deviations: If, for example, large values of a* are always associated with large b* and L* values, then the standard deviation of a* will be smaller than if a*, b*, and L* varied in random sequence with no correlations. The strengths of the correlations between the three pairs of components are expressed in terms of the covariances: Cov a ; b Cov b ; L Cov a ; L

1 n

1 i1 1

n

n P

1 i1 1

n

n P

n P

1 i1

ai

a bi

b

bi

b Li

L

ai

a Li

L

(2.79)

56

2 How Colors Depend on Spectra (Colorimetry)

Now the variances and covariances are entered in a matrix V: 0 1 0 Cov a ; b Cov a ; L Var a u11 Var b Cov b ; L A @ u12 V uik @ Cov a ; b Cov a ; L Cov b ; L Var L u13

u12 u22 u23

1 u13 u23 A u33 (2.80)

This matrix is symmetric, because uik = uki. It is the three-dimensional analog of the variance s2x of the one-dimensional normal distribution. In the one-dimensional case, the precision can be specified in terms of the confidence interval, the interval within which a given percentage of the measurements are expected to fall. Similarly, the precision in the three-dimensional case can be specified by the ellipsoid, which has the point {a*, b*, L*} as its center (reference). The ellipsoid coefficients gik are the elements of the inverse matrix of V; thus* gik G V

1

(2.81)

G is also symmetric, since it was obtained from a symmetric matrix by inversion; gik = gki is also one of the necessary ellipsoid conditions. From this we see the following: Only by using the covariances can the standard deviation ellipsoid be obtained; in general, the ellipsoid is not oriented to the principal axes, because the measures of deviations must be invariant to the coordinate system chosen. If no correlation exists between the measured values of the reference and the test sample, then the additive rule for variances and covariances leads to the following relation for the reference, test sample, and color difference matrices: VD VT + VR or, after substitution of the respective standard deviation matrices, ±1 ±1 G±1 D GT + GR

If GT and GR are equal (GT = GR), then ±1 G±1 D 2 GR

or, after inverting, GD 1=2 GR This relation was used in Section 2.4.3 (eq. 2.72). * For an example of matrix inversion, see Chapter 6.

(2.82)

2.4 Mathematical Statistics of Color Coordinates

57

The preceding arguments used to determine gik thus close the circle: All the standard deviations of color measurement values can be calculated using equations (2.68) to (2.77). The formulae were obtained from the normal form of the ellipsoid G, that is, with ds2cum = 1. A look at Table 2-4, however, shows that according to the w2 distribution this ellipsoid contains only 20 % of all the measured values; we thus say that the ªconfidence intervalº 1 ± a is just 20 %. It would be desirable to have a confidence interval of 70 % (which would roughly correspond to the range of + sx customarily used with the one-dimensional normal distribution). Again from Table 2-4, this confidence interval is obtained with a value ds270 % = 3.665 of the w2 distribution. The following procedure results: ± If the ellipsoid is to be plotted as in Section 2.4.2, the gik should be divided by 3.665. ± If the standard deviations are to be calculated as in Section 2.4.3, the sx values should be multiplied by 3.6651/2 = 1.914. If a different confidence interval is required, the corresponding value for ds2cum from Table 2-4 should be used instead. The statistical concept of significance offers quantitative information as to whether a measured value ± here, the color difference and its composant differences ± is ªtrueº or whether it is falsified solely by measurement errors. This risk is always present when the color differences are very small, of the order of the error deviations. In the language of mathematical statistics, this means that it is necessary to determine whether the color difference found is larger or smaller than a ªcritical valueº t (also called the ªsignificance thresholdº). This value is formed in the same way as illustrated for the measurement error, with one additional step: division by the square root of the number of measurements n1/2. This extra step takes account of the fact that the mean becomes more and more accurate as the number of measurements increases, so that the deviations of the measurements about the mean are increasingly attributed to their real value. The value of t thus is given by the number of measurements n, the standard deviation sx, and the desired confidence interval 1 ± a:

t1

a

1=2 sx ds21 a =n

(ds2cum from Table 2-4)

(2.83)

The measured color difference DF is significant if | DF | 4 |tDF |, and not significant if | DF |^ | tDF |. The principles and methods for determining the significance of color differences are presented in DIN 55600. The standard purposely avoids calculating the standard deviations of the CIELAB coordinates, since the nonlinearity of the relations used for the transformation from the CIE system means that these values do not necessarily have a normal distribution. Even so, there is no objection to applying this system to the CIELAB coordinates themselves. The arithmetic mean of the coordi-

58

2 How Colors Depend on Spectra (Colorimetry)

nates of the reference also corresponds better to the true value than does the color locus of a selected individual preparation. The application to color differences alone is justified because color differences can be represented to a good approximation as differentials. As in the theory of errors, the total differential can be used; higher-order derivatives need not be considered. The total differential in fact represents a linear transformation in a small neighborhood, and since its coefficients in the neighborhood of a color locus are largely constant, it follows that da*, db*, and d L* have just as normal a distribution as the d X, dY, and dZ, or as the dR of the reflectances, to which d X, dY, and dZ are related in a linear function. The total error of a color measurement on a coating is made up of ± Error due to sample preparation ± Error due to measurement The preparation error can be further broken down into ± Error due to sample fabrication (sampling, grinding, etc.) ± Error due to application (application, drawing down) ± Error of homogeneity (constancy over the entire sample) Thus the covariance matrices are related to one another as follows: Vtot Vprep Vmeas Vprep Vsam + Vappl + Vhom

(2.84)

The error matrices are determined as follows: ± Measurement error matrix Vmeas : Make 20 determinations of color differences on the same sample ± Homogeneity error matrix Vhom : Perform 20 color measurements statistically distributed over the entire sample surface ± Application error Vappl : Apply a preparation of sample and a preparation of reference 20 times and measure ± Total error Vtot : Prepare, apply and measure 20 preparations of sample and reference. The covariance matrix for each error is calculated with eq. (2.80). Equations (2.84) then give the preparation error Vprep and the sampling error Vsam as the differences of the V matrices. As a rule, Vmeas is very much less than Vprep, and the colorimetric laboratory must make every effort to keep the latter as small as possible. The ellipsoid coefficients of the several error components (the G matrix) is finally obtained by matrix inversion.

2.4 Mathematical Statistics of Color Coordinates

59

2.4.5 Acceptability The manufacturer of pigments or pigmented coatings is expected to make products that match specified samples (ªreferencesº). The instrument for determining the matches is the human eye; products that pass this examination by the colorist are ªacceptedº and are said to be ªconformingº (to a standard). In general, to say that the test sample and the reference match is not to say that the measurements are absolutely identical; instead, it means that the sample values lie in a specified tolerance range. This initially unknown tolerance range cannot be derived from the general rules of colorimetry but must be determined experimentally in each individual case. The technique involves the coloristic matching of color samples close to the reference. The justification for this procedure was stated in Section 2.3.1; furthermore, none of the existing color difference systems is perfect in exactly reproducing the perceived color differences (not even the CIELAB system, Section 2.3.3, which has become the standard chiefly because of its consistent use). For this reason, a systematic series of graded color samples are placed around the reference in each instance, and this set is presented to the colorist for evaluation. As a rule, the submitted samples are divided into two sets (ªacceptedº and ªnot acceptedº) in accordance with the colorist's judgment. (An intermediate range identified as ªconditionally conformingº can also be established.) The goal of statistical analysis of the colorist judgments is to derive the coefficients of the ªacceptability ellipsoidº, since this supplies the computer with the needed selection criteria in a computer-controlled production control system. The most important procedure for deriving usable estimation functions for the parameters of a distribution is the ªmaximum likelihood methodº. As applied to our three-dimensional case, the steps are as follows: In accordance with equations (2.38) and (2.42), the probability that a test sample i will be judged as conforming to a reference is expressed in terms of Da*, Db*, and DL*, the color differences of the i-th sample. If the samples match the reference, the color differences vanish. Obviously, from equation (2.42), this implies that ds2i = 0 and w = 1; that is, the sample is in principle always judged to conform. In practice, a psychophysical experiment such as the one just described is always assumed to have a certain error rate p (false alarm rate). For example, a sample colorimetrically identical to the reference may not be judged as conforming. Thus, the probability that the colorist will adjudge such a sample as conforming to the reference is equal to q = 1 ± p, and the probability that any sample i will be judged as conforming is q exp (± ds2i /2). The complementary probability, that is, the probability that the sample will be judged as nonconforming, is then 1 ± q exp (± ds2i /2). If the colorist making these judgments is permitted only the choices ªconformingº and ªnonconformingº, the probabilities of these two answers can be linked through the binomial distribution and a likelihood function can be constructed:

60

2 How Colors Depend on Spectra (Colorimetry)

! n Y N M qe ji i1

1 2

ds2i

ji 1

qe

1 2

ds2i

N

ji

(2.85)

In this formula, n is the number of color samples; ji is the number of ªconformingº judgments; and N is the number of colorists making the judgments. The maximum likelihood method approximates the unknown parameters q and g11, g22, g33, g12, g23, g13 by taking values which maximize M. A necessary condition for M, as a differentiable function of q and the gik, to have a maximum (except at the boundary) is that the partial derivatives with respect to q and the gik vanish: uM uM uM uM uM uM uM 0 uq ug11 ug22 ug33 ug12 ug23 ug13

(2.86)

Because the factors in equation (2.85) are nonnegative, M is generally positive at a maximum. The natural logarithm ln M, which is a monotonically increasing function, therefore has a maximum precisely where M has a maximum. This result suggests replacing M with the function ln M, so that instead of equation (2.85) we have 1 ji ds2i ji ln q 2 i1 n P 1 ds2i 2 N ji ln 1 q e const

ln M

n P

i1

(2.87)

and instead of equation (2.86) u ln M u ln M 0 uq ugik

(2.88)

Now, instead of the laborous differentiation of the products, only the sums have to be differentiated. To determine the desired values of gik and p, iterative procedures for zero finding can be applied; these need not be discussed further here. By following the procedure described, we obtain ellipsoids of the probability density in a different way from the method based on the covariance matrix. Thus, the shape and position of such an ellipsoid in color space represents the probability with which a color locus lying on the ellipsoid will be deemed as conforming. This method is somewhat complicated, both experimentally and mathematically, but it is the best of all the methods tested; the mathematical difficulties are taken care of by the development of a functioning program. It must be pointed out that there are simpler methods of estimating the parameters. These are not discussed

2.4 Mathematical Statistics of Color Coordinates

61

here because either they presuppose some simplified version of the psychophysical experiment or else they are not efficient enough. In the equations written above, ds2i is the quadratic expression ds2 of the i-th sample: ds2 g11 Da*2 + g22 Db*2 + g33 DL*2 + 2g12 Da* Db* + + 2g23 Db* DL* + 2g13 Da* DL*

(2.89)

with ellipsoid G = gik. It is often desirable to relate the quadratic expression not to the L* a* b* coordinates but, instead, to the coordinate system spanned by the three orthogonal difference vectors DC*ab, DH*ab, DL*. It will now be shown that this is possible; The new ellipsoid G' = g'ik is obtained by transformation to the orthogonal DC*ab, DH*ab, DL* system. First, the a* and b* of the reference are expressed in terms of its polar coordinates C*ab and hab : a* C*ab cos hab

b* C*ab sin hab

Then the color differences (with DH*ab = 2 [C*ab (C*ab + DC*ab)]1/2 sin (Dhab /2) & C*ab Dhab) are given by the following formulae (see eq. 2.15 and Fig. 2-10): Da* & da* cos hab dC*ab ± C*ab sin hab dhab Db* & db* sin hab dC*ab + C*ab cos hab dhab After substituting these expressions into equation (2.89) and comparing the coefficients ds2 g'11 DC*ab2 + g'22 DH*ab2 + g'33 DL* 2 + + 2g'12 DC*a b DH*a b + 2g'23 DH*ab DL* + 2g'13 DC*a b DL* we obtain the new ellipsoid g'11 = g11 cos2 hab + g12 sin 2 hab + g22 sin2 hab g'22 = g11 sin2 hab ± g12 sin 2 hab + g22 cos2 hab g'33 = g33

1 (g22 ± g11) sin 2 hab 2 g'23 = g23 cos hab ± g13 sin hab g'12 = g12 cos 2 hab +

g'13 = g23 sin hab + g13 cos hab

(2.90)

62

2 How Colors Depend on Spectra (Colorimetry)

The inverse transformation g'ik ? gik is described by the formulas g11 = g'11 cos2 hab ± g'12 sin 2 hab + g'22 sin2 hab g22 = g'11 sin2 hab + g'12 sin 2 hab + g'22 cos2 hab g33 = g'33 1 (g'11 ± g'22) sin 2 hab 2 g23 = g'23 cos hab + g'13 sin hab g12 = g'12 cos 2 hab +

g13 = g'13 cos hab ± g'23 sin hab

2.5

(2.91)

List of Symbols Used in Formulas

a, b, c ab a*, b*, L* a94, b94, L94 a, b, c a a, b, g A B c cum C C, C*ab C94 Cov den d ds2 D DE*ab, DE DE *94 Dhab,Dh DH*ab, DH

magnitudes of a, b, c (as subscript) denotes CIELAB CIELAB coordinates CIE94 coordinates vectors of the ellipsoid axes significance level; 1 ± a, confidence interval direction cosines of s; components of n normalization factor for one-dimensional normal distribution normalization factor for two-dimensional normal distribution CMC parametric factor (as subscript) denotes cumulative probability normalization factor for three-dimensional normal distribution chroma (CIELAB) chroma (CIE94) covariance (as subscript) denotes probability density difference (measured value minus its mean) quadratic form of normal distributions color difference expressed as difference between CIELAB coordinates (test sample minus reference) color difference (CIELAB) color difference (CIELAB 94) hue angle difference (CIELAB) hue difference (CIELAB)

2.5 List of Symbols Used in Formulas

Ds e E Ea*,b* ECMC E94 F F gik G hab , h h94 i j kC, kH, kL l l L* l L94 m max M n n n N p j (l) j q r R R sR, sT sec sn SC, SH, SL sx t t T T W

magnitude of shade (as subscript) denotes limiting value area of ellipsoid circumference of ellipse color distance (CMC) color distance (CIE94) CMC parameter color stimulus in CIE system; CIE color locus matrix element in i-th row and k-th column of G matrix of ellipsoid coefficients hue angle (CIELAB) [in degrees] hue angle (CIE94) number of sample evaluated number of ªconformingª judgments CIE94 parametric factors wavelength scalar factor in secular equation (see a*) CMC parametric factor (see a94) physical measure of intensity (as subscript) denotes maximum likelihood function number of measurements (as subscript) denotes standard illuminant unit vector in direction of s number of colorists frequency (statistics) spectral distribution meridian angle (spherical coordinates) individual probability radius vector reflectance (as subscript) denotes reference circle chords in CIELAB system (as subscript) denotes section line vector of standard deviation in direction of n CIE94 weighting functions standard deviation of quantity x significance threshold (as subscript) denotes point of tangency CMC parameter (as subscript) denotes test pigment polar angle (spherical coordinates)

63

64

2 How Colors Depend on Spectra (Colorimetry)

u, u uik V V

Var,V w x, x x, y, z xl, yl, zl X,Y, Z X,Y, Z X*,Y*, Z* y, y

2.6

auxiliary variables for principal axis directions matrix element in i-th row and k-th column of V CIELAB color locus covariance matrix with subscripts: appl of application hom of homogeneity meas of measurement prep of preparation tot total variance probability function measured value and its arithmetic mean (CIE) chromaticity coordinates tristimulus values of spectral colors; CIE color matching functions (CIE) reference stimuli (CIE) tristimulus values CIELAB value functions measured value and its arithmetic mean

Summary

The basic principle of colorimetry is that, using just three selected lights, all other color stimuli can be simulated fully by additive mixing. On the other hand, a color stimulus can also be prepared from the spectral colors by mixing; thus it has a spectral distribution, which in the case of object colors has been given the name ªspectral reflectanceº. The trichromatic principle makes it possible to construct a threedimensional color space once three reference stimuli (primaries) have been defined. In this color space, the coordinates are to be understood as components of a vector. This trichromatic theory has recently gained physiological confirmation. The CIE color notation system and the CIE standard observer were created on this basis in 1931; the principles are stated in standards. The CIE system imitates the human eye: The huge number of possible optical stimuli is reduced in a meaningful way to a much smaller set that can be comprehended by the mind. The CIE color notation system has, since its creation, proved its unrestricted suitability for use in all technical applications of colorimetry. It permits worldwide understanding as to colors. As to pigment evaluation, however, there are additional demands. The system is not easy to visualize, and physiologically equidistant color differences cannot be determined with it. For ease of understanding, Helmholtz proposed a different three-variable description: brightness, hue, and saturation. In the determination of color differences, one of the principal tasks of colorimetry, there

2.6 Summary

65

was no major progress until recently. For this purpose, a color space must be constructed through matching experiments on samples with small color differences; the best-known system of this type ist the Munsell system. After a CIE recommendation, the CIELAB system (based on the Adams-Nickerson system) has been used in pigment testing for some years. In CIELAB, quantities evaluated physiologically can first be calculated from the CIE tristimulus values, and by taking differences in pairs between the results the CIELAB coordinates are then obtained. This process of forming differences finds its physiological justification in the structure of the nervous system that processes information from the eye. The determination of actual color differences is then accomplished by calculating the vectorial distance between the color loci of the reference and test pigments and its breakdown into the three components lightness, chroma, and hue. Thus color measurement is performed in the CIE system and the results are then transformed into the CIELAB system (preferably with the aid of a computer, since CIELAB lends itself to programming). Despite the success of CIELAB, there are needs for improvement (DL* undervalues the perceived brightness, DC*ab overvalues the perceived saturation). For that, a new formula ªCIE94º has been created. The color system corrects some shortcomings of CIELAB. Even this system has the drawback of not spanning a non-euclidean color space, so that large color differences (ªcolor distancesº) cannot be calculated. A recently developed technique, however, can transform the CIE94 color space to an euclidean color space, thus permitting the calculation of color distances. The CMC color system, originally developed for the textile industry, was also described briefly. This system is gaining in importance for color measurement on coatings as well. The system was later euclideanized so that color distances can be calculated. More recent systems such as DIN99 and CIE2000 were merely mentioned, because they do not yet exist in final form. This chapter dealt briefly with color order systems, which were classified as empirical and colorimetry-based systems. The second group included the DIN Color System and the OSA-UCS system. Special attention was focused on the new RAL Design System with its color atlas, which provides an ideal link between color order and CIELAB. In pigment testing, determining the precision of color measurement is the key to assessing the significance of color differences. The precision serves as a figure of merit both for the colorimetric measurements in full shade comparisons and for the colorimeter being employed (with the help of a collection of samples). The treatment begins with known relations describing the statistics of colorimetric data. The first step is to calculate the variances of the CIELAB coordinates. These are not, however, sufficient to describe the deviations of the measurements; if one colorimetric value shows large deviations, it is important to know whether the other two also vary widely or whether they are stochastically distributed. For this reason, the covariances are also necessary for a complete description. The three variances and the three covariances are entered in a symmetric matrix, the inversion of which

66

2 How Colors Depend on Spectra (Colorimetry)

yields the coefficients of the standard deviation ellipsoid. The equation of the ellipsoid always contains a term on the right-hand side for which the tabulated w2 distribution value for a given confidence interval must be substituted. A relatively new procedure is the use of the resulting ellipsoid for the calculation of errors in the measured CIELAB coordinates, in the color differences, and in the composant color differences. These are equal to the radii of the ellipsoid in the spatial direction corresponding to the coordinate or color difference in question. The formulas for calculating these standard deviations are stated in this chapter, along with formulas useful for visualizing the spatial position of the error ellipsoid. In the manufacture of pigments and pigmented coatings, the requirement of conformity (to a standard of reference) is leading to a more rational procedure for acceptability testing. Rapid development in the computer field has opened up the possibility of letting a computer make the decision as to conformity, using specified criteria. But such criteria cannot be derived from purely colorimetric considerations; they must be obtained by having the responsible colorists perform matching tests on appropriate samples. In order to calculate the ellipsoid coefficients, it is desirable to employ the maximum likelihood method; while this is a old technique, it has recently been applied to this problem in the U.S.A. It has to be kept in mind that misjudgments also occur and must be smoothed out statistically. The likelihood function can be maximized with the help of a formula based on a binomial distribution of judgments. The mathematical operations can be substantial and a computer is needed. The calculation yields ellipsoids of probability density.

2.7

Historical and Bibliographical Notes

The crucial step in color theory occurred when Newton [1] laid the foundations for a scientific understanding of color phenomena by breaking sunlight down into its spectral components and correctly interpreting this process. The invention of the spectrograph by Young [2] also made it possible to measure spectral distributions. Young further discovered empirically the physiological relationships that were later formulated by Grassmann [3]. For the physiological principles of the YoungHelmholtz theory of color vision see, e. g., [4]; Helmholtz himself reported on the trichromatic theory [5]. Nonetheless, it was not until 1931 that a definition of the primary stimuli was agreed on. In that year the CIE, on the basis of the first usable experimental studies of the color matching functions by Wright [6] and Guild [7], decided to propose such primary stimuli (primaries, reference stimuli) as worldwide standards. The curves evaluated by various observers were averaged and the result was defined as the ªCIE standard observerº. The sensory organs as information-processing systems are described in, e. g., [8]. A number of excellent publications on the theoretical principles of colorimetry have appeared both in English [9±12] and in German [13±16]; further citations

2.7 Historical and Bibliographical Notes

67

can also be found in these. Colorimetry with special application to pigments is described by Gall [17]. For the construction of a physiologically equidistant color space see, e. g., [18]; [19] is the Munsell atlas. The DIN Color System was introduced by Richter [20]; the RAL Design System, by Gall [21]. The Adams-Nickerson (AN) system for testing pigments [22], [23], derived from the Munsell system, had been well known for decades when, in 1973, the German Standards Committee (DIN) and later the CIE proposed its testing in the form of the CIELAB system. CIE94 has appeared as CIE Publication No. 116 [24]. The transformation from CIE94 to an euclidean color space is described in [25, 26]. The CMC system was later euclideanized as well [27]. The new DIN99 system has come under sharp criticism [28]. The physiology of color vision is described in, e. g., [29], [30]. A comprehensive treatment of the mathematical statistics of color coordinates can be found in [31]. The theoretical basis for characterizing test errors in the colorimetric evaluation of color differences was set forth earlier and fully developed, in a different context, by Brown and MacAdam [32]. The problem solved by these authors was to determine experimentally the perceptibility threshold for color differences. Their analysis led to ªtolerance ellipsoidsº localized in color space. The reference was located at the center of each such ellipsoid; all colors which were not distinguishable from the reference by the observer are located within the ellipsoid, while outside the ellipsoid are the colors that the observer can distinguish from the reference. It had already been demonstrated that the figure must be an ellipsoid for normally distributed color samples [33]. Later, Robertson also proposed the Brown-MacAdam principle for test errors [34]. The justification is that the two problems have identical mathematical structure: As has been shown, both cases involve the extension of the Gaussian normal distribution from one to three dimensions; see, e. g. [35]. The analysis of the total error into error components is described in [36]. Tables giving the values of statistical functions such as the w2 distribution can also be found in statistics textbook and collections of mathematical tables, e. g. [37]. The acceptability is treated in [39]. The maximum likelihood method goes back to Gauss (1880) and was later generalized by Fisher in 1912 [38]. The principles of the technique used here [39] were set forth in a publication by Billmeyer and co-workers [40] and later recommended by Robertson [41] on behalf of the CIE. Another calculation method is described by Brockes and co-workers [42]. It must not be ignored that cybernetics, more than any other field of knowledge, has contributed enormously to the development of colorimetric test methods. Cybernetics has figured prominently in at least three areas and will help to determine the course of future development: ± Through development of computers for use specifically in color examination. ± Through the application of cybernetic conceptual models to measurement procedures and instruments.

68

2 How Colors Depend on Spectra (Colorimetry)

± Through the application of cybernetic conceptual and analytical methods to the phenomenon of vision [43]. The last of these points is important because an improved knowledge of vision is an essential condition, e. g., for the construction of better colorimeters. On the use of computers in the laboratory see, e. g. [44]. The history of colorimeters and color measuring has been dealt with elsewhere in detail [15], and it is therefore not taken up here.

References [1] [2] [3] [4] [5] [6] [7] [8] [9] [10] [11] [12] [13] [14] [15] [16] [17] [18] [19] [20] [21] [22] [23] [24] [25] [26] [27] [28] [29] [30] [31] [32] [33] [34]

I. Newton: Optics. Innys, London 1704±1730 (reissued by Mc Graw-Hill, New York 1931). T. Young, Phil. Trans. Roy. Soc. London 92 (1802) 12. H. Grassmann, Ann. Phys. (Leipzig) 89 (1853) 69. G. Wald, Angew. Chemie. Internat. Edit. 80 (1968) 857. H. v. Helmholtz: Handbuch der physiologischen Optik. Voss, Leipzig 1911. W. D. Wright, Trans. Opt. Soc. London 30 (1928/29) 141. H. Guild, Phil. Trans. Roy. Soc. London A 230 (1931/32) 149. K. Steinbuch: Automat und Mensch, Springer, New York 1971, 4. edit., 200 ff. W. S. Stiles, G. Wyszecki, Color Science, Wiley & Sons, New York, 2. edit., 1983. D. L. MacAdam, Color Measurement, Springer, New York, 2. edit., 1985. F. W. Billmeyer jr., in Encyclopedia of Chemical Technology, 3. edit., J. Wiley & Sons, New York 1979,Vol. 6, 523. R. W. G. Hunt, Measuring Color, J. Wiley & Sons, New York, 1987. E. Schrædinger, Ann. Phys. (Leipzig) 63 (1920) 397, 427. M. Born, Naturwissenschaften 50 (1963) No. 2, 3. M. Richter, Einfçhrung in die Farbmetrik, W. de Gruyter, Coll. Gæschen, Berlin-Heidelberg 1976. A. Brockes, D. Strocka, A. Berger-Schunn, Bayer-Farben-Revue, Sonderheft 3/2 D, 1986. L. Gall, The Color Science of Pigments, BASF Ludwigshafen, 1971. G. Wyszecki: Farbsysteme, Musterschmidt, Gættingen 1960, 81. A. H. Munsell: Atlas of the Munsell Color System, Wadsworth-Howland, Boston 1915. M. Richter, Farbe I (1953) 85. L. Gall, farbe + lack 98 (1992) 863. E. Q. Adams, J. Opt. Soc. Am. 32 (1942) 168. D. Nickerson, K. F. Stultz, J. Opt. Soc. Am. 34 (1944) 550. Commission Internationale de l'Eclairage, Industrial Color Difference Evaluation, CIE Technical Report No. 116, CIE Central Bureau,Vienna, Austria. H. G. Vælz, Die Farbe 44 (1998) No. 1±3, 1. H. G. Vælz, Die Farbe 44 (1998) No. 3±4, 97. H. G. Vælz, Die Farbe 45 (1999/2000), No. 1±3, 1. H. G. Vælz, Die Farbe 46 (2000), in press. D. H. Hubel, Eye, Brain and Vision, Sci. Am. Lib., New York 1988. J. Walraven, 7th Aic Congress 1993 Budapest, Congress book. H. G. Vælz, farbe + lack 88 (1982), S. 264 und 443. W. R. J. Brown, D. L. MacAdam, J. opt. Soc. Am. 39 (1949) 808. L. Silberstein, D. L. MacAdam, J. opt. Soc. Am. 35 (1945) 32. A. R. Robertson, The specification of the performance characteristics of colorimetric instruments, CIE TC-1.3, June 1973.

2.7 Historical and Bibliographical Notes

69

[35] K. Stange, Angewandte Statistik, Bd. I (1970) u. Bd. 2 (1971), Springer, New York. [36] H. Schmelzer, H. G. Vælz, Signifikanz von Farbabstånden, in DIN-Fachbericht 49, Beuth-Verlag GmbH, Berlin, 1995. [37] W. Abramowitz, I. Stegun, Handbook of Mathematical Functions, Nat. Bur. Stand., Appl. Math. Ser. 55, US-Gov. Print Off., Washington, 3. edit. 1965. [38] E. Kreyszig, Statistische Methoden und ihre Anwendungen, Vandenhoeck u. Ruprecht, Gættingen, 3. edit., 3. reprint, 1974, 174 ff. [39] H. G. Vælz, Toleranzfindung, in DIN-Fachbericht 49, Beuth-Verlag GmbH, Berlin, 1995. [40] F. W. Billmeyer, W. G. Howe, R. M. Rich, J. opt. Soc. Am. 65 (1975) 956. [41] A. R. Robertson, Col. Res. Appl. 3 (1978) Nr. 3, 149. [42] D. Strocka, A. Brockes, W. Paffhausen, Farbe + Design 1980 Nr. 15/16, 75. [43] H. G. Vælz, XI. Fatipec-Kongress 1972 Florence, Edizione Ariminum, Mailand, 43. [44] J. Hengstenberg, K.-H. Schmitt, B. Sturm, O. Winkler (Ed.) Messen, Steuern, und Regeln in der chemischen Technik, Springer New York, 3. edit., 1985.

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

3

How Spectra Depend on the Scattering and Absorption of Light (Phenomenological Theory)

3.1

Introduction

3.1.1 Phenomenological Theory and Its Significance The name ªphenomenological theoryº refers to all theoretical statements about how the radiance of light incident on a layer is affected by absorption and scattering. Such a theory affords the needed physical-theoretical and mathematical tools for describing how the reflection spectrum of a layer can be derived from its absorption and scattering properties as well as its thickness. The model employed is that of light pathways or channels, roughly as known from geometrical optics; the absorption or scattering action of the medium is represented by optical material constants, that is, purely phenomenological quantities. The phenomenological theory treats the medium as a continuum characterized by the physical qualities of absorption and scattering; accordingly, the presence of discrete particles as a necessary (but not sufficient) condition for scattering is of no significance in this theory. Speaking casually, one can say that ªthe phenomenological theory does not know anything about particlesº; in other words, it deals in physical qualities that can be described without reference to pigment particles and their special properties. To attribute absorption and scattering properties to a single particle, one must resort to the ªcorpuscular theoryº (see Chapter 5, also Figs. 1-2 in Chapter 1). Only that theory makes further statements about the optical material constants from phenomenological theory, indeed attributing them to the refractive index, size, and shape of the individual particle. In a certain sense, descriptions of the concentration dependences of the optical constants provide a bridge between the phenomenological and corpuscular theories, defining coefficients related to the pigment or dye concentration and then treating these coefficients as independent of the concentration. In this context, the position of the phenomenological theory of turbid media clearly implies the fundamental importance of the theory for the pigmenting of lacquers, paints, plastics, and so forth, and thus for all matters relating to the application and economics of coloring materials. In this chapter, we will briefly present the many-flux theory as a complete, general phenomenological theory, with a detailend treatment of the four-flux theory, and derive the most important formulas. It will be seen that the theory of Ryde is a special case of the four-flux theory; the well-

72

3 How Spectra Depend on the Scattering and Absorption of Light

known Kubelka-Munk theory, a special case of the two-flux theory; and the Lambert (Lambert-Bouguer) law, a special case of the one-flux theory. Lambert's law and the Kubelka-Munk theory long ago became accepted throughout the pigment and dye world; the four-flux theory, in contrast, has been a presence chiefly in the literature. Nonetheless, it seems important to us to deal with this theory in more depth, since it contains possibilities that have as yet been utilized little or not at all. It includes, for example, the cases in which radiation (either directional or diffuse) is incident on both sides of the layer. Such configurations are encountered everywhere and are also of technical interest (e. g., lamp enclosures that are viewed in both reflected and transmitted light). A further advantage is that the four-flux theory makes it exceedingly easy to handle special cases, not just the two named above (Kubelka-Munk theory, Lambert's law) but also the extreme cases of ªabsorption onlyº and ªscattering onlyº, as well as the limiting cases of a black background and of an opaque (ªoptically infinitely thickº) layer. In the four-flux theory, scattering and absorption are controlled through a few material constants, the scattering and absorption coefficients. After the derivation of the theory, it will be shown how these coefficients can be exactly determined by reflection or transmission measurements.

3.1.2 Many-Flux Theory The many-flux theory is the most generalized version of the phenomenological theory. It is presented briefly here because it can aid in the better unterstanding of absorption and scattering phenomena, thus making for an easier route to the important special cases that will be treated later. The development begins with a coordinate system having position coordinate z and using specified, fixed polar angles y to describe the angular distribution of the radiation. By virtue of the spherical symmetry of the problem, two coordinates will be enough. This coordinate system is illustrated in Figure 3-1. Space is subdivided into conical segments, each labeled with the polar angle y; these bound regions of space shaped like ice-cream cones, each called a ªchannelº. In this way, all light traveling in direction y1 (in the positive z direction perpendicular to the plane bounding the layer) is in channel 1; light between y1 and y2 is in channel 2; and so forth. It is useful to select an even number n of channels so that the channels in the positive and negative z directions will be symmetrical. The radiative transfer problem is described by a differential equation that takes away from each channel the radiances that it emits into all other channels and adds to it the radiances that it receives from all other channels. If there are n channels, dLi s i1 L1 dz + si2 L2 dz ¼ + s in Ln dz

n P j1

s ij Lj dz

(3.1)

73

3.1 Introduction

Fig. 3-1. Many-Flux theory: Subdivision of directions in space into n = 22 channels.

where Li is the radiance in channel i, sij is the scattering coefficient from channel j into channel i, and dz is the path element in which the change described by equation (3.1) takes place. If j = i, the coefficient sjj is the total scattering from channel j into all other channels, including the absorption contribution kj in channel j: s jj = ± kj ±

n P i1

(1 ± dij) s ij (i = 1, 2, ¼ n)

(3.2)

where dij is the Kronecker delta (d = 1 for i = j, d = 0 otherwise). It also has to be considered that the contribution sij is negative if i 4 n/2, since the radiation is traveling opposite to the positive z direction. This situation can be handled by introducing a factor Zi = (n ± 2 i + 1)/ | (n ± 2 i + 1) | , which becomes ±1 for this case but is 1 otherwise. Now equation (3.2) can be rewritten as n dLi X Zi sij Lj dz j1

(i = 1, 2, ¼ n)

(3.3)

The coefficients Zisij = Sij form a matrix S = Sij, while the radiances Li make up a vector L = {L1, L2, ¼, Ln}, so that the fundamental vector differential equation can be written as dL SL dz

(3.4)

The general solution for L can be found in mathematics textbooks: Li

n P j1

Aij Cj elj z

(i = 1, 2, ¼ n)

(3.5)

74

3 How Spectra Depend on the Scattering and Absorption of Light

where the lj are the eigenvalues of the matrix S, the Aij are the eigenvectors Aj = {A1j, A2j, ¼, Anj} corresponding to the lj , and the Cj are constants of integration determined by the boundary conditions. The eigenvalues lk can also be obtained in a well-known way by solving the ªcharacteristic equationº (see also Section 2.4.2): n P j1

sij Ajk ± lk Aik = 0 (i = 1, 2, ¼ n)

(3.6)

This equation can be solved only with powerful computers, since simultaneous differential equations with i = 1, 2, ¼, n have to be integrated. So that the Li can be stated as functions of z, finally, and thus the reflectance R or the transmitance t obtained, the constants of integration Cj must still be eliminated. These may be governed by a great variety of boundary conditions. Conditions of special practical interest are those of the substrates beneath the layer, which have their own reflectance R0, or the change in radiance at the boundary of the layer, which is caused by the discontinuity in refractive index at the surface. These cases will be treated in depth further on, in connection with special phenomenological theories. It remains now to determine the scattering and absorption coefficients sij in this system. Equation (3.6) shows that they are included in the eigenvalues and eigenvectors and can be calculated from these with equation (3.5). If there are n channels, there are n2 coefficients sij ; by the symmetry of the channels in the halfspaces, sn±i+1, n±j+1 = sij for all i, j, leaving n2/2 coefficients.* With eight channels, for example, 64/2 = 32 coefficients are required, and this large number makes the many-flux theory unsuitable for practical use, because just as many measurements would have to be made on coatings in order to determine these coefficients. Another way to determine the coefficients is to specify the radiance distribution of the incident light in terms of appropriate functions of the polar angle. A method has been described in which the radiation distribution is represented by Legendre polynomials, but it remains limited to citations in the literature. Software is available to aid in calculations under the many-flux theory by numerically integrating differential equations (ªimplicitº solution). One difficulty arises in that initial values must be provided for the scattering and absorption coefficients. Of course, the coefficients from Mie calculations (see Chapter 5) could be used, although obtaining them is an intricate and laborious process, but convenient approximate formulas do exist. In summary, the theoretical value of the many-flux theory is great but its practical significance is virtually nil. We employ it here as a basis for understanding some portions of the phenomenological theory that are used in practice and thus serve as principles underlying the results obtained in this book. In particular, we will treat special four-flux, two-flux, and one-flux theories derived directly from the model or else through mathematical integration of the differential equations (ªexplicitº solution). We begin with surface phenomena. * These include n/2 distinct sjj, each of which contains one absorption coefficient.

3.1 Introduction

75

3.1.3 Surface Phenomena In order to determine the absorption and scattering coefficients from the phenomenological theory, it is necessary to use the reflectances prevailing in the interior of the layer under study. They can differ greatly from the reflectances measured at the surface, because of the discontinuity in refractive index that is usually present between air and medium.* When light enters the layer a part of it is reflected. This reflected portion (ca. 4 %) cannot take any further part in scattering phenomena occurring inside the layer, but just the same it can enter the measuring aperture of the colorimeter, thus contributing to the reflectance. An even stronger effect takes place inside the layer: much of the light scattered back from the interior is reflected into the interior again before exiting the layer, thus becoming involved in new scattering processes. The light reflected into the interior of the layer consists in part of totally reflected light, so that this fraction is large (ca. 60 %). This interaction is repeated, and in the end the net radiation leaving the layer governs the reflectance measured at the surface. In view of the relationships, measured reflectances must be ªsurface-correctedº before these values are put into the equations of the phenomenological theory. In other words, the external measured reflectance or reflection factor is converted to the corresponding internal quantities, which can then be subjected to phenomenological analysis. We then speak of ªcorrectedº reflectances or reflection factors; the formulas used have come to be known as the Saunderson correction. One of these formulas will now be derived. The formulas contain, along with the already known reflection coefficient r0 at the interface, two other coefficients. Accordingly, three constants figure in the derivation: r0 : reflection coefficient at the surface for directional light incident perpendicularly from outside r1 : reflection coefficient for light incident diffusely from outside r2 : reflection coefficient for light incident on the surface diffusely from inside the specimen These three coefficients can be calculated with Fresnel's equations (Table 3-1), provided the diffuse light is ideally diffuse, that is, obeys the Lambert cosine distribution. We impose the following condition in order to derive the formula: The layer must be opaque, ªinfinitely thickº as specialists say; furthermore, the light must be ideally diffuse before exiting from the surface, that is, its radiance must not depend on the angle. Naturally, all quantities are generally functions of wavelength. We begin by considering a high-gloss specimen and a 0/d measuring geometry (08 incidence angle, diffuse observation) of the photometer. The radiance of the in* For media in practical use (lacquers, paints, plastics), n & 1.5 is a good approximation to the refractive index.

76

3 How Spectra Depend on the Scattering and Absorption of Light

Table 3-1. Fresnel reflection ocefficients for light of directional and diffuse incidence. Refractive index n

Directional incidence: r0

Ideally diffuse incidence External reflection: Internal reflection: r1 r2

1.40 1.41 1.42 1.43 1.44 1.45 1.46 1.47 1.48 1.49 ? 1.50

0.02778 0.02894 0.03012 0.03131 0.03252 0.03373 0.03497 0.03621 0.03746 0.03873 0.04000

0.0769 0.0784 0.0800 0.0815 0.0830 0.0845 0.0860 0.0875 0.0890 0.0904 0.0919

0.528 0.536 0.543 0.550 0.557 0.564 0.571 0.577 0.584 0.590 0.596

1.51 1.52 1.53 1.54 1.55 1.56 1.57 1.58 1.59 1.60

0.04129 0.04258 0.04389 0.04520 0.04652 0.04785 0.04919 0.05054 0.05189 0.05325

0.0934 0.0948 0.0963 0.0977 0.0992 0.1006 0.1020 0.1035 0.1049 0.1063

0.602 0.608 0.614 0.619 0.624 0.630 0.635 0.640 0.645 0.650

cident light is denoted by L+0 , the internal reflectance by R . Then from Figure 3-2 we have immediately: + L++ 0 L0 (1 ± r0)

L±0

L+0 7 r0

L±1

L=1 (1 ± r2) L+0 (1 ± r0) (1 ± r2) R

L±2 .. .

L+0 (1 ± r0) (1 ± r2) R (r2 R )

+ L=1 L++ 0 7 R L0 (1 - r0) R

L+1 L=1 7 r2 L+0 (1 ± r0) R r2 L=2 L+1 7 R* L+0 (1 ± r0) R r2 R L+2 L=2 7 r2 L+0 (1 ± r0) R r22 R

L±n

L+0 (1 ± r0) (1 ± r2) R (r2 R )n±1 ? P 1 r0 1 r2 R ± + Li L0 r0 1 r2 R i0

3.1 Introduction

77

Fig. 3-2. Surface phenomena: The available radiances outside and inside the layer.

The radiance received by the instrument is the sum of all outward radiances L±i (written at right). The summation is done with the formula for an infinite geometric progression with first term (1 ± r0) (1 ± r2) R and r2 R as common ratio.* The externally measured reflectance R is the ratio between the radiation exiting and the radiation incident, that is (SL±i ) / L+0 : R r0

1

r0 1 r2 R 1 1 r2 R

r2 R r0 r2 R

r0 1

(3.7)

For practical application, this equation is mostly written for R*: R

R 1

r0 1

r0 r2 r2 R

r0

R 1

r0

r0 r2 1

R

(3.8)

The expressions on the right-hand sides are alternative forms. For the ideal white standard with a totally matte surface, R = 1, and so equation (3.7) implies that R is also equal to 1. This means that the correction formulas stated above apply in the same form to matte and glossy specimens. Now let us consider the measuring geometry d/0 (diffuse incidence, 08 observation). By similar arguments, the reflection factor R can be written as R a r0

1

r0 1 r1 R n2 1 r2 R

(3.9)

* More precisely, the reflectance Rg for L=1 would have to be for directional incidence while the reflectances Rdif for all subsequent Li would have to be for diffuse incidence. The slight difference between the two values is definitely of higher order in the context of this correction formula, so that for present puposes we can set Rg = Rdif = R .

78

3 How Spectra Depend on the Scattering and Absorption of Light

The fraction on the right-hand side differs from the one in equation (3.7) by a factor of n2 (1 ± r2) / (1 ± r1), which is equal to 1 for all refractive indices, as can easily be seen by examining Table 3-1. The term ar0 means that it is possible to design the instrument in such a way that the surface-reflection contribution is included (a = 1) or suppressed (a = 0). In the first case, equation (3.9) becomes equation (3.7); in other words, equations (3.7) and (3.8) also hold for the 0/d and d/0 measuring geometries. It can also be shown that the corresponding formulas for the 45/0 geometry are not much different from the ones already stated. This means that the correction formulas written out can be applied universally. For refractive index n = 1.5, Table 3-1 gives r0 = 0.04 and r2 = 0.6. Then the correction formulas become

R 0:04 R

0:384 R 0:36 R 0:04 1 0:6 R 1 0:6 R

R 0:04 R 0:04 0:384 0:6 R 0:04 0:96 0:6 1

(3.10) R

R 0:04 0:36 0:6 R

(3.11)

The R in equation (3.11) must be replaced by R + 0.04 when the measurement is performed with gloss trap (specular exclusion). These formulas have been used in practice for many years.

3.2

Four-Flux Theory

3.2.1 The Differential Equations and Their Integration The ªexplicitº solution of the four-flux theory to be discussed now is based on the model of Figure 3-3. An absorbing and scattering layer of thickness h is traversed by four radiances,* identified by arrow symbols and corresponding to the four channels: ± ± ± ±

Directional incident light: l + Directional light opposite to direction of incidence: l ± Diffuse incident light: L+ Diffuse light opposite to direction of incidence: L±

* The terminology and notation used in this chapter are based on those of DIN 1349; departures have been made whenever there is a possibility of confusion with quantities already defined.

3.2 Four-Flux Theory

79

Fig. 3-3. Four-Flux theory: The radiances, directional (l +, l ±) and diffuse (L+, L±), together with the boundary conditions.

Let z be the position coordinate in the direction of propagation. We now want to know the amount by which the individual radiances decrease or increase as the light traverses the short distance dz. As in the differential statement of Lambert's law, ±k'l + dz is taken away from l + by absorption (here k' is the absorption coefficient for directional light). If scattering is present, l + also loses ±s+l + dz scattered forward and ±s± l + dz scattered backward (s+ and s± are the forward and backward scattering coefficients for directional light). Thus we can write dl + ± (k' + s+ + s± ) l + dz

(3.12)

In distinction to the absorbed fraction, however, the two scattered components do not disappear without trace; they must later be added into the respective radiances for diffuse light. Similarly, in the case of directional light propagating in the opposite direction, we can write for l ± ± dl ± ± (k' + s+ + s ± ) l ± dz

(3.13)

The minus sign on dl ± takes care of the fact that l ± is in the direction opposite to the positive z direction. We now consider the radiance L+ of diffuse light. First, similarly to l +, it loses the absorbed component ±KL+ dz and the scattered component ±SL+ dz (where K is the absorption coefficient and S the scattering coefficient for diffuse light). Further, however, the light scattered from the l + and l ± beams must now be added to L+; these are s+l +dz and s± l ± dz respectively. Finally, the scattering SL±dz from the opposite diffuse light must be added as well, so that dL+ s+ l + dz + s ± l ± dz ± (K + S) L+ dz + SL ± dz

(3.14)

±dL ± s ± l + dz + s+ l ± dz ± (K + S) L ± dz + SL+ dz

(3.15)

and similarly

The coefficients and their definitions are written out once again: k0

1 dl l dz

abs

;

s

1 dl l dz

sca ; forw

s

1 dl l dz

sca back

(3.16)

80

3 How Spectra Depend on the Scattering and Absorption of Light

K

1 dL L dz

abs

;

S

1 dL L dz

sca

(3.17)

By the rule stated at the end of Section 3.1.2, the four-flux theory would require 42/2 = 8 coefficients, of which 4/2 = 2 contain absorption coefficients. The reduction of the remaining six scattering coefficients to three comes about because, in three cases, there is no radiative transfer by scattering: from l + to l ± from L+ to l ± from L± to l +. The associated scattering coefficients are therefore equal to zero. The following abbreviations are now introduced into the equations: a1

K S

(auxiliary variable)

m k' + s+ + s ± (attenuation coefficient)

(3.18)

(3.19)

The system of differential equations then becomes dl dz

m l

dl ml dz

(3.20) (3.21)

dL s+ l + + s ± l ± ± aSL+ + SL ± dz

(3.22)

dL ±s ± l + ± s+ l ± + aSL ± ± SL+ dz

(3.23)

This coupled system of four simultaneous differential equations for the functions l + (z), l ± (z), L+ (z), and L± (z) must now be decoupled and integrated. It will be sufficient to integrate out to the boundary conditions. Thus the integrals of the first two equations can be written immediately. With l + (0) l0+ ;

l ± (h) lh±

(3.24)

l ± lh± e±m (h±z)

(3.25)

we get l + l0+ e±mz ;

3.2 Four-Flux Theory

81

The film thickness h then becomes l + (h) lh+ l0+ e±mh ;

l ± (0) = l0± lh± e±mh

(3.26)

The first two differential equations have now been decoupled and integrated by themselves. These solutions are needed for the integration of the last two equations (3.22) and (3.23). In order to decouple the remaining simultaneous system, one of the two equations must be differentiated; we choose equation (3.22). The derivatives of the directional radiances l + and l ± are replaced by expressions (3.20) and (3.21); dL+/dz and dL±/dz, by espressions (3.22) and (3.23). Using the partial integrals in equation (3.26) along with b

p a2 1 (auxiliary variable)

(3.27)

we obtain finally d2 L b2 S2 L+ ± l0+ [Ss ± + (m + a S) s+ ] e±mz ± dz2 ± lh± [Ss+ ± (m ± aS) s ± ] e±m (h±z)

(3.28)

The homogeneous equation associated with this second-order differential equation has the well-known exponential solution with two constants of integration. For the inhomogeneous equation, two terms with the exponents ±mz and ±m (h ± z) must be considered, so that the solution becomes L+ B1 ebSz + B2 e±bSz ± l+0 p e±mz ± lh± q e±m (h±z)

(3.29)

Here B1 and B2 are the two constants of integration of the second-order differential equation; the boundary conditions will be applied later in order to eliminate these. On the other hand, p and q are fixed in value and can therefore be found immediately by comparing coefficients with differential equation (3.28). For this purpose, expression (3.29) is substituted in (3.28), an the other hand, equation (3.29) is differentiated twice. The comparison of coefficients then gives

p q

Ss m aS s K k0 s s s S s m2 b2 S2 k0 s s 2 K K 2 S Ss

m m2

aS s K k0 s s s S s b2 S2 k0 s s 2 K K 2 S

Accordingly, equation (3.29) is already the general integral.

(3.30) (3.31)

82

3 How Spectra Depend on the Scattering and Absorption of Light

The next step is to impose the boundary conditions on the general integral and its first derivative. The boundary conditions themselves are obtained from the cases z = 0 and z = h for L+ and dL+ / dz; the starting differential equation (3.22) is employed for the latter. We then have L+ (0) B1 + B2 ± l+0 p ± lh± q e±mh L+0

(3.32)

L+ (h) B1 ebSh + B2 e±bSh ± l0+ p e±mh ± lh± q L+h

(3.33)

dL dz

z=0

B1 bS ± B2 bS + l0+ mp ± lh± mq e±mh s+ l0+ + s ± l0± ± aSL0+ + SL0±

dL dz

z=h

(3.34)

B1 bS ebSh ± B2 bS e±bSh + l0+ mp e±mh ± lh± mq + ± ± ± s+ l+ h + s lh ± aSLh + SLh

(3.35)

We recall that l0+, lh±, L+0 , and L±h are given (as incident radiances; see Fig. 3-3). The equation system (3.32)±(3.35) thus contains four further unknowns, B1, B2, L+ h , and ± and L L±0 , which can now be determined from the four equations. Only L+ h 0, the quantities sought, are of interest here. The solutions are L+h l0+ P + lh± Q + L0+

b sinh x + Lh± A A

(3.36)

L0± l0+ Q + lh± P + L0+

sinh x b + Lh± A A

(3.37)

where we have introduced the notation* x bSh ; A a sinh x + b cosh x P

(3.38)

1 (bp + q e±mh sinh x) ± p e±mh A

(3.39)

1 ( p sinh x + bq e±mh) ± q A

(3.40)

Q

* P and Q, unlike p and q, are not constants of the material, since they depend on the film thickness h.

3.2 Four-Flux Theory

83

Equations (3.36) and (3.37) together with (3.26) give the radiances for a layer irradiated from both sides. Interchanging l0+ with lh± and L+0 with L±h takes each equation into the other. This is a necessary condition, because the experimental radiances L+h and L±0 as well as lh+ and l0± must be invariant to reversal of the sides of the layer.

3.2.2 Transmittance and Transmission Factor The most general configuration that can be imagined for the measurement of transmission is described by the following model: ªMixedº irradiation (i. e., directional and diffuse radiation) on the incidence side, observation of total radiation (i. e., directional and diffuse once again) on the observation side. The corresponding formula for the transmittance in the interior of the layer* is as follows (see Fig. 3-3): t

lh L h l0 L 0

(3.41)

If diffuse light is not recorded on the measurement side, L+h vanishes and t is replaced by the transmission factor T. In the most general model, the following equation is obtained by merging (3.26) and (3.36) and the fact that no light is incident on the specimen from the observation side (i. e., lh± = L±h = 0): t (1 ± g) (P + e±mh) + g

b A

(3.42)

where g = L+0 /(l0+ + L+0 ) is the diffuse fraction and 1 ± g = l0+ /(l0+ + L+0 ) the directional fraction of the net incident light. This equation immediately yields the case of irradiation with directional (quasiparallel) light if g is set equal to 0: tg P + e ±mh

(3.43)

This is identical to the equation stated by Ryde if we set k' = 0, for Ryde did not introduce a second absorption coefficient. In the same way, for irradiation with diffuse light (g = 1), tdif

b b A a sinh x b cosh x

(3.44)

* In general, t* = t / t0 (where t0 is the blank value). If there is much scattering in the layer, however, it may become necessary to apply the Saunderson corrections, equation (3.11), writing t in place of R.

84

3 How Spectra Depend on the Scattering and Absorption of Light

This is the transmittance in the Kubelka-Munk theory. The same equation is also obtained, incidentally, if the substitutions s+ = 0, s± = S, and k' = K are made in equation (3.43). This would mean that, as far as scattering and absorption in the interior of the medium are concerned, there is no difference between directional and diffuse radiation: The substitutions lead to p = 1 and q = 0 from equations (3.30) and (3.31), so that equation (3.43) actually does become (3.44). In reality, however, s± cannot be identical to S nor k' with K since the mean path length through the layer for diffuse light is longer than the film thickness. As a consequence, more light is scattered and absorbed than from a directional beam perpendicular to the layer, and this fact must affect the numerical values of the scattering and absorption coefficients. The mean path length of ideally diffuse radiation through a layer is, according to Kubelka, twice the film thickness (corresponding to a incidence angle of 608); hence S and K are about twice as large as s± and k' respectively. Two other configurations of measuring geometries are possible and must be considered. On the irradiation side, suppose that incidence is solely directional and perpendicular to the layer surface, while on the observation side only the quasi-perpendicular directional radiation component is measured. Then what is measured is the transmission factor T*r , which is given directly by equation (3.26): Tr

lh e l0

mh

(3.45)

The second possibility is the transmittance t g , which is obtained if irradiation is directional and the directly transmitted beam lh+ is excluded, so that only the remaining diffuse light is measured. The formula for this case is t g tg

Tr P

(3.46)

All the important transmittance equations for the four-flux theory have now been derived. We need only add the equations obtained by examining the two important extreme cases ± Absorption only (no scattering) ± Scattering only (no absorption) For the ªabsorption onlyº case, we have k', K 4 s+, s±, S; a ? b ? K/S ? ?; m ? k'; and p ? q ? 0. The general tansmittance is then tabs 1

g e

k0 h

ge

Kh

(3.47)

while the transmittance and transmission factor for directional irradiation are given by e tabs;g Tabs;r

k0 h

(3.48)

3.2 Four-Flux Theory

85

and the transmittance for diffuse irradiation by tabs;dif e

Kh

(3.49)

Since there is no incident diffuse light in the case of directional irradiation, the transmittance after exclusion of directional radiation on the measurement side is, as = 0. expected, t abs;g = tabs;g Tabs;r Equation (3.48) is the well-known transmission factor from Lambert's law. In the second extreme case, ªscattering onlyº, s+, s±, S 4 k', K; therefore a ? 1, b ? 0, m ? u = s+ + s±. For p and q, we obtain p ? u = (S + s+)/(s+ + s±) and q ? w = (S ± s±)/(s+ + s±), with u ± w = 1. Taking the limit gives the following for the general transmittance: tsca 1

g

1 w 1 e 1 Sh

uh

1 1 Sh

g

(3.50)

whence, for directional irradiation, tsca;g

1 w 1 e 1 Sh

uh

(3.51)

for diffuse irradiation, tsca;dif

1 1 Sh

(3.52)

while the transmission factor is given by e Tsca;r

uh

(3.53)

and the transmittance after exclusion of directional radiation by t sca;g tsca;g

Tsca;r

1 w 1 e 1 Sh

uh

e

uh

(3.54)

The following auxiliary variables have been used here: u s s ;

w

S s s s

(3.55)

All the equations derived in Section 3.2.2 are summarized and related to one another by the transmission function pedigree of Figure 3-4.

86

3 How Spectra Depend on the Scattering and Absorption of Light

Fig. 3-4. Pedigree of the transmission function.

3.2.3 Reflectance and Reflection Factor As Figure 3-3 shows, the reflectance in the interior of the layer for irradiation with both types of light is given by R

l0 L0 l0 L 0

(3.56)

In the model that serves as basis for the present discussion, the absorbing and scattering layer is applied directly on a substrate. This kind of model is of greatest importance in practice, since it describes lacquer and paint coatings. Because the substrate generally has its own reflection properties, these must be taken into account when the equations of Section 3.2.1 are employed. The intrinsic reflection of the substrate will, in general, give rise to diffusely reflected light, although specularly reflecting substrates are increasingly significant (e. g., for transparent lacquers). For the specular case, the radiance reflected from the substrate is (see Fig. 3-5). lh Rr;0 lh Rr;0 l0 e

mh

(3.57)

3.2 Four-Flux Theory

87

Fig. 3-5. Reflection with substrate.

Here Rr,0 is the reflection factor of the specular substrate; the subscript r identifies the 0/0 geometry (i. e., the angles of incidence and reflection are both 08), while the * identifies the reflection factor as an internal one. If there is no specular reflection, however, only diffuse radiation comes from the substrate; it consists of two components, the first Rg,0 7 l +h originating in directional irradiation and the 7 L +h in diffuse irradiation (here Rg,0 and Rdif,0 are the reflectances of second Rdif,0 the substrate for directional and diffuse irradiation, respectively; see Fig. 3-5). The definition of reflectance in equation (3.56) requires that all the radiation ± directional and diffuse ± must be received on the observation side. The same holds, of course, for the reflectance of the substrate. Accordingly, if specular reflection is present along with diffuse reflection, it must be recalled that the specular reflection has already been taken care of by equation (3.57), so that Rr,0 7 lh+ must be subtracted, else it will be counted twice. The radiance diffusely reflected by the substrate is then Lh± (Rg,0 ± Rr,0) l+h + Rdif,0 L+h

(3.58)

From this with equations (3.26) and (3.36), we obtain an expression containing L±h twice; solution for L±h yields Lh

A A

l0

Rdif ;0 Rg;0

sin x Rr;0 e mh

Rdif ;0 P

Rr;0 Q e mh

L 0

Rdif ;0

b A

(3.59)

Now, with the aid of equation (3.56) and the use of equations (3.26), (3.37), and (3.59), we immediately obtain the reflectance for the general model (parallel and diffuse irradiation):

88

3 How Spectra Depend on the Scattering and Absorption of Light

R

1 g AQ R R R A Rdif ;0 sinh x " # 2 sinh x b g Rdif ;0 A A Rdif ;0 sinh x A

(3.60)

In this expression we have used the notation R Rr;0 e

mh

R Rg;0 b e

A P e

mh

mh

Rdif ;0 bP

R Rr;0 Rdif ;0 e

mh

bQ

b

(3.61)

Q sinh x P e

mh

(3.62)

sinh x

(3.63)

Hence, with g = 0, we have the following for irradiation with directional light: Rg

AQ R R R A Rdif ;0 sinh x

(3.64)

Taking g = 1 leads to the reflectance for irradiation with diffuse light; this equation can be transformed with the easily derived relation sinh2 x ± b2 = A (a sinh x ± b cosh x). Since cosh x/sinh x = coth x, Rdif

1

Rdif ;0 a b coth x a Rdif ;0 b coth x

(3.65)

This is the reflectance in the Kubelka-Munk theory, which we will use frequently. Wholly similarly to the transmission factor Tr , a reflection factor Rr applicable to directionally reflected light can be defined. This is nonzero only when Rr,0 = 0, that is, when there is a specularly reflecting substrate: Rr

l0 Rr;0 e l0

2mh

(3.66)

With a measuring setup that can exclude directional reflected light, a reflectance R g = Rg ± R r can be obtained similarly to the transmittance: R g

A

1 Rdif ;0 sinh x

AQ R

Rr;0 A e

2mh

R R Rr;0 Rdif ;0 e

2mh

sinh x

(3.67)

89

3.2 Four-Flux Theory

As in Section 3.2.2, there are two extreme cases. Let us first consider ªabsorption onlyº. Taking the limit yields the following for the general reflectance: Rabs (1± g) [Rr,0 e±2k'h + (Rg,0 ± Rr,0) e±(k'+K)h] + gRdif,0 e±2Kh

(3.68)

for directional irradiation, Rabs,g Rr,0 e±2k'h + (Rg,0 ± Rr,0) e±(k'+K)h

(3.69)

for diffuse irradiation Rabs,dif Rdif,0 e±2Kh

(3.70)

With an appropriate measuring setup, we can again split into the reflection factor Rabs,r Rr,0 e±2k'h

(3.71)

and the reflectance after exclusion of directional radiation R abs,g (Rg,0 ± Rr,0) e±(2k'+K)h

(3.72)

Taking the limit for the second extreme case, ªscattering onlyº, leads to the general reflectance Rsca

1

g

Qsca 1 Sh R sca R sca R sca

1

Rdif ;0 Sh

g

1 Rdif ;0 Sh Rdif ;0 1 Rdif ;0 Sh 1

1

(3.73)

where the barred expressions are somewhat simplified: R sca Rr,0 e±uh [(1 + Sh) (Psca + e±uh) ± 1]

(3.74)

R sca Rg,0 e±uh + Rdif,0 (Psca ± Qsca Sh)

(3.75)

R sca Rr,0 Rdif,0 e±uh [Qsca ± (Psca + e±uh) Sh]

(3.76)

and Psca

1 [(1 + w) (1 ± e±uh) ± Sh e±uh] 1 Sh

(3.77)

Qsca

1 [Sh ± w (1 ± e-uh)] 1 Sh

(3.78)

The symbols u and w have the same meanings as in equation (3.55).

90

3 How Spectra Depend on the Scattering and Absorption of Light

From the above, we immediately get the expressions for directional light Rsca;g

1

1 Qsca 1 Sh R sca R sca R sca Rdif ;0 Sh 1

and for diffuse light Rsca;dif

1 Rdif ;0 Sh Rdif ;0 1 Rdif ;0 Sh 1

(3.79)

(3.80)

as well as for the reflection factor Rsca;r Rr;0 e

2uh

(3.81)

and the reflectance after exclusion of the directional component: R sca;g

1 Rdif ;0 Sh

1

Rr;0 e

2uh

1

Qsca 1 Sh R sca R sca R sca

1 1

Rdif ;0 Sh

(3.82)

3.2.4 Limiting Cases of Reflection The following limiting cases are of practical interest: ± ± ± ±

The substrate exhibits specular reflection only The substrate exhibits diffuse reflection only The substrate is black The layer is opaque (ªinfinitely thickº)

1) Substrate with exclusively specular reflection The equations for this limiting case are obtained by setting the reflectances and reflection factors of the substrate in equation (3.64) equal (i. e. Rg,0 = Rdif,0 = Rr,0); the equation for directional irradiation is then Rspr;g

1 A

Rr;0

bP

sinh x

hAQ Rr;0 fA e

Q sinh x Rr;0 e

mh

bQ

mh

P e

P e

mh

mh

sinh xgi

(3.83)

For diffuse irradiation, equation (3.65) remains unchanged except that Rr,0 appears in place of Rdif,0. The reflection factor of equation (3.66) does not change either. For the reflectance after exclusion of directional reflected light, we then have

91

3.2 Four-Flux Theory

R spr;g

1 Rr;0

A

Rr;0 e

sinh x mh

bQ

fAQ Rr;0 P A e

mh

b

Q sinh x

P sinh xg

(3.84)

The equations for the two extreme cases, ªabsorption onlyº and ªscattering onlyº, will not be written out here, because they can be obtained effortlessly from equations (3.68) to (3.82) by setting Rg,0 = Rdif,0 = Rr,0. 2) Substrate with exclusively diffuse reflection These equations are derived by setting Rr,0 equal to zero in the respective formulas. First, again, the case of directional irradiation: Rdfr;g

A

1 AQ Rg;0 b e Rdif ;0 sinh x

Qb

mh

Rdif ;0 bP

Rg;0 e mh Rdif ;0 P A Rdif ;0 sinh x

Q sinh x (3.85)

Here too, the case of diffuse irradiation contains nothing not considered in equation (3.65), since that formula does not show Rr,0 at all. Because no directional light can be excluded, the reflectance has the trivial solution Rdif,r = 0, and R dif,g is as in equation (3.85). Once more, the equations for the extreme cases are omitted, being easily derivable from the respective formulas with Rr,0 . 3) Black substrate Now all the reflectances and reflection factors of the substrate are zero. From equation (3.64) with Rr,0 = Rg,0 = Rdif,0 = R = R = R = 0, we have the following; for directional irradiation Rg;b Q

(3.86)

(this is the reflectance in the Ryde theory if k' = 0), and for diffuse irradiation Rdif ;b

1 a b coth x

(3.87)

Again Rr,b = 0, so that the expression for R g,b is the same as equation (3.86). As in the previous derivations, the extreme cases are uninteresting up to ªscattering onlyº. For directional irradiation we have

92

3 How Spectra Depend on the Scattering and Absorption of Light

Rb=sca;g Qsca

1 Sh 1 Sh

and for diffuse irradiation Rb=sca;dif

w 1

Sh 1 Sh

e

uh

(3.88)

(3.89)

4) Infinitely thick layer These important equations are obtained by taking the limit as h ? ?, so that equation (3.86) leads to the following for directional irradiation: Rg;? p a

b

q

(3.90)

Fig. 3-6. Pedigree of the reflection function.

3.2 Four-Flux Theory

93

and equation (3.87), with a2 ± b2 = 1, gives for diffuse irradiation Rdif ;? a

b

(3.91)

The extreme cases yield trivial solutions. All the equations derived in Section 3.2.3 are summarized and related to one another by the reflection function pedigree of Figure 3-6.

3.2.5 Determination of the Coefficients Practical use of the formulas stated in the preceding sections requires that the absorption coefficients k', K and scattering, coefficients S, s+, s± appearing in them be determinable by reflection or transmission measurements. The problem is easy to solve, because that determination can be carried out in two steps. The measurements, labeled with ªdifº contain only the coefficients K and S; these are the typical optical parameters of the Kubelka-Munk theory, to be described in the next section along with methods for their determination. Thus K and S must always be determined first, since these coefficients are assumed known when k', s+, and s± are determined. Accordingly, three coefficients remain to be found, so that three equations have to be employed. The following measurements (all for directional irradiation) are available for the purpose: ± Rr , the reflection factor for (quasi) 0/0 geometry with a specularly reflecting substrate having reflection factor Rr,0 ± Rg,? , the reflectance of the infinitely thick layer ± Rg,b , the reflectance over a black substrate ± Rg,w, the reflectance over a white substrate having reflectance Rg,0w ± Tr, the transmission factor measured with (quasi) 0/0 geometry ± tg , the transmittance Any three of these measurable quantities can be used in determining k', s+, and s±. We will distinguish between determinations based on reflection measurements and those based on transmission measurements. The equations needed are derived from the formulas of Sections 3.2.2 and 3.2.3. All the quantities from the Kubelka-Munk theory can ± because they are (abbreviated terms on the right hand side) known ± be substituted in these formulas. They are tdif Rdif ;1

b t A a b R1

Rdif ;b

sinh x R2 A

(3.92) (3.93) (3.94)

94

3 How Spectra Depend on the Scattering and Absorption of Light

Rdif ;0w R3

(3.95)

These values can either be obtained by direct measurement on black and white drawdowns or calculated from K and S (which are assumed to be known) and h. The notation and relations stated previously are used: K S s p K K 2 1 b a 2 S S x bSh

a 1

A a sinh x b cosh x Special value is attached to the measurement of the film thickness h, which must be done with great care because the error in h strongly influences the accuracy of the calculated absorption and scattering coefficients. It is also vital that the layers on the black and white substrates be equally thick; this can be achieved with black and white glass plates in which the white and black portions are joined together without a ªstepº. The reflection factor Rr , on the other hand, can be measured on a drawdown having a different film thickness hR on the specularly reflecting substrate. 1 Determination of k ', s+, and s± from reflection measurements 1.1 From Rr , Rg,?, Rg,b (and Rr,0) By equations (3.45) and (3.66), Tr

e

mh

Rr Rr;0

!

h 2hR

T

(3.96)

where hR is the film thickness over the specular reflective substrate; also, by equations (3.86) and (3.90) Rg;1 1 p R1 1 q R1 p

tT tT

Rg;b R2

Rg;1

(3.97)

The auxiliary variables p and q are linked to the coefficients by equations (3.30) and (3.31). If these are solved for s+ and s±, the following formulas are obtained: s p m aS qS s pS q m aS

(3.98) (3.99)

95

3.2 Four-Flux Theory

The quantity m needed here follows immediately from equation (3.96): m so that by equation (3.19)

1 1 ln h T

(3.100)

k' m ± (s+ + s ± )

(3.101)

The three coefficients have thus been determined. 1.2 From Rr , Rg,b , Rg,w (and Rg,0w): If Rg,? is difficult of access because of problems in achieving a thick layer, a determination based on a layer over black and white is also possible. The equation for Rg,b is now supplemented by equation (3.85) for Rg,w , specifically the expression following the second equality sign; then, with Q = Rg,b , p and q are obtained as follows from equation (3.86): p

R2 TRg;b C 1

R22 T t

T 1

tT tT

;

q

p R2 Rg;b 1 tT

(3.102)

with T as above. Here 1 C R3

1 R t g;w

Rg;b 1

R2 R3

Rg;0w T

(3.103)

With m as defined previously and the formalism of 1.1, we finally obtain k', s+, and s±. 1.3 From Rg,?, Rg,b , Rg,w (and Rg,0w) This variant does not involve a drawdown on a specularly reflecting substrate. The formulas used are again equations (3.86), (3.90), and (3.85), the expression after the first equality sign in equation (3.85) being taken. The term bP ± Q sinh x is transformed, and then q is substituted with Rg,? from equation (3.90). Solving for p leads to an expression that has the same denominator as the formula for p in equation (3.97). By setting the two expressions equal, we obtain directly a formula for T containing no quadratic expressions: T

R1 Rg;w

Rg;b R2 R3 Rg;1 Rg;w R3 Rg;1 t R1 Rg;0w R3 Rg;1

Rg;b

(3.104)

The subsequent analysis is most easily done with equations (3.97) to (3.101).

96

3 How Spectra Depend on the Scattering and Absorption of Light

2 Determination of k', s+, s± from transmission measurements Initially, only T r from equation (3.45) and t g from (3.43) are available for the determination. But a third equation is needed if the three coefficients are to be obtained; this can be derived from a further transmission measurement, t^ g with a doubled film thickness h. In the case of suspensions, this involves no difficulties; we simply take a cell with twice the thickness. It is possible, however, even for pigmented coatings, provided these are plastic wafers or self-supporting films (films not applied on a substrate ± but optical contact is a special concern here, see Section 3.3.3). All quantities relating to the doubled film thickness are identified by ^ ; then b (3.105) t^ dif t^ A^ R^ dif ;b

sinh 2x R^ 2 A^

(3.106)

Where = a sinh 2 x + b cosh 2 x. Now, by equation (3.43) for t g and t^ g p

R^ 2 T tg R^ 2 T t

T T

R2 ^tg T 2 R2 ^t T 2

q

1 t R2 T g

T

p t

T

(3.107)

If p, q, and T are known, we can go on as in 1.1. We have thus shown how k', s+, and s± can be determined without an excessive degree of complication.

3.3

Kubelka-Munk Theory

3.3.1 Significance and Formalism The two-flux theory is today the most important and successful specialization of the phenomenological theory. It owes its widespread acceptance to three properties: ± It involves only two optical constants (K and S) ± It is easy to work and lends itself to computer programming ± Over a period of decades, it has proved suitable for the description of practical problems.

3.3 Kubelka-Munk Theory

97

The first two of these qualities have their source in the fact that the theory is formulated quite simply, on the basis of the following assumptions: ± Ideally diffuse radiation distribution on the irradiation side ± Ideally diffuse radiation distribution in the interior of the layer ± No consideration of surface phenomena resulting from the discontinuity in refractive index When deviations from the Kubelka-Munk theory are seen in application to practical problems, the reason is nearly always that one or more of these assumptions have been neglected*. The third assumption drops out when the Saunderson corrections are employed, as has become indispensable for most applications today. We have already encountered the basic equations of Kubelka and Munk in deriving the four-flux theory. Because they are so important, however, they are written out explicitly here, except that the subscript ªdifº has been omitted (since there is no radiation other than diffuse). Transmittance: General:

t

b a sinh b S h b cosh b S h

Absorption only:

tabs e

Scattering only:

Kh

(3.110) s. (3.52)

1 R0 a b coth bS h a R0 b coth b S h

(3.111) s. (3.65)

Reflectance: R Absorption only:

(3.109) s. (3.49)

1 1 Sh

tsca

General:

(3.108) s. (3.44)

Rabs R0 e

Scattering only: Rsca

1 1

2Kh

R0 S h R0 R0 S h 1

(3.112) s. (3.70) (3.113) s. (3.80)

The symbols here have the following meanings: K and S are the absorption and scattering coefficients defined as in equation (3.17); R0 is the reflectance of the substrate; the auxiliary variables a and b are defined as in equations (3.18) and (3.27), a = 1 + K / S and b = (a2 ± 1)1/2 ; and finally h is the film thickness. * In such cases, many-flux theories may be helpful; see also the discussion in Section 7.2.3.

98

3 How Spectra Depend on the Scattering and Absorption of Light

3.3.2 Limiting Cases of Reflection Because equations (3.111) to (3.113) also hold for substrates with specular reflection only and with diffuse reflection only, there are just two limiting cases of the reflectance to be treated here: ± Reflectance on black substrate ± Reflectance of the opaque (ªinfinitely thickº) layer To obtain the reflectance on a black substrate, we use the equations from Section 3.3.1, setting R0 equal to zero. General: Rb

1 a b coth b S h

Scattering only: Rsca;b

Sh 1Sh

(3.114) s. (3.87) (3.115) s. (3.89)

For the ªabsorption onlyº case, we get the uninteresting trivial solution Rabs,b. = 0 The easiest way to obtain the reflectance of the infinitely thick layer is to take equation (3.114) to the limit as h ? ?. Then coth bSh ? 1, and with the relation a2 ± b2 = 1 implied by equation (3.27),

R1 a

K b1 S

s K K 2 S S

(3.116) s. (3.91)

Solving for K / S, we obtain the famous ªKubelka-Munk functionº FKM : K 1 R1 2 :FKM 2 R1 S

(3.117)

(The extreme cases ªabsorption onlyº and ªscattering onlyº lead to trivial solutions: Rabs,? = 0 and Rsca,? = 1) For didactic purposes, it may well be desirable to derive the Kubelka-Munk function directly from the differential equations. The typical equations for the Kubelka-Munk theory are obtained from equations (3.22) and (3.23) by setting the directional radiances l + and l ± (Fig. 3-3) equal to zero. Dividing the first equation by SL+ and the second by SL± and using L± /L+ = R , one gets

3.3 Kubelka-Munk Theory

1 1 dL S L dz

99

K 1 R S

1 1 dL K 1 dz S L S

1 R

The ªinfinitely thickº layer is characterized by the fact that a further increase in film thickness does not change the reflectance. Thus the percent changes in radiance per unit increase of film thickness in the incidence direction (1/L 7 dL+/dz) and opposite to the incidence direction (1/L± 7 dL±/dz) must be exactly equal. If both right-hand sides are set equal and the equation is solved for K / S, the limit as R ?R? directly yields the Kubelka-Munk function (3.117). Equation (3.117) is the most important statement of the Kubelka-Munk theory and the most often used of all formulas in the theory. It links the reflectance of the infinitely thick layer with the absorption and scattering coefficients K and S governing the optical process, making R? directly dependent on the ratio of the absorption to the scattering coefficient (and not on the value of either). The equation is also available in tabular form; it has found widest use where information about the ratio of absorption to scattering is to be extracted from reflection measurements. Figure 3-7 is a plot of the Kubelka-Munk function. Typical features are the steep drop from very large values at low reflectance and the branch decreasing slowly toward zero as the reflectance approaches 1. If the variables are interchanged, the reflectance then declines rapidly from unity at low K / S; this fact accounts for the well-known high sensitivity of white specimens to contamination.

Fig. 3-7. The Kubelka-Munk function FKM (R*?).

100

3 How Spectra Depend on the Scattering and Absorption of Light

Fig. 3-8. The function ln FKM (R*?).

If the logarithm of FKM is plotted versus reflectance, the curve of Figure 3-8 results. As can be seen, there is a wide reflectance range in which the curve has a quasilinear shape. The equation for this straight line can be obtained by calculating the point of inflection and the inflectional tangent of the curve. A better approximation can be found by a linear regression calculation in the region of interest: ln F A ± BR?

or

log F A10 ± B10 R?

(3.118)

where A 1.68 ; B 6.182 ; A10 0.7296 ; and B10 2.685 for 0.13 ^ R? ^ 0.73 (i.e. 0.09 ^ Rin,? ^ 0.54).* The values of the coefficients are somewhat dependent on higher accuracy in the lower or the upper part of the range. The values stated above represent a good approximation over the entire region. Between R? = 0.20 and 0.65, the deviation from the true F value is less than 3 %, coming to exceed 20 % only at the bounds cited above. What appears to be a bothersome restriction on the use of the approximation formula is actually not much of a hindrance: the requirements on the accuracy of measurement in the determination of F already restrict the field in which the measurements must be done. Let us consider the relative error of determination of F reflection measurements:

* The subscript ªinº refers to measurement including surface reflection (see Section 6.1.2).

3.3 Kubelka-Munk Theory

d ln F dF dR dR dR F dR

1 R 1 0:6 R dR 1 R R 0:04

101

(3.119)

As Figure 3-9 shows, given a fairly realistic measurement error of dR = 0.001, the relative error of F is smaller than 1% only when measurements are performed with 0.2 ^ Rin,? ^ 0.75 (i. e., 0.33 ^ R? ^ 0.88). The measurement interval does not expand to 0.1 ^ Rin,? ^ 0.88 (i. e., 0.14 ^ R? ^ 0.95) until a 2 % error (dF / F) is allowed. Here we have a reflection counterpart to the spectroscopists' old rule, ªFor extinction measurements, the transmission must always be between 8 and 80 % (or the decadic extinction between 1 and 0.1).º

Fig. 3-9. Relative error of the Kubelka-Munk function F (Rin,?) for a measurement error dR = 0.001.

102

3 How Spectra Depend on the Scattering and Absorption of Light

3.3.3 Determination of the Absorption and Scattering Coefficients The classical method of determining the coefficients is to measure directly the reflectance R ? of the infinitely thick layer and, from this, determine, after Saunderson correction, a and b. Equations (3.116) and (3.27) imply that 1 a 2 ba

1 R1 R1 1 1 R1 2 R1

R1

(3.120)

K and S can be obtained by solving equation (3.111) for S:

S

1 1 Arcoth bh

a R R0 R R0 ; K S a b R R0

1

(3.121)

This procedure requires two coatings: the infinitely thick layer and a coating with thickness h on an arbitrary substrate with reflectance R0. The measured reflectances on these two coatings are R? and R respectively. Accordingly, only three measurements in all (including that of the film thickness h) are needed in order to determine K and S. A second method is to determine the reflectances Rb and Rw of layers of equal thickness h on black and white substrates having known reflectances R0b and R0w . Accordingly, coth x can be eliminated from the two equations (3.111), written for Rb and Rw . The result is an equations for a:

a

1 Rw R0w Rb R0b 1 Rb R0b R0w 2 Rb R0w Rw R0b

Rw

(3.122)

Once a has been obtained, b is also known from equation (3.27). Then, from equation (3.121), K and S follow (as above) if R and R0 are replaced by the pair Rw , R0w or Rb, R0b . The classical method is generally more accurate, as an error analysis on white pigments has shown. Often, the reflectance of the black substrate R0b can be set equal to zero, as described in the preceding section. Equations (3.122) and (3.121) then simplify to

3.3 Kubelka-Munk Theory

Rb R0w Rw Rw Rb R0w

1 a 2 S

1 1 a Rb Arcoth b Rb bh

103 (3.123) (3.124)

Another way to determine K and S is with two transmission measurements, provided the film thickness is doubled for the second measurement. With suspensions, this can be done by using a cell with twice the cell thickness; with wafershaped plastic specimens, by laying one wafer on another. ªOptical contactº is a matter of concern here; it can be insured, for example, by applying an oil film to the surfaces and pressing the two wafers together. Because of the double film thickness there are two measured values t and t^ available to serve as arguments in the respective equations, giving bSh = x in one case and 2 bSh = 2 x in the other. The auxiliary variables a and b are thus not affected by doubling the thickness, since they do not depend on the thickness. The addition theorems for hyperbolic functions make it possible to obtain simple relations for this case: a

1 2

1 t

1 t

t t t

Here we have used the abbreviated notation r 1 1 t t2 t^

(3.125)

(3.126)

The following equation can be used to determine S:

S

1 Arsinh bt bh

(3.127)

104

3 How Spectra Depend on the Scattering and Absorption of Light

3.4

Hiding Power

3.4.1 General The official definition of the hiding power of a pigmented material is ªits ability to hide the color or color differences of the substrateº. The reader may be a little perturbed by the fact that this definition* uses the word ªhideº to explain ªhiding powerº, but in defense of the writers of the standards it must be said that there is scarcely a better way to express what is meant. The model underlying the hiding power relates to a black/white contrast substrate on which the coating is to be applied. The determination of the hiding power value involves ascertaining the film thickness h such that the contrast substrate just vanishes for the eye performing the assessment. The thickness hD (in mm) that statisfies this condition is called the ªhiding layerº; its reciprocal D = 1/hD (in mm±1 = m2/L) is the hiding power value. Like the tinting strength to be discussed further on, it is a measure of effectiveness, since it states the area (in m2) that can be covered with 1 L of paint applied in a hiding coat. If the vanishing of the contrast substrate were actually determined with the colorist's eye, hiding power would be a subjective quantity; to derive a functional method of determination, it is therefore necessary to place the procedure on a colorimetric basis.** For achromatic coatings, the ªcontrast ratioº earlier was used as the hiding criterion; this was the ratio of reflectances on the black and white portions of the substrate for equal film thicknesses. The contrast ratio was specified as 0.98 in order to take account of the 2 % threshold value for brightness perception by the human eye. With colored coatings, brightness contrast is not meaningful, so the hiding criterion was defined some time ago as a certain CIELAB color difference. The criterion DE ab = 1 is commonly employed. The experimental procedure is as follows: Coatings of various thicknesses are applied to the agreed-on contrast substrate. The color difference DE ab between the two contrasting fields is then determined by colorimetry for each of the coatings. If the results are plotted versus the reciprocal of film thickness, the hiding power value in m2/L can be read directly from the diagram at the point corresponding to the criterion DE ab = 1. An example is presented in the experimental section (Chapter 7). This determination procedure has, however, two serious deficiencies that can be seen at first glance: ± Several drawdowns with different film thicknesses must be prepared and measured ± The graphical evaluation is imprecise. * For standards see ªColoring Materials, Termsº in Appendix 1. ** Substrates must, of course, be standardized for an exact method of determination. Reflectance values R0b = 0 and R0w = 0.8 are employed.

3.4 Hiding Power

105

It follows that this method must be rationalized, for it would be desirable to use the minimum number of paint drawdowns and also to employ a computer for the evaluation. The following problem now arises: The Kubelka-Munk theory, next to colorimetry the most important principle for rationalizing an optical pigment testing method, applies only to spectral reflectances. On what wavelength should the measurement and calculation be based? It is for this purpose that the ªprinciple of spectral evaluationº was developed as a link from colorimetry back to the KubelkaMunk theory (Section 3.6). First, however, achromatic coatings will be analyzed. These lend themselves to a direct application of Kubelka-Munk theory provided certain constraints are observed. This section therefore lays the groundwork for the principle of spectral evaluation.

3.4.2 Achromatic Coatings In the ideal case (i. e., when the coating contains no colored substances), the small color difference DE ab remaining between the coating over white and over black can be set equal to the lightness difference DL . The same holds, however, when there is a slight undertone; for a nearly white or nearly gray specimen, the chroma difference and hue difference between white and black must be of a higher order than the lightness difference. Then, by (2.5) and subsequent equations, r r ! 3 Yw 3 Yb (3.128) DEab DL 116 Yw 16 116 Yb 16 116 100 100 where b stands for black and w for white. This equation should be valid for white and light gray coatings, so that the value function for Y 4 0.8856 has been used here. Further, because of the achromatic character, we can set Y/100 = R (i. e., the reflectance independent of l). What is more, we must take into account that the colorist, in the (computationally simulated) application of the hiding power criterion, will select a color matching angle such that the gloss of the specimen surface will not interfere. Thus, for glossy specimens, the colorist ªreflects outº the glossy effect by taking a suitable observation angle; this corresponds to a reflectance of R ± gr0, where g is the degree of gloss. Now the hiding power criterion can be formulated as p p 3 R DEab (3.129) DL 116 3 Rw gr0 gr0 1 s This condition with equations (3.111), (3.10), and (3.120) forms a closed system that makes it possible to calculate the hiding power value. Specifically, for given auxiliary variables a and b, the product S hD = 1/a can be determined. Because S and h in the Kubelka-Munk formulas appear only as their product, if the scattering coefficient S is known along with the value of a, then the hiding power value D can be calculated immediately, for D = 1/hD = a S.

106

3 How Spectra Depend on the Scattering and Absorption of Light

Accordingly, the hiding power value is calculated in a three-step procedure: 1. Determination of auxiliary variables a and b This can be done in either of two ways (see Section 3.3.3): ± R ? is available as a measured value; then by equation (3.120) 1 1 R1 ; b a R1 a 2 R1 ± Rw (along with R0w) and Rb are available as measured values; then by equations (3.123) and (3.27) 1 Rb R0w Rw Rw a Rb R0w 2 p b a2 1 ; R1 a b 2. Calculation of scattering coefficient S Equation (3.124) can be used for the calculation of S: S

1 1 a Rb Arcoth b Rb bh

3. Determination of the factor a The system of equations (3.111), (3.114), (3.10),and (3.129) in complete form, with a = 1/ShD, is Rb

Rw

1 a b coth

b b coth a b R0w b coth a

R0w

1 a

Rb r0 Rw r0

a

b a

1

r0 1 r2 0:36 Rb 0:04 Rb 1 r2 Rb 1 0:6 Rb

1

r0 1 r2 0:36 Rw 0:04 R w 1 r2 Rw 1 0:6 Rw 1 p 3 R gr0 0 b 116

p 3 R gr0 w

(3.130)

3.4 Hiding Power

107

Solution of this system leads to a final equation of at least sixth degree in coth (b / a). Such an equation cannot, however, be solved in elementary functions, and so the function a, which depends on a (or R1 ) and g, cannot be written out explicitly.* An iterative solution procedure must therefore be used, for example Newton's method. For this purpose, the derivatives of the individual equations in the system are needed; with x = 1/a, we have

2

R b

dRb dx

R w

dRw b2 dx a

R b

dRb 1 r0 1 r2 0:384 R b R b dx 1 0:6 Rb 2 1 r2 Rb 2

R w

dRw 1 r0 1 r2 0:384 R w R w dx 1 0:6 Rw 2 1 r2 Rw 2

b a sinh bx b cosh bx

1 2 a R0w R2 0w R0w sinh bx b cosh bx2

(3.131)

Setting the left-hand side of the last equation in (3.130) equal to Z (which must be made zero) gives " # R w R b dZ 1 (3.132) Z 2 2 dx 3 R g r 3 R g r 3 w

0

b

0

These equations can be used with a desk calculator to prepare a table of a as a function of R1 and g. Such a table, for use as a computational aid, is appended to the first publication (see [24] in Section 3.9). Moreover, the tabulated value can be approximated very closely with a nonlinear regression calculation, so that values of a can be obtained from simple quadratic expressions with two coefficients. This computational aid is included in Chapter 7. There are accordingly two ways of obtaining individual a values without using the somewhat unwieldy formulas from above. The hiding power value is then

D

1 aS hD

(3.133)

* Once again (see also the first footnote in Section 2.3.3), it would have been more advantageous to give the value function a logarithmic form. Then the system of equations could have been solved in elementary functions, so that a could have been written explicitly as a function of R1 .

108

3 How Spectra Depend on the Scattering and Absorption of Light

The following measurements are therefore needed in order to determine the hiding power value: ± The reflectance of the infinitely thick layer (R ?) or, in its place, the reflectance over white (Rw) for a film thickness the same as over black, together with the reflectance of the white substrate (R0w) ± The reflectance over black (Rb) ± The degree of gloss of the infinitely thick layer or the coating over white (g) ± The film thickness over black (h) In this way, the goal of rationalization stated in Section 3.4.1 has been achieved. The determination method discussed here is essentially the method of DIN 55984*, except that the standard is based on high-gloss specimens and does not allow for the actual degree of gloss g. The method just described can therefore be regarded as a refinement of the DIN method. It becomes identical with the DIN method if g is set equal to 1 in all the equations.

3.4.3 Scattering and Absorption Components The hiding power is entirely due to the cooperation of scattering and absorption, as has already been shown. The ªscattering componentº and the ªabsorption componentº are those contributions to the hiding power value, expressed as fractions of the total hiding power, that arise from ªhiding power due to scattering aloneº and ªhiding power due to absorption aloneº. To obtain the equations for these components, we take the Kubelka-Munk equations to the limits K ? 0 and S ? 0, respectively. In the assessment of the hiding quality of a coating or pigment, a knowledge of these contributions is important for, say, a white pigment, where only the hiding power contribution due to light scattering is valuable ± in this case, the contribution due to absorption is not useful because absorption components in the case of a white pigment are equivalent to loss of quality. As far as possible, therefore, white pigments should cover solely by virtue of their scattering power, not because they also absorb. But this classification can also be significant for colored pigments; in particular, inorganic pigments are often rated better, the more their hiding is due to scattering. The formulas will now be restated, first for the ªhiding power due to scattering onlyº (equations 3.115 and 3.113): Rb

Sh ; 1Sh

Rw

1 R0w S h R0w 1 R0w S h 1

* For further standards see ªHiding Powerº in Appendix 1.

3.4 Hiding Power

109

and then for the ªhiding power due to absorption onlyº (equation 3.112): Rw R0w e±2Kh

Rb 0 (since R0b 0);

These equations will be used later when the determination of the general hiding power value is discussed. Again, however, the solution needed for rationalization can be stated immediately for achromatic coatings. The ªhiding power due to scattering onlyº Dsca is obtained from equation (3.113) with ab = 1/ (ShD): Rb

1 ; 1 ab

Rw

1

R0w 1 ab 1 R0w ab

(3.134)

These two equations are simply inserted in system (3.130) in place of the first two equations; the iteration then yields Dsca directly. The ªhiding power due to absorption onlyº Dabs can be calculated in a similar way. With equation (3.112) and b = 1/ (KhD), Rb 0 ;

Rw R0w e

2 b

(3.135)

In the case of the absorption component, it is actually possible to solve the system of equations explicitly. We do not need to do this, since it is sufficient to calculate b using equation (3.130) after inserting equations (3.135) in place of the first two equations in the system. Both tables and simple linear formulas are available for the scattering and absorption cases, so that b can be determined; we will become acquainted with these aid in Chapter 7. The ªhiding power due to absorption onlyº Dabs is obtained from 1 bK b a 1 S (3.136) Dabs hD From Dsca and Dabs , the scattering and absorption components dsca and dabs of the hiding power D are calculated as follows: dsca

Dsca ; D

dabs

Dabs D

(3.137)

In many practical examples, it has turned out that a residue is still present after these two components are subtracted. How can this be accounted for? Obviously, that contribution to the hiding power arises from the interaction of scattering and absorption. For if the scattering coefficient increases, the mean distance traveled by light in the layer also grows longer because the light is scattered and rescattered more times. A longer path length, however, necessarily means that more light is absorbed, so there is an additional ªscattering/absorption contributionº, which would not be present if the layer scat-

110

3 How Spectra Depend on the Scattering and Absorption of Light

tered but did not absorb or if it absorbed but did not scatter. This contribution will be called the ªinteraction componentº dint and is given by dint 1 ± dsca ± dabs

(3.138)

The three components given by equations (3.137) and (3.138) can provide much additional information about the hiding power value.

3.5

Transparency

3.5.1 Description and Definition If several layers are printed on a black substrate, one over another, it is generally seen that the layer increasingly displays a more-or-less weak, bright shimmer in comparison to the unprinted black substrate. This shimmer grows stronger as the process is repeated. The same phenomenon is known with lacquers and paints, provided they are sufficiently transparent. It obviously comes about because scattering particles, commonly pigment particles, are present in the medium (ink or paint). If, in an unprejudiced spirit, one first considers ªtransparencyº as a purely optical phenomenon, it is clear that this scattering effect is opposed to it. This argument is the basis for the definition of transparency as applied to the field of pigments. The standards* define transparency as the property of a system (not necessarily a pigmented system) to scatter light as little as possible. Accordingly, the color change on application to a black substrate should be as slight as possible. The transparency of the system is greater, the less color change takes place. Given identical specimen preparation, the transparency of the system can be employed for a comparative assessment of transparent pigments. An expedient approach to the exact definition of a ªtransparency numberº, according to the discussion just presented, is to use the CIELAB color difference as a function of the film thickness h. Figure 3-10 gives such a plot, showing DEab that the reciprocal slope of the tangent at the origin provides a suitable measure for the transparency number T. We then have T cot j

1 1 dDE tan j ab dh

* For standards see ªTransparencyº in Appendix 1.

(3.139) b h=0

3.5 Transparency

111

Fig. 3-10. Definition ot the transparency number T.

Because the color difference has the dimension 1, expression eq. (3.139) has the units of a length. If the film thickness is measured in mm, the transparency number takes on units of 1 mm = 1 L/m2. But what does it mean to state the transparency number T in L/m2 ? According to the definition in equation (3.139), the number T obviously states how many liters of an ink or paint can be printed or spread on one increases by 1. This interpretation square meter of a black substrate before DEab suggests an effectiveness property similar but not identical to the hiding power value. Of two paints, then, the one having the better transparency is the one that can be applied in a thicker coating (i. e., one giving more color) to achieve a given transparency. Like the definition of the hiding power value, this definition immediately im versus plies a method for determining the transparency number. The curve of DEab h is plotted through a few experimental points, and then the tangent at the origin is found graphically or by calculation. If one then works close enough to the origin, a single measured point (aside from the origin = black substrate) is generally sufficient. As in the case of the hiding power, such a procedure lends itself to rationalization. As in the earlier case, one or at most two measurements will be adequate; here, however, the Kubelka-Munk theory, because of its monochromatic character, is not directly applicable. This point will also be taken up in Section 3.6.

3.5.2 Coloring Power By analogy with the transparency number T, a ªcoloring powerº F can be defined. This step is favored by the following argument: of two coatings equal in transparency, the one giving more color is certainly the better. This ability to give color, called coloring power, was not considered in the determination of the transparency

112

3 How Spectra Depend on the Scattering and Absorption of Light

number. The determination of color strength must make use of a white substrate*; versus h is employed. In accordance with the above proceagain a curve of DEab axis is defined as the coloring dure, the angle between the tangent and the DEab power; because of the direct proportionality, this is smaller the steeper the tangent line (Fig. 3-11). The coloring power can be read off the plot: F

dDEab dh

w h=0

(3.140)

Fig. 3-11. Definition of coloring power F in comparison with transparency number T.

Like the hiding power value, F has the dimensions of reciprocal length. Thus it is, once more, an effectiveness property, for F = 1 mm±1 = 1 m2/L means that 1 m2 of the white substrate must be coated with one liter of the paint or ink in order to relative to the white substrate equal to 1. The dimake the color difference DEab mensions of the transparency number and coloring power are thus reciprocals; accordingly, the product of F and T is a quantity having the dimension 1, which we will call the ªtransparency-coloring powerº L. The term ªtransparency-coloring powerº also includes an evaluation of the color-giving property in the sense of the statement, made above, that between two color-giving films of equal transparency the one giving more color is the better. Thus we have L = FT

ªtransparency-coloring powerº

* Standaridized as an ideally white substrate, R0w = 1.

(3.141)

3.5 Transparency

113

We must now look ahead to the next section, where it will be shown that the transparency number T as we have defined it is the reciprocal of the colorimetrically evaluated scattering coefficient S, while the transparency-coloring power F is directly proportional to the colorimetrically evaluated absorption coefficient K. Accordingly, the product in equation (3.141) contains both these coefficients, even though in colorimetrically evaluated form, precisely as in the numerator and denominator of the Kubelka-Munk function K/S. Conversely, to any K/S value a reflectance can be assigned (see, e. g., eq. 3.116), and so from L we call finally calculate a ªtransparency-coloring degreeº G = 1 ± R , which like the reflectance must lie between 0 and 1: G=

p L L 2

L

ªtransparency-coloring degreeº

(3.142)

The quantities L and G are highly suitable for characterizing transparency-coloring action (i. e., along with color-giving action).

3.5.3 Achromatic Coatings In this section we will show that a model analysis based on achromatic systems can also be meaningful in the understanding of transparency. In practice, such systems play virtually no part; the value of such an analysis lies rather in that it will aid us in acquiring important knowledge. We proceed as in the definition of T, equation (3.139), following the established by DL = Lb L0b = Lb ; we then have pattern (see Section 3.4.2) of replacing DEab 1 L b 116 Y b T (A prime denotes the result of applying the operator (d/dh)h=0 to the unprimed quantity). For Y b we must use the linear form of equation (2.6) here because of the nearness to the origin. If Yb /100 = Rb , 1 116 7:787 R b T By the third equation of (3.131), this gives 1 116 7:787 0:384 R b T Provided the layer does not absorb but only scatters, equation (3.115) applies. The above operator then yields R b = S, so that

114

3 How Spectra Depend on the Scattering and Absorption of Light

1 116 7:787 0:384 S 346:9 S T in other words, the transparency number is inversely proportional to the scattering coefficient of the pigmented layer: 1 T 0.002883 (3.143) S A similar analysis can be carried out for the coloring power F. In definition (3.140), DEab is replaced by DL = L0w ± Lw = 1 ± Lw , so that F

L w

116 Y w

The cube-root form of equation (2.5) must be used for the value function Y w . Then, with Yw /100 = Rw and R0w = 1, F

116 R 31 w

116 0:384 R 3 1 0:6 R0w 2 w

This holds provided the layer absorbs only and does not scatter. Then we have the limit equation (3.112) for Rw ; the operator gives R w = ±2 R0w K. With R0w = 1, F

2 116 0:384 1 K 185:6 K 3 1 0:6 12

(3.144)

We thus have the important result that, with the transparency number T and the coloring power F as defined in Sections 3.5.1 and 3.5.2, ± T is inversely proportional to the scattering coefficient S in achromatic, nonabsorbing layers ± F is directly proportional to the absorption coefficient K in achromatic, nonscattering layers This close relationship between T and S, on the one hand, and on the other between F and K is qualitatively the same for chromatic layers. The example also shows clearly that forming the product L = FT gives an expression proportional to K/S. Section 3.6 will now show that S and K in these formulas are represented by the colorimetric integrals of S (l) and K (l) in the case of colored coatings.

3.6 Principle of Spectral Evaluation

3.6

115

Principle of Spectral Evaluation

3.6.1 Description and Significance In order to work out a rational procedure similar to that for the ªachromaticº hiding power (Section 3.4.2), we must face the unanswered question of how to use the Kubelka-Munk theory, which is intrinsically ªspectralº, in solving the problem. The restriction to a single wavelength is typical for achromatic layers, as has been shown. With colored coatings, however, it is not immediately clear whether the measurement and calculation should be done for a preferred wavelength, although everything speaks for the necessity that the entire spectrum should be included in the calculation. But what approach to evaluation then remains open? These are the questions that will be answered once the principle of spectral evaluation has been discovered. The procedure can be described as a feed-back between the Kubelka-Munk theory and colorimetry. As has already been illustrated more than once (e. g., in Sections 3.3.3 and 3.4.2), one determines K and S on a infinitely thick layer and on a finite layer of known thickness over black. The infinitely thick layer can be replaced by a layer over white having the same thickness as the layer over black. This determination of K and S is done not once, but several times for distinct wavelengths spread throughout the visible spectrum. As we have seen, K (l) and S (l) as wavelength-specific constants of a coating govern its optical behavior, so that once they are known it is possible to calculate in advance what reflectances over white and black are to be anticipated at any wavelength in the spectrum and for arbitrary film thicknesses. Now the CIE system is used in determining the color stimulus associated with the spectrum just calculated. Two color stimuli are obtained, one over black and one over white. These imply the corresponding CIELAB coordinates, . This color difference between white and which yield the color difference DEab black must now be subjected to a suitable iterative procedure to make it equal to 1. Now there is a tool for determining by iterative methods the film thickness such that the color difference between white and black will be exactly 1. By going through these purely computational steps, we have simulated the older sampling method for determining the hiding film thickness; the simulation complies fully with the DIN method discussed in Chapter 7. But the determination of hiding power of lacquers, paints, and plastics, just briefly sketched, is merely one example of the usefulness of the principle of spectral evaluation. Later, we will become acquainted with other applications, such as the determination of transparency and the determination of the relative tinting strength of pigments. The universal applicability of the principle to other problems is implied by the fact that it is the key to rationalizing all test methods based on the visual assessment of a match (or fixes difference) between two color drawdowns. With this generalization, it is possible to state the principle in pure form, independent of any special application. Figure 3-12 is an explanatory flowchart.

116

3 How Spectra Depend on the Scattering and Absorption of Light

Fig. 3-12. Flowchart explaining the principle of spectral evaluation.

At the start, the scattering and absorption spectra S (l) and K (l) must be known; that is, these quantities have already been determined on suitable coatings or dyed materials. The variable in the problem, here denoted by w (e. g., film thickness h, scattering coefficient S, absorption coefficient K, pigment volume concentration s,* etc.), is set to an initial value. From it, the reflection spectrum can be calculated with the Kubelka-Munk formulas, and this in turn, with the aid of colorimetry (CIE and CIELAB systems), yields the value of some colorimetric quantity Q for the two color drawdowns being compared. If there is still a difference between the Q found and the nominal Q, this difference (here denoted by DQ) is utilized in calculating a correction to the variable w. The iteration continues until the nominal and actual Q values are sufficiently close together. The w value at this time is the desired value of the variable. In order for the correction Dw to be calculated from DQ, additional information (i. e., formulas not contained in the Kubelka-Munk theory) may be needed.

3.6.2 Application to Hiding Power By the discussion of the achromatic hiding power in Section 3.4.2, it can be stated that the general determination of hiding power with the principle of spectral evalua* If s is selected as variable, a theoretical notion about the concentration dependence of S or K is generally required; see Chapter 4.

3.6 Principle of Spectral Evaluation

117

tion also involves three steps, roughly analogous to those in Section 3.4.2. Specifically, these steps are ± Determination of auxiliary functions a (l) and b (l) ± Determination of scattering coefficient S (l) and absorption coefficient K (l) and iterative calculation to make DEab =1 ± Determination of DEab Now, however, there is the difference that nearly all the quantities to be determined are functions of l. This takes in a (l), b (l), S (l), K (l), and all the R (l) and R (l). In what follows, the l dependences will not be explicitly shown; the notation ª(l)º will appear only as required for clarity. 1. Determination of auxiliary variables a (k) and b (k) The same formulas as in Section 3.3.3 are used here; thus the two auxiliary variables are determined either from R ? or from Rb , Rw , R0b , R0w, all of which must first be transformed into starred quantities by application of the Saunderson correction. In place of equation (3.123), the complete form equation (3.122) is employed, since real black substrates are not always ideally black: a

1 Rw R0w Rb R0b 1 Rb R0b R0w 2 Rb R0w Rw R0b

Rw

As a rule, the l-dependent quantities are now calculated at intervals of 20 nm, that is, with a total of 16 known points, since this is regarded as sufficient for most applications. 2. Determination of the scattering coefficient S (k) and the absorption coefficient K (k) In this step, again the complete computational formula for S must be used, since the white substrate can be used too for the determination of S: S

1 1 Arcoth bh

a R R0 R R0 b R R0

Depending on whether the measured values are Rb , R0b , or Rw, R0w, these are inserted for R and R0 (after application of the Saunderson correction). If, however, the values over both substrates are known, it is desirable to use the R , R0 pair that gives the smaller error of determination for S. To this end, the two errors ± dSb from Rb , R0b ± dSw from Rw , R0w must be compared. The formulas needed are derived from the error propagation law (with dR as error of measurement in the reflectance):

118

3 How Spectra Depend on the Scattering and Absorption of Light

dS2

"

uS uR

# 2 uS 2 dR2 uR0

(3.145)

The partial derivatives are calculated by the chain rule: uS 1 r2 R 2 uS 2:6 1 1 r0 1 r2 uR uR

0:6 R 2

uS uR

(3.146)

and similarly for uS / uR0 with R0 replacing R . Furthermore, uS uR

1 1 uy b h y2 1 uR a R R0 R R0 b R R0

1

where y

(3.147)

and similarly for uS/uR0 with uy/uR0 replacing uy /uR . Finally, uy uR

1

2 a R0 R2 0 b R R0 2

uy uR0

1

2 a R R2 b R R0 2

and

(3.148)

(3.149)

Now both errors of determination dSb and dSw can be calculated with equation (3.145); dR can be set equal to 1 because the two errors are only to be compared. 3. Determination of DE*ab and iterative calculation to make DE*ab = 1 The first step is to specify an initial value h C h0 for the film thickness and to calculate Rw and Rb with the Kubelka-Munk equation (3.111). Both quantities are transformed to uncorrected values with the aid of the inverse Saunderson correction, equation (3.10); at the same time, it is taken into account that the gloss has been reflected away from the observer (see Section 3.4.2), so that R

1

r0 1

r2 R r0 r2 R

g r0

(3.150)

Next, from Rb and Rw, equation (2.3) is used to calculate X, Y, Z by means of the CIE system, for both layers (over white and over black): X

R

x l S l R l dl

(3.151)

3.6 Principle of Spectral Evaluation

119

Here x (l) S (l) stands for the CIE color matching function x given the selected CIE standard illuminant S (l).* In this way, Xb,Yb, Zb and Xw ,Yw , Zw are obtained; these are the CIE tristimulus values of the drawdowns over black and over white. A problem still awaiting solution by the CIE must be mentioned here: how to obtain firm CIE color matching functions x (l), y (l), z (l) for 20 nm intervals. At present, the color matching functions exist only in the form of numerical tables for 5 nm intervals (ISO 7724-1). Without an agreed-on table for 20 nm intervals, it is not certain that two distinct laboratories will obtain the same results. Until 20 nm tables are embodied in standards, it is recommended that the Stearns tables** (see Section 3.7; for examples, see Chapter 7) be employed; these may also be suggested to the CIE for adoption, because the interpolation method used is scientifically well justified. The six CIE tristimulus values are now converted to values X b , Y b , Z b and X w , Y w , Z w by the familiar method (see Section 2.3.3); the cube-root form must be used above the threshold X/Xn = 0.008856 etc., the linear form in other cases. Hence, the differences Da , Db , DL between the layers over black and over white are obtained as differences of the CIELAB color coordinates ab , bb , Lb and aw , bw , then follows. If this value is not yet close enough to unity, h Lw . The value of DEab should be changed in the proper sense and the calculation repeated (iteration loop in Fig. 3-2 with h as variable). For the iteration proper, any zero-finding technique known from numerical ± 1 equal to zero). Because of its many admathematics can be used (to set DEab vantages, Newton's method is recommended here again. The main virtue of this technique is fast convergence; considerable amounts of machine time may be required for other procedures. Newton's method does have the drawback that all the derivatives of the variables must be formed, but this laborious manual computation has to be done only once. The equations needed are stated here. ± 1 to zero, to work with the function It is useful, instead of taking DEab Z = ln DEab ? 0 ,

(3.152)

because the logarithm converges to zero more rapidly. The step-by-step procedure for differentiation with respect to h is as follows:

* The notation S (l) is used to distinguish this function from the wavelength-dependent scattering coefficient S (l). ** See ªColor matching functions in steps of 20 nmº in Appendix 1.

120

3 How Spectra Depend on the Scattering and Absorption of Light

uZ 1 2 uh DEab

uDa uDb uDL Db DL Da uh uh uh uDa ua w uh uh

uab uh

uDb ub w uh uh

ubb uh

uDL uLw uLb uh uh uh ua uX uY 500 uh uh uh ub uY uZ 200 uh uh uh uL uY 116 uh uh

(3.153)

There are two cases: 1) X/Xn ^ 0.008856 etc.

2) X/Xn > 0.008856 etc.

uX 7:787 uX uX X uX etc. etc. uh uh 3X uh Xn uh Z uX u R l x l S l dl etc. uh uh uR 1 r0 1 r2 uR 0:384 uR uh uh 1 r2 R 2 1 0:6 R 2 uh uR bS2 uh a

1 2 a R0 R2 0 R0 sinh bSh b cosh bSh

The derivatives for the two extremal cases, ªscattering onlyª (Rsca ) and ªabsorption onlyª (Rabs ), should also be written out: uRsca S uh 1 uRabs uh

1 R0 R0 Sh 1

2 KR0 e

2Kh

2

2 KRabs

(3.154)

3.6 Principle of Spectral Evaluation

121

So much for the derivatives needed in Newton's method. It goes without saying that these formulas must be worked out back to front; that is, one must begin with the last of the equations just presented, incorporating these into the respective steps of the main program if one wishes to write a computer program. An example of these formulas, which may appear somewhat confusing ± though only at first glance ± appears in Chapter 7 along with a program listing.

3.6.3 Application to Transparency and Coloring Power The distinctive point about the application of the principle of spectral evaluation to transparency and coloring power is that no iteration is required; the values sought are obtained by direct calculation. The reason is that what is being sought is not an optimal film thickness or pigment concentration; instead, the initial slope (at a film thickness of h = 0) of colorimetric quantities versus h is to be determined. In order for the principle to apply to transparency and coloring power, defining relations (3.139) and (3.140) and the formulas derived from them must be replaced by their partial derivatives with respect to h, then taken to the limit as h ? 0. It then are, for the transparency, the becomes clear that the quantities derived from DEab colorimetrically evaluated scattering coefficient and, for the coloring power, the colorimetrically evaluated absorption coefficient. In the following equations, a prime denotes the result of applying the operator (u/uh)h?0 to the unprimed quantity. DE ab

uEab uh

s 2 2 2 ua ub uL uh uh uh h?0

a 500 X

Y ; b 200 Y

h?0

p a 2 b2 L 2

Z ; L 116 Y

(3.155)

This equation is to be used for calculating as ; bs ; Ls with Xs ; Ys ; Zs , and for calculating ak ; bk ; Lk with Xk ; Yk ; Zk ; symbols with subscript s are for transparency, , namely those with k for coloring power. As a result, two values are found for DE ab DEab;s and DEab;k . X s Y s Z s ; Z s 7:787 ; Y s 7:787 X s 7:787 Xn 100 Zn X k X k ; 3 Xn X s

R

x l S l 1

r0 1

Y k

Y k ; 3 100

Z k Z k 3 Zn

(3.156)

(3.157)

R r2 S l dl 0:384 x l S l S l dl (3.158)

122

3 How Spectra Depend on the Scattering and Absorption of Light

(and similarly for Ys ; Zs with x (l) replaced by y (l) and z (l) respectively). Again SÅ (l) denotes the spectrum of the CIE standard illuminant used, and S (l) is the spectral scattering coefficient. R 1 X k 2 x l S l 1

R r0 K l dl 4:8 x l S l K l dl r2

(3.159)

(and similarly for Yk ; Zk with x (l) replaced by y (l) and z (l) respectively). The expressions to the right of the first equality signs in the last two equations allow for the possibility that the spectra of the two reflection coefficients r0 and r2 are known. The equations just stated must, once again, be worked through backwards in the practical calculation, that is, beginning with the last equations. Finally, the transparency number and coloring power are obtained as T

DE ab;k 1000 m2 mL 1 mL m 2 ; F 1000 DE ab;s

(3.160)

The factor 1000 appears twice so that smaller numbers can be used for T and F (in derived units). Now T denotes the number of mL that can spread over 1 m2 before measured against the black substrate becomes equal to 1. Similarly, F denotes DEab of 1 is the number of m2 that can be covered with 1 mL so effectively that a DEab obtained relative to an ideal white. All the equations needed for transparency and coloring power have now been written down. Similarly to what was done in Section 3.5.2, the transparency-coloring power L and the transparency-coloring degree G can be calculated from T and F. All of these equations will be repeated for direct computer processing in the practical portion of Chapter 7. It is now possible to determine hiding power and transparency after a minimum of three spectral reflectance measurements (R ?, Rb , R0b or R ?, Rw , R0w). Modern instruments employing the spectral method offer a suitable tool for color measurement. In conclusion, a further very important point should be noted, again a consequence of the application of the principle of spectral evaluation. The direct determi versus h (Fig. 3-7) is difficult because nation of the tangent to the curve of DEab highly uncertain reflectances close to zero have to be measured. A result obtained by the theoretical analysis based on the principle of spectral evaluation, equations (3.158) and (3.159), namely that S (l) and K (l) in colorimetrically evaluated form satisfy the definitions of T and F, makes it possible to determine S and K at higher reflectances (e. g., over a white substrate) where the uncertainties are much smaller. In this way, the procedure allows the transparency number and color strength to be determined with far smaller errors than when they are obtained from the tangents to the curves at the origin.

3.7 List of Symbols Used in Formulas

3.7

123

List of Symbols Used in Formulas

a, b auxiliary variables in Kubelka-Munk theory CIELAB color coordinates a , b , L A = a sinh x + b cosh x abbreviated notation in four-flux theory = a sinh 2 x + b cosh 2 x same as A for doubled film thickness Aj = {A1j, A2j, ¼, Anj} eigenvectors of many-flux theory a = 1/ (ShD) factor for calculation of hiding power constants of integration in four-flux theory B1, B2 b = 1/ (KhD) factor for determination of hiding power C auxiliary variable for coefficient determination in four-flux theory constant of integration in many-flux theory Cj w variable in principle of spectral evaluation D hiding power value with subscripts: abs due to absorption only sca due to scattering only d components of hiding power value with same subscripts as D, plus int interaction component Da , Db , DL special CIELAB color differences CIELAB color difference DEab DQ difference between actual and nominal Q values dR error of measurement of R dS error of measurement of S Z null function for iterative procedure sign factor in many-flux theory Zi Kubelka-Munk function FKM g degree of gloss G transparency-coloring degree g diffuse radiation component h film thickness with subscript: D hiding layer k' absorption coefficient for directional radiation absorption coefficient in many-flux theory kj K absorption coefficient for diffuse radiation l radiance (directional) radiances (directional) in incidence direction and opposite to incil +, l ± dence direction

124

3 How Spectra Depend on the Scattering and Absorption of Light

L L+, L++ L±, L= L lj m n p, P, q, Q j F r0 r1 r2 R, R , R R; R R; R, R , R

R , R1, R2, R3 R^ s+, s± S

with subscripts: 0 upper boundary of layer h lower boundary of layer transparency-coloring power radiances (diffuse) in incidence direction with same subscripts as l +, l ± radiances (diffuse) opposite to incidence direction with same subscripts as l +, l ± radiance vector eigenvalues in many-flux theory attenuation coefficient number of channels in many-flux theory auxiliary variables in four-flux theory with subscript: sca scattering only (h) slope angle of function DEab coloring power reflection coefficient at the surface for directional light incident at right angle from outside reflection coefficient for diffuse light incident from outside reflection coefficient for diffuse light incident on the surface from the interior of the specimen reflection factors: measured, surface-corrected, and surface-corrected after exclusion of directional radiation with same subscripts as R abbreviated notation in four-flux theory reflectances: measured, surface-corrected, and surface-corrected after exclusion of directional radiation with subscripts: 0 substrate abs extreme case ªabsorption onlyª b black substrate dif diffuse irradiation ex exclusive of surface reflection g directional irradiation in inclusive of surface reflection r perpendicular irradiation and measurement w white substrate ? infinitely thick layer abbreviated notation in four-flux and Kubelka-Munk theories R for doubled film thickness scattering coefficient for directional light in incidence direction and opposite to incidence direction scattering coefficient for diffuse light

3.8 Summary

125

S (l) sij, Sij S t T T, T , T

lamp spectrum matrix of coefficients in many-flux theory matrix of scattering coefficients in many-flux theory abbreviated notation in determination of Kubelka-Munk coefficients transparency number transmission factors: measured, surface-corrected, and surface-corrected after exclusion of directional radiation with same subscripts as R transmittances: measured, surface-corrected, and surface-corrected t, t ; t after exclusion of directional radiation with same subscripts as R t^ transmittance for doubled film thickness u, w auxiliary variables in four-flux theory x = bSh abbreviated notation in four-flux and Kubelka-Munk theories x (l), y (l), z (l) CIE color matching functions X,Y, Z CIE tristimulus values with subscripts: b black substrate n CIE standard illuminant w white substrate CIELAB value functions X ,Y , Z with same subscripts as X,Y, Z x = 1/a variable for calculation of hiding power value y abbreviated notation in calculation of hiding power value z position coordinate

3.8

Summary

The phenomenological theory of absorption and scattering in turbid media is of fundamental significance for the mathematical treatment of the coloration of lacquers, paints, clouded glasses, etc., and thus for all problems associated with the use and economics of pigments and dyes. The most general form of the phenomenological theory seems to be the many-flux theory, whose mathematical formalism is described in full. Typical for this model is an absorbing and scattering medium bounded by two parallel planes. The boundary conditions can allow for many irradiation geometries; the reflection coefficients at the interfaces can be calculated exactly. A calculation for real layers, however, involves heavy use of the computer and is thus not well-suited to daily practice. The correction formulas for surface reflection can be written down immediately and are thus an exception to the above statement.

126

3 How Spectra Depend on the Scattering and Absorption of Light

The four-flux theory is derived as an important special case, and its results are written as a collection of explicit formulas. The links between the four-flux theory on the one hand and the theories of Kubelka-Munk (two-flux) and Ryde/Duntley (special case of four-flux) on the other are discussed. The four-flux theory in this generalized form yields equations for the case of irradiation from both sides, for the transmission, and for the particularly important cases of reflection with substrate and reflection with infinitely thick layer, both with mixed (diffuse and directional) irradiation. What is more, the case of a specularly reflecting substrate is treated, as are the extreme cases where absorption is strongly dominant and where scattering is strongly dominant. It is further shown how the five coefficients can be determined experimentally from reflection or transmission measurements, that is, in particular how the poorly accessible coefficients for directional irradiation can be determined exactly. Finally, the equations of the Kubelka-Munk theory and the formulas for obtaining their coefficients are summarized. The hiding power of scattering and absorbing layers is the most important technical quantity that can be rationalized with the aid of the phenomenological theory. = 1 between the On the basis of the definition in terms of the hiding criterion DEab layers over black and white substrates, the simplified case of achromatic layers is considered; equations for the hiding power applicable to this case can be derived in a direct fashion from the Kubelka-Munk formalism. The hiding power so obtained can be split into a scattering component, an absorption component, and an interaction component, so that additional information can be extracted about the quality of the layer. The transparency number for paints and inks is described and defined. This quantity also makes it possible to characterize the optical performance of transparent pigments. In connection with transparent coatings, a coloring power can also be defined and determined exactly; other quantities describing the transparency-coloring properties can be derived from the transparency number and the coloring power. Finally, the principle of spectral evaluation is thoroughly discussed as a feedback between colorimetry and the Kubelka-Munk theory. Only in this way can the hiding power of chromatic layers be approached in an exact manner. All the needed formulas, including those for a Newton iteration method and for an improved accuracy in the determination of S, are derived. This principle can also be used to advantage for the transparency number.

3.9

Historical and Bibliographical Notes

The absorption-based approach arose out of what was once the most important specialty in physics, an area that received a high degree of early development: astronomy. It was astronomical problems that led to the formulation of what is now known as Lambert's law. Lambert, who lived from 1728 to 1777, was also con-

3.9 Historical and Bibliographical Notes

127

cerned with astronomical topics and was seeking a law to describe the decrease in intensity of starlight as it passed through the atmosphere. The beginnings of this theory may be said to go back to Bouguer in 1729. The first worker to take up the phenomenological theory of scattering was ± we suppose ± Stokes [1], but once again, usable formulations came from astronomy. Because both the Earth's atmosphere and interstellar space contain dust particles, a formula based on absorption alone is not always adequate to predict intensities in astronomy. The first closed phenomenological theory of scattering dates from 1905 and was devised by the astronomer Schuster [2]. Here the model of two ray paths appears for the first time; Schuster, who of course was interested only in transmission behavior, obtained a transmittance formula similar to the later ones of Ryde and Kubelka for diffuse light. More than a decade later, in 1918, Renwick [3], [4] confirmed Schuster's results, but went a step further and treated reflectance as well. The formulas were clumsy, however, and not well-suited to calculating the reflectances of scattering layers. In 1927, Silberstein [5] essentially confirmed Schuster's transmission equation, but this publication contains the first discussion of a model for directional irradiation. Gurevic [6] in turn gave a more thorough treatment of the reflectance. But all the work cited must be regarded as preliminary to the classic publications of Kubelka and Munk [7] and Ryde [8], which came out in 1931. Kubelka and Munk, with no knowledge of prior work, analyzed the reflectance for the diffuse irradiation case with a substrate, deriving the still-used formulations in terms of hyperbolic functions (these first by Kubelka in 1947 [9]). Their main achievement, however, is the application of the equations to hiding power, on the one hand, and on the other to the reflectance of very (ªinfinitelyº) thick layers. The latter aspect is embodied in the Kubelka-Munk function, which found immediate acceptance and is applied to all cases involving scattering layers of high hiding power. The Kubelka-Munk theory gives the first clear expression of the fact that two coefficients are needed in the case of diffuse irradiation (ªtwo-constant theoryº) and that these coefficients can in fact be determined. The Kubelka-Munk theory fails in the case of a highly dilute pigment or a very thin layer (see Section 3.3.1), because the radiation cannot be ideally diffuse and not every ray collides with a pigment particle (ªsieve effectº). With specific application to biological measurements, Fukshanski [10] has devised a theory, but its concepts have not yet been made to work for lacquer and paint coatings. Ryde [8] analyzed transmittance and reflectance for the case of directional irradiation. The two ªdiffuseº coefficients are complemented by two more scattering coefficients, making a total of four. Later, Duntley [11] extended the theory by introducing a second absorption coefficient for directional irradiation; as a result, five coefficients (including the Kubelka-Munk coefficients) are needed for the phenomenological description of scattering and absorbing layers with directional irradiation. In comparison with the Kubelka-Munk theory, the Ryde theory has not gained such wide adoption.

128

3 How Spectra Depend on the Scattering and Absorption of Light

Duntley [11] was also concerned with surface phenomena. The correction formula proposed by Saunderson [12] dates from the year 1942. A good survey of these formulas can be found in Brockes [13]. The complete version of the explicit four-flux theory was published in 1962 [14]. Like the Ryde/Duntley theory, it employs five coefficients; it goes further, however, including equations for two-sided irradiation with diffuse and directional light and for layers with substrates. A second part was added in 1964 [15], now describing the determination of the three ªdirectionalº coefficients. The equations for specularly reflecting substrates, on the other hand, were not included in the publications cited; they are presented for the first time in this book. The first part of the four-flux theory [14] was confirmed a few years later by Billmeyer and co-workers [16], who also introduced another (fourth) scattering coefficient. The comprehensive many-flux theory is due to Mudgett and Richards (1971) [17], whose work marked the completion of the phenomenological theory of scattering and absorption for the time being. The standard work on radiative transfer processes, by Chandrasekhar [18], should also be mentioned here. Recommended monographs, particularly on the use of the Kubelka-Munk theory, are those of Kortçm [19] (in German) and Judd [20]. Experimental applications of the many-flux theories have been described by only a few authors, for example Pauli and Eitle [21], [22], who applied a three-flux theory to color formulation problems. Chapter 6 will give a account of the results obtained by Mudgett and Richards [17] and by Atkins and Billmeyer [23]. The first equations for the hiding power based on scattering and absorption coefficients for diffuse irradiation were included by Kubelka and Munk in their renowned work [7]. In present-day terms, they used the lightness contrast ratio as hiding criterion; as it then turned out, however, this criterion is applicable only to achromatic layers. Standardized methods for the achromatic case were accordingly worked out in the 1950s and 60s and have been used since that time. Not until the advent of the CIELAB system could the desire for more suitable hiding criteria be made possible a comfulfilled. First, in 1981, the introduction of the criterion DEab putational procedure for achromatic layers based on the Kubelka-Munk theory [24]; this duly led to a standard. At the same time, the first description was given of how gloss could be handled in color matching and how the scattering and absorption components of the hiding power could be calculated. It had already been shown that the determination of hiding power from R?, Rs is more accurate than the determination from Rb , R0b , Rw, R0w [25]. A pneumatic apparatus for measuring film thickness was developed by Kåmpf [26] for use in the determination of scattering coefficients, absorption coefficients, hiding power, and transparency. Economic aspects of the hiding power were analyzed by Keifer [27]; these will be taken up in Section 7.4.4. Not until 1964, however, was the principle of spectral evaluation [28], [29] applied in order to make the Kubelka-Munk theory applicable to colored layers. The first procedure used was a graphical one, with the lightness as hiding criterion. Gall [30] then showed how the principle could be rationally applied (by computer

3.9 Historical and Bibliographical Notes

129

programming) when other criteria (color difference) were used in determining the hiding power of inks and paints. Strocka [31] demonstrated that 16 chosen wavelengths (20 nm intervals) would be sufficient for most applications. The tables of Stearns [32] can be expediently employed for the CIE color matching functions (see Chapter 7 for examples). Further improvements followed [33]: iteration with Newton's method, calculation of S for smaller error of determination. On the last point, it should be remarked that the calculation of the error dS in the scattering coefficient as done in Section 3.6.1 is preferable to the computational scheme in [33] because it is simpler. With regard to transparency, the definition generally accepted today was not written until 1976 [34]. This definition provided the basis for a standardized test procedure. The same publication [34] suggested the use of the principle of spectral evaluation in order to create a rational and sufficiently accurate determination method using the Kubelka-Munk coefficients, especially when the calculation can be done in a single pass after the hiding power has been determined [33]. Reference should also be made to a report on experience with diverse methods of hiding power determination [35] and to a summary of the Kubelka-Munk theory in pigment testing [36].

References [1] [2] [3] [4] [5] [6] [7] [8] [9] [10] [11] [12] [13] [14] [15] [16] [17] [18] [19] [20] [21] [22] [23] [24]

G. G. Stokes, Proc. Roy. Soc.11 (1860) 545. A. Schuster, Astrophys. J. 21 (1905) 1. F. F. Renwick, Phot. J. 58 (1918) 140. F. F. Renwick, H. J. Channon, B. V. Storr, Proc. Roy. Soc., Ser. A., 94 (1918) 222. L. Silberstein, Phil. Mag. 4 (1927) 7. M. Gurevic, Phys. Z. 31 (1930) 753. P. Kubelka, F. Munk, Z. techn. Phys. 12 (1931) 593. J. W. Ryde, Proc. Roy. Soc., Ser. A., 131 (1931) 451. P. Kubelka, J. opt. Soc. Am. 38 (1948) 448. L. Fukshanski, J. Math. Biol. 6 (1978) 177. S. Q. Duntley, J. opt. Soc. Am. 32 (1942) 61. J. L. Saunderson, J. opt. Soc. Am. 32 (1942) 727. A. Brockes, Die Farbe 9 (1960) 53. H. G. Vælz,VI. Fatipec-Kongress Wiesbaden 1962, Kongr.-B. (Verlag Chemie, Weinheim) 98. H. G. Vælz,VII. Fatipec-Kongress Vichy 1964, Kongr.-B. (Verlag Chemie, Weinheim) 194. J. K. Beasley, J. T. Atkins, F. W. Billmeyer, jr., Proc. II. Interdisc. Conf. Electromagnet. Scatt. 1967, Congress B. (Gordon & Breach, New York) 765. P. S. Mudgett, L. W. Richards, Appl. Opt. 10 (1971) 1485. S. Chandrasekhar, Radiative Transfer, Clarendon Press, Oxford, 1950. G. Kortçm, Reflexionsspektroskopie, Springer, New York, 1969. D. B. Judd, Color in Business, Science and Industry, 2. Edit., J. Wiley & Sons, New York, 1969. H. Pauli, D. Eitle, 2. AIC-Congress York 1973, Congress B. (A. Hilger, London) 423. D. Eitle, H. Pauli, XIV. Fatipec-Congress, Budapest 1978, Congress B. 209. J. T. Atkins, F. W. Billmeyer, Color. Eng. 6 Nr. 3 (1968) 40. H. G. Vælz, Die Farbe 29 (1981) 297.

130

3 How Spectra Depend on the Scattering and Absorption of Light

[25] H. G. Vælz, Die Farbe 19 (1970) 231. [26] G. Kåmpf, H. G. Vælz, farbe + lack 77 (1981) 629. [27] S. Keifer, Deckvermægen in BAYER-Ringbuch ¹Anorganische Pigmente fçr Anstrich- und Beschichtungsstoffeª, Leverkusen 1973. [28] H. G. Vælz,VII. Fatipec-Congress Vichy 1964, Congress B. (Verlag Chemie, Weinheim) 366. [29] H. G. Vælz, farbe + lack 71 (1965) 725. [30] L. Gali, farbe + lack 72 (1966) 955 and 1973. [31] D. Strocka, 2. AIC-Congress,York 1973, Congress B. (A. Hilger, London) 453. [32] E. I. Stearns, Rev. Ind. Management Text. Sci. 14 (1975) 1. [33] H. G. Vælz, Progr. Org. Coat. 15 (1987) 99. [34] H. G. Vælz, Dtsch. Farb. Z. 30 (1976) 392 and 454. [35] M. Cremer, farbe + lack 90 (1984) 548. [36] H. G. Vælz, Progr. Org. Coat. 13 (1985) 153.

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

4

How Light Scattering and Absorption Depend on the Content of Coloring Material (Beer's Law, Scattering Interaction)

4.1

Introduction

4.1.1 Description and Significance of the Concentration Dependence The complex of ideas to be discussed next occupies a position that is not just central in the interlinked system of fundamental theories (Chapter 1) but is also very significant in practice. Now that we have become aquainted with the absorption and scattering of light as the root cause of the spectral distribution, we must ask how the concentration of dyes or pigments affects scattering and absorption and thus, ultimately, spectra. The link with practical concerns can be understood immediately because this topic relates to all aspects of producing color recipes: not just formulation, but also correction of rematching. The manipulation of pigment concentrations is the formulating colorist's most vital tool. In addition to the concentration dependences of absorption and scattering, however, this chapter also deals with that of the Kubelka-Munk function, especially with regard to special pigment mixtures such as those with white and black pastes. These are particularly relevant to colorimetric pigment testing, because they form the basis for determining the tinting strength and lightening power. The last two concepts will be taken up in the pertinent sections; here it should be noted that the tests are often used for incoming inspection of coloring materials, since they can be performed in a relatively short time. Colorimetric tests of coloring material generally presuppose that dyes are dissolved and pigments are dispersed in a medium. The resulting pigment dispersion should contain the pigments in homogeneously distributed form (optimally dispersed); ªdispersionº as the term is used in colloid chemistry must therefore be dealt with first, and this means providing some essential information about particle size. A section on measures of pigment content then follows.

132

4 How Light Scattering and Absorption Depend on the Content ¼

4.1.2 Pigment Particle Size Along with the optical constants, the key physical features of pigments include geometrical information such as the particle size and shape. The effect of particle size on color properties was mentioned briefly in Section 1.2, which made the point that both the absorption and the scattering properties are strongly influenced by the size and distribution of pigment particles. The terminology of pigment particles will be outlined briefly here as set forth in standards.* The following terms are defined (see also Fig. 4-1): ± Particle: A delimitable unit of a pigment, which can have any form and any structure. ± Primary particle, single particle: A particle that can be identified as an entity with the help of suitable physical methods (optical or electron microscopy). In many cases, it may be a single crystal, but it may also consist of a number of crystallites that coherently scatter X-rays.

Fig. 4-1. Primary particles, aggregates, and agglomerates, after Honigmann and Stabenow. * See ªParticle-Size Analysisº in Appendix 1.

4.1 Introduction

133

± Aggregate: An intergrown combination of primary particles in surface contact with one another such that the surface area is smaller than the sum of the surface areas of the primary particles. ± Agglomerate: A combination of primary particles or aggregates in contact with one another such that the components of the agglomerate are not intergrown with one another and the total surface area is not substantially different from the sum of the individual surface areas. ± Flocculate: An agglomerate that is formed in pigment/binder systems and can be broken down again by low shear forces. The particle size denotes the geometric dimension used to characterize the spatial extent of a particle. Such measures can be ± The particle diameter, that is, the diameter in the case of spherical particles or those bounded by regular figures ± The equivalent diameter, that is, the diameter of a sphere having the same volume as the particle ± The particle surface area, that is, the external surface area (without voids) or internal surface area (including voids) of a particle ± The particle volume, that is, the effective volume (without voids) or apparent volume (including voids) ± The particle mass, that is, the mass of the particle determined by weighing Tables 4-1 and 4-2 present some information on the particle shape and most frequent diameter of pigment particles. The granulometric composition of a pigment is described by its particle-size distribution. Topics relating to this aspect will be discussed in Chapter 5.

4.1.3 Dispersing of Pigments In general, the testing of pigments requires their incorporation into a binder or a plastic material; this holds, in particular, for the color properties. The look of the dry pigment powder, as a rule, affords only a very incomplete picture of the actual color qualities. In order to gain a complete knowledge of the colorimetric properties of a pigment, one would have to work it into a multitude of coating materials* or plastics**. The impulse toward rationalization means that such tests must be limited in number. However, it is often sufficient to do tests in typical systems, those that promote pigment dispersion and allow the color quality of interest to manifest itself fully. A pigment/binder dispersion is a suspension before drying, a solid sol after drying. Accordingly, the concept and relations known from colloid chemistry apply to the description of pigment/binder systems. The dispersing of pigments and fillers in binders is a highly complex process involving subprocesses, some of which have * Standards see ªCoating materialsº in Appendix 1. ** Standards see ªEmulsion paintsº and ªThermoplasticsº in Appendix 1.

134

4 How Light Scattering and Absorption Depend on the Content ¼

Table 4-1. Particle-size properties of some inorganic pigments.

Titanium dioxide, rutile (aftertreated) Titanium dioxide, anatase (untreated) Zinc white Red iron oxide Yellow iron oxide Cadmium sulfoselenides

Particle shape

Modal diameter Dhv, mm

almost spherical almost spherical almost cubic to acicular spherical acicular cubic to spherical

0.18±0.35 0.10±0.20 0.7 ±1.0 0.1 ±0.7 0.1 60.3 to 0.2 60.8 0.2 ±0.4

Table 4-2. Particle sizes of some organic pigments. Modal diameter Dhv, mm Azo (monoazo) pigments Azo (disazo) pigments Phthalocyanines, blue Phthalocyanines, green Polycyclic pigments

0.50±0.55 0.05±0.21 0.06±0.10 0.04±0.08 0.05±0.30

to precede or follow others, some of which can overlap in time. These subprocesses can be systematized and classified under the following three heads: ± Wetting: the displacement of air from the particle surface and the formation of a layer of solvent molecules. ± Disintegration: the disruption and dissipation of agglomerates, involving energy supplied externally (i. e., by dispersing equipment). ± Stabilization: the establishment of repulsive forces between particles (e. g., through solvate shells) in order to maintain the dispersed state already achieved. These repulsive forces must be stronger than the attractive van der Waals forces, which would otherwise cause the pigment to flocculate. As a rule, the quality of dispersing has a crucial effect on the properties of the system. The color properties, in particular the full shade, tinting strength, gloss, and gloss haze, show an especially strong dependence on the state of dispersing. In system made up of various pigments, demixing can occur, and a change in the optical aspect (floating) can result. Floating can be controlled by preliminary coflocculation on the pigments with suitable wetting agents, or by the addition of thickeners. A frequent departure from ideal dispersion takes the form of flocculation. As defined by Keifer, this means any departure from statistical uniformity of the pigment distribution in the medium. Deviations from uniformity commonly result in a loss of optical and coloristic performance. Flocculation also takes in the cases where pigment particles are drawn close together by attractive forces (but do not

4.1 Introduction

135

agglomerate), and where the pigment distribution is distorted by foreign particles. In particular, this always occurs when such particles are larger than the pigment particles, and so any addition of substances having a larger particle size (e. g., fillers) is always problematic. At higher pigment contents, there is no longer any certainty that the voids between pigment particles will be completely filled by the binder. Above a given concentration (the ªcritical pigment volume concentrationº), characteristic anomalies are seen, leading to disrupted and sometimes singular behavior and thus to deterioration of the pigment properties. The color properties are also affected.

4.1.4 Measures of Pigment Content From the standpoint of colloid chemistry, a pigmented medium (lacquer, paint, plastic) is a dispersion, that is, a multiphase system. The terminology and notation originally developed for mixes-phase systems* can be applied to the quantitative description of such systems. Thus the portions of the two components in such a dispersion are described in terms of: ± the mass m (unit: g or kg) ± the volume V (unit: cm3 or L) In this book, composition-related symbols will always appear without subscripts if they refer to pigment, and with the subscript M if they refer to (unpigmented) media. The same will apply to all material constants of the pigment and of the medium, respectively. Accordingly, we define: ± the pigment mass portion (PMP) w as w

m m mM

(unit: 1)

(4.1)

(unit: g 7 cm±3)

(4.2)

± the pigment mass concentration (PMC) b as b

m V VM

± the pigment volume concentration (PVC) s as s

V V VM

* See ªMixtures, Compositonº in Appendix 1.

(unit: 1)

(4.3)

136

4 How Light Scattering and Absorption Depend on the Content ¼

The PMP and PVC are expressed as fractions, often in % (example for PVC: s = 0.0295 = 2.95 %). If the volumes in this formula are replaced by the masses m, mM and the respective densities* R, RM (unit: g cm±3), the PVC becomes: m R m w s m mM mm w m RM R

(unit: 1)

(4.3)

where m RVM mM

R RM

(unit: g)

(4.4)

is the pigment mass equivalent to the medium volume (PVM) and m

R 1 RM

w

(unit: 1)

(4.5)

is the pigment mass equivalent to the medium volume of the mass portion (PMM). For constant portions by weight of the medium, m is a constant (provided the same pigment is used); thus the pigment/medium volume ratio (PMV) defined as c

V m w s VM m m 1 s

(unit: 1)

(4.6)

is an especially convenient measure, since it can be calculated easily from m and m or from s alone. Table 4-3 lists the equations for the quantities just defined. Conversion relations for these measures are stated in matrix form in Table 4-4. If one wishes, for example, to do the conversion w ? s, one begins in the second row (w ?) and follows across to the fourth column (? s) to find equation (4.3). This book will make exclusive use of the measures described here in quantifying the pigment portions in pigmented media. Among them, the pigment volume concentration (PVC) s is the most important, because the optical pigment properties * The use of the same symbol in the standard notation for the density, R, and the spectral reflectance, R (l), is all right because there is no danger of confusion. The same holds for the symbol s, which represents both standard deviation and PVC.

137

4.1 Introduction

Table 4-3. Measures of pigment content in media, with their relationships to masses and densities of pigment and medium. R R VM RM

(4.4) Pigment mass equivalent to the medium volume (PVM)

m mM

(4.1) Pigment mass portion (PMP)

w

(4.2) Pigment mass concentration (PMC)

b R

(4.3) Pigment volume concentration (PVC)

s

m mm

(4.6) Pigment/medium volume ratio (PMV)

c

m m

m m mM m mm

Table 4-4. Conversion relations between measures of pigment content in media, equations (4.7) to (4.15). ?w

(4.7)

Pigment mass portion (PMP) w? Pigment mass concentration (PMC) b? Pigment volume concentration (PVC) s? Pigment/medium volume ratio (PMV) c? Pigment mass equivalent to the medium volume of the mass portion (PMM) m

?b w bR w m

w (4.8) w m

b

R

b

b

(4.11) s w m 1 s (4.13) w m c (4.5) m

R 1 RM

?s (4.3) w s w m

(4.6) w c m

(4.9) b s R

(4.10) b c R b

(4.12) b Rs

s

(4.14) c bR 1c

(4.15) c s 1c

w

?c

(4.6) s c 1 s

c

m m mM

(chiefly the absorption and scattering properties) are referred to volume (not weight, cross section, or surface area). As a consequence, physical quantities such as the scattering and absorption coefficients often display a linear or quasi-linear dependence on the volume fractions. Related to the PVC is the pigment volume portion (PVP, unit : 1) j; it is defined in terms of the partial volumes before mixing, in contrast to s, which is defined in terms of the volumes V and VM after mixing.

138

4 How Light Scattering and Absorption Depend on the Content ¼

This measure is less interesting as far as colorimetric test methods are concerned; in any case, j = s if there is no volume reduction in the mixing process, as in nondrying pastes. Other measures are seen occasionally, such as the pigment surface concentration (in m2/L), which states the amount of pigment particle/medium interfacial area per unit volume in the dispersion. This quantity is sometimes used with latex paints, because it provides a measure of the free surface area exposed not to the medium but to the air, which leads to increased scattering power by virtue of the higher refractive index (e. g., TiO2 in rutile form has a refractive index of 2.75 relative to air but 1.9 relative to binder). The problem arises now and again of converting volumes in finished pigment/ medium mixtures to masses, or masses to volumes. The density of the dispersion RD is needed for this purpose. If there is no volume reduction in the mixing process, the mixture density can be calculated from the components:

1 V VM m mM RD

m mM RM R w 1 w m mM R RM

(unit of R: g cm±3) (4.16)

A comparison with equation (4.5) and (4.7) shows that the mixture density is very easy to obtain if w and s or w and b are known: RD

R b Rs w m w w

(unit: g cm±3)

(4.17)

In general, it should be kept in mind that quantities expressed in other units (e. g., b in g/L) must be multiplied by the appropriate powers of ten to get them in the stated units before equations (4.1) to (4.17) are applied.

4.2

Absorption and Content of Coloring Material

4.2.1 Dyes The absorption coefficients defined in Chapter 3, k '(l) for directional irradiation and K (l) for diffuse irradiation, are not actually constants, for they are also affected by the concentration of the coloring matter used. We now inquire into the dependence on concentration.

4.2 Absorption and Content of Coloring Material

139

Absorbing substances present as molecules or ions in the solution show a strictly linear dependence of absorption on solute concentration. This statement applies to dissolved dyes as well, so that k' k@b b und K kb b

(4.18)

Here b is the concentration by mass in g/L, and the two new quantities kb@ and kb are constants for a given dye, called ªabsorption coefficients per unit mass concentrationº. If k ' and K are measured in m2/L, they have the unit m2/g. Equations (4.18) constitute Beer's law. Deviations from the behavior described are seen only when the solution departs from ideality, that is, when reactions occur between the individual solute molecules or between dye and solvent molecules. Equation (4.18) is sometimes directly combined with (3.48) to yield k@b b

1 1 ln h T

(4.19)

(where h is the layer thickness and T the transmission factor), the whole expression being referred to as the Lambert-Beer law. This is somewhat confusing, because the equation does not describe a single effect discussed by two authors, but two fundamentally separate insights into absorption phenomena in transmission measurements. Equation (4.19), however, states that for a given cell thickness h if the concentration by mass b is known then the absorption coefficient per unit mass concentration k@b can be determined by transmission measurements, and conversely if k@b is known then b can be determined. The latter technique in particular has found wide adoption, e. g., spectroscopic analytical methods.

4.2.2 Pigments If a pigmented medium is now taken in place of the dissolved dye, it seems at first glance that the ideal conditions existing in the solution are now violated. However, the total observed absorption is precisely the sum of all individual absorption contributions of the pigment particles, just as the absorption of the dye solution was the sum of all absorption contributions of the molecules or ions. For this reason Beer's law also holds rigorously for pigments up to high concentrations. Figure 4-2 clearly shows the linear dependence on PVC. The plotted measured values were obtained from the Kubelka-Munk function F = K/S; care was taken to hold the scattering coefficient S constant, since the red iron oxide pigments display scattering of the same order as the TiO2 pigments used in the white paste. As the concentration of the colored pigment was increased, it was therefore necessary to lower the concentration of the white pigment.

140

4 How Light Scattering and Absorption Depend on the Content ¼

Fig. 4-2. Absorption coefficient K for diffuse irradiation (arbitrary units) versus PVC for three red iron oxide pigments (measured at l = 550 nm).

Thus we can write k' k@ s ;

K = ks

(4.20)

for the absorption of pigments; this is again Beer's law, but with the PVC s as the pigment portion. The reason for making this change will become quite evident in the next chapter (see p. 210). The new absorption coefficients referred to the PVC thus have the unit m2/L, since PVC itself has the unit 1. An important remark should be made on the newly-defined ªreferredº coefficients. For both dissolved dyes and dispersed pigments, these coefficients can be formed out of contributions by several species. If there is no interaction between the components, multicomponent systems can be described by simply adding the individual referred coefficients, so that for n distinct pigments we have: k'

n P i1

k@i si ;

K

n P i1

ki si

(4.21)

Thus in, say, a three-component mixture, on can measure k'(l) at three different wavelengths l. If k@i of the individual components are known, three equations can be written; therefrom the concentrations of the three components in the mixture can be calculated. It is expedient to perform these measurements at wavelengths corresponding to the absorption maxima of the components or, when the absorption curves overlap greatly, in ranges that permit each component to be distinguished as clearly as possible from the others.

4.3 Scattering and Pigment Content

141

What was already said about dyes also holds for the validity of Beer's law with regard to the absorption coefficients of pigmented systems. Deviations from ideal dispersion of the pigment/binder system can again result in departures from the linear concentration dependence. The initiating factors are of the same type as in the other case but differ in significance and nomenclature. Specifically, phenomena such as flocculation and agglomeration are implicated, especially at higher pigment concentrations; anomalous effects are also seen near the critical pigment volume concentration.

4.3

Scattering and Pigment Content

4.3.1 Scattering Interaction Because scattering can occur only in the presence of pigments, dyes can now be left out of the analysis. The situation with scattering is somewhat more involved than with absorption. Beer's law, that is, the proportionality between the scattering coefficient and the pigment volume concentration, holds only for low pigment contents.* At higher PVC values, because of the smaller and smaller distances between pigment particles, a scattering interaction occurs, which can be interpreted as particles hindering each other in light scattering. In the literature, ªmultiple scatteringº and ªdependent scatteringº are distinguished by whether the hindrance is due to the same pigment particles or to others. As a result, there are departures from linearity as the measured scattering coefficient falls below the straight line. The curve passes through a maximum and then falls off more-or-less steeply (Fig. 4-3). In other words, simple summing over single-particle scattering properties, as specified by

Fig. 4-3. Scattering of light versus pigment volume concentration. * Up to ca. s ^ 10 %.

142

4 How Light Scattering and Absorption Depend on the Content ¼

Fig. 4-4. Geometry of the scattering interaction.

Beer's law, no longer works as the particles, come to be nearer together. Physically, this problem can be interpreted as the scattering of light on multiple particles, and the parallelism with other multiparticle problems in physics makes it understandable that the problem of scattering interaction cannot be solved generally. The only help that can be expected here must come from theoretical descriptions based on simplified geometrical models. We begin by considering an isodisperse collection of particles regularly distributed in a medium. ªRegularly distributedº means that all particles must have the same distance to all their nearest neighbors. This assumption leads to the arrangement taken up by the sphere centers in a closest packing of spheres. In Figure 4-4, the three-dimensional relationships are shown in a cross section. In deriving an equation to describe the scattering interaction, the quantity of interest is the ratio of the sphere diameter D to the distance R between spheres. As shown in the drawing, the ratio of the volume of the spheres (diameter D) to the volume of the closest-packed spheres (diameter R) is exactly p equal to the pigment volume concentration s divided by p 2=6, the fraction of space filled by closest-packed spheres, so that 1 3 D p s 6 1 3 p p 2 R p 6 6 from which the ratio D/R is s p p D 3 3 2 s 1:105 3 s p R If one examines the central particle in Figure 4-4, one sees immediately that the scattering interaction occurs because the light backscattered into the upper halfspace can no longer travel unhindered past the nearest neighbors. Instead, the scattered light is reduced by some fraction, here ± as a first approximation ± taken proportional to the area fraction covered by the particle. This area fraction p of the individual particle can be read directly from Figure 4-4; it is given approximately by the ratio of the cross-sectional area of the hindering spheres (diameter D) to the area of the hemisphere described by R:

4.3 Scattering and Pigment Content

143

D2 p 1 D 2 4 p 8 R 2 R2 p For closest-packed spheres, there are twelve nearest neighbors. Because only the back half-space is of interest here, six spheres must be considered, so the fraction p must be multiplied by six (giving 6p) in order to obtain a measure of the hindrance. What is more, it must be taken into account that the extent of scattering hindrance must be proportional to the area fraction but not necessarily equal to it. For example, it would certainly be better to replace the geometric cross section of the hindering spheres by the scattering contribution of the individual particle, which must be proportional to the PVC-referred scattering coefficient s (mathematically, this corresponds to multiplying by s). Further, an attenuation factor Z characteristic of the pigment can be inserted in the interaction term; the total amount by which the scattering interaction reduces totoal scattering is then represented by 6p Z s. By the last two equations for p and D/R, this expression can be rewritten as 2

(4.22)

6 p Z s g ss 3 where the abbreviated notation 3 g 4

p ! 2 3 2 3 Z p

has been used. The scattering contribution that remains after the hindrance, according to equation (4.22), is thus 1

2

g ss 3

Because Beer's law is taken to hold at small s, the scattering coefficient is given by: S ss 1

g ss

2 3

(4.23)

This relation is not affected by the fact that the next nearest (and so on) spheres contribute to the hindrance. Their effect can be described by some change in the value of the free parameter g (analogous to the Madelung factors, used in crystallographic lattice-energy calculations). The quantity s appearing for the first time in equation (4.22) is the scattering coefficient per unit PVC, which is defined (more rigorously than in the absorption case) as: dS (4.24) s ds s?0

144

4 How Light Scattering and Absorption Depend on the Content ¼

The coordinates of the maximum on the S versus s curve are obtained as follows from the condition dS /ds = 0: 3 3 2 smax 5 gs Smax

2 5

s 1 3 3 2 ssmax s 5g 5

(4.25)

The possibility of the dependent scattering when several pigments are present means that S cannot generally be expressed as a simple sum of contributions due to the various species as was done for K (eq. 4.21). A sum formulation can be used only when one of the summands dominates and the other contributions are small in comparison. In all other cases, the dependent scattering must be taken care of by adding another interaction term to the sum.

4.3.2 Experimental Test of an Empirical Formula Manipulation of equation (4.23) yields: S s 1 s

gss

2 3

(4.26)

If one makes the change of variable S / s = y and s2/3 = x, one obtains the equation of a straight line: y s ± g s2 x

(4.27)

In this way, the S versus s curve of Figure 4-3 is linearized; equation (4.27) is therefore especially well-suited to an experimental test. In order to verify the applicability of this formula, a series of lacquers with increasing pigment content was prepared. The pigment volume concentrations s lay between 0.5 % and 20 %. Several titanium dioxide pigments differing in scattering properties were used, so that the test would cover the widest possible range of properties. From each pigment, a master batch with a s of roughly 0.45 was prepared by grinding for several hours in a vibratory ball mill. Vehicle was added to thick stock to bring the PVC to the desired final value; then drawdown on black/white paper were made with an automatic Bird applicator. The procedure described in Section 7.2.1 was next followed in order to determine S values for each PVC. When the values obtained were plotted versus the PVC, the typical S versus s curves shown in Figure 4-5 resulted. An x, y plot as described by equation (4.27) was also prepared, and the optimal lines were calculated by a least-squares method. Figure 4-6 presents the results.

4.3 Scattering and Pigment Content

145

Fig. 4-5. S versus s plots for six white pigments.

Fig. 4-6. Linearization of the S versus s curves of Figure 4-5.

The measured points fall quite well on straight lines, providing statisfactory confirmation of the geometrical-empirical formula to the anticipated accuracy. From the intercepts y (0) = y0 and x| y?0 = x0, equation (4.27) gives the parameters s and g: s = y0 ;

g

1 x0 y0

(4.28)

146

4 How Light Scattering and Absorption Depend on the Content ¼

A knowledge of x0 and y0 makes it quite simple to find the coordinates of the maximum.* Equation (4.23) is of fifth degree in s1/3 and, for this reason, cannot be solved explicitly for s. We do not have to propose a graphical solution procedure here, for any desktop computer can be programmed to solve for s by an iterative method given S, g, and s. It must be stated that the simple theoretical model performs well and has been confirmed again and again to within the claimed accuracy. As required by the Kubelka-Munk theory, the relation derived here for the example of white pigments essentially describes pure scattering behavior ± regardless (in the terms of our discussion up to now) of whether absorption takes place along with the scattering. It can therefore be expected that the derived equation will also be valid for layers with colored pigments.

4.4

Systematic Treatment of Pigment/ Achromatic Paste Mixing

4.4.1 Standard Methods of Pigment/Paste Mixing The mixing of pigments with a black or white paste and the colorimetric assessment of the mixture are governed by certain laws, which can be formulated quite generally, regardless of whether the case involves black and colored pigments in a white paste or white pigments in a black paste. This general relationship has not been discussed a great deal; it is based on physical and colorimetric principles that are common to all pigment/paste mixtures. This section will propose a systematic description of mixing methods and state a conservation law for each method. Systematization is needed all the more as a large number of determination methods are employed in practice (see Chapter 8) and no overarching relationship has been seen between these. But such a generalization would seem necessary to the further rationalization of pigment testing methods. The development begins with a system (ªpasteº) that already contains a black or white pigment (ªachromatic pigmentº). The problem is to mix or grind this paste with another pigment (ªtest pigmentº) in such a way that a series of increasing or decreasing pigment volume concentrations of the test pigment are obtained. Several approaches can be taken to this problem; these can be unambiguously delimited

* Equations (4.25), (4.27), and (4.28) immediately yield xmax = 0.6 x0, ymax = 0.4 y0 . In the linearized plit, in other words, the maximum of the S versus s curve liest at 60 % of the x axis intercept and at 40 % of the y axis intercept.

4.4 Systematic Treatment of Pigment/Achromatic Paste Mixing

147

and thus distinguished. These distinctions are not always manifest in the literature, and both vagueness and wrong conclusions have sometimes resulted. Just three methods of pigment/paste mixing are of practical interest. These are, in a sense, three prototypes to which the few remaining methods can also be reduced in principle. At present, however, the three standard methods have no names. So that they can be told apart in the further discussion, the following names are therefore introduced: ± Constant volume method ± Adding pigment method ± Dilution method Every mixture of test pigment and paste is a three-component system comprising the test pigment, the achromatic pigment, and the medium. The new concepts will be explained in what follows, and characteristic features and typical conservation laws for these methods will be stated. The following terminology will be employed: ) s = PVC of test pigment in the mixture sUP = volume concentration of achromatic paste sU = PVC of achromatic pigment (sU = sUPsU0) sU0 = PVC of achromatic pigment in the achromatic paste Constant volume method. In this method, care is taken to make the PVC of the achromatic pigment equal in all mixtures. On moving to a lower PVC of the test pigment in the mixture, the reduction in pigment volume is always made up by the same volume of medium. In other words, the total volume of the mixture is held constant by adding a calculated quantity of binder (Fig. 4-7 a). The conservation law is thus sU const

(4.29)

Adding pigment method. An equal quantity of the achromatic paste is measured out every time in this method, and increasing masses of the test pigment are added to such equal-sized portions. The three-component system is reduced to a binary system in this way, and the conservation law can be drawn directly from Figure 4-7 b: s + sUP 1

(4.30)

Dilution method. The third way of preparing mixtures with decreasing PVC of the test pigment is to take an already ground mixture of pigment with achromatic paste and dilute it down by adding vehicle. Neither the PVC of the achromatic pigment nor the PVC of the test pigment is held constant. What does remain constant is the

148

4 How Light Scattering and Absorption Depend on the Content ¼

Fig. 4-7. The three standard methods of pigment /paste mixing.

ratio between the PVC values of the achromatic pigment and the test pigment (Fig. 4-7 c). Accordingly, the conservation law for the dilution method is: sU sUA const s sA

(4.31)

where subscript A identifies initial values (before dilution).

4.4.2 Importance of the Methods The adding pigment method plays a prominent role because it forms the basis for defining the tinting strength and lightening power (Section 4.6 and 4.7). Weighed quantities of the test pigment are added to equal-sized portions of an achromatic substrate until the mixture visually matches a reference mixture. When this is not done, for example when pigment/achromatic paste mixtures for tinting strength or lightening power determination are prepared by the constant volume method, the values obtained can be expected to differ from the classical values according to the adding pigment method. International standards do not consistently embody a rigorous enough treatment of this point. In view of its importance, the adding pigment

4.4 Systematic Treatment of Pigment/Achromatic Paste Mixing

149

method is also discussed very thoroughly in the subsequent analyses of tinting strength and lightening power. The other two methods have gained some importance in testing practice; this is particularly true of the constant volume method, because it alone permits the PVC of the achromatic pigment to be held constant (conservation law, equation 4.29). This point is important for the relation, derived from the Kubelka-Munk function, between F = K / S and the PVC s of the test pigment. When testing is done with white paste, the constant PVC of the white pigment means that the scattering coefficient S remains virtually unchanged in the mixtures, because the white pigment is dominant. As a result, a plot of F versus s gives a straight line, because the absorption coefficient K is linear in s up to high PVC, as was shown earlier (see Fig. 4-2). Similarly, when white pigments are tested in black paste, the constant PVC of the black pigment in the mixture means that the absorption coefficient K remains unchanged; if 1/F = S / K is plotted versus s, the curve has practically the same shape as the S versus s curve, but this is linear only for low PVC (ªBeer's law rangeº; see Fig. 4-3). The dilution method is also liked by practicians because it involves only one pigment/paste grinding operation. Here again, however, it must be kept in mind that matching of two such paste mixtures for tinting strength or lightening power may give a somewhat different result from the match obtained with the adding pigment method. Not much remains to be added about other methods for pigment/paste mixing. By analogy with the constant volume method, in which the PVC of the achromatic pigment is held constant, one might seek a method in which the PVC of the test pigment remains constant. This is possible if one adds decreasing portions of paste to equal-weight portions of the pigment, adding vehicle to make up for each decrement in paste volume. The method just described is rather uninteresting, because with s = const the PVC of the pigment under study can no longer be varied. The quantity varied is the PVC of the achromatic pigment, so that the technique is a reciprocal variant of the constant volume method with the achromatic and test pigments interchanged. The discussion implies a further possibility, if fixed paste portions and variable pigment portions are replaced by fixed pigment portions and variable paste portions added to them. A closer, examination, however, reveals that this method is not a novel one but is identical with the adding pigment method, since once again a two-component system is involved while the mass balance (conservation law eq. 4.30) is unchanged. Other methods, for instance one using no achromatic stock paste ± weighed portions of achromatic pigment, test pigment, and binder being brought together ± are likewise of little interest and so will not be discusses separately. Practical experience shows that colorimetric data for the tinting strength or lightening power can be determined with certainty only if at least the achromatic pigment is incorporated into the medium in a separate operation. What is more, such methods also lead away from the classical tinting strength match and may give rise to dubious results, e. g., the Reynolds method for lightening power, formerly much used, in which

150

4 How Light Scattering and Absorption Depend on the Content ¼

s + sU = const. Individually, such methods can be related back to one of the three prototypes; the Reynolds method is then seen to be a derivative of the adding pigment method, though not identical with is.

4.5

Kubelka-Munk Functions of Pigment/ Paste Mixture

4.5.1 General Formula The discussion in Section 4.2 and 4.3 leads directly to a formula for the KubelkaMunk function of a pigment/paste mixture if the components of K and S are known: F l

K l KF l KW SF l SW S l

(4.32)

in which subscript F refers to the colored or black pigment and W to the white pigment. At this point, it is unnecessary to include a further interaction term in the denominator to take account of dependent scattering (see Section 4.3), provided one of the two scattering contributions is small in comparison with the other. Table 4-5 compares the magnitudes of the several terms for typical pigment/paste mixtures. KF in the numerator and SW in the denominator are seen to be the dominant terms. This fact suggests that the Kubelka-Munk function might be calculated with the dominant terms (KF /SW) and the deviations taken care of by perturbation terms depending on the weaker terms KW and SF. The l dependences shown in equation (4.32) hold only for colored pigments; they can be ignored for black pigments, so that F itself becomes independent of l. From equation (4.32) it is now possible to derive the Kubelka-Munk functions for pigment/paste mixtures obtained by the three standard mixing methods, both for white pigments in black paste and for black or colored pigments in white paste. The equations of Sections 4.2 and 4.3 for the concentration dependences of K and S are used for the purpose. Aside from the scattering and absorption coefficient per unit concentration, the equations to be derived contain only the concentration of the test pigment; first and second approximations for the three standard mixing methods are obtained from them. The approximations are arrived at by expanding the Kubelka-Munk function as a power series in the test-pigment concentration and then truncating after the linear and quadratic terms, respectively. Because the later terms are much smaller than the linear term of the first approximation, they take on the character of perturba-

151

4.5 Kubelka-Munk Functions of Pigment/Paste Mixture Table 4-5. Typical values of the quantities in equation (4.32). Carbon black pigments, sb = 0.01 In black paste

Absorption coefficient referred to PVC, k, mm±1 Scattering coefficient referred to PVC, s, mm±1

*20000 10

Absorption coefficient K, mm±1 Scattering coefficient S, mm±1 Kubelka-Munk function F Reflectance (corrected) R (l)

Tested in white paste, sw = 0.2 sw =2000 mm±1

*2000 200

TiO2 pigments, sw = 0.2

Colored pigments, s = 0.05

Tested in In white white paste, paste sw = 0.2 sw =2000 mm±1 200 ¼ 20000

5

*2000

Tested in black paste, sb = 0.01 kb =20000 mm±1 *20000 *2000

10 ¼ 1000

1

200

0.1

400

400

400

2000

0.5

0.02 ¼ 2

0.002

0.5

0

0.4

0.2 ¼ 0.8

0.9

0.4

tions and can be handled as corrections to the linear leading term. The result is a advantage for the experimental determination of the perturbation coefficients: the corrections terms in perturbation calculations do not have to be very accurate, i. e., they can exhibit a relative error greater than that of the leading term without impairing the value of the correction.

4.5.2 Black Pigments Mixed with White Paste For black pigments*, by equations (4.20) and (4.23), KF l k s ; SF l s s 1

2

g s3

(4.33)

where g = gs. The Kubelka-Munk functions for the standard mixing methods are obtained by applying the conservation law for each method. Constant volume method. The conservation law in equation (4.29) is sw = const, so that by the equations (4.20) and (4.23) Kw = const and Sw = const. Substitution in equation (4.32) yields the following expression for the Kubelka-Munk function Fb,c * The following convention should always be observed: symbols with no subscript refer to the pigment being tested.

152

4 How Light Scattering and Absorption Depend on the Content ¼

(the first subscript b denotes black pigment, the c stands for the constant volume method): k s1 k s Kw Kw Kw Fb;c 2 2 s Sw s s 1 g s 3 Sw s 1 g s3 1 Sw KW /SW = FW is the Kubelka-Munk function of the white paste after the addition of medium to restore constant volume (i. e., the system without black pigment). The development in the preceding section implies that the second summand in the denominator is very small compared to 1, so that the quotient can be truncated after the second-order term to obtain: # " 2 k s s 5 s s1 1 sg s3 s2 . . . Fb;c FW Kw Sw Sw Sw Multiplying out the brackets and neglecting the terms of order higher than 2 yields: k s s 5 s k s 2 s3 sg s 1 Fb;c FW Kw Sw Sw Sw Kw Sw and, finally, the PVC-dependent Kubelka-Munk function for black pigment/white paste mixtures prepared by the constant volume method: 2 Fb;c

FW

2 cb1 s 1 cb 5 s 3 3

cb2 s

(second approximation)

(4.34)

The coefficients in this equation have the following meanings: cb1

1 k Sw

cb 5 gFW 3

cb2

s Sw

k

k FW s 1 Sw

FW Fb;PU

k Sw

s FW F g g W Fb;PU FW Fb;PU FW s (4.35)

where Fb,PU = k/s = (K / S) | s?0 is the Kubelka-Munk function of the black pigment full shade for PVC in the Beer's law range.

153

4.5 Kubelka-Munk Functions of Pigment/Paste Mixture

Similarly, the first approximation is obtained from equation (4.34) by neglecting terms in higher powers than 1 (which are always very small in comparison with 1) as well as the additive term FW (which is always very small in comparison with Fb,c): 1 Fb;c cb1 s

k s Sw

(first approximation)

(4.36)

Thus, from well-defined premises, we have rigorously derived the well-known linear dependence of the Kubelka-Munk function (first approximation) on PVC for black pigment/white paste mixtures. A far simpler way to reach the same result, of course, is to ascribe all scattering by the paste mixture to the white paste and all absorption by the mixture to the black pigment, as indicated by the right-hand expression in equation (4.36). This procedure, however, leaves it unclear what simplifications have been made and whether these are reasonable. Adding pigment method. The conservation law for this method, from equation (4.30), is s + sWP = 1 (where sWP is the volume concentration of the white paste after addition of the black pigment). The PVC of the white pigment sw in the mixture must be calculated from sWP ; the formula is sw s0w sWP

(4.37)

where s0w is the PVC of the white pigment in the white paste. By the conservation law, it follows that: KW kw sw kw s0w sWP kw s0w (1 ± s) SW

sw sw 1

2 3

h

gw sw sw s0w 1

sw s0w 1

s 1

gw s0w 1 2 3

s 1 2 s 3

2 3

gw s0w 1 1 2 s ... 9

s

2 3

i

After substitution in equation (4.32), the numerator and denominator are divided by 1 ± s; this causes the pigment/medium volume ratio c = s/(1 ± s) (PMV, eq. 4.6) to appear in the numerator and denominator. The PMV thus becomes the appropriate measure of the pigment portion for the adding pigment method, and so the remaining PVC expressions are also replaced by s = c/ (1 + c) & c (1 ± c) (eq. 4.15). Now Fb,a (subscript a for adding pigment method), once again with terms of higher order neglected, becomes Fb;a

sc 1

gc

2 3

k c kw s0w 2 3 sw s0w 1 gw s0w 1

2 c 1 3

c

1 2 c 9

154

4 How Light Scattering and Absorption Depend on the Content ¼

Here kw s0w = KWP in the numerator is the absorption coefficient of the white paste, while isolable expression sw s0w (1 ± gw s2/3 0w ) = SWP is the scattering coefficient of the white paste. The quotient KWP /SWP = FWP denotes the KubelkaMunk function of the white paste, so that Fb;a

k c1 KWP FWP 5 5 1 2 s 3 1 s gw sw s0w c3 c g SWP 3 SWP

5 sw 53 2 gw s c SWP 0w 9

Once again, the quotient expression can be truncated after the quadratic term, because all the summands after the 1 in the denominator are much smaller than 1. Thus the Kubelka-Munk function for black pigment/white paste mixtures prepared by the adding pigment method is 2 Fb;a

FWP

2 zb1 c 1 zb 5 c 3 3

zb2 c

(second approximation)

(4.38)

Rather than write exact expressions for the coefficients, we write them after dropping terms that contribute practically nothing: zb1

k SWP

s FWP FWP g 3 Fb;PU k s 2 sw 53 s s0w zb2 1 gw s SWP 3 SWP zb 5 g

(4.39)

(approximation for black pigments with high light-scattering power, with Fb,PU = k/s = (K/S) | s?0, where Fb,PU is the Kubelka-Munk function of the black pigment full shade in the Beer's law range). About the first approximation, the same statements can be made as in the case of the constant volume method, and the same conclusions drawn, but referred to the PMV: 1

Fb;a zb1 c

k SWP

c

(first approximation)

(4.40)

A comparison of these equations with equations (4.34) and (4.36) for the constant volume method shows that the expressions are completely identical (aside from the

4.5 Kubelka-Munk Functions of Pigment/Paste Mixture

155

reference to PMV), even up to equality of the coefficients (though after simplification)*. Dilution method. The conservation law here is sw /s = const = swA /sA (where the subscript A marks initial values before dilution). Accordingly, equation (4.32) can be written again with s canceled out of the numerator and denominator:

1 Fb;d

ss 1

gs

2 3

sw

" swA s 1 sA

ks kw " ssA 1

2 3

gsA

s sA

gw

#

2 3

s

2 3

swA s sA

2 # 3

swA sA

" sw swA 1

2 3

gw swA

s sA

2 # 3

k sA kw swA

To find the initial value of the Kubelka-Munk function, one stets s ? sA : 2 2 3 3 ssA 1 g sA sw swA 1 gw swA 1 FA k sA kw swA With qD = s/sA, dividing by the first equation and neglecting higher-order terms gives the Kubelka-Munk function for black pigment/white paste mixtures prepared by the dilution method: Fb;d FA

1 1

ub

2

ub qD3

ub 1

1

2 3

qD

(first approximation)

(4.41)

where qD = s/sA is the dilution ratio by volume and FA is the initial value before dilution. This formula has just one coefficient: 5

5

3 2 g ssA3 gw sw swA 3 gw swA ub ssA sw swA

(4.42)

The simplification at right is obtained because we always have swswA 4 ssA (see also Table 4-5). * Here it must be noted that Fb,c and Fb,a are nonetheless two distinct functions; Fb,c is still the KubelkaMunk function of the constant volume method, even when s is replaced by s = c/ (1 + c), and similarly for Fb,a. Likewise, FW and FWP are not the same quantities.

156

4 How Light Scattering and Absorption Depend on the Content ¼

Equation (4.41) is a ª2/3º approximation implied by the second approximation. The zero-th approximation is obtained for s ? 0, that is, infinite dilution: Fb;d ? 1 FA

ub

and is of little interest.

4.5.3 White Pigments Mixed with Black Paste By equations (4.20) and (4.23), the following hold for white pigments*: 2 KW k s ; SW ss 1 g s 3

(4.43)

where g = gs. The Kubelka-Munk functions for the standard mixing methods are once more found by imposing the conservation laws. Constant volume method. The conservation law sb = const now implies Kb = const and Sb = const. For the Kubelka-Munk function Fw,c , equation (4.32) then yields 2 3 s s 1 g s Sb 1 k s Kb Fw;c (where it is advantageous to use the reciprocal). The procedure is now similar to that in Section 4.5.2: Extraction of the Kubelka-Munk function of the black paste (after addition of medium to restore constant volume), Kb/Sb = FB ; division by the denominator; truncation after the second-order term. The result is: 1 2

Fw;c

1 cw1 s 1 FB

cw 5 s

2 3

3

cw2 s

(second approximation)

(4.44)

the PVC-dependent Kubelka-Munk function for white pigment/black paste mixtures prepared by the constant volume method. As in the preceding section, the first approximation is obtained by dropping the higher powers and the 1/FB term: 1 1 Fw;c

cw1 s

s s Kb

(first approximation)

* Quantities relating to the white pigment have no subscripts here.

(4.45)

4.5 Kubelka-Munk Functions of Pigment/Paste Mixture

157

The coefficients now have the following meanings: 1 s k s cw1 Fb Sb Kb Kb cw 5 g 3

cw2

Fb

Fb g Fw;PU

k Kb

(4.46)

where Fb = Kb /Sb and Fw,PU = k / s = (K / S) | s?0 (the Kubelka-Munk functions of, respectively, the black paste and the white pigment full shade in the Beer's law range). Equation (4.45), the first approximation of the Kubelka-Munk function for white pigment/black paste mixtures, expressed as a function of concentration, is ± like equation (4.36) ± one of the most frequently used formulas. Adding pigment method. With the conservation law sBP + s = 1 and the PVC equation for the black pigment, (4.47) sb sBP s0b where s0b is the PVC of the black pigment in the black paste, the derivation of the approximations is similar to the development in Section 4.5.2. The Kubelka-Munk function for white pigment/black paste mixtures prepared by the adding pigment method is 1 2

Fw;z

1 zw1 c 1 FBP

zw 5 c 3

2 3

zw2 c

(second approximation)

(4.48)

or, after dropping higher powers and the 1/FBP term, 1 1 Fw;z

zw1 c

s c KBP

(first approximation)

(4.49)

where the coefficients (approximate values) are s 2 s 53 s 1 gb b s0b zw1 s KBP 3 KBP zw 5 g 3

zw2

k 5 s 53 k gb b s0b s KBP 9 KBP

(4.50)

158

4 How Light Scattering and Absorption Depend on the Content ¼

(approximations for black paste pigments with low light-scattering power, such as carbon black; KBP is the absorption coefficient of the black paste). Dilution method. The conservation law for this method is sb /s = const = sbA /sA (subscript A referring to initial mixture before dilution), so a derivation similar to that in Section 4.5.2 yields the Kubelka-Munk function for white pigments in black paste: Fw;d 1 FA

2 3

uw 1

(4.51)

qD

where FA is the initial value and qD = s/sA is the dilution ratio by volume; the coefficient is 5

5

3 2 gssA3 gb sb sbA g sA3 uw ssA sb sbA

(4.52)

The simplified form at the extreme right holds because we always have ssA 4 sb sbA .

4.5.4 Colored Pigments Mixed with White Paste The l dependence of absorption and scattering has to be considered for colored pigments. The formulas can be found in Section 4.5.2, where the l-dependent quantities are identified as such. Constant volume method. From equations (4.32) to (4.36), the spectral KubelkaMunk function for colored pigments is 2

Fc l

2

FW c1 l s 1 c 5 l s 3 3

c2 l s

(second approximation)

Fc(1) (l) c1 (l) s

(first approximation)

where the coefficients (higher-order terms being dropped) are

(4.53)

(4.54)

4.5 Kubelka-Munk Functions of Pigment/Paste Mixture

c1 l

k l SW

c 5 l g l 3

c2 l

159

s l SW

FW FPU l (4.55)

With regard to the Kubelka-Munk function of colored pigments, however, there is a second aspect of great interest; the question whether Kubelka-Munk functions can be written for the CIE tristimulus values X, Y, Z. If so, there will be a appreciable benefit, for these ªbroad-bandº quantities* could be directly represented as functions of the pigment concentration. This would be wholly similar to what was done for the spectral Kubelka-Munk functions. That this can indeed be done will now be demonstrated for the CIE tristimulus value Y. We start with the l-dependent quantities of equations (4.53) to (4.55): 2 FW 3 c2 ls . . . (4.56) c1 l s 1 c 5 l s Fc l FW Fc l 1 Fc l 3 For an experimental determination of the Kubelka-Munk function to the required accuracy, the spectral reflectance R (l) of the colored pigment/white paste mixture (see Section 3.3.2 and Fig. 3-9) must lie in the range of 0.20 ^ R (l) ^ 0.75. With this restriction and except for the upper part of the range (0.55 ^ Rin ^ 0.75), equation (3.118) implies that ln F = A ± BR . Further, the additive term FW /Fc (l) is small enough compared to 1 that Fc (l) in the formula can be replaced by the first approximation F(1) c (l) = c1 (l) s. Taking logarithms on both sides of the equation leads to 2 FW ln c1 l ln s c 5 l s 3 c2 l s . . . (4.57) A BR l c1 l s 3 On both the left-hand and right-hand sides, the approximate rule ln (1 + e) & e (for small quantities) has Rbeen used. In order to get to the CIE tristimulus value Y, the colorimetric integral yN (l) ¼ dl is applied on both sides of the equation (where yN (l) denotes the CIE color matching function y (l) normalized to the CIE standard illuminant N, that is, already divided by 100). Upon integration, quantities indepenR dent of l remain constant, since yN (l) dl = 1.

* The CIE tristimulus values X, Y, Z (or the reflectometer values R'x, R'y, R'z) are not spectral values now, as required by the Kubelka-Munk theory; instead, each corresponds to a broad band of wavelengths from which it was derived.

160

4 How Light Scattering and Absorption Depend on the Content ¼

Z FW yN l dl A s c1 l R R 2 R y N l ln c1 l dl ln s s 3 y N l c 5 l dl s yN l c2 l dl . . . Y B 100

3

Here Y is the CIE tristimulus value in the interior of the paste (actually Y , but this notation has already been claimed by the value function in the CIELAB system). The three integrals onR the right-hand side are now written by turns as ln c1, c5/3, c2. Now 1/c1 = exp (± yN (l) 7 ln c1 (l) dl); because exp (±ln x) = 1/x, an obvious substitution for the remaining integral on the left is Z y N l 1 dl e c1 l c1 where e is a perturbation term. If this expression is substituted in the equation, the resulting term eFw /s will certainly be small of higher order than the already very small term Fw /(c1 s) and thus can be neglected. Then A

B

Y 100

FW 2 ln c1 ln s c 53 s 3 c1 s

c2 s

A comparison with equation (4.57) reveals full agreement if the following substitutions are made: R (l) by Y /100, c1 (l) by c1, c5/3 (l) by c5/3, and c2 (l) by c2. It is thus possible to go back through the steps from equation (4.57) to (4.56) in reverse order. An equation like (4.56) with the above substitution is obtained. Now the same arguments can be repeated for the other two CIE tristimulus values X and Z in order to obtain similar formulas. Listing all three equations together, we then have the Kubelka-Munk functions of the CIE tristimulus values for colored pigment/white paste mixtures prepared by the constant volume method: 2 FXc 2 FYc 2 FZc

2 FW cX1 s 1 cX 5 s 3 3 2 FW cY1 s 1 cY 5 s 3 3 2 FW cZ1 s 1 cZ 5 s 3 3

cX2 s cY2 s cZ2 s

(4.58)

(second approximation) and 1 FXc cX1 s ;

1 FYc cY1 s ;

(first approximation)

1 FZc cZ1 s

(4.59)

4.5 Kubelka-Munk Functions of Pigment/Paste Mixture

161

where the coefficients are cX1 e cY1 e

R R

x N lln c1 l dl y N lln c1 l dl

R cZ1 e zN lln c1 l dl R cX 5 x N l c 5 l dl 3 3 R cY 5 y N l c 5 l dl 3 3 R cZ 5 zN l c 5 l dl 3 3 R cX2 x N l c2 l dl R cY2 y N l c2 l dl R cZ2 zN l c2 l dl

(4.60)

xN (l), yN (l), and zN (l) being the CIE color matching functions normalized to CIE standard illuminant N. The Kubelka-Munk functions described by equations (4.58) and (4.59) are not identical to the colorimetric integral Rover F (l); in accordance with equations (4.57) ff. they are defined as F X = exp ( xN (l) 7 ln F (l) dl), etc. These are related in the following way to the CIE tristimulus values from the corrected reflectance:

F Xc

F Yc

F Zc

1

2

1

2

1

2

X Xn X 2 Xn

Y 100 Y 2 100

Z Zn Z 2 Zn

(4.61)

162

4 How Light Scattering and Absorption Depend on the Content ¼

where Xn and Zn are the CIE tristimulus values for the standard illuminant and X R x N l R l dl Xn Y R yN l R l dl 100 Z R zN l R l dl Zn

(4.62)

These results complete the proof that the concentration-dependent Kubelka-Munk functions of the CIE tristimulus values can be described by the same formulas commonly used for the spectral values or black pigments (see the above argument and Section 4.5.2), provided the restriction 0.1 5 Rin(l) 5 0.55 is imposed. But this is not an onerous restriction, since in striving for accuracy one will always make certain to take quantities of paste and pigment such that Rin(l) will lie in this range. Adding pigment method. First, the spectral Kubelka-Munk function for colored pigments is 2 Fa l

FWP

2 z1 l c 1 z 5 l c 3

z2 l c

(4.63)

(first approximation)

(4.64)

3

(second approximation)

1

Fa l z1 l c

k l c SW

where the coefficients (without higher-order terms) are z1 l

k l SWP

z 5 l g l 3

FWP FPU l

s l 2 sw 53 s l s0w 1 gw z2 l s l SWP 3 SWP (approximation for colored pigments with high light-scattering power).

(4.65)

4.5 Kubelka-Munk Functions of Pigment/Paste Mixture

163

With regard to the Kubelka-Munk functions of the CIE tristimulus values for the adding pigment method, the same arguments as cited above for the constant volume method lead to similar results, the Kubelka-Munk functions of the CIE tristimulus values of colored pigment/white paste mixtures prepared by the adding pigment method: 2

F Xa 2

F Ya 2

F Za

2 FWP zX1 c 1 zX 5 c 3 3 2 FWP zY1 c 1 zY 5 c 3 3 2 FWP zZ1 c 1 zZ 5 c 3

(second approximation)

zX2 c zY2 c zZ2 c

3

(4.66)

und 1

1

F Xa zX1 c ; F Ya zY1 c ;

1

F Za zZ1 c

(4.67)

(first approximation) where the coefficients are zX1 e zY1 e

R R

x N lln z1 l dl y N lln z1 l dl

R

zZ1 e zN lln z1 l dl R zX 5 x N l z 5 l dl 3 3 R zY 5 y N l z 5 l dl 3 3 R zZ 5 zN l z 5 l dl 3 3 R zX2 x N l z2 l dl R zY2 y N l z2 l dl R zZ2 zN l z2 l dl

(4.68)

Equations (4.61) and (4.62) with appropriate substitutions hold for F Xa, FYa, and F Za.

164

4 How Light Scattering and Absorption Depend on the Content ¼

Dilution method. The spectral Kubelka-Munk function of colored pigment/white paste mixtures, similarly to equation (4.41), are u l 1

Fd l 1 FA l

2 3

qD

(4.69)

where qD = s/sA, FA (l) being the initial value before dilution, and the coefficient is 5

5

3 5 g l s l sA3 gw sw swA 3 gw swA u l s l sA sw swA

(4.70)

Now the Kubelka-Munk functions of the CIE tristimulus values will again be derived. Starting with equation (4.69), we proceed as we did before, taking logarithms to get to the proven equality ln F = A ± BR*, we once more apply the approximations for small quantities on the right-hand side: 2 3 (4.71) B R l RA l 1 qD u l R

Application of the colorimetric integral B Y 100

YA

yN (l) ¼ dl leads immediately to

1

2 3

Z

qD

y N l u l dl

and formal identity with equation (4.71). From here, the steps are repeated in reverse order, yielding the Kubelka-Munk functions of the CIE tristimulus values for colored pigment/white paste mixtures prepared by the dilution method: F Xd 1 F A;Xd F Yd 1 F A;Yd

u X 1 u Y 1

F Zd 1 u Z 1 F A;Zd (qD s/sA)

2

qD3 2 3

qD 2 3

qD

(4.72)

where F A,Xd, F A,Yd, and F A,Zd are the Kubelka-Munk functions of the initial CIE tristimulus values and the coefficients are given by

4.6 Tinting Strength

u X u Y u Z

R R R

165

2

3 x N l u l dl gw swA 2

3 y N l u l dl gw swA 2

3 zN l u l dl gw swA

(4.73)

Equations (4.61) and (4.62), suitable modified, holdF Xd ,FYd , andF Zd . Thus the concentration dependence of the Kubelka-Munk functions of CIE tristimulus values for colored pigments by the dilution method is described by the same law as for black pigments.

4.6

Tinting Strength

4.6.1 Significance and Definition Tinting strength is a fundamental characteristic of coloring materials. It describes one of the most important optical qualities of dyes and pigments in the form of an ªeffectivenessº criterion and is continually used for optical performance comparisons of pigments and dyes. The assessment of the optical performance of pigments is commonly based on the tinting strength and hiding power in a stated medium. When the price is then taken into consideration along with the optical performance, conclusions can be drawn about the economics of a pigment (ªmoney valueº; see Section 7.4.4). As a rule, however, the determination of hiding power involves appreciable experimental effort. It appears much easier to determine the tinting strength, and a first examination reveals no problems in doing so; this approach is normally preferred, even if tinting strength and hiding power do not necessarily lead to the same economic results. Tinting strength is defined as ªa measure of the ability of a coloring matter to impart color, through its absorbing power, to other substancesº*. If one understands a definition as simultaneously being an instruction, telling how to carry out a determination implied by the definition, one comes to a surprising conclusion here: current testing specifications, without exception, define (i. e., tell how to determine) only a ªrelative tinting strengthº relative to a reference coloring matter. The justified question of absolute tinting strength remains largely unanswered, and existing standards say little about it. We can only return to this interesting question further on and seek an answer to it then.

* For standards see ªTinting Strength, Relativeº in Appendix 1.

166

4 How Light Scattering and Absorption Depend on the Content ¼

The concept and definition of relative tinting strength are worded differently for dyes and pigments and at first glance they do not seem to be identical. For dyes, the relative tinting strength is the ratio of the extinction coefficients for the test and reference dyes measured at the absorption maxima of the solutions: Pd

k00b

k00b;R

(4.74)

(Because there is no scattering, the extinction coefficients are equal to the absorption coefficients per unit concentration by mass k@b .) The absorption curves for both dyes should be quite similar. In the pigment field, tinting strength applies only to black and colored pigments, and accordingly there has to exist an analog for white pigments: the ªlightening powerº. The procedural instruction (the ªstandard experimentº) based on the definition of tinting strength or lightening power runs as follows: each of the pigments to be compared is mixed into a white paste (into a black or blue paste for lightening power), and the portion of one of the two pigments is varied until the two drawdowns match, i. e., look the same to an observer. The tinting strength or lightening power is the weight ratio of reference pigments (mass mR) and test pigment (mass m) needed to achieve the same color quality in a white system or the same lightening in a colored system. Thus the defining equation for tinting strength and lightening power is P

mR m

DQ0

mFPconst

(4.75)

where DQ = 0 denotes a match and mFP is the constant portion of white or black paste. Tinting strength and lightening power describe true effectiveness properties, since a tinting strength a factor of two greater signifies that only half as much of this pigment is needed to achieve the same optical effect as with the reference pigment. It is common to supplement the notion of tinting strength with that of ªtinting equivalentº. This is the reciprocal of the tinting strength and thus tells how many parts of a test pigment will have a color-imparting effect equivalent to that of 1 part by weight of the reference pigment. Another way to explain this property is to say that the tinting equivalent is lower for more strongly coloring pigments and higher for less strongly coloring ones, corresponding to the smaller and larger portions of these pigments required. In a formulation calculation context, the tinting strength of a pigment is sometimes linked with its coloristic properties in a arbitrary pigment mixture. Thus one attempts to interpret the tinting strength as the fundamental pigment property for

4.6 Tinting Strength

167

formulation, namely as the substitution ratio when a formula is to be converted. A definition of tinting strength in this sense would not, however, be possible unless the system itself or some general principle of formulation systems were included in the definition. Even if it were, results under this definition would necessarily differ from those under the classical definition. In practice, this means that substitution ratios in general formulas need not be identical with the relative tinting strength (substitution ratio in white). It is essential to keep this point in mind when tinting strength measurements are used to answer questions in formulation calculations. Equation (4.75) provides a basis for a test specification. The standards here have retained the decades-old interpretation of the tinting strength concept as well as its definition, both of which are far older than the standards themselves. As a consequence of the definition, the test is performed in a light-scattering substrate, but for each substrate the vehicle as well as the white pigment must be specified. Today, nondrying vehicles containing a titanium dioxide pigment are common use. A method of tinting strength determination usable in practice must, of course, cover some further points, for example the test pigment concentration, because the relative tinting strength depends not only on the white pigment used and its concentration, but also on the concentration of the colored pigment in the test. The procedure ultimately used may differ in a variety of ways from the standard experiment described above. This fact may well conceal the latent presence of defining equation (4.75) and the system of the standard experiment. This holds, in particular, for photometric techniques derived from the standard experiment. In these methods, a rationalization profit is achieved because only one mixture of white paste with the test pigment need be prepared. As in the case of the hiding power, this economy is the great motivation for using colorimetric methods to determine tinting strength; but the problem of a colorimetric matching criterion arises ± the problem to be discussed now in Section 4.6.2.

4.6.2 Coloristic Matching Criteria for Pigments As has been shown, methods of determining the tinting strength for pigments specify that the reference and test mixtures with white paste are to be ªmatchedº through variation of the pigment portions; when the match is completed, they should appear alike to the colorist. Matching does not present any difficulties to the colorist when the pigments involved have very similar spectra, that is, when the differences in hue and saturation are small. When these differences are greater, criteria based on coloristic experience are applied; the uncertainty of the assessment unavoidably grows larger as the color difference increases. On the other hand, as the spectral curves become less and less similar, a point is soon reached where the determination of relative tinting strength ceases to be meaningful, because the test pigment is no longer such that it can replace the reference in a color formulation. It is thus reasonable to restrict tinting strength determinations and studies to small color differences.

168

4 How Light Scattering and Absorption Depend on the Content ¼

The question of a matching criterion to be used becomes acute (if indeed it has not done so already) when visual matching is abandoned in favor of a colorimetric method. The only way for the colorimeter, and the computer fed by it, to draw on experience comparable to that of the colorist is to render objective the criterion used by colorists. Not until the color quality that the colorist utilizes has been identified and quantified can instructions for the computer be embodied in program form. The problematic aspect of tinting strength determination can be expressed in the question: What colorimetric or physiological criterion governs the optimal replacement of reference by test pigment? There are cases in which the pigment being assessed is fully capable of replacing the reference pigment at a certain concentration; i.g., the color difference between the mixtures of the two pigments with white paste vanishes. With inorganic colored pigments and some organic pigments, however, this is the exception, because in most such cases the differences in tinting strength can mostly be attributed to differences in particle size and particle-size distribution, with the inevitable result of shifts in hue. Because these color differences between test and reference pigments do not result from differences in concentration or unequal tinting strengths, there is no concentration at which the color difference between the two will vanish. The question then arises: What criterion can be applied in order to find the mass ratio at which the reference pigment can be optimally replaced? Is the matching of absorption coefficients (of reflectances) at the absorption maximum (that is the reflection minimum) the proper criterion, as older methods suggest? Or, in the case of pigments differing in color nuance, is it better to seek the concentration such that the color difference between reference and test pigments is a minimum? The applicability test for these criteria is the agreement on the visual match among many colorists. If a working technique is specified and the portion of the test pigment is progressively increased, the resulting colors describe a three-dimensional curve in color space. This curve is called the ªtinting characteristicº of the pigment. If the method is to add a colored pigment to a white paste, say by the constant volume method, then as expected the three-dimensional curve begins near the white locus (color locus of white paste; PVC of colored pigment s = 0) and ends close to the colored pigment full shade (s 4 sw). The nature of the curve between these two points may vary greatly from one pigment to another and from one color range to another. For the CIELAB color space, the tinting characteristic for mixtures with a white preparation (ªreducing whiteº) can even be formulated analytically (though not explicitly). From the PVC-dependent reflection spectra R (l, s) of reducing whites, the CIE tristimulus values X (s), Y (s), Z (s) can be obtained, and from these the CIELAB color locus V (s) = {a (s), b (s), L (s)} can be determined. If the components of a vector depend exclusively on a single variable (s), a three-dimensional curve always exists. Figure 4-8 presents one example of a tinting characteristic for reducing whites. In Equation (4.75), the match is signified by DQ = 0. The quantity Q, the color difference between test and reference pigments, which is to be made equal to zero,

4.6 Tinting Strength

169

Fig. 4-8. Tinting characteristic of a copper phthalocyanine pigment, after a model due to Keifer. (The highest color locus corresponds to the white paste; the negative b axis points toward the observer.)

is called the ªtinting strength criterionº. The selected tinting strength criterion can usually be represented by equipotential surfaces in corlor space (see Fig. 4-9 for L* as tinting strength criterion). One of the pigments to be compared (constant portion by weight) fixes a certain equipotential surface, and the tinting characteristic of the other pigment (variable portion by weight) intersects this surface at a point. The point is the location of the match, and the pigment concentration at this point of the three-dimensional curve is the desired concentration at the match. It should be clear that the value of the tinting strength is more-or-less strongly influenced by what tinting strength criterion is chosen. Accordingly, one can no longer speak of just the ªtinting strengthº; there are as many values of tinting strength as there are tinting strength criteria in use. What follows is a survey of criteria.

170

4 How Light Scattering and Absorption Depend on the Content ¼

Fig. 4-9. Equipotential surfaces of lightness (tinting strength criterion L ) with tinting characteristic of a colored pigment in CIELAB color space.

Tinting Strength Criteria 1) Criteria definable in physiological and simultaneously colorimetric terms ± Lightness L (or CIE tristimulus value Y). This criterion does not require any further explanation. Both quantities, L and Y, lead to the identical match, since DL = 0 and DY = 0 have the same meaning. Figure 4-9 shows the CIELAB color space with equi-lightness surfaces drawn in (planes in this instance). The figure also indicates how the tinting characteristic of a colored pigment intersects the plane of the reference. ± Color depth T . The color depth is a measure of the ªcolorednessº (intensity) of a color perception.* It increases with increasing saturation, but decreases with increasing lightness. Accordingly, in the CIELAB color space, it can be approximately represented as the distance from the white locus (Lw = 100): q q 2 100 L 2 (4.76) T a2 b2 100 L 2 Cab Surfaces of constant color depth are thus spherical shells centered on the white locus, as shown in Figure 4-10. The above formula is, however, too rough for practical use. ± The smallest of the CIE tristimulus values X, Y, Z. This is the CIE tristimulus value that is most strongly governed by the absorption. ± The smallest of the reflectometer values R'x, R'y, R'z . this measure provides a simplification when measurement is done by the tristimulus method. ± Smallest possible color difference DE ab . This tinting strength criterion is already a difference, but it is to be minimized instead of made equal to zero. In the CIELAB color space, the mixture of the reference pigment with white represents a * The term originated in textile dyeing and was coined for use in fastness comparisons, which are to be done not at an equal dye concentration but at an equal ªdepthº of coloration.

4.6 Tinting Strength

171

Fig. 4-10. Equipotential surfaces for color depth (tinting strength criterion T ) with tinting characteristic of a colored pigment, plotted in the CIELAB color space.

point (color locus). On the tinting characteristic of the test pigment, the point is sought that is nearest to the reference color locus. ± Chroma difference DC ab . This criterion is of little importance but is included here to complete the systematic order. 2) Criteria derived from the Kubelka-Munk function F ± Maximum of the spectral Kubelka-Munk function Fmax (l) or minimum of the reflection spectrum Rmin (l). This is a variant of the ªsmallest CIE tristimulus valueº criterion. DFmax (l) = 0 and DRmin (l) = 0 lead to the same match; DRmin (l) is also the tinting strength criterion for dyes in solution.* ± Sum of the colorimetrically evaluated Kubelka-Munk functionsF x,y,z . This criterion is formulated as R F x;y;z x l y l z l F l dl

(4.77)

The sum of the CIE color matching functions, which is multiplied by F (l) has the form of a double-peaked curve (see Fig. 2-4) with a deep notch at 500 nm. It is not immediately obvious why the wavelengths around 500 nm are thus discriminated against in the summation. The criterion originated in the textile field and is used there for tests of dye strength (on the fiber). Recently if has been applied to the determination of the tinting strength of organic pigments (see Section 8.2.3). * Thus the definitions of tinting strength for dyes, equation (4.74), and for pigments, equation (4.75), are identical for this tinting strength criterion.

172

4 How Light Scattering and Absorption Depend on the Content ¼

± Averaged spectral Kubelka-Munk functionF. This is given by R F F l dl

(4.78)

and should take care of the objections raised in connection with the criterion F x,y,z. The integral must be formed by summation; the magnitude of dl is not crucial provided the mixtures with the test and reference pigments are formulated with the same dl. ± Smallest possible variance sum of the spectral Kubelka-Munk functions DF 2 (min), calculated as R R DF 2 min DF 2 l dl F l FR l2 dl ! min: (4.79)

4.6.3 Color Matching Studies One may naturally ask which, among these tinting strength criteria, is the ªrightº one ± or which comes closest to the coloristic match. Two studies have been published that shed some light on this problem; their results will appreciably aid in the selection of a suitable tinting strength criterion. Keifer and the author pursed the question of what criteria colorists apply to assess the tinting strength of inorganic pigments. Six pairs of inorganic pigments corresponding to the principal color directions red, yellow, blue, green, and in addition orange and black were chosen. In each pair, mixtures of the two pigments in reduction displayed a hue difference |DH ab | < 3 after matching. This procedure insured the ªreplaceabilityº of one pigment by the other in a coloration. Mixtures of the pigments with a white paint were prepared; the quantity of one pigment (ªtest pigmentº) was incremented 10 mg at a time, while the quantity of the other (ªreference pigmentº) was held constant. From each test pigment mixture and the reference pigment mixture (the same every time), side-by-side drawdowns were made with a Bird applicator; after these had dried, matching trials and color measurement were performed. Half of the evaluators were experienced colorists skilled in the determination of tinting strength of inorganic pigments; the other half were person who did not meet this qualification but who had done visual color matching before. One result can be stated immediately: The difference between the two groups was non significant. The overall result is therefore not influenced just by coloristic learning processes; it holds some universal significance. The color matchers were given the following question to answer: ªWhich drawndown seems to you to be the best match between reference and test pigments?º For the colorimetric evaluation, the following tinting strength criteria were tested in the study: L , DE ab and Rmin (l). Two forms of the color depth were used, T (eq. 4.75) and Ts according to Gall's improved color depth formula (Section 4.6.5). Figures 4-11 to 4-16 present the results in graphical form, with the various tinting strength criteria identified as in Section 4.6.2. From these graphs it is quite

4.6 Tinting Strength

173

Fig. 4-11. Comparison of tinting strength criteria with visual assessment (heavy arrow) for two red iron oxide pigments.

Fig. 4-12. Same as Figure 4-11, for two cadmium orange pigments.

Fig. 4-13. Same as Figure 4-11, for two yellow iron oxide pigments.

Fig. 4-14. Same as Figure 4-11, for two chromium oxide green pigments (both minima labeled Rmin (l)).

174

4 How Light Scattering and Absorption Depend on the Content ¼

Fig. 4-15. Same as Figure 4-11, for two ultramarine blue pigments.

Fig. 4-16. Same as Figure 4-11, for two black iron oxide pigments.

Fig. 4-17. Statistical analysis of the visual matching of chromium oxide pigments.

Fig. 4-18. Statistical analysis of the visual matching of cadmium orange pigments.

4.6 Tinting Strength

175

clear that the criterion DL = 0 gives the best agreement with the visual assessment (heavy arrow) for each of the six hues tested. The plots also show how much the tinting strength value obtained under the other criteria, which is proportional to the quantity of pigment, can diverge from the visual match. The larger deviations include those of the tinting strength criteria Rmin (l), T , and Ts. Even DE ab comes off poorly with regard to both the positions of the minima and the uncertainty (due to the weakly marked minima). To find out about the reliability of coloristic judgment, the frequency distributions for test pigment selection in color matching trials were calculated and plotted. Two of the resulting curves are presented here. For chromium oxide green (Fig. 4-17), the distribution is relatively narrow (under +1% of the tinting strength); for the more highly saturated cadmium pigment (Fig. 4-18), it is markedly broader (over +2 %). According to these results, coloristic judgment appears to be more reliable for unsaturated color in reduction. The other color matching study that needs to be discussed here is that carried out and reported by GALL, an investigation performed with great care and based on profound knowledge. It differs in several points from the Uerdingen study just described: ± Organic pigments were studied. ± Color depth was taken as the typical tinting strength criterion for the pigments in the study. ± In accordance with the objective, reducing whites were ordered by the specified levels of color depth. ± The color matchers were practiced in working with organic pigments (i. e., pigments commonly having higher color saturation). The samples comprised 18 resp. 22 pigments covering roughly the entire color circle. For every hue, there was a selection from a series of gradations in the concentration of colored pigment in reduction. A mixture (standard) made with a copper phthalocyanine pigment in reduction, adjusted to the specified textile color depth standard, was to be rematched in color depth with the other pigments. The task was as follows: ªFrom each concentration series, select a reducing white that best agrees in color depth ± with the blue standard and ± with the samples already color-matched to the standard.º The textile standards were identified, in the traditional way, with fractions of the ªstandard depth of shadeº (R. T.). the levels studied were 1/1, 1/3, 1/25, and 1/200 R. T. Mixtures with white at 1/3 R. T. made with a further 18 pigments (five red, four yellow, four green, five blue) and lying on ªhue profilesº (i. e., each having the same hue but different saturation) were also prepared and matched. The purpose of doing this was to determine the extent to which the colorist rates a decrease in saturation as an increase in tinting strength.

176

4 How Light Scattering and Absorption Depend on the Content ¼

Table 4-6 presents the matching results. The last column gives the frequency of the assessments falling in a concentration range of +10 % about the average value. It can be seen that the reliability of coloristic judgment is appreciably higher for saturated samples (i. e., the ones with higher CIE tristimulus values) than for unsaturated samles*. The table also shows that the luminance (tristimulus value Y) differs significantly between these samples, which were selected to have equal color depth; the differences are particularly marked in the case of yellow. Table 4-6. Color matching results along the 1/3 R. T. hue profile, after Gall. Color

X

Y

Z

H

Red, standard A B C D E

48.18 41.83 36.96 32.49 28.07 25.26

32.38 29.38 26.28 23.36 21.00 19.12

9.89 9.76 9.48 9.40 9.49 9.66

80 % 67 % 69 % 58 % 59 %

Green, standard A B C D

15.81 15.89 16.04 15.84 15.69

29.23 29.01 28.85 27.90 27.25

24.46 24.03 24.24 23.88 23.53

94 % 98 % 98 % 91%

Blue, standard A B C D E

17.38 16.63 16.41 15.83 15.26 13.94

20.70 19.86 19.78 19.04 18.88 18.72

63.82 60.59 57.72 55.93 50.98 45.76

98 % 96 % 92 % 86 % 78 %

Yellow, standard A B C D

62.05 58.25 56.43 54.75 50.84

64.76 61.39 59.74 57.92 53.97

15.35 15.97 15.83 15.75 15.78

88 % 85 % 78 % 64 %

These studies also included matching of the same samples by ªuneducatedº observers, who arrived at virtually the same results as experienced colorists. The goal of this investigation was the colorimetric establishment of the various color-depth levels. From the color coordinates of the experimentally determined color depths corresponding to the same level, improved formulas for color depth were obtained. The results of these two painstaking color matching studies of tinting strength may at first appear contradictory. How is it possible that one group of colorists uses * The terms ªbrilliantº, ªpureº, and ªhazyº have purposely not been applied to pigments here because they are ambiguous. Further, they appear to contain hidden value judgments.

4.6 Tinting Strength

177

lightness as the tinting strength criterion over a wide range of color depths, while the other group adjudges samples differing greatly in lightness to have the same color depth in the context of a tinting strength determination? The clear up the apparent contradiction, it is necessary to return to the assumptions and constraints in the two studies and the differences that result from them. Table 4-7 briefly sums up the key points for both studies. Different pigments were used: in one case, inorganic pigments, relatively unsaturated, mostly dark in full shade; in the other, organic pigments, relatively saturated in reduction. The inorganic pigments had smaller color differences between test and reference than did the organic pigments. Of the latter, Gall's colorists gave more reliable matches of the more saturated reductions than of the less saturated ones; it was just the other way around with the Uerdingen colorists, and in addition their judgment (because of the smaller color differences) was on the whole more reliable than that of the other group. Table 4-7. Summary of differences between the color matching studies. Study Aspect

Gall

Keifer/Vælz

Tested pigments

Organic pigments

Inorganic pigments

Generally 4 3

Generally 5 3

DE ab

test/reference in reduction after matching Colorists

Experienced in matching organic pigments inorganic pigments

Task

ªEqual color depthº

ªBest matchº

Objective

To improve color depth formulas

To identify best tinting strength criterion

Result

Improved formulas

Lightness

Reliability of judgment

Better on saturated samples than unsaturated

Better on unsaturated samples than saturated; generally much higher than in Gall's study

There would appear to be no arguing with the view that pigments in reduction giving higher saturations are well represented by the color depth as tinting strength criterion, while pigments in reduction giving lower saturations are better evaluated by the lightness as the tinting strength criterion. Another point in favor of this conclusion is that ªuneducatedº matchers in both studies came to almost the same results as experienced colorists ± which appears to prove that the assessment criteria used by the colorists cannot be purely learned ones. It must be kept in mind that the matching in Gall's study was done by colorists whose special experience, not just with organic pigments but also with the problems of formula conversion and rematching, was greater than that of the Uerdingen colorists. Accordingly, it cannot be ruled out that formulation experience influenced the formation of a ªcolor

178

4 How Light Scattering and Absorption Depend on the Content ¼

depthº judgment. This would mean that too much weight was placed on color nuance because it is commonly a serious problem in formula conversions. In turn, this leads too far in the substitution ratio direction in formulas and can lead away from the tinting strength, as was already stated in Section 4.6.1. One important point must not be neglected here: The more unsaturated the color of a pigment in reduction, in other words the nearer its color locus is to the lightness axis in color space, the closer are the two equipotential surfaces of lightness (horizontal plane) and color depth (spherical shell), which ultimately become identical on the lightness axis. Thus it has become usual to use lightness as the tinting strength criterion in evaluating inorganic pigments and color depth as the criterion for organic pigments. In the case of highly saturated yellow pigments, which scatter strongly, both criteria appear to fail; the reason may, however, be an expectation of the tester, who ordinarily uses inorganic yellow pigments less for coloring than for lightening, a function that is of course not regarded in the tinting strength evaluation. Finally, it should be asked why DE ab showed such poor performance in the Uerdingen study* when, as the smallest color difference, it should in face be the decisive criterion. It may again be that this expectation failed because of inadequacies in the CIELAB system. It has already been established that CIELAB regularly understates the lightness and overstates the saturation. A glance at any of Figures 4-11 to 4-16 will reveal what changes come about if DL is multiplied by a quite resonable factor of 4. The DL curve becomes far steeper, so that the DE ab curve is much more strongly dominated by DL ; as a consequence, the minimum of DE ab moves closer to the zero crossing of DL and also becomes more strongly marked. Thus tinting strength criterion min(DE ab ) practically coincides with DL = 0.

4.6.4 Lightness Matching In a rational method for tinting strength determination, a desirable feature would be that the value can be obtained by a simple calculation based on a single reducing white. Because measurements by the tristimulus method directly yield the measurement R'y = Y, the tinting strength criterion DL = DY = 0 indeed satisfies this wish. This section begins by deriving the equation of the relative tinting strength for the criterion Y as a function of the mass of the pigment. The fundamental equation (4.75) requires a relation between m and mR after matching to DY = 0. The Kubelka-Munk function expressed in terms of the PMV c is a suitable way to get mR as a function of m. This approach is particularly convenient, since the tinting strength criterion DY = 0 can obviously be replaced by the corrected values DY = 0 and finally by the Kubelka-Munk functions DF = 0, that is, by setting F = FR (test and reference). Unfortunately, this chain, which looks so plausible, has * According to a communication from Gall, no other known DE formula makes a suitable tinting strength criterion either.

4.6 Tinting Strength

179

a blemish in the form of a weak link. The problem lies in the step from Y = YR to Y = Y R , for R R DY Y YR y l R l RR l dl y l DR l dl 0 (4.80) does not necessarily imply that R DY Y YR y l R l RR l dl Z Z dR DR l dl y l y l DR l dl dR

(4.81)

vanishes. This becomes clear if substitution (3.11) is made for R , RR . The integral on the right would vanish identically with DY = 0 if the derivative dR /dR were constant. This also is nearly given: the factor lies between 0.4 and 2.6, and so there are contributions to the integral, but the crucial point is that these contributions, because of the Y matching performed, must have different signs in different regions of the spectrum, so that they practically cancel out. Figure 8±4 shows the spectra of two red iron oxide pigments in reduction after Y matching. The DR are positive for l = 420 to 540 nm but negative for l = 580 to 700 nm. A quantitative analysis of this example shows that DY 5 0.03 %, which is sufficiently close to zero. Though selected on purpose, this example is typical enough for reflection spectra if mixtures with white after Y matching that it can be generalized: DY** must always be small of higher order than Y and Y R as DY goes to zero. Thus, at a practical level of accuracy, there is justification for setting the two quantities equal, and there is no further obstacle to using the criterion DF = 0. The equations for the Kubelka-Munk functions in Sections 4.5.2 (black pigments) and 4.5.4 (colored pigments) have the same form and can therefore be handled together. The CIE tristimulus value Y for the adding pigment method is described by 2 (4.82) F FWP z1 c 1 z 5 c 3 z2 c 3

Here c = m/m is the volume ratio of pigment to white paste, in accordance with equation (4.6), with m given by equation (4.4): R (4.83) m m WP RWP where mWP and RWP are the mass and density of the white paste and R is the density of the test pigment. The notations F for the Kubelka-Munk function and zi for the coefficients appear in the following forms: F (2) b,a , zbi

for black pigments

F (2) Ya , zYi

for colored pigments

180

4 How Light Scattering and Absorption Depend on the Content ¼

A similar equation then describes the reduced reference pigment: FR

2

FWP zR1 cR 1 zR 5 cR3 3

where cR = mR /mR, mR mWP

zR2 cR

RR RWP

(4.84) (4.85)

and RR is the density of the reference pigment. For easily discerned reasons, the desired function mR (m), or in its place cR (c), must have a structure like that of F (c): 2 cR p0 c 1 p 2 c 3 p1 c DF0

3

After this expression is substituted in equation (4.84), coefficients can be compared with equation (4.82), since F is supposed to be equal to FR. The following are therefore obtained for the coefficients p i : z1 p0 zR1 2

p2 z5

p03 zR 5

p1 z2

p0 zR2

3

3

3

(4.86)

The fundamental equation for the tinting strength can now be written down. By equation (4.83) and (4.85), the requirement mWP = const implies that mR/m = RR /R, so that P 1

mR m

DF0 mWPconst

mR m

mWPconst

cR c

DF=0

" # 2 s 2 RR m 3 m R s 3 p0 1 p 2 p1 p1 R p0 1 p 2 R R m m s 1 s 3 3 1 (first approximation) (4.87) This is the desired equation for the relative tinting strength as a function of the quantity m or the PVC s of the test pigment. The zero-th approximation is obtained by setting higher-order terms equal to zero: P 0

RR p0 R

(zero-th approximation)

(4.88)

4.6 Tinting Strength

181

The coefficients are described again by equations (4.86). They can be experimentally determined by mixing three suitable quantities of pigment with equal quantities of white paste and matching the reference pastes or, more simply, from the Kubelka-Munk functions (4.82) and (4.84) of the test and reference pigments. In testing practice, they are always determined empirically rather than by the laborious calculation from the zi (l). Nonetheless, for the sake of completeness and to identify their source, they must be written out exactly. By equations (4.68) in Section 4.5.4 and (4.86), zY1 z e po 1 zRY1 zR1

R

y N lln zz1 l dl l R1

Z

2 3

p2 z5

p0 zR 5 FWP

p1 z2

p0 zR2

3

3

3

1 SW

Z

y N l

g l y N l FPU l

k l dl kR l

gR l p0 dl FPU;R l 2 3

Z y N l s l

p0 sR l dl

(4.89)

Here k (l), kR (l), and s (l), sR (l) are the absorption and scattering coefficients per unit PVC; g (l) and gR (l) are the attenuation coefficients of the scattering interaction. The first of each pair is for the test pigment, the second for the reference. The formulas for black pigments simplify because the l dependences and thus the integral vanish; p0 & k/kR and so forth. Equation (4.87), however, is not yet well-suited to the rational determination of tinting strength, for it requires a new determination of the pi for every new test pigment, or at least of p0 if one is working with the zero-th approximation. An approach to further rationalization is offered by the use and direct analysis of the Kubelka-Munk functions, which are quickly derived from Y measurements. For this purpose, the functions F^ (test pigment) and F^ R (reference) for equal masses m = mR = m^ are found from equations (4.82) and (4.84), and the quotient of the functions is taken. With the approximations for small quantities, neglecting higherorder terms, one then obtains 2 3 0 1 z z 5 5 ^ 2 R z z R z2 F FWP R2 3A 3 m^ 5 (4.90) 1 R 41 @ 32 f^ m^ 2 ^ z R m m FR FWP R1 R 3 m3 mR Now one forms the ratio to the tinting strength in equation (4.87) for the same ^ so that quantity m, P 1 1 f^

"

R RR

2 3

2 3

#

2 m^ 3 R m 3 RR

p0 zR 5

m^ p0 zR2 m

(4.91)

182

4 How Light Scattering and Absorption Depend on the Content ¼

It is useful to consider the effects of the two perturbation terms on the righthand side. Equation (4.65) shows that the second perturbation term (containing zR2 ) is influenced by the scattering power of the colored pigment while the first (containing zR5/3 ) is influenced only by its much slighter scattering interaction. Accordingly, the first perturbation term can be neglected; the second, on the other hand, may be appreciable in the case of strongly scattering colored pigments. What is more, it must be taken into account that the reference pigment (thus zR2 ) and the mass of pigment m^ are fixed in the practical determination of relative tinting strength, and further that p0 can be replaced by f^7R / RR when higher-order terms are neglected. Finally, then P 1 f^ 1 a f^ Here

F^ f^ F^R

1

(first approximation)

(4.92)

m^ RWP mWP RR

(4.93)

(zero-th approximation)

(4.94)

FWP FWP

;

a zR2

and P 0

F^ F^R

The coefficient a is a constant and need to be determined just once as long as the masses and the reference pigment are not changed. In addition, F^R does not have to be determined anew for every tinting strength test. The effect of the bracketed expression in equation (4.92) is that high tinting strength values are further increased while low ones are reduced. Another important point should be added. When the Kubelka-Munk functions are calculated in order to determine the relative tinting strength with equations (4.92) to (4.94), the surface-corrected CIE tristimulus values Y and Y R are to be obtained from equation (4.62). In tristimulus measurements, however, the spectral reflectances needed are not available. The Y values with the Saunderson corrections applied directly must therefore be used:

Y 100

Y 100

0:04

Y 0:36 0:6 100

(4.95)

(To distinguish these from the exact values, we use the notation Y ++.) But this direct correction has no further consequences, for in this case the chain of equalities DY = DY ++ = DF = 0 always holds rigorously.

4.6 Tinting Strength

183

The zero-th approximation in equation (4.94) is often sufficient for determining the relative tinting strength. Even for pigments with strong intrinsic scattering, it can always be employed for relative tinting strengths in the range of 80 % ^ P ^ 120 %; the difference between P(0) and fÃ due to dropping FWP is less than 0.2 %. For this reason, the zero-th approximation is suitable especially for production control, where only small departures from 100 % relative tinting strength are seen. Because of its continual use all over the world, this is the most commonly employed equation in colorimetric pigment testing. Finally, the use of lightness matching DY = DL = 0 as the tinting strength criterion makes it possible to answer the question of Section 4.6 as to the absolute tinting strength: The coloring power F introduced in Section 3.5.2 can serve this function. The coloring power was defined for the white substrate as the rate of increase in DE ab with film thickness h, beginning at h = 0, that is, at the intrinsic lightness L0w of the substrate. Because of the lightness criterion for the tinting strength, only DL matters, and so DE ab can be replaced by DL ; now, with equations (3.140), (3.155), and (3.157), the Y analog of equation (3.159), and the PVCdependent absorption coefficient K (l = s k (l) of the pigment, one gets F

uDL uh

h?0

116 116Y k Yk 3 100

R 116 4:8 R y N l K l dl 1:856 s y N l k l dl 3 100

A pigmented medium is used for the determination of coloring power, a pigment mixture with white for the determination of relative tinting strength. For the two results to be comparable, the pigment concentration must be the same in both cases. If one takes the same quantity mÃ of test pigment as in the tinting strength test, then since V 5 VM s

V V m^ VM V VM RVM

VM=VWP

In other words, the volume VM if the medium used in determining F should be equal to the volume of white paste in the tinting strength test. Then Z m^ y N l k l dl F 1:856 RVM VM=VWP (4.96) For F to be accepted as the absolute tinting strength, it must be shown that the ratio of two absolute tinting strengths (F relative to FR) gives the same relative tinting strength P obtained from equation (4.88). Since m^ and VM are fixed, R y l k l dl F RR R N (4.97) R FR y N l kR l dl

184

4 How Light Scattering and Absorption Depend on the Content ¼

On the other hand, the relative tinting strength is given to a good approximation by equations (4.88) and (4.89): Z RR RR k l 0 P p0 yN l dl (4.98) R R kR l In general, the quotient of integrals in equation (4.97) is not exactly equal to the integral of the quotient in equation (4.98). But under the assumptions taken in tinting strength determination (only small hue differences allowed, hence similar reference and sample spectra), the two expressions are always so similar that they are nearly equal up to a numerical factor close to 1. Thus if k (l) = const 7 kR (l), F / FR and P (0) come out to the same value; the same is true if k (l) and kR (l) are independent of l (black pigments). Now the coloring power defined by equation (4.96) can indeed be regarded as the absolute tinting strength, provided the quantity mM is such that VM = mM/RM = mWP /RWP = VWP . It should be noted that the absolute tinting strength has as its units not 1 but mm±1 = m2/L (see Section 3.5.2) and, as a consequence, presents itself as yet another effectiveness measure.

4.6.5 Color Depth Matching On the basis of results obtained in the color depth study that was described in Section 4.6.3, Gall was able to work out new formulas for the color depth. The T formula (eq. 4.76) had proved quite inadequate for practical use, but the color depth formulas initially taken over from the textile field also failed to reproduce the results of color matching tests. Typically, the formulas used today* span three discrete surfaces of constant color depth; if a color locus x, y, Y is specified, they give the deviation DTs from these color depth level surfaces. Once again, the surfaces are labeled with fractions, this time of the standard color depth SDS (= standard depth of shade) instead of the older standard depth R. T. Thus the standard gives formulas for DTS,1/3 , DTS,1/9 , and DTS,1/25 (using the notation B1/3 , B1/9 , and B1/25). The reference is always adjusted to the selected SDS, and the quantity mR of the reference is recorded. The test pigment mass m is varied in order to achieve a match (i. e., to make DTS = 0). The formula p (4.99) DTS;i Bi Y s ai j 10 bi gives DTS values for the several color depth levels. Here i Y

denotes the color depth level (1/3, 1/9, or 1/25 times SDS) is the CIE tristimulus value Y

* For standards see ªColor Depthº in Appendix 1.

4.6 Tinting Strength

S

185

is a measure of the saturation, equal to ten times the linear distance between the CIE color locus x, y of the test pigment and the equi-energy stimulus q (4.100) s 10 x xn 2 y yn 2

ai (j) is a factor used in evaluating the saturation measure; it depend on the hue angle j = Arctan [( y ± y0)/(x ± xo)] and, to a slight degree, on the SDS are constants: b1/3 = 29, b1/9 = 41, b1/25 = 56 bi The ai (j) are tabulated in DIN 53235 part 1 (enter the tables with i and j). The convenient formulas (third-degree polynomials) presented in Chapter 8 are preferred for computer calculation. The levels defined by these formulas are again surfaces in color space resembling spherical shells or goblets (Fig. 4-19). To gain some idea of the situation, one can calculate from the bi where these surfaces intersect the lightness axis in CIELAB color space. For DTS = s = 0, equation (4.99), gives ! b1 2 3 Y0; 1 2:92 8:41 10 3 Y0; 1 16:81 9

Y0; 1 31:36 25

Fig. 4-19. Surface of constant color depth Ts (Ts = (1/3) SDS) in the CIE system, after Gall.

The respective lightness value are L0;1=3 = 34.8, L0;1=9 = 48.0, and L0;1=25 = 62.8; thus the lightness range of interest is well spanned. For the sake of rationalization, it is desirable if the test can be performed with a single weighed quantity of pigment. Bringing DTS to zero requires an iteration. The new quantity of pigment mass to add is mi1 mi 0:9DTS

(4.101)

186

4 How Light Scattering and Absorption Depend on the Content ¼

while the m dependence of the CIE tristimulus values Y used in equation (4.99) can be obtained from equation (4.66) or (4.67); the coefficients are determined by appropriate pigment mass additions. It is still better to apply the principle of spectral evaluation immediately. The function F (l) can be obtained from equation (4.63) for individual l values; the needed coefficients zRi for the reference can then be found with one to two pigment quantities. On the other hand, the tristimulus method can also be employed. The basis for this approach comprises equations (4.66) and (4.67) for the Kubelka-Munk functions of the CIE tristimulus values X, Y, Z, or the corresponding equations for the reflectometer values R'x , R'y, R'z. The coefficients here are easily determined with two pigment quantities.

4.7

Special Problems

4.7.1 Lightening Power As defined by standards, lightening power is ªthe ability of a pigment to increase the lightness of a colored, gray, or black mediumº. The lightening power is the relative tinting strength of white pigments, and the definition accords with that of the general relative tinting strength of pigments, equation (4.75). The problem, once again, is to derive a simple relation suitable for rationalizing the procedure; the tool used, once more, is the Kubelka-Munk function. Dispersions of white pigments in black pastes yield reflection spectra virtually independent of l, so that R (l) can be treated as equal to Y/100. Thus DY = DY++ = DF = 0 rigorously. Similarly to the development in Section 4.6.4, the Kubelka-Munk functions of the test and reference pigments are written out in accordance with equation (4.48). Next, an expression is sought for the function cR (c) at matching, which leads in the end to the lightening power equation: P 1 w

" RR 1 p R w0 RR 1 p R w0

2 m 3 pw 2 m 3

pw1

s 2 3 pw 2 s 3 1

m m

pw1

#

s 1

s

(4.102)

(first approximation)

P 0 w

RR R s pw0 R R R sR

(zero-th approximation)

(4.103)

4.7 Special Problems

187

Here, similarly to equation (4.50), pwo

zw1 s zwR1 sR 2

pw 2 zw 5

3 pw0 zwR 5 g

pw1 zw2

pw0 zwR2

3

3

2

3 pw0 gR

3

1 k Kb

pw0 kR

(4.104)

Equation (4.102) has the new feature that both the second and the third terms in brackets are negative (not just the third as in eq. 4.87). Next, the Kubelka-Munk functions for the test and reference pigments are writ^ and the ratio f^w of the two is formed. In contrast ten for equal pigment quantities m, to the previous derivation, an examination of the two perturbation terms shows that the pw2/3 term must be kept because it relates to the attenuation coefficient for the scattering interaction of the white pigment. On the other hand, the intrinsic absorp^ tion of the white pigment (pw1) can be neglected. Division of P(1) w by f w leads, finally, to the equations 1 Pw

h 2 ^ fw 1 aw f^w3

where

aw zwR 5 3

i 1

R m^ BP mBP RR

(first approximation)

2 3

gR

F^wR FBP f^w F^w FBP P 0 w

F^wR F^w

R m^ BP mBP RR

(4.105)

2 3

F^w F^wR

(zero-th approximation)

(4.106)

Equation (4.106) is another formula employed very frequently in pigment testing. It should be noted that the equation for the lightening power has the reference Kubelka-Munk function in the numerator and the test function in the denominator, in other words inverted to the relative tinting strength. The zero-th approximation gives the lightening power in the Beer's law region; outside this region, the first approximation has to be used. The reason has to do with the relatively strong effect on the lightening power due to the scattering interaction. An example is shown in Figure 4-20. Equation (4.106) implies that the

188

4 How Light Scattering and Absorption Depend on the Content ¼

Fig. 4-20. Significance of lightening power.

zero-th approximation is the ratio of the scattering coefficients per unit PMV for the test pigment and reference: P 0 w

mR m

DY=0

sR s

DY=0

s sR

s=sR

s sR

m=mR

(4.107)

No account is taken of the scattering interaction. The lightening power is thus correctly represented by the ratio of scattering coefficients only in the Beer's law range, not at higher PVC. For this reason, the lightening power and the relative scattering power are identical only in the lower range; the difference between them grows larger and larger outside this range. The first approximation requires a determination of gR. An appropriate technique is the dilution method, since g can be obtained directly with equation (4.52). Chapter 8 will describe a method by which the lightening power of white pigments can be determined in a rational manner combining the adding pigment and dilution methods.

4.7.2 Color Differences after Matching The ªcolor difference after color reductionº is the color difference still present after tinting strength matching; its analog after lightening power matching is called the ªshade difference after lightening power matchingº. These are obtained by colorimetry using the CIELAB system; they can be broken down into lightness difference, chroma difference, and hue difference components in the first case, into shade strength and nature of shade in the second (see Section 2.3.3). The color difference between the reduced test and reference pigment are calculated from the CIE tristimulus values of both. The X, Y, Z of the reduced test pigment are measured directly when the tinting strength and lightening power are de-

4.7 Special Problems

189

termined (or the reflectometer values R'x , R'y, R'z , when the tristimulus method is employed); XR, YR, ZR for the reference pigment at matching, on the other hand, have to be calculated. The PMV-dependent Kubelka-Munk functions of the CIE tristimulus values, equations (4.82) and (4.48), are available for this purpose; all that is necessary is to substitute the PMV of the reference at matching, cR = mR/mR, ^ because the mass mR of reference pigment at matchin the formulas, and mR = mP ing is very easily found with fundamental equation (4.75). In the equations that follow, the needed relations will be listed for direct use in tinting strength/lightening power programs. The term with subscript 5/3 is dropped in the case of tinting strength, the term with subscript 2 in that of lightening power, because they are negligible. Thus the color difference after color reduction (tinting strength) is given by FXa;R

2

FWP zXR1 cR 1

zXR2 cR

FYa;R

2

FWP zYR1 cR 1

zYR2 cR

2

FWP zZR1 cR 1

zZR2 cR

FZa;R

(4.108)

while the shade difference after color reduction (lightening power) is 1 2

Fw;Xa;R 1 2

Fw;Ya;R 1 2

Fw;Za;R

1 zw;XR1 cR 1 FBP 1 zw;YR1 cR 1 FBP 1 zw;ZR1 cR 1 FBP

Here cR with

m^ mR P mR mR

mR mWP

2 3

zw;XR 5 cR 3

2 3

zw;YR 5 cR 3

2 3

zw;ZR 5 cR 3

(4.109)

(4.110)

RWP RR

(and also Pw in place of P). When the determination is done by the tristimulus method, the needed coefficients zRi for the reduced reference pigment are deter-

190

4 How Light Scattering and Absorption Depend on the Content ¼

mined once for all with the help of two mixtures containing different quantities of pigment. If the first approximation for the Kubelka-Munk functions is sufficient, one can set FWP = 1/FBP = 0 in the above equation and set the brackets on the right equal to 1. The Kubelka-Munk functions of the CIE tristimulus values immediately imply the (simply) corrected CIE tristimulus values of the reduced reference, in accordance with equation (3.116) or (4.61) (the subscript R is dropped in the equations that follow): X 1 FX Xn

p FX FX 2

Y 1 FY 100

p FY FY 2

Z 1 FZ Zn

p FZ FZ 2

(4.111)

and hence the uncorrected CIE tristimulus values of the reduced reference pigment, in accordance with equation (3.10):

X 0:04 Xn

Y 0:04 100

Z 0:04 Zn

X Xn X 0:6 Xn

0:384 1

Y 100 Y 0:6 100

0:384 1

Z Zn Z 0:6 Zn

0:384 1

(4.112)

Now the CIE tristimulus values X, Y, Z of the reduced test and reference pigment are known, and with the scheme of Section 2.3.3 one can calculate DE ab along with the breakdowns of color or shade difference after matching. Both quantities are strongly affected by particle size, especially in pigments with high light-scattering power. The reason for this behavior will be explained in

4.7 Special Problems

191

Chapter 5. By virtue of this relationship, the color and shade differences after matching can well be used in production control, where they serve as sensitive indicators of any departure from constancy of particle size. Because the only concern is with deviations, simplified results are also adequate here; for example, the difference between the CIE tristimulus values X and Z can be cited, or this difference related to the CIE tristimulus value Y, (Z ± X)/Y.

4.7.3 Change in Tinting Strength Section 4.1.3 treated the steps in the dispersing of pigments: wetting, disintegration, and stabilization. Now the disintegration process need to be examined more closely, since it is directly related to the final tinting strength of the pigment. When pigments are dispersed in binders, it can be observed as a general rule that the relative tinting strength increases as the dispersing effort continues. Therefore the relative tinting strength is an excellent test instrument for describing the dispersing process (ªtinting strength developmentº) and the final dispersed condition. The mathematical instrumentarium of reaction kinetics, well-known from physical chemistry, can be employed for the quantitative description of dispersing over time, since dispersing is a transformation of substances ± of larger particles to smaller ones. For the sake of simplicity, just two classes of particles are considered, the particles to be dispersed (larger) and the particles already dispersed (smaller). It is still amazing that the process of dispersing can be handled by such a simple model and that the results are in such good agreement with observation. First, some conventions: s ? is the total PVC of particles in the mill base; this does not vary during the dispersing process, s is the PVC of fine particles at time t, so that s ? ± s is the PVC of coarse particles. If the PVC is referred to the total PVC, the relative fraction of fine particles is given by n = s/s ? and that of coarse particles by 1 ± n. We now investigate the following cases: ± Size reduction of the coarse particles is due to the grinding action of the large particles themselves ± It results from grinding on the grinding medium and the walls of the grinding vessel ± It is the consequence of grinding by already dispersed (small) particles Case 1: Size reduction by large particles themselves The increase in the fraction of small particles dn over time must be proportional to the squared fraction of coarse particles (1 ± n)2. For a selected coarse particle is reduced in size faster the more coarse particles it encounters (simple proportionality); because the same thing happens with all the coarse particles, however, there must be another proportionality to the fraction of coarse particles (double proportionality): dn kg (1 ± n)2 d t

(4.113)

192

4 How Light Scattering and Absorption Depend on the Content ¼

where kg is the rate of size reduction of coarse particles by coarse particles (units min±1 or h±1). With the initial condition that the initial concentration (at t = 0) of small particles is zero (n (0) = 0), the integral of the differential equations yields 1 1 1 n kg t

(4.114)

as in the case of a second-order reaction. The rate of dispersion kg can also be expressed in terms of the half-time t 0.5 : t0:5

1 kg

(units: min or h)

(4.115)

Now the relative tinting strength can be written in accordance with equations (4.97) and (4.98), with k for the colorimetric y (l) integrals of the absorption coefficients per unit PVC. The absorption coefficient k? (corresponding to the ªfinal tinting strengthº) is taken for the reduced reference pigment. In this way, the pigment is compared with its own final dispersion; as a consequence, there is a single pigment density R = RR. If P0 = k0 / k? is the initial tinting strength, then P

s1 k k1

s k0 s k1 P0 n 1 s1 k1

P0

(4.116)

Rewriting and substitution of equation (4.114) leads to 1 P

P0

1 1

P0

1

1 1 P0 kg t

(4.117)

^ F^ ? in accordance with equation (4.94), in other words makIf now one sets P = F/ ing the relative tinting strength equal to the ratio of the Kubelka-Munk functions for equal pigments masses mÃ, and if one further neglects the (usually very small) initial tinting strength P0, one gets 1 1 1 1 ^ ^ ^ F F1 F1 kg t

(4.118)

This is the well-known Pigenot equation, which states that a straight line results if the reciprocals of the Kubelka-Munk functions for the reduced pigments are plotted versus reciprocal time over the dispersion process. As equation (4.117) shows, the linearity can be improved if the initial function F^ 0 is subtracted from F^ and F^? at the outset. The Pigenot equation holds more-or-less well for many dispersing operations, indicating that the disintegration of coarse particles on themselves is the dominant

4.7 Special Problems

193

Fig. 4-21. Dispersing curves for the size reduction of coarse particles on themselves (1) and on the grinding medium and grinding vessel walls (2). The half-time is the same for both curves, t 0.5 = 1 h.

process in dispersion. The prerequisites for this are satisfied especially in mixtures for dispersion where the pigment concentration is high or the degree of filling of the grinding vessel is high. Curve 1 in Figure 4-21 presents one dispersing curve for this form of size reduction. In the final phase, the last little bit of reduction comes about very slowly because of the declining quantity of coarse particles. Case 2: Size reduction by grinding medium and vessel walls This process corresponds to a first-order reaction, so that the increment of fine particles is simply proportional to the fractional concentration of coarse particles: dn kw (1 ± n) dt

(4.119)

where kw is the rate of size reduction of coarse particles by grinding medium and wall, with units of min±1 or h±1. With the same initial condition as above, the integral comes out to n 1 ± e±kw t The half-time is t0:5

ln 2 0:693 kw kw

(4.120)

(4.121)

with units min or h. If n (t ) is substituted in tinting strength equation (4.116), the result after simplifying and taking logarithms is ln (1 ± P) ln (1 ± P0) ± kw t

(4.122)

Thus a plot on semilog paper, with 1 ± P on the logarithmic scale versus t on the linear scale, will give a straight line.

194

4 How Light Scattering and Absorption Depend on the Content ¼

This disintegration mode dominates when the mill base has a low pigment concentration (and thus also in the final phase) or the filling of grinding medium is high. Figure 4-21 also shows a dispersion curve for this type of disintegration (curve 2). The rate constant was selected so that the same half-time t 0.5 applies to curves 1 and 2. Obviously, this disintegration process is markedly more efficient than size reduction on the particles themselves, at least in the final phase. Case 3: All forms of disintegration In addition to the two modes with which we have already become acquainted, another disintegration process is possible: size reduction of coarse particles on fine ones. While this form will play a rather minor role, it must be allowed for in the global formula. It is not worthwhile, however, to examine it in isolation as we did the other two modes, for it contributes slightly to only the middle portion of the dispersion process. The reason is that there are no small particles at the beginning of the process, while there are no large ones at the end, so that conditions for t = 0 and t = ? cannot be introduced. The increase in the content of small particles for this type of disintegration must be expressed as an interaction term between small and large particles, which is thus proportional to n (1 ± n). The differential equation for all disintegration processes is now dn [kg (1 ± n)2 + kw (1 ± n) + kk n (1 ± n)] dt

(4.123)

where kk is the rate of size reduction of coarse particles by small particles (units min±1 or h±1). With the usual initial condition, the integral is 1 A 1 Bt 1 n e

(4.124)

where A = (kw + kk)/(kg + kw), B = kw + kk, and the half-time is t0:5

1 A ln 1 A 1 B B

A 2

1 3 1 kg kw kk 2 2

(4.125)

The approximation being obtained with A 5 1. the constants A and B can be determined by iteration based on two measurements. A plot versus time does not directly give a straight line as in the previous cases, but for the initial values of n or F^ (i. e., t 5 t 0.5) the smallness of the exponent in equation (4.124) means that the Pigenot equation (4.118) holds to a good approximation. Figure 4-22 shows how n varies with t for rate constants kg = 1, kw = 0.1, and kk = 0.01 h±1.

4.7 Special Problems

195

Fig. 4-22. A dispersing curve for all types of disintegration.

In order to evaluate eq. (4.124), first the quantity n from the Kubelka-Munk functions F of the colored pigment/white paste mixtures is calculated (from eq. 4.116):

n

F F0 F1 F0

(4.126)

where F0 is the initial value and F ? is the final value. When more than two pairs of measurements are being analyzed, the problem is overdetermined, since just two parameters A and B are to be calculated. Curve fitting is done by linearizing eq. (4.124). Writing y = n/(1 ± n) and a = 1/A yields y a (eBt ± 1) The sum of squared errors to be minimized is then P

f2

P

a eBt

1

y2 ! min

Accordingly, the partial derivatives with respect to a and B must vanish. Elimination of a leads to an equation for B: Z

EE 2 E n EY Y

EET ET !0 ETY

(4.127)

where E = exp (Bti), T = ti , Y = yi , n is the number of pairs of measurements, and [ ] is the Gaussian summation symbol. The first derivative

196

4 How Light Scattering and Absorption Depend on the Content ¼

EET EY

Z0 2

ET Y

EE

2 E n ETY EY Y2

2 EETT ETT EET ET ETTY ETY ETY2

(4.128)

is also used for the iterative solution by Newton's method. Because of the danger of an overrun in the numerical memory, a starting value of about B0 = (80 ± 3 ln tn)/3tn is recommended, where tn is the largest t value occurring. The value of A is then A

EET ET ETY

(4.129)

If B becomes very small, the iteration does not converge; if the values oscillate in a very narrow range about zero, we then set B = 0. In this case, A likewise becomes very small, so that B/A = [TY]/[TT ]. For the determination of the three rate constants kg , kk , kw, eq. (4.124) offers only two quantities A, B. A third equation is found by writing eq. (4.123) with the real PVC values instead of the relative values and comparing coefficients with the original equation. The result is kg k0g s1 ;

kw k0w ;

kk k0k s1

(4.130)

that is, kg and kk are proportional to the total concentration s ? , while kw is constant. A second mill base must therefore be made with a different concentration but other conditions the same. The parameters B = kk + kw and B/A = kg + kw are determined from each of the mill bases; we then have four parameters containing the three desired quantities kg , kk , kw . Linear regressions are used (naturally, these are also recommended when there are more than two mill bases). Now (with x = s?) the following equations are formed: y1 B=A B kg kk 2 kw k0g k0k s1 2 kw ax b y2 B=A

B kg

kk k0g

k0k s1 cx

(4.131)

From each pair (or more) of equations of the y1 and y2 types, a, b, and c are obtained directly (or through linear regression), and hence k0g a c=2 ;

k0k a

c=2 ;

kw b=2

Thus the three rate constants are known for any arbitrary PVC.

(4.132)

4.8 List of Symbols Used in Formulas

4.8

List of Symbols Used in Formulas

A, B A, B, a, b, c, a a , b , L Bi = DTSi b c

c D DC ab DE ab DH ab DL DTSi E e Z Z f^ F = K/S

197

constants Variables in the change of strength CIELAB coordinates deviations from surfaces of constant standard color depth with i = 1/3, 1/9, 1/25 pigment mass concentration, PMC (g cm±3) coefficients of the PVC-dependent Kubelka-Munk function for constant volume method with subscripts: b black pigment w white pigment 1 linear term 5/3 term in 5/3 power 2 quadratic term c for colored pigments with same subscripts as c, F particle diameter, mm chroma difference (CIELAB) color difference CIELAB) hue difference CIELAB) lightness difference (CIELAB) see Bi Variable in the change of strength small quantity (e 5 1) attenuation factor of scattering interaction Function in the NEWTON iteration quantity formed from Kubelka-Munk functions with subscript: w white pigment Kubelka-Munk function without subscript: test (sample) with subscripts: a adding pigment method A initial value b black pigment in white paste B black system (constant volume method) BP black paste (adding pigment method) c constant volume method d dilution method PU full shade R reference

198

4 How Light Scattering and Absorption Depend on the Content ¼

F

F^

F (1), F (2) g = gs g h K

k kb k' k b@ k

m

m m n n = s/s ?

W white system (constant volume method) w white pigment in mixture with black paste WP white paste (adding pigment method) Kubelka-Munk function of CIE tristimulus values of colored pigments with subscripts: X,Y, Z CIE tristimulus values see also F Kubelka-Munk function for constant pigment mass m^ with subscripts: 0 initial ? final see also F first and second approximations to Kubelka-Munk function with same subscripts as F attenuation term of scattering interaction coefficient in attenuation term, mm film thickness, mm absorption coefficient for diffuse irradiation, mm±1 with subscripts: F colored or black pigment see also c absorption coefficient referred to PVC, mm±1 absorption coefficient of dye for diffuse irradiation, referred to mass concentration, m2 g±1 absorption coefficient for directional irradiation, mm±1 absorption coefficient of dye for directional irradiation, referred to mass concentration, m2 g±1 reaction rate constant, min±1 or h±1 with subscripts: g size reduction on coarse particles k size reduction on fine particles w size reduction on wall and grinding body mass, g with subscripts: M medium see also F pigment mass equivalent to the medium volume (PVM), g with same subscripts as F pigment mass equivalent to the medium volume of the mass portion (PMM) Number of measurements relative volume fraction of fine particles during dispersing process

4.8 List of Symbols Used in Formulas

P

P (0), P (1) p pi

F j j c Q qD = s/sA R R' R

R (l) R (l) S s s s

relative tinting strength with subscripts: d dye w lightening power 0 initial zero-th and first approximations to relative tinting strength with same subscripts as P are fraction of individual particle (for scattering interaction) coefficients of relative tinting strength (i = 0, 2/3, 1) with subscripts: 0 absolute term 2/3 term in 2/3 power 1 linear term ^ c see also F, F, coloring power, mm±1 = m2 L±1 with same subscripts as F pigment volume portion hue angle in CIE chromaticity diagram pigment/medium volume ratio (PMV) with same subscripts as F any color quality dilution ratio by volume diameter of closest-packed spheres, mm reflectometer value with subscripts x, y, z for the tristimulus method density, g cm±3 with subscripts: D dispersion see also F, m spectral reflectance with same subscripts as F spectral reflectance after Saunderson correction with same subscripts as F scattering coefficient, mm±1 with same subscripts as K scattering coefficient referred to PVC, mm±1 with same subscripts as c measure of saturation in the CIE system pigment volume concentration (PVC) with subscripts: 0b black pigment in black paste 0w white pigment in white paste U achromatic pigment in mixture UA achromatic pigment in mixture, initial value

199

200

4 How Light Scattering and Absorption Depend on the Content ¼

UP achromatic paste in mixture U0 achromatic pigment in achromatic paste T Variable in the change of strength transmission factor T color depth T t time, min or h with subscript: 0.5 half-time V volume, cm3 or L with same subscripts, as F, m V CIELAB color locus u coefficient of PVC-dependent Kubelka-Munk function for dilution method with same subscripts as c u u for colored pigments F with same subscripts as c, w pigment mass portion (PMP) X,Y, Z CIE tristimulus values with subscripts: n for CIE standard illuminant n see also F X ,Y , Z CIE tristimulus value of Saunderson corrected reflection spectrum with same subscripts as F X ++,Y ++, Z ++ CIE tristimulus values after Saunderson correction with same subscripts as F x, y CIE chromaticity coordinates with subscript: n CIE standard illuminant n x (l), y (l), z (l) CIE color matching functions with subscript: N normalized to CIE standard illuminant N Variables in the change of strength Y, y, y1, y2 coefficients of PMV-dependent Kubelka-Munk function for adding zi pigment method with the same subscripts as c z z for colored pigments F with same subscripts as c,

4.9 Summary

4.9

201

Summary

Particle size is one of the most important parameters of a pigment; there is no application-related property that is not affected by it. This chapter reports on the needed definitions (primary particle, agglomerate, aggregate) and the particle-size parameters. The colorimetric properties of pigments are, in practice, always tested after incorporation into a vehicle system. The preparation of the dispersion (the dispersing process) must be done with particular care. Quantitative description of concentration-related phenomena demands clear definitions of measures for the dye and pigment concentrations. The following quantities are derived from the relationships in mixed-phase systems: pigment mass portion (PMP), pigment mass concentration (PMC), pigment volume concentration (PVC), pigment mass equivalent to the medium volume (PVM), pigment mass equivalent to the medium volume of the mass portion (PMM), and pigment/medium volume ratio (PMV). The absorption and scattering coefficients of Chapter 3 are not true constants of a material, since they also depend on the concentration of coloring material. The absorption of dyes and pigments is a linear function of concentration (Beer's law). There remains a real material constant, the ªabsorption coefficient referred to concentrationº (or per unit concentration). If several coloring materials are present, the individual coefficients can generally be summed. In the case of scattering, the relationship is linear only in the initial region (up to a PVC of ca. 10 %). At higher concentrations, the scattering falls increasingly behind the linear function because of the scattering interaction between particles as they come closer and closer together. This effect is included in an earlier published equation having a term in the 2/3 power of the concentration. Experimental tests of this formula have shown good agreement with the actual behavior of the scattering curves for white pigments. The laws for mixtures of pigments with achromatic pastes are systematized by the method used to prepare the mixture. The three most important methods in practice are ± Constant volume method. The PVC of the achromatic pigment in the paste is held constant. It is used chiefly in determining scattering and absorption coefficients ± Adding pigment method. The pigment is added, in measured quantities by weight, to a constant weight of paste. This is the most important of the three methods because it forms the basis for determining the tinting strength of pigments ± Dilution method. After a mixture is prepared, it is diluted by adding more vehicle. This method plays some role in the rationalization of test procedures Each of the preparation methods is characterized by its own conservation law. The concentration-dependent Kubelka-Munk functions for pigment/achromatic paste mixtures are obtained in the following way: the equations for the three stan-

202

4 How Light Scattering and Absorption Depend on the Content ¼

dard mixing methods are derived from a generally valid formula. Application of the proper conservation law in each case yields the equations for black pigments in white paste and white pigments in black paste; separate equations are obtained for the constant volume, adding pigment, and dilution methods. The pigment/medium volume ratio is the appropriate concentration measure for the adding pigment method. The procedure is also used for colored pigment whose spectral KubelkaMunk functions are to be derived. Then it is shown that similar approximate formulas can also be obtained for broad-band spectral distributions, and thus for the CIE tristimulus values. These are of great practical importance when tristimulus instruments are employed. In summary, the equations are all similar except for having different coefficients. Typical for these relations is that the Kubelka-Munk functions are linear in the concentration to a first approximation, while in the second approximation there are perturbation terms in the 5/3 and 2 powers respectively. The tinting strength describes one of the most important optical qualities of coloring materials. It is a measure of the ability to impart color to other substances through absorption. All testing methods give the relative tinting strength, that is, the absorbing power relative to another pigment or dye. In the case of dyes, the relative tinting strength is also logically defined as a relative absorption; for pigments, on the other hand, the definition is plainly a measure of effectiveness, stating the mass ratio of test and reference pigments such that mixtures of the pigments with white paste appear alike. The lightening power (the tinting strength of white pigments) is based on scattering and is determined in black pastes. ± The ªstandard experimentº of tinting strength determination thus consists in matching one pigment to the other in reduction by varying the mass of one pigment added. In matching, which means causing the mixtures to look alike or have the same color, the matching criterion plays a key role. An indispensable step in rationalizing computer-aided methods is to establish the tinting strength criterion. Any such criterion can be thought of as a set of equipotential surfaces in color space, which are intersected by the ªtinting characteristicº (a curve connecting the color loci of mixtures obtained by adding larger and larger amounts of colored pigment to a white paste). Among the tinting strength criteria in use, two are of special significance: the lightness L (or CIE tristimulus value Y) and the color depth. Two color matching studies reported in the literature are consulted in order to establish what tinting strength criteria are preferred by colorists. In one of the studies (on inorganic pigments only), the question to be answered was this: which of the added pigment quantities produces the best match? A comparison with colorimetric data gave the unambiguous answer that the CIELAB lightness L (or CIE tristimulus value Y) is the crucial tinting strength criterion. In the second study (primarily on organic pigments), the one sample was to be chosen that best agreed in color depth with the reference pigment and, simultaneously, with the other samples already selected, right around the color circle. This study resulted in improved formulas for calculating color depth values. Because the inorganic pigments in the first case were nearly all of a dark and not highly saturated full shade, while in the second case the pigments used were more highly saturated,

4.9 Summary

203

current practice is as follows: the lightness criterion is used for inorganic pigments, the color depth criterion for organic ones. There follows a complete derivation of the tinting strength equation expressed as a dependence on pigment concentration for the lightness matching case. As a result of the development, it is found that Y matching is virtually identical with matching based on the Saunderson-corrected Y values, and that this correction can be applied directly to the CIE tristimulus values. Finally, it is shown that the coloring power defined in Chapter 3 can be regarded as an absolute tinting strength. Because the color depth formulas taken over from the textile field were not accurate enough, the studies were utilized in improving these formulas as applied to pigments. To rationalize the determination of tinting strength based on color depth matching, the required mass of the test pigment must be determined by an iterative method; the principle of spectral evaluation is well-suited to this purpose. In the case of lightening power, the white-pigment analog of the relative tinting strength, the Kubelka-Munk function again serves as a tool for rationalization. the needed equations for the lightening power as a function of PVC are derived in a similar way to the tinting strength equations. The zero-th approximation of this equation provides a good description of the behavior in the Beer's law region; at higher pigment concentrations, the first approximation with the perturbation term must be employed. The color difference that remains after matching is called the ªcolor difference after color reductionº in the case of tinting strength and the ªshade difference after lightening power matchingº in the case of lightening power. The CIELAB coordinates are accessible from the CIE tristimulus values (calculated for the pigment mass at matching), and from these in turn the color differences between sample and reference can be obtained. For white pigments, the shade difference after lightening power matching is a particularly suitable tool for the quantitative characterization of the pigment particle size. In the dispersing process, the disintegration of pigment agglomerates is crucial to the quality of the resulting dispersion. It is shown how a quantitative description of the dispersing process can be arrived at with the equations of reaction kinetics. For example: ± The size reduction of large particles on large particles is a second-order reaction and can immediately be described by the well-known PIGENOT equation, which is suitable for linearizing the measured values. ± Size reduction on the vessel wall and grinding medium is described by a first-order reaction equation. ± Size reduction by all mechanisms includes disintegration on small particles already produced. In all three cases, the half-time can be used to characterize the rate of dispersion.

204

4 How Light Scattering and Absorption Depend on the Content ¼

4.10 Historical and Bibliographical Notes Even before Kåmpf's thorough work in 1965 [1], there was a large specialist literature dealing with the effect of particle size on pigment properties (see the bibliography in [1]). The particle-size concepts defined in Section 4.1.1 correspond to the classification of pigment proposed in 1963 by Honigmann and Stabenow [2], which has gained international adoption and has been set forth in standards. As the existence of several ªmean diametersº and other size measures shows, special care is needed when using the term ªparticle sizeº [1±4]. Keifer [5] and Kaluza [6] have worked on problems of flocculation. Next to the production of the individual components, the most important operation in the manufacture of lacquers and paints is the dispersing process, and numerous publications have dealt with this topic (see bibliography in Kaluza [7]). work by von Pigenot [8] on the tinting strength development as a second-order reaction dates from the early 1960s; This line has been followed up by many other authors [9±13], who also considered the first-order reaction. The linear dependence of absorption on dye concentration was discovered by Beer (1825±63) [14], whose work came long after Lambert's law was derived (see Section 3.7). The application of Beer's law to light scattering by pigments did not happen until our century; it was contained, for example, in the first edition of Judd's well-known book [15]. Perturbation terms for the intrinsic scattering of the white or colored pigment being tested, in the form of quadratic terms [16], were initially used for formulation and rematching problems [17]; the first publication of the s2/3 perturbation term was in 1967 [18]. The quasilinear concentration dependence of the Kubelka-Munk function (Chapter 4) is valid over a much broader concentration range than is a logarithmic dependence as suggested by von Pigenot [8]. It is no longer possible to tell when the consensus was reached that the relative tinting strength of pigments should be determined as the ratio of portions by weight added to a white substrate. An early indication is found in a 1932 paper [19]. For the Kubelka-Munk function of reduced black pigments, the famous work of the discoverers (see Section 3.9) already gives a linear dependence on the black pigment concentration (first approximation; see Section 4.5.2). The ratio of the test and reference Kubelka-Munk functions for equal pigment masses, which is easily derived from their remark, is identical to the zero-th approximation for the tinting strength of black pigments, derived in Chapter 4. For colored pigments, the tinting strength criterion is important. The color matching studies discussed in Chapter 4 were performed by Gall [20] and Keifer/Vælz [21]. Gall's publication derives the new color depth equations based on Raabe and Koch's earlier equations for dyed textiles [22]. A table of a (j) factors, needed for computer calculations of color depth shades, appeared later [23]. A rational determination of the tinting strength of colored pigments, based on the principle of spectral evaluation (Section 3.6) and thus suitable for any arbitrary tinting strength criterion, was also developed by Gall [24]. Schmelzer and co-workers have also proposed doing the matching for B = 0 [25].

4.10 Historical and Bibliographical Notes

205

The methods formerly used for lightening power have today been largely forgotten, for the most part with good reason (e. g., the Reynolds method [26]). This does not apply to the procedure of Grassmann and Clausen [27], which uses the fact that the functions log F (R) and F (1/m) have linear shapes over wide range (see Section 3.3.1 and 4.5.3 respectively), so that a straight calibration line is possible. This means that a graphical technique [28] can be used; despite being restricted to the Beer's law region, this technique produced good results in many laboratories before the introduction of computers. Another advance is Keifer's graphical method [29], in which the level of pigmentation is varied and the relative scattering power and shade can be determined simultaneously with the lightening power; this method has been incorporated into standards. A rationalized method for determining the lightening power, suitable for use in present-day laboratories, is described in Chapter 8 [30]. It is based on the equations of Section 4.7.1 for Pw as a function of m. A comprehensive summary of solved and unsolved problems from Chapter 1±4 should also be mentioned [31]. On the determination of dye concentrations, see [32]. For the change in strength, a method was proposed [33, 34] by which the three governing rate constants can be determined by a reaction-kinetic method; disintegration of large particles by grinding action on ± The large particles themselves ± Grinding bodies and the walls of the grinding vessel ± Already dispersed small particles An Example is described in Chapter 8.

References [1] G. Kåmpf, farbe + lack 7 (1965) 353. [2] B. Honigmann, J. Stabenow,VI. Fatipec-Congress Wiesbaden 1962, Congress-B., 89,Verlag Chemie Weinheim. [3] K. Leschonski, Particle Size Analysis and Characterization of a Classification Process, in Ullmann's Encyclopedia of Industrial Chemistry, Vol. B2, 5th edit. 1988, VCH Verlagsgesellschaft Weinheim. [4] T. Allen, Particle Size measurement, 3. Ed. 1981, Chapman & Hall, London/New York. [5] S. Keifer, farbe + lack 79 (1973) 1161. [6] U. Kaluza, farbe + lack 80 (1974) 404. [7] U. Kaluza, Physikalische Grundlagen der Pigmentverarbeitung fçr Lacke und Druckfarben, Edition Lack und Chemie E. Moeller, Filderstadt 1980. [8] D. v. Pigenot,VII. Fatipec-Congress Vichy 1964, Congress B. 249,Verlag Chemie Weinheim. [9] O. J. Schmitz, R. Kroker, P. Pluhar, farbe + lack 79 (1973) 733. [10] U. Zorll, farbe + lack 80 (1974) 17. [11] A. Klaeren, H. G. Vælz, farbe + lack 81 (1975) 709. [12] L. Gall, U. Kaluza, defazet 29 (1975) 102. [13] U. Kaluza, XII. Fatipec-Congress G.-Partenkirchen 1974, Congress B. 233, Verlag Chemie Weinheim.

206 [14] [15] [16] [19] [18] [19] [20] [21] [22] [23] [24] [25] [26] [27] [28] [29] [30] [31] [32] [33] [34]

4 How Light Scattering and Absorption Depend on the Content ¼ A. Beer, Grundriû des photometrischen Kalkçls, Braunschweig 1854. D. B. Judd, Color in business, science and industry, 1952, J. Wiley & Sons, New York. F. Vial, XII. Fatipec-Congr. G.-Partenkirchen 1974, Congr. B. 159. L. Gall, II. AIC-Congress York 1973, Congr. B. 153, A. Hilger, London. H. G. Vælz, Ber. Bunsen-Ges. phys. Chem. 71 (1967) 326. Anonym, Off. Digest Fed. Paint & Varnish Prod. Clubs (1932) 1029. L. Gall, I. AIC-Congress Stockholm 1969, Congr. B. Vol. I, F 6. S. Keifer, H. G. Vælz, farbe + lack 83 (1977) 180 und 278. P. Rabe, O. Koch, Melliand Textilber. 38 (1957) 173. L. Gall, K. Friedrichsen, Defazet 28 (1974) 158. L. Gall, IX. Fatipec-Congress Brçssel 1969, Congr. B. Sec. I, S. 34,Verlag Chim. d. peintures. G. Geiûler, H. Schmelzer, W. Mçller-Kaul, farbe + lack 84 (1978) 139. H. A. Gardner, G. G. Sward, Paint testing manual, 12. Ed., 1962, S. 53, Gardner Lab. Inc., Bethseda (Maryland). W. Graûmann, H. Clausen, Deutsche Farben-Z. 7 (1953) 211. W. Jaenicke, Z. Elektrochem. 60 (1956) 163. S. Keifer, farbe + lack 82 (1976) 811. H. G. Vælz, farbe + lack 88 (1982) 356. H. G. Vælz, Die Farbe 25 (1976) 147. G. Booth, H. Zollinger, K. McLaren, W. G. Sharples, Alan Westwell, Dyes, General Survey, in Ullmann's Encyclopedia of Industrial Chemistry,Vol. 9, 5th edit., 1987,VCH Verlagsgesellschaft Weinheim, p. 73. H. G. Vælz, Prog. Org. Coat. 18 (1990), 289. H. G. Vælz, Prog. Org. Coat. 33 (1998), 101.

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

5

How Light Scattering and Absorption Depend on the Physics of the Pigment Particle (Corpuscular Theory)

5.1

Introduction

5.1.1 Description and Significance of the Corpuscular Theory The term ªcorpuscular theoryº refers to model concepts that form a bridge between the Kubelka-Munk coefficients and two physical optical constants of the pigment particle, the refractive index and the absorption index. The development is centered on the theory of Mie, which links the physical constants, including particle size, with the scattering and absorption properties of the particle. With this theory, we complete the progression discussed in Chapter 1, finally getting from color back to the physics. Chapter 3 briefly outlined what differentiates the Mie theory from the phenomenological theory, which also makes statements about scattering and absorption. Following up what was stated there, one can say in simple language that while the phenomenological theory knows about material properties but not about particles, the Mie theory knows about the particle ± but just one particle. The step from here to ensemble and on to the material constants will involve other models of corpuscular theory. It is obvious why the corpuscular theory is of no importance for dye testing, since there are no discrete particles in dye solutions. In fact, however, it is possible to get along without this theory in pigment testing too, at least as far as direct application is concerned. If it is used here anyway ± if it must be used ± the reason lies in the unique insights permitted by Mie calculations of pigments. These are important for understanding circumstances, properties, and processes having to do with the optics of pigments. Only with its help can we understand why white pigments scatter differently or why otherwise identical colored pigments can exhibit different hues if they differ in particle size. This causal link between color properties and particle size means that methods utilizing the Mie theory are also interesting for the determination of particle sizes and particle-size distributions. Such methods, however, are not colorimetric but purely spectroscopic; they are based on the spectrum alone and therefore were not supposed to be discussed in this book. On the other hand, the scope of these meth-

208

5 How Light Scattering and Absorption Depend on the Physics

ods has grown so broad that a description of them could easily fill another book. All the same, the context of this chapter demands a short exposition of particle-size distributions, since the distributions are needed in order to establish the link between the Mie theory and the scattering and absorption coefficients. We will limit ourselves to explaining the basic terms, also leaving out the methods of determination, which can be found discussed in the extensive specialist literature. Similarly, determination methods for the physical-optical constants can be dealt with only in a cursory and decidedly nonexhaustive way ± so that there will be an opportunity to take up the proper subject, colorimetric test methods for coloring materials, and handle it comprehensively.

5.1.2 Particle-Size Distribution The discussion in this section bears a direct relationship to the descriptions and definitions of Section 4.1.1; we will continue to use the standardized terminology*. The particle-size distribution comes from the statistical analysis of the particle sizes in an ensemble (population). Pigments are manufactured on an industrial high-tonnage basis and thus are never monodisperse. The distribution of a particlesize parameter (chiefly the equivalent diameter) can be described in terms of a particle-size distribution curve. These curves generally depend strongly on the type of dispersing medium, the degree of dispersing, and the method of determination. The wetting power and polarity of the medium, the dispersing work done to disintegrate agglomerates, the tendency to reagglomeration, and other factors play significant roles. For these reasons, the particlesize distribution in most cases must be determined in a different way for each application. Statistical frequencies of the particle-size parameters defined in Section 4.1.1 (particle diameter, equivalent diameter, particle surface area, particle volume, particle mass and also the number of particles) are plotted versus the parameter of interest or some other one. A preferred type of plot for pigments is the ªvolume/diameter distributionº, the function u (D) obtained when the volume frequency is plotted against the diameter. The reason therefore has already been discussed: the fact that optical pigment properties such as scattering and absorption are functions of the volume. The following definitions can be stated: ± Density of distribution: the relative frequency of the particle-size parameter in the particle ensemble as a function of this or some other parameter. Especially prominent among particle-size parameters is the equivalent diameter D, but any other measure can be used in its place. Distribution density functions must always be normalized; that is, the total population must yield 100 % ± Cumulative distribution: the normalized frequency (i. e., the frequency referred to the whole ensemble) summed up to a stated value of the particle-size parameter * See ªParticle-Size Analysisº in Appendix 1.

5.1 Introduction

209

± Size fraction and class: the size fraction is the particle ensemble between two fixed values of the selected particle-size parameter that bound the class ± Mean: of the many possible central measures for the particle-size parameter, some are preferred in practice, such as the arithmetic mean, the mode, and the median of the distribution ± Breadth of distribution: a measure characterizing the dispersivity of the particle size in polydisperse populations Empirical particle-size distributions can be represented by the following means used in practice: ± Tables ± Diagrams, such as histograms (bar charts) or closed curves ± Analytic functions obtained by approximation techniques As a rule, a diagrammatic representation is recommended as the way to gain an overview and to make a quick comparison between pigments. The frequencies can be plotted by class and represented as areas in a histogram or bar chart, as shown in Figures 5-1 (distribution density) and 5-2 (cumulative distribution). The horizontal axis for the plot of distributions is the particle-size parameter, commonly the equivalent diameter. Because the parameter can be chosen freely, however, the frequencies for the number of particles, particle surface area, or particle volume (mass) can also be graphed versus a different particle-size parameter selected as the independent variable. In general, these curves are not identical for a given pigment. Special distributions are defined in special standards*: ± Logarithmic normal (lognormal) distribution ± Power-law distribution ± RRSB distribution

Fig. 5-1. Histogram for volume distribution density of a TiO2 pigment. * See ªParticle-Size Analysisº in Appendix 1.

210

5 How Light Scattering and Absorption Depend on the Physics

Fig. 5-2. Cumulative curve for the volume distribution of a TiO2 pigment.

The lognormal distribution is particularly important for pigments, at least when it can be generated by a nucleation and grain growth process. While nuclei ordinarily have a normal distribution on creation, the growth rate of a particle is usually proportional to its surface area. Integration of this growth rule gives a linear time dependence for the log of the particle diameter; substitution in the normal distribution automatically results in the lognormal distribution. A distribution states the probability of a particle being found between values x and x + dx of the particle-size parameter. The equations needed are therefore completely identical to those derived in Section 2.4.1 for the statistical analysis of color coordinates. For example, the series of equations beginning with (2.25) yield the following for the volume/diameter distribution: u D A e

1 2

ds2

mit ds

x

x s

(5.1)

where now x = ln D. The arithmetic mean is x = ln Dz , which is the logarithm of the median of the distribution. Because the sum of the logarithms between 0 and 1 is exactly as great as the sum between 1 and ?, this value divides the area under the distribution function exactly in half. The normalization factor in front of the exponential function changes to A' = A/D because d (ln D) = dD/D. A German standard (DIN 66 144) gives a lognormal coordinate grid. If the particle-size distribution function obeys the lognormal law, the cumulative frequency curve graphed on this grid yields a straight line. For details of the mathematical treatment, reference must be made to the specialist literature. As examples of the form of logarithmic normal distribution functions, which (for the reasons cited) can often be used with success to describe pigment distributions, Figure 5-3 shows several curves for various median diametersDzv1 ; the breadth of the distribution is the same in each case. The type of central measure, as defined in the standards, will be selected case by case in accordance with the test method used or the type of central measure most pertinent to the pigment property of interest. Depending on the breadth of the distribution, a given ensemble or population can show markedly different values of these central measures.

5.1 Introduction

211

Fig. 5-3. Lognormal distributions. Dzv1 is the median of the lognormal distribution; s is a parameter characterizing the breadth of the distribution (s = const = 1.6).

In particle-size analysis (granulometry), ªshape factorsº are sometimes used. With these, equivalent diameters obtained by one determination method should be converted to ªtrueº particle-size parameters. But the determination and use of shape factors is problematic; a better way to do the same thing is to use the statistical tool for the distribution of anisometric particles. While the frequency for isometric particles can be represented by a one-dimensional distribution curve, for anisometric particles it depends on at least two size parameters (e. g., the length L and the breadth B). Because of the dependence on two variables, a frequency surface w = w (x, y) was shown in Figure 5-4 is obtained. To describe the distribution of, say, acicular pigments, the whole shape of the ªhillº must be known, because only in this way is it possible to handle the correlation between L and B. If the logarithms of L and B are denoted by x respectively, the applicable equations are those beginning with equation (2.32). For the same reasons as in the onedimensional normal distribution case, the means are equal to the logarithms of the medians: x = ln Lz and y = ln Bz ; the normalization factor is then B' = B/(Lz 7Bz). Now equation (2.35) with the quadratic form ds2 = 1 represents the ªstandard-deviation ellipseº, which governs the exponents of the lognormal distribution. The family of such ellipses is the adequate form of visualizing the two-dimensional lognormal distribution; their coefficients yield the lengths of the ellipse axes, their slopes, and the eccentricity. At the same time, the coefficients determine the posi-

Fig. 5-4. Two-dimensional normal distribution.

212

5 How Light Scattering and Absorption Depend on the Physics

tion of the median about which the ellipses of equal cumulative probability are grouped, as well as the maximum value of the probability density, which lies at the center of the constant-height ellipses (loci of equal probability density). One way to represent such distribution graphically is the column chart (Fig. 5-5), here shown for the example of a yellow iron oxide pigment. The lognormal distribution is characterized by the concentric ellipses obtained when cumulative frequency is plotted to a logarithmic scale (Fig. 5-6); the constant probabilities on the curves increase from 10 % to 90 % in 10 % steps. The relative eccentricity of the ellipses is a measure of the correlation between the length L and breadth B of the particles. If the eccentricity is 1, there is a rigorous dependence between L and B and the ellipses degenerate to straight lines. If, on the other hand, the eccentricity goes to 0, L and B are independent of one another and the ellipses become circles. The slope of the ellipse axes indicates how rapidly B increases with increasing L. This type of mathematical analysis also prepares the way for cases involving more parameters, in which case higher-dimensional normal distributions are obtained.

Fig. 5-5. Two-dimensional volume distribution density plotted as log L versus log B (acicular yellow iron oxide pigment).

Fig. 5-6. Family of standard deviation ellipses for the two-dimensional lognormal distribution (yellow iron oxide pigment).

5.1 Introduction

213

The methods of determination* (dispersoid analysis) can be discussed only briefly here. The following are applicable to pigments: ± ± ± ±

Particle counting in electron micrographs Sedimentation analysis Light-scattering analysis Analytical techniques based on other physical volume effects such as electrical conductivity.

Particle counting is the most suitable of these methods for pigments. There are several reasons, a few of which are that counting can be done in the vehicle of interest; it can take place in the degree of dispersing that is under study; and concentration problems arise far less often than in other methods, some of which involve extremely high dilutions. The main advantages of counting are that particle shape is determined directly and that primary particles, agglomerates, and aggregates can be distinguished. Once again, further information can be found in the copious specialist literature.

5.1.3 The Optical Constants: Refractive Index and Absorption Index In all the developments up to this point, light could be treated in a geometrical-optical fashion: as propagating continuously in rays. This model was even adequate for the phenomenological theory. The corpuscular theory, however, involves the interaction of light with matter and the constants of that matter, and so it is necessary to come back to the wave nature of light. Light is electromagnetic radiation, and electromagnetic theory (electrodynamics) is governed by Maxwell's well-known equations, which we need not write down here because they can be found in any textbook. There are two differential equations for the electric and magnetic field vectors; their combination gives the universal wave equation for the electric field vector E (x, y, z, t): DE with D

1 u2 E u2 ut2

u2 u2 u2 ux2 uy2 uz2

(5.2)

is the Laplacian and u is the propagation velocity, cm/s. An enormous variety of phenomena are described by this differential equation; for example, every radio and television program in the world is a solution! Here, one of the simplest cases is * See ªParticle size analysisº in Appendix 1.

214

5 How Light Scattering and Absorption Depend on the Physics

to be examined: that of a homogeneous plane wave in a dielectric, with the oscillation in the x, y plane and propagation in the z direction. The solution for the components of E is Ex A eio t

n z c

Ey A eio t

n zid c

Ez 0

(5.3)

where o = 2 pn is the angular frequency, s±1 ; n is the frequency, s±1 ; c is the velocity of light in vacuum, cm/s; A and B are amplitude factors; d is a phase constant (if there is a phase shift between Ex and Ey); and n = c / u is the refractive index. These equations mark the first appearance in electromagnetic theory of a material constant, the refractive index , that links the propagation velocity u in the dielectric and the propagation velocity c in vacuum. If damped waves are also allowed, n has to be replaced by the complex refractive index n n (1 ± ik)

(5.4)

where k is the absorption index. This damping constant, like the refractive index itself, is dimensionless. How n and k can be further related to physical and molecular constants is not of interest here. In connection with absorption and scattering problems involving pigments, however, the experimental determination of these quantities is important. It is necessary to look back at the wave equation in order to explain this point briefly. Suppose one writes this equation for a wavefront incident on the plane surface of a dielectric (x, y plane) at angles j, W. Elementary wave arguments lead to the following conditions that must be satisfied by the electric and magnetic field vectors at the interface: for the reflected wave (i = incident, r = reflected) Wr Wi

(reflection law)

(5.5)

and for the transmitted wave (media 1 and 2) sin W1 n2 sin W2 n1

refraction law (Snell's law)

(5.6)

A boundary condition is needed if one is to answer the question what fraction of the incident radiation is reflected. The condition of continuous amplitudes at the interface is therefore imposed. As a result, the four famous Fresnel equations are obtained; here we use only the two that concern reflection:

5.1 Introduction

rk

sin W1 W2 sin W1 W2

2

tan W1 W2 and rk tan W1 W2

2

215 (5.7)

The reflection coefficient has been analyzed into a component in the place of incidence (r|| and a component perpendicular to that plane (r\). The angles W1 and W2 are linked by Snell's refraction law, equation (5.6). These equations were used earlier in Section 3.1.3. Thus, for normal incidence (W1 = 0), r0 is found very easily (with the approximation sin e & e for small angles; n1 = 1, n2 = n): r0

W1 W2 W1 W2

2

0

12 W1 2 B W2 1 C n 1 C B @ W1 A n1 1 W2

The other coefficients are found by integrating over the half-space. If the complex refractive indices are introduced for n1 and n2 in equation (5.6), two appropriate measurements have been done in equations (5.7), and n1 and k1 are known, then two equations are obtained from which the unknown optical constants n2 (l) and K2 (l) can be determined. This calculation used to be rather time-consuming, but in the computer age it has lost some of its terror. The reflection measurement should not be done at the air/specimen interface; instead, the specimen should be placed in contact with a material having a higher refractive index. The interfaces for this reflection measurement must be highly planar (i. e., as smooth as possible) and polished surfaces. These brief remarks have pointed up all the difficulties that stand in the way of the direct determination of n and k for pigments. The bounding surfaces of pigment particles are in the submicroscopic range, far too small for a reflection measurement ± to say nothing of the fact that ªgoodº surfaces (chemically homogeneous and identical with the pigment material) often cannot be obtained at all. For these reasons, the n (l) and k (l) values used for pigments often have to be the values measured on single crystals of the same material. This substitution is not without its own problems, since it has been shown for many pigments that the particle surfaces can differ chemically from the compact material. For example, TiO2 particles in their normal state have their surfaces covered with OH groups, and the same holds for other inorganic pigments. Organic pigments may also display chemical surface alterations resulting from the production process. As the particle size decreases, the area/volume ratio increases in inverse proportion to the diameter, so that the relative area of a particle measuring 0.1 mm is already a factor of 10 greater than that of a 1 mm particle. The chemical nature of the surface thus becomes rapidly more significant as the particle size decreases, with obvious impact on the optical constants. Thus no one up to now has been able to judge the extent to which constants measured on single crystals are also valid for

216

5 How Light Scattering and Absorption Depend on the Physics

Table 5-1. Refractive indices and optimal particle sizes for some white pigments and fillers at a wavelength of l = 550 nm. Compound, structure

Mean refractive index in contact with Vacuum Vehicle

TiO2, rutile TiO2, anatase a-ZnS, sphalerite ZrO2, baddeleyite ZnO2, zincite Basic lead carbonate Basic lead sulfate BaSO4, barite

2.80 2.55 2.37 2.17 2.01 2.01 1.93 1.64

1.89 1.72 1.60 1.47 1.36 1.36 1.30 1.11

Optimal particle size (in contact with vehicle) Dopt, mm 0.19 0.24 0.29 0.37 0.48 0.48 0.57 1.60

pigments. One would do well to take a skeptical stance toward them and treat results obtained by them (e. g., in Mie calculations) as rough approximations at first. Another source of trouble is that many pigments are optically anisotropic; that is, their n and k values depend on direction. The optical constants referred to the crystal axes can differ widely, as Table 5-2 shows. Averaged constants may be characteristic of pigment populations, depending on the directional distribution of the crystallites. Table 5-2. Refractive indices of important inorganic colored pigments (after Landolt-Bærnstein). Mineral

Chemical formula

Eskolaite Greenockite Goethite Hematite

a-Cr2O3 CdS a-FeOOH a-Fe2O3

Cobalt blue

CoAl2O4

Carbon (Note 2) Crocoite Magnetite Minium Ultramarine

C PbCrO4 Fe3O4 Pb3O4 (Note 3)

l nm 671 589 589 686 blue red 578 671 589 671

Note 1. Mean refractive index. Note 2. Arc carbon. Note 3. Chemical formula [AlSiO4]6(SO4)(S, Cl)2(Na, Ca)8

n no na

ne nb

ng

2.5 (Note 1) 2.506 2.275 2.988 1.74 > 1.78 1.97 2.31 2.42 2.42 1.50

± 2.529 2.409 2.759 ± ± ± 2.37 ± ± ±

± ± 2.415 ± ± ± ± 2.66 ± ± ±

5.2 Mie Theory

217

Another technique for direct determinations on fairly compressible pigments is to press the powder into a compact tablet. Because of residual air included in the compact, mixing rules for the refractive index must be employed in evaluating the data. The surface chemical effects are thus included, at least as an average, and any anisotropy present is at least partly smoothed out. Finally, the immersion method should be mentioned. When larger pigment particles are examined under the microscope, at least the real refractive index n can be determined from the point at which the bounding lines of the crystal vanish. Because of optical anisometry, even this method yields only rough approximations. In the case of the more strongly refracting pigments, there is also a lack of suitable highly refractive liquids or low-melting solids. A further hindrance is that the procedures are laborious and costly and, as a rule, give only the refractive index at a random wavelength or an average over the visible range of wavelengths. In conclusion, it must be stated that exact values for the optical constants of pigments are hardly ever known, even though a knowledge of these values is essential for the development of new products and all analyses of optical performance require them.

5.2

Mie Theory

5.2.1 Integration of the Wave Equation Our theoretical knowledge about the dependence of scattering and absorption on particle size and pigment refractive index is largely based on results derived from Mie theory. The complex of mathematical and physical knowledge that has been gained with this theory would occupy a whole book of its own. If an attempt is made here to trace the essential lines of thought in the theory, it will be done in quite brief form and under restrictive assumptions. For simplicity, the treatment is done with an eye to one objective, understanding the results of the theory as they apply to pigments. The model is a dielectric sphere on which a plane wavefront is incident. Application of the wave equation reveals that the sphere is excited into oscillation; as a oscillating multipole, it then acts as the center from which new waves are emitted. These waves are superposed on one another. First, in wave equation (5.2) ± including the Laplacian ± one must separate the time function and rewrite the equation as a harmonic oscillation for the polar coordinates r, j, W suitable to the problem. The result is called the Helmholtz equation. Its solutions can be found in textbook of theoretical physics. Any such solution can be written as a sum over products of three complex-valued functions; for example, the radial component of the electric field vector E is given by

218

5 How Light Scattering and Absorption Depend on the Physics

Er

1 P j1

Aj n; a Yj W Fj j

Along with the refractive index n, this includes the typical dimensionless parameter a

D p n0 l

(5.8)

where D is the particle diameter and n0 is the refractive index (relative to vacuum) of the medium surrounding the particle. The complex-valued functions have the following meanings: A (n, a): spherical Bessel function (n is the refractive index of the particle relative to the surrounding medium) Y (W): spherical functions (spherical Legendre polynomials) F (j): exponential function The summation takes care of the superposition of excited partial vibrations. In order to get to intensities, one must form the absolute squares of E. Two expressions are obtained: I|| for the ray parallel to the incidence/observation plane and I\ for the ray perpendicular to that plane. These are enough to describe unpolarized light. For specified sphere parameters n, a, these functions depend only on W (by the axial symmetry of the system); they can also be taken from tables (see Section 5.3). If the complex refractive index n* = n (1 ± ik) is formally introduced, the formulas once again include absorption. The solutions of the Mie theory for small particles show that the entire particle oscillates symmetrically as a dipole, along and opposite to the propagation direction of the incident wave. In the case of larger particles, multipole oscillations also occur; what is more, the secondary waves do not oscillate in phase. Figure 5-7 shows the first three partial oscillations as field lines on the surface of the sphere. The vibration place of the light ray generating the waves is in the plane of the drawing, so that the direction of propagation is perpendicular to the drawing plane. This is a symmetry plane of the process, and so the front hemispheres shown must be complemented by the back hemispheres, on which the curves fall into congruent patterns. Secondary waves outside the sphere are generated by the incident plane wave. For very small particles, the whole particle oscillates as a dipole; the excitation is symmetric, in and opposite to the propagation direction of the incident wave. Larger particles experience multipole oscillations; the secondary waves oscillate in unequal phases, and the superposition of the partial waves yields an increasingly complicated spatial distribution with a growing number of maxima and minima. There is also a decrease in the fraction scattered into the back half-space relative to the front half-space (see Fig. 5-8 for an example).

5.2 Mie Theory

219

Fig. 5-7. The first three partial oscillation modes of a dielectric sphere after Mie.

Fig. 5-8. Polar diagram for the emission distribution of a scattering sphere having n = 1.7 and a = 4.3, after J. Thiemann. (The center of the scattering particle is to be imagined at the cross+).

Similar calculations have been done for cubical, cylindrical, and ellipsoidal particles. These calculations are exceedingly complex, so that approximations are only used in practice. For the anisometric particles under consideration, one obtains a simplified scheme of two absorption and two scattering functions, one each perpendicular and parallel to the longitudinal axis of the particle.

5.2.2 Absorption and Scattering of the Particle Ensemble The solutions I || and I\ of the Mie theory will now be related to the Kubelka-Munk scattering and absorption coefficients. For it, with I || and I\, the fractions scattered into the space surrounding the sphere and absorbed in the sphere must be summed. This is done by integrating over the area 4p of the unit sphere* and dividing by the particle cross section D2p/4. the integral over j can be written out immendiately (I || and I\ do not depend on j):

* In the case of scattering, integration over the back hemisphere, i. e., 0 5 W 5 p /2, is also recommended.

220

5 How Light Scattering and Absorption Depend on the Physics

Z2p Zp 1 1 Q 2 dj f W Ik Ik sin W dW D p 4p j0 W0 4 2 2 D p

Zp

f W Ik n ; a; W Ik n ; a; W sin W dW

0

In this way, expressions not containing j and W are obtained: the scattering cross section QS (n, a) (real part) and the absorption cross section QA (n*, a) (imaginary part). The function f (W) takes care of the fact that the Mie theory (directional incidence of light) is not based on the same geometry as the Kubelka-Munk theory (diffuse incidence, plane-parallel layer). For absorption, fA = 2 in agreement with Kubelka's assumption in Section 3.2.2; for scattering, according to Mudgett and Richards, fS = (3/8) (1 ± cos W). The quantities QA and QS are dimensionless; they represent the ratios of the optically effective cross sections to the geometrical cross section: qopt qA 2 qgeo Dp 4 qS QS n; a 2 Dp 4

QA n ; a

i. e. qA l; n; k; D qS l; n; D

D2 p QA n ; a 4

D2 p QS n; a 4

For practical use, the quantitative reference must be made to the pigment particle, for knowing how much one pigment particle scatters or absorbs is less important than knowing how much 1 L or 1 kg of pigment does. The single-particle quantities k1, s1 referred to volume are obtained by dividing by the particle volume V = D3p/6 and using equation (5.8): k1 l; n; k; D s1 l; n; D

qA 3 3 p n0 QA l; n ; a QA l; n ; a V 2l 2D a qS 3 3 p n0 QS l; n; a QS l; n; a V 2l 2D a

(5.9)

5.2 Mie Theory

221

In the case of monodisperse particles, the quotient Q / a is thus proportional to the Kubelka-Munk coefficients. The spectral Kubelka-Munk coefficients referred to PVC, on the other hand, are generally constants of the material for ensembles of polydisperse distributions. They are thus obtained by summing the contributions over the particle-size distribution u (D): k l; n; k s l; n

R1 0

R1 0

u D k1 l; n; k; D dD u D s1 l; n; D dD

(5.10)

In the case of distributions of anisometric particles u (L, B),the angular distributions must also be known if one wishes to use a sum formula on the above pattern. If a random distribution (i. e., no preferred direction) is assumed, u (L, B) can be written, similarly to the above case, provided the scattering and absorption cross sections parallel and perpendicular to the axis of the acicular or platy particle are known (see Section 5.2.1). Two important special cases should be examined: those where the particles are very small and very large relative to the wavelength. Approximations will be obtained in both cases. For absorption, a fairly simple summary can be given: Thus, for particles smaller than a certain limiting size, absorption is independent of D; for large particles, absorption falls off as 1/D. An explanation of this behavior will follow in Section 5.2.3. The effect of particle size is somewhat more complicated for scattering. For large particles, scattering also decreases as 1/D (Fresnel reflection), since the sphere acts as a reflecting mirror. We have 3 n 1 2 QS where QS r0 s1 2D n1 In the small-particle case, Rayleigh scattering is obtained. The small sphere is excited only to dipole oscillations. The result is QS

8 4 2 aM 3

where

M

n2 1 n2 2

Here we are in the realm of molocular scattering, where the scattering cross section decreases as* a4*1/l4. This relation explains, say, why the sky is blue: The molecules of the atmosphere scatter violet light (l = 400 nm) more strongly than red * In this text, * denotes proportionality.

222

5 How Light Scattering and Absorption Depend on the Physics

(l = 700 nm) by a factor of (700/400)4 & 10. The sky is blue, rather than violet, because the solar spectrum contains far less violet than blue and because the sensitivity of the human eye rapidly falls off toward zero as the wavelength becomes shorter. Rayleigh scattering ceases to be important in the particle-size range of pigments, because Mie scattering dominates it by some orders of magnitude.

5.2.3 Scattering Behavior of Pigments Using the behavioral rules outlined above, van de HULST gave an equation for nonabsorbing spheres and for n = 1 + e: 4 4 sin b 2 1 b b where b 2a |n ± 1|

Qext 2

cos b (5.11)

where the extinction cross section ± the flux scattered away into all of space related to the geometrical cross section ± is described as a function of a and n. This is one of the most important formulas in the whole field of Mie theory, for it describes the essential features of scattering. It is valid not just for n close to 1 but even for n = 2. This can be seen from the curves of Figure 5-9, which shows scattering curves for refractive indices 0.8 5 n 5 1.5. The b scale at bottom applies to all five curves; there is a different a scale for each n.

Fig. 5-9. Total scattering cross section Qext calculated by Mie theory for n = 1.5, 1.33, 0.93, and 0.8.

5.2 Mie Theory

223

The most striking fact is the succession of maxima and minima. These extreme values result from interference between the refracted and transmitted light; maxima occur where the superposed waves reinforce, minima where they cancel. For small particles, the curves ought to begin as a4 (Rayleigh scattering), but equation (5.11) does not properly reflect this fact. The ordinates Qext increase systematically for larger n because of grazing reflection. From the van de Hulst calculated values, linear regression analysis yields the relation Qmax 2.716 n + 0.3235

(5.12)

The first minimum (ªfirst Mie minimumº) can still be clearly measured for isodisperse populations (e. g., latexes). The existence of the principal maximum immediately implies that an optimal value a must exist. Hence it follow that ± There must be a particle size optimal with respect to lightening power ± For a given particle size, there exists a wavelength at which the scattering takes on maximal values Because what is wanted is a proportionality to the Kubelka-Munk PVC-referred coefficients s1 (eq. 5.9), only scattering into the back half-space is to be counted. Semiquantitatively, this fraction can be set roughly proportional to Qext for a constant refractive index. Then, from the maximal value bopt & 4, Figure 5-9, immediately gives D p n0 n 1 4 (5.13) bopt 2 a n 1 2 l If the refractive index is given, an expression can be obtained for the optimal aopt ; if l is given, the optimal particle size can thus be found. In the case of TiO2 in rutile form (n = nTiO2 /nmedium = 2.8/1.5 & 1.9), for l = 550 nm we obtain Dopt

bopt l 4 0:55 0:26 mm 2 p 1:5 0:9 2 p n0 n 1

(5.14)

which is fairly close to the experimental value (see Table 5-1). Improved values are obtained if bopt is taken not at the maximum of Qext but at the maximum of Qext/a as suggested by equation (5.9). The division shifts the optimum to somewhat smaller values, giving bopt = 2.93, resulting in a Dopt of 0.19 mm for rutile. Figure 5-10 presents scattering curves of Qext /a for well-known white pigments, calculated with van de Hulst formula (5.11). As the refractive index decreases, the optimal particle size, typically, grows larger and less scattering takes place. Finally, when the refractive index approaches that of the vehicle, Qext/a decreases as 1/a, the behavior seen for Fresnel reflection, and vanishes. The optimal particle sizes for bopt = 2.93 were calculated with equation(5.13) and are listed in Table 5-1.

224

5 How Light Scattering and Absorption Depend on the Physics

Fig. 5-10. Scattering curves (plots of Qext /a versus particle size) for some white pigments and fillers.

The wavelength dependence of scattering can be determined with equation (5.11); the curve for n = 1 + e (Fig. 5-9) can also be used in a semiquantitative analysis. The plot in terms of a * 1/l must be read from right to left in order to trace what happens as the wavelength increases. The presence of the maximum indicates that particles smaller than Dopt preferentially scatter short-wavelength light while those larger than Dopt preferentially scatter long-wavelength light. This situation explains how white pigments in gray pastes can produce a colored shade through selective scattering: Finely-divided white pigments give bluish hues while larger ones give brownish hues.

5.2.4 Absorption Behavior of Pigments Van de Hulst also gives an equation for the absorption, but we need not discuss this because, fortunately, BROCKES has done systematic Mie calculations for fixed n and k. His curves (Fig. 5-11) are log-log plots of QA /a versus a for a range of n and nk. They imply the following: ± For very small particles, absorption is independent of a and thus of particle size. In other words, absorption will not increase on further size reduction. As the absorption index grows larger, absorption increases ± For very large particles, absorption is approximately the same for all refractive indices and absorption indices, falling off hyperbolically. The particle absorbs and reflects in accordance with its cross section, so that QA /a decreases as 1/D ± The uppermost curve in Figure 5-11 is for pigments with high absorption index k but low refractive index n, such as carbon black pigments. It shows that the optimal particle size is less than an identifiable limit ± The lowermost curve is for pigments with small absorption index k but high refractive index n, such as most inorganic pigments. This curve has distinct maxima, which should be thought of as higher and steeper than the log-log plot shows

5.2 Mie Theory

225

Fig. 5-11. Absorption curves of QA /a (log-log plot), after Brockes.

One other important point should be mentioned because it is overlooked many times. At the positions k (l0) of absorptions in the spectrum, the refractive index behaves in a anomalous way as described by the well-known dispersion formula n

1

k l0 2 l0 1 l

Figure 5-12 presents an example of the refractive index discontinuity for real pigments that exhibit absorption peaks of finite breath. Because the scattering shows a direct dependence on n, it also has a discontinuity. The rule is that the refractive index drops abruptly on the rising edge of the absorption and rises abruptly on the falling edge. This behavior of the scattering characteristic may well lead to remarkable color effects. There are cases of pigments in which absorption and scattering are antagonistic and others in which they vary in the same sense. The red iron oxide pigments can serve as an example of the second type. For particles smaller than Dopt, equation (5.13) says that lmax must also become shorter, if one would hold the maximum. this means that the position of maximal scattering shifts toward shorter wave-

Fig. 5-12. Absorption and anomalous refractive index.

226

5 How Light Scattering and Absorption Depend on the Physics

lengths: The red takes on a yellow cast. The absorption maximum shifts at the same time, also to shorter wavelengths, and this effect strengthens the yellow cast. For particles larger than Dopt , yellow is taken away in both ways, and the pigment becomes redder. In pigment reduction with TiO2, such coarse pigments are actually seen to take on a marked blue cast. Two factors can account for this effect: First, the absorption of the red pigment moves toward longer wavelengths, thus setting blue light free; second, the scattering increases suddenly because of the anomalous dispersion of the TiO2 pigment, whose strong absorption ends near 400 nm. The Mie theory has made it possible to predict the reflection spectrum of a pigment, and thus its color properties, given the complex refractive index, the concentration, and the particle-size distribution. We have now reached the goal stated in Chapter 1 by tracing the amazing range of optical qualities seen in coloring materials ± their technical color properties ± back to measurable physical quantities.

5.3

List of Symbols used in Formulas

a = Dpn0 /l A, B A (n, a) b = 2a | n ± 1| B B Bz c d ds2 D Dz E I k k1 k l L Lz M n

parameter in the Mie theory amplitude factors spherical Bessel function parameter in the van de Hulst equation normalization factor for two-dimensional normal distribution breadth of anisometric particle, mm median particle breadth, mm velocity of light in vacuum, cm/s phase constant quadratic form of normal distributions particle diameter, mm median particle diameter, mm electric field vector radiance factor, W cm±2 absorption coefficient per unit PVC, mm±1 single-particle absorption coefficient per unit PVC, mm±1 absorption index wavelength, nm length of anisometric particle, mm median particle length, mm abbreviated notation: M = (n2 ± 1)/(n2 + 2) (real) refractive index with subscript: 0 of the medium

5.4 Summary

n* = n (1 ± ik) n = c/u o = 2pn j F (j) q

Q r r s s1 s W Y (W) u u (D) x

5.4

227

complex refractive index frequency, s±1 angular frequency, s±1 meridian angle in spherical coordinates exponential function optically effective cross section, cm2 with subscripts: A absorption cross section ext total scattering cross section (nonabsorbing sphere) S scattering cross section effective cross section with same superscripts as q reflection coefficient distance from origin in spherical coordinates scattering coefficient per unit PVC, mm±1 single-particle scattering coefficient per unit PVC, mm±1 standard deviation, a parameter of distribution breadth polar angle in spherical coordinates spherical function propagation velocity, cm/s volume distribution of diameter general particle-size parameter

Summary

The corpuscular theory finally relates the material constants for absorption and scattering to the individual particle and its physical properties. At the center of the analysis is the Mie theory, which derives scattering and absorption properties from a few fundamental physical quantities. It is therefore important only for pigments, not for dyes, although even for pigments it yields insights that could not be received in any other way. The basic physical quantities are particle size, refractive index, and absorption index. Because a pigment ensemble comprises fractions differing in particle size, the statistics ± the particle-size distribution ± must here be treated. The optical scattering and absorption properties are volume-dependent, so that the preferred way of representing these data is the distribution density of volume versus diameter: u (D). The following concepts are discussed: distribution density, cumulative distribution, size fraction and class, measures of central tendency, and measures of distribution breadth. Representations include tables, diagrams, and analytic functions. When unlike pigments are to be compared, plots of distribution density and cumulative distribution are particularly useful. When distributions are to be described by analytic functions, the logarithmic normal (lognormal), power-law, and RRSB distribu-

228

5 How Light Scattering and Absorption Depend on the Physics

tions can be used; of these, the lognormal is especially well-suited to pigment distributions. In this distribution, the central measure is the median. For describing anisometric (e. g., acicular or platy) particles, the tools of mathematical statistics are also available. The two-dimensional lognormal distribution of particle length L and breadth B also yields a graphical representation and makes it possible to calculate the parameters and central measures. The eccentricity of the calculated standarddeviation ellipse is a measure of the correlation between length and breadth. The principle can be extended when more than two particle-size parameters are needed. This chapter gave only a brief discussion of methods used to determine the particle-size distribution. The phenomena treated here require for the first time that the wave nature of light must be considered. From the differential equation that describes oscillation processes (wave equation), the homogeneous plane-wave solution is derived; it contains the refractive index n as a constant. For absorption, there is also a damping constant k; the complex refractive index n* is formed by k together with n. Reflection and refraction laws are effortlessly derived from the wave equation by postulating continuity at the interface between two media. An attempt to obtain the fraction reflected and transmitted leads to the Fresnel equations, with whose aid n and k can be determined from reflection measurements. Because of the small size of pigment particles, unfortunately, such direct measurements are exceedingly difficult. In practice, it is necessary to employ physical constants measured on large single crystals instead, and ultimately this substitution is not satisfactory. What is more, the optical anisotropy of most pigments makes it hard to determine and use the constants. Reflection measurements to obtain the constants can be done on pressed pigment powders if the material is sufficiently compressible. The immersion method has sometimes been used to determine n. At present, there are just a few values of the optical constants directly measured on the pigment. The Mie theory, which uses a model of a plane wave incident on a dielectric sphere, is discussed as it aids in understanding pigment phenomena. The theory of differential equations gives solutions containing a = Dpn0 /l as a typical parameter. These are also functions of the angles j and W in the three-dimensional coordinate system. After introducing the complex refractive index, one can split the solutions into scattering and absorption parts. The results show that the spherical particle acts as an emission center for new waves that interfere with one another. Even anisometric particles have been calculated with the Mie theory. The procedure for linking the radiance factors in Mie theory to the KubelkaMunk coefficients involves first integrating over the solid angle (giving scattering cross section and absorption cross section). The result is divided by the sphere volume and then summed over the particle-size distribution. The same technique can be used with anisometric particles if the angle-dependent cross section values are known. Rayleigh scattering on very small particles (not important for pigments) and Fresnel reflection on very large particles are discussed. A formula stated by van de Hulst is examined as a way of describing how the scattering cross section depends on the refractive index and the parameter a. The

5.5 Historical and Bibliographical Notes

229

result displays maxima and minima, which can be attributed to interference between the partial oscillations. The principal maximum shows that there must be optimal particle sizes, or optimal wavelengths, for scattering. From the position of the principal maximum, the optimal particle sizes for well-known white pigments and fillers are derived along with the scattering curves. This procedure provides an explanation for the shade of white pigments in gray pastes. The laws describing the absorption of inorganic and organic pigments are obtained from Mie calculations performed by Brockes. Once again, maxima appear. Anomalous dispersion, seen at absorption edges, also has some effect. The results also account for the hue shift in iron oxide pigments when the particle size changes. The Mie theory makes it possible to calculate in advance the color properties of pigments.

5.5

Historical and Bibliographical Notes

The significance of particle size to the pigment properties has already been referred to, as have the various particle-size parameters; see [1±4] in Section 4.10. These prior publications also deal with the parameters and representations suitable for particle-size distributions. A special analysis of the logarithmic normal distribution appears in [1]. The mathematical treatment and representation of distributions of anisometric particles was first published just a few years ago [2]. The MIE theory [3], dating from 1908, is based on the principles of classical electrodynamics, which has been covered in textbooks [4], [5]. MIE derived this theory as a physical explanation of the color displayed by gold sols having various particle sizes; it was a complete success. The application to very small particles is due to Raleigh [6]. Manual Mie calculations used to be very tedious because of the summations that had to be done, but later workers [7±9] have performed calculations for a range of refractive indices; one much-used set of tables is due to Lowan [10]. Nonspherical particles such as cubes and ellipsoids have also been calculated [11]. Although there were no calculations for refractive indices in the range of 1.6 5 n 51.9, the very range of interest for pigments, an attempt was made at an early point to generalize the results into a single universal scattering function, with the object of predicting optimal particle sizes for the most important pigments. One such procedure is described by Jaenicke ([26] in Chapter 4). the approach taken in this book to determining the optimal particle size with respect to scattering was devised by van de Hulst, whose monograph Light Scattering by Small Particles [12] is the best treatment of this area. Kerker's book on scattering [13] should also be cited, as should the book by Kortçm ([19] in Chapter 3). Computers have greatly simplified the process of doing Mie calculations; this capability has been heavily used, for example by Dettmar [14] for higher refractive indices. Dettmar also performed the calculations for iron oxide pigments ci-

230

5 How Light Scattering and Absorption Depend on the Physics

ted by Brossmann [15] and those for the absorption of pigment particles, which were used by Brockes [16] in the publication discussed in Section 5.2.4. The application of Mie calculations to practical problems has been reported by Maikowski [17], Hauser and Honigmann [18], and Hediger and Pauli [19]. An interesting test is the one carried out by Felder [20]: spherical pigment particles made of a soft material (dyed PVA) were deformed into ellipsoidal particles by stretching the medium in which they were embedded. The results revealed how absorption changes on the transition from spheres to ellipsoids. The literature on methods for finding the optical constants of pigments by the immersion method is rather sparse; the same can be said for measurements done on colored pigments (see, e. g., [21]). In methods based on pressed powder measurements, the presence of residual air in the compact means that refractive index mixing rules must be employed [22]. Given two reflection measurements, the Fresnel equations simultaneously yield n and k, as Nassenstein has shown [23]. Unfortunately, this technique applies only to easily compressible pigments, a class that does not include inorganic pigments. Some work remains to be done in this direction.

References [1] J. Aitchinson, J. A. C. Brown, The Lognormal Distribution, Cambridge University Press, London, 5. Repring 1973. [2] H. .Vælz, farbe + lacke 90 (1984) 642 und 752. [3] G. Mie, Ann. Physik 25 (1908) 377. [4] G. Joos, Leerbuch der Theoretischen Physik, Geest & Portig, 7. edit., Leipzig 1950. [5] J. Honerkamp, H. Ræmer, Grundlagen der klassischen Theoretischen Physik, Springer, New York 1986. [6] J. W. Rayleigh, Proc. Roy. Soc., Ser. A, 90 (1914) 219. [7] H. Blumer, Z. Physik 32 (1925); 38 (1926) 920; 39 (1926) 195. [8] E. J. Meehan, H. Beattle, J. Optc. Soc. Am. 49 (1959) 735. [9] R. D. Murley, J. Phys. Chem. 64 (1960) 161. [10] A. N. Lowan, Tables of scattering functions for spherical particles, in Nat. Bur. Stand., Appl. Math. Ser. 4 (1949), US Gov. Print. Off. Washington 1948. [11] R. Gans, Ann. Physik 37 (1912) 881. [12] H. C. van de Hulst, Light scattering by small particles, J. Wiley & Sons, London 1957. [13] M. Kerker, The scattering of light, Academic Press, New York etc. 1969. [14] H. J. Metz, H.-K. Dettmar, Kolloid-Z. 192 (1963) 107. [15] R. Broûmann, AIC Color 69 Stockholm, Congr. B. Vol. 2, 15. [16] A. Brockes, Optik 21 (1964) 550. [17] M. A. Maikowski, Z. Elektrochem. 71 (1967) 313. [18] P. Hauser, B. Honigmann, farbe + lack 81 (1975) 1005. [19] H. Hediger, H. Pauli, XIX. Fatipec Congress Aachen 1988, Congr. B. II, 503. [20] B. Felder, Helv. Chim. Act. 49 (1966) 440. [21] V. Koutnik, Chem. Prumysl (Chem. Ind. CSSR) 11 (1964) 604. [22] W. Heller, Gov. Res. Rep. US Opt. Commerce, Nr. AD 608 337 (1964). [23] H. Nassenstein, AIC Color 65, Luzern, Congr. B 12.

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

Part II Test Methods

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

6

Measurement and Evaluation of Object Colors

6.1

Reflection and Transmission Measurement

6.1.1 Gloss Measurement and Assessment When light falls on a body, part of it is generally reflected at the surface of the body, even before the absorption and scattering processes described in Chapter 1 can take place in the interior of the layer (Fig. 1-1). The fraction reflected at the surface, as described by the Fresnel equation, is a function of the refractive index n and the angle of incidence. For perpendicular irradiation, the reflected fraction is given by r0 = (n ± 1)2/(n + 1)2 ; for paint and lacquer films with refractive indices of n & 1.5, this formula gives r0 & 0.04. The fraction increases very slowly with increasing angle of incidence and attains high values only at grazing incidence, that is, at incidence angles just below 908 (Fig. 6-1).

Fig. 6-1. Fresnel reflection at some surfaces.

234

6 Measurement and Evaluation of Object Colors

If the fraction reflected at the surface is plotted as an indicatrix, that is, as a function of the observation angle e2 in polar coordinates, two extreme cases can be identified: ± Directional reflection only (Fig. 6-2) ± Diffuse reflection only (Fig. 6-3)

Fig. 6-2. Specular (directional) reflection.

Fig. 6-3. Diffuse reflection.

The first case corresponds to regular specular reflection; in the second case, numerous microscopically small irregularities at the surface give rise to backscattering independent of the angle. The indicatrix here obeys the Lambert cosine law: r = cos W. Real paint and lacquer coatings commonly exhibit a mixture of the two extreme behaviors. It should be emphasized that this reflected light is no longer available to take part in absorption and scattering processes in the coating. As a consequence, the effect of surface reflection must be properly considered in color evaluation. We will hear more on this point in Section 6.1.2. Here, what is of interest about surface reflection is whether it is directional or contains directional components. One speaks of the ªglossº of a surface and distinguishes between ªhigh glossº and ªmat glossº (Fig. 6-4). These terms do not only refer to the purely physical phenomenon of surface reflection but rather to a visual experience. It follows that gloss has a physiological component plus a psychological one.

6.1 Reflection and Transmission Measurement

235

Fig. 6-4. Indicatrices for a nearly mat surface (1) and a high-gloss surface (2).

Studies of the way in which observers evaluate gloss have identified at least two types of observers: ± The ªanalyzingº observer, who considers the sharpness with which reflected objects (e. g., window cross) are imaged ± The ªintegratingº observer, who considers intensity contrasts of the reflected light; for example, the ªGolden Helmetº (formerly attributed to Rembrandt) gives the illusion of gloss without reflective surfaces, simply through the juxtaposition of light and dark. In visual gloss evaluation, as a rule, the evaluator includes varying proportions of both observers. It is immediately clear that the observer behavior just described can scarcely be imitated by any gloss measurement technique with a purely physical basis. The situation is similar to that in colorimetry, though in that instance the dilemma could be resolved by postulating a standard observer and basing definitions on matching judgments. It is not entirely out of the question that a similar approach might work in gloss evaluation; it is, however, made difficult by the two modes of visual assessment and the accidental mixing of these modes. In view of these circumstances, the gloss has to be determined as a function of observation angle in the great majority of cases. The preferred type of plot is the polar gloss indicatrix, as shown in Figure 6-4, but a bell-shaped curve in Cartesian coordinates is quite usual. Such a distribution curve is analogous to the spectral distribution in colorimetry (Chapter 2); the fact that no ªstandard gloss observerº exists here stands in the way of a more physiologically-oriented treatment of the measured values. The complete gloss curve is measured with a gonioreflectometer (goniophotometer), a instrument in which the angle of incidence can be set to any value and a probe (photocell) is placed on the observation side (Fig. 6-5). The probe is traversed across the cone of scattered light as the intensity distribution is measured and plotted. The resulting curve (indicatrix) can often be described in terms of a few parameters, chiefly the maximum value and half-value width. The proper functioning of a goniophotometer imposes certain requirements on construction, chiefly relating to the parallelism of the ray path and the aperture

236

6 Measurement and Evaluation of Object Colors

Fig. 6-5. Diagram of the reflectometer with ray paths.

angle on the observing side. These essential detail can be found in standards*. The same standards also describe simplified glossmeters in which definite aperture angles are set for three distinct incidence angles (208, 608, 858). The viewing angle should be equal to the angle of incidence and must not differ from it by more than +0.18. The incidence angles are recommended as follows for best differentiation in various applications: ± 208 for high-gloss specimens ± 608 for specimens with moderate gloss ± 858 for mat specimens Suitable primary standards are plane, polished plates of black glass having a refractive index of 1.567 for a wavelength of 589 nm. For each of the three incidence angles, the reflectometer reading for this standard is set equal to 100. If the refractive index differs from the stated value, the reflectometer reading for each of the three angles can be calculated with the Fresnel equations (which are stated in DIN 67530). Two gloss-related effects due to pigmentation should be mentioned here. First, it is often observed that the gloss initially decreases as the pigment concentration increases; at higher concentrations, particularly just before the critical pigment volume concentration is reached, the gloss may increase again. The cause of this phenomenon lies in the fact that the pigment particles become more and more ordered as the critical condition is approached; at the critical concentration they take on a close-packed configuration with binder filling the voids. This change is accompanied by smoothing of the surface, which was irregular at low concentrations because of individual pigment particles protruding from it. Second, when the mirror * See ªGloss, Measurementº in Appendix 1.

6.1 Reflection and Transmission Measurement

237

image of a very bright, small source of light in such a paint film is examined, a halo is seen around the image of the source (ªgloss hazeº). An incandescent filament thus appears as if viewed through a thin veil; that is, diffuse reflection is more intense in directions near the specular angle than far from it. Gloss haze is due to microscopic irregularities in the outermost layers of the surface, which may be present because, for example, inadequate pigment dispersing has left pigment agglomerates behind. The effect is easily measured with the goniophotometer by making the aperture angle as small as possible and traversing the measuring probe over a few degrees about the specular angle. Gloss effects with metal-effect paints are also caused by pigments (metaleffect pigments). Because the optical phenomena on such coatings have to be characterized by color measurement, they will not be described until later (Section 6.2.4). The term ªgloss developmentº denotes the variation of the degree of gloss as a function of the dispersing time. As a rule, gloss development is a way of gaining information about the progress of the dispersion process (Section 4.1.2). The measure used, as set forth in ISO 8781-3, is the dispersing work required to attain a given reflectometer value. Alkyd resin system* and alkyl/melamine resin systems** can be used as test media. These test methods, similarly to those for tinting strength development (Section 4.7.3 and 8.2.4), makes it possible to compare pigments, mill base compositions dispersing equipment, or dispersing processes. Preparation method: The test and reference pigments are dispersed in a suitable vehicle in accordance with suitable conditions (vehicle and conditions are to be agreed on). As the dispersing process continues, samples are taken from the batch and applied to a substrate; after drying or stoving, reflectometer values are measured.** Evaluation method: A diagram is prepared showing the reflectometer value (ordinate) versus the dispersing work (abscissa), that is, the dispersing time or stage. A curve is fitted to the point and, from the curve, the dispersing work required to attain a pre-estabilshed reflectometer value is read off.

6.1.2 Measurement and Evaluation Conditions We now turn back to the discussion in Section 2.1.2, where it was shown what geometrical configurations are used in the measurement of reflectance, reflection factor, transmittance, and transmission factor. Now we will explain how these geometries can be realized in instruments; it will be seen that the geometrical conditions of irradiation and observation, the ªmeasuring conditionsº, play a vital part***. * See ªEase of Dispersionº in Appendix 1. ** See ªGloss Measurementº in Appendix 1. *** See ªColorimetryº in Appendix 1.

238

6 Measurement and Evaluation of Object Colors

Fig. 6-6. The 45/0 geometry.

We begin with the 45/0 geometry, as illustrated in Figure 6-6. The source aperture angle should be no larger than 208, the receptor aperture angle no larger than 108. For specimens with surface texture, the reflection factor Rc depends on the orientation of the specimen relative to the direction of incidence; the predominant texture direction should be parallel to the plane of incidence. The figure also shows that the rays are not directional but conical (quasiparallel). In geometries with diffuse irradiation or diffuse observation, an integrating sphere is used to create a hemispherical distribution of flux. Figure 6-7, for example, shows the use of the integrating sphere for the 8/d geometry (reflectance Rc). If incidence on the specimen is diffuse (hemispherical), the setup of Figure 6-8 is em-

Fig. 6-7. Integrating sphere used in measurement of Rc (8/d geometry).

6.1 Reflection and Transmission Measurement

239

Fig. 6-8. Intregrating sphere used to create diffuse irradiation (a and b show alternative configurations).

ployed, giving the d/8 geometry (reflection factor Rdif ). Here the specimen and standard are measured in a comparative method; they are placed at the respective ports in the sphere either simultaneously or one at a time. Geometries involving the integrating sphere have this peculiarity: If the directionally reflected fraction of the radiation is absorbed or allowed to escape from the sphere (ªgloss exclusionº by a ªgloss trapº), what is measured is solely the scattered reflection without directional components (Fig. 6-7). Geometries with gloss exclusion therefore give values similar to those for the 45/0 geometry, in which, similarly, the directional components on the observing side are not measured. Whenever necessary to maintain this distinction, the subscript letters ªinº (inclusive, with surface reflection) or ªexº (exclusive, without surface reflection) will be added to the symbols for the reflection values. The decision whether or not to measure the directional components of the reflected radiation is extremely important for the measurement of nonluminous perceived colors. As a consequence, the geometries just described can also be classified by whether the surface reflection is included or excluded*: ± Method A: Geometry 8/d (reflectance Rin,c) or d/8 (reflection factor Rin,dif ), with no gloss trap in either case. The surface reflection is included in the measurement. Evaluation: Before calculating the color difference in accordance with * For standards see ªColor Differencesº in Appendix 1.

240

6 Measurement and Evaluation of Object Colors

ISO 7724/3, a correction for the surface reflection (r0 = 0.04; see preceding section) must be subtracted from the measured values. ± Method B: Geometry 45/0 (reflection factor Rc), resp. 8/d or 0/d both with gloss exclusion (reflectance Rex,c), and their inverses. The surface reflection is not measured. Evaluation: The color difference is calculated in accordance with ISO 7724/3, directly from the measured values (i. e., without the subtractive correction for surface reflection). In Method A, the color differences determined between test and reference specimen are those having to do with differences in coloring materials. The results are generally not affected by differences in specimen surface quality. Accordingly, Method A is particularly suitable for pigment testing. The only exception is in the fullshade determination of black pigments (see Section 6.2.2). If the gloss changes, the total surface reflection, which consists of a directional and a diffuse component, remains constant when Method A is employed for the measurement. Because the total surface reflection is included in the measurement and a correction must be made by subtracting the surface reflection from the measured value, color differences obtained in this way are strictly due to differences or changes in the interior of the system. If the measured values were used directly (i. e., without subtracting the surface reflection) for calculating color differences, the results would be too small because of the convexity of the cube-root curves for X ,Y , and Z (see Chapter 2). This holds particularly for color-saturated or dark specimens. Essentially, the effect of calculating out the surface reflection is that color differences are roughly the same as seen by an observer looking in a ªgloss-freeº manner at high-gloss specimens, that is, if the surface reflection were ªreflected outº at the time of observation. In the case of mat specimens, the color differences are equal to what an observer would see if diffuse surface reflection were eliminated, that is, if a coat of lacquer binding medium were applied to the specimen to render it glossy and the specimen were then examined in a gloss-free manner. Colorimetric evaluation by this method, then, has a direct visual analog only for highgloss specimens. In Method B, the color differences found between test and reference specimen are those that stem from the coloring materials as well as differences in surface quality. Accordingly, specimen color differences come out approximately the same as in visual color matching with gloss exclusion. If a specimen loses its gloss, as in the course of a durability test, the diffuse fraction in the surface reflection becomes larger, so that Method B yields a larger measured value. The method therefore gives integral color differences that include differences in coloring materials together with surface gloss differences. The method is therefore not well-suited to routine pigment testing, because comparisons between pigments must be free of coating surface effects. On the other hand, in the case of durability tests, a change in gloss is to be determined by a separate gloss measurement. nonetheless, Method B can yield marked departures from visual assessment, frequently because of the heavy angular dependence of the surface reflection for semi-mat specimens of because of the gloss haze for gloss specimens. These deviations are especially ap-

6.1 Reflection and Transmission Measurement

241

parent when the 45/0 geometry is not exactly observed for visual matching of specimens with gloss haze; often, the illumination employed for matching is not directional or the angle of incidence deviates from 458. Following this discussion, it should be emphasized that similar to identical results can be obtained with these two methods only on high-gloss specimens. In all other cases, the measuring method must be selected on the basis of what information is desired: Is the difference in the interior of two specimens (difference due chiefly to pigments or dyes) wanted, or the total difference (including surface effects)? Differences in gloss will thus result in unequal color differences, not just unequal between Methods A and B but from one instrument to another (depending on the accuracy of the measuring geometry in the instruments). Special problems in colorimetry arise when coloring materials must be examined in media whose surfaces are not smooth or homogeneous but display more-orless regular textures and variable degrees of gloss. Again, Method A or B can be Table 6-1. Criteria for selection of measurement geometry given the type of sample and the measurement objective I

Bulk properties of sample

Suitable measurement geometries

1

Isotropically scattering, covering (covering lacquer, plastic)

d/8, 45/0

2

Anisotropically scattering

Goniospectrometer (45/0 and d/8; reliability of test is limited)

3

Transparent (sheet materials, films)

d/8 or d/0 in transmission; d/8 or 45/0 or goniospectrometer if applied on scattering substrate

4

Slightly scattering (sheet materials, blow-molded products)

Errors due to edge losses with thick samples; smaller measuring spot and larger illuminated spot recommended, or sample can be placed in the sphere, d/8, 45/0. For transmission measurements, d/8 or d/0. It is necessary to state clearly whether total transmission or directional transmission is at issue and to agree on method.

5

Inhomogeneous, cloudy, spotted

d/8, 45/0; large measurement port and multiple measurements. For constraints see I, 1 to I, 3.

6

Fluorescing

Use CIE standard illuminant D65; 45/0 or (if applicable) d/8.

7

Thermochromic

Monochromatic illumination, d/8, 45/0. Use flash illumination or, if using continuous illumination, wait for temperature equilibrium. For constraints see I, 1 to I, 3.

8

Phototropic

Monochromatic illumination, d/8, 45/0. For constraints see I, 1 to I, 3.

9

Slightly reflective

Polychromatic illumination, 45/0 (d/8 with gloss trap if applied behind glass and measured through glass). Computational removal of gloss contribution from surface reflection is problematic.

242

6 Measurement and Evaluation of Object Colors

Table 6-1. (continued) II Surface characteristics

Suitable measurement geometries Measurement objective: overall assessment (final inspection)

Measurement objective: bulk assessment of sample (inspection of coloring matter)

1

Glossy and smooth (lacquer)

d/8 with computational removal of surface reflection; 45/0

d/8 with computational removal of surface reflection; 45/0

2

Ideally matte

d/8, d/0, 45/0

d/8, d/0, 45/0 with computational removal of surface reflection

3

Matte, silkily reflective, textured (embossing sheets)

All instruments if surface d/8 with computational removal is identical; otherwise, go- of surface reflection only with niospectrometer or, if jus- closed surfaces (lacquers, etc.) tified, 45/0

4

With gloss haze

45/0

45/0 or d/8 with computational removal of surface reflection

5

After chalking

45/0, geniospectrometer

d/8 after polishing or lacquer application; computational removal of surface reflection

employed, but the 08 geometries should be preferred so that the azimuthal dependence will be minimized in the measurement. It is desirable to use circularly symmetrical irradiation, for example circular/0 or d/0 (see Table 6-1). Agreements between the interested parties must always take account of the following points: ± Whenever possible, the same model of instrument should be used, but in any case the same measuring geometry. If possible, a check should be made in order to verify that the selected geometry yields color coordinates that are compatible with visual evaluation. ± An attempt should be made to create color reference standards whose surfaces match as closely as possible the surfaces of the color specimens to be tested. ± Acceptability can be determined only on the basis of color sample collections that have been visually evaluated by experienced colorists. The collection of color samples must be large enough that measurements lead to statistically reliable limits on the acceptable color differences (see Section 6.5).

6.2 Practical Evaluation of Color Differences

6.2

243

Practical Evaluation of Color Differences

6.2.1 Preparation of Specimens Preparation of the dispersion must be preceded by proper sampling. This is done with a suitable sampling device such as a scoop or thief for solids and appropriate equipment for liquids of high and low viscosity*. Good dispersion is essential for testing pigments in vehicles. Various standards** afford guidance in the selection of test media and dispersing methods. The standards describe media and techniques suitable for testing the dispersion properties of pigments, but these are also valid for colorimetric testing. There are problems in the testing of pigments in latex vehicles, because reproducible measurements are virtually impossible in these media. If such tests are unavoidable, special care must be taken in the choice of vehicle and the preparation of specimens. A second group of standards covers the testing of pigments in plastics. These include a detailed description of how to prepare basic mixtures and specimens. In solvent-based systems containing more than one pigment (and frequently also in full-shade systems), flocculation can give rise to color changes (ªrub-out effectº), especially when mechanical force is employed during application and drying. This behavior can be utilized to indicate a tendency to unwanted flocculation in the Rub-out test: Apply liquid system to cardboard or sheet metal; after stated time under exhaust hood, rub part of surface with a finger until the color difference between rubbed and unrubbed surfaces has reached largest possible value and remains constant, as indicated by resistance to rubbing. From color measurements on rubbed and unrubbed surfaces, determine color difference*** (see Section 6.2.3). In the remainder of Part II, specimen preparation techniques used with a number of test methods are described in more detail.

6.2.2 Color Measuring All color measurements start with the reflection values for the color sample. In principle, any instrument used for color measurement includes the following main components: ± Illumination device ± Monochromator (or wide-band filter) * For standards see ªSamplingº in Appendix 1. ** See ªEase of Dispersionº in Appendix 1. *** See ªColor Differencesº in Appendix 1.

244

6 Measurement and Evaluation of Object Colors

± Sample holder ± Radiation-measuring device A common arrangement has the monochromator and sample holder interchangeable to give two distinct configurations (Fig. 6-9). In the chain lamp-specimenchromator-detector, the specimen is irradiated with polychromatic light; in the other case, irradiation is monochromatic. The light source may be a halogen lamp, a xenon arc lamp, or a xenon flash lamp. Heating of the specimen and resulting changes of color coordinates must be anticipated with the xenon arc lamp.

Fig. 6-9. Paths followed by light in colorimeters with (1) monochromatic and (2) polychromatic irradiation.

The instrument is calibrated with a black standard (hollow light trap) for the zero and a BaSO4 white standard* (see Section 2.1.2). For practical tests, working standards calibrated to BaSO4 (secondary standard) are usually employed as white standards for the ideal matte white surface. In Chapter 2, it was shown that color measurement can be reduced to determining x, y, and Y; this means, according to the equations presented there, the measurement of the CIE tristimulus values* X, Y, Z. The product R 7 S or R 7 S for reflection measurements, resp. t 7 S or T 7 S for transmission measurements, must be multi y, z (see Table 7-4) in order to obtain plied by the CIE color matching functions x, the three curves shown in the last row of Figure 6-10; X, Y, and Z are given by the areas under these curves. The areas, in turn, are equal to the integrals in equation (2.3), and because these admit of two different interpretations, there are two distinct types of measuring instruments: ± Tristimulus method (tristimulus colorimeters) The transmission curves of optical filters together with the lamp spectrum and etc., so that the measured intensithe detector sensitivity correspond to the S 7 x, ties yield the CIE tristimulus values after a simple calculation * See ªColorimetryº in Appendix 1.

245

6.2 Practical Evaluation of Color Differences

Fig. 6-10. Schematic representation of color measurement.

± Spectral method (spectrophotometers) The reflection curve is measured with a spectrograph. Built-in analog computers S 7 y, S 7 z, then inor internal or external digital computers multiply by the S 7 x, tegrate. Both types are used in colorimetry; the manufacturers have developed photometers, and recent years have seen improvements in them. A tristimulus colorimeter has, instead of the monochromator, three wide-band filters whose transmission curves combine with the source spectrum and the photometer characteristic to give the reflectometer values** R'x, R'y, R'z . The CIE tristimulus values are obtained directly from these values as R0 R0 X=Xn 0:798 x 0:202 z 100 100 0 Y Ry Z=Zn R0z =100

(6.1)

where Xn and Zn are the CIE tristimulus values of the CIE standard illuminant. (Because x has two maxima, X is made up of R'x and R'z ). In spectrophotometers, the monochromator uses optics (entrance and exit slits, prisms, interference filters, optical gratings) to split up the visible spectrum into bands 10±20 nm wide. Gratings and filters have completely displaced prisms in modern instruments, because of their higher transparency, constancy of optical dispersion, and lower manufacturing cost. Interference filters take two distinct forms: a single filter with fixed wavelength and a graded filter continuously traversing the ** According to the standards, reflectometer values are symbolized by R' (to distinguish them from reflection factors R); see ¹Photometric Properties of Materialsª in Apendix 1.

246

6 Measurement and Evaluation of Object Colors

spectrum. The bell-shaped transmission curves of interference filters, however, exhibit relatively large half-value widths (ca. 20 nm), so that deviations relative to gratings can occur in spectra having steep slopes. The sample holder is matched to the desired geometry, usually 0/d, 8/d, or 45/0. The light-measuring device, finally, can be either a photomultiplier (for low irradiation intensities) or a silicon cell (for higher intensities). Silicon elements process the input signals in quasi-parallel fashion, so that instruments so equipped can offer measuring cycles shorter than 3 s. In the past ± usually on grounds of cost and short cycle times ± tristimulus instruments dominated in the fields of production control and other applications as well. The situation has been changing since new technologies have made it possible Table 6-2. Sample computation based on color measurement. (Figures in italics represent handwritten entries.) CIE color notation a) Spectral method Wave- Refleclength tance

Pigment: test

b) Tristimulus method

CIE color matching functions

Reflectometer values (C/28)

l (nm)

R (l)

x C/2 (l)

R 7 x

y C/2 (l)

R 7 y

zC/2 (l)

R 7 z

400 420 440 460 480 500 520 540 560 580 600 620 640 660 680 700

0.0126 0.0125 0.0119 0.0119 0.0122 0.0125 0.0137 0.0176 0.0357 0.0967 0.1726 0.2072 0.2226 0.2403 0.2675 0.3010

0.044 2.926 7.680 6.633 2.345 0.069 1.193 5.588 11.751 16.801 17.896 14.031 7.437 2.728 0.749 0.175

0.0006 0.0366 0.0914 0.0789 0.0286 0.0009 0.0163 0.0983 0.4195 1.6247 3.0888 2.9072 1.6555 0.6555 0.2004 0.0527

0 0.085 0.513 1.383 3.210 6.884 12.882 18.268 19.606 15.989 10.684 6.264 2.897 1.003 0.271 0.063

0 0.0011 0.0061 0.0165 0.0392 0.0861 0.1765 0.3215 0.6999 1.5461 1.8441 1.2979 0.6449 0.2410 0.0725 0.0190

0.187 14.064 38.643 38.087 19.464 5.725 1.450 0.365 0.074 0.026 0.012 0.003 0 0 0 0

0.0024 0.1758 0.4599 0.4532 0.2375 0.0716 0.0199 0.0064 0.0026 0.0025 0.0021 0.0006 0 0 0 0

P CIE tristimulus values CIE chromaticity coordinates

:

10.96

7.01

1.44

F X

F Y

F Z

F x

X X Y Z 0.5649

y F

Y X Y Z 0.3613

R'x = 13.71 R'y = 7.01 R'z = 1.22

F X =0.7827R'x +0.1987R'x 10.721 + 0.242 = 10.96

F Y = R'y 7.01

F Z = 1.182 7 R'z 1.44 CIE tristimulus values

6.2 Practical Evaluation of Color Differences

247

Table 6-3. Sample computation of color differences. (Figures in italics represent handwritten entries.) CIELAB color coordinates p X 3 X=98:07

Pigment: test

0.4817

L = 116 7 Y ± 16

31.83

Y

p 3 Y=100

0.4123

a = 500 7 (X ± Y )

34.70

Z

p 3 Z=118:22

0.2296

b = 200 7 (Y ± Z )

36.54

Note: If radicand r ^0.008856 then: X = 7.787 7 r + 0.138 (similarly for Y and Z ) CIELAB color differences Reference (R):

Test (T):

D = T± R

L

30.71

31.38

DL

1.12

a

35.45

34.70

Da

± 0.75

b

35.62

36.54 p a2 b2

Db

0.92

DCab

0.14

Chroma difference

1.63

Color difference

C ab C ab

50.25

50.39

p DL2 Da2 Db2 q 2 2 jDHab j DEab DL2 DCab DE ab

aR bT

aT bR

DHab Sign jDHab j

1.18 +59.33 +1.18

Lightness difference

) Sign(60) = +1 + Sign ( < 0) = ±1 Hue difference

to build fast spectral instruments at competitive prices. Another factor here is that tristimulus photometers cannot tell metameric color samples apart, because these instruments do not recognize metamerism. After color measurements have been performed on the test and reference specimens, the X, Y, Z are transformed into the CIELAB system so that the color differences can be calculated for the full-shade determination. Practical (manual, so to speak) evaluations of colorimetric data for both tristimulus and spectral methods are illustrated in Tables 6-2 and 6-3. The values of the CIE

248

6 Measurement and Evaluation of Object Colors

color matching functions used here, are those from Stearns' 20 nm table* (see Chapter 3). The example shows very clearly the burden of computation that used to be necessary and has now been taken off the colorimetrist's back by the computer age.

6.2.3 Full Shade A standardized test of dry pigment powder is possible for white pigments**. In the procedure, the CIE tristimulus value Y can be determined as a way of characterizing the lightness of white pigment and filler powders in pressed form. A suitable powder press has to be used to prepare the tablets. The measured Y value depends on a number of factors (rate of pressing, degree of compaction, surface texture, etc.), so that specimen preparation conditions must be clearly agreed on. Naturally, the CIE tristimulus value Yof the powder has no power to indicate the lightness of the pigment in media; it is suitable ± at most ± as a supplementary receiving inspection method for pigments. Thus the colorimetric values obtained on such tablets are not in any way typical, for the color of colored, white, and black pigments must be evaluated in suitable media (binders, vehicles). This means that final paint and lacquer coatings as well as plastics can be evaluated by the methods. Full-shade testing is described in separate standards*** for black, white, and colored pigments. These also define the terms ªfull shadeº and ªmass toneº, which were formerly used inconsistently. A full-shade system is a pigment/vehicle dispersion with a single pigment, and the color of such a system in a optically hiding layer is called the full shade. In contrast, the mass tone is a full-shade system in a non-hiding layer. Thus no mass tone is unambiguously defined unless information is provided on the preparation, composition, application, and substrate; many mass tones can be made with the same fullshade system, differing in film thickness and substrate properties. A special role in pigment testing is played by the test media**** used, first because of their actual effect and second because the use of suitable media makes it possible not only to avoid certain problems (inadequate dispersion, flocculation, etc.; see Section 4.1.2) but also to achieve certain economies. Chief among the latter are time savings in the testing procedure; one time-saving step is the use of nondrying pastes as vehicles. In addition to the time saving, the measured values also gain in significance, because full-shade measurements on pigmented pastes exhibit much smaller preparation errors than those on dried vehicles. Other proposals for test systems and their preparation can be found in Section 6.2.1. A good vehicle for nondrying pastes (DIN 55983) is an alkyd resin, Alkydal L 64 (Bayer AG). This binder combines the advantages of easy dispersion with the suppression of any tendency for the pigment to flocculate. * ** *** ****

See ªColor matching functions in steps of 20 nmº in Appendix 1. See ªLightnessº and ªReflection Factorº in Appendix 1. See ªColor in Full-Shade Systemsº in Appendix 1. See ªCoating materialsº in Appendix 1.

6.2 Practical Evaluation of Color Differences

249

Preparation method: Mix 97 % by weight Alkydal with 3 % by weight Aerosil 200 (Degussa), taking steps to prevent dust losses. Pass the mixture through a triple-roll mill twice. Weigh out 3 g of this mixture and a quantity of pigment such as to give a PVC of 10±20 %. Put the Aerosil paste in the middle of the lower plate of an automatic muller, scatter the pigment on the test medium; work together with a spatula without applying pressure. Next, distribute the paste in dots or a circle about 35 mm away from the center of the lower plate. A useful marking technique is to place beneath the lower glass plate a ring-shaped paper pattern with an inside diameter of 40 mm and an outside diameter of ca. 100 mm. Add a 25 kg weight to the upper plate. Wipe as much as possible of the paste from the spatula onto the upper plate. Mull the paste in two stages of 25 revolutions each. Transfer the finished pigmented paste to a special paste film holder made of metal or polyamide (see Fig. 6-11) and draw down with the doctor blade included. Among drying systems (DIN 55 983), air-drying systems are preferred to stove-drying ones because the preparation errors are smaller in the first case. Espectially

Fig. 6-11. Paste film holder with doctor blade, corresponding to DIN 55 983 (dimensions in mm).

250

6 Measurement and Evaluation of Object Colors

good choices are Alkydal F 48 (Bayer AG) and URALAC 6008 (Scado GmbH), both in 50 % solution. URALAC does not require and additional dryer and dries in 1±2 h (see also DIN 53 238 Part 30); Alkydal has to have a dryer added. Preparation method: Weigh out 5 g of the test medium and the quantity of pigment to give a PVC of 10±20 %. Using an automatic muller, proceed as before. Apply hiding coats of the finished reference and test pigment mixtures to a suitable substrate (glass plate, metal sheet, contrast card, lacquered or aluminiumlined cardboard), employing the same procedure in each case; the use of a Bird applicator is desirable. Coatings are hiding if a coating applied on a black/white contrast substrate exhibits a color difference DE ab after drying. Measurement method: Using a suitable colorimeter, measure test and reference preparations in such a way that the measurement conditions for Method A (i. e., use of integrating sphere with no gloss trap, correction by subtracting surface reflection; see Section 6.1.2 are fulfilled. Depending on the configuration of the measuring apparatus, either the reflectance R or the reflection factor R is obtained (in tristimulus instruments, the reflectometer values R'x , R'y, R'z are obtained). The corrections for surface reflection must be subtracted from each such quantity. Evaluation is done with the CIELAB formulas, equations (2.5) to (2.14). Figure 6-12 shows a computer printout illustrating the calculations for a fullshade measurement on yellow iron oxide pigments. Special aspects in the evaluation for white pigments have already been discussed (Section 2.3.3). In this instance, it is preferable to state as the color designation the Program ªFULL SHADE COLOREDº Full shade of colored pigments, according to ISO 787-25 *************** Date: ..-..-.. Pigment: Iron oxide yellow Reference is A Test is B Binder: Alkydal L 64 PVC: 20 % Colorimeter, Standard observer: N.N., C/28 Measuring conditions: d/8 (incl.) Input: ******************************************************** R'(x) R'(y) R'(z) Reference 17.00 10.57 4.95 Test 15.96 10.39 5.26 Output:******************************************************* a* b* L* C*(ab) h(ab) Reference 34.6 38.3 30.8 51.7 47.98 Test 30.6 33.4 30.4 45.3 47.58 Color differences Delta Delta E*(ab) a* 6.4 ±4.0

Delta b* ±4.9

Delta L* ±.4

Delta C*(ab) ±6.3

Delta H*(ab) ±.3

Delta h(ab) ±.48

Fig. 6-12. Full shade, colored, yellow iron oxide (computer output).

6.2 Practical Evaluation of Color Differences

251

ªhue of near-white specimensº* and its strength Ds (eq. 2.15). Figure 6-13 presents an example for titanium dioxide pigments. Similar considerations apply for black pigments and gray coatings: The recommended statement of the result is ªhue of near-black (or gray) specimensº instead of color differences (Section 2.3.3). Another special point is the more stringent requirements on the colorimeter for the full-shade measurement of black pigments. These conditions, which are met by few instruments today, relate to the display (five decimal places for reflection measurements, three for CIE tristimulus values), zero adjustment (calibration with a hollow light trap as special black standard), and reproducibility (standard deviation of CIE tristimulus values less than 0.001). An example, based on a full-shade measurement of black iron oxide pigments, appears in Figure 6-14. Program ªFULL SHADE WHITEº Full shade of white pigments, according to ISO 787-25 **************** Relative hue of near white specimens ****************************** Date: ..-..-.. Pigment: Titanium dioxide Reference is A Test is B Binder: Alkydal L 64 PVC: 20 % Colorimeter, Standard observer: N.N., C/28 Measuring Conditions: d/8 (incl.) Input: ******************************************************* R'(x) R'(y) R'(z) Reference 94.52 93.91 91.48 Test 94.54 94.18 92.55 Output: ****************************************************** Color difference Hue Delta (E*(ab)) Delta (L*) Type Magnitude Delta (s) .6 .1 blue .6 Fig. 6-13. Full shade, white (relative hue of near-white specimens), titanium dioxide (computer output). Program ªFULL SHADE BLACKº Full shade of black pigments, according to ISO 787-25 *************** Relative hue of near black specimens Date: ..-..-.. Pigment: Iron oxide black Reference is A Test is B Binder: Alkydal L 64 PVC: 20 % Colorimeter, Standard observer: N.N., C/28 Measuring Conditions: d/8 (excl.) Input: ****************************************************** R'(x) R'(y) R'(z) Reference .491 .442 .471 Test .369 .348 .429 Output:***************************************************** Color difference Hue Delta (E*(ab)) Delta (L*) Type Magnitude Delta (s) 1.3 ±.8 blue green .9 Fig. 6-14. Full shade, black, black iron oxide (computer output). * See ªHue of Near-White Specimensº in Appendix 1.

252

6 Measurement and Evaluation of Object Colors

The full-shade determination of dyes in solution is accomplished with colorimeters capable of transmission measurements. The CIELAB evaluation is similar to that for nonluminous perceived colors. Determinations of CIELAB color differences are described, as secondary procedures, in a number of other standards, for example under methods for determining the thermostability of plastics*.

6.2.4 Special Problems Metamerism (see Section 2.2.2) is commonly of secondary significance for pigment testing, though in practice it is much more important and can therefore become a factor in special testing situations. In formulation (as also in the pigmenting of lacquers and paints), one often cannot simulate the reflection spectrum of a given color, because (among other reasons) to do so would require having an unlimited number of pigments on hand. Instead, one has to be satisfied with reproducing the three CIE tristimulus values, even though this means that the new color will match only for the precise illuminant used. Such ªmetamericallyº matched colors will therefore show differences between the ªdaylightº color (under CIE standard illuminant C or D65) and the ªincandescent light colorº (under CIE standard illuminant A). In order to describe how much the color equality of two objects under a certain illuminant changes on a change of illuminant, the metamerism index** is employed. The color difference between the originally matching colors under the new illuminant is expressed in the perceptually-based CIELAB system. Figure 6-15 shows reflectance curves for two metameric specimens.

Fig. 6-15. Spectral reflectance for two yellow specimens having the same appearance in CIE standard illuminant D65 for the 108 observer. * See ªPVCº, and ªThermosplasticsº in Appendix 1. ** See ªMetamerism Indexº in Appendix 1.

6.2 Practical Evaluation of Color Differences

253

Even more important in pigment testing is the variety of metamerism called ªgeometricº. While normal metamerism involves a change in color when the illuminant is changed, in geometric metamerism a color change is brought about when the irradiation or viewing geometry relative to the specimen is altered. A special form of geometric metamerism is encountered in the Silking effect, where the reflectance changes when the specimen is rotated about the surface normal. Several conditions must hold for the Silking effect to occur. The first condition is a anisometric pigment, one made up of acicular, bladed, or rod-shaped particles, whose scattering and absorption coefficients are different in the principal axis direction and perpendicular to this axis. What is more, the pigmented medium must be applied in such a way that the particles are oriented, that is, in a quasi-parallel arrangement. The Silking effect can be measured only in geometries involving directional fluxes (e. g., 45/0). In practice, the Silking effect can be rather a problem, for example producing the ªpicture-frame effectº when a painting job has been finished up by painting once more around the edge of a large area in order to equalize the coat. Thermochromism is the property of coloring materials that show changes in reflection with changes in temperature. When performing colorimetric measurements on thermochromic specimens, it is necessary to wait for temperature equalization or, better, to use an irradiation source that does not heat up the specimen (monochromatic source or flash lamps). The following method is a suitable way of testing for the effect: Measure specimen a number of times in succession without removing it from the measuring port. Determine color differences relative to first measurement and note the time up to which differences remain constant. It should be noted that thermochromism can also be pretended by a change in the moisture content of the specimen. Fluorescence occurs when absorbed radiation is reflected after a very short time (ca. 10±6 s) in the longer-wavelength visible. If the reflection is delayed for a longer time, the behavior is called phosphorescence. Both these phenomena come under the general heading of luminescence. Fluorescent coloring materials can be used in molecularly dissolved form or as fluorescent pigments. Often, fluorescent coloring materials in low concentrations are added to paints or inks to enhance their brilliance (ªoptical brightenersº); the attenuated fluorescence is not perceived as luminosity but as greater brightness or saturation. The exciting radiation can lie in a more-or-less wide range of wavelengths, between 350 and 550 nm, depending on the chemical nature of the colorant; similarly, the fluorescent radiation is generally not monochromatic. Media and coatings that contain fluorescent coloring materials are, in fact, self-luminous, at least to the degree that the reflection is caused by them. Nonetheless, they are treated as nonluminous perceived colors, that is, referred to a mat white surface, so that reflectances R 4 1 can occur. Fluorescent object colors also differ from ordinary nonluminous perceived colors in that the reflectance and color stimulus depend

254

6 Measurement and Evaluation of Object Colors

on whether the incident light contains sufficient exciting radiation. For this reason, fluorescent specimens must be irradiated with the illuminant to which the measured values will be referred, that is, under which they will be visually matched. The content of fluorescent radiation is proportional to the intensity of the exciting radiation, and so if the incident radiation is deficient in the exciting range then there will be little fluorescent light; as a consequence, the measured color will no longer match with the visual results. This means that specimens must not be monochromatically irradiated for the spectral method; hence the only candidate configuration is number 2 in Figure 6-9. Figure 6-16 presents curves for a ªrightº and a ªwrongº measurement; the absorptions can be seen clearly in the ªrightº curve.

Fig. 6-16. Spectral reflectance for a fluorescent red color, measured in a ªwrongº configuration (number 1 in Figure 6-9) and a ªrightº one (number 2 in Figure 6-9).

Furthermore, mirrors and lenses in the instrument, and particularly the integrating sphere, will more-or-less strongly alter the spectral makeup of the incident radiation and, as implied by the discussion just presented, can again lead to changes in the color loci. It is therefore recommended that Method B of Section 6.1.2 be employed for these measurements, but only in the 45/0 geometry. Lamps with a daylight-like spectrum can be used to irradiate the specimen, because daylight contains sufficient radiation in the ultraviolet near 400 nm. This is why high-pressure xenon lamps or xenon flash tubes are used in instruments. CIE standard illuminant C is not appropriate because it is deficient in this radiation; at present, illuminant D65 lacks a technical implementation that can be used for routine measurements. Metal-effect paints, also called simply ªmetallicsº, are made with metal-effect pigments (Section 1.2). Their color properties are governed mainly by specular reflection on blade-shaped pigment particles, which are relatively large in diameter (up to 20 mm) and are predominantly oriented parallel to the paint surface. The fundamental physical processes of absorption and scattering observed on pigmented coatings are here joined by specular reflection. The interplay and interaction of these three processes give rise to the attractive aspect of a metal-effect paint. The directional distribution of the returned radiation depends heavily on the irradiation

6.3 Test Errors

255

angle and the viewing angle, so that significant and abrupt changes of lightness and hue can occur (lightness flop, hue flop). There are major difficulties associated with unsolved problems in color measurement on metallics. To determine the overall behavior, goniometric methods would have to be applied on both the irradiation and viewing sides of the system; this would lead to a multitude of plotted curves or measured values. Rationalization will not be possible until the colorimetric characterization of such paints can be acomplished with a limited number of angle settings, but no theoretical general approach has yet been devised to this problem. The situation is not much better with regard to instruments, plainly because of the lack of theoretical initiatives. One goniometric instrument that used to be available has now disappeared from the market, and devices that can be set to at least certain predetermined angles are slow in coming out. The present state of the art comprises instruments with conventional features, but these permit only the study of special aspects. Given these circumstances, for example, the only way to acquire new information about the conditions for hue and lightness flop is to analyze the scattered and reflected components separately to whatever extent this is possible. Problems with nacreous pigments stem from the need to measure interference colors. This again involves an angle-dependent indicatrix, so that conventional colorimeters fall down. Only the beginnings of a approach to measurement exist now; development into routine lab methods will have to wait. Generally accepted techniques for measurements on metal-effect and nacreous pigments are not yet in prospect. The methods gap is due to a lack of both theory and apparatus. Unfortunately, there is an intimate interaction between theory and hardware. This example shows that even colorimetric problems cannot be solved until the right instrument is available.

6.3

Test Errors

6.3.1 Calculation of the Standard Deviation Ellipsoid A number of computer programs are needed for the calculations demonstrated in Section 2.4. These can be classified into four groups: ± ± ± ±

Calculation of the coefficients of the ellipsoid Visualization of the resulting ellipsoid Calculation of test errors and significance Calculation of acceptability

It is desirable to program these calculations for a suitable computer. The calculation of ellipsoid coefficients is preceded by measurements performed in a ªreproducibility seriesº of a least 20 color samples. This term refers to

256

6 Measurement and Evaluation of Object Colors

a series of preparations made in the same way with the same pigments. The program takes the CIELAB coordinates (two decimal places) as input and calculates the means and the standard deviation ellipsoid. First, the arithmetic means of the color coordinates a , b , and L are calculated. By substituting these means into the successive formulas, it calculates the barred values of the polar coordinates C ab and hab (to two decimal places) with equations (2.8) and (2.9).

Program ªSTANDARD DEV. ELL.º Standard deviation ellipsoid, according to DIN 55600 ********************** Date: ..-..-.. Pigment: Chromium oxide green Binder: Alkydal F 48 PVC: 10 % Dispersing equipment: Automatic Muller, 2*100 Rev. Colorimeter (Measuring conditions, Standard observer): N.N., d/88, C/28 Input: ************************************************************ Pigment is A No. a* b* L* 1 ±19.09 16.08 45.48 2 ±19.10 16.12 45.37 3 ±19.10 16.01 45.39 4 ±19.09 16.10 45.36 5 ±19.02 16.06 45.36 6 ±19.06 16.12 45.47 7 ±19.12 16.16 45.36 8 ±19.11 16.06 45.41 9 ±19.10 16.09 45.47 10 ±19.15 16.10 45.43 11 ±19.08 16.15 45.43 12 ±19.08 16.03 45.46 13 ±19.13 16.20 45.36 14 ±19.09 16.07 45.46 15 ±19.09 16.14 45.40 16 ±19.13 16.16 45.46 17 ±19.11 16.12 45.47 18 ±19.14 16.17 45.44 19 ±19.10 16.12 45.37 20 ±19.14 16.11 45.39 Output:*********************************************************** Means: a*= ±19.10 b*=16.11 L*= 45.42 C*(ab) = 24.99 h(ab) = 139.858 Ellipsoid (70 %): g(1,1) = 424.7 g(2,2) = 152.3 g(3,3) = 139.5 g(1,2) = 137.5 g(2,3) = 21.64 g(1,3) = 22.62 Fig. 6-17. Means and calculated standard deviation ellipsoid for 20 preparations of a chromium oxide pigment (computer output).

6.3 Test Errors

257

Next, the variances and covariances are calculated (equations 2.78 and 2.79) and arrayed to form the covariance matrix V (equation 2.80). The program now inverts the matrix (equation 2.81) to get G. Appropriate software is often available for matrix inversion on the computer; an individual sample calculation is presented here. The formula is gik = u^ ik =det V, where det V denotes the determinant of matrix V, u^ ik is the cofactor of element uik, obtained from matrix V by deleting the i-th row and the k-th column and taking the determinant of the matrix that remains, with the sign (±1)i+k. The program requests the desired probability, divides the coefficients by the appropriate significance level ds2cum (Table 2-4), and rounds the gik to four significant figures. It outputs the means and the coefficients of the standard deviation ellipsoid for the desired probability. The programming is not very complicated and can well be done on a mediumsized desktop computer. Figure 6-17 presents a typical printout. With the aid of such a program, the CIELAB coordinates for 20 preparations of a chromium oxide pigment have been transformed to the means and the coefficients gik of the standard deviation ellipsoid for a 70 % confidence interval. A (very detailed) sample computation is contained in DIN 55600-2. In this instance, the 70 % confidence interval means that 70 % of all measured values lie inside the ellipsoid, or that there is a 70 % probability of an individual measurement lying in the interior (see also Section 2.4.1).

6.3.2 Visualization of the Ellipsoid It has proved useful in practice to visualize the ellipsoid in the CIELAB color space. When comparing two series of color measurements, it is often not enough to state just the standard deviations associated with the measurements; detailed conclusions about a measurement or preparation method can be arrived at only when the location and orientation of the error ellipsoid in color space are accessible for comparison. Two programs are needed for this purpose: ± Calculation of principal axes ± Projection of the ellipsoid onto the principal planes of the CIELAB color space (plot program) For the calculation of principal axes, the gik of the ellipsoid become the inputs. The program first verifies that the coefficients do pertain to a ellipsoid (and not to a different second-order surface); this is done with equation (2.47). If the result is affirmative, the secular equation (2.51) is then solved, for example by the trigonometric method. From its roots la, lb, lc, the three principal axes of the ellipsoid are then obtained as vectors a, b, c, each expressed in terms of its Cartesian coordinates a , b , L (equations 2.45±2.48) and its three-dimensional polar coordinates r, j, W (equation 2.49). An example in the form of a computer printout is given in Figure 6-18. The calculation relates to the total error ellipsoid, which will be described more fully in

258

6 Measurement and Evaluation of Object Colors

Section 6.3.3. The three principal axes are expressed as vectors a, b, c, each with its components. Listed next are the three-dimensional polar coordinates (one length plus polar angles; see Fig. 2-14). A quick comparison of the lengths of the three principal axes shows that one is very long ( | a | = 0.1606) and two are shorter. One of the short axes ( | b | = 0.0762) is roughly 3.5 times as long as the other ( | c | = 0.02 133). The ellipsoid is thus shaped like a surfboard or a somewhat flattened cigar with an elliptical cross section; the long axis of the cigar is some eight times as long as the short axis and twice as long as the longer axis of the cross-sectional ellipse. The polar angles give the spatial orientation of the figure: The long axis (a) lies in the positive quadrant (a and b positive, j positive) of the color plane and also in the positive octant of the CIELAB color space (L and W also positive). It is nearer to be b axis than to the a axis of the three-dimensional coordinate system (j = 74.18 closer to 908 than to 08), and also somewhat nearer to the color plane than to the L axis of the coordinate system (W = 66.18 closer to 908 than to 08). Program ªSEMIAXESº Ellipsoid semiaxes, according to VÚLZ, Industrial Color Testing ********* Input: Ellipsoid coefficients*************************************** g(1,1) = 228,5 g(2,2) = 345,9 g(3,3) = 1835 g(1,2) = 104,7 g(2,3) = ±730 g(1,3) = ±344,1 Output: Semiaxes *********************************************** Vector a* b* L* Långe Phi Theta a b c

.0402 .0725 ±.00382

.1412 ±.02294 ±.00788

.0652 .00493 .01945

.1606 .0762 .02133

74.108 ±17.558 ± 115.838

66.088 86.298 24.258

Fig. 6-18. Calculation of principal axes of a total error ellipsoid (computer output).

Next we come to the plot program for the ellipsoid projections. After the gik are input, the coefficients of the three projected ellipses (in the a, b, a, L, and b, L planes, equation 2.60) are calculated along with the axes (equation 2.61) and the paired section lines (equation 2.65), and these results are output by the plotter*. Figure 6-19 presents an example, a plot of the total error ellipsoid from Section 6.3.3 and Figure 6-18. With some practice, one can gain an idea of the position and orientation in three-dimensional color space by examining the plot. Fig. 6-19 (left-hand side) shows the three projections, i. e. a vertical and two horizontal projections; these are superimposed to simplify the display (Fig. 6-19, right-hand side). The outermost points of the projections are connected in pairs by section lines (dotted). If a color plotter is available, each of the three projections can be drawn in a different color. * In all plots, the horizontal axis is named first and the vertical axis second; thus the phrase ªa*,b* planeº denotes the plane with coordinates a* (abscissa) and b* (ordinate).

6.3 Test Errors

259

Fig. 6-19. Total error ellipsoid represented by projections in the principal planes of the CIELAB color space (from 20 preparations).

As has already been shown, the ellipsoid represented here has the shape of a flattened cigar. The projections bear out the description just obtained: The b, L projection clearly shows the lengthwise orientation, and it together with the two others shows the flattening of the figure. It should be noted that the ellipse axes drawn are not identical with the principal axes of the ellipsoid but are merely their projections. In order to get a still better idea of the three-dimensional shape of the figure, the ellipsoid can also be represented in its own principal-axis system. As equation (2.53) suggests, the three axis lengths, in the form of their reciprocal squares, are simply substituted in equation (2.52) and g12, g23, and g13 are simultaneously set equal to zero. The plot for the total error ellipsoid transformed in this way is illustrated in Figure 6-20. It confirms what has been said about the shape of the figure.

6.3.3 Total Error and Its Components The total error of a colorimetric pigment test is made up of the error of preparation and the error of measurement. Because the error of measurement is commonly very small, preparation methods are crucial for the size and location of the total error ellipsoid. If the preparation error is too large, an attempt must be made to split it into several contributions so that error sources can be identified and eliminated.

260

6 Measurement and Evaluation of Object Colors

Fig. 6-20. Total error ellipsoid of Figure 6-19, each projection into its own principal-axis plane.

In the example under discussion, the color dispersions for the measurement of the total error are prepared by the paste method of Section 6.2.2. The measurement of the tristimulus reflectometer values R'x , R'y, R'z was carried out by Method A of Section 6.1.2 (88/d) as follows: Measure R'x , R'y, R'z on one preparation in quick succession. Measure the next preparation after about 2 min, and so forth. After every five preparations, measure preparation No. 1 in order to recalibrate colorimeter to the values acquired on this preparation at the outset. The differences between actual and nominal values in recalibration were always less than 0.05 reflectometer units. The reproducibility series (dispersions of a pigment) used to define the total error ellipsoid was independent of random variations after 20 preparations. Confirmation of this claim is obtained by comparing Figure 6-19, the ellipsoid containing all 20 preparations, with the ellipsoids based on groups of 10 from the 20 preparations (Figure 6-21 and 6-22). These total error ellipsoids were determined for pastes (binder Alkydal L 64) pigmented with a red iron oxide pigment (10 % PVC). In contrast to the total error, the error of measurement is supposed to show how much the measured values will differ when repeated measurements are done on one and the same preparation within a series; the cause of this error lies in short-term instabilities of the instrument. Place on the instrument, 20 times, exactly the same portion of a selected preparation (e. g., No. 1 of the pastes prepared for the total error ellipsoid of Figure 6-19). After each placement (at time intervals of 3 min), measure the reflectometer values R'x , R'y, R'z without recalibrating the instrument. Figure 6-23 presents an ellipsoid for the error of measurement derived in this way. It has a somewhat different appearance from the total error ellipsoid of Figure 6-19,

6.3 Test Errors

261

Fig. 6-21. Total error ellipsoid of the first 10 preparations from Figure 6-19.

Fig. 6-22. Total error ellipsoid of the last 10 preparations from Figure 6-19.

being more discus-shaped, flattened in the direction of the a , L diagonals. To reduce or eliminate the scatter of the measured values due to long-term instabilities of the instrument, the same procedure as described for the total error must be employed: Maintain a time interval of 2 min between every two measurements; recalibrate colorimeter after every five measurements. In addition, perform each of the 20 measurements for this measurement error ellipsoid in the two minute pause between every two of the 20 measurements for the total error ellipsoid. This methodology insures that the measurement error ellipsoid is contained inside the total error ellipsoid. The measurement error ellipsoid acquired in this way is shown in Figure 6-24. It is much smaller than the ellipsoid in Figure 6-23 and also differs in shape and orientation.

262

6 Measurement and Evaluation of Object Colors

Fig. 6-23. Ellipsoid of measurement error, with no recalibration of instrument (measurement interval 3 min).

Fig. 6-24. Measurement error ellipsoid contained in the total error ellipsoid of Figure 6-19. (Measurement interval 2 min, instrument recalibrated after every five measurements.)

Certain fluctuations in the values resulting from specimen preparation can be eliminated or at least reduced if they are caused by ± ± ± ± ± ±

Weighing errors Lack of constancy in dispersing Inhomogeneities due to flocculation or floating of pigments Surface defects produced when drawing down the pastes Temperature effects Moisture effects

A reduction in the preparation error can be achieved if the error components can be identified and the larger error contributions minimized through changes in the preparation process.

6.4 Significance

263

Fig. 6-25. Ellipsoid of preparation error, contained in the total error ellipsoid of Figure 6-19.

The gik values characterizing the preparation error are formed, as stated in equation (6.2), by writing the covariance matrices (total error minus measurement error) and inverting the resulting difference matrix. The relative contributions of preparation and measurement error to the total error can be determined by comparing the ellipsoids for the total error (Figure 6-19), the preparation error (Figure 6-25), and the measurement error (Figure 6-24). Note the differences in size, shape, and (in part) orientation of the ellipsoids in figures 6-24 and 6-25. The preparation error ellipsoid is nearly as large as, and also quite similar in appearance to, the total error ellipsoid of Figure 6-19 (surfboard); thus it can be said that the preparation error is the dominant constituent of the total error in this example. The preparation error can be splitted up further (eq. 2.84).

6.4

Significance

6.4.1 Calculation of Standard Deviations Now, with the equations in Section 2.4.3, there is no further difficulty in calculating standard deviations. The standard deviations of the color coordinates will be calculated on the basis of a test error ellipsoid gik associated with these standard deviations. It is advisable once again to write a program using equations (2.68) to (2.75). A printout appears in Figure 6-26; the program was tested on the reference from the color difference test with red iron oxide pigments (see below). When comparing standard deviations in order to evaluate errors, it should be kept in mind that the confidence intervals of the three dimensional normal distribution here are systematically different from the confidence intervals of the ordinary

264

6 Measurement and Evaluation of Object Colors

Program ªST. DEV. COORD.º Standard deviations of CIELAB coordinates, according to DIN 55600 Input: *************************************************** Pigment is Red iron oxide A Medium: Alkydal L 64 Dispersing: Automatic muller Colorimeter: Tristimulus Nr. 2 Means: a* = 27.02 b* = 19.76 L* = 39.40 C*(ab) = 33.47 (h(ab)) = 36.188 Ellipsoid: g(1,1) = 146.7 g(2,2) = 137.60 g(3,3) = 192.0 g(1,2) = ±50.49 g(2,3) = ±134.0 g(1,3) = ±30.52 Output: ************************************************** Sigma(a*) = .08 Sigma(b*) = .09 Sigma(L*) = .07 Sigma(C*(ab)) = .10 Sigma(h(ab)) = .188 Fig. 6-26. Standard deviations of color coordinates (computer output).

one-dimensional distribution. In the 3D case, we consider the 70 % ellipsoid, assuming the associated standard deviation equal to s, by analogy with the onedimensional case. In the 1D case, ca. 95 % of the measured values fall between twice the positive standard deviation and twice the negative standard deviation (+2s), but the situation with the 3D distribution is different: As Table 2-4 shows, replacing the 70 % with the 95 % confidence interval changes the value obtained to (7.81/3.665)1/2 s &+1.5 7 s. The other values of interest are found in a similar way; Table 6-4 offers a comparison. Table 6-4. Comparison of confidence intervals for one- and three-dimensional normal distributions. Confidence interval

1D

3 D (s = s (70 %))

70 % 90 % 95 % 99 % 99.5 % 99.9 %

+1.04 s & +s +1.64 s +1.96 s & +2 s +2.58 s +2.81 s +3.09 s & +3 s

+1 s = +s +1.31 s +1.46 s &+1.5 s +1.76 s +1.87 s +2.11 s &+2 s

The procedure for standard deviations of color differences is exactly the same. Another computer printout is given in Figure 6-27 (reference and test of a red iron oxide pigment). In the case of color differences, it is commonly not enough to state the standard deviations alone, especially when these are of the same order of magnitude as the measured values. It is important to ask whether a color difference is significant, in other words, to perform a test of significance. This will take account of the number of measurements from which the mean color differences were obtained.

6.4 Significance

265

Program ªST. DEV. DIFF.º Standard deviations of CIELAB color differences, according to DIN 55600 Input: ******************************************************* Standard is Red iron oxide A Test is Red iron oxide B Medium: Alkydal L 64 Dispersing: Automatic muller Colorimeter: Spectral Nr. 3 Means: Delta(a*) = ± .03 Delta(b*) = ±1.20 Delta(L*) = ± .71 Delta(h(ab)) = ±1.678 Delta(H*(ab)) = ± .96 Delta(C*(ab)) = ± .71 Delta(E*(ab)) = 1.39 Ellipsoid: g(1,1) = 135.7 g(2,2) = 99.50 g(3,3) = 484.7 g(1,2) = 36.37 g(2,3) = ±165.1 g(1,3) = ±190.0 Output: ***************************************************** Sigma(Delta(a*)) = .09 Sigma(Delta(b*)) = .10 Sigma(Delta(L*)) = .05 Sigma(Delta(h(ab)) = .148 Sigma(Delta(H*(ab) = .08 Sigma(Delta(C*(ab)) = .15 Sigma(Delta(E*(ab)) = .14 Fig. 6-27. Standard deviations of color differences (computer output).

6.4.2 Test of Significance In Section 6.3.3 is was shown that 20 preparations are ordinarily both necessary and sufficient for the calculation of standard deviations. The same applies to the test of significance. Once again, it is useful to write a computer program based on the information and formulas in Section 2.4.4. Such a program can be generated by combining our sample programs STANDARD DEV.ELL. for color differences (Figure 6-17) and ST.DEV.DIFF. (Figure 6-27). The procedure begins with values evaluated by the CIELAB method (Section 2.3.3), that is, test and reference are measured one right after the other. The covariances to be formed will depend on the sequence of measurements, since they are supposed to describe relationships between two distinct measured quantities. Thus the results will include not only colorimetric relationships (e. g., a and b are calculated from the same CIE tristimulus value Y, and in addition the CIE color matching functions from which the X,Y, Z and ultimately the a , b are formed may overlap considerably) but also common differences in the method of preparing the color samples as well as short-term fluctuations of the colorimeters. It is therefore necessary to leave the measurements in the order in which they were acquired, forming the differences between two successive measurements of test and reference. If, on the other hand, an earlier ellipsoid is used again for the reference and it is desired to dispense with the separate determination of the gik for the color-differ-

266

6 Measurement and Evaluation of Object Colors

ence ellipsoid, equation (2.72) can be employed again because there is no correlation between the measurements on the reference and on the test. First, as in Section 6.3.1, the means of the color measures aR ; bR ; LR ; aT ; bT ; LT ; and of the differences Da ; Db ; DL are formed. Because it is always the case that Da aT aR and so on, it is enough to obtain two of each triplet of means (of aR ; aT ; Da , etc.) by averaging, then simply use these relations to find the third. In series measurements against the same reference, the quantities aR ; bR ; LR are already in hand and all that is necessary is to form the means of the Da , Db , DL . This can be done when the covariance matrix is calculated, since the same sums are used in both cases. It should be pointed out again that only statistical fluctuations, in the sense of stochastically independent events, may enter into the variance and covariance calculation in the determination of standard deviations or significances. As a result, systematic errors, which lie outside the bounds of probability theory, must be carefully eliminated by appropriate means. Systematic errors include heating of the speProgram ªSIGNIº, Page 3 Significance of CIELAB color differences, according to DIN 55600 **** Output: Significance test*************************************** Number of measurements: n = 20 Conf. int. Color differences (abs.) Crit. value Color difference is 70 % 95 % 99 %

Delta(a*) Delta(a*) Delta(a*)

= .03 = .03 = .03

> .02 ^.03 ^.03

significant non-signif. non-signif.

70 % 95 % 99 %

Delta(b*) Delta(b*) Delta(b*)

= 1.20 = 1.20 = 1.20

> .02 > .03 > .04

significant significant significant

70 % 95 % 99 %

Delta(L*) Delta(L*) Delta(L*)

= .71 = .71 = .71

> .01 > .01 > .02

significant significant significant

70 % 95 % 99 %

Delta(C*(ab)) = .71 Delta(C*(ab)) = .71 Delta(C*(ab)) = .71

> .03 > .05 > .06

significant significant significant

70 % 95 % 99 %

Delta(h(ab)) = 1.678 Delta(h(ab)) = 1.678 Delta(h(ab)) = 1.678

> .038 > .058 > .068

significant significant significant

70 % 95 % 99 %

Delta(H*(ab)) = .96 Delta(H*(ab)) = .96 Delta(H*(ab)) = .96

> .03 > .04 > .05

significant significant significant

70 % 95 % 99 %

Delta(E*(ab)) = 1.39 Delta(E*(ab)) = 1.39 Delta(E*(ab)) = 1.39

> .03 > .05 > .05

significant significant significant

Fig. 6-28. Test of significance (n = 20; computer output).

6.4 Significance

267

cimen in the instrument during the measurement, miscalibration of the instrument, and other such constant and regular deviations. The standard deviation ellipsoid generated in the test of significance described here is valid for ± A given reference pigment with color locus aR , bR , LR ± A given binder ± A given dispersing method ± A given type of colorimeter All these items must therefore be noted every time a dispersion ellipsoid is calculated. If such an ellipsoid already exists, the procedure for determining the significance can also be applied to other color differences under the same conditions (i. e., same reference, same vehicle, same dispersing method, same instrument type). Figure 6-28 is a significance test listing for a red iron oxide pigment, based on measurements of 20 specimens (n = 20). It is worth mentioning here that Da* is so Program ªSIGNIº, Page 3 Significance of CIELAB color differences, according to DIN 55600***** Output: Significance test *************************************** Number of measurements: n = 1 Conf. int. Color differences (abs.) Crit. value Color difference is 70 % 95 % 99 %

Delta(a*) Delta(a*) Delta(a*)

= .05 = .05 = .05

^.09 ^.13 ^.15

non-signif. non-signif. non-signif.

70 % 95 % 99 %

Delta(b*) Delta(b*) Delta(b*)

= 1.12 = 1.12 = 1.12

> .10 > .15 > .18

significant significant significant

70 % 95 % 99 %

Delta(L*) Delta(L*) Delta(L*)

= .66 = .66 = .66

> .05 > .07 > .08

significant significant significant

70 % 95 % 99 %

Delta(C*(ab)) = .60 Delta(C*(ab)) = .60 Delta(C*(ab)) = .60

> .15 > .22 > .26

significant significant significant

70 % 95 % 99 %

Delta(h(ab)) = 1.648 Delta(h(ab)) = 1.648 Delta(h(ab)) = 1.648

> .148 > .218 > .258

significant significant significant

70 % 95 % 99 %

Delta(H*(ab)) = .95 Delta(H*(ab)) = .95 Delta(H*(ab)) = .95

> .08 > .12 > .15

significant significant significant

70 % 95 % 99 %

Delta(E*(ab)) = 1.30 Delta(E*(ab)) = 1.30 Delta(E*(ab)) = 1.30

> .14 > .20 > .24

significant significant significant

Fig. 6-29. Test of significance (n = 1, computer output).

268

6 Measurement and Evaluation of Object Colors

small for the higher confidence levels (95 % and higher) that it is no longer significant, while all the other color differences are still significant. Another example, this one for a single color measurement (n = 1) with an already existing dispersion ellipsoid, appears in Figure 6-29. The analysis is based on one measurement of the 20 in the same example. It should be noted that the critical values are higher, but the only additional rejection is for Da and confidence level 70 %.

6.5

Acceptability

6.5.1 Specimen Preparation Growing interest in colorimetric production control, not just for pigment but also for textile dyes, has slowed down the process of creating test methods based on proposals made in the literature. In any such method, two aspects must be given special attention: ± The preparation of color samples needed for matching ± The clear statement of task for colorists who take part in matching The determination of acceptability calls for a collection of samples. When testing the acceptability of pigments, full-shade systems (air drying systems) as discussed in Section 6.2.3, with side-by-side drawdowns of test and reference, can be prepared. It is recommended that color samples be created with systematic departures all around the color locus of the reference pigment. Such a group of samples might be prepared by adding to the reference small amounts of suitable pigments in the directions of the four color red, yellow, green, and blue, while seeking to remain in the a , b plane, that is maintaining DL = 0 (see Figure 6-30). This requirement comes about because lightness differences are weighted much more heavily in visual evaluation than are CIELAB chroma or hue differences of equal magnitude. Experience in matching tests shows that a lightness difference as small as | DL | 4 0.3 between reference and test will cause the color differences ± even if chroma and hue are equal ± to be deemed unacceptable. This point again calls attention to a weakness of the CIELAB system: Lightness differences are underestimated. In addition to the samples with pure hue-direction deviations, further samples with deviations in the lighter/darker direction should also be manufactured. The available set of samples must, of course, be sufficiently large. The number of samples to be matched can grow quite large if every one is laid next to every other one in the form of side-by-side drawdowns (like test and reference). An example: Suppose there are three difference steps in the four color directions and in each light/dark direction; then the total number of color samples including the reference is 3 7 6 + 1 = 19 (see Figure 6-30). If every sample is laid next to every other (19 7 18)/2 = 171 side-by-side drawdowns must be matched. The number of

6.5 Acceptability

269

Fig. 6-30. Color samples deviating systematically from a gray reference (the spacing between samples is greatly exaggerated for clarity).

ªdoubleº drawdowns increases rapidly with the number of deviating steps away from the reference. Adding just one more step in each of the six directions raises the total number of double drawdowns to (25 7 24)/2 = 300. Numbers of this order are also required because the orientation of the acceptability ellipsoid is initially unknown. It is therefore useful to do preliminary matches by colorists of a few typical drawdowns in order to determine rough acceptability limits. The difference steps selected on the basis of these preliminary trials should then extend out to twice the acceptability limits, so that the desired ellipsoid will definitely lie inside the region spanned by the samples. The trick of laying every color sample next to every other one not only increases the number of double drawdowns to be matched, but also permits a closer approach to the desired normal distribution. In any case, not too much importance should be attached to departures from the normal distribution that result from this procedure. If the requirement of normally distributed measurements were taken too strictly, there would be virtually no possibility of applying statistical methods to practical problems, for intact normal distributions are quite rare in practice. Textbooks state that it is sufficient for the random sample to have a single-peaked distribution, and this will always be the case here because the reference color locus lies at the center of the ellipsoid.

270

6 Measurement and Evaluation of Object Colors

6.5.2 Matching and Color Measurement Well-defined conditions for color matching have already been implied by the requirement of a clear task statement for the colorists. Where the resultant acceptability ellipsoid is intended for later use in production control, say of pigments or paints, the colorists should be selected from those who are daily involved in batch inspection, so that they can take advantage of their experience in this form of matching. The difference between acceptability* and perceptibility of a color difference is that perceptibility characterizes the visual threshold for small color differences, while acceptability represents the range of color differences that manufacturer, purchaser, user, and consumer are prepared to accept. Acceptability must, further, be in accord with the variations resulting from the methods used to produce the coloring materials and media. If acceptability limits are set so narrow that they are smaller than the fluctuations due to process variations, it is no longer possible to make a product in conformity with the standard. If, on the other hand, they are set too wide, there is a danger that they will be rejected by consumers as excessive. All these relationships and insights become part of the experienced colorist's background ± and thus the task in hand is to embody this experience in the acceptability ellipsoid, so that the computer can be supplied with the information needed for colorimetric production control. The following points are crucial for color matching proper, and must be treated with special care**: ± The illuminant under which colors are matched ± The geometric conditions of color matching ± The physiological conditions of color matching The illuminant should be chosen from among the well-known CIE standard illuminants (Section 6.1.1). For artificial average daylight, corresponding to illuminant D65, the standard gives a method for determining the quality of the lamp spectrum with the help of test color pairs. A factor working against the use of illuminant D65, however, is that no satisfactory technical implementation has yet been devised; CIE standard illuminant C is better realizable. The lamp service time must be monitored (elapsed time indicator). The geometric conditions have to do with the direction of incidence and the viewing direction (e. g., 08 incidence and 458 viewing), the aperture angle of the irradiation, and the position and size of the specimen. Physiological conditions include the visual capabilities of the viewer (ability to distinguish color, color-normality), the luminance level, the state of adaptation of the eye, the surroundings (e. g., gray, CIE tristimulus value Y = 25), and the field of view. * The use of the term ªtoleranceº in place of ªacceptabilityº is sometimes noted. This usage is not recommended, because tolerances correspond just as well to perceptibility. ** See ªColor Matchingº in Appendix 1.

6.5 Acceptability

271

The conditions listed here must be fixed exactly; they should correspond to the situation previously existing in coloristic-visual production control. It is helpful to have a suitable matching room (light box) painted gray on the inside, in which appropriate light sources and a pivoting specimen stage with angular scale are mounted. In matching, all the double drawdowns are shuffled at random like a deck of cards, then matched in a single pass. The color samples are arranged by the colorist in two groups: ± Conforming with the standard (ªYesº), that is, accepted ± Not conforming with the standard (ªNoº), that is, not accepted In reports of matching trials of this type, it is sometimes stated that even experienced colorists suffer from a ªtestº psychosis and feel themselves in a stress situation as a result. The consequence is usually an excessively strict set of decisions, that is, too many rejections. To counter this effect, it may be useful to allow two passes for matching the samples. In the first pass, the task is to classify as ªcolor difference perceptibleº or ªnot perceptibleº. In the second pass, the actual task is set: to classify as ªcolor difference acceptableº or ªnot acceptableº. In this way, the colorist is enabled to differentiate better between color differences that he can just see (though this question is not asked) and color differences that he does perceive but just regards as conforming. These two passes can be combined into one if the colorist is asked to form three groups: ± No difference perceptible: accepted ± Conforming with the standard despite difference: accepted ± Not conforming with the standard, difference too great: not accepted The first and second groups together form the ªYesº group; the third is the ªNoº group. The number j of ªYesº evaluations is tabulated for each of the numbered samples. Naturally, special care is necessary in color measurement as well, because any error made in this operation can lead to incorrect decisions later on in colorimetric production control. The requirement must be that the color measurements take place within a short time of matching by the colorist, because samples may be subject to color changes due to aging phenomena. It is desirable to sandwich the matching task between two color measurements, whose results should be averaged. Every individual measurement is tabulated under the same sample number as in matching.

6.5.3 Evaluation and Example Calculation of the ellipsoid coefficients with the likelihood function of equation (2.87) requires an appropriate computer program. Finding the maximum amounts to determining the zeroes of the partial derivatives of ln M. All methods for finding parameters by iteration, such as Newton's method (there is no difficulty in forming

272

6 Measurement and Evaluation of Object Colors

the second derivative), as well as other numerical methods, are candidates for this operation. Once the initial values for the gik and p are specified, the Da , Db , DL associated with specimen number i are input to equation (2.42) together with the number ji of ªYesº judgments: ds2 g11 Da2 g22 Db2 g33 DL2 2 g12 Da Db 2 g23 Db DL 2 g13 Da DL Aside from p = 0 the initial values for the iterative procedure should be as close to the expected values as possible given the approximate knowledge of the acceptability ellipsoid. This will prevent convergence problems. If little is known about the expected ellipsoid, it is also possible to begin with values g11 = g22 = g33 = 1 and g12 = g23 = g13 = 0. A calculation can take some minutes, depending on the number of double drawdowns, the number of colorists, the type of computer, and the iterative method chosen. As discussed in Section 2.4.5, this procedure yields the coefficients gik of the acceptability ellipsoid plus a ªfalse alarm rateº p = 1 ± q. This rate points to the reproducibility of the color-matching experiment; if one works carefully, it can be held as small as desired. If there are problems with convergence, different initial values for the gik should be tried. The resulting acceptability ellipsoid can, for example, form the basis for computer-aided colorimetric production control. The following approach seems practicable: The 50 % and 75 % ellipsoids are calculated by dividing the gik by the ds2den factors from Table 2-4. Two concentric ellipsoids result; these divide the color space into three regions. If a color locus is inside the inner ellipsoid, it is ªconforming to the referenceº; if it is outside the outer ellipsoid, it is ªnot conformingº. But if the color locus is in the region between the two ellipsoids, it can be identified as ªtentatively conformingº. The confidence limits of an acceptability test must not be confused with the confidence limits of the tolerances for mass-produced articles in production control (e. g., length of nails, cross-sectional area of thermometer capillaries). The 50 % confidence level here means that half of colorists will accept this specimen; the 75 % level means that three-fourths of colorists will accept the specimen. Accordingly, 50 % can be viewed as the limit of acceptability, since here there are equal numbers of ªYesº and ªNoº judgments. A specimen that more than half of colorists reject is thus rightly deemed ªnot acceptedº. What is more, the ellipsoids represent the result of psychophysical experiments (color matching by colorists), and so human shortcomings (errors, blunders, and prejudices) enter into them and ªblurº the acceptability limits. Ultimately, the uncertainty due to the significance, that is, the effect of the (much smaller) test error ellipsoid, must also be taken into account. These are the reasons for the recommended confidence limits; the ªtentativeº region defined by them provided a good buffer between the two effects (see also Section 6.5.4).

273

6.5 Acceptability

Fig. 6-31. Acceptability ellipsoids (projections).

Figure 6-31 presents an example of two such ellipsoids. The drawing was produced by a plot program as discussed in Section 2.4.2. Table 6-5 lists the ellipsoid coefficients. The use of a computer to determine conformity or nonconformity can then be implemented roughly as illustrated in the following examples. Suppose there are three specimens, with are to be tested for conformity to the standard. Their color differences relative to a reference are given in Table 6-6. Using the gik, the program calculates the squared distances from the reference ds250 % and ds275 %. These are entered in the right-hand columns of Table 6-6. The values indicate that Specimen 1 is conforming because ds275 % < 1 Specimen 2 is tentatively conforming because ds250 % < 1 and ds275 % > 1 Specimen 3 is not conforming because ds250 % > 1 Table 6-5. 50 % and 75 % acceptability ellipsoids for a pigment. Ellipsoid

g11

g22

g33

g12

g23

g13

50 % 75 %

2.063 4.97

0.520 1.253

9.83 23.69

0.558 1.345

0.0845 0.2037

2.069 4.99

Table 6-6. Inspection of three specimens for conformity to the standard. Specimen

Da

Db

DL

ds250 %

ds275 %

Judgment

1 2 3

0.2 0.2 0.3

0.3 0.3 0.4

0.1 0.2 0.2

0.38 0.76 1.05

0.92 1.84 2.54

Yes Tentative No

274

6 Measurement and Evaluation of Object Colors

In this way, the acceptability can be calculated by the computer and output as a ªYesº, ªNoº, or ªTentativeº on the printer. The form of the ellipsoids in Figure 6-31 once again makes it clear how much the lightness differences are underestimated by the CIELAB system. Strictly speaking, such a statement can be arrived at only with perceptibility ellipsoids, but in fact there is little doubt in specialist circles that acceptability is not entirely independent of perceptibility. Perceptibility ellipsoids in an intact color-difference system would have to be spheres in the color space; acceptability ellipsoids should be expected to display a greater similarity to a sphere. Practical trials have shown again and again that this is not the case. Accordingly, in no case known up to the present can the acceptability be characterized by citing a DE ab value alone (corresponding to the radius of this sphere). Often the agreed-on limits include not only DE ab but also the components DC ab and DH ab . One must, however, keep in mind that this expedient is nothing more than that, because such limits do not exactly divide acceptable from non-acceptable color differences. Figure 6-32 illustrates this statement clearly. If limits [DC ab ] and [DH ab ] were taken, the color locus P would be wrongly accepted; in reality, it should be rejected because it lies outside the ellipsoid. Thus it has to be stressed that a statistically correct division into acceptable and unacceptable can be accomplished only with the acceptability ellipsoid. In the field of standards development*, the first efforts are now being made to deal with the acceptability problem. In theses, however, on should perhaps see nothing more than preliminary attempts to establish the first solid methods. In a further step, the ªColorº subcommittee of the German Standards Committee (DIN) has repared a report titled ªMethods of Agreement on Color Tolerancesº (see [38] and [39] in Section 2.7). Its report should help remedy the information gap that now exists among manufacturers and users in this field. A trend that should not be emulated is the practice of some software vendors who deal with the acceptability of textile dyes but do not disclose the color-difference formulas or the test criteria used. One might well ask whether this secrecy is a attempt to mask the inadequate scientific basis for the algorithms! Even if it is not,

Fig. 6-32. Acceptability ellipsoid. [DC ab ] and [DH ab ] are agreedon limits. The color locus P is wrongly judged conforming to the standard. * See ªColor tolerances for automative paintsº in Appendix 1.

6.5 Acceptability

275

the result is very negative because it prevents discussion of the systems, possible recommendations for improving the color-difference formulas, and ± ultimately ± advances in what is today the most important specialty area of our field.

6.5.4 Acceptability and Test Errors It has been shown that the acceptability ellipsoid is a useful criterion for the approval of color formulations, since it decides what color differences are tolerated. The test error ellipsoid (total error ellipsoid, See Section 6.3.3), in contrast, tells only how well a color laboratory can perform the tests. Nonetheless, test errors are of some importance in acceptability testing, because from what has been said it should be clear that the acceptability ellipsoid can be meaningfully applied only when it is much larger than the total test error ellipsoid. The term ªtest error ellipsoidº here denotes the 2 s ellipsoid, whose confidence interval roughly corresponds to the 3 s interval in the one-dimensional case (see Table 6-4). If one uses the method described in Section 6.5.3, with 50 % and 75 % acceptability ellipsoids, this problem does not arise. The reason is that the color measurements used in finding the acceptability ellipsoids already contained errors. It is true that the errors average out on the whole, but they do contribute to increasing the standard deviation, and thus the colorist's uncertainty. If, accordingly, the region between the 50 % and 75 % ellipsoids is regarded as a ªtentativeº region, this ªgray areaº takes care of the test error in the great majority of cases. As a quantitative treatment shows, the error ellipsoid in this case can have linear dimensions as large as 1/5 of those of the 50 % acceptability ellipsoid. If this is so, then the exact size and shape of the total error ellipsoid no longer play any decisive role, because the figure vanishes in the ªtentativeº region. This 1 : 5 requirement is more than satisfied in many practical cases because test errors are commonly much smaller. The question now arises what has to happen if the linear dimensions of the error ellipsoid are larger than 20 % of the acceptability ellipsoid. First, the color lab must make an effort to reduce the total error below this threshold. The measures by which this can be accomplished are described in Section 6.3.3. It is desirable to state the 1 : 5 limit in terms of the coefficients of the two ellipsoids. There is a linear factor of five between the two ellipsoids if the traces of the two ellipsoid matrices differ by a factor of 52 = 25: tr (GT) > 25 tr (GA) or, written out in full: A A gT11 gT22 gT33 > 25 gA 11 g22 g33

where GA is the acceptability ellipsoid, and GT is the test error ellipsoid. If this limit cannot be maintained, it will be necessary to combine the test error ellipsoid with the acceptability ellipsoid. Two cases must be distinguished:

276

6 Measurement and Evaluation of Object Colors

± A color difference that is just acceptable can be rejected as a result of test error, because it appears to be shifted outside the acceptability ellipsoid ± A color difference that is just unacceptable can be accepted as a result of test error, because it appears to be shifted inside the acceptability ellipsoid Only the second of these cases is dangerous, since it gives the appearance of acceptability when there is none. For this reason, the best way to deal with excessively large test error is to diminish the acceptability ellipsoid by the test error ellipsoid. This must be done through the covariance matrices, as shown i Section 6.3.3. We then have GA 1 VA

1 GT 1 GA corr ;

that is

VT VA corr :

This relation is illustrated in a obvious way by Figure 6-33. After subtraction, the matrices must be re-inverted so that the corrected acceptability ellipsoid. GA(corr) can be obtained. The correction must be carried our with both the 50 % and 75 % acceptability ellipsoid, using the same error ellipsoid.

Fig. 6-33. Schematic representation of the integration of the test error ellipsoid into the acceptability ellipsoid.

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

7

Determination of Hiding Power and Transparency

7.1

Measurement of Film Thickness

7.1.1 Selection of Method Any determination of hiding power, transparency, or color strength requires a knowledge of the spectral scattering and absorption coefficients; in other words, these must generally be determined first. For this purpose, paint or plastic layers are prepared and used in reflection measurements with suitable photometers. This information is enough for the calculation of the relative scattering and absorption coefficients (relative to a reference pigment). For the absolute quantities, which are needed for the determination of hiding power and transparency, reflection measurements alone are not sufficient: the thickness of the layer must also be determined, as the equations in Section 3.3.3 show. The significance of film-thickness measurement in the determination of scattering, absorbing, and hiding power and transparency is immediately evident from an error analysis: If one form the differential of ln S in equation (3.124), one sees that the percent error of the scattering coefficient dS/S = ±dh/h is absolutely equal to the percent error of the film thickness. Films used in such determinations often have to be so thin that the substrate has a marked effect on the reflectance; with highly pigmented media, films only 25±35 mm thick may well occur. If the error in the thickness measurement is 3 mm (a level that is not attained by all methods), the relative error will be ca. 10 %, and this will propagate in linear fashion to the scattering or absorption coefficient. The fact that the film-thickness measurement alone has such a heavy influence on the final result is not tolerable, however, because smaller errors would be necessary even if the only requirement imposed were that of conformity to a standard. What follows is a survey of methods commonly used to termine film thickness. These are also listed in standards*, along with brief descriptions and error ranges. We follow this classification, adding the pneumatic method and also creating higher-level groupings.

* See ªFilm Thicknessº in Appendix 1.

278

7 Determination of Hiding Power and Transparency

± Mechanical methods Dial-gauge or micrometer methods Pneumatic method ± Optical methods Wedge cut method Profile measuring method (only for transparent films with known refractive index; not nondestructive) Microscopic measurement of film thickness by cross section method (not nondestructive) ± Chemical methods Gravimetric method Titrimetric method (not nondestructive) ± Electrical and magnetic methods (require metallic substrates) Coulometric method Capacitive method Eddy-current method Magnetic method ± Methods based on absorption of scattering (not applicable to all pigments or all substrates) Beta-ray backscatter method X-ray fluorescence method The selection of methods suitable for the determination of the absorbing, scattering, and hiding power must be based on the following considerations: ± ± ± ± ± ± ± ± ± ±

Range: 0±2000 mm Accuracy: +0.5 mm (better still, +0.2 mm) Noncontact measurement (no contact with the film) Nondestructive measurement Measurement on small areas, under 4 mm2 Measurement in same film areas where photometric measurements are performed Measurement independent of vehicle and pigment, pigment volume concentration, and film surface quality Method suitable for opaque black/white glass plates between 2 and 8 mm thick as substrates Measurement of mean film thickness (i. e., for films with no smooth surface) possible if necessary partly or fully automated measurement with printout of results

These requirements imply right away that most of the methods listed above are not candidates. A short list includes just four methods: dial-gauge/micrometer, wedgecut, gravimetric, and pneumatic. All other techniques are unsuitable, chiefly because they are not nondestructive or do not permit the use of glass plates as substrates. Nor do the other methods satisfy the accuracy requirements. The first three

7.1 Measurement of Film Thickness

279

of the short list methods, indeed, do not entirely fulfill some of the requirements (in particular, errors of measurement are too large; what is more, the dial-gauge/micrometer and wedge cut methods also require the destruction of the film, if only in small areas), as will be discussed in depth.

7.1.2 Gravimetric,Wedge Cut, and Dial-Gauge/Micrometer Methods The basic procedure in the gravimetric methods is to determine the mass of the film per unit area by weighing, in a analytical balance, a known area of the substrate with and without the film and taking the mass difference. Since the density of the coating material at the time of weighing is known, the mean film thickness can then be calculated. The overall uncertainty of the method is around +5 %; film ranging from under 1 mm up to 1 mm in thickness can be measured. These methods have some drawbacks that make them more difficult to use and, in terms of accuracy and speed, severely limit their application in determining the scattering coefficient, absorption coefficient, and hiding power. They are integral methods yielding only a mean film thickness over a large known surface area: Thickness variations cannot be detected and characterized; in other words, these methods do not meet the test that the thickness should be measured where the reflection measurement is done. What is more, the limited relative sensitivity of commercial analytical balances means that the accuracy is strongly dependent on the weight of the substrate. For example, the balance must have a relative sensitivity better than 2 7 105 (e. g., 1 mg in 200 g) if 1 mm variations are to be determined to 10 % accuracy on glass substrates. Another problem with these methods is that the coating density must be exactly determined or calculated; in pigmented coatings, this usually means that the PVC, the density of the pigment, and the density of the medium must be known. In the wedge cut method, a sharp cutting tool is used to make a scratch in the film, creating a wedge-shaped cut with a certain inclination angle. The specimen is placed under a measuring microscope or profile measuring microscope and the horizontal dimension of the cut is measured. From this measurement and the known section angle, the film thickness is calculated. The uncertainty is around +10 %, and films from 10 mm to 2 mm thick can be measured. In coating systems, it is also possible to measure the thickness layer by layer, provided the layers can be distinguished by color or structure. Of-the-self instruments ± a cutting device and a measuring microscope ± can be employed. The cutter has a hard-metal blade (usually replaceable) having a known edge angle and a guidance system that positions the blade in a consistent way relative to the film surface. A suitable measuring microscope will have a magnification of 506 and a scale with 100 divisions. Commercial profile measuring microscopes have 200±4006 magnification. When a measuring microscope is used to deter-

280

7 Determination of Hiding Power and Transparency

mine the projection b of the section flank, the film thickness h is calculated from b and the section angle a (see Fig. 7-1). The film thickness h is read directly off the profile cut under the profile measuring microscope. A number of factors can falsify the results given by these methods: ± Surface roughness requires more individual measurements if a representative average is to be obtained. The rougher the surface, the more uncertain the measurement ± Deformation of the coating occurs frequently when none-too-strong coatings are cut; as a result, the method cannot be used for such films ± Errors can also result from breaking of the cut edges, especially with extrabrittle paint coatings

Fig. 7-1. Wedge cut (schematic).

Even though the cut requires only a relatively small area, this method cannot really be classed as nondestructive, because the cut has to be made quite near the place where the reflection measurement is to be carried out. The dial-gauge/micrometer method involves measuring the height of the coating surface relative to a fixed datum plane and then measuring the height of the substrate after removal of the film. The difference in height gives the film thickness. This method has been reported to have +20 % uncertainty. Below 20 mm, it has a absolute uncertainty of at least +3.6 mm. Coatings from 3 mm up to several mm thick can be measured. A commercial standard instrument comprises a measuring table, a fixture for the specimen, and a dial gauge mounted so that it can be moved over the table. Any mechanically contacting instruments or suitable micrometers can be employed, regardless of whether measured values are acquired mechanically, optically, or electronically. The measuring area of the dial gauge is a sphere or spherical cap whose radius, for metrological reasons, should be as large as possible (at least 1.5 mm); the force applied must not exceed a maximum value (1.5 N). The requirements are even more stringent for the measurement of organic coatings, such as the ones of concern here: The radius must be ca. 30 mm, the force between

7.1 Measurement of Film Thickness

281

0.1 and 0.5 N. Ordinary varnish solvents or paint removers are used to remove the coating from the measurement area. Aside from not being nondestructive, this method has the drawback that the measuring device exerts a mechanical reaction on the object being measured, and the pressure is great enough to produce errors through local deformation of the coating even when the force applied is relatively slight. There are limits on how much the measuring sphere of the dial gauge can be enlarged, because otherwise a sphere with too large a diameter will measure only maximum values on rough surfaces, not the desired mean values over small specimen areas. In order to extrapolate to zero applied force, extensive series of measurements and costly calculations would have to be done.

7.1.3 Pneumatic Method The pneumatic method is really a variety of the dial-gauge method and almost ideally satisfies all the requirements of Section 7.1.1. It permits the nondestructive, non-contact, and also very accurate point-by-point determination of film thickness at locations where the film reflectances are also measured. The method is independent of the binder and pigment content and, in the case of rough surfaces, permits the measurement of the mean coating thickness in small regions, which is the quantity of interest in practice. Pneumatic distance measurement techniques are based on the fact that the volume of an air stream is governed by the narrowest cross section of the flow channel. Any change in the smallest cross section will alter the quantity of air flowing through the channel per unit time. In the pneumatic method of measuring film thickness, the air stream from a measuring nozzle is directed against the surface of the test film in such a way that the spacing between the film and the nozzle outlet is the most constricted part of the channel. With the substrate fixed in place, differences in coating thickness alter the smallest flow cross section. Two kinds of measurement are made on this principle, volume and pressure. The method described here employs the pressure principle, because the components available on the market for this method are more resistant to wear and less susceptible to malfunction, over a wider linear range, than the ones available for the volume method. In the pressure method, the pressure drop is measured within the air stream ahead of the exit from the nozzle. The pressure drop is a function of the flow rate and thus of the slit size, that is, the clearance between the nozzle and the coating surface (Fig. 7-2). Off-the-shelf instruments (for other purposes) offer transformation ratios of up to 2 7 104 ; that is, a difference of 1 mm results in a 20 mm shift in the manometer water level. Special models have accuracies down to 0.025 mm. Figure 7-3 is a diagram of a pneumatic instrument for measurements of film thickness. The names of the part are indicative of their functions. The ball-bearing posts (2) insure plane-parallel movement of the nozzle guide plate (3) over the

282

7 Determination of Hiding Power and Transparency

Fig. 7-2. Pneumatic measurement of film thickness (schematic diagram of pressure method).

Fig. 7-3. Apparatus for pneumatic measurement of film thickness. 1, baseplate; 2, ball-bearing guides; 3, adjustable nozzle guide plate; 4, top plate; 5, handwheel (or servomotor); 6, glass flat held in place by point supports and edge stops; 7, four measuring nozzles; 8, precision inductive dial gauge.

baseplate (1), exact to +1 mm. The column assembly and the measuring nozzles are available commercially (see [26] in Section 3.7); the apparatus as a whole must be shop-fabricated. To determine the scattering and absorption coefficients or the hiding power and transparency of paint films, black or white plane-parallel glass plates (100 mm 6 100 mm 6 5 mm) are used. The reflectance of the applied coating is measured on each of four circular regions; the thickness of the paint film is then measured at four fixed points in the same regions, with the four nozzles of the

7.2 Scattering and Absorption Coefficients

283

pneumatic apparatus. The glass plate rests on three points in the apparatus and is fixed in place by three edge stops. Because the linear range of the nozzles (Fig. 7-2) is not wide enough to give the needed high sensitivity at the coating thicknesses encountered in practice, the pneumatic nozzles are used solely as null indicators. The nozzle guide plate is lowered to a constant, specified distance away from the coating surface. The actual clearance measurement is done separately, with a precision inductive dial gauge to the side of the glass plate; over a linear range of up to 2 mm, this guarantees a maximum error no greater than 0.02 mm. When the measurement is performed semiautomatically, the nozzle guide plate is lowered by hand and the value for the uncoated glass flat is recorded. In the subsequent measurement on the coated plate, this value is input by means of a digital setpoint adjuster. In the fully automatic device, the plate is raised and lowered by a servomotor controlled by the nozzles. The absolute film thickness is output in analog or digital form(with the aid of an analog-digital converter). High accuracies can be achieved with the pneumatic method. The absolute error of measurement can be held under 0.3 mm, which corresponds to coefficients of variation smaller than 1% for a film 30 mm thick. The accuracy is higher than that of the dial gauge method because no mechanical pressure is exerted on the specimen.

7.2

Scattering and Absorption Coefficients

7.2.1 Kubelka-Munk Coefficients S and K of White Pigments Methods for determining the scattering coefficient S are set forth in standards*. What these methods yield is not the absolute S but a relative (i. e., referred to a reference pigment) scattering coefficient per unit mass. Such results can be meaningfully compared only if the measurements are performed with equal masses of pigment or equal PVC values. Therefore, the S values obtained (m2/L) of the pigment/binder mixtures are then referred to the pigment mass concentration PMC, i. e., to the mass of pigment (m2/g). The exclusive use of relative values has to do with results from round-robin tests performed by DIN, which showed that absolute scattering coefficients could be reproduced comparatively well in the same laboratory but no adequate agreement was possible from one laboratory to another. In contrast, relative scattering powers showed quite satisfactory agreement. Those results are no longer consid* See ªScattering Power, Relativeº in Appendix 1.

284

7 Determination of Hiding Power and Transparency

ered entirely representative for present-day conditions, because essential technical elements of specimen preparation (such as dispersing equipment and methods) and color measurement (such as the calibration of instruments) have been substantially improved since they were reported. There are, accordingly, virtually no objections to absolute measurement today, even when the same techniques are employed. The standards distinguish between ± Black-ground method ± Gray-paste method (Because of its intimate link to the determination of lightening power in the Beer's law region, the gray-paste method will be described in Section 8.3.2) Black-ground method The black-ground method* is based on evaluating the Kubelka-Munk equations over a black substrate, as described in Section 3.3.3. The German standard initially leaves preparation methods (medium used, pigment concentration, dispersing conditions, coating application conditions) open ± these are to be agreed on between testing laboratories ± and limits itself to specifying the measurement and evaluation procedure. The pigment for test and the reference pigment are dispersed in the agreed-on medium. From the resulting pigmented media, a non-hiding coat over black and an optically infinitely thick coating are prepared. Instead of the reflectances in the middle of the visible spectrum, the CIE tristimulus value Y is measured for each coating. The calculation employs this Y value, plus either the pigment mass concentration (b) and film thickness (h) or the pigment mass per unit area (mF) of the non-hiding coat**; in either case, the methods of determination must be agreed on. This point shows a second reason that relative coefficients are attractive: the possibility of doing away with the little-loved measurement of film thickness. (In other words, if the pigment mass per unit area mF can be obtained without it, e. g., from the formulation, then the film thickness does not have to be measured.) An example of this procedure will be described further on. The colorimeter should be set up to measure the CIE tristimulus value Y. The parties must agree as to whether method A or B will be used for the measurement. Black glass plates having a plane surface and CIE tristimulus values Y 5 5 are to be used as substrates; these are available commercially. The test cannot be done with pastes (no well-defined film thickness), only with solid films or plastic films or plastic wafers. In the last two of these cases, a contact liquid (e. g., immersion oil) must be used to establish optical contact between the specimen and the substrate. * See ªScattering Power, Relative, Black-ground Methodº in Appendix 1. ** Not to be confused with the pigment surface concentration (see Section 4.1.4).

7.2 Scattering and Absorption Coefficients

285

Measurement method: Measure CIE tristimulus values Y for the coatings under standard illuminant D65 or C at several points of the coating. The number of points to be measured should be dictated by the size of the sample port and the size of the surface regions on which the film thickness and pigment mass per unit area are determined. Determine Y values to four decimal places and average the measured values on each coating to obtain Y1 (hiding coat) and Yb (non-hiding coat). Select the thickness of the non-hiding coat such that the difference between Y1 and Yb is a least two units. Evaluation method: Apply surface correction (eq. 3.11) to measured CIE tristimulus values Y, setting Y /100 = R (or R, depending on configuration) in each case. When measuring high-gloss specimens by method B of Section 6.1.2, add 0.04 to the R values before applying the correction. From the corrected reflectances R , calculate auxiliary variables a and b with equations (3.118) and (3.119). From a, b, and the corrected reflectance Rb , calculate to found decimal places the product Sh from equation (3.124): Sh

1 1 x1 Arcoth x ln b 2b x 1 where x

1

(7.1)

a Rb b Rb

Here Rb is the corrected reflectance over black, and a and b are the auxiliary variables in the Kubelka-Munk theory. Now, with Sh, b, and h or from Sh and mF first calculate the scattering coefficient per unit PMC b, SP = S/b: SP

S Sh Sh b bh mF

(7.2)

Here b is the pigment mass concentration (PMC) and mF is the pigment mass per unit area, g/cm2. The formula to be used from (7.2) will depend on whether b and h or mF is determined experimentally. The test and reference values of b or mF should be as nearly equal as possible. From the values SP,T (test pigment) and SP,R (reference pigment), calculate the relative scattering power per unit pigment mass as Sr

SP;T SP;R

(7.3)

Annexes of the German standard give very detailed examples of preparation, measurement, and calculation procedures. Annex 1 cites as test medium a longoil alkyd resin modified with linseed oil; as dispersing equipment, high-speed impeller mills and single-roll and triple-roll mills. The method used to determine pigment mass per unit area in this example is to detach 100 cm2 of the film with the help of a solvent, then combust and ignite the film.

286

7 Determination of Hiding Power and Transparency

Annex 2 contains another example with PVC-P (plasticized polyvinyl chloride) plasticizer containing materials. The dispersing equipment is a mixing roll; the film is brought into contact with the black glass plates by an immersion oil used as contact liquid. The pigment mass per unit area is determined gravimetrically, with the aid of the pigment mass portion known from the preparation. The following description of a test is based on this example and also relates to PVC-P materials. Preparation method: Test medium: PVC-P materials (basic mixture A*) Dispersing equipment: mixing roll with heating; speed 30 min±1, roll width 350 mm, roll diameter 150 mm Film preparation device: multi-platen press with heating Colorimeter for method A Substrate: black glass plate with CIE tristimulus value Y ^ 4 Contact liquid: immersion oil, refractive index 1.515 Formula: 1 g TiO2 pigment + 99 g basic mixture A for test and reference In double-roll mill, premix quantity of basic mixture at 1308C until plastic. Uniformly add pigment and mix (friction 1 : 1.2, total mixing time 8 min). Prepare two mixtures each from reference and test. Using spacers (1 mm thick) in the multi-platen press, press films of the pigmented media at 140 8C (pressing time 5 min, pressure 1500 N/cm2). Cut films into pieces 500 mm 6 40 mm. The CIE tristimulus values Y are measured in the way already described. The condition 2 ^ Y1 ± Yb ^ 6 is virtually fulfilled. For the layer of infinite thickness, pieces (at least four) were stacked on the black glass plate together with immersion oil until the CIE tristimulus value Y remained constant. The pigment mass per unit area was determined as mF = mf w/F, where w is the pigment mass portion, w = m / (m + mM), F is the area, m is the weight of pigment, mM the weight of basic mixture A, and mf the weight of the film. By way of example, Figure 7-4 shows a printout of the results from one such test. Note that the quantity determined according to the standard and in the above examples is the relative scattering coefficient per unit pigment mass. Theoretically, this is identical to the zero-th approximation of the lightening power P(0) W (Section 4.7.1). In comparing two pigments, it is often more informative to compare the relative scattering coefficient SV per unit pigment volume, which is obtained by multiplying the mass coefficient by the density ratio: SV = (RT /RR) Sr (see Section 8.3.2 for more detail). Thus, for pigments of equal density SV = Sr. As has been shown, the method described can be used without change for determining the absolute S and K values as well. Of course, the film thickness h must be measured, but once this is done, the scattering coefficient S is obtained by simply * See ªPVC, Plasticized, Basic Mixturesº in Appendix 1.

7.2 Scattering and Absorption Coefficients

287

Program ªS(Rel)º Relative scattering power of white pigments (Black ground method), according to ISO 787-24 *********************************** Date: ..± ..± .. Binder: PVC-P Apparatus: Double-roll mill Colorimeter: N.N., d/8, C/2 Multi-platen press Manufacturing method: Black glass plates Method C1.1.5, recipe X, Contact liquid Dispersing method: C Input: ************************************************** |Reference is TiO2-1 |Test is TiO2-2 | PVC: .312 % | PVC: .328 % | PMP: 1.00 % | PMP: 1.00 % Film |Area No |cm2

Mass g

Y(inf) Y(b) |Area | cm2

Mass g

Y(inf) Y(b)

1 2 3 4

3.606 3.671 3.443 3.447

82.7 83.2 82.6 82.8

4.461 4.173 3.825 3.673

86.5 86.5 85.9 86.0

|20.44 |19.71 |19.33 |19.03

80.8 81.3 80.5 80.9

|21.22 |21.32 |20.71 |20.28

83.1 83.2 82.6 82.8

Output: ************************************************* |Reference |Test Film |Pigment mass Scatt. coeff. |Pigment mass Scatt. coeff. Nr. |per area per unit mass |per area per unit mass |kg/m2 m2/kg |kg/m2 m2/kg 1 2 3 4

|.01764 |.01957 |.01781 |.01811

897.4 938.3 844.5 890.7

Means: 892.7 Relative scattering power: 91.5 %

|.02102 |.01957 |.01847 |.01811

765.5 833.9 814.8 852.6 816.7

Fig. 7-4. Relative scattering powers of white pigments (computer output).

dividing the experimental product Sh (eq. 7.1) by h. The absorption coefficient is then given by equation (3.121): K = S (a ± 1). If h is measured in mm, S and K will have units mm±1 = m2/L. Finally, it should be recalled that the scattering coefficient is a nonlinear function of the pigment concentration. The product Sh is then also a nonlinear function of pigment concentration, so that doubling the pigment mass per unit area and simultaneously halving the film thickness will not necessarily preserve the same value for Sh. The product will, however, be constant if both the concentration and the doubled concentration lie in the Beer's law region. The standard takes this point into account by prescribing that the PVC be reported. Outside the Beer's law range, it is not possible to calculate the lightening power (the mass ratio at which the scattering power of the test is equal to that of the reference; see Chapter 4) from the relative scattering power, because of the nonlinear relationship between scattering

288

7 Determination of Hiding Power and Transparency

power and pigment content. In general, then, there is non expectation that relative scattering powers will be in agreement with lightening powers for given test and reference pigments.

7.2.2 Kubelka-Munk Coefficients S and K of Black and Colored Pigments In principle, the method described in the preceding section is also applicable to determining the Kubelka-Munk coefficients of black and colored pigments. All that changes is that white glass plates can be used instead of black ones with dark pigments. It is still better to use commercially available black/white glass plates right from the outset. These measure 10 cm 6 10 cm and consist of a black part and a white part cemented together. The crucial point for a consistent film thickness over the black and white parts is that there must be no step at the transition. The CIE tristimulus value Y of the white part should be 80 +2, while that of the black part should be < 5. It is also desirable to use these black/white plates for the hiding coat; reflection measurements will quickly tell whether the Y difference between the coat over black and the coat over white is less than a significance threshold (e. g., 0.002). A point to remember is that the determination of the coefficients from a non-hiding coat over black or white, together with a hiding coat, is generally more accurate than the determination based on a film of equal thickness over black and white (see Section 3.7). The reason for this gain in accuracy is that the determination of the auxiliary variable a requires just one measurement in the first case (R1 , eq. 3.120) but four in the second case (Rb , Rw, R0b , R0w, eq. 3.122), so that the error of the reflection measurement acts on the error of a four times. The measurement of R1 should be dispensed with only when special difficulties are encountered in applying the hiding coat, for example with poorly hiding pigments. For a program, it is advantageous to ask first whether a measurement of R1 is available; if it is, a is calculated from R1 . A further gain in accuracy comes about because either Rb, R0b, or Rw, R0w can be substituted in equation (3.120) for S, provided that all four measurements have been done. It is desirable to take the pair that gives the smaller error in S, as was shown in Section 3.6.2 (eqs. 3.145 to 3.149). With this improvement, the program automatically looks for the best way to calculate S and K. As an aid to programming, the calculations are listed in full in Table 7-1. Accuracy problems in the determination of S and K can arise if the pigment has a very high absorption. In order to differentiate R and R0, the films must then be made very thin or the pigment concentration must be greatly reduced. There are, however, limits to how far either change can be carried: Usable films less than 30 mm thick are difficult to make, while excessive dilution of the pigment means that not all incident photons hit a pigment particle (ªsieve effectº; see Section 3.7), so that the premises of the Kubelka-Munk theory may not be fulfilled. In such

7.2 Scattering and Absorption Coefficients

289

Table 7-1. Formulas for calculating the error of S. Primed symbols denote partial derivatives (u / ux) with respect to the variable x identified by the subscript. y S

a R R0 R R0 b R R0

1

1 Arcoth y bh 1 b2 h y2

z

(3.121) (same as eq. (3.124))

1

(3.148, 3.149)

where 1) s sb R Rb R0 R0b y yb z zb 2) sw Rw R0w yw zw sR

z

sR0 z

1

1

2 a R0 R2 0 R R0 2

2 a R R2 R R0 2

(3.147)

where 1) R Rb R0 R0b z zb sR sRb sR0 sR0b 2) Rw R0w zw sRw sR0w R

dR 1 1 1 r2 R 2 dR R dR 1 r0 1 r2 dR

(3.146)

(derivative of Saunderson correction) where 1) R R 0b R R0b 2) R 0w R0w 3) R b Rb 4) R w Rw dS 2 s2R R 2 s2R R 2 0 0

where 1) dS dSb sR sRb sR0 sR0b R R b R 0 R 0b 2) dSw sRw sR0w R w R 0w If dS2b < dS2w then it is preferable to calculate S from R0b, Rb ; otherwise, from R0w, Rw.

(3.145)

Fig. 7-5. Flowchart for calculation of S (l) and K (l).

290 7 Determination of Hiding Power and Transparency

7.2 Scattering and Absorption Coefficients

291

cases, there is nothing to do but use other methods to determine S (e. g., in white or black pastes; see Chapter 8). If S and K are used in determining the hiding power or transparency, the strongly absorbing regions of the spectrum can be neglected entirely in the evaluation in certain cases since the hiding layer practically depends upon the weakly absorbing regions (see example below). Figure 7-5 presents a flowchart for the determination of S and K. In a long loop, the wavelength-dependent reflectances are input and checked for logic (e. g., R must always lie between R0 and R1 regardless of the substrate) and accuracy (the difference between R and R0 or between R and R1 must be at least 0.02), and the Saunderson correction is applied to all values. Next comes a conditional jump based on whether R1 is present or not. If all the other four reflectances are present (regardless of whether R1 is), the error calculation is done by two methods: over black substrate and over white substrate. The S (and K) values with the smallest error are output. An example will illustrate the method. Consider the determination of S and K for a paint containing a yellow iron oxide pigment. The paint was prepared in accordance with the ªdrying systemº method (see Section 6.2.3); the vehicle was Alkydal F48 and the PVC was equal to 1%. The measured reflection spectra Rb, Rw, R0b , R0w are shown in Figure 7-6. A printout of the results appears in Figure 7-7, while Figure 7-8 is a plot of the spectral S and K values. This is a highly instructive example, showing that the required accuracy makes it impossible to determine S and K at short wavelengths, at least for the selected concentration and coating thickness. The program has generated a message (ªPigment mass per unit area too largeº) that implies a suggestion to reduce the coating thickness and/or the pigment concentration. Where S is calculable, the last column in Figure 7-7 states whether the calculation was based on Rb or Rw . As in Section 7.2.1, the gray-paste method of ISO 787-24 should also be mentioned. Absolute scattering and absorption coefficients can also be determined by this method. Because of the close interrelationship with the relative tinting strength or lightening power, this method is discussed in Chapter 8.

Fig. 7-6. Reflection spectra of a yellow iron oxide pigment in a alkyd resin paint (reflectances are Rb over black, Rw over white, Rob for black substrate, R0w for white substrate).

292

7 Determination of Hiding Power and Transparency

Program ªS AND Kº Scattering and absorption coefficients (Black ground method), according to DIN 53164 ****************************************** Date: ..-..-.. Pigment: Yellow iron oxide A Binder: Alkydal F 48 PVC: 1% Preparation: Instruction 00 Film thickness measurement: gravimetric Colorimeter, Standard observer: N.N., d/8(incl) Input:********************************************************* Film thickness h: .0476 mm Lambda Rho(inf) Rho(b) Rho(w) Rho/0,b) Rho(0,w) nm 400 --.053 .053 .048 .671 420 --.056 .056 .048 .721 440 --.063 .063 .048 .760 460 --.068 .068 .048 .784 480 --.073 .073 .048 .801 500 --.092 .092 .048 .817 520 --.129 .154 .048 .838 540 --.192 .300 .048 .848 560 --.258 .504 .048 .857 580 --.260 .579 .048 .864 600 --.250 .583 .048 .872 620 --.236 .568 .048 .883 640 --.229 .568 .048 .893 660 --.219 .579 .048 .901 680 --.217 .608 .048 .905 700 --.218 .643 .048 .914 Output: ******************************************************* KUBELKA-MUNK Coefficients Lambda a b S K Calculated nm 1/mm 1/mm from: 400 420 440 460 480 500 520 540 560 580 600 620 640 660 680 700

Pigment mass per unit area too large Pigment mass per unit area too large Pigment mass per unit area too large Pigment mass per unit area too large Pigment mass per unit area too large Pigment mass per unit area too large 2.462 2.250 14.23 20.81 1.538 1.169 16.48 8.87 1.184 0.633 19.49 3.580 1.137 0.540 18.25 2.492 1.144 0.556 17.07 2.461 1.170 0.607 15.77 2.680 1.180 0.627 15.05 2.715 1.187 0.640 13.88 2.598 1.170 0.607 13.38 2.276 1.148 0.564 13.19 1.952

Rho(w) Rho(w) Rho(w) Rho(w) Rho(w) Rho(w) Rho(w) Rho(w) Rho(w) Rho(w)

Fig. 7-7. Determination of spectral S and K values (computer output).

7.2 Scattering and Absorption Coefficients

293

Fig. 7-8. Scattering coefficient S and absorption coefficient K for a yellow iron oxide pigment.

7.2.3 Four-Flux Coefficients s+, s±, k' The computational method described in Chapter 3 fully cover the region of technical interest with regard to accuracy and complexity. The two-flux (Kubelka-Munk) and four-flux calculations in ªexplicitº form (Section 3.2 and 3.3) are simple enough that they can be performed on a desktop computer (beyond fundamental operations, only exponential and log functions are required). There is, however, a mild constraint on reliability. On the other hand, ªimplicitº many-flux calculations, that is, based on numerical integration of the differential equations, are best carried out on a medium-sized or large digital computer; the results are as reliable as the best experimental data. Even if many-flux calculations are mathematically rather complicated and tedious, they have taken on a standard form since the renowned publications of Mudgett and Richards, so that most of the work can now be done with readily available subroutines. If is therefore most remarkable that only a few publications have dealt with even the experimental aspects of many-flux theories and the four-flux theory in particular. Our first example is taken directly from Mudgett and Richards ([17] in Section 3.9). The authors report how values of the coefficients s+, s± and k ' can be obtained from S and K with the calculable coefficients of the Legendre polynomials. This means that values for these coefficients can be derived from the KubelkaMunk coefficients with the aid of approximation formulas. What is more, however, the authors cite experimental data based on measurements on plastic wafers. The specimens in the first series were colored with a TiO2 (rutile) pigment; those in the second series, with a red dye. As a consequence, the scattering and absorption coefficients were measurable separately.

294

7 Determination of Hiding Power and Transparency

The measured transmittances and reflectances were compared with the values obtained by the authors from scattering and absorption coefficients that had been calculated by the method just mentioned, that is, from series of Legendre polynomials. The agreement was excellent. The coefficients for the surface reflection were also found close to the known values r0 = 0.04 and r2 = 0.6. The coefficients referred to S and K had the following values: s+/S 2.306, s±/S = 0.464, k'/K = 0.5 These figures provide strong confirmation of Kubelka's conjecture that the absorption coefficient in the parallel flux (k ') would be half as large as in the diffuse flux (K) (see Section 3.2.2). This hypothesis also holds to a good approximation for the backscattering coefficients (s±, S). As expected, the coefficient s+ is much larger than S ± more than twice as large. With these results, equation (3.19) can now be used to calculate m/S s+/S + s±/S + k'/S 2.306 + 0.464 + (a ± 1)/2 2.270 + a/2 which will be needed for the calculation of p and q with equations (3.30) and (3.31). Equation (3.90) with the specified values of Rdif,1 (or Rdif,1 after the Saunderson correction) then yields the reflectance Rg,1 for directional irradiation. We have used these data in calculating, for the first time, the (uncorrected) reflectances Rg,1 over the reflectance range of 0.05 to 1. There is no problem with expanding the scope in this way, because mixtures of TiO2 and the red dye can be prepared experimentally for any K/S. The results appear in Table 7-2, which shows the actually expected values (i. e., after Saunderson back-correction); as expected, only small differences (50.05) are seen between the reflectances for the directional and diffuse cases, with the latter values being somewhat higher throughout the series. This is also in agreement with expectations, for there is less scattering per unit path length for the directionally incident flux than for the diffuse one. The transfer of a photon from the forward to the backward direction thus requires, on average, a longer path length than in the diffuse case. What is more, experiment has not yet provided sufficiently sure confirmation for these differences between diffuse and directional irradiation; they are too large to be excused as ªuncertainty of measurementº or ªpoor linearity at moderate reflectancesº. The reason cannot be identified with exactness; undoubtedly it is a fact that the conditions ªdirectionalº and ªdiffuseº cannot be realized precisely enough. Conventional instruments allow measurements only with conical, quasi-parallel, or diffuse irradiation, and the d/d geometry cannot be implemented neatly. Other implications of the Mudgett and Richards work include the following: The phase function for a scattering medium can be obtained from Mie equations if the scattering is due to approximately spherical particles, or from pure scattering experiments if optically thin layers can be fabricated. Similar methods can be used for determining the absorption coefficient, insuring that the scattering and absorb-

7.2 Scattering and Absorption Coefficients

295

Table 7-2. Reflectances for diffuse and directional irradiation, calculated from data of Mudgett and Richards. Rdif,?

Rg,?

0.05 0.10 0.15 0.20 0.25 0.30 0.35 0.40 0.45 0.50 0.55 0.60 0.65 0.70 0.75 0.80 0.85 0.90 0.95 1.00

0.046 0.083 0.125 0.168 0.213 0.259 0.306 0.354 0.403 0.452 0.503 0.554 0.607 0.660 0.714 0.769 0.826 0.883 0.941 1.000

ing characteristics of the medium are described adequately for use in many-flux methods. For a simpler but less accurate calculation, the two-flux or four-flux method can be employed along with the empirical relations stated above for the effective scattering and absorption coefficients. Two problems that must be allowed for in two-and four-flux calculations relate to the angular distribution of the radiant flux in the interior of the medium. The internal surface reflection coefficients react directly to changes in this angular distribution, as do the effective scattering and absorption coefficients. What causes the errors in the two-flux calculation is that the radiant flux departs more from the approximate diffuse distribution as the K / S ratio increases. Such deviations occur in layers with low pigment concentration (e. g., translucent plastics) or very thin layers (e. g., printing inks). It might be possible to counter these effects with relatively simple empirical algorithms in many practical cases, for example in order to achieve better and faster convergence for color formulations. The second application example appears in a publication of Atkins and Billmeyer (see [23] in Section 3.9). The authors compared the results of four-flux calculations with experimental results on TiO2 specimens. They find a value of s+/(s+ + s±) = 0.84 for the forward scattering as a fraction of total scattering of a directional radiant flux. In the Mudgett and Richards example, the fraction was

296

7 Determination of Hiding Power and Transparency

2.306/(2.306 + 0.464) = 0.832; this represents a good result, although it must be kept in mind that the two results are not for the same TiO2 pigment. Finally, the literature does not report any test to determine s+, s±, and k ' using the formulas of Section 3.2.5. The computational derivation of these coefficients would greatly simplify the problems that arise with translucent specimens and in color formulations. Once coefficients were determined, the laborious procedure involving implicit many-flux theories could be rendered superfluous.

7.3

Transparency

7.3.1 Single-Point and Multi-Point Methods Transparency is significant for a wide variety of applications (transparent lacquers, printing inks, etc.). That uniform testing standards* have nonetheless been devised can be attributed to the fact that such applications have in common one physical phenomenon, transparence. What is more, in view of the broad range of applications, no preparation method has been prescribed, so this point must be covered by an agreement between the parties. It should be noted that transparent pigments have to be dispersed with special care, because their small particle size means that they exhibit extremely strong adhesion forces. A preparation method will be set forth in Section 7.3.2. The standards therefore stop with general provisions that must always be considered (geometry used in measurements, corrections to be applied, calculation of results). What is determined is the transparency number of a medium, which can be unpigmented or pigmented. If the specimen preparation conditions (vehicle system, application method, film thickness, pigment concentration) are held constant, transparent pigments can also be subjected to comparative evaluation by this method. The definition of the transparency number T is expanded somewhat from the definition stated in Section 3.5.1. In Figure 3-10, the film thickness (abscissa) could be replaced by the mass of the coating (at constant pigment concentration) of by the pigment concentration (at constant film thickness) without changing the nature of the curves. The h in equation (3.139) could then be replaced by the mass of the system per unit area (e. g., the ªink loadº in the testing of printing inks) or the pigment concentration. It goes without saying that the units of the transparency number T will vary from case to case. If, for example, the pigment mass per unit area (unit g/m2, especially suitable for testing of transparent pigments) is taken as the pigment portion, the transparency number will have units of g/m2 too, and Tm then tells how much pigment is required to coat 1 m2 of substrate so that the color difference is DE ab = 1. * See ªTransparencyº in Appendix 1.

7.3 Transparency

297

The test is performed by coating a black/white substrate and using a colorimeter to measure the color differences over the black substrate relative to ideal black. As a rule, the measured values have to be corrected before the color difference is calculated, because the coating filters the light incident on the substrate and reflected from it. This correction, which should take care of the departure of the real substrate from an ideally black substrate, is applied by preparing a drawdown of the same thickness on the white substrate. The transparency number is obtained from the color difference at one or more film thicknesses (if the pigment concentrations are equal) or at one or more concentrations (if the film thicknesses are equal). The black/white glass plates must fulfill the same requirements as in Section 7.2.2. With regard to the geometry of the colorimeter, care must be taken to minimize the effect of specimen surface characteristics on the measured value. On principle, method A of Section 6.1.2 can be used if the value of surface reflection is subtracted. In the case of high-gloss plane specimens, however, the measurement can be carried out by method B of Section 6.1.2 (45/0 or 8/d(ex)). For non-highgloss specimens, overlacquering is recommended; this step is essential in the case of bronzing specimens, particularly such as occur with printing inks. The needed correction of the measured values to eliminate the effect of the real black substrate is based on the filter action of the coating, mentioned above. This is found as the ratio of the reflectometer value R' (R' = R or R' = R) of the coating over white (R'w) to the value of the white substrate (R'0w). The reflectometer value for the black substrate (R'0b) is multiplied by this ratio and the product is subtracted from the specimen reflectometer value R'b : R0corr R0b

R00b

R0w R00w

(7.4)

If the measurement is done by the tristimulus method, the same computational scheme is applied to the reflectometer values R'x , R'y, R'z or the CIE tristimulus values X, Y, Z. The CIELAB color differences are calculated by the method of Section 6.2.2. Because the transparency number so defined is a function of h, its determination requires at least two specimens differing in film thickness (multi-point method); the transparency number obtained in this way is valid in the range between the two thicknesses h1 and h2, which should differ by at least ten times the standard deviation of the h measurement. With the color differences DE1 and DE2 measured on the two films, the transparency number becomes T

h h2

h1 DE2 h1

h DE1 DE1

(7.5)

where h is an arbitrary film thickness or pigment mass per unit area lying between h1 and h2.

298

7 Determination of Hiding Power and Transparency

If the two specimens differing in film thickness have roughly equal transparency numbers, that is, when the increase in color difference is approximately linear for small film thicknesses or pigment concentrations, the transparency number can be determined in a simpler way: The multi-point method reduces to the single-point method. The formula then simplifies to a form identical to equation (3.139): T

h

(7.6)

h DEab

These methods of determination have the drawback that the coloring power or tinting strength cannot be taken into the evaluation of two transparent pigments without more details. The standards therefore suggest determining transparency numbers after tinting strength matching for the respective film thicknesses or pigment concentrations. This problem will be treated more fully in the method (see the next section) based on the principle of spectral evaluation and using the transparencycoloring power and transparency-coloring degree defined in Section 3.5. An example of the two-point method follows. The test system is a transparent yellow iron oxide pigment in an alkyd resin, 1% PVC. The following were measured: Film thicknesses h1 = 0.035 mm h2 = 0.052 mm

Color differences relative to ideal black DE1 = 12.83 DE2 = 18.87

Now the two-point formula gives T

h

h 0:035 18:87 0:052 0:035

12:83 12:83

h 355:3 h 0:39

This implies, for a film thickness of, say, h = 0.045 mm, a transparency number of T = 0.002748 L/m2 = 2.748 mL/m2. If the only measured values available were those for the first point, h1 and DE1, the single-point formula (eq. 7.6) would yield T = 0.002727 L/m2 = 2.727 mL/m2. Multiplying this value by the PVC of s = 0.01 and the pigment density of R = 4.08 g/mL yields a transparency number related to the pigment mass of Tm = 0.1113 g/m2. This value is also obtained if the pigment mass per unit area is determined instead of the film thickness and substituted for h.

7.3.2 Method Based on Principle of Spectral Evaluation The calculation employs the equations of Section 3.6.3. To make the programming easier, a flowchart is presented in Figure 7-9 and the required formulas in closed form are summarized in Table 7-3. In addition to the equations needed for calculat-

7.3 Transparency

299

Fig. 7-9. Flowchart for determination of transparency by the principle of spectral evaluation.

Table 7-3. Calculation of transparency number, coloring power, transparency-coloring power, and transparency-coloring degree. Primes denote application of the operator (u/uh)h?0 to the respective unprimed quantities. R R s rl 1 r0 1 r2 Sl dl R k 2

Z rl

1 1

r0 Kl dl r2

(3.158) (3.159)

where 1) R s X s R k X k rl x l (CIE color matching functions) 2) Y s Y k y l Z k 3) Z s z l R s R s 7:787 Rn

(3.156)

1 R k R k 3 Rn

(3.157)

where 1) R s X s R k X k R s X s R k X k Rn Xn 2) Y s Y k Y s Y k Yn Z k Z s Z k 3) Zs Zn a 500 X

Y ; b 200 Y

where 1) a a s b bs 2) a k bk DE ab

(CIE stristimulus values of standard illuminant)

Z ; L 116 Y

(3.155)

L L s X X s Y Y s Z Z s L k X k Y k Z k

q a 2 b2 L 2

where 1) DE ab DE ab;s a a s b bs L L s L k 2) DEab;k bk a k

Transparency number: Coloring power:

T = 1000/DE ab;s

F=

DE ab;k /1000

Transparency-coloring power: L = T 7 F p Transparency-coloring degree: G = L L 2

mL 7 m±2 2

m 7 mL

(3.160)

±1

(3.141) L

(3.142)

300

7 Determination of Hiding Power and Transparency

ing the transparency number, those for the coloring power F, the transparency-coloring power L, and the transparency-coloring degree G are also listed. The determination of transparency will now be demonstrated for an example. A transparent red iron oxide pigment is prepared in an alkyd resin vehicle, and the preparations are applied in ± a non-hiding coat over white ± an opaque coat The reflection spectra are then measured. After the film thickness has been determined for the non-hiding coat, the Kubelka-Munk coefficients S and K can be determined from it and the two spectra (calculation outlined in Section 7.2.2). then, by using a program running on a desktop computer, the transparency number, coloring power, transparency-coloring power, and transparency-coloring degree are calculated. Preparation method: Precondition the test pigment at 1058; determine density* and loss on ignition** (needed for analytical determination of PVC of finished paint). Use Alkydal F481 in the following preparation: 87.5 g Alkydal, 52 % in white spirit 0.57 g Ca octoate, 4 % 10.3 g white spirit 0.9 g Ascinine R55 0.74 g Bayer OL silicone oil, 5 % in xylene Add dryer (to 95 g clear paint): 0.36 g Co octoate, 6 % in xylene 0.91 g Pb octoate, 24 % in xylene Calculate PVC from pigment density and loss on ignition for pigment and paint (both by titrimetric determination of iron content). At 7.5 % PVC, disperse in agate vessels on planetary mill. Terminate dispersion operation only when coarseness 510 mm***. To prepare non-hiding coatings, dilute paint to 1% PVC and apply by a spinning film spreader on(black/)white glass plates according to Section 7.2.2. After 24 h drying, coatings should have thicknesses between 30 and 70 mm. Measure film thicknessses with pneumatic device (method of Section 7.1.3). For hiding coat, dilute starting paint to 5 % PVC (because hiding is difficult to achieve with 1% PVC); apply in several coats, allowing to dry between coats (ca. 15 min required). Place in fresh-air cabinet dryer for at least 72 h dry completely.

* See ªDensity of Pigmentsº in Appendix 1. ** See ªLoss on Ignitionº in Appendix 1. *** See ªFineness of Grindº in Appendix 1.

7.3 Transparency

301

Measurement and evaluation method: Measure reflection spectra with spectrophotometer (method A of Section 6.1.2). Determine scattering and absorption coefficients in 20 nm intervals as in Section 7.2.2. Use CIE color matching functions from Stearns' tables* (Table 7-4 and 7.4 a; see also Section 3.6.7 and [32] in Section 3.9). Next, the S and K values obtained are input to the calculation of the transparency number and the other transparency quantities. Figure 7-10 is a printout of such a calculation. Program ªTRANSPº Transparency number, Coloring Power, Transparency, Degree of Transparency, according to VÚLZ, Industrial Color Testing ****************************** Date: ..-..-.. Pigment: Red iron oxide (transp.) B Binder: Alkydal F 481 Preparation: Instruction N.N. S and K evaluation: PVC 1%, gravimetr. film thickness measurement: .0473 mm Meûgeråt u. Lichtart/Beobachter: N.N., d/8(in): C/28 Input: ************************************************************* Lambda S K nm 1/mm 1/mm 400 2.187 133.9 420 2.474 146.7 440 2.268 126.5 460 2.057 102.5 480 1.557 84.3 500 1.556 71.8 520 1.311 59.0 540 1.357 46.4 560 1.193 28.54 580 1.038 15.62 600 1.003 8.77 620 0.963 5.91 640 0.921 4.38 660 0.887 3.424 680 0.869 2.747 700 0.840 2.160 Output: ************************************************************ TRANSPARENCY NUMBER T: 1.518 ml/qm COLORING POWER Phi: 24.86 qm/ml TRANSPARENCY-COLORING POWER L: 37.74 TRANSPARENCY-COLORING DEGREE G: 98.7 % Abb. 7-10. Determination of transparency number, coloring power, transparency, transparency-coloring power, and transparency-coloring degree of a transparent red iron oxide pigment based on the principle of spectral evaluation (computer output). * See ªColor matching functions in steps of 20 nmº in Appendix 1.

302

7 Determination of Hiding Power and Transparency

Table 7-4. CIE color matching functions in 20 nm intervals after Stearns (28 standard observer). C/28 y (l)

x (l)

400 420 440 460 480 500 520 540 560 580 600 620 640 660 680 700

0.044 2.926 7.680 6.633 2.345 0.069 1.193 5.588 11.751 16.801 17.896 14.031 7.437 2.728 0.749 0.175

±0.001 0.085 0.513 1.383 3.210 6.884 12.882 18.268 19.606 15.989 10.684 6.264 2.897 1.003 0.271 0.063

0.187 14.064 38.643 38.087 19.464 5.725 1.450 0.365 0.074 0.026 0.012 0.003 0 0 0 0

0.136 2.548 6.680 6.364 2.190 0.051 1.342 5.778 11.290 16.260 17.922 14.047 7.029 2.507 0.707 0.166

0.002 0.070 0.455 1.322 2.939 6.822 14.121 19.013 18.861 15.462 10.673 6.288 2.734 0.922 0.256 0.060

0.628 12.221 33.666 36.507 18.157 5.515 1.621 0.389 0.069 0.025 0.012 0.003 0 0 0 0

98.044

100.000

118.102

95.017

100.000

108.813

P

z (l)

x (l)

D65/28 y (l)

l (nm)

z (l)

Tab. 7-4 a. CIE color matching functions in 20 nm intervals after Stearns (108 standard observer). C/108 y (l)

x (l)

400 420 440 460 480 500 520 540 560 580 600 620 640 660 680 700

0.143 3.593 7.663 6.330 1.837 0.061 1.958 6.555 12.618 16.960 17.157 12.833 6.566 2.291 0.604 0.127

0.011 0.373 1.252 2.732 5.344 8.752 12.591 16.615 17.777 14.582 10.079 5.979 2.731 0.898 0.234 0.049

0.581 17.172 39.355 36.753 16.979 4.151 0.924 0.221 0.004 ±0.002 0 0 0 0 0 0

0.251 3.232 6.679 6.096 1.721 0.059 2.184 6.810 12.165 16.467 17.233 12.894 6.226 2.111 0.573 0.120

0.023 0.330 1.106 2.620 4.938 8.668 13.846 17.355 17.157 14.148 10.105 6.020 2.587 0.827 0.222 0.047

1.090 15.383 34.376 35.355 15.897 3.997 1.046 0.237 0.002 ±0.002 0 0 0 0 0 0

97.296

100.000

116.137

94.825

100.000

107.381

P

z (l)

x (l)

D65/108 y (l)

l (nm)

z (l)

7.4 Hiding Power

7.4

303

Hiding Power

7.4.1 General (Graphical Method) According to an ISO standard*, a ªhiding power valueº is used to characterize the hiding power of pigmented media such as paints and plastic films. The standard does not contain instructions for preparation, and it leaves open such questions as the method used to measure the film thickness. It is general in application (i. e., for both chromatic and achromatic coatings) and even offers a way of obtaining hiding power values on arbitrary contrast substrates**. The hiding power value is defined (consistently with Section 3.4.1) as the area of a well-defined contrast substrate such that a hiding layer can be created with a unit volume or unit mass of the pigmented medium. ªHiding layerº means that a stated hiding criterion ± here, an agreed-on color difference between the two fields of the contrast substrate supporting the layer ± is satisfied. In comparison with the definition in Section 3.4, however, the present definition of hiding power value is extended in the same way that we treated the transparency number (Section 7.3.1). There are, accordingly, two hiding power values: ± Dv in m2/L, the area such that a hiding layer can be created with 1 L of the pigmented medium ± Dm in m2/kg, the area such that a hiding layer can be created with 1 kg of the pigmented medium If the pigmented concentration is held constant, the hiding power values of pigments can be compared. Up to ca. 10 % PVC, the hiding power value can actually be corrected for the nominal concentration by linear interpolation (see Chapter 4, ªBeer's Lawº). In order to determine the hiding power value, coatings made of the pigmented medium and having various thicknesses are applied to the contrast substrate. After the films have dried, the color differences between the two contrasting fields are determined. A plot of color difference (ordinate) versus the reciprocal of the film thickness or of the mass per unit area (absciassa) is prepared. The hiding power value is obtained by going to the ordinate value of the agreed-on hiding power criterion and reading off the corresponding abscissa. The reason for using the reciprocals is that a quasilinear plot results; what is more, the abscissa, found as just described, gives the hiding power value directly with no further calculation. As a rule, the contrast substrates are the black/white glass plates described in Section 7.2.2, with nominal Y values of Y 5 5 for the black and Y = 80 + 2 for the white parts. The standard also permits the use of black/white contrast cards, but these can no longer be recommended because they amplify the errors of measure* See ªHiding Power, Pigmented Mediaº in Appendix 1. ** For other standards see ªHiding Powerº in Appendix 1.

304

7 Determination of Hiding Power and Transparency

ment to an unacceptable degree and also because pneumatic measurement of the film thickness is not possible with cards. A gray/brown contrast substrate is also permitted; the CIE tristimulus value are specified as ± Gray field: X = 30 + 2, Y = 32 + 2, Z = 33 + 2 ± Brown field: X = 9 + 1, Y = 9 + 1, Z = 8.5 + 1 If a hiding power value is to be determined on a free film, that is, a film that has no optical contact to a substrate, a hollow light trap is to be used for the black substrate (special black standard, see Section 6.2.2) and a BaSO4 white standard for the white (see Section 2.1.2). The mass per unit area of a free film can be determined very accurately by weighing a piece whose area has been measured. Most commonly, however, it is possible to produce an optical contact with the substrates described above. The film together with a suitable contact liquid (having approximately the same refractive index as the specimen) is placed on the contrast substrate, and a rubber roller is used to press it against the substrate and expel any included air. Just as described in Section 6.2.2 for full-shade determinations on colored media, the colorimetric measurement on the contrasting fields is done by method A of Section 6.1.2. The DE ab values are determined on at least four distinct films. One of the methods of Section 7.1 is used to measure the film thickness. If Dm is desired, the mass of the medium per unit area must be determined; if no free film is available for a direct determination, the formula mF = RM h makes it possible to calculate mF from the density RM of the medium. Now DE ab is plotted versus the reciprocal of h or mF, and a curve is fitted to the points. From the hiding power criterion (DE ab = 1 is preferred), a vertical is dropped to the horizontal axis and the hiding power value is read off. Figure 7-11 presents an example of the evaluation method (yellow iron oxide pigment, 5 % PVC in alkyd resin paint). The hiding power value obtained is 17.9 m2/L.

Fig. 7-11. Graphical determination of hiding power value Dv for a yellow iron oxide pigment.

7.4 Hiding Power

305

The hiding power value is strongly influenced by the substrate contrast, increasing with decreasing contrast. On the other hand, the final result is also affected by what hiding criterion is selected; as the critical DE ab decreases, the hiding power value also falls off. For this reason, the commonly used criterion DE ab = 1 represents a good compromise between the weaker contrast substrates often found in practice and the need for a lower critical color difference due to the lower perceptual threshold of the human eye.

7.4.2 Achromatic Case Another German standard* also defines a hiding power value as in the preceding section. As before, the pigment concentration, test medium, and dispersing must be agreed on between the parties. The hiding criterion is now the lightness difference DL = 1, because the small color difference between the coating over white and black can be set equal to the lightness difference in the ideal case (i. e., if the coating really is achromatic). Hiding and non-hiding coats of the pigmented medium for test are applied and the CIE tristimulus value Y are measured. From these results and the film thickness or the mass of medium per unit area (measured on the nonhiding coat), the hiding power value Dv or Dm is determined from tables, with formulas, or by a iterative calculation. The following method is an extension of the one found in the standard, specifically in two points (see Section 3.4.2): ± Inclusion of gloss in the computer-simulated matching ± Calculation of scattering and absorption components of the hiding power value. The discussion of the preceding section can be adapted to cover the preparation of the pigmented layers and the measurement of the CIE tristimulus values Y and film thickness or mass per unit area. The calculation of hiding power values was described fully in Section 3.4.2; R is now replaced by Y /100 as it was there. After application of the Saunderson correction to the measured values and calculation of the auxiliary variables a and b, the scattering coefficient and the factor a are calculated. The three approaches mentioned above can now be used: 1) The a table (see [24] in Section 3.7). Because a depends only on the CIE tristimulus value Y1 of the hiding coat and its degree of gloss g, the table is entered with two parameters R1 and g, and a is either read off directly or found by linear interpolation. The table is restricted to the range 0.7 5 R1 5 1, corresponding to 50 5 Y1 5 100. The standard also gives a table starting directly from the measured Y1 (i. e., bypassing the Saunderson correction), but this leaves g out of account; the a table in the standard has only the values for the g = 1 column. The table need not be reproduced here, because the second approach now to be described will be more convenient and offer sufficient accuracy. * See ªHiding Power, White and Light Gray Mediaº in Appendix 1.

306

7 Determination of Hiding Power and Transparency

2) Nonlinear regression equations. They are y0 a02 R1 a01 R1 a00

(7.7)

y1 a12 R1 a11 R1 a10

(7.8)

Once y0 and y1 are known, a is calculated from their values and g: a y0 + g ( y1 ± y0)

(7.9)

It has proved useful to split the region of interest (0.7 5 R1 5 1) into three parts: Region I: 0.7 ^ R1 5 0.9 Region II: 0.9 ^ R1 5 0.97 Region III: 0.97 ^ R1 5 1 The coefficients aik needed for the calculation are listed in Table 7-5. The formulas are quite accurate, with error less than 0.2 % in all cases. Tab. 7-5. Coefficients for the calculation of a (R1 , g) with the regression formulas.

a00 a01 a02 a10 a11 a12

Region I 0.7 ^ R1 < 0.9

Region II 0.9 ^ R1 < 0.97

Region III 0.97 ^ R1 ^ 1

0.88869 ±1.32952 0.47622 0.86519 ±1.28370 0.45315

1.30598 ±2.23071 0.96232 1.27680 ±2.17282 0.93288

5.53410 ±10.96049 5.46863 5.53121 ±10.95552 5.46579

3) Direct (iterative) calculation. The equations of Section 3.4.2 are used. Figure 7-12 gives a flowchart of the calculation along with all needed equations. In principle, the hiding power values can also be calculated for black and dark gray coatings; the algorithm must then include tests for the selection of the value function (R ± gr0 5 0.008856?) as well as formulas valid for the lower range. If, however, a method based on the principle of spectral evaluation is available (see the next section), there is no need for these modifications because the method is applicable generally to chromatic and achromatic layers. Finally, the hiding power values are calculated with equation (3.133). In the iterative procedure (3) with the equations of Section 3.4.3, there is no difficulty in calculating the scattering and absorption components of the hiding power. When the a table (1) or the regression formulas (2) are employed, computational aids are called for. The tabular solutions use equations (3.133) and (3.136): Dsca aS S ;

Dabs bK K bK (a ± 1) S

7.4 Hiding Power

307

Fig. 7-12. Flowchart for iterative determination of hiding power value of white and light gray coatings.

308

7 Determination of Hiding Power and Transparency

Table 7-6. The functions aS (g) (ªhiding power due to scattering aloneº) and bK (g) (ªhiding power due to absorption aloneº). g

aS

bK

0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9 1

0.042298 0.042222 0.042146 0.042070 0.041993 0.041917 0.041840 0.041763 0.041686 0.041608 0.041531

0.42342 0.41732 0.41071 0.40347 0.39542 0.38630 0.37571 0.36290 0.34841 0.34779 0.34779

Here aS and bK depend only on the degree of gloss g; Table 7-6 gives their values. If formulas are preferred, the two values are given by aS 0.042298 ± 0.000767 g

(7.10)

For bK, two cases are distinguished: g < 0.8063: bK ± (0.05986g + 0.04386) g + 0.42263 g60.8063: bK 0.34779 (independent of g)

(7.11)

The values from these equations differ by less than 0.3 % from the tabulated values. Parts 2 and 3 of the German standard give two very thoroughly worked-out examples of the determination of hiding power values for white specimens. The pigmented medium in Part 2 is an air-drying alkyd resin paint with a TiO2 pigment; in Part 3, a plasticized polyvinyl chloride (PVC-P) also with a TiO2 pigment. What follows here is a earlier example (TiO2 pigment in alkyd resin paint) with film thickness measurement by the gravimetric method; the computer printout appears in Figure 7-13. The hiding power value and its components are obtained with an iterative routine based on the flowchart of Figure 7-12. The calculation gives a = 0.05 861, the same result as found in the a table. Equation (7.9) for 0.9 ^ R? 5 0.97 (Region II) yields a = 0.05 864, which differs by 0.05 % from the calculated value. The hiding power value is then Dv = 14.17 m2/L in both cases. For the scattering and absorption components, equations (3.133), (3.136), and (3.137) give the same results as the iterative calculation: dsca = 71.2 % and dabs = 1.1%. One point in favor of using this method for white pigments is that the result is easily derived from tables or simple formulas. There is, however, another point

7.4 Hiding Power

309

Program ªHIDING WHITEº Hiding power of white and light gray media, according to DIN 55984 (extended method) *************************************************** Date: ..-..-.. Pigment: TiO2-Z Binder: Alkydal F 48 PVC: 27.23 % Preparation: Instruction PP Film thickness measurement: gravimetr. Colorimeter, Standard Observer: N.N., d/0 (incl.), C/2 degr Input: ************************************************************* Film thickness h: .0473 mm Gloss degree g (of Rho(b)): .764 Reflectances: Rho(b): .8030 Rho(inf): .8688 Output:************************************************************ Auxiliary quantities: a = 1.0018854 b = 0.061435 Scattering coefficient: S(v) = 241.73 l/mm Hiding power value: D(v) = 14.17 m2/l Scattering component: Delta(sca) = 71.2 % Absorption component: Delta(abs) = 1.1% Interaction component: Delta(int) = 27.7 % Fig. 7-13. Deterimination of hiding power value for a white paint containing a titanium dioxide pigment (computer output).

grounded in the hiding power criterion. The hiding power value obtained by this method will be the same as in Section 7.4.1 only with extrapolation to DL = 1 (instead of DE ab ) in the graphical evaluation. For a nearly white or nearly gray specimen, the chroma and hue differences between white and black should be of a higher order than the lightness difference, but this condition is not always adequately fulfilled. The effect is exaggerated because the CIELAB system underestimates lightness differences and overestimates chroma differences. As a result, the undertone in many cases becomes an effect of less than second order. This difference between the hiding power criteria manifests itself in the following way: Two specimens equal in lightness, one being a neutral white and the other exhibiting a slight yellow undertone, would have the same hiding power value over a black/ white contrast substrate if the evaluation were based on DL = 1, but if it were based on DE ab then the yellow-toned specimen would have a higher DE ab between black and white than the neutral specimen, since it would have a chroma difference DC ab contributing to the color difference DE ab . To make DE ab equal to 1, as specified by the criterion, the layer would have to be made thicker, and this would lead to a lower hiding power value. Accordingly, when comparing white pigments, it may sometimes be useful to determine the hiding power in accordance with the criterion DL = 1. In the evaluation with DE ab = 1, a yellow-toned specimen will therefore have a lower hiding power than a color-neutral specimen of the same lightness. The next section will show how this effect can show up in the scattering and absorption components of the hiding power.

310

7 Determination of Hiding Power and Transparency

A determination of the contrast ratio of white latex paints* is mentioned only peripherally. Such determinations tell nothing beyond whether a stated contrast over black and white is or is not attained at a given film thickness. They do not provide unambiguous information about what hiding power can be achieved or about the effectiveness of the paint.

7.4.3 Based of Principle of Spectral Evaluation The basis for determining the hiding power with the principle of spectral evaluation was treated in great depth in Section 3.6.2, which also presents the equations (repeated here in Table 7-7 as a programming aid). Figure 7-14 is a flowchart for the procedure including determinations of S and K (see Section 7.2.2). After the required data and the film thickness have been input, the program requests the needed reflectances as a function of wavelength in 20 nm steps. The CIE color matching functions are taken from Stearns' table (Table 7-4; see Section 3.6.2 and [32] in Section 3.9). In each pass through this first loos, the scattering and absorption coefficients associated with this wavelength are calculated and output. When the loop terminates, the second loop is performed; it iterates h up to the hiding coat. A suitable iterative method must be used; that is, the change in film thickness must be derived from the residual difference between the actual color difference and the nominal value 1. When a color difference of 1 has been reached (to the required accuracy), the reciprocal of the hiding film thickness is output as the hiding power value. In Section 3.6.2, Newton's method was also recommended for this calculation and the equations for the method were written out. Table 7-8 again lists these formulas as a programming aid; here the prime denotes a partial derivative with respect to h. The flowchart in Figure 7-15 shows, in the nested loop, the iterative calculation of the hiding power and its components in accordance with Table 7-8. An example (chromium oxide green) is given Figure 7-16; the reflectances of the substrates, of the non-hiding coat over black and white, and of the hiding coat are shown. Figure 7-17 is a printout generated by the program for the same pigment; the calculations of transparency, coloring power, and so forth have now been included. The program yields basically the same hiding power values as the procedure of Section 7.4.1. If, however, the procedure of Section 7.4.2 (achromatic layer) is used, departures may show up because of the DL = 1 hiding power criterion. The effect of the hiding power criterion on the final result was discussed in the preceding section, where it was stated that white specimens showing an undertone may have lower hiding power values than neutral white specimens of equal lightness if DE ab = 1 is selected as the hiding power criterion. A further consequence of this behavior is that the ªhiding power due to scattering aloneº, as calculated with the * See ªEmulsion Paintsº in Appendix 1.

7.4 Hiding Power

311

Table 7-7. Formulas needed for determination of the hiding power. Specified as measured values: (I) R1 Reflectance of hiding coat R Reflectance of non-hiding coat R0 Reflectance of substrate OR (II) R0b R0w Rb Rw R

Reflectance of black substrate Reflectance of white substrate Reflectance over black Reflectance over white R

1

r0

r0 r2 1

(3.8)

R

(Saunderson-correction r0 = 0.04; r2 = 0.6; or r0 (l), r2 (l) as inputs) 1) R R1 R R1 2) R0b R0b 3) R0w R0w 4) Rb Rb 5) Rw Rw

where

(I) a

1 R1 R1

(3.120)

or (II) a

1 Rw R0w Rb R0b 1 Rb R0b R0w 2 Rb R0w Rw R0b

b

p a2 1

S

1 1 Arcoth bh

Rw

(3.122) (3.120)

a R R0 R R0 (Scattering coefficient; R, R0 from I or II) b R R0

(3.121)

K (a ± 1) S (absorption coefficient) Begin iteration loop: With h = h0 as initial value R

1

where

R

1

R0 a b coth bSh a b coth bSh R0

(3.111)

1) R Rb R0 R0b 0 2) Rw R0w 0.9048 (from R0w = 0.8) r0 1

r2 R r0 r2 R

g r0

(3.150)

312

7 Determination of Hiding Power and Transparency

Table 7-7. Continuation (Saunderson back-correction with allowance for gloss) 1) R Rb R Rb 2) Rw Rw

where Rb

R

rl Sl Rb;l dl ;

Rw

R

rl Sl Rw;l dl

(Sl = S (l), standard illuminant) where

(3.151)

1) Rb Xb Rw Xw rl x l (CIE color matching functions) 2) Yb Yw y (l) 3) Zb Zw z (l) Branch in program: A) R/Rn >p0.008856 B) R/Rn ^ 0.008856 R 3 R=Rn R 7.787 7 R/Rn + 0.138 where

(2.5) (2.6)

1) R Xb R X b Rn X n (CIE tristimulus values of standard illuminant) 2) Y b Yb Yn 3) Z b Zb Zn 4) X w Xw Xn 5) Y w Yw Yn 6) Z w Zw Zn

End of branch a 500 (X ± Y*) b 200 (Y ± Z ) L 116 7 Y ± 16 where

1) a ab b bb L Lb X Xb Y Yb Z Zb 2) aw bw Lw Xw Yw Zw

Dr rw where

DEab

(2.7)

rb

(2.11)

1) Dr Da rw aw rb ab 2) Db bw bb 3) DL Lw Lb p Da2 Db2 DL2

Return to beginning of loop (eq. 3.111) after applying correction to h; continue until DE ab = 1.

(2.10)

7.4 Hiding Power

Fig. 7-14. Flowchart for determination of hiding power with the principle of spectral evaluation.

313

314

7 Determination of Hiding Power and Transparency

Table 7-8. Formulas for h iteration (Newton's method). Prime denotes partial derivative u/uh of the unprimed quantity. See Table 7-7 for specified inputs. After equation (3.111) of Table 7-7, insert: R

a

bS 2 1 R0 2 a R0 R0 sinh bSh b cosh bSh2

(3.153)

1) R R b R0 R0b 0 2) R w R0w 0.9048 (from R0w = 0.8)

where

On grounds of computational economy, it is desirable to calculate the three hyperbolic functions in equations (3.111) and (3.153) as follows: E = exp (bSh), sinh bSh = x = (E ± 1/E)/2; cosh bSh = y = (E + 1/E)/2; coth bSh = y/x. After equation (3.150) of Table 7-7, insert: R

1

where

1

r0 1 r2 R r2 R 2 1) R R b R Rb R R b 2) R w Rw R w

After equation (3.151) of Table 7-7, append: where

4) Rb X b Rw X w Rs;l R b l Rw;l R w l 5) Y b Y w R w (l) R b (l) 6) Z b Z w R w (l) R b (l)

After equations (2.5) and (2.6) of Table 7-7, insert: R R b R R w A) R b b ; R w w ; 3 Rb 3 Rw where

R b R w B R b 7:787 ; R w 7:787 Rn Rn

1) R b X b R w X w Rb Xb Rw Xw R b X b R w X w Y w Y b Y w 2) Y b Yb Yw Z w Z b Z w 3) Z b Zb Zw

After equation (2.7) of Table 7-7, insert: a 500 X where

Y ;

b 200 Y

L 116 Y

1) a a b b bb L L b X X b Y Y b Z Z b L w X w Y w Z w 2) a w bw

After equation (2.11) of Table 7-7, append: where

Z ;

4) Dr Da rw a w r a b 5) Db bw bb Lw L b 6) DL

7.4 Hiding Power

315

Table 7-8. Continuation After equation (2.10) of Table 7-7, insert: Z = ln DEab

Z

(ln x converges to 0 faster than x ± 1)

1 2 DEab

Da Da Db Db DL DL Z Z

hn1 hn

(new value h = hn+1)

(3.152)

If jhn1 hn j 1 < 10 6 ; then h hD and D hn hD Special cases 1. ªDue to scattering aloneº Delete equation (3.111) of Table 7-7 and equation (3.153) of Table 7-8 and replace with: 1 R0 S h R0 1 R0 S h 1 2 1 R0 R S 1 R0 S h 1

R

(3.113) (3.154)

as equation (3.133) with h hD;sca ;

Dsca

1 ; hD;sca

dsca

Dsca D

(scattering component)

2. ªDue to absorption aloneº Delete equation (3.111) of Table 7-7 and equation (3.153) of Table 7-8 and replace with: R R0 e

2Kh

R

;

2 K R

(3.112), (3.154)

as equation (3.133) with h hD;abs ;

Dabs

1 ; hD;abs

dabs

Dabs D

(absorption component)

For each of cases 1 and 2, the same iteration loop can be used as in Table 7-7, supplemented by equations (3.153), (3.152), (1.133) (see above) dint 1 ± dsca ± dabs

(interaction component)

(3.137), (3.138)

316

7 Determination of Hiding Power and Transparency

Fig. 7-15. Flowchart for determination of hiding power in accordance with the principle of spectral evaluation (Newton's method).

Fig. 7-16. Reflection spectra of a chromium oxide pigment in alkyd resin paint (reflectances: Rb over black, Rw over white; R1 , hiding coat; R0b , black substrate; R0w, white substrate.

7.4 Hiding Power Program ªHIDING COLOREDº Hiding power and Transparency of Colored Pigments, according to the Principle of Spectral Evaluation (VÚLZ, Industrial Color testing) ******************************************************* Date: ..-..-.. Pigment: Chrome oxide green Binder: Alkydal F 48 r0,r2: Standard values Gloss degree: 94% PVC: .98 % Film thickness: .05796 mm Measuring conditions: d/8 (incl) Rho(inf): measured Rho(b): Input from keyboard Rho/0b): Input from keyboard Rho(w): Input from keyboard Rho(0w): Input from keyboard Input: ***************************************************************************** Lambda Rho(inf) Rho(0b) Rho(0w) Rho(b) Rho(w) 400 nm .1328 .0446 .5145 .1214 .1641 420 .1155 .0453 .5650 .1104 .1415 440 .0783 .0452 .6231 .0766 .0928 460 .0687 .0452 .6866 .0677 .0803 480 .0749 .0445 .7442 .0737 .0894 500 .0963 .0443 .7753 .0931 .1209 520 .1678 .0440 .7968 .1467 .2360 540 .2088 .0439 .8071 .1699 .3052 560 .1476 .0439 .8229 .1287 .2079 580 .1022 .0438 .8249 .0948 .1367 600 .0912 .0436 .8246 .0864 .1203 620 .0977 .0436 .8270 .0917 .1313 640 .1130 .0434 .8252 .1038 .1574 660 .1407 .0434 .8258 .1232 .2051 680 .1751 .0431 .8243 .1431 .2650 700 .2086 .0430 .8192 .1587 .3234 Output:**************************************************************************** KUBELKA-MUNK-Coefficients, related to PVC 1% Lambda a b K (1/mm) S (1/mm) Calculated from 400 nm 2.474 2.263 12.77 8.661 Rho(w) 420 2.931 2.755 15.42 7.984 Rho(w) 440 5.360 5.266 22.77 5.221 Rho(w) 460 7.026 6.954 25.88 4.295 Rho(w) 480 5.845 5.758 23.94 4.941 Rho(w) 500 3.778 3.643 18.62 6.704 Rho(w) 520 1.9411 1.664 9.371 9.958 Rho(w) 540 1.6114 1.264 6.722 10.99 Rho(w) 560 2.204 1.964 10.86 9.014 Rho(w) 580 3.461 3.313 16.31 6.630 Rho(w) 600 4.112 3.988 18.15 5.831 Rho(w) 620 3.696 3.559 16.78 6.222 Rho(w) 640 3.015 2.845 14.15 7.019 Rho(w) 660 2.320 2.093 10.80 8.182 Rho(w) 680 1.8664 1.576 8.004 9.238 Rho(w) 700 1.6125 1.265 6.089 9.940 Rho(w) TRANSPARENCY Standard Illuminant/Standard Observer: C/2 degr Transparency number T .2602 ml/m2 Coloring power Phi 4.607 m2/ml Transparency-coloring power L 1.199 Transparency-coloring degree G 75.9% HIDING POWER Hiding power value D 6.171 m2/l Scattering component p(sca) 3.04% Absorption component p(Abs) 40.18% Interaction component p(Ww) 56.78% **********************************************************************************

Fig. 7-17. Determination of hiding power, including transparency (computer output).

317

318

7 Determination of Hiding Power and Transparency

scheme described above, may be larger than the hiding power itself; in other words, the scattering component of the hiding power may be more than 100 %. The unavoidable conclusion is that the interaction component is negative. In such a case, absorption makes only a small positive direct contribution; on the other hand, the interaction makes a clearly larger negative contribution to the hiding power, since the undertone that reduces the hiding power comes about only through the interaction of scattering and absorption. This statement is illustrated by the example in Figure 7-18, where a white pigment with a slight yellow undertone was used.

Fig. 7-18. Hiding power of a white pigment in alkyd resin paint (example of negative interaction component of hiding power).

The program described here seems to be a sort of final step in the determination of hiding power for arbitrary paints. The hiding power can be determined with a computer program that leaves virtually nothing to be desired. As has been shown, the determination of transparency (and the transparency quantities) has also been integrated into the program. At the same time, this program illustrates the universal applicability of the principle of spectral evaluation.

7.4.4 Economic Aspects Any statement about hiding power, regardless of whether it is expressed as Dv in m2/L or as Dm in m2/kg, is a statement about effectiveness. This becomes particularly obvious if hiding power values are plotted versus the pigment volume concentration. The flowchart of Figure 7-19 makes clear what steps are required in order to plot the D versus s curve (curve of hiding power value versus PVC). Figure 7-20 shows Dv versus s curves for two TiO2 pigments (one anatase and one rutile). The plot demonstrates not only the well-known superiority of rutile pigments, but also the existence of a maximum in the D curves for both pigments,

7.4 Hiding Power

319

Fig. 7-19. Flowchart for determination of hiding power of white pigments as a function of PVC.

Fig. 7-20. Hiding power value Dv, versus PVC (TiO2 pigments in alkyd resin paint).

each maximum lying at a PVC value of around 30 %. Further, the curves show the relationships between rutile and anatase with regard to a hiding coat (run a horizontal from one curve to the other). The maximum hiding power value of 21 m2/L for anatase, at 29 % PVC, is already reached by the rutile pigment at a PVC of 13 %. In other word, substantial amounts of pigment can be saved. On the other hand, more binder must be used; the actual saving is not seen until the costs of pigment and binder for the hiding coats are added up. A cost analysis based on the Dv versus s plot is quite possible, as KEIFER has shown (see [27] in Section 3.9). The reciprocals of the ordinate values 1/Dv = hD give the dry film thicknesses; the abscissa values s and the densities of the pigment and medium give the mass fractions; and these are multiplied by the respective prices. The sum of the cost contributions for pigment and medium yields the desired total cost fL of the hiding coat of paint. The formulas are

320

7 Determination of Hiding Power and Transparency

f hD sRP fM hD (1 ± s) RM PM

(7.12)

fL f + fM hD [(RP ± RM PM) s + RM PM] where f is the cost per unit area, US$/m2 ; R is the density, g/cm3( = kg/L); s is the PVC; P is the price per unit weight, US$/kg; hD is the hiding film thickness, mm( = L/m2); and the subscripts have the following meanings: no subscript, pigment; M, medium (unpigmented); L, pigmented paint. Figure 7-21 presents cost curves obtained in this way. The total cost (fL) curves show the expected distinct minima. From this plot it can be deduced that a hiding coat made with anatase pigment has a much higher total cost than one made with rutile pigment; the difference ranges from 25 % to 30 %, depending on the PVC. The component curves (f and fM) show that not only the cost of the pigment but also the cost of the medium used to create a hiding coat are higher for anatase.

Fig. 7-21. Costs of hiding coats versus PVC.

The explanation of this result is that, when an optically less capable pigment is used at a given PVC, hiding requires a thicker film. This thicker coat, however, contains not just more pigment but also more of the medium. Hence it is easy to see that even small differences in the optical properties of pigments have major effects on the cost calculation. The minimum in the cost curve of Figure 7-21 shows how much pigment must be used in order to obtain the least expensive hiding coat. The position of the cost minimum depends on the shape of the Dv versus s curve, as has been shown. If the prices per unit volume for pigment and vehicle were equal (RP = RMPM), the price minimum in Figure 7-21 would coincide with the hiding power maximum in Figure 7-20, as can be inferred from equation (7.12). If the prices change, the minimum shifts and a new curve has to be plotted. For example, suppose the price

7.4 Hiding Power

321

of the pigment goes up; then the cost minimum moves toward lower PVC. This means that it has become more economical to use less pigment, even though the new pigmented medium hides less well and so must be applied in a thicker coat to hide. The method described here makes it possible to arrive at correct assessments of pigments ± with respect to optical performance and economics ± on the basis of the hiding power versus PVC curve. Such results cannot be achieved through simple estimation.

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

8

Determination of Tinting Strength and Lightening Power

8.1

Content of Coloring Material

8.1.1 Dyes Organic dyes can be quantitatively determined by methods based on physical optics or by chemical analysis. The recommended way to determine dye concentrations in solutions is through the concentration-dependent Kubelka-Munk function, which is discussed in Section 8.2 in connection with tinting-strength determination of dyes. For the test methods described here, the determination of concentration is not so important, because tests are commonly performed on preparations (paint, resin, aqueous solution) made up with a known quantity of dye in the first place. This survey will be a brief one making no claim of completeness. When determination problems occur in relation to dyes, the extensive specialist literature must be consulted (see [3] in Section 1.4 and [32] in Section 4.10). Chemical methods for determining the concentration of dyes can be employed only when the constitution of the dye, or at least its molecular weight, is known. The first technique to mention is elemental analysis, but only when the dye contains an element that the medium does not. Other methods are applicable to a dye dissolved in a liquid. The most important of such methods ± because they are valid for nearly all groups of dyes ± are reduction methods. Titanium(III) sulfate or titanium trichloride is used as reducing agent. Azo dyes in (acidic) aqueous solution can be titrated directly or indirectly; the same holds for a number of heterocyclic dyes. Azo and anthraquinone dyes can also be determined by oxidizing with chromic acid and measuring the volume of nitrogen evolved. Other basic dyes can also be determined by oxidimetric titration with cerium(IV) sulfate. Precipitation methods are sometimes used for the quantitative determination of anionic dyes (e. g., with cetyl triammonium bromide in chloroform). In the case of basic dyes, anion-active compounds such as alkylsulfonates are suitable for precipitation titrimetry. Some of the techniques listed are also appropriate when several dissolved dyes must be determined at the same time (dye mixtures).

324

8 Determination of Tinting Strength and Lightening Power

8.1.2 Pigments Again, in most test methods the quantity and hence the concentration of pigment are known from the outset. Even so, concentration determination may be useful, as for example in the determination of S by the black-ground method, already discussed. Procedures for the determination of pigment contents are set forth in standards*: ± Centrifuge methods, chiefly for production control by the producer and incoming inspection by the consumer (not suitable for separation of carbon black or finely divided SiO2) ± Incineration methods (not suitable for determination of organic pigments) ± Filtration methods (also suitable for the separation of carbon black and finely divided SiO2) Of these groups, centrifuge and filtration methods are applicable chiefly to liquid paints; incineration, on the other hand, is also appropriate for determinations on surface coating finishes and other coatings as well as plastics. The residue generally contains all the non-combustible particles, that is, pigments, fillers, and other solid additives. Any of the three methods will require an analytical balance, a desiccator, and an oven. Centrifuge Methods The quantity determined is the mass fraction of solid particles insoluble in the selected solvent. A sample is diluted with a solvent or mixture of solvents, and the solid particles are separated by centrifugation. The solid material is dried and weighed, and the pigment content is calculated as a fraction. The following apparatus is required in addition to those listed above: a laboratory centrifuge with cups and taring device, and a ball-type stirrer. A low-boiling solvent should be chosen if possible. Incineration Methods The solvent is first evaporated off from the sample; the residue is then ashed at 450 8C if carbonates are present, at 700±900 8C otherwise. The pigment content is determined from the mass of the residue, either directly of after an analysis. Additional apparatus required includes porcelain crucible, crucible tongs, muffle furnace, or fast ashing device. Filtration Methods The sample is mixed with a suitable organic solvent or mixture of solvents, then with a solution of KOH in methanol. The mixture is filtered through a glass filter crucible with filter aid. The solid matter recovered is dried and then weighed. The * See ªPigment Contentº in Appendix 1.

8.2 Relative Tinting Strength

325

pigment content is calculated from the mass of the solid component. The following additional equipment will be needed: glass filter crucible, safety pipet, filter aid, KOH solution in methanol (1 mol/L), analytical-grade methanol. With many pigments and pigment mixtures, a simple determination of the residue is not enough; the residue must be subjected to analysis and examination. The analytical methods for inorganic pigments are contained in standards*.

8.2

Relative Tinting Strength

8.2.1 Dyes A method for determining the relative tinting strength of dyes in solution is described in standards**; the procedure is a spectrophotometric one. On the basis of the relative tinting strength as defined for dyes (Section 4.6.1), the absorption coefficients (or extinction coefficients) are determined at the absorption maximum and the ratio is taken. The dye solutions must not scatter light, and the absorption curves must be highly similar in nature; that is, only dyes similar in hue may be compared. This kind of test applies to dyes such as are used in paints, inks, and so forth. The solution media (solvents but also binders) employed in preparing the solutions must satisfy the following requirements: The dyes must be completely soluble in the medium, the resulting solutions must be stable, and the results of the measurement must be such that they can be extended to lab practice. Solutions of the test dye and reference are prepared; these should have concentrations as nearly equal as possible. In addition to the usual laboratory apparatus (pipets, volumetric flasks, analytical balance), a spectrophotometer or filter photometer with the proper glass cuvettes is necessary. No particular solution medium is specified, but the following are especially suitable: ± N-Methyl-2-pyrrolidone (particularly good for basic, oil-soluble, and metal complex dyes) ± Dimethylformamide ± Dimethylsulfoxide When concentrated dye solutions must be further diluted, the above list can be supplemented with ± ± ± ±

Toluene 2-Ethoxyethanol Ethanol Water

* For a Listing, see [1] in Section 1.4. ** See ªTinting Strength, relative, Dyes in Solutionº in Appendix 1.

326

8 Determination of Tinting Strength and Lightening Power

Binders and other additives (acids, bases, complexing agents, surfactants, antioxidants, etc.) can also be used as part of the medium. Preparation method: Weigh out suitable amounts of solid dyes (e. g., 0.1 or 1 g) or dye solutions, with accuracy to 0.0001 g. Quantitatively transfer weighed samples to volumetric flasks (100 or 250 mL) and completely dissolve in solution medium. In the case of solid dyes, it is useful to predissolve the material (stirrer, heating). Fill volumetric flasks, homogenize contents, and dilute in one or more steps to a concentration for measurement such that the transmittance is 10±30 % (corresponds to concentrations of 2 to 40 mg/L). Measurement method: Within one hour after preparation (protect from light until measurement), measure transmission/extinction at the absorption maximum of the solutions; in the same cuvette, measure blank value (solution medium used).Take difference in extinction between measurement and blank (unless using a two-beam instrument).From it, calculate absorption coefficients k@ b per unit mass concentration (specific extinction coefficients), using the formula k@ b = E/(h 7 b), where E is extinction, h is length of path of the cuvette, and b is mass concentration of dye. The relative tinting strength is then found as the ratio of k@ b values between test and reference dyes. Figure 8-1 is a computer printout from a determination of relative tinting strength for dyes. Standard deviations obtained in round-robin tests between laboratories were less than 2 %; in repetitions by the same laboratory, ca. 1%. Program ºP(REL), DYEº Relative Tinting Strength of dyes in solution, according to DIN 55978 ********* Date: ..-..-.. Colorimeter: Spectral ABC Cuvette: 10 mm Input:************************************************************* Test: Red dye T Reference: Red dye R Measured solution: Instruction Dye/3 Measured wavelength: 505 nm Mass concentration: Test: 19 mg/l Standard: 20 mg/l Extinctions; Test: 1.6094 Standard: 1.6607 Output: *********************************************************** Relative Tinting Strength: 102 % ****************************************************************** Fig. 8-1. Determination of relative tinting strength of dyes in solution (computer output).

8.2 Relative Tinting Strength

327

8.2.2 Inorganic Black and Colored Pigments (Lightness Matching) Effective methods for determining the relative tinting strength and color difference after color reduction on inorganic black and colored pigments can be found in standards*, which set forth the conditions that must always be fulfilled if erroneous results are to be avoided. The ISO standard is concerned with some of the tinting strength criteria discussed in Section 4.6.2. The following criteria are permitted: ± Minimum (X,Y, Z) ± the smallest of the CIE tristimulus values ± CIE tristimulus value Y (or lightness L ) ± Color depth TS What is more, instructions for determining the color difference after color reduction are given. The ISO standard includes the use of the zero-th approximation (see Section 4.6.4) to rationalize the determination of tinting strength with the aid of the Kubelka-Munk function. It describes an alkyd resin paste method with which the spectral absorption coefficients per unit mass and the relative tinting strength can be determined. The tinting strength criterion is Rmin (l), the reflectance at the absorption maximum (or else min (R'x , R'y, R'z ), i. e., the smallest of the reflectometer values). Thus the prerequisites exist for an effective method in the case of inorganic pigments; the tinting strength criterion is the CIE tristimulus value Y (i. e., the lightness L ); see Section 4.6.3. The following equipment is needed: ± ± ± ±

Triple-roll mill Automatic muller Paste film holder (see Section 6.2.3) or other suitable paste support Colorimeter (spectrophotometer or tristimulus instrument) Preparation method: White pigment paste with the following composition (by mass): ± 40 parts TiO2 (type R2 of ISO 591; e. g., Bayertitan R-KB2) ± 56 parts Alkydal L 64 (Bayer AG) ± 4 parts Ca stearate Thoroughly mix ingredients on order to wet the solids. Pass through triple-roll mill until grindometer test** yields a value 55 mm. Store paste in airtight container. Place 3 g of white pigment paste on lower plate of muller; spread 0.12 g of inorganic pigment (test or reference) on it and mix with spatula. Distribute mixture

* See ªTinting Strength, Relativeº in Appendix 1. ** See ªFineness of Grindº in Appendix 1.

328

8 Determination of Tinting Strength and Lightening Power

in form of a circular ring. Mull in four stages of 25 revolutions each with a weight (1 kN) applied; after each stage, collect paste and redistribute. Measurement method: Measure CIE tristimulus value Y (also X and Z for color difference after color reduction) or reflectometer value R'y (also R'x and R'z if necessary) of the reducing white on the paste film holder. Preferred procedure is method A of Section 6.1.2 (i. e., with surface reflection included). Evaluation: Apply Saunderson corrections to all CIE tristimulus values (eq. 4.95). use equation (4.61) to calculate Kubelka-Munk functions F, FR ; use equation (4.94) to calculate tinting strength. The tinting strength obtained in this way is identical to the relative absorption coefficient per unit mass, so the F values must first be divided by the pigment mass concentrations unless precisely 0.12 g of test and reference pigments was taken. To determine the color difference after color reduction, convert CIE tristimulus values X and Z of reference to matching concentration (with help of Kubelka-Munk functions and the relative tinting strength P just determined). From the CIE tristimulus values after Saunderson back-correction, calculate CIELAB coordinates by known method, and thence color differences. In the case of black pigments, it may be desirable to report the relative hue* as specified in Section 2.3.3 instead of the hue and chroma differences. The flowchart for this determination appears in Figure 8-2; Table 8-1 lists the needed computational steps as an aid to programming. Here the reference is matched to the test pigment; this is recommended because the test is performed at ^ If the test were matched to the reference, a fixed PVC value corresponding to m. the pigment concentration would vary with the relative tinting strength of the test pigment. The summary of computational steps also shows how the measured CIE tristimulus values of the reference are converted to the CIE tristimulus values at matching. An example in the form of spectral reflection curves for reducing whites is presented in Figures 8-3 and 8-4. In the first case, the curves are for equal masses of test and reference; in the second, the curves are plotted after lightness matching. Finally, Figure 8-5 is a printout of a tinting strength determination. For most purposes, the use of the zero-th approximation to obtain the tinting strength as described here is entirely adequate ± for example, for production control. If there should be a need for a comparison between inorganic pigments with high light scattering power or a very great difference in tinting strength, so that more that +20 % departures from 100 % relative tinting strength occur, then the first approximation is recommended (Section 4.6.4, eq. 4.92). The factor a in equation (4.93) depends on the reference alone and can easily be determined once for all. * See ªHue, Relative, of Near White Specimensº in Appendix 1.

8.2 Relative Tinting Strength

329

Fig. 8-2. Flowchart for determination of relative tinting strength of black and inorganic colored pigments.

330

8 Determination of Tinting Strength and Lightening Power

Table 8-1. Formulas needed for calculating relative tinting strength and color difference after color reduction for inorganic colored and black pigments. ^ Y; ^ Z; ^ X^ R ; Y^ R ; Z^ R or R^ 0 ; R^ 0 ; R^ 0 ; R^ 0 ; R^ 0 ; R^ 0 Given: X; x y z x;R y;R z;R R^

R^

0:04

1 F^

;

0:36 0:6 R^

^ n where 1) R^ X=X ^ 2) Y=100 ^ 3) Z=Zn 4) X^ R =Xn 5) Y^ R =100 6) Z^ R =Zn P 0

F^Y F^Y;R

R^ 2 2 R^

eqs. (4.95), (4.61)

R^ X^ =Xn F^ F^X 0:782R^ 0x 0:198R^ 0z =98 R^ y =100 Y^ =100 F^Y ^ ^ F^Z Rz =100 Z =Zn F^X;R 0:782R^ 0x;R 0:198R^ z;R =98 X^ B =Xn R^ y;R =100 Y^ R =100 F^Y;R F^Z;R R^ 0z;R =100 Z^ R =Zn

or P 1 f^ 1 a f^

F^Y FWP with f^ F^Y;R FWP

1

(a is determined experimentally) q ^ R F^R P F^B P 2 ; R 1 FR P

eqs. (4.92, 4.93, 4.94)

0:384 R R 1 0:6 R R

RR 0:04

eqs. (4.111), (4.112)

where 1) F^R F^X;R R RR XR =Xn R XR =Xn 2) F^Y;R YR =100 YR =100 3) F^Z;R ZR =Zn ZR =Zn

Two cases: A) R ^ 0.008856

B) R > 0.008856 p R 3 R

R 7.787 R + 0.138 where 1) 2) 3) 4) 5) 6)

a 500 X where 1) X 2) Da aT DEab

eq. (2.5)

^ n R X R X=X T ^ Y=100 YT ^ n Z=Z ZT XR =Xn XR YR =100 YR ZR =Zn ZR

Y ; XT XR

aR ;

b 200 Y Y

YT YR

Db bT

Z bR ;

Z ; ZT ZR

a

L 116 Y aT aR

DL LT

b

LR ;

p Da2 Db2 DL2

DCab

q 2 a2 T bT

L

eq. (2.7)

LT LR eq. (2.11)

eq. (2.12)

Dhab Arctan DHab

16

eq. (2.10)

q 2 a2 R bR

bT b Arctan R aT aR q 2 2 2 DEab DL DCab

bT bR

eq. (2.14) (same sign as Dhab)

eq. (2.13)

8.2 Relative Tinting Strength

331

Fig. 8-3. Spectral reflectance of two red iron oxide pigments in reducing white (equal added pigment masses).

Fig. 8-4. Example from Fig. 8-3 after Y matching.

332

8 Determination of Tinting Strength and Lightening Power

Program ªP(REL)º Relative Tinting Strength by means of lightness matching, according to ISO 787-24 (modified) ******************************************************************* Date: ..-..-.. Standard is A Test is B Medium and white paste: according to ISO 787-24 Colorimeter, Standard Observer: N.N., C/28 Measuring conditions: d/8 (incl) Input: ************************************************************** Masses: White paste: 3 g Pigment: .12 g Reflectometer values: Reference: Test: R'(x) 47.74 47.02 R'(y) 41.03 39.93 R'(z) 39.68 38.18 Output: ************************************************************* Relative Tinting Strength: P = 108 % Tinting Equivalent: 1/P = 93% CIELAB Coordinates after matching: Reference: Test: a* = 15.0 15.7 b* = 1.7 2.2 L* = 69.4 69.4 Color difference after reduction: Delta(E*(ab)) = .9 Delta(L*) = .0 Delta(C*(ab)) = .8 Delta(H*(ab)) = .4 Delta(h(ab)) = 1.58 Fig. 8-5. Relative tinting strength of a red iron oxide pigment by lightness matching.

The accuracy with which tinting strength and color difference after color reduction are determined for inorganic pigments can be improved somewhat with a recent method (DIN 55 603). the method is again based on Y-matching, but now the principle of spectral evaluation is employed.

8.2.3 Organic Pigments (ªFIAFº Method Based on Principle of Spectral Evaluation) The principles of this section were established by Gall (see [19], [23] in Section 4.10), whose work has become the basis for standards*. The German standard defines ªstandard color depthsº and gives a procedure for the preparation of color depth standards (i. e., color samples of known standard color depth); these are used * See ªTinting Strength, Relativeº and ªColor Depthº in Appendix 1.

8.2 Relative Tinting Strength

333

as controls in both visual and colorimetric matching. The same standard provides instructions for bringing about the standard color depth in color samples. We follow the standards in determining the relative tinting strength of organic colored pigments and in describing Gall's ªFIAFº method, a computer-aided method of colorimetric tinting strength determination by iterative color depth matching based on the principle of spectral evaluation*. The color depth standards are available commercially; they should be calibrated, that is, they should indicate the CIE tristimulus values and the color depth parameter B = DTS (deviation from the color depth level), measured in the prescribed way. The visual adjustment of color samples to a given color depth level is of secondary importance in practice, so only the colorimetric technique needs explanation here. The color depth standards are necessary when results from different instruments or different laboratories are to be compared. Corrections to the measured CIE tristimulus values with respect to the nominal values of the calibrated standards take the form of ratios: Xcorr = (XS /XM) 7 X, where XS is the nominal value for calibration and XM is the value measured on the standard (and similarly for Y and Z). Ordinary paint bases (white enamels) are used as test media (see Section 8.2.4 for examples); naturally, pastes can also be used as in Section 8.2.2. Gall's method is contrasted to the method based on Y matching described in Section 8.2.2, where on Y value was specified and the second was adjusted; in the color depth matching method, both reducing whites (test and reference) must be adjusted to the specified color depth level**. The ratio of the masses of pigment required are input to the fundamental equation (4.75), which gives the relative tinting strength. The formulas needed for this procedure were already introduced in Section 4.5.6. The method results in the value DTS = B of a selected standard color depth being made equal to zero for test and reference through variation of the amounts of pigment added to the white paste. Now it is possible to describe Gall's FIAF method, which functions on the principle of spectral evaluation. A flowchart is shown in Figure 8-6. From the input reflection spectrum R (l) at 16 chosen wavelengths (20 nm intervals), the computer calculates the CIE tristimulus values X, Y, Z, the CIE chromaticity coordinates x, y, and thence DTS . A check is then made in order to see whether DTS = 0 to a sufficiently good approximation. If not, the mass-referred spectral Kubelka-Munk function F/m are calculated from the Saunderson-corrected reflection spectrum, then multiplied by a appropriately modified mass of pigment. From the result, the new CIE tristimulus values and DTS are calculated. This loop is repeated until DTS = 0. As a rule, two to four times around the loop will be required; five may be needed in quite rare cases. Once the target match for test and reference has been found, the * The letters FIAF stand for the German phrase ªFarbstårke durch iterativen Angleich der Farbtiefenº, with the meaning stated above. ** Schmelzer and co-workers propose the following departure from the standard: Test and reference are adjusted to the same (nonzero) value of B. Drawback: It is not possible to report the standard color depth level (SDS).

334 8 Determination of Tinting Strength and Lightening Power

Fig. 8-6. Flowchart of FIAF program for calculating relative tinting strength and color difference after color reduction by Galls method.

8.2 Relative Tinting Strength

335

tinting strength is output as the ratio of the two masses (along with the tinting strength equivalent if appropriate); in addition, the color difference after color reduction and the lightness, chroma, and hue differences are included in the output. Table 8-2 lists the needed equations as an aid to programming. A problem is presented by the a (j) factors (see Section 4.6.5): The standard includes long tables for ªmanualº searching and calculating. Gall and Friedrichsen have written convenient formulas for computer calculations based on third-degree polynominals; these are excerpted here for 1/1, 1/3, 1/9, 1/25, and 1/200 SDS and for illuminant/observer combinations C/28 and D65/108 (Tables 8-3 and 8-4), so that there is no need to reproduce the full tables. The formula for calculation is a(j) a(j0) + K1 W + K2 W 2 + K3 W 3 where W = (j ± j0)/100. A flowchart for the computer calculation is shown in Figure 8-7; the coefficients of the polynomials (tabulated values) must be stored in the computer memory. Figure 8-8 gives a printout by way of example. Two blue pigments were tested; the resulting value of the relative tinting strength is around 126 %. The example is instructive in that a relative tinting strength based on lightness matching can also be determined from these data. It is only 117 %; thus, less of the reference pigment would have to be added for matching. But this also means that the color difference after color reduction will change. It is found that DE ab is smaller than in the color depth matching method. The difference can be attributed primarily to a smaller chroma difference (saturation); the hue difference, on the other hand, is larger. These results imply that a greater difference in nuance is accepted when lightness matching is employed, even though in the case of color depth matching this larger difference would be perceived as interfering. This may indicate that questions of color formulation must be accorded more weight in color depth matching, while lightness differences are more significant in the case of Y matching. As Table 8-2 and equation 4.64 show, the zero-th approximation is employed in calculating the relative tinting strength. This is justified even for higher pigment concentrations, since organic pigments commonly have a lower refractive index (in the neighborhood of 1) and thus only slight light-scattering power. Thus the use of the zero-th approximation is proper even outside the Beer's law range, and therefore even at high relative tinting strength values differing by more than +20 % from 100 % ± as in the example. For organic black pigments, it is desirable to employ Y matching; the procedure of Section 8.2.2 can thus be used. Another method (ISO 787-26) has gained acceptance for organic pigments along with the FIAF method. The tinting strength is quantified as the sum of the colorimetrically evaluated Kubelka-Munk function F x,y,z (see eq. 4.77). This quantity is matched in a similar way to the Y value as described in Section 4.6.4. The formulas of Figure 8-2 and Table 8-1 can be used provided the tinting strength criterion just identified is employed.

336

8 Determination of Tinting Strength and Lightening Power

Table 8-2. Formulas needed for calculating relative tinting strength and color difference after color reduction for organic colored pigments. Given: R (l), RR (l) with 16 chosen wavelengths spaced 20 nm apart X Y Z x

R

x l R l dl

R R

y l R l dl z l R l dl

(2.3)

X ; X Y Z

y

Y X Y Z

(2.4)

q s 10 x xn 2 y yn 2 j Arctan

y x

yn xn

(4.100)

a(j) from subroutine, Fig. 8-7, Tables 8-3 and 8-4 DTS

p Y s a j

b 1 19 ; 1

R l F l f l

10 bi

b 1 29 ; 3

b 1 41 ; 9

(4.99) b 1 56 ; 25

b

1 200

73

R l 0:04 0:36 0:6 R l 1

(3.11)

R l2 2 R l

(3.117)

F l m

(4.64)

m i1 m i 0:9DTS

(4.101)

f l m i1 F l

(4.64)

R l 1 F l R l

p F l F l 2

(3.116)

0:384 R l 0:04 1 0:6 R l

(3.10)

Iteration yields mend ; hence mend ! Fend l ! Rend l ! Rend l ! X; Y; Z : Hence a , b , L and aR , BR , LR and hence DE ab , DC ab , Dhab, DH ab

) as in Tab. 8-1

For black pigments: shade difference after color reduction as in Table 8-7.

8.2 Relative Tinting Strength

337

Table 8-3. Polynomial coefficients for calculating the a (j) factors in the determination of DTS, standard illuminant C,28 observer. Range

j8

a (j)

K1

K2

K3

1/1 SDS

1 2 3 4 5 6 7 8

0 56 88 200 228 244 328 344

2.1620 3.7730 3.8850 2.6205 1.7110 1.1170 2.1700 2.0510

2.1146 2.2982 ±1.4047 ±0.71265 ±2.5648 3.6796 ±1.0190 ±1.4617

5.6685 ±11.750 0.86005 ±7.2510 ±57.746 ±4.1844 4.7036 15.468

±7.6914 17.685 ±0.54797 ±6.4238 316.03 1.5426 ±18.645 ±12.263

1/3 SDS

1 2 3 4 5 6 7 8 9

0 52 156 188 216 252 276 308 344

1.9710 3.5230 3.4910 2.8560 2.1300 0.7710 2.1770 2.4000 2.2240

1.8854 0.56964 ±0.36932 ±2.8126 ±2.7444 ±0.42114 2.7983 ±0.49271 ±2.9558

7.2139 ±0.97366 ±5.5142 ±2.3760 ±25.405 70.0632 ±12.018 3.1561 ±5.1289

±9.8081 0.38087 1.4815 11.254 62.615 ±182.87 17.020 ±8.7220 85.152

1/9 SDS

1 2 3 4 5 6 7 8

0 48 92 188 224 244 288 344

2.3380 3.5020 4.0690 3.0610 1.7010 1.0100 2.5250 2.7690

±0.89972 5.2484 ±0.36496 ±1.7819 ±5.8311 4.6563 1.5168 ±0.85358

11.961 ±17.432 0.64710 ±3.7832 14.461 ±0.21240 ±1.5772 ±31.714

±10.490 19.165 ±1.4171 4.8936 ±12.941 5.7842 ±0.63062 125.77

1/25 SDS

1 2 3 4 5 6 7 8 9 10

0 24 44 72 104 144 196 220 236 296

2.3990 2.4540 3.7250 4.1260 4.7880 4.6710 3.2310 1.9640 1.2040 2.9080

±3.0667 6.0507 6.8347 ±0.30389 3.5030 ±1.6006 ±3.9918 ±8.6798 3.0071 0.41689

16.380 19.039 ±38.741 5.6079 ±17.579 ±3.7578 ±3.5840 27.377 4.0166 ±1.0629

±10.999 ±87.763 69.481 5.6553 20.218 2.9038 ±7.4141 ±17.633 ±7.1562 ±1.2985

1/200 SDS

1 2 3 4 5 6 7 8 9 10 11 12 13

0 20 56 88 104 140 196 216 232 248 264 304 344

5.7810 4.0900 4.0750 6.2600 6.9570 6.8870 5.0030 3.5420 3.4160 5.3360 6.8390 7.5100 7.0040

±8.2288 ±6.2950 3.9274 6.7537 2.3532 ±2.5572 ±4.1350 ±4.1230 0.28516 19.078 4.3458 ±1.0073 ±5.1011

±7.5625 27.716 13.590 ±11.422 ±12.454 4.1401 ±31.582 16.913 121.20 ±110.38 ±12.814 1.2544 ±17.707

32.188 ±28.732 ±14.148 ±22.258 14.924 ±9.9624 78.570 24.602 ±299.69 311.44 15.352 ±4.7446 10.250

338

8 Determination of Tinting Strength and Lightening Power

Table 8-4. Polynomial coefficients for calculating the a (j) factors in the determination of DTS, standard illuminant D65, 108 observer. Range

j8

a (j)

K1

K2

K3

1/1 SDS

1 2 3 4 5 6 7

0 60 156 224 240 268 340

2.250 3.973 3.127 1.987 1.285 2.185 2.142

1.85034 1.51213 ±1.21851 ±4.00696 7.42688 0.822426 ±1.032

8.68115 ±6.23596 5.39038 ±47.8125 ±17.5547 0.741241 8.05627

±11.6328 3.89874 ±8.91809 284.023 8.95508 ±2.73209 ±0.828125

1/3 SDS

1 2 3 4 5 6 7 8

0 52 140 196 236 252 276 340

2.040 3.669 3.524 2.710 1.101 1.351 2.504 2.319

1.8064 1.4459 1.21893 ±0.562195 ±4.18735 7.98462 1.54935 ±2.57889

9.15625 ±3.59046 ±8.80359 ±9.45264 16.9717 ±9.83203 ±3.91061 ±4.03809

±12.6865 2.00006 7.20239 1.99219 118.672 ±14.2773 1.62125 50.0312

1/9 SDS

1 2 3 4 5 6 7

0 52 148 224 244 280 336

2.345 3.94 3.864 1.756 1.438 2.785 2.932

±0.634155 2.40570 ±1.28906 ±4.93951 5.80115 1.67851 ±1.5271

11.2192 ±4.96634 1.00537 ±20.8896 ±1.04980 ±3.35052 ±15.6045

±7.88379 2.47712 ±3.8938 188.117 ±12.9629 1.46381 49.1836

1/25 SDS

1 2 3 4 5 6 7 8

0 28 56 96 148 224 244 292

2.36 3.035 4.1268 4.7271 4.636 1.6873 1.8945 3.1622

±3.05167 8.93835 ±0.28082 2.57528 ±2.0782 ±5.801 6.0961 0.66899

11.0864 ±15.2949 5.0835 ±6.64651 0.12793 28.7262 ±8.30859 ±3.24585

1/200 SDS

1 2 3 4 5 6 7 8

0 28 80 120 208 232 248 280

5.68 3.646 6.203 7.464 4.17 3.555 6.779 7.935

±9.19458 ±0.990845 14.1318 ±1.57855 ±8.99036 4.26904 10.6932 ±0.109528

±19.9785 12.063 ±49.8843 1.25879 23.0088 215.078 ±40.9404 0.637939

30.0801 ±9.64844 ±1.5747 2.61005 ±3.27197 27.2941 2.31348 0.796387 95.9844 ±1.34961 56.0981 ±4.22656 15.7344 ±723.844 58.8066 ±5.00452

8.2 Relative Tinting Strength

339

Fig. 8-7. Flowchart for computer calculation of DTS (after Gall and Friedrichsen).

340

8 Determination of Tinting Strength and Lightening Power

Program ªFIAFº Relative Tinting Strength by means of Color Depth matching, according to DIN 53235 and 55986 ******************** Date: ..-..-.. Color Depth level: 1/3 ST Standard is A Test is B Medium and white paste according to ISO 787-24 Colorimeter, Standard Observer: N.N., C/28 Measurement Conditions: d/8 (incl) Input: ******************************************* Masses: White paste: 3 g Pigment: .3 g Spectral Reflectances: on-line colorimeter Output:****************************************** Relative Tinting Strength: P = 126 % Tinting Equivalent: 1/P = 80 % CIELAB Coordinates of 1/3 ST: Reference: Test: a* = ±10.5 ±11.2 b* = ±27.8 ±28.2 L* = 72.4 73.0 Color Difference after reduction: Delta(E*(ab)) = 1.1 Delta(L*) = .6 Delta(C*(ab)) = .7 Delta(H*(ab)) = ±.6 Delta(h(ab)) = ±1.18 Fig. 8-8. Relative tinting strength of a blue pigment by color depth matching (FIAF method) (computer output).

8.2.4 Change in Tinting Strength Test methods are set forth in the standard* for lacquer binding media and plastics. Test and reference pigments are dispersed in agreed-on vehicles in accordance with agreed-on conditions. Methods and vehicles listed in Section 6.2.1 are recommended. From the mill base, samples are taken after specified dispersion stages and mixed with a white paint (same vehicle) or with a specified white paste. The reflectances are then measured, and the Kubelka-Munk function F of the test and reference mixtures are calculated from the results. The standard still prescribes R (l) (min) as the tinting strength criterion; that is, the F value is to be determined at the reflection minimum (i. e., the absorption maximum). It goes without saying that different criteria (in particular the CIE tristimulus value Y) can be employed as agreed on. Along with an analytical balance and porcelain dishes, the method requires the following:

* See ªChange in Tinting Strengthº in Appendix 1.

8.2 Relative Tinting Strength

341

± Bird applicator or paint spray gun ± Substrate material (glass plates, sheet metal, cardboard; also paste film holders as discussed in Section 6.2.3) ± Perforated cardboard template (for covering in measurements on pastes) ± Spatula ± Automatic muller ± Colorimeter (spectral or tristimulus) ± Oven ± White paint (20 % TiO2) or white paste (40 % TiO2) made up with same vehicle as used in mill base The standard distinguishes between: ± Low-viscous mill bases ± High-viscous, pastelike mill bases Preparation method 1 for low-viscous mill bases Dispersing: generally with oscillatory shaking machine. Withdraw samples after fixed time intervals (initial sample after shortest dispersion time or stage, final sample after longest reasonable dispersion time or stage; tinting strength must reach at least 90 % of potential final value). Reducing white: Mix 3 g of ground mill base with such a quantity of white paint (generally 30 g) that a certain color quality as agreed on (an agreed-on color depth, according to the standard) is achieved. Application: Apply reducing whites to substrates with Bird applicator or spray gun. Check hiding of the coat with contrast cards and rub-out test (see Section 6.2.1). Preparation method 2 for high-viscous, pastelike mill bases Dispersing: generally with automatic muller, otherwise same as method 1. Reducing white: Mix 5 g of white paste with such a quantity of colored pigment paste (generally 0.1 to 0.5 g) that a certain color quality as agreed on (an agreed-on color depth according to the standard) is achieved. Disperse mixture in four stages of 25 revolutions in the automatic muller. After every stage, homogenize with spatula and collect toward center of plate. Application: Apply reducing whites to substrates with Bird applicator. Check hiding with contrast cards and rub-out test (see Section 6.2.1). Measurement and evaluation method Measure CIE tristimulus values Y (in the standard, reflectance at the absorption maximum), apply Saunderson correction, and calculate Kubelka-Munk functions F. use perforated template when measuring pastelike specimens. When rub-out effect is marked (i. e., DE ab > 10), measure the rubbed area. Plot F versus rubbing time or stages also plot the reciprocals 1/F versus 1/t in a Pigenot diagram.

342

8 Determination of Tinting Strength and Lightening Power

A practical example will now be described for the change in strength evaluated by the method of Section 4.7.3. A semitransparent iron oxide pigment was chosen. A planetary ball mill was used for dispersing; the method was that of ISO 8780-4 appropriately modified. Alkydal F 48 (Bayer AG) was selected as the vehicle, and formulation was carried out in accordance with DIN 53238-30. Mill bases with PVC values of 5 %, 7.5 % and 10 % were prepared, and samples were taken from these after, 5, 10, 20, 60, 120, and 240 min. The change in strength was determined experimentally as set forth in ISO 8781-1; the tinting strength determinations were done in accordance with ISO 787-24. For this purpose the samples taken from the mill base were incorporated into a stabilized white paste of Alkydal L 64 (Bayer AG), and the pastes were measured colorimetrically on the paste film holder (DIN 55893). The CIE tristimulus values Y were used in determining the Kubelka-Munk functions F and in the subsequent calculations. The initial and final values F0 and F1 were employed for the determination of the relative PVC values n (eq. 4.126). The 5 minute value was taken for F0 ; for F1, a value obtained from a nonlinear regression of 1/F over all measured values at t = 0 was employed (the Pigenot line yields an unusable value). The use of F0 as initial value shifts the time scale: the new 0 minute value is the old 5 minute value, so that the sampling times must now be associated with times t' = t ± 5, that is, 0 (= F0), 5, 15, 55, 115, and 235 min. Figure 8-9 shows the measured points for B and B / A obtained with eqs. (4.127) to (4.130); these define the lines (determined by curve fitting) that are also re-

Fig. 8-9. Parameters as a function of PVC.

8.2 Relative Tinting Strength

343

Fig. 8-10. Dispersion rate constants as a function of PVC.

Fig. 8-11. Dispersion curves: KUBELKA-MUNK functions (measure of the tinting strength) as a function of the dispersion time.

344

8 Determination of Tinting Strength and Lightening Power

quired by eq. (4.130). Next, eqs. (4.130) to (4.132) were used to calculate the variations of the three rate constants; Figure 8-10 presents the results. With the calculated constants, the F (t) curves representing the change of strength for the three mill bases were calculated with eqs. (4.124) and (4.126); the results are plotted in Figure 8-11. The calculated curves are in remarkably good agreement with the experimental points. To make the calculation traceable, at least in the second half, Table 8-5 lists the most important intermediate results. The end results in Table 8-6 are the rate constants and the half-value times. It should be noted that the dispersing resistance of a pigment is correctly described by the half-value time, while the increase in tinting strength IS (ISO 8781-1) is not appropriate for this purpose. These results yield new information about the dispersing resistance of pigments, which could not be acquired in any other way. First it should be stated that the halfvalue times, and thus the dispersing resistances, decrease with increasing PVC. But the most striking fact is that kk is negative. This can only mean that no size reduction of large particles on small ones occurs: the small particles are reagglomerating and thus becoming large particles again. The constant kg overrides the negative effect of kk , however, so that disintegration on the large particles themseleves is the dominant process. At low PVC, on the other hand, disintegration on the vessel wall and grinding bodies goes faster than disintegration on coarse particles; this result holds up to about 3 % PVC (Figure 8-10). The F (t) curves in Figure 8-11 show a steeper rise and a flatter final phase at higher PVC values, thus expressing the fact that the disintegration of large particles on other such particles, that is, the secondorder reaction, is intensified (as expected) and the other processes become less important as the PVC rises. The increase in strength IS as defined in ISO 8781-1 is not informative as to the dispersing process, and it is not worthwhile listing it as well. Table 8-5. Intermediate values. PVC

B/A

B

y1

y2

a, b, c

k'

5.0 % 7.5 % 10.0 %

0.0532 0.0779 0.0870

0.00817 0.00518 0.00073

0.0614 0.0830 0.0878

0.0450 0.0727 0.0863

a = 0.527 b = 0.03738 c = 0.901

k'g = 0.714 k'k = ±0.1868 k'w = 0.01892

Table 8-6. Final values PVC

kg [min±1]

kk [min±1]

kw [min±1]

t0,5 [min]

5.0 % 7.5 % 10.0 %

0.03571 0.0536 0.0714

±0.00934 ±0.01401 ±0.01868

0.01892 0.01892 0.01892

16.7 13.3 11.1

8.3 Lightening Power

8.3

345

Lightening Power

8.3.1 Graphical Method Instructions for the graphical method are provided in standards*. The determination is based on the lightening power as defined in equation (4.75): It is the mass of reference white pigment that, when added to a colored paste of stated composition, yields the same lightness as with the reference pigment. A calibration curve, showing the CIE tristimulus value Y for the reference colored paste as a function of PVC, is used in the evaluation. In order to determine the lightening power, one disperses the test pigment, at an agreed-on concentration, in a certain quantity of the agreed-on colored paste. In this way, what is measured is the CIE tristimulus value Y for the mixture with colored or black base. From the calibration curve (measured Y values versus white pigment PVC of reference), the nominal PVC is read off; this is the value that would give the same CIE tristimulus value Y. The lightening power is then obtained as the ratio of masses calculated from the two PVC values. It is useful to plot, over the calibration curve, the associated curve from which the lightening power can be read off directly. The method can be further simplified by plotting Y directly against the pigment mass (instead of the PVC). The lightening power curve then becomes a straight line. The standards present examples of lightening power determination by a gray paste method and a blue paste method. The composition of the black paste is chosen such that the concentration of the black pigment in the gray pastes remains constant for all PVC values; this corresponds to the constant volume method. Here we go through the example, but using the adding pigment method for simplicity; in this technique, the Y values are plotted directly against the added masses of white pigment, so that only one black paste has to be prepared. Aside from the analytical balance, spatula, doctor blade, and so forth, the following apparatus will be needed: ± ± ± ±

Triple-roll mill Automatic muller Colorimeter Measuring setup for measurements on pastes, such as the paste film holder of Section 6.2.3 Preparation method: First prepare master carbon black paste: Carefully stir by hand 18.7 g Flammruss 101 (Degussa) 81.3 g Alkydal L64 (Bayer)

* See ªLightening Power of White Pigmentsº and ªScattering Power, Gray Paste methodº in Appendix 1.

346

8 Determination of Tinting Strength and Lightening Power

and pass through the triple-roll mill six times. Composition of the black paste for, say, a PVC of 15 % of the reference (density R = 4.1 g/cm3): ± 91.72 g Alkydal L64 ± 5.11 g Aerosil 200 (Degussa) ± 3.17 g master carbon black paste (see above) For other black paste compositions for other test PVC values or other pigment densities, see Table 8-7. Table 8-7. Compositions of black pastes. Pigment volume concentration (PVC)

Composition of black paste, g Alkydal Aerosil L 64 200 g g

Carbon black paste (Section 8.3.1)

Volume of white pigment per 2.50 g black paste (cm3)

5% 6% 7% 8% 9% 10 % 11% 12 % 13 % 14 % 15 % 16 % 17 % 18 % 19 % 20 % 21% 22 % 23 % 24 % 25 %

92.04 92.02 91.98 91.95 91.92 91.89 91.86 91.82 91.79 91.75 91.72 91.68 91.64 91.60 91.56 91.52 91.48 91.43 91.39 91.34 91.30

2.84 2.87 2.90 2.93 2.96 2.99 3.03 3.06 3.10 3.13 3.17 3.21 3.25 3.29 3.33 3.37 3.41 3.45 3.50 3.54 3.59

0.123 0.149 0.176 0.203 0.251 0.259 0.288 0.318 0.349 0.380 0.412 0.444 0.478 0.512 0.547 0.583 0.620 0.658 0.697 0.737 0.777

5.12 5.12 5.12 5.12 5.12 5.12 5.12 5.12 5.12 5.11 5.11 5.11 5.11 5.11 5.11 5.11 5.11 5.11 5.11 5.11 5.11

In order to generate the calibration curve of the reference, add increasing masses of white pigment to equal masses of black paste and place on the lower plate of the automatic muller. After mixing, distribute in the form of a circular ring. Mull in four stages of 25 revolutions each, under pressure of 1.5 N/cm2. After each stage, rehomogenize and redistribute. Prepare and measure each calibration paste twice.

8.3 Lightening Power

347

Testing method: Mix together 2.5 g of black paste and 1.684 g of test pigment, using the method described above. Measure the CIE tristimulus value Y of the resulting gray paste. From the calibration curve, read off the mass to be added such that the reference will exhibit the same Y value as the test. The calibration diagram for the example is shown in Figure 8-12 along with the lightening power line. From the curve it can be inferred that a reference quantity of 1.250 g corresponds to the Y value of the test, so that the lightening power is Pw = 1.250/1.684 = 74%. This value is also read directly off on the upper line. Figure 8-12 further contains the CIE tristimulus value X and Z of the reference, measured at the same time. With their help, the X and Z values of the reference at matching can be read off; these can be further analyzed together with the measured test tristimulus value in order to obtain the shade difference after color reduction (see Section 2.3.3). If the calibration curve were plotted as Y versus the logarithm of the added mass (instead of versus the mass itself), a straight line would again be obtained in the Beer's law range of PVC, according to equations (3.118) and (4.49). Such a calibration line is the basis for Grassmann and Clausen's method of determining the lightening power (see Section 4.8). It has been shown that the increase in the scattering interaction outside the Beer's law range (see Fig. 4-20) means no linear variation of lightening power with PVC can be expected. The advantage of the standard method is that it permits light-

Fig. 8-12. (Bottom) Calibration curve for Y with CIE tristimulus values X and Z. (Top) Lightening power versus added pigment mass of reference.

348

8 Determination of Tinting Strength and Lightening Power

ening power (and shade difference after color reduction) to be determined as a function of the PVC of the reference pigment. For this purpose, a special black paste as characterized in Table 8-7 must be prepared from the master carbon black paste for every new PVC. The procedure described above ± recording of a calibration curve, etc. ± must then be repeated for every PVC. It is clear that the method of determination needs a good deal of rationalization. This is the subject of the sections that follow.

8.3.2 Rationalized Method The method is described in the standards*. The Kubelka-Munk function is used for rationalization. As in Section 8.2.1, gray pastes with equal added masses of white pigment are prepared and their CIE tristimulus values Y are measured. After Saunderson correction of the Y values (eq. 4.112), the Kubelka-Munk functions F (eq. 3.117) are calculated for the reference and test. The ratio of scattering coefficients per unit pigment mass concentration then gives the relative scattering coefficient of the test pigment per unit mass (eq. 4.106). This is identical with lightening power, but only in the Beer's law range. The relative scattering coefficient itself is usually better stated in terms of volume; the conversion from the mass-referred quantity is easily given by the reference/test density ratio (eq. 4.103). When relative scattering coefficients obtained by this method are compared with those from the black-ground method of Section 7.2.1, the unlike nature of the methods means that complete agreement cannot always be expected. The apparatus and materials for this test are as listed in Section 8.3.1, and the same master carbon black paste is again prepared. The ISO standard describes the analysis at a fixed test PVC of 17 %; the German standard allows other PVC values, and it includes a table giving the required paste compositions for PVC values in 1% steps from 5 % to 25 % (see Table 8-7). In parallel to the lightening power, the shade difference after lightening power matching can also be calculated from the pigment mass added to match. The formulas for this calculation are collected in Table 8-8 as a programming aid. A printout of results appears in Figure 8-13. This method can be employed only in the Beer's law range; at higher pigment concentrations, the values contain errors, that is, they no longer agree with the values obtained by the Y matching method of Section 8.3.1. In such cases, it is necessary to use the first approximation of the lightening power, equation (4.105). This means that aw must be determined; it contains pigment data for the reference alone. The coefficient gR of the scattering interaction of the reference white pigment occurs in it. This is expediently determined by using the dilution method (see section 4.4.1), or simply from two gray mixtures containing quantities of the reference * See ªLightening Power of White Pigmentsº and ªScattering Power, Relative, Gray Paste Methodº in Appendix 1.

8.3 Lightening Power

349

Table 8-8. Formulas needed to calculate lightening power and shade difference after lightening power matching in the Beer's law range. ^ Y; ^ Z^ and X^ R ; Y^ R ; Z^ R for equal added pigment masses m^ Given: X; R^ 1 F^

R^

0:04

(4.112)

0:36 0:6 R^ R^ 2 2 R^

(3.117)

^ where 1) R^ Y=100 2) X^ R =Xn 3) Y^ R =100 4) Z^ R =Zn Pw

R^ Y^ =100 X^ R =Xn Y^ R =100 Z^ R =Zn

F^ F^Y F^X;R F^Y;R F^Z;R

F^Y;R F^Y

(4.106)

FX;R F^X;R Pw ;

FZ;R F^Z;R Pw

(4.67)

Then continue as in Table 8-1 (eqs. 4.111ff.). The CIELAB coordinates are substituted in the formulas for shade difference after color lightening power matching: Ds

p Da2 Db2 ;

Dj Arctan

Db Da

(2.16)

From Table 2-3, Dj ? nature of undertone.

that differ as widely as possible; in this case, two expressions are obtained from equation (4.48) (we now drop the subscript R): 2 1 1 3 (8.3) z1 c1 1 z 5 c1 j1 F1 FBP 3 2 1 1 3 j2 z1 c2 1 z 5 c2 F2 FBP 3 and thence g z5 3

j1 c2

j2 c1

j1 c2

j2 c1

5 3

(8.4)

5 3

The desired factor aw is calculated with equation (4.105): 2

aw g c^ 3

where

m^ c^ m

and m mBP

R RBP

350

8 Determination of Tinting Strength and Lightening Power

Program ªLPº Lightening Power, according to ISO 787-24 ********** Date: ..-..-.. Reference is A Test is B Medium and black paste: according to ISO 787-24 Colorimeter/Standard Observer: N.N., C/28 Measuring Conditions: d/8 (incl) Input:**************************************** Masses: Black paste: 2.5 g Pigment: 2.0 g Reflectometer values: Reference: Test: R'(x) 46.88 46.81 R'(y) 48.08 48.79 R'(z) 52.50 55.84 Output:************************************** Lightening Power: 105 % Lightness: 74.9 Color Difference after matching Type: Magnitude: blue Delta(s) = 2.8 Fig. 8-13. Lightening power and shade difference after lightening power matching for a white pigment, obtained by the rationalized method (computer output).

As a computational example, the values from Annex 1 of the German standard can be used again: m1 = 0.520 g, m6 = 2.062 g, Y1 = 32.6, Y6 = 50.4. The transformations made are, first the Saunderson correction (Y ? Y ++) and, second, the calculation of the Kubelka-Munk functions (Y ++ ? F); see Table 8-8 for the formulas: Y1++/100 (32.6/100 ± 0.04)/(0.36 + 0.6 7 32.6/100) = 0.515 Y++ 6 /100 0.700 1/F1 2 7 0.515/(1 ± 0.515)2 4.372 1/F6 15.61. Now, with 1/FBP = 0.027, equation (8.3) gives j1 = 4.372 ± 0.027 = 4.35 and j2 = 15.59. Given mBP = 3 g, RBP = 1.285 g/cm3, R = 4.1 g/cm3, and m = 3 7 4.1/ 1.285 = 9.57 g, the PMV values are found to be c1 = 0.520/9.57 = 0.0543 and c6 = 0.2155. By equation (8.4), then, g = (4.35 7 0.2155 ± 15.59 7 0.0543)/ (4.35 7 0.21555/3 ± 15.59 7 0.05435/3) = 0.422. Finally, with m^ = 1.689 g, equation (4.105) yields aw = 0.422(11.689/9.57)2/3 = 0.1328. In the DIN example (see Fig. 8-12), the mixture of the test gray paste has a CIE tristimulus value Y = 44.0. If the associated F value is substituted in equation (4.105) together with the value just calculated for aw, the result is a lightening power of P(1) w = 74 % ± in extremely good agreement with the graphical solution (whereas the zero-th approximation

8.3 Lightening Power

351

would have given P(0) w = 76 %). Thus the example shows that the first approximation still supplies correct values far away from 100 % lightening power. If X and Z (or R'x and R'z ) are measured at the same time, then from any pair of values (X1, X6 and Z1, Z6) the coefficients zX1, zX5/3 and zZ1, zZ5/3 of the KubelkaMunk functions FX and FZ of the reference can be caluclated with equation (4.109). Thus the CIE tristimulus values XR and ZR of the reference at matching are accessible, and from these together with X, Z of the test, the shade difference after lightening power matching can be determined. Even with this new method, a black paste must be mixed for every new PVC, and new gray mixtures must be prepared. Section 8.3.3 will show how the entire curve of lightening power versus PVC can be obtained from a single gray mixture.

8.3.3 PVC Dependence from One Gray Mixture This method requires only a single mixture of pigment with black paste but yields values for the lightening power throughout the PVC range of interest. The key to the method is a rather simple relation with which the dilution method (Section 4.4.1) can be used to obtain the coefficient zw5/3 = g (eq. 4.52). Accordingly, one need only dilute the initial gray paste in a known ratio with additional vehicle ± i. e., the black paste without black pigment ± in order to calculate g from the two Kubelka-Munk functions. This test can be performed much more quickly than any of the determinations that have been discussed, because the pacing step is mixing in the automatic muller. All that is required for dilution is more stirring. One of the preparation methods set forth above can be employed for the preparation of the starting mixture. The algorithm uses equations (4.51) and (4.52) to calculate g, then equation (4.48) to calculate the other coefficient z1. If both coefficients are known for both test and reference, equation (4.102) can be used with pw1 = 0 to draw or plot the full curve of lightening power versus PVC. Table 8-9 lists out the formulas needed for programming, and Figure 8-14 shows a flowchart for the procedure. The data needed for the dilution require some separate calculations; these are also described in Table 8-9. First, the volumetric dilution factor qD = s/ sA is fixed. The volume ratio of white pigment/black paste mixture (ªgray pasteº, subscript GP) VGP to medium VM to be added is then derived from sA = V/VGP and s = V/(VGP + VM), where V is the volume of white pigment: VM 1 VGP qD and mM mGP

RM RGP

1

1 qD

1

(8.5)

352

8 Determination of Tinting Strength and Lightening Power

Table 8-9. Formulas needed for calculation of lightening power and shade difference after lightening power matching as functions of PVC. Given: c^ A ; X^ A ; Y^ A ; Z^ A ^ X; ^ Y; ^ Z^ c;

before dilution

of test and reference (subscript R)

after dilution

Saunderson correction and calculation of Kubelka-Munk functions of all values with equations (4.112) and (3.117), (see Table 8-8): gY

1

F^Y;A

F^Y;A 2

sA3

F^Y 2

s3

where s

c 1c

(4.51), (4.52)

similarly gX, gZ of test and reference: jA

1 FY;A

1 ; FBP

zY1

jA cA 1

(4.48)

2

gY cA3

similarly zX1 , zZ1 of test and reference: pwo

zY1 ; zY1;R

P 1 w

RR pw0 1 R

1 FX;A 1 FZ;A

pw 2 gY 3

2

3 pwo gY;R

pw1 0

(4.104)

s 2 3 1 s 3 1 s s 23 1 1 g zX1 P 1 P X w w FBP 1 s 1 s 1 s s 23 1 1 g zZ1 P 1 P Z w w FBP 1 s 1 s pw 2

(4.102) (4.109) (4.66)

Then continue as in Table 8-1 (eqs. 4.111 ff.). The CIELAB coordinates are analyzed to give shade difference after lightening power matching, as in Table 8-8 (eq. 2.16 and Table 2-3). Lightening power and shade difference after lightening power matching can be plotted (manually or by computer) versus s. Dilution data: If sA is to be lowered to s by dilution, the volumetric dilution factor is qV = s/sA. The following must then be calculated: m mSP w

R 4:4 ; RBP

m 4:1 ; m mBP

c

m 4:6 ; m

RGP

s

Rs 4:17 ; w

c 1c mM mGP

(4.15) RM RGP

1 qD

1

(8.5)

8.3 Lightening Power

353

Fig. 8-14. Flowchart for determining lightening power and shade difference after lightening power matching as functions of PVC from a single gray mixture.

354

8 Determination of Tinting Strength and Lightening Power

To convert columes to masses, the density of the gray paste must be known. It can be found in the following way: First, the PVM m (eq. 4.4) and thence, with the PMV c (eq. 4.6), the PVC s in the gray paste are calculated (eq. 4.15). Together with the PMP w, equation (4.1), the density RGP of the gray paste is then obtained with equation (4.17). The prodecure can be illustrated by an example. The starting values are as follows: m = 5 g, mBP = 6.5 g, R = 3.957 g/cm3, RBP = 1.286 g/cm3. Then m = 6.5 7 3.957/1.286 = 20.00 g, c = 5/20 = 0.2500, s = 0.25/(1 + 0.25) = 0.200, w = 5/(5 + 6.5) = 0.435, RGP = 3.957 7 0.2/0.435 = 1.819 g/cm3. If the PVC is to be reduced from 20 % to 0.5 % by dilution, qD = 0.005/0.2 = 0.025. The mass of med-

Fig. 8-15. Lightening power versus PVC for three rutile pigments (series 1).

Fig. 8-16. Lightening power versus PVC for three rutile pigments (series 2).

8.3 Lightening Power

355

ium required for 0.5 g of gray paste is then obtained from equation (8.5): mM = (0.5 7 1.231/1.839) 7 (1/0.025 ± 1) = 13.05 g. Figures 8-15 and 8-16 give plotted curves of lightening power versus PVC for a total of six white pigments, all against the same reference. The curves show that pigments initally having a better relative lightening power may well become worse at higher PVC, and vice versa. It should be kept in mind that lightening power values for PVC s 4 30 % do not necessarily represent reality, because of the possibility of a pigment concentration exceeding the critical PVC. In calculating the shade difference after lightening power matching, one proceeds in an analogous way. Again, equations (4.52) and (4.109) are used to calculate g and z1 from the Kubelka-Munk functions of the CIE tristimulus values X and ^ w is substituted in the equations. Similarly to Z, and the mass added at matching mP what was done in Table 8-1 and 8-7, the strength and nature of the undertone are then inferred; they can also be plotted in suitable form as functions of the PVC. This test can be performed in less than 20 minutes (up to plotting of the curves). At our current level of knowledge, an interim goal ± a more rational test for lightening power has thus been attained with the method just described.

Appendix 1 Listing of Standards Key words Change in tinting strength (see Dispersion and PVC) Coating materials, terms and definitions

ISO

ASTM

BS

NF

JIS

DIN

4618-1 to 4

D 16

2015

T 36-001 T 36-005

K 5500

Color depth Color differences: CIELAB

55945 EN ISO 4618-2 to -4 EN 971-1 53235-1 to 2

7724-3

D 1729 D 2244 E 308

3900-D10

T 36-004-3

K 5600-4-6

6174

T 36-004-2

K 5600-4-5

6176 53236 55600

CIE94 CMC DIN99 Conditions/evaluation of measurement Significance Color in full-shade systems: Black pigments Colored pigments White pigments Color matching Color matching functions in steps of 20 nm Color measurement (see also Color differences) Color tolerances for automotive paints Colorimetry Coloring materials: Classification

7724-6 7724-4

6923

7724-2 787-25 787-25 787-25 3668 7724-2 7724-1 to 6 7724-2

3900-D9 D 3022 D 3022 D 2805

3900-D1

T 30-061

K 5400

E 308 E 259 E 308

4764 3900-D8 3900-D9

T 36-004-1 T 36-004-2

K 5600-4-4 K 5600-4-5

55985-2 55985 55983 6173-1 ISO 3668 53218 6175-1 to 2 5033-1 to 9 55944

Automatic muller Bead mill Change in gloss Change in tinting strength Fineness of grind (see below) High speed impeller mill Introduction Oscillatroy shaking machine Triple roll mill Emulsion paints Film thickness

8780-5 8780-4 8781-3 8781-1

Fineness of grind Gloss, measurement Hiding power: Color difference method Contrast ratio (opacity): of light-colored paints General introduction Pigmented media Wedge-shaped layer

787-23 787-10

ASTM

D 153

D 387

8780-3 8780-1 8780-2 8780-6

BS 2015

NF

JIS

EN ISO 787-23 EN ISO 787-23

T 31-201 T 31-202

K 5101

EN ISO 8780-5 EN ISO 8780-4 EN ISO 8781-3 EN ISO 8781-1

T 31-210-5 T 31-210-4 T 31-220-3 T 31-220-1

EN ISO 8780-3 EN ISO 8780-1 EN ISO 8780-2 EN ISO 8780-6

T 31-210-3 T 31-210-1 T 31-210-2 T 31-210-6

2808 1524 8781-2 2813 6504-4 6504-3 6504-0 6504-5

D 1210 D 523 D 5307

3900-C6 EN ISO 8781-2 3900-D5 EN ISO 2813

T 30-120 to 125 EN 21524 T 31-220-1 T 30-064

K 5101

K 5101 K 5400 K 5101 K 5400 K 5600-4-7

DIN 55943 EN ISO 787-10 EN ISO 787-1 6164-1 to 3 53238-30 53238-33 53238-31 53238-32 EN ISO 8780-5 EN ISO 8780-4 EN ISO 8781-3 EN ISO 8781-1 EN ISO 8780-3 EN ISO 8780-1 EN ISO 8780-2 EN ISO 8780-6 53778-3 EN ISO 2064 EN ISO 2808 EN 21524 EN ISO 8781-2 67530 EN ISO 2813

3900-D11 D 2805

3900-D7

55987 55601

Appendix 1

ISO 4618-1

358

Key words Terms and definitions Density of pigments: Centrifuge method Pyknometer method DIN Color System Dispersion, ease of: Alkyd resin and alkyd melamine system: Drying by oxidation: Stoving type

Key words White and light-colored paints White and light gray media Hue of near white specimens Hue relative of near white specimens Lightening power of white pigments Lightness: Emulsion paints (see above) White pigment powders Loss on ignition (Red iron oxide pigments) Metamerism index Mixtures, Composition Particle-size analysis Basic terms:

ASTM D 2805

BS 3900-D7

NF

7724-5 787-24

D 2745

3483-A5 EN ISO 787-24

T 30-023 T 31-228

1248

D 3721

3981

T 31-002

JIS

5775-6 13320-1 13319 13322 13321 9276-1 9276-2 9276-4

13318-1 to 3 13317-1 to 3 13323-1

ISO 13320-1 3406-1 to 9 ISO 13319 D 1366

D 3360

DIN 55984 55980 55981 53165 55982 53163 55913-1 6172 1310

3406-8

X 11-666-1 X 11-671 X 11-696 X 11-672

ISO 9276-1

X 11-632-1

66141 66144 66143 66145

Z 8820 T 30-044 Z 8822 X 11-685-1 to 3 X 11-680-1 to 3 Z 8821

66160 66111 66115

359

5036-1, 3 to 4 55678-1 to 3

Appendix 1

Electrical sensing zone Image analysis method Photon correlation spectroscopy Representation: Basic terms Logarith. normal diagram Power function grid RRSB grid Sedimentation methods: Balance method Basic standards Centrifugal liquid Gravitational liquid Pipette method Single particle light interaction method Photometric properties of materials Pigment content

ISO 6504-1

Thermoplastics Tinting strength, relative: Carbon black Change in (see Dispersion and PVC) Colorimetric method Dyes in solution FIAF method (see Color depth) Inorganic pigments

ASTM

BS

NF

JIS

DIN 53773-1 53773-2 53775-1 53775-7 53775-3 53774-1 53774-2

15528

D 3925

EN ISO 15528

T 30-048

787-24 6504-1

3483-A6

EN ISO 787-24

31

5775

X 02-001

K 4001 K 5101 K 5400

EN ISO 15528

ISO 787-24 53164 Z 8202

1301-1 to -3 1303 1304 EN 12877-1 to 2

D 3349 55986 55978 55603

Appendix 1

Scattering power, relative: Gray paste method Black ground method Significances (see Color differences) Symbols for use in formulas

ISO

360

Key words PVC, paste: Basic mixture Test specimen preparation PVC, plasticized: Basic mixture Change in tinting strength Test specimen preparation PVC, unplasticized: Basic mixture Test specimen preparation Radiometric properties of materials (see Photometric properties of materials) Reflectometer (see Gloss) Residual color difference (see Tinting strength) Sampling

Key words Lightness method Organic pigments (see Color depth) Photometric methods Visual Weighted K/S value method Transmission of optical radiation Transparency (Pigmented/unpigmented systems)

ISO

ASTM

BS

NF

787-24

D 387 D 3022 D 4838

EN 787-24

T 30-031 T 31-228

55978 EN ISO 787-24

EN ISO 787-1

T 30-027 T 31-227

EN ISO 787-16 1349

787-16 787-26

JIS

DIN 55603

1349-1 to 2 55988

Appendix 1

361

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

Subject Index

A absorbing power 3±9, 71±130, 131±196, 207±226 ± test method 233±235, 254, 255, 325±327 absorption coefficient 11, 71±130, 137±141, 207±226 ± four-flux theory 78±83, 138±141, 291±296 ± Kubelka-Munk theory 78±81, 138±141, 282±296 ± ± determination 283±296 ± ± ± error 287±293 ± ± per unit mass 138, 327, 328 ± ± ± relative, determination 327 ± ± per unit volume 150±152, 191, 192, 219±226 ± many-flux theory 72±75 ± test methods 252, 253, 282±296, 327±333 absorption cross-section 11, 219±222, 224±226 absorption index 11, 213±217, 224±226 absorption maximum 140, 141, 167, 168, 325, 327, 340 acceptability 16, 59±62, 241, 242, 277; see also ellipsoid, acceptability adding-pigment method 146±149, 327, 328 agglomerate 132, 208, 236, 237 aggregate 132 anisotropy, optical 215, 216 application error 58 B basic conditions (CIE94) 36, 37 Beer's law 138±140 ± region 140±144, 284, 335±338 black standard see colorimeters black value 251, 252 brightness see lightness C characteristic equation 47, 74, 257, 258 chi-square distribution 45, 57

chroma 29, 105, 169±171 ± test methods 247±252, 308, 329 chroma difference, principles 32±34, 105, 169±171 ± test methods 247±252, 308, 329 CIE chromaticity coordinates 23±26, 246, 333 CIE chromaticity diagram 25, 274, 275 Cie color matching functions 23±26, 118, 119, 160±161, 243±248, 299 CIE color notation system 20±26, 116, 184, 185, 247, 248 CIE standard colorimetric system see CIE color notation system CIE standard illuminants 17, 119, 160±163, 246, 255 CIE standard observer See CIE color notation system CIE tristimulus values 23±26, 119, 159±165 ± test methods 243±248, 284, 327±329 CIELAB color space 31, 36, 168±171, 257±259, 273, 274 CIELAB coordinates 28±36, 115±117, 168, 249, 250±252, 329 CIELAB system 28±36, 116, 118, 188±191, 246±248, 308, 309 CIE94 system 36±38 CMC system 38±39 coating materials 3 ± thickness see film thickness colloid chemistry 131, 133±138 color depth 169±171, 327, 332, 333 ± criteria 184±186, 332, 333 ± level see standard depth of shade ± matching 184±186, 328±333, 335±337 ± standards 328±333 color difference 15, 104, 105, 167±171 ± after color reduction 188±191, 327±333; see also shade difference ± test methods 239±242, 296, 329

364

Subject Index

color formulation 15, 167±169, 177, 178, 294±295, 335±337 color identification code 15 Color Index 41 color matching 172±187, 267±276 ± trichromatic, theory 23 color measurement 10, 15±17, 278 ± errors 54±57, 100, 101, 259±263 ± ± ellipsoid 257±260 ± ± preparation 249, 259±263 ± ± ± ellipsoid 260±263 ± test errors 255±263 ± ± ellipsoid 255±263 color mixing 20 color, object see object color color order systems 39±41 color plane 29, 33±35 color rendering 15 color sample 39, 241±243, 332, 333 color saturation see saturation color space, absolute 27, 40 ± CIELAB see CIELAB color space ± euklidean 37, 39 color stimulus 9±12, 15, 27, 115, 253, 254, 267, 268 color systems 15, 26 ± perceptual 26±36 ± physiologically equidistant 7, 28 color tolerances see acceptability colorimeters 17±19, 76±78, 237±242, 285, 327, 328 ± black standard 243, 244, 251, 252, 303, 304 ± calibration 243, 244, 284, 332, 333 ± light sources 242±244, 269, 270 ± measuring conditions 19, 76±78, 237±242, 253, 254, 285, 286, 287, 327, 328 ± sample illumination 253, 254 ± spectrophotometer see spectral method ± three-filter see tristimulus method ± trichromatic matching 23, 27 ± white standard 19, 244, 303±304 colorimetry 10±12, 15±50, 178, 179, 234, 235, 332, 333 coloring material 3±9, 208, 240±242; see also dyes; pigments coloring power 111±113, 121±123, 182±184, 277, 297, 298 ± condition (measurement) see colorimeter ± determination 299

confidence interval, level 57, 247, 248, 255±257, 264, 271, 272 conformity (with standard) see acceptability constant-volume method 146±149, 345 contrast ratio 104, 105, 308, 309 contrast substrate 104±110, 144, 145, 249, 287, 288 corpuscular theory 71, 207±226 cosine distribution, Lambert's 76, 234, 235 covariance 54±56, 58, 255, 256, 264, 265 ± matrix 55, 56, 255, 256 critical value see confidence interval D daylight color 252, 253 dilution method 146±149, 348 DIN Color system 41 dispersing (dispersion) of pigments see pigments, dispersing dispersing resistance 344 dispersion (colloid chemistry) 131±138, 241±243 ± density 137, 138 dispersion, anomalous (optics) 225, 226 distribution ± cumulative 218, 219 ± density 217, 218 ± width 218, 219 see also normal distribution; lognormal distribution dye 71, 131±138, 323±325 ± content 71, 131±206, 254, 255, 323±325 ± test methods 240, 241, 252±255, 267, 268, 323±325 E effectiveness 104, 183, 184, 318±321 ellipse ± axes 212 ± coefficients 43 ± eccentricity 212 ± standard deviation 43, 212, 213 ellipsoid ± acceptability 59, 267±276 ± coefficients 52±55, 255±263 ± conditions 46, 51±55, 257, 258 ± normal form 46, 47, 50, 57 ± principal axes 46±49, 257±260 ± ± system 47, 259, 260 ± projections 49, 257±260

Subject Index ± radius 51 ± standard deviation 44±51, 55, 56, 255±257 see also color measurement, errors equi-energy stimulus 25 equivalent diameter 133 Eurocolor system 41 F FIAF method 184±187, 228±240 fillers (extenders) 3, 133, 134, 215, 216, 249, 324 film thickness 11, 78±81, 138, 139 ± test methods 249, 277±287, 315, 316 ± measurement 277±283 ± ± chemical, electrical, magnetic, optical methods 278 ± ± dial-gauge micrometer methods 280±282 ± ± errors 277 ± ± gravimetric methods 279, 303, 304 ± ± pneumatic methods 281±283, 300, 301, 303, 304, 318, 319 ± ± wedge cut method 279, 280 floating 134, 262, 263 flocculation 132, 134, 242, 243 fluorescence 253, 254 four-flux theory 71, 72, 74, 78±96, 291±293 Fresnel equations 233, 236, 237 Fresnel reflection 221±224, 233 full shade 134, 239±241 ± black 231, 240, 247±252 ± chromatic 247±252 ± ± determination 303, 304 ± white 247±252 full-shade system 242, 243, 247, 248, 267, 268 G gloss 105, 134, 234, 296 ± degree of 108, 236, 237, 240, 241, 305±308, 315, 316 ± high 234, 240, 241, 285, 296, 297 ± mat 234, 240, 241 ± measurement 233±238 gloss angle 236, 237 gloss exclusion (trap) 239±241 gloss haze 134, 336±341 gloss indicatrix 234, 235, 255, 256 glossmeters 234, 235, 254±256 goniophotometers see glossmeters Grassmann's laws 20 gray scale 29

365

H Helmholtz equation 217, 218 hiding criterion 104, 105, 301±303, 311, 312 hiding power 104±110, 115±121, 164±166, 277±321 ± economic aspects 318±321 hiding power value 104, 106±110, 277, 301±321 ± absorption component 108, 109, 306±308, 315, 316 ± achromatic, determination 304±309 ± graphical determination 301±308, 311, 312 ± interaction component 109, 110, 308, 309, 311, 312, 315, 316 ± scattering component 108, 109, 306±308, 315 histogram 209, 212 homogeneity error 58 hue 26, 27, 53, 54, 105, 167, 168 ± test methods 249, 250, 308, 325 hue angle 29, 250, 251 ± difference 32, 33, 250, 251 hue difference 32±34, 53, 54, 105, 172 ± test methods 249, 250, 308, 329 hue (shade, undertone) 33±35, 188±191, 249±252, 327, 328 ± near-black specimens 249±252 ± near-gray specimens 105, 249±252, 308 ± near-white specimens 105, 249±252, 308 I immersion method 216, 217 incandescent light color 252, 253 infinitely thick layer 92, 93, 284 integrating sphere 237±240, 249, 253, 254 K Kubelka-Munk ± function 97±101, 139, 140, 195, 323, 327±329 ± ± error of determination 100, 101 ± theory 11, 72, 145, 146, 149±165, 219, 220, 283±293 L Lambert's law 72, 78, 79, 85, 86, 138, 139 light absorption power see absorbing power light scattering power see scattering power

366

Subject Index

lightening power 131, 148, 149, 165, 166, 186±188 ± determination 345±355 ± ± graphical 345±348 ± ± per unit PVC 350±355 ± ± rationalized method 347±351 ± test methods 284, 287±291, 345±355 ± ± Reynolds 149, 150 lightness 26, 27, 168, 169, 247±252, 310, 311, 327, 329 ± difference 32±34, 104, 105, 247±250, 304, 305 ± matching 178±187, 327±333 likelihood see maximum likelihood method lognormal distribution 209, 211±213 ± two-dimensional 211±213 M many-flux theory 71±75, 291±293, 294±296 mass tone 247, 248 matching criteria see tinting strength criteria matrix inversion 255±257, 262, 263 maximum likelihood method 59, 272 measurement error 58 metallics 4, 254, 255 metamerism 23, 246, 251±253 ± geometrical see Silking effect ± index 252, 253 Mie minimum 222, 223 Mie theory 11, 74, 207, 217±226, 294, 295 Munsell system 28, 36, 40 N nacreous pigments 4, 255 Natural Color System 40 Newton's method (approximation) 107, 120, 121, 196, 272, 314±316 nonluminous perceived color see object color non-self-radiating medium 17 normal distribution ± logarithmic see lognormal distribution ± one-dimensional 42, 209±211, 259, 260 ± three-dimensional 42±45, 259, 260, 264, 269, 270 ± two-dimensional 43 O object color 17, 19, 23, 233±276 one-flux theory see Lambert's law optical brighteners 253, 254

optical contact 285±287, 303, 304 OSA-UCS (color order system) 41 Ostwald color system 41 P parametric factors (CIE94) 36±38 partial oscillations 217±222 particle size ± fractions 218, 219 ± optimal 222±224, 225, 226 ± parameters 133, 208±213 particle-size 11, 71, 131±133, 207±223, 296, 297 ± analysis 212, 213 ± distribution 133, 167, 168, 208±213, 220, 221, 225, 226 ± ± analysis based on volume effects 213 ± ± class 209±211 ± ± light scattering analysis 213 particles 11, 71, 131±138, 207±226 ± anisometric 211, 219, 220, 252, 253 ± counting 213 ± diameter 133, 208, 215, 216 ± form 131±133, 220, 221 ± mass 133, 208 ± number 208 ± ± analysis see particle-size analysis ± ± distribution see particle-size distribution ± surface area 133, 208, 215±217 ± test methods 236, 237, 252, 253, 296, 297 ± volume 133, 209±211, 215, 216, 220, 221 paste film holder 249, 250, 346, 347 perceptibility 16, 269, 270, 273, 274 phenomenological theory 71±130, 207 Pigenot equation 191±193 pigment content 11, 71, 131±138, 213 ± determination, centrifuge method 324 ± ± filtration method 324, 325 ± ± incineration method 324 ± test methods 236, 237, 324, 325 pigment distribution see particle-size distribution pigment mass 135 ± concentration (PMC) 135±137, 283±285, 327, 328, 347, 348 ± equivalent to the medium volume (PVM) 136, 137, 179, 180, 351, 354 ± equivalent to the medium volume of the mass portion (PMM) 136, 137 ± per unit area 284 ± portion (PMP) 135±137, 283

Subject Index pigment/medium volume ratio (PMV) 136, 137, 347, 348 pigment particle see particle pigment/paste mixing 146±165 pigment surface area see particles, surface area pigment surface concentration 137, 138 pigment volume see particles, volume ± concentration (PVC) 116, 135±138, 236, 237, 279 ± ± critical 134, 140, 141, 354, 355 ± portion (PVP) 137, 138 pigments 3±9, 131±138, 207±226 ± black 4, 5, 146, 147, 151±156, 239±241, 287±293, 327±333 ± colored 4, 6±8, 108, 146, 147, 157±165, 207±226 ± ± test methods 247±252, 256±258, 287±293, 327±333 ± density 136, 137, 279, 346 ± dispersing (dispersion) 132±135, 208±213, 236, 237, 284, 340, 341 ± ± equipment 241, 242, 284, 327, 328, 341, 345±347 ± ± rate of 191±196, 342±344 ± ± resistance 196, 344 ± fluorescent 4±5, 253, 254 ± interference 4, 255, 256 ± luminescent 4±5, 253±255 ± luster 4 ± metal-effect 4, 236, 237, 254, 255 ± nacreous 4, 255, 256 ± phosphorescent 5, 253±255 ± test methods 236, 237, 283, 324, 325 ± transparent 325±329 ± visual 23 ± white 4±5, 108, 109, 146, 147, 156±158, 207±226 ± ± test methods 247±252, 283±288 PMC see pigment mass concentration PMM see pigment mass equivalent to the medium volume of the mass portion PMP see pigment mass portion PMV see pigment/medium volume ratio polarized light 214, 215, 217±219 power-law distribution 209 preparation error 58 primary particle 132, 143 primary stimulus 20, 21, 24, 27 probability, cumulative 44, 212

367

probability density 44, 212 production monitoring (control) 15±17, 182, 183, 249, 327, 328 PVC see pigment volume concentration PVM see pigment mass equivalent to the medium volume PVP see pigment volume portion R radiance factor 18 radiative transfer 66, 67 RAL Color Register 40, 41 RAL-Design-System 41 rate constants (dispersing) 191±196, 342±344 Rayleigh scattering 221, 222 reaction kinetics 191±196 reference stimulus see primary stimulus reflectance 10±12, 17±19, 71±130, 150±152, 225, 226 ± errors of measurement 100, 101, 277, 287±293 ± test methods 233±242, 277 reflection see also reflectance ± coefficients 75±76, 122, 214, 215, 233±242, 293, 294 ± factor 17±19, 75±78, 233±242, 277, 327 ± law 224, 225 ± specular 86±91, 234, 254, 255 reflectometer values 169±171, 236, 296, 297, 327, 328 refractive index 11, 71, 213±217, 233 ± complex 213, 214, 218, 219 ± mixing rules 216, 217 retina 31 rhodopsins 23 RRSB distribution 209 rub-out test ± determination 341 ± method 242, 243 Ryde theory 71, 84 S sampling 241, 242 ± error 58 saturation 26±27, 40, 167, 168, 175±177, 253, 254 Saunderson correction 75, 151, 152, 285, 327±329 ± dependent (multiple) see scattering interaction

368

Subject Index

scattering coefficient 11, 71±130, 138, 139±146, 207±226 ± four-flux theory 78±83, 137, 138, 291±296 ± Kubelka-Munk theory 78±81, 143, 144, 277, 282±296 ± ± error of determination 117, 118, 277, 287±293 ± ± per unit mass 283±293, 347±351 ± ± per unit volume 143, 150, 151, 220, 221, 286, 287, 347, 348 ± ± ± relative see scattering power, relative ± many-flux theory 71±75 ± test methods 252, 253, 283±296 scattering cross-section 11, 219±225 scattering interaction 11, 140±144, 348±351 scattering power 4, 9, 10, 71±130, 131±196, 207±226 ± relative 277, 283, 284 ± ± black-ground method 284±288, 347, 348 ± ± determination, paste methods 347±351 ± test methods 233±242, 277, 340, 341 SDS see standard depth of shade secular equation see characteristic equation sedimentation analysis 213 shade difference after color reduction 188±191, 332, 333, 336±348; see also hue (shade, undertone) shape factor 212 sieve effect (Kubelka-Munk theory) 288 significance 16, 57, 58, 247±249, 255±257, 262±268 ± level see confidence interval ± test 264±268 Silking effect 252, 253 size reduction see pigments, dispersing (dispersion) Snell's law 214, 215 special color differences 27±28, 119, 239±242, 304, 305, 329 spectral colors 20±21 spectral evaluation, principle of 115±118, 298±301, 328±340 spectral locus 21, 26 spectral luminosity curve (spectral luminous efficiency function) 26 spectral method 121, 122, 243, 244, 298±300, 325±327 stabilization see pigments, dispersing (dispersion) standard depth of shade 175, 328±334

standard deviation 42, 43, 51±55, 257, 258, 327 standard deviation ellipse see ellipse, standard deviation standard deviation ellipsoid see ellipsoid, standard deviation standard illuminants 23, 24, 37 standard observer see SIE color notation system surface chemistry 215±217 surface correction see Saunderson correction surface reflection 75±78, 97, 233±242, 279, 327, 328 T thermochromism 253 tinting characteristic 168±171 tinting strength 164±187 ± absolute 166, 167, 182, 183 ± change in (increase in strength) 191±196, 236, 237, 340±344 ± criteria 167±172, 327 ± matching 297, 298, 329±333 ± relative 115, 131, 236, 237, 283, 284, 323±355 ± ± of coloring maerials, determination 325±341 ± ± of pigments, inorganic, determination 327±333 ± ± of pigments, organic, determination 328±340 tinting strength equivalent 166, 167, 332, 333 total error 58 transmission see transmission factor; transmittance transmission factor 19, 82±86, 138, 139 ± test method 233±242, 291±295, 325, 326 transmittance 19, 74 ± test methods 233±242, 291±293, 325, 326 transparency 110±114, 121±123, 277±321 ± number 110±114, 122, 123, 277, 296±299 ± ± single-point method determination 297±300 ± ± two-point method 296±300 transparency-coloring degree 113, 122 ± determination 297, 298, 317 ± transparency-coloring power 112, 122 trichromatic principle 21±23 tristimulus method 169±171, 243±248, 297, 298, 327±333 two-flux theory see Kubelka-Munk theory

Subject Index V van de Hulst formula 221±225 van der Waals forces 133 vision, color 23 ± cones 23, 31 see also pigments, visual volume distribution 209, 213

W wave equation 213, 214, 217, 218 wavelength 11, 115, 140, 141, 213±217 ± test methods 222±226, 288±291 Weber-Fechner law 28 wetting 133 white locus see equi-energy stimulus white standard see colorimeters

369

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

Name Index

A Abramowitz, W. 69 Adams, E. Q. 67, 68 Aitchinson, J. 230 Allen, T. 205 Atkins, J. T. 128, 129, 295 B Beasley, J. K. 129 Beattle, H. 230 Beer, A. 131, 139±141, 143, 149, 152, 154, 157, 187, 188, 204, 205, 284, 287, 303, 335, 347±348, 349 Berger, A. 68 Berger-Schunn see Berger Bessel, F. W. 218 Billmeyer, F. W., Jr. 68, 69, 128, 129, 295 Blumer, H. 230 Booth, G. 13, 206 Born, M. 68 Bouguer, P. 72, 127 Brockes, A. 68, 69, 128, 129, 230 Brossmann, R. 230 Brown, J. A. C. see Aitchinson Brown, W. R. J. 67, 68 Bçchel, K. H. 13 Bçchner, W. see Bçchel Buxbaum, G. 13 C Chandrasekhar, S. 128, 129 Channon, H. J. 129 Clausen, H. 205, 206, 347 Cremer, M. 130 D Descartes, R. 235, 257 Dettmar, H.-K. 229, 230 Duntley, S. Q. 127±129

E Eitle, D. 128, 129 Euclid 40 F Fechner, G. T. 28 Felder, B. 230 Fisher, R. A. 67 Fresnel, A. J. 75, 76, 214, 215, 221, 223, 230, 233, 236, 243 Friedrichsen, K. 206, 335, 337±339 Fritzsche, E. 13 Fukshanski, L. 127, 129 G Gall, L. 67, 68, 128, 130, 172, 175±178, 184± 186, 204±206, 328±339 Gans, R. 230 Gardner, H. A. 206 Gauss, F. K. (C. F.) 16, 45, 67 Geissler, G. 206 Grassmann, H. 20, 66, 68, 205, 206, 347 Grassmann, W. see Clausen Guild, H. 66, 68 Gurevic, M. 127, 129 H Hauser, P. 230 Hediger, H. 230 Heine, H. 13 Heller, W. 230 Helmholtz, H. von 23, 66, 68, 217 Hengstenberg, J. 69 Herbst, W. 13 Honerkamp, J. 230 Honigmann, B. 132, 205, 230 Howe,W. G. 69 Hubel, D. H. 68 Hunger, K. see Herbst Hunt, R. W. G. 68

372

Name Index

J Jaenicke,W. 206, 229 Joos, G. 230 Judd, D. B. 128, 129, 204, 206 K Kaluza, U. 204, 205 Kåmpf, G. 128, 130, 204, 205 Keifer, S. 128, 130, 134, 169, 172, 177, 204± 206, 319 Kerker, M. 229, 230 Klaeren, A. 205 Koch, O. 204, 206 Kæhler, P. see Buxbaum Kortçm, G. 128, 129, 229 Koutnik,V. 230 Kreyszig, E. 69 Kroker, R. 205 Kronecker, L. 73 Kubelka, P. 294 and see Munk L Lambert, J. H. 72, 75, 79, 85, 86, 126, 139, 204, 234 Laplace, P. S. 213, 217 Legendre, A. M. 74, 293, 294 Leschonski, K. 205 Lowan, A. N. 229, 230 M MacAdam, D. L. 67, 68 Madelung, E. 143 Maikowski, M. A. 230 Maxwell, J. C. 213 McLaren, K. see Booth Meehan, E. J. see Beattle Metz, H. J. 230 Mie, G. 11, 74, 207, 208, 217±226, 229, 230, 294 Mudgett, P. S. 128, 129, 220, 293, 295 Mçller-Kaul, W. see Geissler Munk, F. 11, 72, 84, 86, 88, 92, 93, 96±103, 105±109, 113±122, 127±129, 139, 146±165, 171, 178±184, 204, 219, 220, 223, 283±293, 300, 317, 323, 327±329, 333, 335, 340, 342, 343, 348, 350±353, 355 Munsell, A. H. 28, 35, 40, 65, 67, 68 Murley, R. D. 230

N Nassenstein, H. 230 Newton, I. 66, 68, 107, 119, 120, 129, 271, 314 Nickerson, D. see Adams O Ostwald, W. 23, 41 P Paffhausen, W. 69 Panek, P. see Buxbaum Pauli, H. 128, 129, 230 Pigenot, D. von 192, 194, 204, 205, 342 Pluhar, P. see Kroker R Rabe, P. see Koch Rayleigh, J. W. 221, 222, 229, 230 Rembrandt van Rijn, H. 235 Renwick, F. F. 127, 129 Reynolds, C. E. 149, 150, 205 Rich, R. M. see Howe Richards, L. W. see Mudgett Richter, M. 67, 68 Robertson, A. R. 67±69 Ræmer, H. see Honerkamp Ryde, J. W. 71, 83, 86, 91, 92, 127±129 S Saunderson, J. L. 75, 83, 97, 102, 117, 118, 128, 129, 182, 289±291, 294, 305, 311±313, 328, 329, 333, 334, 348, 350, 352, 353 Schliebs, R. see Bçchel Schmelzer, H. 69, 204, 206, 333 Schmitt, K.-H. see Hengstenberg Schmitz, O. J. see Kroker Schrædinger, E. 68 Schuster, A. 127, 129 Sharples, W. G. see Booth Silberstein, L. 68, 127, 129 Snell (Snellius van Roijen), W. S. 214 Stabenow, J. 132, 204, 205 Stange, K. 69 Stearns, E. I. 119, 129, 130, 247, 302 Stegun, I. see Abramowitz Steinbuch, K. 68 Stiles, W. 68 Stokes, G. G. 127, 129 Storr, B. V. see Channon

Name Index Strocka, D. 69, 129, 130 Stultz, K. F. 68 Sturm, B. see Hengstenberg Suzuki, S. see Okuda Sward, G. G. see Gardner T Thiemann, J.

219

V van de Hulst, H. C. 222, 223, 229, 230 van der Waals, J. D. 134 Vial, F. 206 Vælz, H. G. 13, 65, 66, 68, 129, 130, 177, 204±206, 230

W Wald, G. 68 Walraven, J. 68 Weber, E. H. see Fechner Westwell, A. see Booth Winkler, O. see Hengstenberg Winter, G. see Bçchel Woditsch, P. see Buxbaum Wright, W. D. 66, 68 Wyszecki, G. 68 Y Young, T.

23, 66, 68

Z Zollinger, H. see Booth Zorll, U. 205

373

View more...
Hans G. Vælz

Industrial Color Testing

Kinh Tang Nguyen Quoc Thiet

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

Hans G. Vælz

Industrial Color Testing Fundamentals and Techniques

Second, Completely Revised Edition

Translated by Ben Teague

Weinheim 7 New York 7 Chichester 7 Brisbane 7 Singapore 7Toronto

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

Dr. Hans G. Vælz Deswatines-Straûe 78 D-47800 Krefeld (formerly: Bayer AG, Krefeld-Uerdingen, Germany)

This book was carefully produced. Nevertheless, author, translator and publisher do not warrant the information contained therein to be free of errors. Readers are advised to keep in mind that statements, data, illustrations, procedural details or other items may inadvertently be inaccurate.

First Edition 1995 Second, Completely Revised Edition 2001

Library of Congress Card No.: Applied for. British Library Cataloguing-in-Publication Data: A catalogue record for this book is available from the British Library. Die Deutsche Bibliothek ± CIP-Cataloguing-in-Publication Data: A catalogue record for this publication is available from Die Deutsche Bibliothek.

WILEY-VCH Verlag GmbH, D-69469 Weinheim (Federal Republic of Germany), 2001 Printed on acid-free paper. All rights reserved (including those of translation into other languages). No part of this book may be reproduced in any form ± by photoprinting, microfilm, or any other means ± nor transmitted or translated into a machine language without written permission from the publishers. Registered names, trademarks, etc. used in this book, even when not specifically marked as such, are not to be considered unprotected by law. Composition: ProSatz Unger, D-69469 Weinheim Printing: Strauss Offsetdruck GmbH, D-69509 Mærlenbach Bookbinding: Wilhelm Osswald & Co., D-67433 Neustadt/Weinstraûe Printed in the Federal Republic of Germany

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

Preface to the Second Edition

The first English edition having sold out in just a few years, the publisher has decided to bring out a new one. In the meantime, changes in the field have necessitated many alterations in text and content, as well as the revision of some sections of the book. Chapter 2 contains a new Section 2.3.4 titled ªNew Systems: CIE94 and CMC.º The analysis of errors of measurement in Section 2.4.4 has been expanded. A greatly improved method for determining the change in tinting strength is now set forth in Section 4.7.3. In Section 6.1.2, a table has been added to the discussion of evaluation conditions. New methods for determining the tinting strength of inorganic and organic pigments are now discussed in Chapter 8, and the tables for the calculation of the depth of color have been updated. The example (Section 8.2.4) for the calculation of the change in tinting strength has been modified to take advantage of the new technique described in Chapter 4. Finally, the listing of standards at the end of the book has been expanded; the author expresses his gratitude to Dipl.-Chem. B. Reinmçller of DIN, Deutsches Institut fçr Normung, Berlin, and his colleagues for their exemplary work in updating the list. Mrs. K. Sora of Wiley-VCH has provided intelligent help in creating this new edition. The new text material has been translated into English by Mr. B. Teague. The contributions of both are gratefully acknowledged. Krefeld, March 2000

Hans G. Vælz

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

Preface to the English Edition

The English version of my book is appearing just four years after the successful German edition entitled Industrielle Farbprçfung. It is closely based on the German text. Revisions have been necessary in only a few passages to correct errors and update (and sometimes expand) the literature citations. Furthermore, equations that are essential for theoretical understanding and practical application have been enclosed in boxes for emphasis. New material in the colorimetric part includes the CIELAB 92 color-difference system (Section 2.3.3) and the RAL Design color-order system (Section 2.3.4). A greatly simplified and clearer description has been given for the proposition (important in the determination of tinting strength) that equality of the CIE tristimulus values Y in lightness matching implies equality of the Kubelka-Munk functions, that is, that DY = DFY = 0 (Section 4.6.4 and 4.7.1). In connection with tests of significance, it is shown how the error of preparation can be separated into specific error components (Section 6.3.3). To aid the understanding of confidence levels in relation to acceptability, an explanatory paragraph has been inserted in Section 6.5.3, and the same chapter has been expanded by the new Section 6.5.4, ªAcceptability and Test Errors.º The index of standards (Appendix 1) is completely new. Organized through keyword, it lists standards of the International Organization for Standardization (ISO), the European Committee for Standardization (CEN), and several national standards bodies: the American Society for Testing and Materials (ASTM), the British Standards Institution (BSI), the Association Franaise de Normalisation (AFNOR), the Japanese Industrial Standards (JIS), and the Deutsches Institut fçr Normung (DIN). An important role in the preparation of this table was again performed by Mr. E. Fritzsche of DIN, Berlin, to whom I would like to express my gratitude. I am also grateful to my colleague and successor, Dr. H. Heine, Krefeld, for his generous assistance, to Mr. Ben Teague for a sympathetic translation, and to Mrs. Karin Sora of VCH Publishers for her helpful collaboration. Krefeld, July 1994

Hans G. Vælz

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

Preface

This book is directed chiefly to all technical personnel who are involved with pigments and dyes, whether as manufacturers, converters, or consumers. It is often not enough to be familiar with the procedure used in a test; more must be known about the quantity being measured and the way in which it varies as a function of other parameters ± in brief, about its physicochemical habit, which is embedded in the well-known fields of chemistry and physics. This is especially important when test methods are to be rationalized; rationalization requires computers, and all computer use is based on applied mathematics. Effective rationalization is possible only when the mathematical and physical background of the quantities being measured is kept fully in view. The lack of suitable worked-out examples to illustrate test methods often creates difficulties in practice as well. This book should help close the gap by providing at least one practical example for each of the test methods described. The book should, however, also offer some utility to the scientist engaged in research and development work on pigments and dyes. Discussion of principles makes up a substantial part of the text, and many suggestions and hints are included to further the scientist's work. On the other hand, anyone working in research or development but lacking a knowledge of both the principles and the state of the art will scarcely be in a position to advance the colorimentric properties of these substances. A third audience ± so the author hopes ± will find the book beneficial: university lecturers and students in the natural sciences. The study of colorimetry in the testing of coloring material is a perfect example of the interdisciplinary effect of chemistry, physical chemistry, physics, theoretical physics, mathematics, and cybernetics (informatics). It goes without saying that one must understand the principles of each discipline before one can understand their interaction. There is, however, another point: The integrative components of the knowledge assembled in this book are hardly taught (if at all) in our universities and colleges of technology ± colorimetry and Kubelka-Munk theory being just two examples. Even beyond the field of coloring materials, both these bodies of knowledge have significant roles to play in many other technical areas, and it is hard to comprehend that people with university-level diplomas even today are entering the colorant manufacturing and converting industries without ever having come in contact with either topic. In choosing the contents of this book from the disciplines named, the author has adopted a standard that he considers trustworthy, one that has continually aided him

VIII

Preface

in distinguishing key topics from less important ones: He wanted to write the book he wishes had been available when he entered the field of pigment testing. Naturally, such a wish is a bit of a fantasy, for it is only now that this book could be written in its present form. Some three-quarters of the test methods described there did not even exist then. The same holds, in modified form, for the principles; while certain branches of knowledge had already been developed 30 years ago, they were not yet relevant for our field ± the statistical analysis of color coordinates is one of many topics that might be mentioned. Finally, the introduction of the computer in colorimetric testing has led to major changes in recent years. To avert misunderstandings, some special points relating to text selection should be stated in advance. The title of the book should be read as referring to the colorimetric examination of pigments and dyes in media; thus, all tests not carried out in mixtures with a lacquer, paint, plastic, or other coating are excluded (e. g., on textile fibers or in printing inks). The chapter on ªColorimetryº has been kept short even though it threatened to grow into another whole volume. In other words, this book does not wish to be mistaken for a textbook on colorimetry. The only aspects of that field that are covered are topics essential for the context of the book. Similarly, one will search in vain for instructions on color formulation and correction calculations. These operations do not come under the heading of pigment and dye testing, even if they must be preceded by testing. Similarly, the application of Mie theory in the determination of particle-size distributions is not covered, for it is based not on colorimetric methods but on general spectroscopic methods. In Chapter 2, on the other hand, a comparatively large proportion has been devoted to the statistical analysis of color coordinates. The reasons for this are that these applications are relatively novel in practice and that key topics such as acceptability (tolerances) are related to them. New in Chapter 3 are the fourflux equations for specular substrates, which may prove to be of interest in the future. Chapter 4 offers ± for the first time, as far as the author is aware ± a theoretical mathematical justification for the universal practice of treating wideband measurements (e. g., reflectometer values) or color coordinates (e. g., CIE tristimulus values) as spectral values in Kubelka-Munk analysis and of matching not the tristimulus values but their Kubelka-Munk functions. In Chapter 5, instructions are given for extending Mie calculations to the particle-size distribution of anisometric (i. e., bladed or rodshaped) pigments. While the text was in preparation, a number of colleagues expressed willingness to read it and offer vital suggestions and corrections. The entire text was read by Dr. H. Heine (Krefeld-Uerdingen), Dr. S. Keifer (Krefeld-Uerdingen), and A. van Leendert (Krefeld). The following experts made themselves available to read portions of the text: Dr. L. Gall (Ludwigshafen), Dr. W. Herbst (FrankfurtHæchst), Prof. G. Kåmpf (Leverkusen), Prof. J. Krochmann (Berlin), Dr. H. Pauli (Basel), Dr. K. Sommer (Krefeld-Uerdingen), Dr. J. Spille (Leverkusen), Dr. J. Thiemann (Leverkusen), Dr. J. Wiese (Krefeld-Uerdingen), and Dr. K. Witt (Berlin). Mrs. E. Lechner and Mr. E. Fritzsche of DIN, Berlin, have prepared the exemplary listing of the standards cited. The author would like to take this oppor-

Preface

IX

tunity to thank all these colleagues for their helpfulness and their valuable advice and suggestions. I am grateful to Bayer AG for its continuing interest and assistance in the writing of this book, and to VCH Publishers for its intelligent collaboration and valuable advice. Krefeld, November 1989

Hans G. Vælz

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

Contents

Part I Principles 1 Introduction 1.1 1.2 1.3 1.4

1 3

Coloring Materials 3 Color Properties 9 Summary 12 Historical and Bibliographical Notes

12

2 How Colors Depend on Spectra (Colorimetry)

15

2.1 Introduction 15 2.1.1 Concerns and Significance of Colorimetry 15 2.1.2 Reflection and Transmission 17 2.2 CIE Standard Colorimetric System 20 2.2.1 Spectral Distribution and Color Stimulus 20 2.2.2 Trichromatic Principle 21 2.2.3 CIE System 23 2.3 Sensation-Based Systems 26 2.3.1 Lightness, Hue, Saturation 26 2.3.2 Physiologically Equidistant Systems 27 2.3.3 CIELAB System 28 2.3.4 New Systems: CIE94 and CMC 36 2.3.5 Color Order Systems 39 2.4 Mathematical Statistics of Color Coordinates 42 2.4.1 Normal Distribution in Three Dimensions 42 2.4.2 Standard Deviation Ellipsoid 46 2.4.3 Standard Deviations 51 2.4.4 Color Measurement Errors and Significance 55 2.4.5 Acceptability 59 2.5 List of Symbols Used in Formulas 62 2.6 Summary 64 2.7 Historical and Bibliographical Notes 66

XII

Contents

3 How Spectra Depend on the Scattering and Absorption of Light (Phenomenological Theory) 71 3.1 Introduction 71 3.1.1 Phenomenological Theory and Its Significance 71 3.1.2 Many-Flux Theory 72 3.1.3 Surface Phenomena 75 3.2 Four-Flux Theory 78 3.2.1 The Differential Equations and Their Integration 78 3.2.2 Transmittance and Transmission Factor 83 3.2.3 Reflectance and Reflection Factor 86 3.2.4 Limiting Cases of Reflection 90 3.2.5 Determination of the Coefficients 93 3.3 Kubelka-Munk Theory 96 3.3.1 Significance and Formalism 96 3.3.2 Limiting Cases of Reflection 98 3.3.3 Determination of the Absorption and Scattering Coefficients 102 3.4 Hiding Power 104 3.4.1 General 104 3.4.2 Achromatic Coatings 105 3.4.3 Scattering and Absorption Components 108 3.5 Transparency 110 3.5.1 Description and Definition 110 3.5.2 Coloring Power 111 3.5.3 Achromatic Coatings 113 3.6 Principle of Spectral Evaluation 115 3.6.1 Description and Significance 115 3.6.2 Application to Hiding Power 116 3.6.3 Application to Transparency and Coloring Power 121 3.7 List of Symbols Used in Formulas 123 3.8 Summary 125 3.9 Historical and Bibliographical Notes 126 4 How Light Scattering and Absorption Depend on the Content of Coloring Material (Beer's Law, Scattering Interaction) 131 4.1 Introduction 131 4.1.1 Description and Significance of the Concentration Dependence 131 4.1.2 Pigment Particle Size 132 4.1.3 Dispersing of Pigments 133 4.1.4 Measures of Pigment Content 135

Contents

XIII

4.2 Absorption and Content of Coloring Material 138 4.2.1 Dyes 138 4.2.2 Pigments 139 4.3 Scattering and Pigment Content 141 4.3.1 Scattering Interaction 141 4.3.2 Experimental Test of an Empirical Formula 144 4.4 Systematic Treatment of Pigment/ Achromatic Paste Mixing 146 4.4.1 Standard Methods of Pigment/Paste Mixing 146 4.4.2 Importance of the Methods 148 4.5 Kubelka-Munk Functions of Pigment/ Paste Mixture 150 4.5.1 General Formula 150 4.5.2 Black Pigments Mixed with White Paste 151 4.5.3 White Pigments Mixed with Black Paste 156 4.5.4 Colored Pigments Mixed with White Paste 158 4.6 Tinting Strength 165 4.6.1 Significance and Definition 165 4.6.2 Coloristic Matching Criteria for Pigments 167 4.6.3 Color Matching Studies 172 4.6.4 Lightness Matching 178 4.6.5 Color Depth Matching 184 4.7 Special Problems 186 4.7.1 Lightening Power 186 4.7.2 Color Differences after Matching 188 4.7.3 Change in Tinting Strength 191 4.8 List of Symbols Used in Formulas 197 4.9 Summary 201 4.10 Historical and Bibliographical Notes 204 5 How Light Scattering and Absorption Depend on the Physics of the Pigment Particle (Corpuscular Theory) 207 5.1 Introduction 207 5.1.1 Description and Significance of the Corpuscular Theory 5.1.2 Particle-Size Distribution 208 5.1.3 The Optical Constants: Refractive Index and Absorption Index 213 5.2 Mie Theory 217 5.2.1 Integration of the Wave Equation 217 5.2.2 Absorption and Scattering of the Particle Ensemble 219 5.2.3 Scattering Behavior of Pigments 222 5.2.4 Absorption Behavior of Pigments 224

207

XIV

Contents

5.3 List of Symbols used in Formulas 226 5.4 Summary 227 5.5 Historical and Bibliographical Notes 229 Part II Test Methods

232

6 Measurement and Evaluation of Object Colors

233

6.1 Reflection and Transmission Measurement 233 6.1.1 Gloss Measurement and Assessment 233 6.1.2 Measurement and Evaluation Conditions 237 6.2 Practical Evaluation of Color Differences 243 6.2.1 Preparation of Specimens 243 6.2.2 Color Measuring 243 6.2.3 Full Shade 248 6.2.4 Special Problems 252 6.3 Test Errors 255 6.3.1 Calculation of the Standard Deviation Ellipsoid 255 6.3.2 Visualization of the Ellipsoid 257 6.3.3 Total Error and Its Components 259 6.4 Significance 263 6.4.1 Calculation of Standard Deviations 263 6.4.2 Test of Significance 265 6.5 Acceptability 268 6.5.1 Specimen Preparation 268 6.5.2 Matching and Color Measurement 270 6.5.3 Evaluation and Example 271 6.5.4 Acceptability and Test Errors 275 7 Determination of Hiding Power and Transparency

277

7.1 Measurement of Film Thickness 277 7.1.1 Selection of Method 277 7.1.2 Gravimetric,Wedge Cut, and Dial-Gauge/ Micrometer Methods 279 7.1.3 Pneumatic Method 281 7.2 Scattering and Absorption Coefficients 283 7.2.1 Kubelka-Munk Coefficients S and K of White Pigments 283 7.2.2 Kubelka-Munk Coefficients S and K of Black and Colored Pigments 288 7.2.3 Four-Flux Coefficients s+, s±, k' 293

Contents

7.3 Transparency 296 7.3.1 Single-Point and Multi-Point Methods 296 7.3.2 Method Based on Principle of Spectral Evaluation 7.4 Hiding Power 303 7.4.1 General (Graphical Method) 303 7.4.2 Achromatic Case 305 7.4.3 Based of Principle of Spectral Evaluation 310 7.4.4 Economic Aspects 318 8 Determination of Tinting Strength and Lightening Power

XV

298

323

8.1 Content of Coloring Material 323 8.1.1 Dyes 323 8.1.2 Pigments 324 8.2 Relative Tinting Strength 325 8.2.1 Dyes 325 8.2.2 Inorganic Black and Colored Pigments (Lightness Matching) 327 8.2.3 Organic Pigments (ªFIAFº Method Based on Principle of Spectral Evaluation) 332 8.2.4 Change in Tinting Strength 340 8.3 Lightening Power 345 8.3.1 Graphical Method 345 8.3.2 Rationalized Method 348 8.3.3 PVC Dependence from One Gray Mixture 351 Appendix: List of DIN, DIN ISO, and ISO Standards Cited Subject Index Name Index

363 371

357

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

Part I Principles

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

1

Introduction

1.1

Coloring Materials

This book deals with color-imparting substances and the color phenomena which they produce. The general term for all coloring substances is ªcoloring materialsº;* and includes, in particular, pigments and dyes. Pigments are substances consisting of particles that are practically insoluble in the application medium. They are used chiefly as coloring materials but can also be employed for other properties in special applications (e. g., anti-corrosion or magnetic pigments). The demarcation between pigments and fillers was formerly somewhat problematic as it cannot be stated in terms of a limiting refractive index. However they can be differentiated according to their application. In contrast to pigments, a filler is not employed to impart color but to impart certain technical properties to the coating or to increase the volume of the coating material. Such a convention does not rule out the possibility that certain substances can find use as both pigments and fillers. However, there is a large group of substances that act as pigments in the great majority of cases (e. g., TiO2 is never used as a filler). When we speak of pigments, we are referring to this group. This statement also applies to the present book. Pigments can be classified according to a variety of criteria; here we generally follow the standard scheme and speak of two classes: ± Inorganic pigments ± Organic pigments The next step in classification is according to their origin: ± Natural pigments ± Synthetic pigments Economically, synthetic pigments are very much more significant than natural pigments, and they will therefore be our exclusive focus in the following classification.

* For standards see ªColoring Materials, Termsº in Appendix 1.

4

1 Introduction

According to standards*, inorganic and organic pigments are broken down as follows: ± White pigments. Their optical effect depends on the nonselective scattering of light. Examples, inorganic: titanium dioxide pigments, zinc sulfide pigments, lithopone, lead white, zinc white; organic: white resin powders. ± Black pigments. The optical effect of black pigments is based on the nonselective absorption of light. Examples, inorganic: carbon black, black iron oxide; organic: aniline black. ± Colored pigments. Colored pigments act by selective absorption of light, often combined with selective scattering. Examples, inorganic: iron oxide pigments, cadmium pigments, ultramarine pigments, chrome yellow, molybdate red, nickel rutile yellow, cobalt blue; organic: azo pigments, quinacridone pigments, dioxazine pigments, perylene pigments, phthalocyanine pigments, lake colors based on azo dyes and triphenylmethane dyes. ± Luster pigments. These are metallic particles or particles with high refractive indices. They are predominantly planar in structure and orientation, which produces gloss effects (see below for further classification). ± Luminescent pigments. These pigments fluoresce or phosphoresce (see below for further classification). The last two groups require additional explanation. Luster (gloss) pigments include: ± Metal-effect pigments. These consist of lamellar metal particles (in contrast, powdered zinc and lead are referred to as anticorrosive ªmetallic pigmentsº and do not belong to this group). Examples, inorganic only: gold bronze, aluminum bronze. ± Nacreous pigments. These pigments consist of transparent lamellar particles, which produce a pearl-like (nacreous) gloss by multiple reflection when in a parallel orientation. Examples, inorganic: specially prepared basic lead carbonate, bismuth oxychloride, titanium dioxide precipitated on mica; organic: fish scale. ± Interference pigments. If the lamellae have the appropriate thickness, iridescence effects are produced by interference. Example, inorganic: iron oxide on mica. Luminescent pigments include the following types: ± Fluorescent pigments. Their optical effect is based on selective absorption of light with simultaneous luminescence. Excitation is achieved by high-energy radiation such as ultraviolet or short-wavelength visible light. * For standards see ªColoring Materials, Classificationº in Appendix 1.

1.1 Coloring Materials

5

Examples, inorganic: pigments for display tubes and fluorescent lamps, radioactive luminescent pigments; organic: 2-hydroxy-1-naphthaldazine. ± Phosphorescent pigments. The optical effect of phosphorescent pigments is based on selective absorption and scattering of light plus delayed luminescence. Excitation is achieved by high-energy radiation such as ultraviolet or short-wavelength visible light. Examples, inorganic only: zinc sulfide/alkaline-earth sulfides doped with heavy-metal ions. The chemical makeup of pigments will only be dealt with briefly to discuss the hues which are obtainable. Inorganic pigments, with a few exceptions, are oxides, sulfides, oxide hydroxides, silicates, sulfates, and carbonates. In general, they consist of individual particles which are uniform in chemical composition (e. g., iron oxide red is a-Fe2O3). Organic pigments, in principle, are also powders of uniform composition; the two major groups are azo pigments and polycyclic pigments. The colors associated with individual pigments are listed in four tables: ± ± ± ±

White and black pigments: Table 1-1 Inorganic colored pigments: Table 1-2 Organic colored pigments, azo pigments: Table 1-3 Organic colored pigments, polycyclic pigments: Table 1-4

Table 1-1. White and black pigments.

Inorganic pigments

Organic pigments

Chemical class

White pigments

Black pigments

Oxides

Titanium dioxide Zinc white

Black iron oxide Iron-manganese black Spinel black

Sulfides

Zinc sulfide Lithopone

Carbon and carbonates

White lead

Perylene pigments Others

Carbon black Perylene black

White resin powders

Aniline black Anthraquinone black

6

1 Introduction

Table 1-2. Inorganic colored pigments. Chemical class

Green

Blue-green

Blue

Violet

Oxides and hydrated oxides Iron oxide pigments

Chromium oxide pigments

Mixed phase oxides

Red

Orange, brown

Yellow

Yellowgreen

Red iron Brown iron Yellow iron oxide oxide oxide Mixed brown (spinel and corundum phases) Chromium oxide green

Hydrated chromium oxide green

Cobalt green

Cobalt blue

Nickel rutile yellow Chromium rutile yellow Cadmium sulfoselenide

Sulfides and sulfoselenides

Cadmium sulfide

Cadmium mercury sulfide Chromate pigments

Chrome green

Molybdate red

Ultramarine pigments

Ultramarine green, Ultramarine blue, Ultramarine violet Ultramarine red

Iron blue pigments

Iron blue

Others

Manganese blue

Cobalt and manganese violet

Chrome orange

Chrome yellow Zinc yellow Alkalineearth chromates

Cadmium zinc sulfide

1.1 Coloring Materials

7

Table 1-3. Organic colored pigments: azo pigments. Blue Monoazo pigments

Disazo pigments

Others

Violet

Red

Orange, brown

Yellow

Monoazo orange pigments (also as lakes*)

Monoazo yellow pigments (also as lakes**)

Yellow- Green green

Diaryl yellow pigments Disazopyrazolone pigments

b-Naphthol pigments (also as lakes*)

Bisacetoacetic acid arylide pigments Metal complex pigments**

Naphthol AS pigments (also as lakes*) Naphthalenesulfonic acid pigments in lake form Benzimidazolone pigments Disazo condensation pigments Isoindoline pigments Isoindolinone pigments * Pigments in lake form are Me salts between sulfonic acid and/or carboxylic acid groups of dyes and metal salts (Me = alkaline earth, Na, Mn). ** Me complexes with azo or azomethine groups (Me = Ni, Co, Fe, Cu, Zn).

8

1 Introduction

Table 1-4. Organic colored pigments: polycyclic pigments. Yellow- Green Bluegreen green Aromatic and heterocyclic pigments

Blue

Violet

Phthalocyanine pigments

Red

Orange, brown

Yellow

Quinacridone pigments Perylene pigments Perinone pigments Thioindigo pigments

Anthraquinone pigments

Flavanthrone yellow pigments

Triarylcarbonium pigments

Pyranthrone pigments Dioxazine Anthpigments anthrone pigments

Anthrapyrimidine pigments Quinophthalone pigments

Dyes are coloring materials which are soluble in the application medium. Dyes used to be exclusively natural products, but these are of virtually no commercial importance today. It is not difficult to classify all dyes in a similar way to pigments. However, the main area of application for dyes is in textile coloring as although their ease of dispersion makes them advantageous for use in coatings and plastics, dyes are often less lightfast than pigments in these media. Special types are, however, significant in the plastics industry. We do not need to classify dyes as in Tables 1-3 and 1-4 because it would look the same. Along with the classifications already mentioned, other ways of breaking down the classes of pigments and dyes are possible. For example, they might be listed by application. The industrial synthesis of coloring materials is now subject to rigorous monitoring by qualitative and quantitative chemical analysis performed in plant laboratories, quality control laboratories and special research laboratories. The chemical analysis of raw materials, intermediates, end products, by-products, and waste products serves not only to meet quality requirements, but also to satisfy environmental protection standards. Final inspection, which also considers physical properties and application qualities, takes place in properly equipped testing laboratories; this process can no longer even be thought of without the aid of computers. The principles and methods of testing, as specifically applicable to coloristic pigment and dye properties, are the subject of this book.

1.2 Color Properties

9

The creation of international standards by the ISO (International Organization for Standardization) and of national standards by AFNOR, ASTM, BSI, DIN, JIS*, and other bodies has not only made it possible to state unambiguously what requirements pigments have to meet, but has also led to greater progress towards universally accepted test methods (see Appendix 1).

1.2

Color Properties

All color phenomena that we can observe in coatings have their origin in the interaction between the coating material and visible light, i. e., the electromagnetic radiation in the wavelength range of 400 to 700 nm. Special importance is attached to the fact that such coatings need not be homogeneous but can exhibit typical inhomogeneities due to the presence of discrete pigment particles. The physical processes that result from this interaction can be broken down into a few elementary processes. When a photon enters into a dyed or pigmented coating, three processes can determine its subsequent fate (Fig. 1-1): ± The photon collides with a dye molecule or a pigment particle and is absorbed. ± The photon collides with a pigment particle and is scattered. ± The photon passes through the coating without collision (assuming that the surrounding medium does not absorb) and is scattered and/or absorbed by the substrate. The fundamental physical and optical properties of coloring materials are thus their absorbing and scattering powers. Inhomogeneity of the coating is not a necessary condition for absorption; even homogeneous coatings can absorb if they contain light-absorbing substances, such as dissolved dyes. The case is different for light scattering, which can occur only in a coating that has the following properties: ± The coating is heterogeneous in composition.** ± Its individual components differ in refractive index.

* AFNOR = Association Franaise de Normalisation ASTM = American Society for Testing and Materials BSI = British Standards Institution DIN = Deutsches Institut fçr Normung JIS = Japanese Industry Standard ** Light scattering on molecules can be ignored here because it is orders of magnitude less than scattering on multimolecular pigment particles.

10

1 Introduction

Fig. 1-1.Absorption and scattering of light in a coating with colored pigment particles. a: Directionally incident white light b: Gray substrate c: Directly reflected light d: Diffusely reflected light

In a somewhat simplified scheme, forward and backward scattering are distinguished by whether the light is scattered in the direction of incidence (into the front half-space) or in the opposite direction (into the back half-space). White pigments have very little absorbing power in comparison to their scattering power. Black pigments, on the other hand, have very little scattering power relative to their absorbing power. Colored pigments, as a rule, feature selectivity in both absorbing and scattering power, i. e., they show wavelength-dependent behavior. This explains how the two elementary processes of absorption and scattering give rise to what we can measure: the reflection spectrum, the spectral reflectance R (l) between wavelengths 400 and 700 nm.* Pigmented coatings, and thus indirectly pigments themselves, can be unambiguously characterized by their reflection spectra. But the human eye cannot see reflection spectra; it merely communicates color stimuli to the brain. The missing link in the chain is the conversion of reflection spectra to color stimuli; this is accomplished by colorimetry. Modern testing of coloring materials is able to establish an almost perfect connection between the color stimulus (and hence the optical properties of the pigments) and fundamental physical quantities. The point of making such a connection is to be able to operate under well-known rules of physics. The schematic diagram shown in Figure 1-2 will aid in unterstanding these relationships. Key physical quantities are listed at the bottom left, while application properties of importance in practice are shown at the top left of the diagram. Particularly important are the boxed entries in between, which represent theoretical ideas that link the technical properties with the physical ones. The following relationships exist: ± Colorimetry relates the perceived color quality to the color stimulus F and this, in turn, to the reflection spectrum R (l). ± Kubelka-Munk theory relates R (l) to the scattering coefficient S (l), absorption coefficient K (l), and coating thickness h. * The symbols employed in each subsequent chapter are listed at the end of that chapter. See also ªSymbols for use in formulasº in Appendix 1.

1.2 Color Properties

11

Fig. 1-2. Schematic diagram showing relationships between color properties and theoretical fundamentals.

± Multiple scattering theory relates S to the scattering cross section QS (D, l) of the individual particle and the pigment concentration s. (The absorption coefficient K is directly proportional to the absorption cross section QA (D, l) and s.) ± Mie theory, finally, relates QS (D, l) and QA (D, l) to the particle size D, the wavelength l, the refractive index n, and the absorption index k; the last two optical properties are constants of the material. In practice, either downward or upward motion is possible. For instance, to determine the hiding power it is first necessary to obtain the Kubelka-Munk coefficients by color measurements (moving downward) so that the expected color stimulus of the hiding layer can then be calculated (moving upward). A separate chapter in this book is devoted to each of the four theoretical complexes listed above. The ideas behind modern test methods are rather difficult, since they are based on the light source/sample/eye/brain configuration and the methods must reproduce it. The need to simulate this very complicated system leads to the insight that further progress is possible only if new problems with an even greater degree of difficulty can be handled. ªSimpleº test methods such as appear in the specialist literature from time to time cannot be expected to solve these problems. The only promising approach is to enhance our knowledge and understanding of the cybernetic and physico-chemical principles involved in the perception of optical stimuli by the eye and associated organs. The objection sometimes heard, that new and complicated methods entail excessive calculation effort, long ago lost its justification when powerful and economical computers became available, which meant that calculations could be done in quite a short time. This is one of the key conditions that have led to advances in this field, i. e., the remarkably fast development in computer technology. Only by virtue of this development have present-day colorimetric and testing laboratories been able to formulate such complex testing programs in a objective fashion and to perform tests such as those described in this book in a prompt and efficient manner.

12

1 Introduction

1.3

Summary

The terms ªcoloring materialsº, ªpigmentº, and ªdyeº are defined and explained in this chapter. The usual classification of pigments is according to chemical nature (inorganic, organic) and genesis (natural, synthetic). The subclasses of white, black, colored, luster, and luminescent pigments are also characterized. Inorganic pigments consist of oxides, oxide hydroxides, silicates, sulfates, sulfides, and carbonates; organic pigments are divided into two major groups, the azo pigments and polycyclic pigments. Dyes can be classified under criteria similar to those of organic pigments. The industrial synthesis of pigments and dyes today is subject to monitoring by analytical and physical-chemical methods, which would be inconceivable without the aid of computers. The existing international and national standards are of great importance for both specifications and test methods. This book is concerned with colorimetric methods used for testing coloring materials in media. The starting point is therefore the interaction of light with a coating. Typical phenomena are described: the light can be scattered and/or absorbed. While absorption of light is apparent in the case of dyes and pigments, scattering is expected only when pigments are present. White pigments are characterized by a high scattering power with very little absorption; black pigments by a high absorbing power. Colored pigments feature selective absorption, and frequently selective scattering as well. For pigment and dye testing, the color can be related to fundamental physical quantities from color stimulus to the spectrum, to scattering and absorption, to refractive and absorption indices, and to wavelength and particle size. These relationships are used in an appropriate sequence when establishing test methods. The current state of the art in color test is chiefly due to advances in computer technology, which have offered ways to perform many testing jobs in an economical way.

1.4

Historical and Bibliographical Notes

It can be presumed that the use of coloring materials for coloring by human beings goes back to the origins of cultural history. The oldest artifacts that have come down to us are the well-known cave paintings, made with natural inorganic pigments. It must not be overlooked that the materials and the fundamental knowledge available at that time were limited even though artistic expressiveness and craft knowledge were already highly advanced. It was a long historical path [1], [2], [3] that led to the present high level of scientific and technological development in the areas of inorganic pigments [4], [5], [6], organic pigments [2], and dyes [3]. An important factor in this progress was the elucidation of the principles underlying the optical and colorimetric properties of dyes and pigments, together with the result-

1.4 Historical and Bibliographical Notes

13

ing advances in objective testing and evaluation methods. The methods in use today are the subject of this book. Stages of development that have occurred mainly in recent decades can be researched in survey articles [1], [7], [8]. The development of standardization in parallel with testing techniques is covered in [9]. Standards for the specifications of inorganic pigments see [5]. Each chapter in Part I of this book contains a section of historical and bibliographical notes together with a list of references.

References [1] H. Heine, H. G. Vælz, Pigments, Inorganic, Introduction, in Ullmann's Encyclopedia of Industrial Chemistry, 5. edit.,VCH Weinheim 1992,Vol. A 20, 245. [2] W. Herbst, K. Hunger, Industrial Organic Pigments,VCH Weinheim 1993. [3] G. Booth, H. Zollinger, K. McLaren, W. G. Sharples, A. Westwell, Dyes, General Survey, in Ullmann's Encyclopedia of Industrial Chemistry, 5. edit.,VCH Weinheim 1987,Vol. A 9, 73. [4] G. Buxbaum (Ed.), Industrial Inorganic Pigments,VCH Weinheim 1993. [5] G. Buxbaum, H. Heine, P. Kæhler, P. Panek, P. Woditsch, Anorganische Pigmente, in Winnacker/ Kçchler, Chemische Technologie 4. edit., Vol. 3, Anorganische Technologie II, Hanser, Mçnchen 1983, 349. [6] W. Bçchner, R. Schliebs, G. Winter, K. H. Bçchel, Industrial Inorganic Chemistry, VCH Weinheim 1988. [7] H. G. Vælz, Progr. Org. Coat 1 (1973). [8] H. G. Vælz, Angew. Chem. Internat. edit. 14 (1975) 655. [9] E. Fritzsche, farbe + lack, 80 (1974) 731.

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

2

How Colors Depend on Spectra (Colorimetry)

2.1

Introduction

2.1.1 Concerns and Significance of Colorimetry Colorimetry, the techniques based on it, and the colorimetric way of thinking have become the norm in all fields of technology that deal with colors in any way. The special uses of colorimetry can be summed up under the following headings: ± Color identification codes. Color names are verbal descriptions; they offer little help in the unique identification or labeling of colors. Scientists, however, are accustomed to describing a phenomenon objectively in terms of a measuring unit and number. ± Systematic description of color phenomena. Colorimetric concepts make it possible to construct logical and meaningful color systems based on easily understood principles. ± Evaluation of color differences. The quantification of color differences is one of the principal tasks of colorimetry. It is vital, for example, in production control of coloring materials, varnishes, paints, etc. ± Color rendering. Color rendering involves the evaluation of color differences between the object and the reproduction, as in color television or color photography. ± Colorimetric color formulation. Colorimetry makes it possible to fulfil an ancient wish, to calculate in advance the components and the proportions needed to obtain a desired color. The color properties of coatings, which are the subject of this book, involve all of these points to a greater or lesser degree. We will return to the meaning of color difference in this context. The testing of coloring materials involves measuring them between a given specimen (ªreference sampleº) and a specimen to be evaluated (ªtest sampleº). The objective determination of color differences is essential for the following areas: ± Development of new products. Key factors in technical progress are the continuous improvement of products which are already being produced and the creation of new coloring materials. Indispensable to both, however, is a fundamental

16

2 How Colors Depend on Spectra (Colorimetry)

knowledge of colorimetric relationships and the testing and inspection methods derived from them. Analysis of optical performance can no longer be done without colorimetric testing methods based on exact scientific principles. ± Production control. Human beings use their visual apparatus, consisting of eye, nervous system, and brain, to match and assess coloring substances. This represents an information-processing system in the cybernetic sense, with the special feature that the output of this system gives rise to both physiological and physiological effects. It follows that assessment is generally not free of human prejudices, and so there is a pressing need for objective measurement techniques. ± Understanding between manufacturer and purchaser. Objective measurements are crucial so that the parties to a transaction understand each other clearly, and especially so in an area as emotionally charged as color. Thus it is easier to agree on acceptable deviations from rated values by referring to unimpeachable measuring methods than it would be to agree on how great a color difference can ªjust be seenº. When we raise the question of color deviations and measurement errors, we are in the domain of statistical analysis of color measurements. Such analysis is important for the following: ± Significance. The questioner wishes to know how precisely colors are being measured, that is, whether there is a significant difference between the measured color values for the two specimens being compared. A color comparison demands a knowledge of the significance level, which has to be tested in each case. Only when the significance level is known can one decide whether it is low enough for color comparisons to be made in a specific situation. This knowledge is needed even when color values for the same collection of samples, as measured with different types of instruments, are to be compared. What is called for in this situation is not a measure of the quality of color measurement, but a measure of the quality of the colorimeter. Given a suitable set of color samples covering the entire color space, it should be possible to compare the precisions of the colorimeters. ± Acceptability. This term refers to the limits within which measured color values must lie in order for the purchaser to classify them as ªconforming to a standard.º Acceptability must not be confused with the perceptibility of color differences, which is a threshold forming the upper limit of the region in which colors cannot be distinguished. Acceptability, in contrast, is based on a convention and on the experience of colorists. It has to do with the region within which specimens are assessed to ªconformº, that is, conform to a specified type or reference specimen. This means that some perceptible color differences may well still be acceptable. Both the criteria of significance and acceptability are built up on the same mathematical principles and require the same mathematical apparatus, namely the extension of the Gaussian normal distribution from one to three dimensions. Because

2.1 Introduction

17

these applications of well-known mathematical principles are fairly new and unusual in everyday colorimetric practice, a section is devoted to them alone. Colorimetry is discussed only as much as is necessary and sufficient in light of the theme and context of this book. Monographs and other literature on colorimetry are listed in Section 2.7.

2.1.2 Reflection and Transmission The reflection spectrum mentioned in Section 1.1 is the spectral distribution typical of object colors, and it forms the starting point for any measurement of them. It seems necessary to look more closely at the widely-used terms ªreflectanceº and ªreflection factorº. First, what are ªobject colorsº ? The standards* give the following answer: They are ªnon-luminous perceived colorsº i. e. colors of ªnon-self-radiatingº media that require illumination for their visibility. Color perception thus only takes place with light which illuminates the non-self-radiating medium. Certain standard sources have been defined as illuminants for colorimetry*; those of interest here are ± Standard Illuminant A for incandescent light ± Standard Illuminant C for artificial daylight ± Standard Illuminant D65 for natural daylight at a color temperature of 6504 K Reflection and transmission are purely physical phenomena; the related measurable quantities describe properties of how materials interact with radiation. These quantities are defined in the standards**. Of the many factors that influence them, the ones of interest here are those directly related to radiation: the direction of incidence, the direction of observation, and the aperture angles of the incident and observed beams (Fig. 2-1). Three configurations of the observed radiation are consistent with good technical realization: ± Directional (the beam consists of quasi-parallel rays) ± Conical (the beam has the shape of a narrow cone) ± Hemispherical (the beam is uniformly distributed over the half-space) In reflection measurements, the name of the result depends on the following measuring conditions: ± Reflectance R (hemispherical observation) ± Reflection factor R (conical observation) ± Radiance factor b (directional observation) If the illumination condition is included in the classification, nine geometries must be listed since there are three possibilities for illumination and three for viewing * For standards see ªColorimetryº in Appendix 1. ** For standards see ªPhotometric Properties of Materialsº in Appendix 1.

18

2 How Colors Depend on Spectra (Colorimetry)

Fig. 2-1. Nomenclature of the parameters. e1, e2, angles of incidence and reflection; j, azimuth angle.

(each can be parallel or rather quasi-parallel, conical, or hemispherical). Each of the illumination configurations is represented by a subscript on the symbol R, R, or b (Table 2-1): dif, diffuse (hemispherical case); g, directional; c, conical. Of the nine combinations, however, only three are common in colorimetry and realized in colorimeters. In the list below, the illumination geometry comes first and is followed by the observation geometry: ± Conical/hemispherical ± Hemispherical/conical ± Conical/conical

Reflectance Rc Reflectance factor Rdif Reflection factor Rc

Table 2-1. The nine types of reflectance measurement (after DIN 5036-3). Geometry

Quantity

Symbol

Illumination

Viewing

hemispherical hemispherical hemispherical

hemispherical conical directional

reflectance reflection factor radiance factor

Rdif Rdif bdif

conical conical conical

hemispherical conical directional

reflectance reflection factor radiance factor

Rc Rc bc

directional directional directional

hemispherical conical directional

reflectance reflection factor radiance factor

Rg Rg bg

The preferred measuring conditions are as follows (Fig. 2-2): ± For Rc, 08/diffuse and 88/diffuse (abbreviated 0/d and 8/d respectively) ± For Rdif , diffuse/08 and diffuse/88 (d/0 and d/8) ± For Rc, 458/08 and 08/458 (45/0 and 0/45) All measurements of surface colors in reflected light are referred to the ideal matte white surface, which reflects the incident radiation with a reflectance R = 1 inde-

2.1 Introduction

19

Fig. 2-2. Measuring conditions for colorimetry.

pendent of the angle. Because this perfect white standard is not technically realizable, a real reflection standard (secondary standard) must be adopted for colorimetry. The standard features a set of fixed values and deviates as little as possible from the ideal. It consists of a circular tablet pressed from pulverized barium sulfate*. The rated values for tested commercial barium sulfate powder are specified in Germany by the Physikalisch-Technische Bundesanstalt PTB (Federal PhysicalTechnical Institute); a tablet pressed from such powder can be employed for instrument calibration, either directly or by means of a working standard. A special point to note is that the surface of the specimen whose surface color is to be determined may exhibit peculiar reflectance behavior typical of the surface itself. If this point is not considered, measured color values may be falsified (see Section 6.1.2 for further detail). Object colors can also be evaluated in transmitted light, as in the case of plastic films, dye solutions, and the like. The property sought in such cases is the transmission. There are again three configurations for measuring the transmission** of object colors, and the terminology is analogous to that used in reflection measurement (with the following preferred measuring conditions): ± Transmittance tc, 0/d ± Transmission factor Tdif, d/0 ± Transmission factor Tc, 0/e2 (e2 is an arbitrary observation angle) If both incidence and observation angles are 08 (geometry 0/0), the transmission factor is symbolized by Tr .

* For standards see ªColorimetryº in Appendix 1. ** For standards see ªTransmission of optical radiationº in Appendix 1.

20

2 How Colors Depend on Spectra (Colorimetry)

2.2

CIE Standard Colorimetric System

2.2.1 Spectral Distribution and Color Stimulus In the context of physiological processes of color vision, colors are sensory impressions. If the psychological reactions associated with color vision are also considered, they are experiences. For this reason, it first appears contradictory to apply the term ªmetricº, meaning measurement, to colors. It will be shown that the discussion is actually about a metrical arrangement of equality judgments, in which the human eye functions solely as a null indicator. The starting point for the development is the well-known fact that any color stimulus can be prepared from the spectral colors by mixing. Thus a spectral distribution j (l) can be measured with a spectrograph. The product j (l) dl is the intensity corresponding to the narrow wavelength interval between l and l + dl in the spectrum. If we use the term ªcolor stimulusº and the symbol F for the color sensation registered by the eye, then there must be a correlation between the spectral distribution j (l) and F. Determining how these quantities are related involves knowing not only the purely physical circumstances but also the laws describing the physiology of colors, which can be summarized roughly as follows: If three suitable spectral distributions are selected, other color stimuli can be perfectly reproduced through additive mixing of these three ªreference stimuliº (also called ªprimariesº). The desired result is always achieved with a unique mixing ratio. It must be added that these mixtures are always prepared by the mixing of lights (ªadditiveº color mixing), as distinct from the use of successive optical filters each having its own transmission behavior (ªsubtractiveº color mixing). The physiological behavior just described is a summary of the rules called ªGrassmann's lawsº. If the addition of color stimuli is now defined as their mixing, the multiplication of a color stimulus by a number is also defined. For example, multiplication by the factor 2 corresponds to the addition of two identical color stimuli, etc. Now Grassmann's laws can be written out as follows: F = X7X + Y7Y + Z7Z or F = m (x 7 X + y 7 Y + z 7 Z)

(2.1)

where m = X + Y + Z, x = X/m, y = Y/m, and z = Z/m. Here X, Y and Z are called ªtristimulus valuesº; x, y, and z are called ªchromaticity coordinatesº; m is a physical measure of intensity; and X, Y, and Z are the reference stimuli. From the above definition of addition, it also follows that changing from reference stimuli X, Y, Z to different reference stimuli X',Y', Z' involves a linear (ªaffineº) transformation.

21

2.2 CIE Standard Colorimetric System

2.2.2 Trichromatic Principle The task of colorimetry is now to determine m, x, and y; the determination of z is redundant, since x + y + z = 1. The chromaticity coordinates form a 3-manifold, and this fact suggests analogy with the three dimensions of solid geometry. Indeed, in view of the addition rule, X,Y, and Z can be thought of as three-dimensional vectors forming a trihedral in which the color stimulus is a vector F = {X, Y, Z}. The above equations also show that the wavelength dependence of F is wholly contained in X,Y, Z (or x, y, z), since the reference stimuli are fixed color stimuli. The spectral colors therefore constitute a one-dimensional manifold and lie on a three-dimensional curve (ªspectral locusº) whose points can be labeled with the associated wavelengths l. Any color stimulus F = {X,Y, Z}, by virtue of the intensity distribution j (l), can be reproduced from the spectral colors by mixing, hence the sums taken over the spectral loci must give the tristimulus values exactly. This result can now be briefly derived: A color equation as in eq. (2.1) can be written for the spectral color having the wavelength 400 nm: F400 = x400 7 X + y400 7 Y + z400 7 Z where xl , yl , zl are the tristimulus values of the spectral colors. Now it must be remembered that this spectral color, in the color stimulus F being analyzed, is represented solely by the contribution j400 given by the distribution function j (l). The contributions of the spectral colors at 10 nm intervals are then j400 7 F400 j400 x400 7 X j400 y400 7 Y + j400 z400 7 Z + j410 7 F410 j410 x410 7 X j410 y410 7 Y + j410 z410 7 Z .. . + j700 7 F700 j700 x700 7 X j700 y700 7 Y + j700 z700 7 Z F

7P 00 l400

jl Fl

7P 00 l400

jl xl X

700 P l400

7P 00

jl yl Y

X7X

l400

Y7Y

jl zl Z (sum) Z7Z

Taking the sum of the components gives the initial color stimulus; comparison of coefficients then yields the tristimulus values of the color stimulus: X

700 P l400

jl xl ;

Y

700 P l400

jl yl ;

Z

700 P l400

jl zl

(2.2)

22

2 How Colors Depend on Spectra (Colorimetry)

If the intervals are sufficiently small, the sums go over to integrals, so that

X Y Z

700 R 400 700 R 400 700 R 400

j l x l dl j l y l dl j l z l dl

(2.3)

These formulae give the sought relation between F and j (l). For object colors, j (l) is the spectral distribution of the reflectance R (l) or of the reflection factor R (l) as measured under illumination with white* (ªequal-energyº) light (see Fig. 2-3 for examples). If light with a different spectral distribution S (l) is used for illumination, the reflected light will have a distribution R (l) 7 S (l), and j (l) in the integrals above must be replaced by this product. The ªcolor matching functionsº x (l), y (l), z (l) can be determined experimentally by the following procedure: On a trichromatic matching colorimeter, observers reproduce the individual spectral colors, each with an intensity of m = 1, from the primaries X, Y, Z by mixing. The relative mixing proportions are then determined for every l.

Fig. 2-3. Reflection spectra of some pigments in lacquer binders. * Or of the transmittance t (l) or the transmission factor T (l), in the case of light passing through a medium.

2.2 CIE Standard Colorimetric System

23

It should not be forgotten that this Young-Helmholtz theory of trichromatic color matching has been brilliantly confirmed by physiological research. Three and only three different visual receptors with photosensitive pigments are found in the human eye, their chemical constitutions have been determined (rhodopsins), and their spectral sensitivities have been measured. For color vision there are three types of receptors (cones), each of which contains one and only one such visual pigment. Thus a color stimulus can be defined by three tristimulus values, which are of the nature of integrals. Two color stimuli are then alike if the respective values of their integrals are equal. But the integrals change if either of the factors R (l) or S (l) is replaced by a different function. In general, this occurs if the same sample is illuminated with a different type of light: The two colored surfaces are then no longer alike but have a different appearance. If two colors appear alike only under certain conditions (e. g., under a certain type of illumination), they are, logically, said to be ªlooking alikeº or, in Ostwald's term, ªmetamericº; the phenomenon is called ªmetamerismº.

2.2.3 CIE System The colorimetric system currently in use all over the world is suggested and introduced by the CIE (Commission Internationale de l'Eclairage, International Commission on Illumination). The system includes fixed definitions of the reference stimuli X,Y, Z and the color matching functions x (l), y (l), z (l). In order that all actual colors can be described, color stimuli lying outside of the spectral locus were introduced (ªvirtual stimuliº); these three primary stimuli are obtained from three spectral colors by an affine transformation. The CIE principles are reflected in ISO Standard 7724*. The quantities X, Y, Z are called ªCIE tristimulus valuesº; x, y, z, ªCIE chromaticity coordinatesº; and x (l), y (l), z (l), ªCIE color matching functionsº. There are two sets of color matching functions, for 28 and 108 fields of view, which have been found experimentally to differ somewhat (Fig. 2-4). The CIE tristimulus values** are calculated with equations (2.3): R X = x (l) R (l) dl R Y = y (l) R (l) dl R Z = z (l) R (l) dl If light other than pure white light is used for illumination, R (l) must be replaced by the product R (l) 7 S (l), as shown previously. A number of ªCIE standard illu* For further standards see ªColorimetryº and ªColoring materialsº in Appendix 1. ** Because no limits of integration other than 400 and 700 nm are used, these are omitted from here on.

24

2 How Colors Depend on Spectra (Colorimetry)

Fig. 2-4. CIE color matching functions for 28 and 108 fields of view. (The circles at top right, viewed from a distance of ca. 8±9 cm, show the size ratio of the two fields of view.)

minantsº S (l) have been defined (see Section 2.1.2 and standards*). Table 2-2 presents some values. From the tristimulus values, the CIE chromaticity coordinates are calculated as x

X Y ; y X Y Z X Y Z

(2.4)

These are treated as coordinates in the color plane and define the CIE chromaticity diagram. Table 2-2. CIE tristimulus values and CIE chromaticity coordinates of some illuminants. (Yn = 100.00 for all standard illuminants and observers.) CIE illuminant A C D 65

Xn

28-standard observer Zn xn

109.85 98.07 95.05

35.58 118.22 108.90

0.4476 0.3001 0.3127

108-standard observer Zn xn

yn

Xn

0.4074 0.3162 0.3290

111.14 97.28 94.81

35.20 116.14 107.34

0.4512 0.3104 0.3138

yn 0.4059 0.3191 0.3310

The system exhibits the following properties (see Fig. 2-5): ± In the x, y chromaticity diagram, the additive mixture of two color stimuli lies on the straight line connecting the components, at a position determined by the center of gravity principle. * For standards see ªColorimetryº in Appendix 1.

2.2 CIE Standard Colorimetric System

25

± The shoe-sole-shaped locus of spectrum colors (ªspectral locusº) in the x, y plane is cut off below by the purple line. Colors lying on this line do not occur in the spectrum but are obtained as mixtures of red and violet. ± In the case of equal-energy illumination*, the ªequi-energy stimulusº or white locus lies at xw = yw = zw = 1/3. ± The CIE color matching function y (l) coincides with the spectral luminosity curve V (l) of the human eye. In place of m, the luminance Y = m 7 y is cited as a third color coordinate (along with x and y).

Fig. 2-5. CIE chromaticity diagram.

* Otherwise, the equi-energy stimulus is the color locus of the illuminant (standard illuminant); see Table 2-1.

26

2 How Colors Depend on Spectra (Colorimetry)

Another interesting fact of physiology should also be mentioned here. From the discussion it follows that there may be a very great number of spectral distributions R (l) that belong to one and the same color stimulus F (metameric colors). Because the human eye can distinguish of the order of 100 spectral colors and a roughly similar number of brightness levels, it should be possible to prepare the respectable number of 100100 distinguishable spectral distributions by mixing. In practice, however, by virtue of the trichromatic principle, the eye can only distinguish 1003 colors. The eye and the organs responding to it in the perceptual system thus perform a tremendous reduction in the quantity of information offered. In cybernetic terms, the huge amount of information contained in a single color stimulus (600± 700 bits), which would be nearly impossible to process in a reasonably short time, is reduced in a consistent way to some 20 bits, a quantity of information that the consciousness is well able to process in one second, as we know from a comparison with other sensory organs.

2.3

Sensation-Based Systems

2.3.1 Lightness, Hue, Saturation The CIE system offers a worldwide understanding of colors. Using the three numerical values x, y, and Y (and some few additional pieces of information*), the recipient of a communication can localize the color locus under consideration without having seen the color. Since this system came into existence, it has proved suitable for many different technical applications of color, including color television. In order to assess colored systems and pigments, however, there are additional demands. The two most important shortcomings are that it is hard to visualize information in the CIE system and that it is not suitable for direct determination of physiologically equidistant color differences. A few explanatory words follow: ± Difficulty of visualization: The values of x, y, and Y make it possible to put colors in a systematic order. It is hard, however, to visualize the nature of a color with only the coordinate values. As a way of coping with this problem, colors are classified and ordered according to another three properties so that one may come to an understanding with other parties. These are brightness (one can rank colors as ªbrighterº and ªdarkerº), hue (corresponding, in a way yet to be defined, to the spectral colors), and saturation (every color is regarded as a mixture of the ªsaturatedº hue and white; the color is more saturated the smaller the content of white). * For example, information on the geometry of the colorimeter, the standard illuminant used, and exclusion of surface reflection (all of which can be established once and for all).

2.3 Sensation-Based Systems

27

± Physiologically equidistant color differences: The introduction of the concepts of brightness, hue, and saturation has made it easier to visualize information in the system. The second difficulty, that of determining color differences, still remains. A glance at Figure 2-5 shows that the CIE chromaticity diagram cannot represent physiologically equidistant differences: The greens (from blue-green to yellow-green) occupy more than half the area enclosed by the spectral locus, while all other colors must make do with what remains. The determination of color differences is so important in practice that it must be deemed one of the principal tasks of colorimetry. One can also understand directly that the CIE diagram cannot correctly reproduce all color differences at once. The chromaticity diagram is based on the equality of color stimuli, since the mixing experiment (Section 2.2.2), in which the color matching functions are determined from the primary stimuli on the trichromatic matching colorimeter, involves using the eye solely as a kind of ªnull indicatorº for the equality of the reference and matched colors. The chromaticity diagram represents only a suitable (but arbitrary) metrical arrangement of equality judgments. In color difference measurements, however, the distinction between two color stimuli is of importance. Distinctions can be determined only through new color matching tests performed in a different way. The next section will go into more detail on this point.

2.3.2 Physiologically Equidistant Systems To determine color differences objectively, one needs to start with a notion that plays an idealized role in the physiology of colors. This is the concept of ªabsolute color spaceº, which can be thought of as a three-dimensional arrangement of color stimuli such that the distance between two color stimuli in an arbitrary spatial direction corresponds to the perceived difference. A color space with these properties cannot, however, be derived on a purely theoretical basis; its structure must be determined experimentally through color matching tests on samples having small color differences. As discussed in the previous section, such a space can be constructed with the color qualities of brightness, hue, and saturation. A configuration like that shown in Figure 2-6 results. The material needed for this purpose comprise a large number of color samples arranged by steps of hue, saturation, and finally brightness, and having physiologically equidistant differences. The derived solid is an onion-shaped body with an irregular boundary (for example, more hues can be distinguished in the dark blue than in the light red). The vertical axis is the gray scale. A horizontal cut yields a color plane like that shown in Figure 2-6; the ªringsº of the onion are loci of equal saturation. There are a number of systems built up in this way which vary in the type of color samples employed, the illumination, etc. Probably the most widely used system of this type is the Munsell system, which is available in

28

2 How Colors Depend on Spectra (Colorimetry)

Fig. 2-6. Color order based on qualities; hue, saturation, and brightness.

the form of an atlas. Brightness, hue, and saturation are termed value, hue, and chroma respectively in the Munsell system. When calculating color differences, one looks for conversion relations between the CIE system (in which color measurement must be done) and the sensationbased color system. Once these relations are known, the color differences can be calculated. Many color-difference systems have been developed, largely as a result of industrial color examination requirements. The acceptance of the CIELAB system, however, has pushed these into the background, and they need not be discussed further.

2.3.3 CIELAB System The CIELAB system has been adopted worldwide for the examination of pigmented coatings. This system, derived from the Munsell system, uses the three spatial coordinates a* (red-green axis), b* (yellow-blue axis), and L* (lightness axis) for brightness. In Figure 2-6, the a* axis is approximately the line connecting red and blue-green, while the b* axis is approximately the line connecting yellow and violet; the L* axis is the vertical lightness axis. The name ªCIELABº is a contraction from CIE and L*a*b*. In order to calculate the CIELAB coordinates, X, Y, and Z are first converted to the ªvalue functionsº X*, Y*, and Z*. The functional relation used is similar to the logarithm function and preserves physiologically equidistant (uniform) brightness steps (in a similar way to the Weber-Fechner law): r r r X 3 Y 3 Z ; Y ; Z X Xn Yn Zn

3

(2.5)

(here Xn, Yn, and Zn are the CIE tristimulus values for the illuminant used, with Yn = 100 for all standard illuminants). For X / Xn, Y /100, and Z / Zn ^ 0.008 856, however,

2.3 Sensation-Based Systems

X 7:787

X 0:138 Xn

Y 7:787

Y 0:138 100

Z 7:787

Z 0:138 Zn

29

(2.6)

With these X*,Y*, and Z* values, the a*, b*, and L* are then obtained as follows:

a* 500 (X* ± Y*) b* 200 (Y* ± Z*) L* 116 Y* ± 16

(2.7)

The color locus in the color plane (a*,b* plane) can also be described in polar coordinates: C ab

p a2 b2

(chroma, as radius vector); b hab Arctan a (hue angle, as polar angle).

(2.8) (2.9)

The expression for L* in equation (2.7) calls for some explanation. Why was the simpler form L* = 100 (Y /100)1/3, which is also similar to the logarithm function, not chosen? The answer is that the equation was based on color matching tests with gray color samples differing in brightness, which the matching colorists had to arrange on an equidistant gray scale from dark to light. The points in the diagram (Fig. 2-7) show the result for which approximation was made. It turned out that the simpler curve was too steep in the middle range, so it was ªstretchedº with a factor of 116 (instead of 100), then shifted downward by subtracting 16 so that it passed through the data points, and the condition L*(100) = 100 was restored. After this shifting, however, the curve no longer cut the Y axis at the origin but rather at a Y 4 0, so that L*5 0 below this value. Negative lightness values are meaningless, so the convention was adopted that this portion of the

30

2 How Colors Depend on Spectra (Colorimetry)

Fig. 2-7. Derivation of the L* curve (see text for explanation).

Fig. 2-8. Derivation of the L* curve (see text for explanation).

curve be replaced by the tangent to the curve that also passes through the origin* (Fig. 2-8). For the point of tangency (Yt, L*t ), we have dL*/dY)Yt = L*t /Yt, so that according to equations (2.5) and (2.7) ! r Lt 1 Y t 16 and 116 3 Yt 100 Yt dL dY

Yt

116 Y t 2=3 3 100 100

* Unfortunately, a logarithmic formulation was not immediately chosen when the CIELAB system was established; for example, L* = 100 Y* = 100 7 log (1 + 13 Y /100)/log 14 or a similar formula.

2.3 Sensation-Based Systems

31

Setting the right-hand sides equal gives solutions for the coordinates of the point of tangency: Yt 3 16 3 0:008856 ; 100 2 116 Lt

3 16 2

1 8

so that the equation of the tangent line becomes L*(Y) = (L*t /Yt ) 7 Y. Using equation (2.7),Y* is then given by Y

L Y 16 100 Lt Y 16 Y 7:787 0:138 ; 116 Y t 100 116 116 100

which is just equation (2.6) within the range from Y0 = 0 to Yt = 0.8856. Note that Y*(0) 4 0; for X*(X) and Z*(Z), equality of this equation must nonetheless be preserved so that the additive term 0.138 disappears when differences are taken for a* and b* in equation (2.7). Although the formation of differences for a* and b* in equations (2.7) seems strange at first, it has a physiological justification. In the retina, the primary excitation of the cones is processed in six types of nerve cells, four of which function in a ªspectrally opponentº antagonistic manner while the other two act in a ªspectrally nonopponentº alinear manner. The spectrally nonopponent processors form the black/white system, the spectrally opponent ones the color system. If one imagines two colors measured on pigmented coatings as radius vectors in the CIELAB color space, namely VT = {a*T, b*T, L*T } for the test sample (T) and VR = {a*R , b*R , L*R } for the reference sample (R), then DE*ab = |VT ±VR| is the color difference in the CIELAB space, measured in ªCIELAB unitsº: DEab

p Da2 Db2 DL2

(2.10)

with the components Da* = a*T ± a*R Db* = b*T ± b*R DL* = L*T ± L*R

(2.11)

In the following presentation, all differences notated as D will be defined in this sense, namely as test sample minus reference sample. A significant advantage of the CIELAB system is that the color difference can be broken down into components in another way: into brightness, ªchromaº (corre-

32

2 How Colors Depend on Spectra (Colorimetry)

sponding to saturation), and ªhueº (corresponding to the hue component used earlier), in analogy to the way the color space was constructed (Fig. 2-9): DL LT

LR

DC ab C ab;T

(lightness difference as above) 2 1=2 2 1=2 C ab;R a2 a2 T bT R bR

(2.12)

(chroma difference) DH ab DE2 ab

DL2

DC 2 ab

1=2

(2.13)

(hue difference)

Fig. 2-9. CIELAB system: breaking down of color differences into components.

DH*ab is positive if a*R b*T ± a*T b*R > 0 and negative if not. It represents the L* component of the vector product VR 6 VT and characterizes the sense of rotation in the associated vector plane. If the coincidence of the vector VR of the reference sample with the vector VT of the test sample involves a counterclockwise rotation of VR, then DH*ab is positive, and vice versa. The hue angle component is finally given by

33

2.3 Sensation-Based Systems

hab;R Arctan bT =aT

Dhab hab;T

Arctan bR =aR :

(2.14)

The sign convention for DH*ab ensures that DH*ab and Dhab will have the same sign. When these are compared with the other differences, it must not be neglected that Dhab is measured in degrees rather than CIELAB units, and thus has a different metric from these other differences. A note on the geometric meaning of DH*ab : From Figure 2-10 and equation (2.10), it follows that the line segment RT is the projection of DE*ab on the a*, b* color plane and has a length given by 2

RT Da2 Db2 DE2 ab

DL2

while, on the other hand, it can be calculated from the chromas of the test sample and reference sample and the angle between them (CR = C*ab,R , CT = C*ab,T, DC = C*ab , Dh = Dhab): 2

RT C 2R C 2T

2 C R C T cos Dh

Fig. 2-10. Geometric meaning of DH* ab (see text for explanation).

From equations (2.13) and (2.12), it follows that DH*ab2 is then: 2 DH 2 ab DEab

DL2

2

DC 2 RT

C T

C R 2 2 C R C T 1

cos Dh

In terms of the half-angle, 2 2 2 C C 1 cos Dh=2 sin Dh=2 4 C R C T sin2 Dh=2 DH 2 R T ab The right-hand side is simply the product of the two chords (Fig. 2-10) associated with CR and CT respectively, sR = 2CR sin (Dh /2) and sT = 2CT sin (Dh /2), so that the hue difference p (2.15) DH*ab sR sT

34

2 How Colors Depend on Spectra (Colorimetry)

is the geometric mean of the two chords associated with the hues of the reference sample and the test sample. For nearly achromatic, (i. e., nearly white, black, or gray) samples*, it is usually advantageous to break DE*ab down in a different way, because the usual breakdown as in equations (2.11) to (2.14) can lead to poor agreement with the observed color qualities. For example, suppose the color locus of the reference sample lies at or close to the zero point of the CIELAB system (a*R & b*R & 0) while the color locus of the test sample lies at an arbitrary distance from the zero point (a*T = 0, b*T = 0). Since Da* = a*T and Db* = b*T, the hue difference is then given by equation (2.13) as 2 DH 2 ab DE ab

DL2

2 2 C 2 ab Da Db

2 a2 T bT 0 :

This, however, does not agree with the shade actually observed in the direction of the test sample. For this reason it is better to calculate this direction and the reference sample-totest sample distance in the a*, b* color plane, as corresponding to segment RT in Figure 2-10. Its length Ds can be found for example, using equation (2.10) with DL* = 0; the direction angle of the shade Dj is obtained as tangent from the fraction Db* / Da*: Ds

p Da2 Db2 ;

Dj Arctan

Db Da

(2.16)

To simplify the evaluation, the color plane is divided into octants beginning at h = 22.58, and a color name is assigned to each of the resulting sectors (see Fig. 2-11). Table 2-3 then offers a very simple method of evaluation (with tan 22.58 & 0.4 and tan 67.58 & 2.5). For the example worked out above (a*R & 0, b*R & 0), the formula p q 2 Ds Da2 Db2 a2 T bT 6 0 correctly gives the strength while the nature of the shade follow from Db*/ Da* = b*T /a*T. The definitions and equations of the CIELAB system** are set forth in standards***. Accompanying the system when it was introduced was a recommendation * For standards see ªHue of near white specimensº and ªHue relative of near white specimensº in Appendix 1. ** On the notation: the * was selected to avoid confusion with the similarly named quantities in the earlier Adams-Nickerson system. The subscript ªabº is necessary because there is also a CIE color system with coordinates L*, u*, and u* (the ªCIELUVº system). Because CIELUV is not used for pigmented coatings, it will not be discussed here. *** For standards see ªColor Differencesº in Appendix 1.

2.3 Sensation-Based Systems

35

Fig. 2-11. Subdivision of the CIELAB color plane for calculation of the shade of achromatic samples.

Tab. 2-3. Color names Sign of Db*

+

±

±

Sign of Da*

+

yellow (Y)

|Db*/Da*| > 2.5

yellow-green (YG)

yellow-red (orange) (YR)

0.4 to 2.5

green (G)

red (R)

< 0.4

blue-green (BG)

blue-red (violet) (BR)

0.4 to 2.5

blue (B)

> 2.5

for its preferential use and testing. This proved to be justified, for the system has now gained widespread acceptance. A model of the CIELAB color space appears in Figure 2-12. The crossed cords indicate where the a* and b* axes cross; the cord running from the left foreground to the right background lies in the plane of the a* axis (left foreground is red, a* 4 0), while the cord running from right to left lies in the plane of the b* axis (right is yellow, b* 4 0). The circles marked on the plates are spaced 10 CIELAB units apart. As in the Munsell system, it is significant that there are a large number of distinguishable dark violet and light yellow hues. The formalism of the CIELAB system can easily be programmed into a desktop computer, which can also be linked on-line with a colorimeter.

36

2 How Colors Depend on Spectra (Colorimetry)

Fig. 2-12. Model of the CIELAB color space.

2.3.4 New Systems: CIE94 and CMC Despite the initial success of the CIELAB system, it should be noted that there is still room for improvement. For instance, the differences obtained by breaking down color differences are not always correctly reproduced when the system is applied to pigmented coatings. The following discrepancies are regularly established: ± Perceived brightness differences are undervalued by the CIELAB lightness difference DL*. ± Perceived saturation differences are overvalued by the CIELAB chroma difference DC*ab. Details on these points will be presented further on, in the practical section. The only remedies at this point comprise changes in the system which would eliminate these problems while preserving the differential-geometric properties. For these reasons, the CIE has proposed a new color difference formula based on CIELAB. The new ªCIE94º formula is:

DE94

s 2 DC ab 2 DH ab 2 DL kC SC kH SH kL SL

(2.17)

2.3 Sensation-Based Systems

37

where SL = 1, SC = 1 + 0.045 C*ab,R , SH = 1 + 0.015 C*ab,R (C*ab,R is the chroma of the reference). Here the ki are the parameters of externally imposed conditions, such as conditions specific to a certain application or conditions differing from the standard conditions. The standard conditions are as follows: Illuminant D65, ca. 1000 lx, surroundings gray L* = 50, ca. 100 cd/m2, sample size over 48, sample pair without gap between, homogeneous texture, 0 5 DE*94 5 5. Under these conditions, kL = kC = kH = 1. If neither of the two samples has been defined as the reference, C*ab should be taken equal to the geometric mean of C*ab,1 and C*ab,2. For coating color testing, the weaknesses of the CIE system can be compensated by a suitable choice of parametric factors, for example kH/kC = 1 and 3^ kH /kL^ 4. The formula is based on the CMC (l : c) formula but the correction terms are restricted to the chroma effect only. This is a drawback, since it must result in uncorrected color differences in the unsaturated and achromatic region. Another disadvantage is that color differences are no longer Euclidean, and spanning of a color space is therefore not possible. Two later publications have shown that the non-Euclidean CIE94 space can be transformed to an Euclidean color space so that even large color differences (ªcolor distancesº) can be calculated. Equation (2.17) was found to have two defects that must be corrected: ± The formula is not invariant to reference/sample exchange; contrary to CIE claims, the difference is not negligible. ± It is not normalized; that is, it does not use the just-accepted color difference as unit and thus is not commensurable with other color differences (e. g. with CIELAB). The first problem is remedied by the introduction of the mean C ab (see eq. 2.22 below), which is appropriate to the system as the geometric mean is not. The second is dealt with by multiplying the right-hand side of eq. (2.17) by kH . The CIE is expected to change these points. New Euclidean coordinates a94, b94, L94, C94, h94 are introduced for the transformation. It is necessary to take hab,1 and hab,2 such that their difference satisfies 08^ hab,2 ± hab,1 ^ 1808 (by interchanging the color loci if appropriate). The color difference E94 is then obtained by integrating the line element (2.17) according to the following scheme:

L94

kH L kL

(2.18)

C 94

kH ln 1 0:045 C ab 0:045 k C

(2.19)

h94 Ghab

with

G

C ab C 94 1 0:015 C ab

(2.20)

38

2 How Colors Depend on Spectra (Colorimetry)

Here 1 C 94;1 C 94;2 2 q 1 0:045 C ab;1 1 0:045 C ab;2 C 94

C ab

1 0:045

1

(2.21) (2.22)

(This formula is derived from eq. (2.21) by substituting all three C94 values with eq. (2.19).) a94 C94 cos h94 ;

b94 C94 sin h94

and finally E94

q 2 2 2 L L a a b b 94;2 94;1 94;2 94;1 94;2 94;1

(2.23)

A special case arises if h94,2 ± h94,1 4 1808: q 2 E94 L94;2 L94;1 2 C 94;2 C 94;1 These formulas hold for arbitrarily large color differences in the CIE94 space. A number of color laboratories have recently had good experience with another color-difference system, the CMC* system, and so the CMC (l : c) formulas are stated here:

DECMC

s 2 2 DL DC ab DH ab 2 lSL cSC SH

(2.24)

Here 0:040975 L ; if L* 616, 1 0:01765 L or SL 0.511, if L* < 16 0:0638 C ab SC 0:638 1 0:0131 C ab SH (FT + 1 ± F) SC SL

* CMC: Colour Measurement Committee of the Society of Dyers and Colourists in the British Standards Institution (BSI). For standards see ªColor differences: CMCº in Appendix 1.

2.3 Sensation-Based Systems

39

C 2 ab with F q 4 C ab 1900 and T 0.36 + |0.4 cos (358 + hab)| , if ±158^ hab ^ 1648, or T 0.56 + |0.2 cos (1688 + hab)| , if 1648 < hab < 3458 If there is not reference, L*, C*ab and hab must be replaced by the arithmetic means of the values at the two color loci. The factors used in the textile industry are c = l = 1; suitable values are anticipated for other industries. A later publication has shown how to transform this relation into a Euclidean color space and also revealed that it shares the shortcomings of the CIE94 equation. They are corrected by ± Allways using the arithmetic means for L*, C*ab and hab to preserve invariance to interchanging the reference and sample ± Dividing the Si functions by 0.638 to make the results commensurable with other color systems The BSI is expected to modify the CMC formulas accordingly. The transformation to a Euclidean space (ªEuclideanizationº) makes the formulas somewhat more complicated; the reader is referred to the original publication (see Section 2.7). The most recent development can only be sketched here. The German standard DIN 6176 embodies a new Euclidean color system called DIN99. Because it does not appear to have achieved its final form and because, moreover, it has little hope of international acceptance, it will not be discussed here. The CIE, too, has recently stated a new color-difference formula, CIE2000, although it has not yet been officially promulgated. Once again, a description must wait.

2.3.5 Color Order Systems Color order systems arose from the practical requirement that manufacturer and purchaser should have a common vocabulary for the manufacture of colored objects. The origins of such systems go back a long way, and from the very beginning there has been an effort to verify all orderings visually on the basis of a suitable collection of color samples. This means, however, that the difficulty inherent in any color order system was programmed into it from the start, i. e., color samples are subject to the restrictions of whether the coloring materials (pigments or dyes) are available. The controversy therefore exists already: of whether available coloring materials (or their mixtures) should be systematized, or whether a new system should be developed for color appearance. This dilemma has not yet been resolved by any color order system; it is apparent, and a problem, more or less in all systems to be discussed.

40

2 How Colors Depend on Spectra (Colorimetry)

What distinguishes such color order systems from the physiologically equidistant systems discussed earlier? This justifiable question has no easy answer, for if both systems were perfect from the physiological standpoint then they would have to be identical. In other words, the ªabsolute color spaceº (to the extent that it is Euclidean for color differences as well) would offer the ideal metric for both requirements. This fact provides the best starting point for describing the distinction. A physiologically equidistant system imposes more stringent requirements: In general, it must satisfy the postulate that the geometry of the color space is Euclidean, since otherwise it would be difficult to give an unambiguous definition of color differences (i. e., distances between color loci). Color order systems do not require this postulate, since they generally involve merely some ordering (often a naive one) of color samples. Although the samples possess some systematic features, these are not always immediately obvious. Most of these systems employ the qualities of brightness, hue, and saturation for ordering. Color order systems are still important for the classification of pigments and dyes, but play no role at all in the colorimetric inspection of colorants. This book could thus meet its objectives without taking these systems into account; the bestknown representatives will, however, be discussed briefly, because a description of them lay lead to a deeper understanding of the problems encountered in colorimetry. We have chosen the following classification in the knowledge that it is not free of arbitrariness: ± Empirical color order systems ± Colorimetry-based color order systems 1) Empirical Systems Of all the empirical systems, the Munsell system is the most important; we introduced this system in Section 2.3.2. The system approximately satisfies the postulates of a physiologically equidistant system; otherwise it would not have been such a simple matter to make it the basis for the CIELAB system. New editions of the color samples and color atlases for the Munsell system are available. The Natural Color System (NCS) was developed in Sweden and is in use there. It takes the form of a color atlas. The three variables are blackness s, chroma c, and hue f. Certain limitations became apparent after the introduction of the system: it does not span the full color space occupied by coloring materials, and it does not always give reproducible color identification codes for glossy samples. Like any empirical system, NCS is not tied to colorimetry, and so it cannot be directly converted to other color systems. A set of tristimulus values is, however, defined for one set of measuring conditions. ªRAL-Farbregister 840 HRº (RAL Color Register) is not a color order system in the narrow sense. It imposes a numbered order, with color names, on industrially manufactured coloring materials required by public authorities (railways, postal service, etc.) and by makers of consumer goods. The ordering is not highly systematic

2.3 Sensation-Based Systems

41

and features only a rough orientation to color relationships (e. g., 3 = red). Colors can be obtained as samples (paint chips); one example is RAL 3013 ªTomato Redº. The RAL Register has recently been linked to the DIN Color System through colorimetry (see below). The Color Index is also not strictly a color order system, since it lacks consistency. It includes names based on origin (ªgeneric namesº) and numbers based on chemical makeup (ªconstitution numbersº) for individual pigments. Adequate differentiation is possible only for organic pigments. 2) Colorimetry-Based Systems Among schemes based on colorimetry, the DIN Color System* should be mentioned first because it features the most complete systematization and offers many advantages. It employs the measures blackness value D, hue T, and saturation S; these are linked to the CIE system. The available color samples include only matte colors. The division of the color circle into 24 parts makes the system somewhat unclear. Because it is not widely used except in Germany, this system is not likely to become an international standard. The Optical Society of America Uniform Color Scales System (OSA-UCS) should also be mentioned. It offers a set of formulae (link to CIE) and a collection of color samples. This system is virtually restricted to the U.S.A. The Ostwald system is really only of historical interest, especially as no sample collections are available. All the color order systems mentioned up to now share the problem that they do not permit direct determination of color differences between the test sample and the reference sample or between two specimens. To make such a determination, it is necessary to use a color difference system, most commonly the CIELAB system. This in turn is possible only for the colorimetry-based order systems. The best way to avoid having to work with two fundamentally different coordinate systems (the selected color order system and the CIELAB system) would be to employ CIELAB (which spans a color space) as an order system. This is the approach taken in the new RAL Design System (RAL-DS) (a successor to the Eurocolor system, which is no longer available). The notation is directly derived from the CIELAB coordinates: hue H = hab , lightness L = L*, and chroma C = C*ab. Thus 090. 80. 70 would denote a yellow color (hab = 908) with lightness 80 and chroma 70. The RAL-DS color atlas serves as the collection of color samples. Given the stated reservations about the CIELAB system, this color order system unites all the advantages that such a system can at present. First, it offers a simple connection to colorimetry; second, it permits direct color difference determination in the same system; and since CIELAB has become accepted for color difference measurement anyway, RAL-DS should lead to an international consensus. Along with national reservations, it appears that the main obstacle to agreement on a binding color order system is conservativism. * See ªDIN Color Systemº in Appendix 1.

42

2 How Colors Depend on Spectra (Colorimetry)

2.4

Mathematical Statistics of Color Coordinates

2.4.1 Normal Distribution in Three Dimensions The values obtained from a color measurement are generally the coordinates of a color locus in color space; that is, they are components of three-dimensional vectors. This is why it is more complicated to determine, for example, a measurement error in three dimensions than in one. The components of three dimensional vectors can no longer be treated as independent variables; it must be taken into account that correlations exist between the components, and statistical analysis must allow for these correlations. For example, a* and b* are formed from the same tristimulus value Y; furthermore, the color matching functions x (l), y (l) and z (l), which lead to the tristimulus values X, Y, and Z used in calculating a*, b*, and L*, have significant overlaps (see Fig. 2-4). Mathematical treatment must therefore be oriented to extending the normal distribution from one to three dimensions. For one-dimensional variables, the probability that a measured value will lie between x and x + dx is 1 2

w dx A e where A

sx and V

n 1 P xi n i1

(2.26)

x

x

(2.25)

(2.27)

sx

(mean)

(2.28)

p V (standard deviation) 1

n

dx

1 p sx 2 p

ds

x

ds2

n P

1 i1

xi

2 x

(variance)

(2.29)

If ds2 = 1, then from equation (2.27) the limiting value xe is xe x sx

(2.30)

2.4 Mathematical Statistics of Color Coordinates

43

and, from equation (2.25), the frequency is pden

w

e

wmax

1 2

0:6

(2.31)

(wmax A) This means that the probability of encountering a measured value at xe = x + sx is 60 % as great as that of encountering the mean value. In the case of two-dimensional vectors r = {x, y}, the probability that the measured value lies between r and r + dr is given by 1 2

w dx dy B e where

ds2

dx dy

p det G B 2p g11 g12 and G g12 g22 det G g 11 g 22

g212

(2.32)

(2.33)

(determinant)

(2.34)

ds2 g11 dx2 + 2 g12 dx dy + g22 dy2

(2.35)

y ± y} dr {dx, dy} r ± r = {x ± x,

(2.36)

x

n 1P x; n i1

y

n 1P y (means) n i1

(2.37)

The expression ds2 is thus replaced by the quadratic expression in equation (2.35). If ds2 is set equal to a constant, the function dy (dx) describes an ellipse in the dx, dy plane. For ds2 = 1, this ellipse is called a ªstandard deviation ellipseº. It represents the two-dimensional analog of the standard deviation sx which is the measure of deviations in the one-dimensional case. G is the matrix formed from the coefficients of the ellipse, and det G is its determinant. The step to the third dimension now presents no difficulty. Because the quantities whose deviation is of interest here are always color differences, the remainder of the development can be stated in terms of the CIELAB color space. The formula for the probability that a triple of measured values lies between V = {a*, b*, L*} and V + dV = {a* + da*, b* + db*, L* + dL*} is now w da* db* dL* C e

1 2

ds2

da* db* dL*

(2.38)

44

2 How Colors Depend on Spectra (Colorimetry)

where

p det G C 2 p3=2 0 1 g11 g12 g13 G @ g12 g22 g23 A g13 g23 g33

(2.39) (2.40)

(symmetric matrix of ellipsoid coefficients) det G g11 g22 g33 + 2 g12 g23 g13 ± g11 g223 ± g22 g213 ± g33 g212

(2.41)

(determinant of G) ds2 g11 da*2 + g22 db*2 + g33 dL*2 + 2g12 da* db* + 2g23 db* dL* + + 2g13 da* dL*

(2.42)

dV {da , db , dL } V ± V {a ± a , b ± b , L ± L } a

n n n 1 P 1 P 1 P a ; b b ; L L n i1 n i1 n i1

(means)

(2.43) (2.44)

The exponent in the normal distribution is dominated by a quadratic form, which for ds2 = const describes an ellipsoid in the color space. The normal form ds2 = 1 now represents the ªstandard deviation ellipsoidº. The probability of encountering a measured value on the ellipsoid is, once again, ca. 60 % of the probability of the mean, since equation (2.31) holds here as well. The following statistic applies to frequency information based on the probability density: (2.45) pden exp 1=2 ds2den and ds2den 2 ln 1=pden Here, as we already know from equation (2.42), ds2den signifies a certain ellipsoid. The collection of concentric ellipsoid with parameter pden, for example with pden in 10 % steps as listed in Table 2-4, forms an image of the three dimensional normal distribution w (a*, b*, L*). To be distinguished from this is statistical information based on the cumulative probability. The cumulative probability is found by summing the probability densities between certain limits of integration, for example from zero (i. e., the mean itself) up to an ellipsoid ds2cum specified as the limit of integration. The values answer the following question: How many measured values are located inside the ellipsoid ds2cum ? If one refers to the set of all measured values, the cumulative frequency pcum is obtained; this again yields a family of concentric ellipsoids, but

2.4 Mathematical Statistics of Color Coordinates

45

Table 2-4. ds2 values for the three-dimensinal normal distribution versus frequency p, for the probability density (subscript den) and the cumulative probability (subscript cum). p

ds2den

ds2cum

0% 10 % 20 % 30 % 40 % 50 % 60 % 70 % 75 % 80 % 90 % 95 % 99 % 99.5 % 100 %

? 4.61 3.219 2.408 1.833 1.386 1.022 0.713 0.575 0.446 0.2016 0.1026 0.02010 0.01025 0

0 0.584 1.005 1.424 1.869 2.366 2.946 3.665 4.11 4.64 6.25 7.81 11.35 12.84 ?

now these image the cumulative distribution. This family of bounding ellipsoids obeys another well-known statistic, the chi-square distribution with three degrees of freedom: dsR2cum 1 x1=2 e x=2 dx (2.46) pcum 2 p1=2 0 which can also be tabulated. Table 2-4 includes recently re-calculated values of the cumulative frequency of the three-dimensional normal distribution for pcum at 10 % intervals, plus some further values in the range beyond 90 %. In the one-dimensional case, probability density and cumulative probability can also be represented in terms of simple graphs (Gaussian bell-shaped curve or Sshaped cumulative curve). In the three-dimensional case, distributions can be visualized only through families of ellipsoids, as shown here; furthermore, this is a representation suitable to the problem under consideration. The next section will discuss how the spatial position of ellipsoids can be visualized by projection into the three principal planes of the color space. The determination of the typical coefficients gik for the standard deviation ellipsoid is presented in Sections 2.4.4 and 2.4.5.

46

2 How Colors Depend on Spectra (Colorimetry)

2.4.2 Standard Deviation Ellipsoid The equation of an ellipsoid (2.42) is a special case of the equation for the general surface of order two. The necessary and sufficient conditions for the coefficients gik to describe an ellipsoid are as follows: 3 P gii > 0 g ii > 0 i 1; 2; 3; i: e:; tr G ^ i > 0 i 1; 2; 3; i: e:; det G

3 P i1

i1

^i >0 det G

det G > 0

(2.47)

^i Here tr (G) is the trace and det G the determinant of matrix G (eq. 2.40); the G are the cofactors (the 2 6 2 matrices left after the i-th row and the i-th column are deleted). Explicitly, tr (G) g11 + g22 + g33 3 P i1

^ i det G ^ 1 det G ^ 2 det G ^ 3 (g11 g22 ± g212) + (g22 g33 ± g223) + det G + (g11 g33 ± g213)

det G = g11 g22 g33 + 2g12 g23 g13 ± g11 g223 ± g22 g213 ± g33 g212

(2.48)

In order to judge the spatial orientation of the ellipsoid, it is important to know the positions of its principal axes. The partial derivatives of normal form in equation (2.42) are calculated for this purpose; the three partial derivatives are simultaneously the components of the gradient on the surface E = ds2 : 8 9 g 11 a g12 b g 13 L ; = < uE uE uE grad E ; ; 2 g 12 a g22 b g 23 L ; 2 G V (2.49) : ; ua ub uL g 13 a g23 b g 33 L ; The gradient is normal to the ellipsoid surface (Fig. 2-13). The axes of the ellipsoid (i. e., the vectors a, b, and c) have the property that the gradient is parallel to each axis; mathematically: 1 grad E G 7 V {la*, lb*, lL*} l 7 V 2 (l = scalar factor)

(2.50)

The second and last expressions lead to three equations for the three unknown coordinates, each for one principal axis of the ellipsoid.

2.4 Mathematical Statistics of Color Coordinates

47

Fig. 2-13. Gradients on the ellipsoid surface (see text for explanation).

For the system of equations to have solutions for a*, b*, and L*, the functional determinant (ªcharacteristic polynomialº of matrix G) must vanish. This requirement gives the ªcharacteristic equationº of G, also called the ªsecular equationº: 0 1 g12 g 13 g 11 l g22 l g 23 A det G l E det @ g 12 g 13 g23 g33 l l3

a2 l2 a1 l

where a0 det G ;

a1

3 P i1

a0 0

^i; det G

(2.51)

a2 tr G

(see eq. 2.48) (E = identity matrix) This is a third-degree equation in l and can be solved by well-known methods. Its ªcharacteristicº roots or eigenvalues la, lb, and lc are all real; each is associated with one of the ellipsoid axes a, b, c. The coordinate system spanned by the three ellipsoid axes is called the ªprincipal axis systemº. If the gradients in the three directions a, b, c are formed with equation (2.50), each gradient, expressed in the principal axis system, has just one component in one of the three axis directions. In this way, G from equation (2.40) becomes a diagonal matrix in which only the three diagonal components are nonzero; these positions are occupied by la, lb, and lc. From equation (2.42) this corresponds to a normal form reduced to the coefficients of the quadratic terms gii, with g11 = la, g22 = lb, and g33 = lc. From the principal axis equation of the ellipsoid a2 b2 L2 2 2 1 a2 c b

(2.52)

48

2 How Colors Depend on Spectra (Colorimetry)

it follows that the lengths of the principal axes are 1 a j aj p la 1 b j bj p lb 1 c jc j p lc

(2.53)

If we have one root l, two of equations (2.50) give the ratios u = a* / L* and u = b* / L*, that is, the directions of the principal axes: u

a g 12 g 33 L g 23 g 11

l l

g 13 g 23 g 12 g 13

u

b g12 g 33 L g13 g 22

l l

g 13 g 23 g 12 g 23

(2.54)

Then, for the principal axis a, the system of equations (2.53) and (2.54) yields a2a a2b a2L

1 la

aa ua ; aL

ab ua aL

(2.55)

and with a = {aa*, ab*, aL*} 1 aL q la 1 u2a u2a aa ua aL ab ua aL

(2.56)

and similar solutions for b and c. The axis directions can also be characterized in terms of the polar coordinate angles j and W (Fig. 2-14):

49

2.4 Mathematical Statistics of Color Coordinates

tan ja tan Wa

ab ua ; aa ua q a2a a2b aL

q u2a u2a

(2.57)

and similarly for jb, Wb and jc, Wc.

Fig. 2-14. Three-dimensional polar coordinates.

To arrive at a three-dimensional picture of the position and orientation of the ellipsoid in color space, it is useful to calculate the projections of the ellipsoid on the coordinate planes and plot these, using a plotter connected to the computer if possible. The projection on the a*, b* plane is defined by the condition that the gradient has no L* component (Fig. 2-15):

Fig. 2-15. Projections of the ellipsoid (see text for explanation).

50

2 How Colors Depend on Spectra (Colorimetry)

1 uE g13 a g23 b g33 L 0 2 uL

(2.58)

from which it follows that 1 g13 a g23 b g33

L

(2.59)

Now the normal form of the ellipsoid equation (2.42) becomes Ea*b* = g'11 a*2 + g'22 b*2 + 2 g'12 a* b* = 1 where g'11 g11

g213 g33

g'22 g22

g223 g33

g'12 g12

g13 g23 g33

(2.60)

Equation (2.60) is the desired ellipse in the a*, b* plane (horizontal projection).The two axes of this ellipse are obtained from the ªsmallº secular equation det

g011 l0 g012

g012

g022

l0

0

(2.61)

which is quadratic. By analogy to equation (2.54), its two solutions l0a ; l0b imply two linear equations for the axes: b

1 l0 g012

g011 a

(2.62)

The three projections of the ellipsoid can so be calculated and then drawn as a horizontal and two vertical projections. To do this, it is desirable to connect pairs of exterior points by ªsection linesº. These are determined as follows: The gradient of equation (2.60) also has no b* component: 1 uEa b g012 a g022 b 0 2 u b Then b

g012 a g022

(2.63)

(2.64)

2.4 Mathematical Statistics of Color Coordinates

51

From equation (2.60) it now follows that the lines are tangent to the ellipse at +a*sec : 1/2 asec g022 = g011 g022 g02 (2.65) 12 2 by virtue of the ellipse conditions). (g'11 g'22 > g'12 The projections, axes, and section lines for the other two coordinates are calculated in a similar fashion, using appropriately modified equations.

2.4.3 Standard Deviations We refer to the discussion in Section 2.4.1; given the coefficients of the standard deviation ellipsoid, we now wish to calculate the standard deviations of the color measurements. In color space, the standard deviation is a vector s, defined as the point on the ellipsoid to which s points. Because the components of a vector can be expressed as a direction and a magnitude, the vectorial standard deviation of direction n is described by sn {asn , bsn , gsn} where

(2.66)

sn | sn |

Here n = {a, b, g} is a unit vector, which accordingly has to characterize only the direction of sn. Its components are the direction cosines, that is, the cosines of the angles between sn and the three coordinate axes. Substitution in the normal form of the standard deviation ellipsoid, equation (2.42), yields ds2 (g11 a2 + g22 b2 + g33 g2 + 2 g12 ab + 2 g23 bg + 2 g13 ag) 7 s2n = 1 so that for sn 1 sn q g11 a2 g22 b2 g33 g2 2 g12 a b 2 g23 bg 2 g13 a g

(2.67)

Here sn gives the length of the ellipsoid radius in spatial direction n. Thus, if a specified spatial direction is substituted in Equation (2.67), the radius for this direction is obtained. For a color coordinate or a color difference (or a difference obtained by breaking down the color difference) having the direction of n, the radius found is the desired standard deviation sn. The task thus consists of determining only the directions of the color coordinates or color difference and its differences obtained by breaking down the color difference, then substituting these in equation (2.67).

52

2 How Colors Depend on Spectra (Colorimetry)

We begin with the color coordinates*. The calculation is particularly simple for the standard deviations of a*, b*, and L*. For a*, aa = 1 and ba = ga = 0. Substitution in equation (2.67) gives the following for sa (similarly for sb and sL ): 1 sa p ; g11

1 sb p ; g22

1 sL p g33

(2.68)

The standard deviations of C*ab and hab also follow from the coefficients of the ellipsoid. For C*ab, aC

a cos h ; C

bC

b sin h ; C

gC 0

Hence it follows that 1 sC p g11 cos2 h 2 g12 sin h cos h g22 sin2 h C p 2 g11 a 2 g12 ab g22 b2

(2.69)

The direction in which hab can vary is given by the chord perpendicular to C*ab, s = 2sH. The magnitude is + (s /2) = + sH (Fig. 2-16): aH = ± sin h ;

bH = cos h ; gH = 0

1 sH p 2 g11 sin h 2 g12 sin h cos h g22 cos2 h

(2.70)

To calculate sh, half the chord must be divided by C = C*ab and converted back to an angle by taking the arctangent: sh Arctan

1 p 2 C g11 sin h 2 g12 sin h cos h g22 cos2 h

1 Arctan p g11 b2 2 g12 ab g22 a2

(2.71)

* To simplify the notation, the subscript ab and the * are dropped from the color coordinates and color differences; thus C = C*ab, DE = DE* ab, etc.

2.4 Mathematical Statistics of Color Coordinates

53

Fig. 2-16. Calculation of sh (see text for explanation).

Now on to the standard deviations of the color differences. Here the standard deviation ellispoid GD, of the color differences must be known. It is defined as in equation (2.40) except that the gik are now replaced by gDik ; da*, db*, and dL* by the differences dDa* = Da* ± Da*, dDb* = Db* ± Db*, and dDL* = DL* ± DL*, where Da*, Db*, DL* are the arithmetic means. We use arguments presented in the next section (Section 2.4.4), where it is shown that the difference ellipsoid GD is linked to the coordinate ellipsoid GR of the reference by the relation GD gDik 1=2 gRik 1=2 GR

(2.72)

Thus, if GD has not been determined separately, i. e., if only the reference ellipsoid GR is available, then the coefficients of GD can be calculated with equation (2.72). If, on the other hand, only GD is known, then GR can be obtained from equation (2.72). Proceeding in the same way as before, we substitute the direction cosines of the respective color differences in equation (2.67), thus obtaining the following relationships. For the differences Da*, Db*, DL*: 1 1 1 sDa q ; sDb q ; sDL q gD11 gD22 gD33

(2.73)

For the hue difference DH*ab : The hue difference is perpendicular (see Fig. 2-10) to the bisector of the angle h0 = (1/2)(hR + hT).

54

2 How Colors Depend on Spectra (Colorimetry)

Therefore,

aDH ± sin h0 ; bDH cos h0 ;

gDH 0

so that by equations (2.67) and (2.70) sDH sH (gDik , h0)

(2.74)

For the hue angle Dhab : Its standard deviation is the angle associated with sDH, that is, tan sDh = sDH /OW (Fig. 2-10). The length OW can be expressed in either of two ways, in terms of DH or OH, or in terms of both. From Figure 2-10 and equation (2.15), it is also easy to show that OH2 = CRCT. Accordingly, sDh Arctan 2 sDh =DH tan Dh=2 n o Arctan sDh = CR CT 1=2 cos Dh=2 n 1=2 o Arctan sDh = CR CT DH=22

(2.75)

For the chroma difference DC*ab : Because, in general, the chromas of reference sample and test sample differ in direction (Fig. 2-10), their standard deviations sC,R and sC,T must be calculated separately using equation (2.69). This must be done with the ellipsoid GR of the reference sample; if it is not available, equation (2.72) is employed to calculate it from GD. Then, by the additive rule for variances, 1=2 sDC s2C;R s2C;T

(2.76)

For the color difference DE*ab : The direction cosines are aDE

Da Db DL ; bDE ; gDE DE DE DE

The magnitude of the standard deviation is then DE sDE q gD11 Da2 gD22 Db2 gD33 DL2 2 gD12 Da Db 2 gD23 Db DL 2 gD13 Da DL (2.77)

2.4 Mathematical Statistics of Color Coordinates

55

The equations fulfill the objective: The standard deviations of the three color coordinates, the chroma, and the hue angle, as well as the standard deviations of the color difference and of all its composant differences, can now be calculated. All that is necessary to know are the six coefficients gDik of the standard deviation ellipsoid of the differences (or gRik of the reference) for a specified threshold confidence level.

2.4.4 Color Measurement Errors and Significance The ellipsoid coefficients gik needed for all the calculations in the preceding section can be determined by known methods. Firstly, from the number of measurements n, the arithmetic means are formed in accordance with equation (2.44), then the variances of a*, b*, and L* are formed: Var a Var b Var L

1 n

1 i1 1

n

n P

1 i1 1

n

n P

n P

1 i1

ai

a 2 ;

bi

b 2 ;

Li

L 2 ;

(2.78)

In the case of vector quantities, the variances alone are not enough to characterize the deviations in space. Correlations between the individual components must also be taken into account and can strongly influence their standard deviations: If, for example, large values of a* are always associated with large b* and L* values, then the standard deviation of a* will be smaller than if a*, b*, and L* varied in random sequence with no correlations. The strengths of the correlations between the three pairs of components are expressed in terms of the covariances: Cov a ; b Cov b ; L Cov a ; L

1 n

1 i1 1

n

n P

1 i1 1

n

n P

n P

1 i1

ai

a bi

b

bi

b Li

L

ai

a Li

L

(2.79)

56

2 How Colors Depend on Spectra (Colorimetry)

Now the variances and covariances are entered in a matrix V: 0 1 0 Cov a ; b Cov a ; L Var a u11 Var b Cov b ; L A @ u12 V uik @ Cov a ; b Cov a ; L Cov b ; L Var L u13

u12 u22 u23

1 u13 u23 A u33 (2.80)

This matrix is symmetric, because uik = uki. It is the three-dimensional analog of the variance s2x of the one-dimensional normal distribution. In the one-dimensional case, the precision can be specified in terms of the confidence interval, the interval within which a given percentage of the measurements are expected to fall. Similarly, the precision in the three-dimensional case can be specified by the ellipsoid, which has the point {a*, b*, L*} as its center (reference). The ellipsoid coefficients gik are the elements of the inverse matrix of V; thus* gik G V

1

(2.81)

G is also symmetric, since it was obtained from a symmetric matrix by inversion; gik = gki is also one of the necessary ellipsoid conditions. From this we see the following: Only by using the covariances can the standard deviation ellipsoid be obtained; in general, the ellipsoid is not oriented to the principal axes, because the measures of deviations must be invariant to the coordinate system chosen. If no correlation exists between the measured values of the reference and the test sample, then the additive rule for variances and covariances leads to the following relation for the reference, test sample, and color difference matrices: VD VT + VR or, after substitution of the respective standard deviation matrices, ±1 ±1 G±1 D GT + GR

If GT and GR are equal (GT = GR), then ±1 G±1 D 2 GR

or, after inverting, GD 1=2 GR This relation was used in Section 2.4.3 (eq. 2.72). * For an example of matrix inversion, see Chapter 6.

(2.82)

2.4 Mathematical Statistics of Color Coordinates

57

The preceding arguments used to determine gik thus close the circle: All the standard deviations of color measurement values can be calculated using equations (2.68) to (2.77). The formulae were obtained from the normal form of the ellipsoid G, that is, with ds2cum = 1. A look at Table 2-4, however, shows that according to the w2 distribution this ellipsoid contains only 20 % of all the measured values; we thus say that the ªconfidence intervalº 1 ± a is just 20 %. It would be desirable to have a confidence interval of 70 % (which would roughly correspond to the range of + sx customarily used with the one-dimensional normal distribution). Again from Table 2-4, this confidence interval is obtained with a value ds270 % = 3.665 of the w2 distribution. The following procedure results: ± If the ellipsoid is to be plotted as in Section 2.4.2, the gik should be divided by 3.665. ± If the standard deviations are to be calculated as in Section 2.4.3, the sx values should be multiplied by 3.6651/2 = 1.914. If a different confidence interval is required, the corresponding value for ds2cum from Table 2-4 should be used instead. The statistical concept of significance offers quantitative information as to whether a measured value ± here, the color difference and its composant differences ± is ªtrueº or whether it is falsified solely by measurement errors. This risk is always present when the color differences are very small, of the order of the error deviations. In the language of mathematical statistics, this means that it is necessary to determine whether the color difference found is larger or smaller than a ªcritical valueº t (also called the ªsignificance thresholdº). This value is formed in the same way as illustrated for the measurement error, with one additional step: division by the square root of the number of measurements n1/2. This extra step takes account of the fact that the mean becomes more and more accurate as the number of measurements increases, so that the deviations of the measurements about the mean are increasingly attributed to their real value. The value of t thus is given by the number of measurements n, the standard deviation sx, and the desired confidence interval 1 ± a:

t1

a

1=2 sx ds21 a =n

(ds2cum from Table 2-4)

(2.83)

The measured color difference DF is significant if | DF | 4 |tDF |, and not significant if | DF |^ | tDF |. The principles and methods for determining the significance of color differences are presented in DIN 55600. The standard purposely avoids calculating the standard deviations of the CIELAB coordinates, since the nonlinearity of the relations used for the transformation from the CIE system means that these values do not necessarily have a normal distribution. Even so, there is no objection to applying this system to the CIELAB coordinates themselves. The arithmetic mean of the coordi-

58

2 How Colors Depend on Spectra (Colorimetry)

nates of the reference also corresponds better to the true value than does the color locus of a selected individual preparation. The application to color differences alone is justified because color differences can be represented to a good approximation as differentials. As in the theory of errors, the total differential can be used; higher-order derivatives need not be considered. The total differential in fact represents a linear transformation in a small neighborhood, and since its coefficients in the neighborhood of a color locus are largely constant, it follows that da*, db*, and d L* have just as normal a distribution as the d X, dY, and dZ, or as the dR of the reflectances, to which d X, dY, and dZ are related in a linear function. The total error of a color measurement on a coating is made up of ± Error due to sample preparation ± Error due to measurement The preparation error can be further broken down into ± Error due to sample fabrication (sampling, grinding, etc.) ± Error due to application (application, drawing down) ± Error of homogeneity (constancy over the entire sample) Thus the covariance matrices are related to one another as follows: Vtot Vprep Vmeas Vprep Vsam + Vappl + Vhom

(2.84)

The error matrices are determined as follows: ± Measurement error matrix Vmeas : Make 20 determinations of color differences on the same sample ± Homogeneity error matrix Vhom : Perform 20 color measurements statistically distributed over the entire sample surface ± Application error Vappl : Apply a preparation of sample and a preparation of reference 20 times and measure ± Total error Vtot : Prepare, apply and measure 20 preparations of sample and reference. The covariance matrix for each error is calculated with eq. (2.80). Equations (2.84) then give the preparation error Vprep and the sampling error Vsam as the differences of the V matrices. As a rule, Vmeas is very much less than Vprep, and the colorimetric laboratory must make every effort to keep the latter as small as possible. The ellipsoid coefficients of the several error components (the G matrix) is finally obtained by matrix inversion.

2.4 Mathematical Statistics of Color Coordinates

59

2.4.5 Acceptability The manufacturer of pigments or pigmented coatings is expected to make products that match specified samples (ªreferencesº). The instrument for determining the matches is the human eye; products that pass this examination by the colorist are ªacceptedº and are said to be ªconformingº (to a standard). In general, to say that the test sample and the reference match is not to say that the measurements are absolutely identical; instead, it means that the sample values lie in a specified tolerance range. This initially unknown tolerance range cannot be derived from the general rules of colorimetry but must be determined experimentally in each individual case. The technique involves the coloristic matching of color samples close to the reference. The justification for this procedure was stated in Section 2.3.1; furthermore, none of the existing color difference systems is perfect in exactly reproducing the perceived color differences (not even the CIELAB system, Section 2.3.3, which has become the standard chiefly because of its consistent use). For this reason, a systematic series of graded color samples are placed around the reference in each instance, and this set is presented to the colorist for evaluation. As a rule, the submitted samples are divided into two sets (ªacceptedº and ªnot acceptedº) in accordance with the colorist's judgment. (An intermediate range identified as ªconditionally conformingº can also be established.) The goal of statistical analysis of the colorist judgments is to derive the coefficients of the ªacceptability ellipsoidº, since this supplies the computer with the needed selection criteria in a computer-controlled production control system. The most important procedure for deriving usable estimation functions for the parameters of a distribution is the ªmaximum likelihood methodº. As applied to our three-dimensional case, the steps are as follows: In accordance with equations (2.38) and (2.42), the probability that a test sample i will be judged as conforming to a reference is expressed in terms of Da*, Db*, and DL*, the color differences of the i-th sample. If the samples match the reference, the color differences vanish. Obviously, from equation (2.42), this implies that ds2i = 0 and w = 1; that is, the sample is in principle always judged to conform. In practice, a psychophysical experiment such as the one just described is always assumed to have a certain error rate p (false alarm rate). For example, a sample colorimetrically identical to the reference may not be judged as conforming. Thus, the probability that the colorist will adjudge such a sample as conforming to the reference is equal to q = 1 ± p, and the probability that any sample i will be judged as conforming is q exp (± ds2i /2). The complementary probability, that is, the probability that the sample will be judged as nonconforming, is then 1 ± q exp (± ds2i /2). If the colorist making these judgments is permitted only the choices ªconformingº and ªnonconformingº, the probabilities of these two answers can be linked through the binomial distribution and a likelihood function can be constructed:

60

2 How Colors Depend on Spectra (Colorimetry)

! n Y N M qe ji i1

1 2

ds2i

ji 1

qe

1 2

ds2i

N

ji

(2.85)

In this formula, n is the number of color samples; ji is the number of ªconformingº judgments; and N is the number of colorists making the judgments. The maximum likelihood method approximates the unknown parameters q and g11, g22, g33, g12, g23, g13 by taking values which maximize M. A necessary condition for M, as a differentiable function of q and the gik, to have a maximum (except at the boundary) is that the partial derivatives with respect to q and the gik vanish: uM uM uM uM uM uM uM 0 uq ug11 ug22 ug33 ug12 ug23 ug13

(2.86)

Because the factors in equation (2.85) are nonnegative, M is generally positive at a maximum. The natural logarithm ln M, which is a monotonically increasing function, therefore has a maximum precisely where M has a maximum. This result suggests replacing M with the function ln M, so that instead of equation (2.85) we have 1 ji ds2i ji ln q 2 i1 n P 1 ds2i 2 N ji ln 1 q e const

ln M

n P

i1

(2.87)

and instead of equation (2.86) u ln M u ln M 0 uq ugik

(2.88)

Now, instead of the laborous differentiation of the products, only the sums have to be differentiated. To determine the desired values of gik and p, iterative procedures for zero finding can be applied; these need not be discussed further here. By following the procedure described, we obtain ellipsoids of the probability density in a different way from the method based on the covariance matrix. Thus, the shape and position of such an ellipsoid in color space represents the probability with which a color locus lying on the ellipsoid will be deemed as conforming. This method is somewhat complicated, both experimentally and mathematically, but it is the best of all the methods tested; the mathematical difficulties are taken care of by the development of a functioning program. It must be pointed out that there are simpler methods of estimating the parameters. These are not discussed

2.4 Mathematical Statistics of Color Coordinates

61

here because either they presuppose some simplified version of the psychophysical experiment or else they are not efficient enough. In the equations written above, ds2i is the quadratic expression ds2 of the i-th sample: ds2 g11 Da*2 + g22 Db*2 + g33 DL*2 + 2g12 Da* Db* + + 2g23 Db* DL* + 2g13 Da* DL*

(2.89)

with ellipsoid G = gik. It is often desirable to relate the quadratic expression not to the L* a* b* coordinates but, instead, to the coordinate system spanned by the three orthogonal difference vectors DC*ab, DH*ab, DL*. It will now be shown that this is possible; The new ellipsoid G' = g'ik is obtained by transformation to the orthogonal DC*ab, DH*ab, DL* system. First, the a* and b* of the reference are expressed in terms of its polar coordinates C*ab and hab : a* C*ab cos hab

b* C*ab sin hab

Then the color differences (with DH*ab = 2 [C*ab (C*ab + DC*ab)]1/2 sin (Dhab /2) & C*ab Dhab) are given by the following formulae (see eq. 2.15 and Fig. 2-10): Da* & da* cos hab dC*ab ± C*ab sin hab dhab Db* & db* sin hab dC*ab + C*ab cos hab dhab After substituting these expressions into equation (2.89) and comparing the coefficients ds2 g'11 DC*ab2 + g'22 DH*ab2 + g'33 DL* 2 + + 2g'12 DC*a b DH*a b + 2g'23 DH*ab DL* + 2g'13 DC*a b DL* we obtain the new ellipsoid g'11 = g11 cos2 hab + g12 sin 2 hab + g22 sin2 hab g'22 = g11 sin2 hab ± g12 sin 2 hab + g22 cos2 hab g'33 = g33

1 (g22 ± g11) sin 2 hab 2 g'23 = g23 cos hab ± g13 sin hab g'12 = g12 cos 2 hab +

g'13 = g23 sin hab + g13 cos hab

(2.90)

62

2 How Colors Depend on Spectra (Colorimetry)

The inverse transformation g'ik ? gik is described by the formulas g11 = g'11 cos2 hab ± g'12 sin 2 hab + g'22 sin2 hab g22 = g'11 sin2 hab + g'12 sin 2 hab + g'22 cos2 hab g33 = g'33 1 (g'11 ± g'22) sin 2 hab 2 g23 = g'23 cos hab + g'13 sin hab g12 = g'12 cos 2 hab +

g13 = g'13 cos hab ± g'23 sin hab

2.5

(2.91)

List of Symbols Used in Formulas

a, b, c ab a*, b*, L* a94, b94, L94 a, b, c a a, b, g A B c cum C C, C*ab C94 Cov den d ds2 D DE*ab, DE DE *94 Dhab,Dh DH*ab, DH

magnitudes of a, b, c (as subscript) denotes CIELAB CIELAB coordinates CIE94 coordinates vectors of the ellipsoid axes significance level; 1 ± a, confidence interval direction cosines of s; components of n normalization factor for one-dimensional normal distribution normalization factor for two-dimensional normal distribution CMC parametric factor (as subscript) denotes cumulative probability normalization factor for three-dimensional normal distribution chroma (CIELAB) chroma (CIE94) covariance (as subscript) denotes probability density difference (measured value minus its mean) quadratic form of normal distributions color difference expressed as difference between CIELAB coordinates (test sample minus reference) color difference (CIELAB) color difference (CIELAB 94) hue angle difference (CIELAB) hue difference (CIELAB)

2.5 List of Symbols Used in Formulas

Ds e E Ea*,b* ECMC E94 F F gik G hab , h h94 i j kC, kH, kL l l L* l L94 m max M n n n N p j (l) j q r R R sR, sT sec sn SC, SH, SL sx t t T T W

magnitude of shade (as subscript) denotes limiting value area of ellipsoid circumference of ellipse color distance (CMC) color distance (CIE94) CMC parameter color stimulus in CIE system; CIE color locus matrix element in i-th row and k-th column of G matrix of ellipsoid coefficients hue angle (CIELAB) [in degrees] hue angle (CIE94) number of sample evaluated number of ªconformingª judgments CIE94 parametric factors wavelength scalar factor in secular equation (see a*) CMC parametric factor (see a94) physical measure of intensity (as subscript) denotes maximum likelihood function number of measurements (as subscript) denotes standard illuminant unit vector in direction of s number of colorists frequency (statistics) spectral distribution meridian angle (spherical coordinates) individual probability radius vector reflectance (as subscript) denotes reference circle chords in CIELAB system (as subscript) denotes section line vector of standard deviation in direction of n CIE94 weighting functions standard deviation of quantity x significance threshold (as subscript) denotes point of tangency CMC parameter (as subscript) denotes test pigment polar angle (spherical coordinates)

63

64

2 How Colors Depend on Spectra (Colorimetry)

u, u uik V V

Var,V w x, x x, y, z xl, yl, zl X,Y, Z X,Y, Z X*,Y*, Z* y, y

2.6

auxiliary variables for principal axis directions matrix element in i-th row and k-th column of V CIELAB color locus covariance matrix with subscripts: appl of application hom of homogeneity meas of measurement prep of preparation tot total variance probability function measured value and its arithmetic mean (CIE) chromaticity coordinates tristimulus values of spectral colors; CIE color matching functions (CIE) reference stimuli (CIE) tristimulus values CIELAB value functions measured value and its arithmetic mean

Summary

The basic principle of colorimetry is that, using just three selected lights, all other color stimuli can be simulated fully by additive mixing. On the other hand, a color stimulus can also be prepared from the spectral colors by mixing; thus it has a spectral distribution, which in the case of object colors has been given the name ªspectral reflectanceº. The trichromatic principle makes it possible to construct a threedimensional color space once three reference stimuli (primaries) have been defined. In this color space, the coordinates are to be understood as components of a vector. This trichromatic theory has recently gained physiological confirmation. The CIE color notation system and the CIE standard observer were created on this basis in 1931; the principles are stated in standards. The CIE system imitates the human eye: The huge number of possible optical stimuli is reduced in a meaningful way to a much smaller set that can be comprehended by the mind. The CIE color notation system has, since its creation, proved its unrestricted suitability for use in all technical applications of colorimetry. It permits worldwide understanding as to colors. As to pigment evaluation, however, there are additional demands. The system is not easy to visualize, and physiologically equidistant color differences cannot be determined with it. For ease of understanding, Helmholtz proposed a different three-variable description: brightness, hue, and saturation. In the determination of color differences, one of the principal tasks of colorimetry, there

2.6 Summary

65

was no major progress until recently. For this purpose, a color space must be constructed through matching experiments on samples with small color differences; the best-known system of this type ist the Munsell system. After a CIE recommendation, the CIELAB system (based on the Adams-Nickerson system) has been used in pigment testing for some years. In CIELAB, quantities evaluated physiologically can first be calculated from the CIE tristimulus values, and by taking differences in pairs between the results the CIELAB coordinates are then obtained. This process of forming differences finds its physiological justification in the structure of the nervous system that processes information from the eye. The determination of actual color differences is then accomplished by calculating the vectorial distance between the color loci of the reference and test pigments and its breakdown into the three components lightness, chroma, and hue. Thus color measurement is performed in the CIE system and the results are then transformed into the CIELAB system (preferably with the aid of a computer, since CIELAB lends itself to programming). Despite the success of CIELAB, there are needs for improvement (DL* undervalues the perceived brightness, DC*ab overvalues the perceived saturation). For that, a new formula ªCIE94º has been created. The color system corrects some shortcomings of CIELAB. Even this system has the drawback of not spanning a non-euclidean color space, so that large color differences (ªcolor distancesº) cannot be calculated. A recently developed technique, however, can transform the CIE94 color space to an euclidean color space, thus permitting the calculation of color distances. The CMC color system, originally developed for the textile industry, was also described briefly. This system is gaining in importance for color measurement on coatings as well. The system was later euclideanized so that color distances can be calculated. More recent systems such as DIN99 and CIE2000 were merely mentioned, because they do not yet exist in final form. This chapter dealt briefly with color order systems, which were classified as empirical and colorimetry-based systems. The second group included the DIN Color System and the OSA-UCS system. Special attention was focused on the new RAL Design System with its color atlas, which provides an ideal link between color order and CIELAB. In pigment testing, determining the precision of color measurement is the key to assessing the significance of color differences. The precision serves as a figure of merit both for the colorimetric measurements in full shade comparisons and for the colorimeter being employed (with the help of a collection of samples). The treatment begins with known relations describing the statistics of colorimetric data. The first step is to calculate the variances of the CIELAB coordinates. These are not, however, sufficient to describe the deviations of the measurements; if one colorimetric value shows large deviations, it is important to know whether the other two also vary widely or whether they are stochastically distributed. For this reason, the covariances are also necessary for a complete description. The three variances and the three covariances are entered in a symmetric matrix, the inversion of which

66

2 How Colors Depend on Spectra (Colorimetry)

yields the coefficients of the standard deviation ellipsoid. The equation of the ellipsoid always contains a term on the right-hand side for which the tabulated w2 distribution value for a given confidence interval must be substituted. A relatively new procedure is the use of the resulting ellipsoid for the calculation of errors in the measured CIELAB coordinates, in the color differences, and in the composant color differences. These are equal to the radii of the ellipsoid in the spatial direction corresponding to the coordinate or color difference in question. The formulas for calculating these standard deviations are stated in this chapter, along with formulas useful for visualizing the spatial position of the error ellipsoid. In the manufacture of pigments and pigmented coatings, the requirement of conformity (to a standard of reference) is leading to a more rational procedure for acceptability testing. Rapid development in the computer field has opened up the possibility of letting a computer make the decision as to conformity, using specified criteria. But such criteria cannot be derived from purely colorimetric considerations; they must be obtained by having the responsible colorists perform matching tests on appropriate samples. In order to calculate the ellipsoid coefficients, it is desirable to employ the maximum likelihood method; while this is a old technique, it has recently been applied to this problem in the U.S.A. It has to be kept in mind that misjudgments also occur and must be smoothed out statistically. The likelihood function can be maximized with the help of a formula based on a binomial distribution of judgments. The mathematical operations can be substantial and a computer is needed. The calculation yields ellipsoids of probability density.

2.7

Historical and Bibliographical Notes

The crucial step in color theory occurred when Newton [1] laid the foundations for a scientific understanding of color phenomena by breaking sunlight down into its spectral components and correctly interpreting this process. The invention of the spectrograph by Young [2] also made it possible to measure spectral distributions. Young further discovered empirically the physiological relationships that were later formulated by Grassmann [3]. For the physiological principles of the YoungHelmholtz theory of color vision see, e. g., [4]; Helmholtz himself reported on the trichromatic theory [5]. Nonetheless, it was not until 1931 that a definition of the primary stimuli was agreed on. In that year the CIE, on the basis of the first usable experimental studies of the color matching functions by Wright [6] and Guild [7], decided to propose such primary stimuli (primaries, reference stimuli) as worldwide standards. The curves evaluated by various observers were averaged and the result was defined as the ªCIE standard observerº. The sensory organs as information-processing systems are described in, e. g., [8]. A number of excellent publications on the theoretical principles of colorimetry have appeared both in English [9±12] and in German [13±16]; further citations

2.7 Historical and Bibliographical Notes

67

can also be found in these. Colorimetry with special application to pigments is described by Gall [17]. For the construction of a physiologically equidistant color space see, e. g., [18]; [19] is the Munsell atlas. The DIN Color System was introduced by Richter [20]; the RAL Design System, by Gall [21]. The Adams-Nickerson (AN) system for testing pigments [22], [23], derived from the Munsell system, had been well known for decades when, in 1973, the German Standards Committee (DIN) and later the CIE proposed its testing in the form of the CIELAB system. CIE94 has appeared as CIE Publication No. 116 [24]. The transformation from CIE94 to an euclidean color space is described in [25, 26]. The CMC system was later euclideanized as well [27]. The new DIN99 system has come under sharp criticism [28]. The physiology of color vision is described in, e. g., [29], [30]. A comprehensive treatment of the mathematical statistics of color coordinates can be found in [31]. The theoretical basis for characterizing test errors in the colorimetric evaluation of color differences was set forth earlier and fully developed, in a different context, by Brown and MacAdam [32]. The problem solved by these authors was to determine experimentally the perceptibility threshold for color differences. Their analysis led to ªtolerance ellipsoidsº localized in color space. The reference was located at the center of each such ellipsoid; all colors which were not distinguishable from the reference by the observer are located within the ellipsoid, while outside the ellipsoid are the colors that the observer can distinguish from the reference. It had already been demonstrated that the figure must be an ellipsoid for normally distributed color samples [33]. Later, Robertson also proposed the Brown-MacAdam principle for test errors [34]. The justification is that the two problems have identical mathematical structure: As has been shown, both cases involve the extension of the Gaussian normal distribution from one to three dimensions; see, e. g. [35]. The analysis of the total error into error components is described in [36]. Tables giving the values of statistical functions such as the w2 distribution can also be found in statistics textbook and collections of mathematical tables, e. g. [37]. The acceptability is treated in [39]. The maximum likelihood method goes back to Gauss (1880) and was later generalized by Fisher in 1912 [38]. The principles of the technique used here [39] were set forth in a publication by Billmeyer and co-workers [40] and later recommended by Robertson [41] on behalf of the CIE. Another calculation method is described by Brockes and co-workers [42]. It must not be ignored that cybernetics, more than any other field of knowledge, has contributed enormously to the development of colorimetric test methods. Cybernetics has figured prominently in at least three areas and will help to determine the course of future development: ± Through development of computers for use specifically in color examination. ± Through the application of cybernetic conceptual models to measurement procedures and instruments.

68

2 How Colors Depend on Spectra (Colorimetry)

± Through the application of cybernetic conceptual and analytical methods to the phenomenon of vision [43]. The last of these points is important because an improved knowledge of vision is an essential condition, e. g., for the construction of better colorimeters. On the use of computers in the laboratory see, e. g. [44]. The history of colorimeters and color measuring has been dealt with elsewhere in detail [15], and it is therefore not taken up here.

References [1] [2] [3] [4] [5] [6] [7] [8] [9] [10] [11] [12] [13] [14] [15] [16] [17] [18] [19] [20] [21] [22] [23] [24] [25] [26] [27] [28] [29] [30] [31] [32] [33] [34]

I. Newton: Optics. Innys, London 1704±1730 (reissued by Mc Graw-Hill, New York 1931). T. Young, Phil. Trans. Roy. Soc. London 92 (1802) 12. H. Grassmann, Ann. Phys. (Leipzig) 89 (1853) 69. G. Wald, Angew. Chemie. Internat. Edit. 80 (1968) 857. H. v. Helmholtz: Handbuch der physiologischen Optik. Voss, Leipzig 1911. W. D. Wright, Trans. Opt. Soc. London 30 (1928/29) 141. H. Guild, Phil. Trans. Roy. Soc. London A 230 (1931/32) 149. K. Steinbuch: Automat und Mensch, Springer, New York 1971, 4. edit., 200 ff. W. S. Stiles, G. Wyszecki, Color Science, Wiley & Sons, New York, 2. edit., 1983. D. L. MacAdam, Color Measurement, Springer, New York, 2. edit., 1985. F. W. Billmeyer jr., in Encyclopedia of Chemical Technology, 3. edit., J. Wiley & Sons, New York 1979,Vol. 6, 523. R. W. G. Hunt, Measuring Color, J. Wiley & Sons, New York, 1987. E. Schrædinger, Ann. Phys. (Leipzig) 63 (1920) 397, 427. M. Born, Naturwissenschaften 50 (1963) No. 2, 3. M. Richter, Einfçhrung in die Farbmetrik, W. de Gruyter, Coll. Gæschen, Berlin-Heidelberg 1976. A. Brockes, D. Strocka, A. Berger-Schunn, Bayer-Farben-Revue, Sonderheft 3/2 D, 1986. L. Gall, The Color Science of Pigments, BASF Ludwigshafen, 1971. G. Wyszecki: Farbsysteme, Musterschmidt, Gættingen 1960, 81. A. H. Munsell: Atlas of the Munsell Color System, Wadsworth-Howland, Boston 1915. M. Richter, Farbe I (1953) 85. L. Gall, farbe + lack 98 (1992) 863. E. Q. Adams, J. Opt. Soc. Am. 32 (1942) 168. D. Nickerson, K. F. Stultz, J. Opt. Soc. Am. 34 (1944) 550. Commission Internationale de l'Eclairage, Industrial Color Difference Evaluation, CIE Technical Report No. 116, CIE Central Bureau,Vienna, Austria. H. G. Vælz, Die Farbe 44 (1998) No. 1±3, 1. H. G. Vælz, Die Farbe 44 (1998) No. 3±4, 97. H. G. Vælz, Die Farbe 45 (1999/2000), No. 1±3, 1. H. G. Vælz, Die Farbe 46 (2000), in press. D. H. Hubel, Eye, Brain and Vision, Sci. Am. Lib., New York 1988. J. Walraven, 7th Aic Congress 1993 Budapest, Congress book. H. G. Vælz, farbe + lack 88 (1982), S. 264 und 443. W. R. J. Brown, D. L. MacAdam, J. opt. Soc. Am. 39 (1949) 808. L. Silberstein, D. L. MacAdam, J. opt. Soc. Am. 35 (1945) 32. A. R. Robertson, The specification of the performance characteristics of colorimetric instruments, CIE TC-1.3, June 1973.

2.7 Historical and Bibliographical Notes

69

[35] K. Stange, Angewandte Statistik, Bd. I (1970) u. Bd. 2 (1971), Springer, New York. [36] H. Schmelzer, H. G. Vælz, Signifikanz von Farbabstånden, in DIN-Fachbericht 49, Beuth-Verlag GmbH, Berlin, 1995. [37] W. Abramowitz, I. Stegun, Handbook of Mathematical Functions, Nat. Bur. Stand., Appl. Math. Ser. 55, US-Gov. Print Off., Washington, 3. edit. 1965. [38] E. Kreyszig, Statistische Methoden und ihre Anwendungen, Vandenhoeck u. Ruprecht, Gættingen, 3. edit., 3. reprint, 1974, 174 ff. [39] H. G. Vælz, Toleranzfindung, in DIN-Fachbericht 49, Beuth-Verlag GmbH, Berlin, 1995. [40] F. W. Billmeyer, W. G. Howe, R. M. Rich, J. opt. Soc. Am. 65 (1975) 956. [41] A. R. Robertson, Col. Res. Appl. 3 (1978) Nr. 3, 149. [42] D. Strocka, A. Brockes, W. Paffhausen, Farbe + Design 1980 Nr. 15/16, 75. [43] H. G. Vælz, XI. Fatipec-Kongress 1972 Florence, Edizione Ariminum, Mailand, 43. [44] J. Hengstenberg, K.-H. Schmitt, B. Sturm, O. Winkler (Ed.) Messen, Steuern, und Regeln in der chemischen Technik, Springer New York, 3. edit., 1985.

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

3

How Spectra Depend on the Scattering and Absorption of Light (Phenomenological Theory)

3.1

Introduction

3.1.1 Phenomenological Theory and Its Significance The name ªphenomenological theoryº refers to all theoretical statements about how the radiance of light incident on a layer is affected by absorption and scattering. Such a theory affords the needed physical-theoretical and mathematical tools for describing how the reflection spectrum of a layer can be derived from its absorption and scattering properties as well as its thickness. The model employed is that of light pathways or channels, roughly as known from geometrical optics; the absorption or scattering action of the medium is represented by optical material constants, that is, purely phenomenological quantities. The phenomenological theory treats the medium as a continuum characterized by the physical qualities of absorption and scattering; accordingly, the presence of discrete particles as a necessary (but not sufficient) condition for scattering is of no significance in this theory. Speaking casually, one can say that ªthe phenomenological theory does not know anything about particlesº; in other words, it deals in physical qualities that can be described without reference to pigment particles and their special properties. To attribute absorption and scattering properties to a single particle, one must resort to the ªcorpuscular theoryº (see Chapter 5, also Figs. 1-2 in Chapter 1). Only that theory makes further statements about the optical material constants from phenomenological theory, indeed attributing them to the refractive index, size, and shape of the individual particle. In a certain sense, descriptions of the concentration dependences of the optical constants provide a bridge between the phenomenological and corpuscular theories, defining coefficients related to the pigment or dye concentration and then treating these coefficients as independent of the concentration. In this context, the position of the phenomenological theory of turbid media clearly implies the fundamental importance of the theory for the pigmenting of lacquers, paints, plastics, and so forth, and thus for all matters relating to the application and economics of coloring materials. In this chapter, we will briefly present the many-flux theory as a complete, general phenomenological theory, with a detailend treatment of the four-flux theory, and derive the most important formulas. It will be seen that the theory of Ryde is a special case of the four-flux theory; the well-

72

3 How Spectra Depend on the Scattering and Absorption of Light

known Kubelka-Munk theory, a special case of the two-flux theory; and the Lambert (Lambert-Bouguer) law, a special case of the one-flux theory. Lambert's law and the Kubelka-Munk theory long ago became accepted throughout the pigment and dye world; the four-flux theory, in contrast, has been a presence chiefly in the literature. Nonetheless, it seems important to us to deal with this theory in more depth, since it contains possibilities that have as yet been utilized little or not at all. It includes, for example, the cases in which radiation (either directional or diffuse) is incident on both sides of the layer. Such configurations are encountered everywhere and are also of technical interest (e. g., lamp enclosures that are viewed in both reflected and transmitted light). A further advantage is that the four-flux theory makes it exceedingly easy to handle special cases, not just the two named above (Kubelka-Munk theory, Lambert's law) but also the extreme cases of ªabsorption onlyº and ªscattering onlyº, as well as the limiting cases of a black background and of an opaque (ªoptically infinitely thickº) layer. In the four-flux theory, scattering and absorption are controlled through a few material constants, the scattering and absorption coefficients. After the derivation of the theory, it will be shown how these coefficients can be exactly determined by reflection or transmission measurements.

3.1.2 Many-Flux Theory The many-flux theory is the most generalized version of the phenomenological theory. It is presented briefly here because it can aid in the better unterstanding of absorption and scattering phenomena, thus making for an easier route to the important special cases that will be treated later. The development begins with a coordinate system having position coordinate z and using specified, fixed polar angles y to describe the angular distribution of the radiation. By virtue of the spherical symmetry of the problem, two coordinates will be enough. This coordinate system is illustrated in Figure 3-1. Space is subdivided into conical segments, each labeled with the polar angle y; these bound regions of space shaped like ice-cream cones, each called a ªchannelº. In this way, all light traveling in direction y1 (in the positive z direction perpendicular to the plane bounding the layer) is in channel 1; light between y1 and y2 is in channel 2; and so forth. It is useful to select an even number n of channels so that the channels in the positive and negative z directions will be symmetrical. The radiative transfer problem is described by a differential equation that takes away from each channel the radiances that it emits into all other channels and adds to it the radiances that it receives from all other channels. If there are n channels, dLi s i1 L1 dz + si2 L2 dz ¼ + s in Ln dz

n P j1

s ij Lj dz

(3.1)

73

3.1 Introduction

Fig. 3-1. Many-Flux theory: Subdivision of directions in space into n = 22 channels.

where Li is the radiance in channel i, sij is the scattering coefficient from channel j into channel i, and dz is the path element in which the change described by equation (3.1) takes place. If j = i, the coefficient sjj is the total scattering from channel j into all other channels, including the absorption contribution kj in channel j: s jj = ± kj ±

n P i1

(1 ± dij) s ij (i = 1, 2, ¼ n)

(3.2)

where dij is the Kronecker delta (d = 1 for i = j, d = 0 otherwise). It also has to be considered that the contribution sij is negative if i 4 n/2, since the radiation is traveling opposite to the positive z direction. This situation can be handled by introducing a factor Zi = (n ± 2 i + 1)/ | (n ± 2 i + 1) | , which becomes ±1 for this case but is 1 otherwise. Now equation (3.2) can be rewritten as n dLi X Zi sij Lj dz j1

(i = 1, 2, ¼ n)

(3.3)

The coefficients Zisij = Sij form a matrix S = Sij, while the radiances Li make up a vector L = {L1, L2, ¼, Ln}, so that the fundamental vector differential equation can be written as dL SL dz

(3.4)

The general solution for L can be found in mathematics textbooks: Li

n P j1

Aij Cj elj z

(i = 1, 2, ¼ n)

(3.5)

74

3 How Spectra Depend on the Scattering and Absorption of Light

where the lj are the eigenvalues of the matrix S, the Aij are the eigenvectors Aj = {A1j, A2j, ¼, Anj} corresponding to the lj , and the Cj are constants of integration determined by the boundary conditions. The eigenvalues lk can also be obtained in a well-known way by solving the ªcharacteristic equationº (see also Section 2.4.2): n P j1

sij Ajk ± lk Aik = 0 (i = 1, 2, ¼ n)

(3.6)

This equation can be solved only with powerful computers, since simultaneous differential equations with i = 1, 2, ¼, n have to be integrated. So that the Li can be stated as functions of z, finally, and thus the reflectance R or the transmitance t obtained, the constants of integration Cj must still be eliminated. These may be governed by a great variety of boundary conditions. Conditions of special practical interest are those of the substrates beneath the layer, which have their own reflectance R0, or the change in radiance at the boundary of the layer, which is caused by the discontinuity in refractive index at the surface. These cases will be treated in depth further on, in connection with special phenomenological theories. It remains now to determine the scattering and absorption coefficients sij in this system. Equation (3.6) shows that they are included in the eigenvalues and eigenvectors and can be calculated from these with equation (3.5). If there are n channels, there are n2 coefficients sij ; by the symmetry of the channels in the halfspaces, sn±i+1, n±j+1 = sij for all i, j, leaving n2/2 coefficients.* With eight channels, for example, 64/2 = 32 coefficients are required, and this large number makes the many-flux theory unsuitable for practical use, because just as many measurements would have to be made on coatings in order to determine these coefficients. Another way to determine the coefficients is to specify the radiance distribution of the incident light in terms of appropriate functions of the polar angle. A method has been described in which the radiation distribution is represented by Legendre polynomials, but it remains limited to citations in the literature. Software is available to aid in calculations under the many-flux theory by numerically integrating differential equations (ªimplicitº solution). One difficulty arises in that initial values must be provided for the scattering and absorption coefficients. Of course, the coefficients from Mie calculations (see Chapter 5) could be used, although obtaining them is an intricate and laborious process, but convenient approximate formulas do exist. In summary, the theoretical value of the many-flux theory is great but its practical significance is virtually nil. We employ it here as a basis for understanding some portions of the phenomenological theory that are used in practice and thus serve as principles underlying the results obtained in this book. In particular, we will treat special four-flux, two-flux, and one-flux theories derived directly from the model or else through mathematical integration of the differential equations (ªexplicitº solution). We begin with surface phenomena. * These include n/2 distinct sjj, each of which contains one absorption coefficient.

3.1 Introduction

75

3.1.3 Surface Phenomena In order to determine the absorption and scattering coefficients from the phenomenological theory, it is necessary to use the reflectances prevailing in the interior of the layer under study. They can differ greatly from the reflectances measured at the surface, because of the discontinuity in refractive index that is usually present between air and medium.* When light enters the layer a part of it is reflected. This reflected portion (ca. 4 %) cannot take any further part in scattering phenomena occurring inside the layer, but just the same it can enter the measuring aperture of the colorimeter, thus contributing to the reflectance. An even stronger effect takes place inside the layer: much of the light scattered back from the interior is reflected into the interior again before exiting the layer, thus becoming involved in new scattering processes. The light reflected into the interior of the layer consists in part of totally reflected light, so that this fraction is large (ca. 60 %). This interaction is repeated, and in the end the net radiation leaving the layer governs the reflectance measured at the surface. In view of the relationships, measured reflectances must be ªsurface-correctedº before these values are put into the equations of the phenomenological theory. In other words, the external measured reflectance or reflection factor is converted to the corresponding internal quantities, which can then be subjected to phenomenological analysis. We then speak of ªcorrectedº reflectances or reflection factors; the formulas used have come to be known as the Saunderson correction. One of these formulas will now be derived. The formulas contain, along with the already known reflection coefficient r0 at the interface, two other coefficients. Accordingly, three constants figure in the derivation: r0 : reflection coefficient at the surface for directional light incident perpendicularly from outside r1 : reflection coefficient for light incident diffusely from outside r2 : reflection coefficient for light incident on the surface diffusely from inside the specimen These three coefficients can be calculated with Fresnel's equations (Table 3-1), provided the diffuse light is ideally diffuse, that is, obeys the Lambert cosine distribution. We impose the following condition in order to derive the formula: The layer must be opaque, ªinfinitely thickº as specialists say; furthermore, the light must be ideally diffuse before exiting from the surface, that is, its radiance must not depend on the angle. Naturally, all quantities are generally functions of wavelength. We begin by considering a high-gloss specimen and a 0/d measuring geometry (08 incidence angle, diffuse observation) of the photometer. The radiance of the in* For media in practical use (lacquers, paints, plastics), n & 1.5 is a good approximation to the refractive index.

76

3 How Spectra Depend on the Scattering and Absorption of Light

Table 3-1. Fresnel reflection ocefficients for light of directional and diffuse incidence. Refractive index n

Directional incidence: r0

Ideally diffuse incidence External reflection: Internal reflection: r1 r2

1.40 1.41 1.42 1.43 1.44 1.45 1.46 1.47 1.48 1.49 ? 1.50

0.02778 0.02894 0.03012 0.03131 0.03252 0.03373 0.03497 0.03621 0.03746 0.03873 0.04000

0.0769 0.0784 0.0800 0.0815 0.0830 0.0845 0.0860 0.0875 0.0890 0.0904 0.0919

0.528 0.536 0.543 0.550 0.557 0.564 0.571 0.577 0.584 0.590 0.596

1.51 1.52 1.53 1.54 1.55 1.56 1.57 1.58 1.59 1.60

0.04129 0.04258 0.04389 0.04520 0.04652 0.04785 0.04919 0.05054 0.05189 0.05325

0.0934 0.0948 0.0963 0.0977 0.0992 0.1006 0.1020 0.1035 0.1049 0.1063

0.602 0.608 0.614 0.619 0.624 0.630 0.635 0.640 0.645 0.650

cident light is denoted by L+0 , the internal reflectance by R . Then from Figure 3-2 we have immediately: + L++ 0 L0 (1 ± r0)

L±0

L+0 7 r0

L±1

L=1 (1 ± r2) L+0 (1 ± r0) (1 ± r2) R

L±2 .. .

L+0 (1 ± r0) (1 ± r2) R (r2 R )

+ L=1 L++ 0 7 R L0 (1 - r0) R

L+1 L=1 7 r2 L+0 (1 ± r0) R r2 L=2 L+1 7 R* L+0 (1 ± r0) R r2 R L+2 L=2 7 r2 L+0 (1 ± r0) R r22 R

L±n

L+0 (1 ± r0) (1 ± r2) R (r2 R )n±1 ? P 1 r0 1 r2 R ± + Li L0 r0 1 r2 R i0

3.1 Introduction

77

Fig. 3-2. Surface phenomena: The available radiances outside and inside the layer.

The radiance received by the instrument is the sum of all outward radiances L±i (written at right). The summation is done with the formula for an infinite geometric progression with first term (1 ± r0) (1 ± r2) R and r2 R as common ratio.* The externally measured reflectance R is the ratio between the radiation exiting and the radiation incident, that is (SL±i ) / L+0 : R r0

1

r0 1 r2 R 1 1 r2 R

r2 R r0 r2 R

r0 1

(3.7)

For practical application, this equation is mostly written for R*: R

R 1

r0 1

r0 r2 r2 R

r0

R 1

r0

r0 r2 1

R

(3.8)

The expressions on the right-hand sides are alternative forms. For the ideal white standard with a totally matte surface, R = 1, and so equation (3.7) implies that R is also equal to 1. This means that the correction formulas stated above apply in the same form to matte and glossy specimens. Now let us consider the measuring geometry d/0 (diffuse incidence, 08 observation). By similar arguments, the reflection factor R can be written as R a r0

1

r0 1 r1 R n2 1 r2 R

(3.9)

* More precisely, the reflectance Rg for L=1 would have to be for directional incidence while the reflectances Rdif for all subsequent Li would have to be for diffuse incidence. The slight difference between the two values is definitely of higher order in the context of this correction formula, so that for present puposes we can set Rg = Rdif = R .

78

3 How Spectra Depend on the Scattering and Absorption of Light

The fraction on the right-hand side differs from the one in equation (3.7) by a factor of n2 (1 ± r2) / (1 ± r1), which is equal to 1 for all refractive indices, as can easily be seen by examining Table 3-1. The term ar0 means that it is possible to design the instrument in such a way that the surface-reflection contribution is included (a = 1) or suppressed (a = 0). In the first case, equation (3.9) becomes equation (3.7); in other words, equations (3.7) and (3.8) also hold for the 0/d and d/0 measuring geometries. It can also be shown that the corresponding formulas for the 45/0 geometry are not much different from the ones already stated. This means that the correction formulas written out can be applied universally. For refractive index n = 1.5, Table 3-1 gives r0 = 0.04 and r2 = 0.6. Then the correction formulas become

R 0:04 R

0:384 R 0:36 R 0:04 1 0:6 R 1 0:6 R

R 0:04 R 0:04 0:384 0:6 R 0:04 0:96 0:6 1

(3.10) R

R 0:04 0:36 0:6 R

(3.11)

The R in equation (3.11) must be replaced by R + 0.04 when the measurement is performed with gloss trap (specular exclusion). These formulas have been used in practice for many years.

3.2

Four-Flux Theory

3.2.1 The Differential Equations and Their Integration The ªexplicitº solution of the four-flux theory to be discussed now is based on the model of Figure 3-3. An absorbing and scattering layer of thickness h is traversed by four radiances,* identified by arrow symbols and corresponding to the four channels: ± ± ± ±

Directional incident light: l + Directional light opposite to direction of incidence: l ± Diffuse incident light: L+ Diffuse light opposite to direction of incidence: L±

* The terminology and notation used in this chapter are based on those of DIN 1349; departures have been made whenever there is a possibility of confusion with quantities already defined.

3.2 Four-Flux Theory

79

Fig. 3-3. Four-Flux theory: The radiances, directional (l +, l ±) and diffuse (L+, L±), together with the boundary conditions.

Let z be the position coordinate in the direction of propagation. We now want to know the amount by which the individual radiances decrease or increase as the light traverses the short distance dz. As in the differential statement of Lambert's law, ±k'l + dz is taken away from l + by absorption (here k' is the absorption coefficient for directional light). If scattering is present, l + also loses ±s+l + dz scattered forward and ±s± l + dz scattered backward (s+ and s± are the forward and backward scattering coefficients for directional light). Thus we can write dl + ± (k' + s+ + s± ) l + dz

(3.12)

In distinction to the absorbed fraction, however, the two scattered components do not disappear without trace; they must later be added into the respective radiances for diffuse light. Similarly, in the case of directional light propagating in the opposite direction, we can write for l ± ± dl ± ± (k' + s+ + s ± ) l ± dz

(3.13)

The minus sign on dl ± takes care of the fact that l ± is in the direction opposite to the positive z direction. We now consider the radiance L+ of diffuse light. First, similarly to l +, it loses the absorbed component ±KL+ dz and the scattered component ±SL+ dz (where K is the absorption coefficient and S the scattering coefficient for diffuse light). Further, however, the light scattered from the l + and l ± beams must now be added to L+; these are s+l +dz and s± l ± dz respectively. Finally, the scattering SL±dz from the opposite diffuse light must be added as well, so that dL+ s+ l + dz + s ± l ± dz ± (K + S) L+ dz + SL ± dz

(3.14)

±dL ± s ± l + dz + s+ l ± dz ± (K + S) L ± dz + SL+ dz

(3.15)

and similarly

The coefficients and their definitions are written out once again: k0

1 dl l dz

abs

;

s

1 dl l dz

sca ; forw

s

1 dl l dz

sca back

(3.16)

80

3 How Spectra Depend on the Scattering and Absorption of Light

K

1 dL L dz

abs

;

S

1 dL L dz

sca

(3.17)

By the rule stated at the end of Section 3.1.2, the four-flux theory would require 42/2 = 8 coefficients, of which 4/2 = 2 contain absorption coefficients. The reduction of the remaining six scattering coefficients to three comes about because, in three cases, there is no radiative transfer by scattering: from l + to l ± from L+ to l ± from L± to l +. The associated scattering coefficients are therefore equal to zero. The following abbreviations are now introduced into the equations: a1

K S

(auxiliary variable)

m k' + s+ + s ± (attenuation coefficient)

(3.18)

(3.19)

The system of differential equations then becomes dl dz

m l

dl ml dz

(3.20) (3.21)

dL s+ l + + s ± l ± ± aSL+ + SL ± dz

(3.22)

dL ±s ± l + ± s+ l ± + aSL ± ± SL+ dz

(3.23)

This coupled system of four simultaneous differential equations for the functions l + (z), l ± (z), L+ (z), and L± (z) must now be decoupled and integrated. It will be sufficient to integrate out to the boundary conditions. Thus the integrals of the first two equations can be written immediately. With l + (0) l0+ ;

l ± (h) lh±

(3.24)

l ± lh± e±m (h±z)

(3.25)

we get l + l0+ e±mz ;

3.2 Four-Flux Theory

81

The film thickness h then becomes l + (h) lh+ l0+ e±mh ;

l ± (0) = l0± lh± e±mh

(3.26)

The first two differential equations have now been decoupled and integrated by themselves. These solutions are needed for the integration of the last two equations (3.22) and (3.23). In order to decouple the remaining simultaneous system, one of the two equations must be differentiated; we choose equation (3.22). The derivatives of the directional radiances l + and l ± are replaced by expressions (3.20) and (3.21); dL+/dz and dL±/dz, by espressions (3.22) and (3.23). Using the partial integrals in equation (3.26) along with b

p a2 1 (auxiliary variable)

(3.27)

we obtain finally d2 L b2 S2 L+ ± l0+ [Ss ± + (m + a S) s+ ] e±mz ± dz2 ± lh± [Ss+ ± (m ± aS) s ± ] e±m (h±z)

(3.28)

The homogeneous equation associated with this second-order differential equation has the well-known exponential solution with two constants of integration. For the inhomogeneous equation, two terms with the exponents ±mz and ±m (h ± z) must be considered, so that the solution becomes L+ B1 ebSz + B2 e±bSz ± l+0 p e±mz ± lh± q e±m (h±z)

(3.29)

Here B1 and B2 are the two constants of integration of the second-order differential equation; the boundary conditions will be applied later in order to eliminate these. On the other hand, p and q are fixed in value and can therefore be found immediately by comparing coefficients with differential equation (3.28). For this purpose, expression (3.29) is substituted in (3.28), an the other hand, equation (3.29) is differentiated twice. The comparison of coefficients then gives

p q

Ss m aS s K k0 s s s S s m2 b2 S2 k0 s s 2 K K 2 S Ss

m m2

aS s K k0 s s s S s b2 S2 k0 s s 2 K K 2 S

Accordingly, equation (3.29) is already the general integral.

(3.30) (3.31)

82

3 How Spectra Depend on the Scattering and Absorption of Light

The next step is to impose the boundary conditions on the general integral and its first derivative. The boundary conditions themselves are obtained from the cases z = 0 and z = h for L+ and dL+ / dz; the starting differential equation (3.22) is employed for the latter. We then have L+ (0) B1 + B2 ± l+0 p ± lh± q e±mh L+0

(3.32)

L+ (h) B1 ebSh + B2 e±bSh ± l0+ p e±mh ± lh± q L+h

(3.33)

dL dz

z=0

B1 bS ± B2 bS + l0+ mp ± lh± mq e±mh s+ l0+ + s ± l0± ± aSL0+ + SL0±

dL dz

z=h

(3.34)

B1 bS ebSh ± B2 bS e±bSh + l0+ mp e±mh ± lh± mq + ± ± ± s+ l+ h + s lh ± aSLh + SLh

(3.35)

We recall that l0+, lh±, L+0 , and L±h are given (as incident radiances; see Fig. 3-3). The equation system (3.32)±(3.35) thus contains four further unknowns, B1, B2, L+ h , and ± and L L±0 , which can now be determined from the four equations. Only L+ h 0, the quantities sought, are of interest here. The solutions are L+h l0+ P + lh± Q + L0+

b sinh x + Lh± A A

(3.36)

L0± l0+ Q + lh± P + L0+

sinh x b + Lh± A A

(3.37)

where we have introduced the notation* x bSh ; A a sinh x + b cosh x P

(3.38)

1 (bp + q e±mh sinh x) ± p e±mh A

(3.39)

1 ( p sinh x + bq e±mh) ± q A

(3.40)

Q

* P and Q, unlike p and q, are not constants of the material, since they depend on the film thickness h.

3.2 Four-Flux Theory

83

Equations (3.36) and (3.37) together with (3.26) give the radiances for a layer irradiated from both sides. Interchanging l0+ with lh± and L+0 with L±h takes each equation into the other. This is a necessary condition, because the experimental radiances L+h and L±0 as well as lh+ and l0± must be invariant to reversal of the sides of the layer.

3.2.2 Transmittance and Transmission Factor The most general configuration that can be imagined for the measurement of transmission is described by the following model: ªMixedº irradiation (i. e., directional and diffuse radiation) on the incidence side, observation of total radiation (i. e., directional and diffuse once again) on the observation side. The corresponding formula for the transmittance in the interior of the layer* is as follows (see Fig. 3-3): t

lh L h l0 L 0

(3.41)

If diffuse light is not recorded on the measurement side, L+h vanishes and t is replaced by the transmission factor T. In the most general model, the following equation is obtained by merging (3.26) and (3.36) and the fact that no light is incident on the specimen from the observation side (i. e., lh± = L±h = 0): t (1 ± g) (P + e±mh) + g

b A

(3.42)

where g = L+0 /(l0+ + L+0 ) is the diffuse fraction and 1 ± g = l0+ /(l0+ + L+0 ) the directional fraction of the net incident light. This equation immediately yields the case of irradiation with directional (quasiparallel) light if g is set equal to 0: tg P + e ±mh

(3.43)

This is identical to the equation stated by Ryde if we set k' = 0, for Ryde did not introduce a second absorption coefficient. In the same way, for irradiation with diffuse light (g = 1), tdif

b b A a sinh x b cosh x

(3.44)

* In general, t* = t / t0 (where t0 is the blank value). If there is much scattering in the layer, however, it may become necessary to apply the Saunderson corrections, equation (3.11), writing t in place of R.

84

3 How Spectra Depend on the Scattering and Absorption of Light

This is the transmittance in the Kubelka-Munk theory. The same equation is also obtained, incidentally, if the substitutions s+ = 0, s± = S, and k' = K are made in equation (3.43). This would mean that, as far as scattering and absorption in the interior of the medium are concerned, there is no difference between directional and diffuse radiation: The substitutions lead to p = 1 and q = 0 from equations (3.30) and (3.31), so that equation (3.43) actually does become (3.44). In reality, however, s± cannot be identical to S nor k' with K since the mean path length through the layer for diffuse light is longer than the film thickness. As a consequence, more light is scattered and absorbed than from a directional beam perpendicular to the layer, and this fact must affect the numerical values of the scattering and absorption coefficients. The mean path length of ideally diffuse radiation through a layer is, according to Kubelka, twice the film thickness (corresponding to a incidence angle of 608); hence S and K are about twice as large as s± and k' respectively. Two other configurations of measuring geometries are possible and must be considered. On the irradiation side, suppose that incidence is solely directional and perpendicular to the layer surface, while on the observation side only the quasi-perpendicular directional radiation component is measured. Then what is measured is the transmission factor T*r , which is given directly by equation (3.26): Tr

lh e l0

mh

(3.45)

The second possibility is the transmittance t g , which is obtained if irradiation is directional and the directly transmitted beam lh+ is excluded, so that only the remaining diffuse light is measured. The formula for this case is t g tg

Tr P

(3.46)

All the important transmittance equations for the four-flux theory have now been derived. We need only add the equations obtained by examining the two important extreme cases ± Absorption only (no scattering) ± Scattering only (no absorption) For the ªabsorption onlyº case, we have k', K 4 s+, s±, S; a ? b ? K/S ? ?; m ? k'; and p ? q ? 0. The general tansmittance is then tabs 1

g e

k0 h

ge

Kh

(3.47)

while the transmittance and transmission factor for directional irradiation are given by e tabs;g Tabs;r

k0 h

(3.48)

3.2 Four-Flux Theory

85

and the transmittance for diffuse irradiation by tabs;dif e

Kh

(3.49)

Since there is no incident diffuse light in the case of directional irradiation, the transmittance after exclusion of directional radiation on the measurement side is, as = 0. expected, t abs;g = tabs;g Tabs;r Equation (3.48) is the well-known transmission factor from Lambert's law. In the second extreme case, ªscattering onlyº, s+, s±, S 4 k', K; therefore a ? 1, b ? 0, m ? u = s+ + s±. For p and q, we obtain p ? u = (S + s+)/(s+ + s±) and q ? w = (S ± s±)/(s+ + s±), with u ± w = 1. Taking the limit gives the following for the general transmittance: tsca 1

g

1 w 1 e 1 Sh

uh

1 1 Sh

g

(3.50)

whence, for directional irradiation, tsca;g

1 w 1 e 1 Sh

uh

(3.51)

for diffuse irradiation, tsca;dif

1 1 Sh

(3.52)

while the transmission factor is given by e Tsca;r

uh

(3.53)

and the transmittance after exclusion of directional radiation by t sca;g tsca;g

Tsca;r

1 w 1 e 1 Sh

uh

e

uh

(3.54)

The following auxiliary variables have been used here: u s s ;

w

S s s s

(3.55)

All the equations derived in Section 3.2.2 are summarized and related to one another by the transmission function pedigree of Figure 3-4.

86

3 How Spectra Depend on the Scattering and Absorption of Light

Fig. 3-4. Pedigree of the transmission function.

3.2.3 Reflectance and Reflection Factor As Figure 3-3 shows, the reflectance in the interior of the layer for irradiation with both types of light is given by R

l0 L0 l0 L 0

(3.56)

In the model that serves as basis for the present discussion, the absorbing and scattering layer is applied directly on a substrate. This kind of model is of greatest importance in practice, since it describes lacquer and paint coatings. Because the substrate generally has its own reflection properties, these must be taken into account when the equations of Section 3.2.1 are employed. The intrinsic reflection of the substrate will, in general, give rise to diffusely reflected light, although specularly reflecting substrates are increasingly significant (e. g., for transparent lacquers). For the specular case, the radiance reflected from the substrate is (see Fig. 3-5). lh Rr;0 lh Rr;0 l0 e

mh

(3.57)

3.2 Four-Flux Theory

87

Fig. 3-5. Reflection with substrate.

Here Rr,0 is the reflection factor of the specular substrate; the subscript r identifies the 0/0 geometry (i. e., the angles of incidence and reflection are both 08), while the * identifies the reflection factor as an internal one. If there is no specular reflection, however, only diffuse radiation comes from the substrate; it consists of two components, the first Rg,0 7 l +h originating in directional irradiation and the 7 L +h in diffuse irradiation (here Rg,0 and Rdif,0 are the reflectances of second Rdif,0 the substrate for directional and diffuse irradiation, respectively; see Fig. 3-5). The definition of reflectance in equation (3.56) requires that all the radiation ± directional and diffuse ± must be received on the observation side. The same holds, of course, for the reflectance of the substrate. Accordingly, if specular reflection is present along with diffuse reflection, it must be recalled that the specular reflection has already been taken care of by equation (3.57), so that Rr,0 7 lh+ must be subtracted, else it will be counted twice. The radiance diffusely reflected by the substrate is then Lh± (Rg,0 ± Rr,0) l+h + Rdif,0 L+h

(3.58)

From this with equations (3.26) and (3.36), we obtain an expression containing L±h twice; solution for L±h yields Lh

A A

l0

Rdif ;0 Rg;0

sin x Rr;0 e mh

Rdif ;0 P

Rr;0 Q e mh

L 0

Rdif ;0

b A

(3.59)

Now, with the aid of equation (3.56) and the use of equations (3.26), (3.37), and (3.59), we immediately obtain the reflectance for the general model (parallel and diffuse irradiation):

88

3 How Spectra Depend on the Scattering and Absorption of Light

R

1 g AQ R R R A Rdif ;0 sinh x " # 2 sinh x b g Rdif ;0 A A Rdif ;0 sinh x A

(3.60)

In this expression we have used the notation R Rr;0 e

mh

R Rg;0 b e

A P e

mh

mh

Rdif ;0 bP

R Rr;0 Rdif ;0 e

mh

bQ

b

(3.61)

Q sinh x P e

mh

(3.62)

sinh x

(3.63)

Hence, with g = 0, we have the following for irradiation with directional light: Rg

AQ R R R A Rdif ;0 sinh x

(3.64)

Taking g = 1 leads to the reflectance for irradiation with diffuse light; this equation can be transformed with the easily derived relation sinh2 x ± b2 = A (a sinh x ± b cosh x). Since cosh x/sinh x = coth x, Rdif

1

Rdif ;0 a b coth x a Rdif ;0 b coth x

(3.65)

This is the reflectance in the Kubelka-Munk theory, which we will use frequently. Wholly similarly to the transmission factor Tr , a reflection factor Rr applicable to directionally reflected light can be defined. This is nonzero only when Rr,0 = 0, that is, when there is a specularly reflecting substrate: Rr

l0 Rr;0 e l0

2mh

(3.66)

With a measuring setup that can exclude directional reflected light, a reflectance R g = Rg ± R r can be obtained similarly to the transmittance: R g

A

1 Rdif ;0 sinh x

AQ R

Rr;0 A e

2mh

R R Rr;0 Rdif ;0 e

2mh

sinh x

(3.67)

89

3.2 Four-Flux Theory

As in Section 3.2.2, there are two extreme cases. Let us first consider ªabsorption onlyº. Taking the limit yields the following for the general reflectance: Rabs (1± g) [Rr,0 e±2k'h + (Rg,0 ± Rr,0) e±(k'+K)h] + gRdif,0 e±2Kh

(3.68)

for directional irradiation, Rabs,g Rr,0 e±2k'h + (Rg,0 ± Rr,0) e±(k'+K)h

(3.69)

for diffuse irradiation Rabs,dif Rdif,0 e±2Kh

(3.70)

With an appropriate measuring setup, we can again split into the reflection factor Rabs,r Rr,0 e±2k'h

(3.71)

and the reflectance after exclusion of directional radiation R abs,g (Rg,0 ± Rr,0) e±(2k'+K)h

(3.72)

Taking the limit for the second extreme case, ªscattering onlyº, leads to the general reflectance Rsca

1

g

Qsca 1 Sh R sca R sca R sca

1

Rdif ;0 Sh

g

1 Rdif ;0 Sh Rdif ;0 1 Rdif ;0 Sh 1

1

(3.73)

where the barred expressions are somewhat simplified: R sca Rr,0 e±uh [(1 + Sh) (Psca + e±uh) ± 1]

(3.74)

R sca Rg,0 e±uh + Rdif,0 (Psca ± Qsca Sh)

(3.75)

R sca Rr,0 Rdif,0 e±uh [Qsca ± (Psca + e±uh) Sh]

(3.76)

and Psca

1 [(1 + w) (1 ± e±uh) ± Sh e±uh] 1 Sh

(3.77)

Qsca

1 [Sh ± w (1 ± e-uh)] 1 Sh

(3.78)

The symbols u and w have the same meanings as in equation (3.55).

90

3 How Spectra Depend on the Scattering and Absorption of Light

From the above, we immediately get the expressions for directional light Rsca;g

1

1 Qsca 1 Sh R sca R sca R sca Rdif ;0 Sh 1

and for diffuse light Rsca;dif

1 Rdif ;0 Sh Rdif ;0 1 Rdif ;0 Sh 1

(3.79)

(3.80)

as well as for the reflection factor Rsca;r Rr;0 e

2uh

(3.81)

and the reflectance after exclusion of the directional component: R sca;g

1 Rdif ;0 Sh

1

Rr;0 e

2uh

1

Qsca 1 Sh R sca R sca R sca

1 1

Rdif ;0 Sh

(3.82)

3.2.4 Limiting Cases of Reflection The following limiting cases are of practical interest: ± ± ± ±

The substrate exhibits specular reflection only The substrate exhibits diffuse reflection only The substrate is black The layer is opaque (ªinfinitely thickº)

1) Substrate with exclusively specular reflection The equations for this limiting case are obtained by setting the reflectances and reflection factors of the substrate in equation (3.64) equal (i. e. Rg,0 = Rdif,0 = Rr,0); the equation for directional irradiation is then Rspr;g

1 A

Rr;0

bP

sinh x

hAQ Rr;0 fA e

Q sinh x Rr;0 e

mh

bQ

mh

P e

P e

mh

mh

sinh xgi

(3.83)

For diffuse irradiation, equation (3.65) remains unchanged except that Rr,0 appears in place of Rdif,0. The reflection factor of equation (3.66) does not change either. For the reflectance after exclusion of directional reflected light, we then have

91

3.2 Four-Flux Theory

R spr;g

1 Rr;0

A

Rr;0 e

sinh x mh

bQ

fAQ Rr;0 P A e

mh

b

Q sinh x

P sinh xg

(3.84)

The equations for the two extreme cases, ªabsorption onlyº and ªscattering onlyº, will not be written out here, because they can be obtained effortlessly from equations (3.68) to (3.82) by setting Rg,0 = Rdif,0 = Rr,0. 2) Substrate with exclusively diffuse reflection These equations are derived by setting Rr,0 equal to zero in the respective formulas. First, again, the case of directional irradiation: Rdfr;g

A

1 AQ Rg;0 b e Rdif ;0 sinh x

Qb

mh

Rdif ;0 bP

Rg;0 e mh Rdif ;0 P A Rdif ;0 sinh x

Q sinh x (3.85)

Here too, the case of diffuse irradiation contains nothing not considered in equation (3.65), since that formula does not show Rr,0 at all. Because no directional light can be excluded, the reflectance has the trivial solution Rdif,r = 0, and R dif,g is as in equation (3.85). Once more, the equations for the extreme cases are omitted, being easily derivable from the respective formulas with Rr,0 . 3) Black substrate Now all the reflectances and reflection factors of the substrate are zero. From equation (3.64) with Rr,0 = Rg,0 = Rdif,0 = R = R = R = 0, we have the following; for directional irradiation Rg;b Q

(3.86)

(this is the reflectance in the Ryde theory if k' = 0), and for diffuse irradiation Rdif ;b

1 a b coth x

(3.87)

Again Rr,b = 0, so that the expression for R g,b is the same as equation (3.86). As in the previous derivations, the extreme cases are uninteresting up to ªscattering onlyº. For directional irradiation we have

92

3 How Spectra Depend on the Scattering and Absorption of Light

Rb=sca;g Qsca

1 Sh 1 Sh

and for diffuse irradiation Rb=sca;dif

w 1

Sh 1 Sh

e

uh

(3.88)

(3.89)

4) Infinitely thick layer These important equations are obtained by taking the limit as h ? ?, so that equation (3.86) leads to the following for directional irradiation: Rg;? p a

b

q

(3.90)

Fig. 3-6. Pedigree of the reflection function.

3.2 Four-Flux Theory

93

and equation (3.87), with a2 ± b2 = 1, gives for diffuse irradiation Rdif ;? a

b

(3.91)

The extreme cases yield trivial solutions. All the equations derived in Section 3.2.3 are summarized and related to one another by the reflection function pedigree of Figure 3-6.

3.2.5 Determination of the Coefficients Practical use of the formulas stated in the preceding sections requires that the absorption coefficients k', K and scattering, coefficients S, s+, s± appearing in them be determinable by reflection or transmission measurements. The problem is easy to solve, because that determination can be carried out in two steps. The measurements, labeled with ªdifº contain only the coefficients K and S; these are the typical optical parameters of the Kubelka-Munk theory, to be described in the next section along with methods for their determination. Thus K and S must always be determined first, since these coefficients are assumed known when k', s+, and s± are determined. Accordingly, three coefficients remain to be found, so that three equations have to be employed. The following measurements (all for directional irradiation) are available for the purpose: ± Rr , the reflection factor for (quasi) 0/0 geometry with a specularly reflecting substrate having reflection factor Rr,0 ± Rg,? , the reflectance of the infinitely thick layer ± Rg,b , the reflectance over a black substrate ± Rg,w, the reflectance over a white substrate having reflectance Rg,0w ± Tr, the transmission factor measured with (quasi) 0/0 geometry ± tg , the transmittance Any three of these measurable quantities can be used in determining k', s+, and s±. We will distinguish between determinations based on reflection measurements and those based on transmission measurements. The equations needed are derived from the formulas of Sections 3.2.2 and 3.2.3. All the quantities from the Kubelka-Munk theory can ± because they are (abbreviated terms on the right hand side) known ± be substituted in these formulas. They are tdif Rdif ;1

b t A a b R1

Rdif ;b

sinh x R2 A

(3.92) (3.93) (3.94)

94

3 How Spectra Depend on the Scattering and Absorption of Light

Rdif ;0w R3

(3.95)

These values can either be obtained by direct measurement on black and white drawdowns or calculated from K and S (which are assumed to be known) and h. The notation and relations stated previously are used: K S s p K K 2 1 b a 2 S S x bSh

a 1

A a sinh x b cosh x Special value is attached to the measurement of the film thickness h, which must be done with great care because the error in h strongly influences the accuracy of the calculated absorption and scattering coefficients. It is also vital that the layers on the black and white substrates be equally thick; this can be achieved with black and white glass plates in which the white and black portions are joined together without a ªstepº. The reflection factor Rr , on the other hand, can be measured on a drawdown having a different film thickness hR on the specularly reflecting substrate. 1 Determination of k ', s+, and s± from reflection measurements 1.1 From Rr , Rg,?, Rg,b (and Rr,0) By equations (3.45) and (3.66), Tr

e

mh

Rr Rr;0

!

h 2hR

T

(3.96)

where hR is the film thickness over the specular reflective substrate; also, by equations (3.86) and (3.90) Rg;1 1 p R1 1 q R1 p

tT tT

Rg;b R2

Rg;1

(3.97)

The auxiliary variables p and q are linked to the coefficients by equations (3.30) and (3.31). If these are solved for s+ and s±, the following formulas are obtained: s p m aS qS s pS q m aS

(3.98) (3.99)

95

3.2 Four-Flux Theory

The quantity m needed here follows immediately from equation (3.96): m so that by equation (3.19)

1 1 ln h T

(3.100)

k' m ± (s+ + s ± )

(3.101)

The three coefficients have thus been determined. 1.2 From Rr , Rg,b , Rg,w (and Rg,0w): If Rg,? is difficult of access because of problems in achieving a thick layer, a determination based on a layer over black and white is also possible. The equation for Rg,b is now supplemented by equation (3.85) for Rg,w , specifically the expression following the second equality sign; then, with Q = Rg,b , p and q are obtained as follows from equation (3.86): p

R2 TRg;b C 1

R22 T t

T 1

tT tT

;

q

p R2 Rg;b 1 tT

(3.102)

with T as above. Here 1 C R3

1 R t g;w

Rg;b 1

R2 R3

Rg;0w T

(3.103)

With m as defined previously and the formalism of 1.1, we finally obtain k', s+, and s±. 1.3 From Rg,?, Rg,b , Rg,w (and Rg,0w) This variant does not involve a drawdown on a specularly reflecting substrate. The formulas used are again equations (3.86), (3.90), and (3.85), the expression after the first equality sign in equation (3.85) being taken. The term bP ± Q sinh x is transformed, and then q is substituted with Rg,? from equation (3.90). Solving for p leads to an expression that has the same denominator as the formula for p in equation (3.97). By setting the two expressions equal, we obtain directly a formula for T containing no quadratic expressions: T

R1 Rg;w

Rg;b R2 R3 Rg;1 Rg;w R3 Rg;1 t R1 Rg;0w R3 Rg;1

Rg;b

(3.104)

The subsequent analysis is most easily done with equations (3.97) to (3.101).

96

3 How Spectra Depend on the Scattering and Absorption of Light

2 Determination of k', s+, s± from transmission measurements Initially, only T r from equation (3.45) and t g from (3.43) are available for the determination. But a third equation is needed if the three coefficients are to be obtained; this can be derived from a further transmission measurement, t^ g with a doubled film thickness h. In the case of suspensions, this involves no difficulties; we simply take a cell with twice the thickness. It is possible, however, even for pigmented coatings, provided these are plastic wafers or self-supporting films (films not applied on a substrate ± but optical contact is a special concern here, see Section 3.3.3). All quantities relating to the doubled film thickness are identified by ^ ; then b (3.105) t^ dif t^ A^ R^ dif ;b

sinh 2x R^ 2 A^

(3.106)

Where = a sinh 2 x + b cosh 2 x. Now, by equation (3.43) for t g and t^ g p

R^ 2 T tg R^ 2 T t

T T

R2 ^tg T 2 R2 ^t T 2

q

1 t R2 T g

T

p t

T

(3.107)

If p, q, and T are known, we can go on as in 1.1. We have thus shown how k', s+, and s± can be determined without an excessive degree of complication.

3.3

Kubelka-Munk Theory

3.3.1 Significance and Formalism The two-flux theory is today the most important and successful specialization of the phenomenological theory. It owes its widespread acceptance to three properties: ± It involves only two optical constants (K and S) ± It is easy to work and lends itself to computer programming ± Over a period of decades, it has proved suitable for the description of practical problems.

3.3 Kubelka-Munk Theory

97

The first two of these qualities have their source in the fact that the theory is formulated quite simply, on the basis of the following assumptions: ± Ideally diffuse radiation distribution on the irradiation side ± Ideally diffuse radiation distribution in the interior of the layer ± No consideration of surface phenomena resulting from the discontinuity in refractive index When deviations from the Kubelka-Munk theory are seen in application to practical problems, the reason is nearly always that one or more of these assumptions have been neglected*. The third assumption drops out when the Saunderson corrections are employed, as has become indispensable for most applications today. We have already encountered the basic equations of Kubelka and Munk in deriving the four-flux theory. Because they are so important, however, they are written out explicitly here, except that the subscript ªdifº has been omitted (since there is no radiation other than diffuse). Transmittance: General:

t

b a sinh b S h b cosh b S h

Absorption only:

tabs e

Scattering only:

Kh

(3.110) s. (3.52)

1 R0 a b coth bS h a R0 b coth b S h

(3.111) s. (3.65)

Reflectance: R Absorption only:

(3.109) s. (3.49)

1 1 Sh

tsca

General:

(3.108) s. (3.44)

Rabs R0 e

Scattering only: Rsca

1 1

2Kh

R0 S h R0 R0 S h 1

(3.112) s. (3.70) (3.113) s. (3.80)

The symbols here have the following meanings: K and S are the absorption and scattering coefficients defined as in equation (3.17); R0 is the reflectance of the substrate; the auxiliary variables a and b are defined as in equations (3.18) and (3.27), a = 1 + K / S and b = (a2 ± 1)1/2 ; and finally h is the film thickness. * In such cases, many-flux theories may be helpful; see also the discussion in Section 7.2.3.

98

3 How Spectra Depend on the Scattering and Absorption of Light

3.3.2 Limiting Cases of Reflection Because equations (3.111) to (3.113) also hold for substrates with specular reflection only and with diffuse reflection only, there are just two limiting cases of the reflectance to be treated here: ± Reflectance on black substrate ± Reflectance of the opaque (ªinfinitely thickº) layer To obtain the reflectance on a black substrate, we use the equations from Section 3.3.1, setting R0 equal to zero. General: Rb

1 a b coth b S h

Scattering only: Rsca;b

Sh 1Sh

(3.114) s. (3.87) (3.115) s. (3.89)

For the ªabsorption onlyº case, we get the uninteresting trivial solution Rabs,b. = 0 The easiest way to obtain the reflectance of the infinitely thick layer is to take equation (3.114) to the limit as h ? ?. Then coth bSh ? 1, and with the relation a2 ± b2 = 1 implied by equation (3.27),

R1 a

K b1 S

s K K 2 S S

(3.116) s. (3.91)

Solving for K / S, we obtain the famous ªKubelka-Munk functionº FKM : K 1 R1 2 :FKM 2 R1 S

(3.117)

(The extreme cases ªabsorption onlyº and ªscattering onlyº lead to trivial solutions: Rabs,? = 0 and Rsca,? = 1) For didactic purposes, it may well be desirable to derive the Kubelka-Munk function directly from the differential equations. The typical equations for the Kubelka-Munk theory are obtained from equations (3.22) and (3.23) by setting the directional radiances l + and l ± (Fig. 3-3) equal to zero. Dividing the first equation by SL+ and the second by SL± and using L± /L+ = R , one gets

3.3 Kubelka-Munk Theory

1 1 dL S L dz

99

K 1 R S

1 1 dL K 1 dz S L S

1 R

The ªinfinitely thickº layer is characterized by the fact that a further increase in film thickness does not change the reflectance. Thus the percent changes in radiance per unit increase of film thickness in the incidence direction (1/L 7 dL+/dz) and opposite to the incidence direction (1/L± 7 dL±/dz) must be exactly equal. If both right-hand sides are set equal and the equation is solved for K / S, the limit as R ?R? directly yields the Kubelka-Munk function (3.117). Equation (3.117) is the most important statement of the Kubelka-Munk theory and the most often used of all formulas in the theory. It links the reflectance of the infinitely thick layer with the absorption and scattering coefficients K and S governing the optical process, making R? directly dependent on the ratio of the absorption to the scattering coefficient (and not on the value of either). The equation is also available in tabular form; it has found widest use where information about the ratio of absorption to scattering is to be extracted from reflection measurements. Figure 3-7 is a plot of the Kubelka-Munk function. Typical features are the steep drop from very large values at low reflectance and the branch decreasing slowly toward zero as the reflectance approaches 1. If the variables are interchanged, the reflectance then declines rapidly from unity at low K / S; this fact accounts for the well-known high sensitivity of white specimens to contamination.

Fig. 3-7. The Kubelka-Munk function FKM (R*?).

100

3 How Spectra Depend on the Scattering and Absorption of Light

Fig. 3-8. The function ln FKM (R*?).

If the logarithm of FKM is plotted versus reflectance, the curve of Figure 3-8 results. As can be seen, there is a wide reflectance range in which the curve has a quasilinear shape. The equation for this straight line can be obtained by calculating the point of inflection and the inflectional tangent of the curve. A better approximation can be found by a linear regression calculation in the region of interest: ln F A ± BR?

or

log F A10 ± B10 R?

(3.118)

where A 1.68 ; B 6.182 ; A10 0.7296 ; and B10 2.685 for 0.13 ^ R? ^ 0.73 (i.e. 0.09 ^ Rin,? ^ 0.54).* The values of the coefficients are somewhat dependent on higher accuracy in the lower or the upper part of the range. The values stated above represent a good approximation over the entire region. Between R? = 0.20 and 0.65, the deviation from the true F value is less than 3 %, coming to exceed 20 % only at the bounds cited above. What appears to be a bothersome restriction on the use of the approximation formula is actually not much of a hindrance: the requirements on the accuracy of measurement in the determination of F already restrict the field in which the measurements must be done. Let us consider the relative error of determination of F reflection measurements:

* The subscript ªinº refers to measurement including surface reflection (see Section 6.1.2).

3.3 Kubelka-Munk Theory

d ln F dF dR dR dR F dR

1 R 1 0:6 R dR 1 R R 0:04

101

(3.119)

As Figure 3-9 shows, given a fairly realistic measurement error of dR = 0.001, the relative error of F is smaller than 1% only when measurements are performed with 0.2 ^ Rin,? ^ 0.75 (i. e., 0.33 ^ R? ^ 0.88). The measurement interval does not expand to 0.1 ^ Rin,? ^ 0.88 (i. e., 0.14 ^ R? ^ 0.95) until a 2 % error (dF / F) is allowed. Here we have a reflection counterpart to the spectroscopists' old rule, ªFor extinction measurements, the transmission must always be between 8 and 80 % (or the decadic extinction between 1 and 0.1).º

Fig. 3-9. Relative error of the Kubelka-Munk function F (Rin,?) for a measurement error dR = 0.001.

102

3 How Spectra Depend on the Scattering and Absorption of Light

3.3.3 Determination of the Absorption and Scattering Coefficients The classical method of determining the coefficients is to measure directly the reflectance R ? of the infinitely thick layer and, from this, determine, after Saunderson correction, a and b. Equations (3.116) and (3.27) imply that 1 a 2 ba

1 R1 R1 1 1 R1 2 R1

R1

(3.120)

K and S can be obtained by solving equation (3.111) for S:

S

1 1 Arcoth bh

a R R0 R R0 ; K S a b R R0

1

(3.121)

This procedure requires two coatings: the infinitely thick layer and a coating with thickness h on an arbitrary substrate with reflectance R0. The measured reflectances on these two coatings are R? and R respectively. Accordingly, only three measurements in all (including that of the film thickness h) are needed in order to determine K and S. A second method is to determine the reflectances Rb and Rw of layers of equal thickness h on black and white substrates having known reflectances R0b and R0w . Accordingly, coth x can be eliminated from the two equations (3.111), written for Rb and Rw . The result is an equations for a:

a

1 Rw R0w Rb R0b 1 Rb R0b R0w 2 Rb R0w Rw R0b

Rw

(3.122)

Once a has been obtained, b is also known from equation (3.27). Then, from equation (3.121), K and S follow (as above) if R and R0 are replaced by the pair Rw , R0w or Rb, R0b . The classical method is generally more accurate, as an error analysis on white pigments has shown. Often, the reflectance of the black substrate R0b can be set equal to zero, as described in the preceding section. Equations (3.122) and (3.121) then simplify to

3.3 Kubelka-Munk Theory

Rb R0w Rw Rw Rb R0w

1 a 2 S

1 1 a Rb Arcoth b Rb bh

103 (3.123) (3.124)

Another way to determine K and S is with two transmission measurements, provided the film thickness is doubled for the second measurement. With suspensions, this can be done by using a cell with twice the cell thickness; with wafershaped plastic specimens, by laying one wafer on another. ªOptical contactº is a matter of concern here; it can be insured, for example, by applying an oil film to the surfaces and pressing the two wafers together. Because of the double film thickness there are two measured values t and t^ available to serve as arguments in the respective equations, giving bSh = x in one case and 2 bSh = 2 x in the other. The auxiliary variables a and b are thus not affected by doubling the thickness, since they do not depend on the thickness. The addition theorems for hyperbolic functions make it possible to obtain simple relations for this case: a

1 2

1 t

1 t

t t t

Here we have used the abbreviated notation r 1 1 t t2 t^

(3.125)

(3.126)

The following equation can be used to determine S:

S

1 Arsinh bt bh

(3.127)

104

3 How Spectra Depend on the Scattering and Absorption of Light

3.4

Hiding Power

3.4.1 General The official definition of the hiding power of a pigmented material is ªits ability to hide the color or color differences of the substrateº. The reader may be a little perturbed by the fact that this definition* uses the word ªhideº to explain ªhiding powerº, but in defense of the writers of the standards it must be said that there is scarcely a better way to express what is meant. The model underlying the hiding power relates to a black/white contrast substrate on which the coating is to be applied. The determination of the hiding power value involves ascertaining the film thickness h such that the contrast substrate just vanishes for the eye performing the assessment. The thickness hD (in mm) that statisfies this condition is called the ªhiding layerº; its reciprocal D = 1/hD (in mm±1 = m2/L) is the hiding power value. Like the tinting strength to be discussed further on, it is a measure of effectiveness, since it states the area (in m2) that can be covered with 1 L of paint applied in a hiding coat. If the vanishing of the contrast substrate were actually determined with the colorist's eye, hiding power would be a subjective quantity; to derive a functional method of determination, it is therefore necessary to place the procedure on a colorimetric basis.** For achromatic coatings, the ªcontrast ratioº earlier was used as the hiding criterion; this was the ratio of reflectances on the black and white portions of the substrate for equal film thicknesses. The contrast ratio was specified as 0.98 in order to take account of the 2 % threshold value for brightness perception by the human eye. With colored coatings, brightness contrast is not meaningful, so the hiding criterion was defined some time ago as a certain CIELAB color difference. The criterion DE ab = 1 is commonly employed. The experimental procedure is as follows: Coatings of various thicknesses are applied to the agreed-on contrast substrate. The color difference DE ab between the two contrasting fields is then determined by colorimetry for each of the coatings. If the results are plotted versus the reciprocal of film thickness, the hiding power value in m2/L can be read directly from the diagram at the point corresponding to the criterion DE ab = 1. An example is presented in the experimental section (Chapter 7). This determination procedure has, however, two serious deficiencies that can be seen at first glance: ± Several drawdowns with different film thicknesses must be prepared and measured ± The graphical evaluation is imprecise. * For standards see ªColoring Materials, Termsº in Appendix 1. ** Substrates must, of course, be standardized for an exact method of determination. Reflectance values R0b = 0 and R0w = 0.8 are employed.

3.4 Hiding Power

105

It follows that this method must be rationalized, for it would be desirable to use the minimum number of paint drawdowns and also to employ a computer for the evaluation. The following problem now arises: The Kubelka-Munk theory, next to colorimetry the most important principle for rationalizing an optical pigment testing method, applies only to spectral reflectances. On what wavelength should the measurement and calculation be based? It is for this purpose that the ªprinciple of spectral evaluationº was developed as a link from colorimetry back to the KubelkaMunk theory (Section 3.6). First, however, achromatic coatings will be analyzed. These lend themselves to a direct application of Kubelka-Munk theory provided certain constraints are observed. This section therefore lays the groundwork for the principle of spectral evaluation.

3.4.2 Achromatic Coatings In the ideal case (i. e., when the coating contains no colored substances), the small color difference DE ab remaining between the coating over white and over black can be set equal to the lightness difference DL . The same holds, however, when there is a slight undertone; for a nearly white or nearly gray specimen, the chroma difference and hue difference between white and black must be of a higher order than the lightness difference. Then, by (2.5) and subsequent equations, r r ! 3 Yw 3 Yb (3.128) DEab DL 116 Yw 16 116 Yb 16 116 100 100 where b stands for black and w for white. This equation should be valid for white and light gray coatings, so that the value function for Y 4 0.8856 has been used here. Further, because of the achromatic character, we can set Y/100 = R (i. e., the reflectance independent of l). What is more, we must take into account that the colorist, in the (computationally simulated) application of the hiding power criterion, will select a color matching angle such that the gloss of the specimen surface will not interfere. Thus, for glossy specimens, the colorist ªreflects outº the glossy effect by taking a suitable observation angle; this corresponds to a reflectance of R ± gr0, where g is the degree of gloss. Now the hiding power criterion can be formulated as p p 3 R DEab (3.129) DL 116 3 Rw gr0 gr0 1 s This condition with equations (3.111), (3.10), and (3.120) forms a closed system that makes it possible to calculate the hiding power value. Specifically, for given auxiliary variables a and b, the product S hD = 1/a can be determined. Because S and h in the Kubelka-Munk formulas appear only as their product, if the scattering coefficient S is known along with the value of a, then the hiding power value D can be calculated immediately, for D = 1/hD = a S.

106

3 How Spectra Depend on the Scattering and Absorption of Light

Accordingly, the hiding power value is calculated in a three-step procedure: 1. Determination of auxiliary variables a and b This can be done in either of two ways (see Section 3.3.3): ± R ? is available as a measured value; then by equation (3.120) 1 1 R1 ; b a R1 a 2 R1 ± Rw (along with R0w) and Rb are available as measured values; then by equations (3.123) and (3.27) 1 Rb R0w Rw Rw a Rb R0w 2 p b a2 1 ; R1 a b 2. Calculation of scattering coefficient S Equation (3.124) can be used for the calculation of S: S

1 1 a Rb Arcoth b Rb bh

3. Determination of the factor a The system of equations (3.111), (3.114), (3.10),and (3.129) in complete form, with a = 1/ShD, is Rb

Rw

1 a b coth

b b coth a b R0w b coth a

R0w

1 a

Rb r0 Rw r0

a

b a

1

r0 1 r2 0:36 Rb 0:04 Rb 1 r2 Rb 1 0:6 Rb

1

r0 1 r2 0:36 Rw 0:04 R w 1 r2 Rw 1 0:6 Rw 1 p 3 R gr0 0 b 116

p 3 R gr0 w

(3.130)

3.4 Hiding Power

107

Solution of this system leads to a final equation of at least sixth degree in coth (b / a). Such an equation cannot, however, be solved in elementary functions, and so the function a, which depends on a (or R1 ) and g, cannot be written out explicitly.* An iterative solution procedure must therefore be used, for example Newton's method. For this purpose, the derivatives of the individual equations in the system are needed; with x = 1/a, we have

2

R b

dRb dx

R w

dRw b2 dx a

R b

dRb 1 r0 1 r2 0:384 R b R b dx 1 0:6 Rb 2 1 r2 Rb 2

R w

dRw 1 r0 1 r2 0:384 R w R w dx 1 0:6 Rw 2 1 r2 Rw 2

b a sinh bx b cosh bx

1 2 a R0w R2 0w R0w sinh bx b cosh bx2

(3.131)

Setting the left-hand side of the last equation in (3.130) equal to Z (which must be made zero) gives " # R w R b dZ 1 (3.132) Z 2 2 dx 3 R g r 3 R g r 3 w

0

b

0

These equations can be used with a desk calculator to prepare a table of a as a function of R1 and g. Such a table, for use as a computational aid, is appended to the first publication (see [24] in Section 3.9). Moreover, the tabulated value can be approximated very closely with a nonlinear regression calculation, so that values of a can be obtained from simple quadratic expressions with two coefficients. This computational aid is included in Chapter 7. There are accordingly two ways of obtaining individual a values without using the somewhat unwieldy formulas from above. The hiding power value is then

D

1 aS hD

(3.133)

* Once again (see also the first footnote in Section 2.3.3), it would have been more advantageous to give the value function a logarithmic form. Then the system of equations could have been solved in elementary functions, so that a could have been written explicitly as a function of R1 .

108

3 How Spectra Depend on the Scattering and Absorption of Light

The following measurements are therefore needed in order to determine the hiding power value: ± The reflectance of the infinitely thick layer (R ?) or, in its place, the reflectance over white (Rw) for a film thickness the same as over black, together with the reflectance of the white substrate (R0w) ± The reflectance over black (Rb) ± The degree of gloss of the infinitely thick layer or the coating over white (g) ± The film thickness over black (h) In this way, the goal of rationalization stated in Section 3.4.1 has been achieved. The determination method discussed here is essentially the method of DIN 55984*, except that the standard is based on high-gloss specimens and does not allow for the actual degree of gloss g. The method just described can therefore be regarded as a refinement of the DIN method. It becomes identical with the DIN method if g is set equal to 1 in all the equations.

3.4.3 Scattering and Absorption Components The hiding power is entirely due to the cooperation of scattering and absorption, as has already been shown. The ªscattering componentº and the ªabsorption componentº are those contributions to the hiding power value, expressed as fractions of the total hiding power, that arise from ªhiding power due to scattering aloneº and ªhiding power due to absorption aloneº. To obtain the equations for these components, we take the Kubelka-Munk equations to the limits K ? 0 and S ? 0, respectively. In the assessment of the hiding quality of a coating or pigment, a knowledge of these contributions is important for, say, a white pigment, where only the hiding power contribution due to light scattering is valuable ± in this case, the contribution due to absorption is not useful because absorption components in the case of a white pigment are equivalent to loss of quality. As far as possible, therefore, white pigments should cover solely by virtue of their scattering power, not because they also absorb. But this classification can also be significant for colored pigments; in particular, inorganic pigments are often rated better, the more their hiding is due to scattering. The formulas will now be restated, first for the ªhiding power due to scattering onlyº (equations 3.115 and 3.113): Rb

Sh ; 1Sh

Rw

1 R0w S h R0w 1 R0w S h 1

* For further standards see ªHiding Powerº in Appendix 1.

3.4 Hiding Power

109

and then for the ªhiding power due to absorption onlyº (equation 3.112): Rw R0w e±2Kh

Rb 0 (since R0b 0);

These equations will be used later when the determination of the general hiding power value is discussed. Again, however, the solution needed for rationalization can be stated immediately for achromatic coatings. The ªhiding power due to scattering onlyº Dsca is obtained from equation (3.113) with ab = 1/ (ShD): Rb

1 ; 1 ab

Rw

1

R0w 1 ab 1 R0w ab

(3.134)

These two equations are simply inserted in system (3.130) in place of the first two equations; the iteration then yields Dsca directly. The ªhiding power due to absorption onlyº Dabs can be calculated in a similar way. With equation (3.112) and b = 1/ (KhD), Rb 0 ;

Rw R0w e

2 b

(3.135)

In the case of the absorption component, it is actually possible to solve the system of equations explicitly. We do not need to do this, since it is sufficient to calculate b using equation (3.130) after inserting equations (3.135) in place of the first two equations in the system. Both tables and simple linear formulas are available for the scattering and absorption cases, so that b can be determined; we will become acquainted with these aid in Chapter 7. The ªhiding power due to absorption onlyº Dabs is obtained from 1 bK b a 1 S (3.136) Dabs hD From Dsca and Dabs , the scattering and absorption components dsca and dabs of the hiding power D are calculated as follows: dsca

Dsca ; D

dabs

Dabs D

(3.137)

In many practical examples, it has turned out that a residue is still present after these two components are subtracted. How can this be accounted for? Obviously, that contribution to the hiding power arises from the interaction of scattering and absorption. For if the scattering coefficient increases, the mean distance traveled by light in the layer also grows longer because the light is scattered and rescattered more times. A longer path length, however, necessarily means that more light is absorbed, so there is an additional ªscattering/absorption contributionº, which would not be present if the layer scat-

110

3 How Spectra Depend on the Scattering and Absorption of Light

tered but did not absorb or if it absorbed but did not scatter. This contribution will be called the ªinteraction componentº dint and is given by dint 1 ± dsca ± dabs

(3.138)

The three components given by equations (3.137) and (3.138) can provide much additional information about the hiding power value.

3.5

Transparency

3.5.1 Description and Definition If several layers are printed on a black substrate, one over another, it is generally seen that the layer increasingly displays a more-or-less weak, bright shimmer in comparison to the unprinted black substrate. This shimmer grows stronger as the process is repeated. The same phenomenon is known with lacquers and paints, provided they are sufficiently transparent. It obviously comes about because scattering particles, commonly pigment particles, are present in the medium (ink or paint). If, in an unprejudiced spirit, one first considers ªtransparencyº as a purely optical phenomenon, it is clear that this scattering effect is opposed to it. This argument is the basis for the definition of transparency as applied to the field of pigments. The standards* define transparency as the property of a system (not necessarily a pigmented system) to scatter light as little as possible. Accordingly, the color change on application to a black substrate should be as slight as possible. The transparency of the system is greater, the less color change takes place. Given identical specimen preparation, the transparency of the system can be employed for a comparative assessment of transparent pigments. An expedient approach to the exact definition of a ªtransparency numberº, according to the discussion just presented, is to use the CIELAB color difference as a function of the film thickness h. Figure 3-10 gives such a plot, showing DEab that the reciprocal slope of the tangent at the origin provides a suitable measure for the transparency number T. We then have T cot j

1 1 dDE tan j ab dh

* For standards see ªTransparencyº in Appendix 1.

(3.139) b h=0

3.5 Transparency

111

Fig. 3-10. Definition ot the transparency number T.

Because the color difference has the dimension 1, expression eq. (3.139) has the units of a length. If the film thickness is measured in mm, the transparency number takes on units of 1 mm = 1 L/m2. But what does it mean to state the transparency number T in L/m2 ? According to the definition in equation (3.139), the number T obviously states how many liters of an ink or paint can be printed or spread on one increases by 1. This interpretation square meter of a black substrate before DEab suggests an effectiveness property similar but not identical to the hiding power value. Of two paints, then, the one having the better transparency is the one that can be applied in a thicker coating (i. e., one giving more color) to achieve a given transparency. Like the definition of the hiding power value, this definition immediately im versus plies a method for determining the transparency number. The curve of DEab h is plotted through a few experimental points, and then the tangent at the origin is found graphically or by calculation. If one then works close enough to the origin, a single measured point (aside from the origin = black substrate) is generally sufficient. As in the case of the hiding power, such a procedure lends itself to rationalization. As in the earlier case, one or at most two measurements will be adequate; here, however, the Kubelka-Munk theory, because of its monochromatic character, is not directly applicable. This point will also be taken up in Section 3.6.

3.5.2 Coloring Power By analogy with the transparency number T, a ªcoloring powerº F can be defined. This step is favored by the following argument: of two coatings equal in transparency, the one giving more color is certainly the better. This ability to give color, called coloring power, was not considered in the determination of the transparency

112

3 How Spectra Depend on the Scattering and Absorption of Light

number. The determination of color strength must make use of a white substrate*; versus h is employed. In accordance with the above proceagain a curve of DEab axis is defined as the coloring dure, the angle between the tangent and the DEab power; because of the direct proportionality, this is smaller the steeper the tangent line (Fig. 3-11). The coloring power can be read off the plot: F

dDEab dh

w h=0

(3.140)

Fig. 3-11. Definition of coloring power F in comparison with transparency number T.

Like the hiding power value, F has the dimensions of reciprocal length. Thus it is, once more, an effectiveness property, for F = 1 mm±1 = 1 m2/L means that 1 m2 of the white substrate must be coated with one liter of the paint or ink in order to relative to the white substrate equal to 1. The dimake the color difference DEab mensions of the transparency number and coloring power are thus reciprocals; accordingly, the product of F and T is a quantity having the dimension 1, which we will call the ªtransparency-coloring powerº L. The term ªtransparency-coloring powerº also includes an evaluation of the color-giving property in the sense of the statement, made above, that between two color-giving films of equal transparency the one giving more color is the better. Thus we have L = FT

ªtransparency-coloring powerº

* Standaridized as an ideally white substrate, R0w = 1.

(3.141)

3.5 Transparency

113

We must now look ahead to the next section, where it will be shown that the transparency number T as we have defined it is the reciprocal of the colorimetrically evaluated scattering coefficient S, while the transparency-coloring power F is directly proportional to the colorimetrically evaluated absorption coefficient K. Accordingly, the product in equation (3.141) contains both these coefficients, even though in colorimetrically evaluated form, precisely as in the numerator and denominator of the Kubelka-Munk function K/S. Conversely, to any K/S value a reflectance can be assigned (see, e. g., eq. 3.116), and so from L we call finally calculate a ªtransparency-coloring degreeº G = 1 ± R , which like the reflectance must lie between 0 and 1: G=

p L L 2

L

ªtransparency-coloring degreeº

(3.142)

The quantities L and G are highly suitable for characterizing transparency-coloring action (i. e., along with color-giving action).

3.5.3 Achromatic Coatings In this section we will show that a model analysis based on achromatic systems can also be meaningful in the understanding of transparency. In practice, such systems play virtually no part; the value of such an analysis lies rather in that it will aid us in acquiring important knowledge. We proceed as in the definition of T, equation (3.139), following the established by DL = Lb L0b = Lb ; we then have pattern (see Section 3.4.2) of replacing DEab 1 L b 116 Y b T (A prime denotes the result of applying the operator (d/dh)h=0 to the unprimed quantity). For Y b we must use the linear form of equation (2.6) here because of the nearness to the origin. If Yb /100 = Rb , 1 116 7:787 R b T By the third equation of (3.131), this gives 1 116 7:787 0:384 R b T Provided the layer does not absorb but only scatters, equation (3.115) applies. The above operator then yields R b = S, so that

114

3 How Spectra Depend on the Scattering and Absorption of Light

1 116 7:787 0:384 S 346:9 S T in other words, the transparency number is inversely proportional to the scattering coefficient of the pigmented layer: 1 T 0.002883 (3.143) S A similar analysis can be carried out for the coloring power F. In definition (3.140), DEab is replaced by DL = L0w ± Lw = 1 ± Lw , so that F

L w

116 Y w

The cube-root form of equation (2.5) must be used for the value function Y w . Then, with Yw /100 = Rw and R0w = 1, F

116 R 31 w

116 0:384 R 3 1 0:6 R0w 2 w

This holds provided the layer absorbs only and does not scatter. Then we have the limit equation (3.112) for Rw ; the operator gives R w = ±2 R0w K. With R0w = 1, F

2 116 0:384 1 K 185:6 K 3 1 0:6 12

(3.144)

We thus have the important result that, with the transparency number T and the coloring power F as defined in Sections 3.5.1 and 3.5.2, ± T is inversely proportional to the scattering coefficient S in achromatic, nonabsorbing layers ± F is directly proportional to the absorption coefficient K in achromatic, nonscattering layers This close relationship between T and S, on the one hand, and on the other between F and K is qualitatively the same for chromatic layers. The example also shows clearly that forming the product L = FT gives an expression proportional to K/S. Section 3.6 will now show that S and K in these formulas are represented by the colorimetric integrals of S (l) and K (l) in the case of colored coatings.

3.6 Principle of Spectral Evaluation

3.6

115

Principle of Spectral Evaluation

3.6.1 Description and Significance In order to work out a rational procedure similar to that for the ªachromaticº hiding power (Section 3.4.2), we must face the unanswered question of how to use the Kubelka-Munk theory, which is intrinsically ªspectralº, in solving the problem. The restriction to a single wavelength is typical for achromatic layers, as has been shown. With colored coatings, however, it is not immediately clear whether the measurement and calculation should be done for a preferred wavelength, although everything speaks for the necessity that the entire spectrum should be included in the calculation. But what approach to evaluation then remains open? These are the questions that will be answered once the principle of spectral evaluation has been discovered. The procedure can be described as a feed-back between the Kubelka-Munk theory and colorimetry. As has already been illustrated more than once (e. g., in Sections 3.3.3 and 3.4.2), one determines K and S on a infinitely thick layer and on a finite layer of known thickness over black. The infinitely thick layer can be replaced by a layer over white having the same thickness as the layer over black. This determination of K and S is done not once, but several times for distinct wavelengths spread throughout the visible spectrum. As we have seen, K (l) and S (l) as wavelength-specific constants of a coating govern its optical behavior, so that once they are known it is possible to calculate in advance what reflectances over white and black are to be anticipated at any wavelength in the spectrum and for arbitrary film thicknesses. Now the CIE system is used in determining the color stimulus associated with the spectrum just calculated. Two color stimuli are obtained, one over black and one over white. These imply the corresponding CIELAB coordinates, . This color difference between white and which yield the color difference DEab black must now be subjected to a suitable iterative procedure to make it equal to 1. Now there is a tool for determining by iterative methods the film thickness such that the color difference between white and black will be exactly 1. By going through these purely computational steps, we have simulated the older sampling method for determining the hiding film thickness; the simulation complies fully with the DIN method discussed in Chapter 7. But the determination of hiding power of lacquers, paints, and plastics, just briefly sketched, is merely one example of the usefulness of the principle of spectral evaluation. Later, we will become acquainted with other applications, such as the determination of transparency and the determination of the relative tinting strength of pigments. The universal applicability of the principle to other problems is implied by the fact that it is the key to rationalizing all test methods based on the visual assessment of a match (or fixes difference) between two color drawdowns. With this generalization, it is possible to state the principle in pure form, independent of any special application. Figure 3-12 is an explanatory flowchart.

116

3 How Spectra Depend on the Scattering and Absorption of Light

Fig. 3-12. Flowchart explaining the principle of spectral evaluation.

At the start, the scattering and absorption spectra S (l) and K (l) must be known; that is, these quantities have already been determined on suitable coatings or dyed materials. The variable in the problem, here denoted by w (e. g., film thickness h, scattering coefficient S, absorption coefficient K, pigment volume concentration s,* etc.), is set to an initial value. From it, the reflection spectrum can be calculated with the Kubelka-Munk formulas, and this in turn, with the aid of colorimetry (CIE and CIELAB systems), yields the value of some colorimetric quantity Q for the two color drawdowns being compared. If there is still a difference between the Q found and the nominal Q, this difference (here denoted by DQ) is utilized in calculating a correction to the variable w. The iteration continues until the nominal and actual Q values are sufficiently close together. The w value at this time is the desired value of the variable. In order for the correction Dw to be calculated from DQ, additional information (i. e., formulas not contained in the Kubelka-Munk theory) may be needed.

3.6.2 Application to Hiding Power By the discussion of the achromatic hiding power in Section 3.4.2, it can be stated that the general determination of hiding power with the principle of spectral evalua* If s is selected as variable, a theoretical notion about the concentration dependence of S or K is generally required; see Chapter 4.

3.6 Principle of Spectral Evaluation

117

tion also involves three steps, roughly analogous to those in Section 3.4.2. Specifically, these steps are ± Determination of auxiliary functions a (l) and b (l) ± Determination of scattering coefficient S (l) and absorption coefficient K (l) and iterative calculation to make DEab =1 ± Determination of DEab Now, however, there is the difference that nearly all the quantities to be determined are functions of l. This takes in a (l), b (l), S (l), K (l), and all the R (l) and R (l). In what follows, the l dependences will not be explicitly shown; the notation ª(l)º will appear only as required for clarity. 1. Determination of auxiliary variables a (k) and b (k) The same formulas as in Section 3.3.3 are used here; thus the two auxiliary variables are determined either from R ? or from Rb , Rw , R0b , R0w, all of which must first be transformed into starred quantities by application of the Saunderson correction. In place of equation (3.123), the complete form equation (3.122) is employed, since real black substrates are not always ideally black: a

1 Rw R0w Rb R0b 1 Rb R0b R0w 2 Rb R0w Rw R0b

Rw

As a rule, the l-dependent quantities are now calculated at intervals of 20 nm, that is, with a total of 16 known points, since this is regarded as sufficient for most applications. 2. Determination of the scattering coefficient S (k) and the absorption coefficient K (k) In this step, again the complete computational formula for S must be used, since the white substrate can be used too for the determination of S: S

1 1 Arcoth bh

a R R0 R R0 b R R0

Depending on whether the measured values are Rb , R0b , or Rw, R0w, these are inserted for R and R0 (after application of the Saunderson correction). If, however, the values over both substrates are known, it is desirable to use the R , R0 pair that gives the smaller error of determination for S. To this end, the two errors ± dSb from Rb , R0b ± dSw from Rw , R0w must be compared. The formulas needed are derived from the error propagation law (with dR as error of measurement in the reflectance):

118

3 How Spectra Depend on the Scattering and Absorption of Light

dS2

"

uS uR

# 2 uS 2 dR2 uR0

(3.145)

The partial derivatives are calculated by the chain rule: uS 1 r2 R 2 uS 2:6 1 1 r0 1 r2 uR uR

0:6 R 2

uS uR

(3.146)

and similarly for uS / uR0 with R0 replacing R . Furthermore, uS uR

1 1 uy b h y2 1 uR a R R0 R R0 b R R0

1

where y

(3.147)

and similarly for uS/uR0 with uy/uR0 replacing uy /uR . Finally, uy uR

1

2 a R0 R2 0 b R R0 2

uy uR0

1

2 a R R2 b R R0 2

and

(3.148)

(3.149)

Now both errors of determination dSb and dSw can be calculated with equation (3.145); dR can be set equal to 1 because the two errors are only to be compared. 3. Determination of DE*ab and iterative calculation to make DE*ab = 1 The first step is to specify an initial value h C h0 for the film thickness and to calculate Rw and Rb with the Kubelka-Munk equation (3.111). Both quantities are transformed to uncorrected values with the aid of the inverse Saunderson correction, equation (3.10); at the same time, it is taken into account that the gloss has been reflected away from the observer (see Section 3.4.2), so that R

1

r0 1

r2 R r0 r2 R

g r0

(3.150)

Next, from Rb and Rw, equation (2.3) is used to calculate X, Y, Z by means of the CIE system, for both layers (over white and over black): X

R

x l S l R l dl

(3.151)

3.6 Principle of Spectral Evaluation

119

Here x (l) S (l) stands for the CIE color matching function x given the selected CIE standard illuminant S (l).* In this way, Xb,Yb, Zb and Xw ,Yw , Zw are obtained; these are the CIE tristimulus values of the drawdowns over black and over white. A problem still awaiting solution by the CIE must be mentioned here: how to obtain firm CIE color matching functions x (l), y (l), z (l) for 20 nm intervals. At present, the color matching functions exist only in the form of numerical tables for 5 nm intervals (ISO 7724-1). Without an agreed-on table for 20 nm intervals, it is not certain that two distinct laboratories will obtain the same results. Until 20 nm tables are embodied in standards, it is recommended that the Stearns tables** (see Section 3.7; for examples, see Chapter 7) be employed; these may also be suggested to the CIE for adoption, because the interpolation method used is scientifically well justified. The six CIE tristimulus values are now converted to values X b , Y b , Z b and X w , Y w , Z w by the familiar method (see Section 2.3.3); the cube-root form must be used above the threshold X/Xn = 0.008856 etc., the linear form in other cases. Hence, the differences Da , Db , DL between the layers over black and over white are obtained as differences of the CIELAB color coordinates ab , bb , Lb and aw , bw , then follows. If this value is not yet close enough to unity, h Lw . The value of DEab should be changed in the proper sense and the calculation repeated (iteration loop in Fig. 3-2 with h as variable). For the iteration proper, any zero-finding technique known from numerical ± 1 equal to zero). Because of its many admathematics can be used (to set DEab vantages, Newton's method is recommended here again. The main virtue of this technique is fast convergence; considerable amounts of machine time may be required for other procedures. Newton's method does have the drawback that all the derivatives of the variables must be formed, but this laborious manual computation has to be done only once. The equations needed are stated here. ± 1 to zero, to work with the function It is useful, instead of taking DEab Z = ln DEab ? 0 ,

(3.152)

because the logarithm converges to zero more rapidly. The step-by-step procedure for differentiation with respect to h is as follows:

* The notation S (l) is used to distinguish this function from the wavelength-dependent scattering coefficient S (l). ** See ªColor matching functions in steps of 20 nmº in Appendix 1.

120

3 How Spectra Depend on the Scattering and Absorption of Light

uZ 1 2 uh DEab

uDa uDb uDL Db DL Da uh uh uh uDa ua w uh uh

uab uh

uDb ub w uh uh

ubb uh

uDL uLw uLb uh uh uh ua uX uY 500 uh uh uh ub uY uZ 200 uh uh uh uL uY 116 uh uh

(3.153)

There are two cases: 1) X/Xn ^ 0.008856 etc.

2) X/Xn > 0.008856 etc.

uX 7:787 uX uX X uX etc. etc. uh uh 3X uh Xn uh Z uX u R l x l S l dl etc. uh uh uR 1 r0 1 r2 uR 0:384 uR uh uh 1 r2 R 2 1 0:6 R 2 uh uR bS2 uh a

1 2 a R0 R2 0 R0 sinh bSh b cosh bSh

The derivatives for the two extremal cases, ªscattering onlyª (Rsca ) and ªabsorption onlyª (Rabs ), should also be written out: uRsca S uh 1 uRabs uh

1 R0 R0 Sh 1

2 KR0 e

2Kh

2

2 KRabs

(3.154)

3.6 Principle of Spectral Evaluation

121

So much for the derivatives needed in Newton's method. It goes without saying that these formulas must be worked out back to front; that is, one must begin with the last of the equations just presented, incorporating these into the respective steps of the main program if one wishes to write a computer program. An example of these formulas, which may appear somewhat confusing ± though only at first glance ± appears in Chapter 7 along with a program listing.

3.6.3 Application to Transparency and Coloring Power The distinctive point about the application of the principle of spectral evaluation to transparency and coloring power is that no iteration is required; the values sought are obtained by direct calculation. The reason is that what is being sought is not an optimal film thickness or pigment concentration; instead, the initial slope (at a film thickness of h = 0) of colorimetric quantities versus h is to be determined. In order for the principle to apply to transparency and coloring power, defining relations (3.139) and (3.140) and the formulas derived from them must be replaced by their partial derivatives with respect to h, then taken to the limit as h ? 0. It then are, for the transparency, the becomes clear that the quantities derived from DEab colorimetrically evaluated scattering coefficient and, for the coloring power, the colorimetrically evaluated absorption coefficient. In the following equations, a prime denotes the result of applying the operator (u/uh)h?0 to the unprimed quantity. DE ab

uEab uh

s 2 2 2 ua ub uL uh uh uh h?0

a 500 X

Y ; b 200 Y

h?0

p a 2 b2 L 2

Z ; L 116 Y

(3.155)

This equation is to be used for calculating as ; bs ; Ls with Xs ; Ys ; Zs , and for calculating ak ; bk ; Lk with Xk ; Yk ; Zk ; symbols with subscript s are for transparency, , namely those with k for coloring power. As a result, two values are found for DE ab DEab;s and DEab;k . X s Y s Z s ; Z s 7:787 ; Y s 7:787 X s 7:787 Xn 100 Zn X k X k ; 3 Xn X s

R

x l S l 1

r0 1

Y k

Y k ; 3 100

Z k Z k 3 Zn

(3.156)

(3.157)

R r2 S l dl 0:384 x l S l S l dl (3.158)

122

3 How Spectra Depend on the Scattering and Absorption of Light

(and similarly for Ys ; Zs with x (l) replaced by y (l) and z (l) respectively). Again SÅ (l) denotes the spectrum of the CIE standard illuminant used, and S (l) is the spectral scattering coefficient. R 1 X k 2 x l S l 1

R r0 K l dl 4:8 x l S l K l dl r2

(3.159)

(and similarly for Yk ; Zk with x (l) replaced by y (l) and z (l) respectively). The expressions to the right of the first equality signs in the last two equations allow for the possibility that the spectra of the two reflection coefficients r0 and r2 are known. The equations just stated must, once again, be worked through backwards in the practical calculation, that is, beginning with the last equations. Finally, the transparency number and coloring power are obtained as T

DE ab;k 1000 m2 mL 1 mL m 2 ; F 1000 DE ab;s

(3.160)

The factor 1000 appears twice so that smaller numbers can be used for T and F (in derived units). Now T denotes the number of mL that can spread over 1 m2 before measured against the black substrate becomes equal to 1. Similarly, F denotes DEab of 1 is the number of m2 that can be covered with 1 mL so effectively that a DEab obtained relative to an ideal white. All the equations needed for transparency and coloring power have now been written down. Similarly to what was done in Section 3.5.2, the transparency-coloring power L and the transparency-coloring degree G can be calculated from T and F. All of these equations will be repeated for direct computer processing in the practical portion of Chapter 7. It is now possible to determine hiding power and transparency after a minimum of three spectral reflectance measurements (R ?, Rb , R0b or R ?, Rw , R0w). Modern instruments employing the spectral method offer a suitable tool for color measurement. In conclusion, a further very important point should be noted, again a consequence of the application of the principle of spectral evaluation. The direct determi versus h (Fig. 3-7) is difficult because nation of the tangent to the curve of DEab highly uncertain reflectances close to zero have to be measured. A result obtained by the theoretical analysis based on the principle of spectral evaluation, equations (3.158) and (3.159), namely that S (l) and K (l) in colorimetrically evaluated form satisfy the definitions of T and F, makes it possible to determine S and K at higher reflectances (e. g., over a white substrate) where the uncertainties are much smaller. In this way, the procedure allows the transparency number and color strength to be determined with far smaller errors than when they are obtained from the tangents to the curves at the origin.

3.7 List of Symbols Used in Formulas

3.7

123

List of Symbols Used in Formulas

a, b auxiliary variables in Kubelka-Munk theory CIELAB color coordinates a , b , L A = a sinh x + b cosh x abbreviated notation in four-flux theory = a sinh 2 x + b cosh 2 x same as A for doubled film thickness Aj = {A1j, A2j, ¼, Anj} eigenvectors of many-flux theory a = 1/ (ShD) factor for calculation of hiding power constants of integration in four-flux theory B1, B2 b = 1/ (KhD) factor for determination of hiding power C auxiliary variable for coefficient determination in four-flux theory constant of integration in many-flux theory Cj w variable in principle of spectral evaluation D hiding power value with subscripts: abs due to absorption only sca due to scattering only d components of hiding power value with same subscripts as D, plus int interaction component Da , Db , DL special CIELAB color differences CIELAB color difference DEab DQ difference between actual and nominal Q values dR error of measurement of R dS error of measurement of S Z null function for iterative procedure sign factor in many-flux theory Zi Kubelka-Munk function FKM g degree of gloss G transparency-coloring degree g diffuse radiation component h film thickness with subscript: D hiding layer k' absorption coefficient for directional radiation absorption coefficient in many-flux theory kj K absorption coefficient for diffuse radiation l radiance (directional) radiances (directional) in incidence direction and opposite to incil +, l ± dence direction

124

3 How Spectra Depend on the Scattering and Absorption of Light

L L+, L++ L±, L= L lj m n p, P, q, Q j F r0 r1 r2 R, R , R R; R R; R, R , R

R , R1, R2, R3 R^ s+, s± S

with subscripts: 0 upper boundary of layer h lower boundary of layer transparency-coloring power radiances (diffuse) in incidence direction with same subscripts as l +, l ± radiances (diffuse) opposite to incidence direction with same subscripts as l +, l ± radiance vector eigenvalues in many-flux theory attenuation coefficient number of channels in many-flux theory auxiliary variables in four-flux theory with subscript: sca scattering only (h) slope angle of function DEab coloring power reflection coefficient at the surface for directional light incident at right angle from outside reflection coefficient for diffuse light incident from outside reflection coefficient for diffuse light incident on the surface from the interior of the specimen reflection factors: measured, surface-corrected, and surface-corrected after exclusion of directional radiation with same subscripts as R abbreviated notation in four-flux theory reflectances: measured, surface-corrected, and surface-corrected after exclusion of directional radiation with subscripts: 0 substrate abs extreme case ªabsorption onlyª b black substrate dif diffuse irradiation ex exclusive of surface reflection g directional irradiation in inclusive of surface reflection r perpendicular irradiation and measurement w white substrate ? infinitely thick layer abbreviated notation in four-flux and Kubelka-Munk theories R for doubled film thickness scattering coefficient for directional light in incidence direction and opposite to incidence direction scattering coefficient for diffuse light

3.8 Summary

125

S (l) sij, Sij S t T T, T , T

lamp spectrum matrix of coefficients in many-flux theory matrix of scattering coefficients in many-flux theory abbreviated notation in determination of Kubelka-Munk coefficients transparency number transmission factors: measured, surface-corrected, and surface-corrected after exclusion of directional radiation with same subscripts as R transmittances: measured, surface-corrected, and surface-corrected t, t ; t after exclusion of directional radiation with same subscripts as R t^ transmittance for doubled film thickness u, w auxiliary variables in four-flux theory x = bSh abbreviated notation in four-flux and Kubelka-Munk theories x (l), y (l), z (l) CIE color matching functions X,Y, Z CIE tristimulus values with subscripts: b black substrate n CIE standard illuminant w white substrate CIELAB value functions X ,Y , Z with same subscripts as X,Y, Z x = 1/a variable for calculation of hiding power value y abbreviated notation in calculation of hiding power value z position coordinate

3.8

Summary

The phenomenological theory of absorption and scattering in turbid media is of fundamental significance for the mathematical treatment of the coloration of lacquers, paints, clouded glasses, etc., and thus for all problems associated with the use and economics of pigments and dyes. The most general form of the phenomenological theory seems to be the many-flux theory, whose mathematical formalism is described in full. Typical for this model is an absorbing and scattering medium bounded by two parallel planes. The boundary conditions can allow for many irradiation geometries; the reflection coefficients at the interfaces can be calculated exactly. A calculation for real layers, however, involves heavy use of the computer and is thus not well-suited to daily practice. The correction formulas for surface reflection can be written down immediately and are thus an exception to the above statement.

126

3 How Spectra Depend on the Scattering and Absorption of Light

The four-flux theory is derived as an important special case, and its results are written as a collection of explicit formulas. The links between the four-flux theory on the one hand and the theories of Kubelka-Munk (two-flux) and Ryde/Duntley (special case of four-flux) on the other are discussed. The four-flux theory in this generalized form yields equations for the case of irradiation from both sides, for the transmission, and for the particularly important cases of reflection with substrate and reflection with infinitely thick layer, both with mixed (diffuse and directional) irradiation. What is more, the case of a specularly reflecting substrate is treated, as are the extreme cases where absorption is strongly dominant and where scattering is strongly dominant. It is further shown how the five coefficients can be determined experimentally from reflection or transmission measurements, that is, in particular how the poorly accessible coefficients for directional irradiation can be determined exactly. Finally, the equations of the Kubelka-Munk theory and the formulas for obtaining their coefficients are summarized. The hiding power of scattering and absorbing layers is the most important technical quantity that can be rationalized with the aid of the phenomenological theory. = 1 between the On the basis of the definition in terms of the hiding criterion DEab layers over black and white substrates, the simplified case of achromatic layers is considered; equations for the hiding power applicable to this case can be derived in a direct fashion from the Kubelka-Munk formalism. The hiding power so obtained can be split into a scattering component, an absorption component, and an interaction component, so that additional information can be extracted about the quality of the layer. The transparency number for paints and inks is described and defined. This quantity also makes it possible to characterize the optical performance of transparent pigments. In connection with transparent coatings, a coloring power can also be defined and determined exactly; other quantities describing the transparency-coloring properties can be derived from the transparency number and the coloring power. Finally, the principle of spectral evaluation is thoroughly discussed as a feedback between colorimetry and the Kubelka-Munk theory. Only in this way can the hiding power of chromatic layers be approached in an exact manner. All the needed formulas, including those for a Newton iteration method and for an improved accuracy in the determination of S, are derived. This principle can also be used to advantage for the transparency number.

3.9

Historical and Bibliographical Notes

The absorption-based approach arose out of what was once the most important specialty in physics, an area that received a high degree of early development: astronomy. It was astronomical problems that led to the formulation of what is now known as Lambert's law. Lambert, who lived from 1728 to 1777, was also con-

3.9 Historical and Bibliographical Notes

127

cerned with astronomical topics and was seeking a law to describe the decrease in intensity of starlight as it passed through the atmosphere. The beginnings of this theory may be said to go back to Bouguer in 1729. The first worker to take up the phenomenological theory of scattering was ± we suppose ± Stokes [1], but once again, usable formulations came from astronomy. Because both the Earth's atmosphere and interstellar space contain dust particles, a formula based on absorption alone is not always adequate to predict intensities in astronomy. The first closed phenomenological theory of scattering dates from 1905 and was devised by the astronomer Schuster [2]. Here the model of two ray paths appears for the first time; Schuster, who of course was interested only in transmission behavior, obtained a transmittance formula similar to the later ones of Ryde and Kubelka for diffuse light. More than a decade later, in 1918, Renwick [3], [4] confirmed Schuster's results, but went a step further and treated reflectance as well. The formulas were clumsy, however, and not well-suited to calculating the reflectances of scattering layers. In 1927, Silberstein [5] essentially confirmed Schuster's transmission equation, but this publication contains the first discussion of a model for directional irradiation. Gurevic [6] in turn gave a more thorough treatment of the reflectance. But all the work cited must be regarded as preliminary to the classic publications of Kubelka and Munk [7] and Ryde [8], which came out in 1931. Kubelka and Munk, with no knowledge of prior work, analyzed the reflectance for the diffuse irradiation case with a substrate, deriving the still-used formulations in terms of hyperbolic functions (these first by Kubelka in 1947 [9]). Their main achievement, however, is the application of the equations to hiding power, on the one hand, and on the other to the reflectance of very (ªinfinitelyº) thick layers. The latter aspect is embodied in the Kubelka-Munk function, which found immediate acceptance and is applied to all cases involving scattering layers of high hiding power. The Kubelka-Munk theory gives the first clear expression of the fact that two coefficients are needed in the case of diffuse irradiation (ªtwo-constant theoryº) and that these coefficients can in fact be determined. The Kubelka-Munk theory fails in the case of a highly dilute pigment or a very thin layer (see Section 3.3.1), because the radiation cannot be ideally diffuse and not every ray collides with a pigment particle (ªsieve effectº). With specific application to biological measurements, Fukshanski [10] has devised a theory, but its concepts have not yet been made to work for lacquer and paint coatings. Ryde [8] analyzed transmittance and reflectance for the case of directional irradiation. The two ªdiffuseº coefficients are complemented by two more scattering coefficients, making a total of four. Later, Duntley [11] extended the theory by introducing a second absorption coefficient for directional irradiation; as a result, five coefficients (including the Kubelka-Munk coefficients) are needed for the phenomenological description of scattering and absorbing layers with directional irradiation. In comparison with the Kubelka-Munk theory, the Ryde theory has not gained such wide adoption.

128

3 How Spectra Depend on the Scattering and Absorption of Light

Duntley [11] was also concerned with surface phenomena. The correction formula proposed by Saunderson [12] dates from the year 1942. A good survey of these formulas can be found in Brockes [13]. The complete version of the explicit four-flux theory was published in 1962 [14]. Like the Ryde/Duntley theory, it employs five coefficients; it goes further, however, including equations for two-sided irradiation with diffuse and directional light and for layers with substrates. A second part was added in 1964 [15], now describing the determination of the three ªdirectionalº coefficients. The equations for specularly reflecting substrates, on the other hand, were not included in the publications cited; they are presented for the first time in this book. The first part of the four-flux theory [14] was confirmed a few years later by Billmeyer and co-workers [16], who also introduced another (fourth) scattering coefficient. The comprehensive many-flux theory is due to Mudgett and Richards (1971) [17], whose work marked the completion of the phenomenological theory of scattering and absorption for the time being. The standard work on radiative transfer processes, by Chandrasekhar [18], should also be mentioned here. Recommended monographs, particularly on the use of the Kubelka-Munk theory, are those of Kortçm [19] (in German) and Judd [20]. Experimental applications of the many-flux theories have been described by only a few authors, for example Pauli and Eitle [21], [22], who applied a three-flux theory to color formulation problems. Chapter 6 will give a account of the results obtained by Mudgett and Richards [17] and by Atkins and Billmeyer [23]. The first equations for the hiding power based on scattering and absorption coefficients for diffuse irradiation were included by Kubelka and Munk in their renowned work [7]. In present-day terms, they used the lightness contrast ratio as hiding criterion; as it then turned out, however, this criterion is applicable only to achromatic layers. Standardized methods for the achromatic case were accordingly worked out in the 1950s and 60s and have been used since that time. Not until the advent of the CIELAB system could the desire for more suitable hiding criteria be made possible a comfulfilled. First, in 1981, the introduction of the criterion DEab putational procedure for achromatic layers based on the Kubelka-Munk theory [24]; this duly led to a standard. At the same time, the first description was given of how gloss could be handled in color matching and how the scattering and absorption components of the hiding power could be calculated. It had already been shown that the determination of hiding power from R?, Rs is more accurate than the determination from Rb , R0b , Rw, R0w [25]. A pneumatic apparatus for measuring film thickness was developed by Kåmpf [26] for use in the determination of scattering coefficients, absorption coefficients, hiding power, and transparency. Economic aspects of the hiding power were analyzed by Keifer [27]; these will be taken up in Section 7.4.4. Not until 1964, however, was the principle of spectral evaluation [28], [29] applied in order to make the Kubelka-Munk theory applicable to colored layers. The first procedure used was a graphical one, with the lightness as hiding criterion. Gall [30] then showed how the principle could be rationally applied (by computer

3.9 Historical and Bibliographical Notes

129

programming) when other criteria (color difference) were used in determining the hiding power of inks and paints. Strocka [31] demonstrated that 16 chosen wavelengths (20 nm intervals) would be sufficient for most applications. The tables of Stearns [32] can be expediently employed for the CIE color matching functions (see Chapter 7 for examples). Further improvements followed [33]: iteration with Newton's method, calculation of S for smaller error of determination. On the last point, it should be remarked that the calculation of the error dS in the scattering coefficient as done in Section 3.6.1 is preferable to the computational scheme in [33] because it is simpler. With regard to transparency, the definition generally accepted today was not written until 1976 [34]. This definition provided the basis for a standardized test procedure. The same publication [34] suggested the use of the principle of spectral evaluation in order to create a rational and sufficiently accurate determination method using the Kubelka-Munk coefficients, especially when the calculation can be done in a single pass after the hiding power has been determined [33]. Reference should also be made to a report on experience with diverse methods of hiding power determination [35] and to a summary of the Kubelka-Munk theory in pigment testing [36].

References [1] [2] [3] [4] [5] [6] [7] [8] [9] [10] [11] [12] [13] [14] [15] [16] [17] [18] [19] [20] [21] [22] [23] [24]

G. G. Stokes, Proc. Roy. Soc.11 (1860) 545. A. Schuster, Astrophys. J. 21 (1905) 1. F. F. Renwick, Phot. J. 58 (1918) 140. F. F. Renwick, H. J. Channon, B. V. Storr, Proc. Roy. Soc., Ser. A., 94 (1918) 222. L. Silberstein, Phil. Mag. 4 (1927) 7. M. Gurevic, Phys. Z. 31 (1930) 753. P. Kubelka, F. Munk, Z. techn. Phys. 12 (1931) 593. J. W. Ryde, Proc. Roy. Soc., Ser. A., 131 (1931) 451. P. Kubelka, J. opt. Soc. Am. 38 (1948) 448. L. Fukshanski, J. Math. Biol. 6 (1978) 177. S. Q. Duntley, J. opt. Soc. Am. 32 (1942) 61. J. L. Saunderson, J. opt. Soc. Am. 32 (1942) 727. A. Brockes, Die Farbe 9 (1960) 53. H. G. Vælz,VI. Fatipec-Kongress Wiesbaden 1962, Kongr.-B. (Verlag Chemie, Weinheim) 98. H. G. Vælz,VII. Fatipec-Kongress Vichy 1964, Kongr.-B. (Verlag Chemie, Weinheim) 194. J. K. Beasley, J. T. Atkins, F. W. Billmeyer, jr., Proc. II. Interdisc. Conf. Electromagnet. Scatt. 1967, Congress B. (Gordon & Breach, New York) 765. P. S. Mudgett, L. W. Richards, Appl. Opt. 10 (1971) 1485. S. Chandrasekhar, Radiative Transfer, Clarendon Press, Oxford, 1950. G. Kortçm, Reflexionsspektroskopie, Springer, New York, 1969. D. B. Judd, Color in Business, Science and Industry, 2. Edit., J. Wiley & Sons, New York, 1969. H. Pauli, D. Eitle, 2. AIC-Congress York 1973, Congress B. (A. Hilger, London) 423. D. Eitle, H. Pauli, XIV. Fatipec-Congress, Budapest 1978, Congress B. 209. J. T. Atkins, F. W. Billmeyer, Color. Eng. 6 Nr. 3 (1968) 40. H. G. Vælz, Die Farbe 29 (1981) 297.

130

3 How Spectra Depend on the Scattering and Absorption of Light

[25] H. G. Vælz, Die Farbe 19 (1970) 231. [26] G. Kåmpf, H. G. Vælz, farbe + lack 77 (1981) 629. [27] S. Keifer, Deckvermægen in BAYER-Ringbuch ¹Anorganische Pigmente fçr Anstrich- und Beschichtungsstoffeª, Leverkusen 1973. [28] H. G. Vælz,VII. Fatipec-Congress Vichy 1964, Congress B. (Verlag Chemie, Weinheim) 366. [29] H. G. Vælz, farbe + lack 71 (1965) 725. [30] L. Gali, farbe + lack 72 (1966) 955 and 1973. [31] D. Strocka, 2. AIC-Congress,York 1973, Congress B. (A. Hilger, London) 453. [32] E. I. Stearns, Rev. Ind. Management Text. Sci. 14 (1975) 1. [33] H. G. Vælz, Progr. Org. Coat. 15 (1987) 99. [34] H. G. Vælz, Dtsch. Farb. Z. 30 (1976) 392 and 454. [35] M. Cremer, farbe + lack 90 (1984) 548. [36] H. G. Vælz, Progr. Org. Coat. 13 (1985) 153.

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

4

How Light Scattering and Absorption Depend on the Content of Coloring Material (Beer's Law, Scattering Interaction)

4.1

Introduction

4.1.1 Description and Significance of the Concentration Dependence The complex of ideas to be discussed next occupies a position that is not just central in the interlinked system of fundamental theories (Chapter 1) but is also very significant in practice. Now that we have become aquainted with the absorption and scattering of light as the root cause of the spectral distribution, we must ask how the concentration of dyes or pigments affects scattering and absorption and thus, ultimately, spectra. The link with practical concerns can be understood immediately because this topic relates to all aspects of producing color recipes: not just formulation, but also correction of rematching. The manipulation of pigment concentrations is the formulating colorist's most vital tool. In addition to the concentration dependences of absorption and scattering, however, this chapter also deals with that of the Kubelka-Munk function, especially with regard to special pigment mixtures such as those with white and black pastes. These are particularly relevant to colorimetric pigment testing, because they form the basis for determining the tinting strength and lightening power. The last two concepts will be taken up in the pertinent sections; here it should be noted that the tests are often used for incoming inspection of coloring materials, since they can be performed in a relatively short time. Colorimetric tests of coloring material generally presuppose that dyes are dissolved and pigments are dispersed in a medium. The resulting pigment dispersion should contain the pigments in homogeneously distributed form (optimally dispersed); ªdispersionº as the term is used in colloid chemistry must therefore be dealt with first, and this means providing some essential information about particle size. A section on measures of pigment content then follows.

132

4 How Light Scattering and Absorption Depend on the Content ¼

4.1.2 Pigment Particle Size Along with the optical constants, the key physical features of pigments include geometrical information such as the particle size and shape. The effect of particle size on color properties was mentioned briefly in Section 1.2, which made the point that both the absorption and the scattering properties are strongly influenced by the size and distribution of pigment particles. The terminology of pigment particles will be outlined briefly here as set forth in standards.* The following terms are defined (see also Fig. 4-1): ± Particle: A delimitable unit of a pigment, which can have any form and any structure. ± Primary particle, single particle: A particle that can be identified as an entity with the help of suitable physical methods (optical or electron microscopy). In many cases, it may be a single crystal, but it may also consist of a number of crystallites that coherently scatter X-rays.

Fig. 4-1. Primary particles, aggregates, and agglomerates, after Honigmann and Stabenow. * See ªParticle-Size Analysisº in Appendix 1.

4.1 Introduction

133

± Aggregate: An intergrown combination of primary particles in surface contact with one another such that the surface area is smaller than the sum of the surface areas of the primary particles. ± Agglomerate: A combination of primary particles or aggregates in contact with one another such that the components of the agglomerate are not intergrown with one another and the total surface area is not substantially different from the sum of the individual surface areas. ± Flocculate: An agglomerate that is formed in pigment/binder systems and can be broken down again by low shear forces. The particle size denotes the geometric dimension used to characterize the spatial extent of a particle. Such measures can be ± The particle diameter, that is, the diameter in the case of spherical particles or those bounded by regular figures ± The equivalent diameter, that is, the diameter of a sphere having the same volume as the particle ± The particle surface area, that is, the external surface area (without voids) or internal surface area (including voids) of a particle ± The particle volume, that is, the effective volume (without voids) or apparent volume (including voids) ± The particle mass, that is, the mass of the particle determined by weighing Tables 4-1 and 4-2 present some information on the particle shape and most frequent diameter of pigment particles. The granulometric composition of a pigment is described by its particle-size distribution. Topics relating to this aspect will be discussed in Chapter 5.

4.1.3 Dispersing of Pigments In general, the testing of pigments requires their incorporation into a binder or a plastic material; this holds, in particular, for the color properties. The look of the dry pigment powder, as a rule, affords only a very incomplete picture of the actual color qualities. In order to gain a complete knowledge of the colorimetric properties of a pigment, one would have to work it into a multitude of coating materials* or plastics**. The impulse toward rationalization means that such tests must be limited in number. However, it is often sufficient to do tests in typical systems, those that promote pigment dispersion and allow the color quality of interest to manifest itself fully. A pigment/binder dispersion is a suspension before drying, a solid sol after drying. Accordingly, the concept and relations known from colloid chemistry apply to the description of pigment/binder systems. The dispersing of pigments and fillers in binders is a highly complex process involving subprocesses, some of which have * Standards see ªCoating materialsº in Appendix 1. ** Standards see ªEmulsion paintsº and ªThermoplasticsº in Appendix 1.

134

4 How Light Scattering and Absorption Depend on the Content ¼

Table 4-1. Particle-size properties of some inorganic pigments.

Titanium dioxide, rutile (aftertreated) Titanium dioxide, anatase (untreated) Zinc white Red iron oxide Yellow iron oxide Cadmium sulfoselenides

Particle shape

Modal diameter Dhv, mm

almost spherical almost spherical almost cubic to acicular spherical acicular cubic to spherical

0.18±0.35 0.10±0.20 0.7 ±1.0 0.1 ±0.7 0.1 60.3 to 0.2 60.8 0.2 ±0.4

Table 4-2. Particle sizes of some organic pigments. Modal diameter Dhv, mm Azo (monoazo) pigments Azo (disazo) pigments Phthalocyanines, blue Phthalocyanines, green Polycyclic pigments

0.50±0.55 0.05±0.21 0.06±0.10 0.04±0.08 0.05±0.30

to precede or follow others, some of which can overlap in time. These subprocesses can be systematized and classified under the following three heads: ± Wetting: the displacement of air from the particle surface and the formation of a layer of solvent molecules. ± Disintegration: the disruption and dissipation of agglomerates, involving energy supplied externally (i. e., by dispersing equipment). ± Stabilization: the establishment of repulsive forces between particles (e. g., through solvate shells) in order to maintain the dispersed state already achieved. These repulsive forces must be stronger than the attractive van der Waals forces, which would otherwise cause the pigment to flocculate. As a rule, the quality of dispersing has a crucial effect on the properties of the system. The color properties, in particular the full shade, tinting strength, gloss, and gloss haze, show an especially strong dependence on the state of dispersing. In system made up of various pigments, demixing can occur, and a change in the optical aspect (floating) can result. Floating can be controlled by preliminary coflocculation on the pigments with suitable wetting agents, or by the addition of thickeners. A frequent departure from ideal dispersion takes the form of flocculation. As defined by Keifer, this means any departure from statistical uniformity of the pigment distribution in the medium. Deviations from uniformity commonly result in a loss of optical and coloristic performance. Flocculation also takes in the cases where pigment particles are drawn close together by attractive forces (but do not

4.1 Introduction

135

agglomerate), and where the pigment distribution is distorted by foreign particles. In particular, this always occurs when such particles are larger than the pigment particles, and so any addition of substances having a larger particle size (e. g., fillers) is always problematic. At higher pigment contents, there is no longer any certainty that the voids between pigment particles will be completely filled by the binder. Above a given concentration (the ªcritical pigment volume concentrationº), characteristic anomalies are seen, leading to disrupted and sometimes singular behavior and thus to deterioration of the pigment properties. The color properties are also affected.

4.1.4 Measures of Pigment Content From the standpoint of colloid chemistry, a pigmented medium (lacquer, paint, plastic) is a dispersion, that is, a multiphase system. The terminology and notation originally developed for mixes-phase systems* can be applied to the quantitative description of such systems. Thus the portions of the two components in such a dispersion are described in terms of: ± the mass m (unit: g or kg) ± the volume V (unit: cm3 or L) In this book, composition-related symbols will always appear without subscripts if they refer to pigment, and with the subscript M if they refer to (unpigmented) media. The same will apply to all material constants of the pigment and of the medium, respectively. Accordingly, we define: ± the pigment mass portion (PMP) w as w

m m mM

(unit: 1)

(4.1)

(unit: g 7 cm±3)

(4.2)

± the pigment mass concentration (PMC) b as b

m V VM

± the pigment volume concentration (PVC) s as s

V V VM

* See ªMixtures, Compositonº in Appendix 1.

(unit: 1)

(4.3)

136

4 How Light Scattering and Absorption Depend on the Content ¼

The PMP and PVC are expressed as fractions, often in % (example for PVC: s = 0.0295 = 2.95 %). If the volumes in this formula are replaced by the masses m, mM and the respective densities* R, RM (unit: g cm±3), the PVC becomes: m R m w s m mM mm w m RM R

(unit: 1)

(4.3)

where m RVM mM

R RM

(unit: g)

(4.4)

is the pigment mass equivalent to the medium volume (PVM) and m

R 1 RM

w

(unit: 1)

(4.5)

is the pigment mass equivalent to the medium volume of the mass portion (PMM). For constant portions by weight of the medium, m is a constant (provided the same pigment is used); thus the pigment/medium volume ratio (PMV) defined as c

V m w s VM m m 1 s

(unit: 1)

(4.6)

is an especially convenient measure, since it can be calculated easily from m and m or from s alone. Table 4-3 lists the equations for the quantities just defined. Conversion relations for these measures are stated in matrix form in Table 4-4. If one wishes, for example, to do the conversion w ? s, one begins in the second row (w ?) and follows across to the fourth column (? s) to find equation (4.3). This book will make exclusive use of the measures described here in quantifying the pigment portions in pigmented media. Among them, the pigment volume concentration (PVC) s is the most important, because the optical pigment properties * The use of the same symbol in the standard notation for the density, R, and the spectral reflectance, R (l), is all right because there is no danger of confusion. The same holds for the symbol s, which represents both standard deviation and PVC.

137

4.1 Introduction

Table 4-3. Measures of pigment content in media, with their relationships to masses and densities of pigment and medium. R R VM RM

(4.4) Pigment mass equivalent to the medium volume (PVM)

m mM

(4.1) Pigment mass portion (PMP)

w

(4.2) Pigment mass concentration (PMC)

b R

(4.3) Pigment volume concentration (PVC)

s

m mm

(4.6) Pigment/medium volume ratio (PMV)

c

m m

m m mM m mm

Table 4-4. Conversion relations between measures of pigment content in media, equations (4.7) to (4.15). ?w

(4.7)

Pigment mass portion (PMP) w? Pigment mass concentration (PMC) b? Pigment volume concentration (PVC) s? Pigment/medium volume ratio (PMV) c? Pigment mass equivalent to the medium volume of the mass portion (PMM) m

?b w bR w m

w (4.8) w m

b

R

b

b

(4.11) s w m 1 s (4.13) w m c (4.5) m

R 1 RM

?s (4.3) w s w m

(4.6) w c m

(4.9) b s R

(4.10) b c R b

(4.12) b Rs

s

(4.14) c bR 1c

(4.15) c s 1c

w

?c

(4.6) s c 1 s

c

m m mM

(chiefly the absorption and scattering properties) are referred to volume (not weight, cross section, or surface area). As a consequence, physical quantities such as the scattering and absorption coefficients often display a linear or quasi-linear dependence on the volume fractions. Related to the PVC is the pigment volume portion (PVP, unit : 1) j; it is defined in terms of the partial volumes before mixing, in contrast to s, which is defined in terms of the volumes V and VM after mixing.

138

4 How Light Scattering and Absorption Depend on the Content ¼

This measure is less interesting as far as colorimetric test methods are concerned; in any case, j = s if there is no volume reduction in the mixing process, as in nondrying pastes. Other measures are seen occasionally, such as the pigment surface concentration (in m2/L), which states the amount of pigment particle/medium interfacial area per unit volume in the dispersion. This quantity is sometimes used with latex paints, because it provides a measure of the free surface area exposed not to the medium but to the air, which leads to increased scattering power by virtue of the higher refractive index (e. g., TiO2 in rutile form has a refractive index of 2.75 relative to air but 1.9 relative to binder). The problem arises now and again of converting volumes in finished pigment/ medium mixtures to masses, or masses to volumes. The density of the dispersion RD is needed for this purpose. If there is no volume reduction in the mixing process, the mixture density can be calculated from the components:

1 V VM m mM RD

m mM RM R w 1 w m mM R RM

(unit of R: g cm±3) (4.16)

A comparison with equation (4.5) and (4.7) shows that the mixture density is very easy to obtain if w and s or w and b are known: RD

R b Rs w m w w

(unit: g cm±3)

(4.17)

In general, it should be kept in mind that quantities expressed in other units (e. g., b in g/L) must be multiplied by the appropriate powers of ten to get them in the stated units before equations (4.1) to (4.17) are applied.

4.2

Absorption and Content of Coloring Material

4.2.1 Dyes The absorption coefficients defined in Chapter 3, k '(l) for directional irradiation and K (l) for diffuse irradiation, are not actually constants, for they are also affected by the concentration of the coloring matter used. We now inquire into the dependence on concentration.

4.2 Absorption and Content of Coloring Material

139

Absorbing substances present as molecules or ions in the solution show a strictly linear dependence of absorption on solute concentration. This statement applies to dissolved dyes as well, so that k' k@b b und K kb b

(4.18)

Here b is the concentration by mass in g/L, and the two new quantities kb@ and kb are constants for a given dye, called ªabsorption coefficients per unit mass concentrationº. If k ' and K are measured in m2/L, they have the unit m2/g. Equations (4.18) constitute Beer's law. Deviations from the behavior described are seen only when the solution departs from ideality, that is, when reactions occur between the individual solute molecules or between dye and solvent molecules. Equation (4.18) is sometimes directly combined with (3.48) to yield k@b b

1 1 ln h T

(4.19)

(where h is the layer thickness and T the transmission factor), the whole expression being referred to as the Lambert-Beer law. This is somewhat confusing, because the equation does not describe a single effect discussed by two authors, but two fundamentally separate insights into absorption phenomena in transmission measurements. Equation (4.19), however, states that for a given cell thickness h if the concentration by mass b is known then the absorption coefficient per unit mass concentration k@b can be determined by transmission measurements, and conversely if k@b is known then b can be determined. The latter technique in particular has found wide adoption, e. g., spectroscopic analytical methods.

4.2.2 Pigments If a pigmented medium is now taken in place of the dissolved dye, it seems at first glance that the ideal conditions existing in the solution are now violated. However, the total observed absorption is precisely the sum of all individual absorption contributions of the pigment particles, just as the absorption of the dye solution was the sum of all absorption contributions of the molecules or ions. For this reason Beer's law also holds rigorously for pigments up to high concentrations. Figure 4-2 clearly shows the linear dependence on PVC. The plotted measured values were obtained from the Kubelka-Munk function F = K/S; care was taken to hold the scattering coefficient S constant, since the red iron oxide pigments display scattering of the same order as the TiO2 pigments used in the white paste. As the concentration of the colored pigment was increased, it was therefore necessary to lower the concentration of the white pigment.

140

4 How Light Scattering and Absorption Depend on the Content ¼

Fig. 4-2. Absorption coefficient K for diffuse irradiation (arbitrary units) versus PVC for three red iron oxide pigments (measured at l = 550 nm).

Thus we can write k' k@ s ;

K = ks

(4.20)

for the absorption of pigments; this is again Beer's law, but with the PVC s as the pigment portion. The reason for making this change will become quite evident in the next chapter (see p. 210). The new absorption coefficients referred to the PVC thus have the unit m2/L, since PVC itself has the unit 1. An important remark should be made on the newly-defined ªreferredº coefficients. For both dissolved dyes and dispersed pigments, these coefficients can be formed out of contributions by several species. If there is no interaction between the components, multicomponent systems can be described by simply adding the individual referred coefficients, so that for n distinct pigments we have: k'

n P i1

k@i si ;

K

n P i1

ki si

(4.21)

Thus in, say, a three-component mixture, on can measure k'(l) at three different wavelengths l. If k@i of the individual components are known, three equations can be written; therefrom the concentrations of the three components in the mixture can be calculated. It is expedient to perform these measurements at wavelengths corresponding to the absorption maxima of the components or, when the absorption curves overlap greatly, in ranges that permit each component to be distinguished as clearly as possible from the others.

4.3 Scattering and Pigment Content

141

What was already said about dyes also holds for the validity of Beer's law with regard to the absorption coefficients of pigmented systems. Deviations from ideal dispersion of the pigment/binder system can again result in departures from the linear concentration dependence. The initiating factors are of the same type as in the other case but differ in significance and nomenclature. Specifically, phenomena such as flocculation and agglomeration are implicated, especially at higher pigment concentrations; anomalous effects are also seen near the critical pigment volume concentration.

4.3

Scattering and Pigment Content

4.3.1 Scattering Interaction Because scattering can occur only in the presence of pigments, dyes can now be left out of the analysis. The situation with scattering is somewhat more involved than with absorption. Beer's law, that is, the proportionality between the scattering coefficient and the pigment volume concentration, holds only for low pigment contents.* At higher PVC values, because of the smaller and smaller distances between pigment particles, a scattering interaction occurs, which can be interpreted as particles hindering each other in light scattering. In the literature, ªmultiple scatteringº and ªdependent scatteringº are distinguished by whether the hindrance is due to the same pigment particles or to others. As a result, there are departures from linearity as the measured scattering coefficient falls below the straight line. The curve passes through a maximum and then falls off more-or-less steeply (Fig. 4-3). In other words, simple summing over single-particle scattering properties, as specified by

Fig. 4-3. Scattering of light versus pigment volume concentration. * Up to ca. s ^ 10 %.

142

4 How Light Scattering and Absorption Depend on the Content ¼

Fig. 4-4. Geometry of the scattering interaction.

Beer's law, no longer works as the particles, come to be nearer together. Physically, this problem can be interpreted as the scattering of light on multiple particles, and the parallelism with other multiparticle problems in physics makes it understandable that the problem of scattering interaction cannot be solved generally. The only help that can be expected here must come from theoretical descriptions based on simplified geometrical models. We begin by considering an isodisperse collection of particles regularly distributed in a medium. ªRegularly distributedº means that all particles must have the same distance to all their nearest neighbors. This assumption leads to the arrangement taken up by the sphere centers in a closest packing of spheres. In Figure 4-4, the three-dimensional relationships are shown in a cross section. In deriving an equation to describe the scattering interaction, the quantity of interest is the ratio of the sphere diameter D to the distance R between spheres. As shown in the drawing, the ratio of the volume of the spheres (diameter D) to the volume of the closest-packed spheres (diameter R) is exactly p equal to the pigment volume concentration s divided by p 2=6, the fraction of space filled by closest-packed spheres, so that 1 3 D p s 6 1 3 p p 2 R p 6 6 from which the ratio D/R is s p p D 3 3 2 s 1:105 3 s p R If one examines the central particle in Figure 4-4, one sees immediately that the scattering interaction occurs because the light backscattered into the upper halfspace can no longer travel unhindered past the nearest neighbors. Instead, the scattered light is reduced by some fraction, here ± as a first approximation ± taken proportional to the area fraction covered by the particle. This area fraction p of the individual particle can be read directly from Figure 4-4; it is given approximately by the ratio of the cross-sectional area of the hindering spheres (diameter D) to the area of the hemisphere described by R:

4.3 Scattering and Pigment Content

143

D2 p 1 D 2 4 p 8 R 2 R2 p For closest-packed spheres, there are twelve nearest neighbors. Because only the back half-space is of interest here, six spheres must be considered, so the fraction p must be multiplied by six (giving 6p) in order to obtain a measure of the hindrance. What is more, it must be taken into account that the extent of scattering hindrance must be proportional to the area fraction but not necessarily equal to it. For example, it would certainly be better to replace the geometric cross section of the hindering spheres by the scattering contribution of the individual particle, which must be proportional to the PVC-referred scattering coefficient s (mathematically, this corresponds to multiplying by s). Further, an attenuation factor Z characteristic of the pigment can be inserted in the interaction term; the total amount by which the scattering interaction reduces totoal scattering is then represented by 6p Z s. By the last two equations for p and D/R, this expression can be rewritten as 2

(4.22)

6 p Z s g ss 3 where the abbreviated notation 3 g 4

p ! 2 3 2 3 Z p

has been used. The scattering contribution that remains after the hindrance, according to equation (4.22), is thus 1

2

g ss 3

Because Beer's law is taken to hold at small s, the scattering coefficient is given by: S ss 1

g ss

2 3

(4.23)

This relation is not affected by the fact that the next nearest (and so on) spheres contribute to the hindrance. Their effect can be described by some change in the value of the free parameter g (analogous to the Madelung factors, used in crystallographic lattice-energy calculations). The quantity s appearing for the first time in equation (4.22) is the scattering coefficient per unit PVC, which is defined (more rigorously than in the absorption case) as: dS (4.24) s ds s?0

144

4 How Light Scattering and Absorption Depend on the Content ¼

The coordinates of the maximum on the S versus s curve are obtained as follows from the condition dS /ds = 0: 3 3 2 smax 5 gs Smax

2 5

s 1 3 3 2 ssmax s 5g 5

(4.25)

The possibility of the dependent scattering when several pigments are present means that S cannot generally be expressed as a simple sum of contributions due to the various species as was done for K (eq. 4.21). A sum formulation can be used only when one of the summands dominates and the other contributions are small in comparison. In all other cases, the dependent scattering must be taken care of by adding another interaction term to the sum.

4.3.2 Experimental Test of an Empirical Formula Manipulation of equation (4.23) yields: S s 1 s

gss

2 3

(4.26)

If one makes the change of variable S / s = y and s2/3 = x, one obtains the equation of a straight line: y s ± g s2 x

(4.27)

In this way, the S versus s curve of Figure 4-3 is linearized; equation (4.27) is therefore especially well-suited to an experimental test. In order to verify the applicability of this formula, a series of lacquers with increasing pigment content was prepared. The pigment volume concentrations s lay between 0.5 % and 20 %. Several titanium dioxide pigments differing in scattering properties were used, so that the test would cover the widest possible range of properties. From each pigment, a master batch with a s of roughly 0.45 was prepared by grinding for several hours in a vibratory ball mill. Vehicle was added to thick stock to bring the PVC to the desired final value; then drawdown on black/white paper were made with an automatic Bird applicator. The procedure described in Section 7.2.1 was next followed in order to determine S values for each PVC. When the values obtained were plotted versus the PVC, the typical S versus s curves shown in Figure 4-5 resulted. An x, y plot as described by equation (4.27) was also prepared, and the optimal lines were calculated by a least-squares method. Figure 4-6 presents the results.

4.3 Scattering and Pigment Content

145

Fig. 4-5. S versus s plots for six white pigments.

Fig. 4-6. Linearization of the S versus s curves of Figure 4-5.

The measured points fall quite well on straight lines, providing statisfactory confirmation of the geometrical-empirical formula to the anticipated accuracy. From the intercepts y (0) = y0 and x| y?0 = x0, equation (4.27) gives the parameters s and g: s = y0 ;

g

1 x0 y0

(4.28)

146

4 How Light Scattering and Absorption Depend on the Content ¼

A knowledge of x0 and y0 makes it quite simple to find the coordinates of the maximum.* Equation (4.23) is of fifth degree in s1/3 and, for this reason, cannot be solved explicitly for s. We do not have to propose a graphical solution procedure here, for any desktop computer can be programmed to solve for s by an iterative method given S, g, and s. It must be stated that the simple theoretical model performs well and has been confirmed again and again to within the claimed accuracy. As required by the Kubelka-Munk theory, the relation derived here for the example of white pigments essentially describes pure scattering behavior ± regardless (in the terms of our discussion up to now) of whether absorption takes place along with the scattering. It can therefore be expected that the derived equation will also be valid for layers with colored pigments.

4.4

Systematic Treatment of Pigment/ Achromatic Paste Mixing

4.4.1 Standard Methods of Pigment/Paste Mixing The mixing of pigments with a black or white paste and the colorimetric assessment of the mixture are governed by certain laws, which can be formulated quite generally, regardless of whether the case involves black and colored pigments in a white paste or white pigments in a black paste. This general relationship has not been discussed a great deal; it is based on physical and colorimetric principles that are common to all pigment/paste mixtures. This section will propose a systematic description of mixing methods and state a conservation law for each method. Systematization is needed all the more as a large number of determination methods are employed in practice (see Chapter 8) and no overarching relationship has been seen between these. But such a generalization would seem necessary to the further rationalization of pigment testing methods. The development begins with a system (ªpasteº) that already contains a black or white pigment (ªachromatic pigmentº). The problem is to mix or grind this paste with another pigment (ªtest pigmentº) in such a way that a series of increasing or decreasing pigment volume concentrations of the test pigment are obtained. Several approaches can be taken to this problem; these can be unambiguously delimited

* Equations (4.25), (4.27), and (4.28) immediately yield xmax = 0.6 x0, ymax = 0.4 y0 . In the linearized plit, in other words, the maximum of the S versus s curve liest at 60 % of the x axis intercept and at 40 % of the y axis intercept.

4.4 Systematic Treatment of Pigment/Achromatic Paste Mixing

147

and thus distinguished. These distinctions are not always manifest in the literature, and both vagueness and wrong conclusions have sometimes resulted. Just three methods of pigment/paste mixing are of practical interest. These are, in a sense, three prototypes to which the few remaining methods can also be reduced in principle. At present, however, the three standard methods have no names. So that they can be told apart in the further discussion, the following names are therefore introduced: ± Constant volume method ± Adding pigment method ± Dilution method Every mixture of test pigment and paste is a three-component system comprising the test pigment, the achromatic pigment, and the medium. The new concepts will be explained in what follows, and characteristic features and typical conservation laws for these methods will be stated. The following terminology will be employed: ) s = PVC of test pigment in the mixture sUP = volume concentration of achromatic paste sU = PVC of achromatic pigment (sU = sUPsU0) sU0 = PVC of achromatic pigment in the achromatic paste Constant volume method. In this method, care is taken to make the PVC of the achromatic pigment equal in all mixtures. On moving to a lower PVC of the test pigment in the mixture, the reduction in pigment volume is always made up by the same volume of medium. In other words, the total volume of the mixture is held constant by adding a calculated quantity of binder (Fig. 4-7 a). The conservation law is thus sU const

(4.29)

Adding pigment method. An equal quantity of the achromatic paste is measured out every time in this method, and increasing masses of the test pigment are added to such equal-sized portions. The three-component system is reduced to a binary system in this way, and the conservation law can be drawn directly from Figure 4-7 b: s + sUP 1

(4.30)

Dilution method. The third way of preparing mixtures with decreasing PVC of the test pigment is to take an already ground mixture of pigment with achromatic paste and dilute it down by adding vehicle. Neither the PVC of the achromatic pigment nor the PVC of the test pigment is held constant. What does remain constant is the

148

4 How Light Scattering and Absorption Depend on the Content ¼

Fig. 4-7. The three standard methods of pigment /paste mixing.

ratio between the PVC values of the achromatic pigment and the test pigment (Fig. 4-7 c). Accordingly, the conservation law for the dilution method is: sU sUA const s sA

(4.31)

where subscript A identifies initial values (before dilution).

4.4.2 Importance of the Methods The adding pigment method plays a prominent role because it forms the basis for defining the tinting strength and lightening power (Section 4.6 and 4.7). Weighed quantities of the test pigment are added to equal-sized portions of an achromatic substrate until the mixture visually matches a reference mixture. When this is not done, for example when pigment/achromatic paste mixtures for tinting strength or lightening power determination are prepared by the constant volume method, the values obtained can be expected to differ from the classical values according to the adding pigment method. International standards do not consistently embody a rigorous enough treatment of this point. In view of its importance, the adding pigment

4.4 Systematic Treatment of Pigment/Achromatic Paste Mixing

149

method is also discussed very thoroughly in the subsequent analyses of tinting strength and lightening power. The other two methods have gained some importance in testing practice; this is particularly true of the constant volume method, because it alone permits the PVC of the achromatic pigment to be held constant (conservation law, equation 4.29). This point is important for the relation, derived from the Kubelka-Munk function, between F = K / S and the PVC s of the test pigment. When testing is done with white paste, the constant PVC of the white pigment means that the scattering coefficient S remains virtually unchanged in the mixtures, because the white pigment is dominant. As a result, a plot of F versus s gives a straight line, because the absorption coefficient K is linear in s up to high PVC, as was shown earlier (see Fig. 4-2). Similarly, when white pigments are tested in black paste, the constant PVC of the black pigment in the mixture means that the absorption coefficient K remains unchanged; if 1/F = S / K is plotted versus s, the curve has practically the same shape as the S versus s curve, but this is linear only for low PVC (ªBeer's law rangeº; see Fig. 4-3). The dilution method is also liked by practicians because it involves only one pigment/paste grinding operation. Here again, however, it must be kept in mind that matching of two such paste mixtures for tinting strength or lightening power may give a somewhat different result from the match obtained with the adding pigment method. Not much remains to be added about other methods for pigment/paste mixing. By analogy with the constant volume method, in which the PVC of the achromatic pigment is held constant, one might seek a method in which the PVC of the test pigment remains constant. This is possible if one adds decreasing portions of paste to equal-weight portions of the pigment, adding vehicle to make up for each decrement in paste volume. The method just described is rather uninteresting, because with s = const the PVC of the pigment under study can no longer be varied. The quantity varied is the PVC of the achromatic pigment, so that the technique is a reciprocal variant of the constant volume method with the achromatic and test pigments interchanged. The discussion implies a further possibility, if fixed paste portions and variable pigment portions are replaced by fixed pigment portions and variable paste portions added to them. A closer, examination, however, reveals that this method is not a novel one but is identical with the adding pigment method, since once again a two-component system is involved while the mass balance (conservation law eq. 4.30) is unchanged. Other methods, for instance one using no achromatic stock paste ± weighed portions of achromatic pigment, test pigment, and binder being brought together ± are likewise of little interest and so will not be discusses separately. Practical experience shows that colorimetric data for the tinting strength or lightening power can be determined with certainty only if at least the achromatic pigment is incorporated into the medium in a separate operation. What is more, such methods also lead away from the classical tinting strength match and may give rise to dubious results, e. g., the Reynolds method for lightening power, formerly much used, in which

150

4 How Light Scattering and Absorption Depend on the Content ¼

s + sU = const. Individually, such methods can be related back to one of the three prototypes; the Reynolds method is then seen to be a derivative of the adding pigment method, though not identical with is.

4.5

Kubelka-Munk Functions of Pigment/ Paste Mixture

4.5.1 General Formula The discussion in Section 4.2 and 4.3 leads directly to a formula for the KubelkaMunk function of a pigment/paste mixture if the components of K and S are known: F l

K l KF l KW SF l SW S l

(4.32)

in which subscript F refers to the colored or black pigment and W to the white pigment. At this point, it is unnecessary to include a further interaction term in the denominator to take account of dependent scattering (see Section 4.3), provided one of the two scattering contributions is small in comparison with the other. Table 4-5 compares the magnitudes of the several terms for typical pigment/paste mixtures. KF in the numerator and SW in the denominator are seen to be the dominant terms. This fact suggests that the Kubelka-Munk function might be calculated with the dominant terms (KF /SW) and the deviations taken care of by perturbation terms depending on the weaker terms KW and SF. The l dependences shown in equation (4.32) hold only for colored pigments; they can be ignored for black pigments, so that F itself becomes independent of l. From equation (4.32) it is now possible to derive the Kubelka-Munk functions for pigment/paste mixtures obtained by the three standard mixing methods, both for white pigments in black paste and for black or colored pigments in white paste. The equations of Sections 4.2 and 4.3 for the concentration dependences of K and S are used for the purpose. Aside from the scattering and absorption coefficient per unit concentration, the equations to be derived contain only the concentration of the test pigment; first and second approximations for the three standard mixing methods are obtained from them. The approximations are arrived at by expanding the Kubelka-Munk function as a power series in the test-pigment concentration and then truncating after the linear and quadratic terms, respectively. Because the later terms are much smaller than the linear term of the first approximation, they take on the character of perturba-

151

4.5 Kubelka-Munk Functions of Pigment/Paste Mixture Table 4-5. Typical values of the quantities in equation (4.32). Carbon black pigments, sb = 0.01 In black paste

Absorption coefficient referred to PVC, k, mm±1 Scattering coefficient referred to PVC, s, mm±1

*20000 10

Absorption coefficient K, mm±1 Scattering coefficient S, mm±1 Kubelka-Munk function F Reflectance (corrected) R (l)

Tested in white paste, sw = 0.2 sw =2000 mm±1

*2000 200

TiO2 pigments, sw = 0.2

Colored pigments, s = 0.05

Tested in In white white paste, paste sw = 0.2 sw =2000 mm±1 200 ¼ 20000

5

*2000

Tested in black paste, sb = 0.01 kb =20000 mm±1 *20000 *2000

10 ¼ 1000

1

200

0.1

400

400

400

2000

0.5

0.02 ¼ 2

0.002

0.5

0

0.4

0.2 ¼ 0.8

0.9

0.4

tions and can be handled as corrections to the linear leading term. The result is a advantage for the experimental determination of the perturbation coefficients: the corrections terms in perturbation calculations do not have to be very accurate, i. e., they can exhibit a relative error greater than that of the leading term without impairing the value of the correction.

4.5.2 Black Pigments Mixed with White Paste For black pigments*, by equations (4.20) and (4.23), KF l k s ; SF l s s 1

2

g s3

(4.33)

where g = gs. The Kubelka-Munk functions for the standard mixing methods are obtained by applying the conservation law for each method. Constant volume method. The conservation law in equation (4.29) is sw = const, so that by the equations (4.20) and (4.23) Kw = const and Sw = const. Substitution in equation (4.32) yields the following expression for the Kubelka-Munk function Fb,c * The following convention should always be observed: symbols with no subscript refer to the pigment being tested.

152

4 How Light Scattering and Absorption Depend on the Content ¼

(the first subscript b denotes black pigment, the c stands for the constant volume method): k s1 k s Kw Kw Kw Fb;c 2 2 s Sw s s 1 g s 3 Sw s 1 g s3 1 Sw KW /SW = FW is the Kubelka-Munk function of the white paste after the addition of medium to restore constant volume (i. e., the system without black pigment). The development in the preceding section implies that the second summand in the denominator is very small compared to 1, so that the quotient can be truncated after the second-order term to obtain: # " 2 k s s 5 s s1 1 sg s3 s2 . . . Fb;c FW Kw Sw Sw Sw Multiplying out the brackets and neglecting the terms of order higher than 2 yields: k s s 5 s k s 2 s3 sg s 1 Fb;c FW Kw Sw Sw Sw Kw Sw and, finally, the PVC-dependent Kubelka-Munk function for black pigment/white paste mixtures prepared by the constant volume method: 2 Fb;c

FW

2 cb1 s 1 cb 5 s 3 3

cb2 s

(second approximation)

(4.34)

The coefficients in this equation have the following meanings: cb1

1 k Sw

cb 5 gFW 3

cb2

s Sw

k

k FW s 1 Sw

FW Fb;PU

k Sw

s FW F g g W Fb;PU FW Fb;PU FW s (4.35)

where Fb,PU = k/s = (K / S) | s?0 is the Kubelka-Munk function of the black pigment full shade for PVC in the Beer's law range.

153

4.5 Kubelka-Munk Functions of Pigment/Paste Mixture

Similarly, the first approximation is obtained from equation (4.34) by neglecting terms in higher powers than 1 (which are always very small in comparison with 1) as well as the additive term FW (which is always very small in comparison with Fb,c): 1 Fb;c cb1 s

k s Sw

(first approximation)

(4.36)

Thus, from well-defined premises, we have rigorously derived the well-known linear dependence of the Kubelka-Munk function (first approximation) on PVC for black pigment/white paste mixtures. A far simpler way to reach the same result, of course, is to ascribe all scattering by the paste mixture to the white paste and all absorption by the mixture to the black pigment, as indicated by the right-hand expression in equation (4.36). This procedure, however, leaves it unclear what simplifications have been made and whether these are reasonable. Adding pigment method. The conservation law for this method, from equation (4.30), is s + sWP = 1 (where sWP is the volume concentration of the white paste after addition of the black pigment). The PVC of the white pigment sw in the mixture must be calculated from sWP ; the formula is sw s0w sWP

(4.37)

where s0w is the PVC of the white pigment in the white paste. By the conservation law, it follows that: KW kw sw kw s0w sWP kw s0w (1 ± s) SW

sw sw 1

2 3

h

gw sw sw s0w 1

sw s0w 1

s 1

gw s0w 1 2 3

s 1 2 s 3

2 3

gw s0w 1 1 2 s ... 9

s

2 3

i

After substitution in equation (4.32), the numerator and denominator are divided by 1 ± s; this causes the pigment/medium volume ratio c = s/(1 ± s) (PMV, eq. 4.6) to appear in the numerator and denominator. The PMV thus becomes the appropriate measure of the pigment portion for the adding pigment method, and so the remaining PVC expressions are also replaced by s = c/ (1 + c) & c (1 ± c) (eq. 4.15). Now Fb,a (subscript a for adding pigment method), once again with terms of higher order neglected, becomes Fb;a

sc 1

gc

2 3

k c kw s0w 2 3 sw s0w 1 gw s0w 1

2 c 1 3

c

1 2 c 9

154

4 How Light Scattering and Absorption Depend on the Content ¼

Here kw s0w = KWP in the numerator is the absorption coefficient of the white paste, while isolable expression sw s0w (1 ± gw s2/3 0w ) = SWP is the scattering coefficient of the white paste. The quotient KWP /SWP = FWP denotes the KubelkaMunk function of the white paste, so that Fb;a

k c1 KWP FWP 5 5 1 2 s 3 1 s gw sw s0w c3 c g SWP 3 SWP

5 sw 53 2 gw s c SWP 0w 9

Once again, the quotient expression can be truncated after the quadratic term, because all the summands after the 1 in the denominator are much smaller than 1. Thus the Kubelka-Munk function for black pigment/white paste mixtures prepared by the adding pigment method is 2 Fb;a

FWP

2 zb1 c 1 zb 5 c 3 3

zb2 c

(second approximation)

(4.38)

Rather than write exact expressions for the coefficients, we write them after dropping terms that contribute practically nothing: zb1

k SWP

s FWP FWP g 3 Fb;PU k s 2 sw 53 s s0w zb2 1 gw s SWP 3 SWP zb 5 g

(4.39)

(approximation for black pigments with high light-scattering power, with Fb,PU = k/s = (K/S) | s?0, where Fb,PU is the Kubelka-Munk function of the black pigment full shade in the Beer's law range). About the first approximation, the same statements can be made as in the case of the constant volume method, and the same conclusions drawn, but referred to the PMV: 1

Fb;a zb1 c

k SWP

c

(first approximation)

(4.40)

A comparison of these equations with equations (4.34) and (4.36) for the constant volume method shows that the expressions are completely identical (aside from the

4.5 Kubelka-Munk Functions of Pigment/Paste Mixture

155

reference to PMV), even up to equality of the coefficients (though after simplification)*. Dilution method. The conservation law here is sw /s = const = swA /sA (where the subscript A marks initial values before dilution). Accordingly, equation (4.32) can be written again with s canceled out of the numerator and denominator:

1 Fb;d

ss 1

gs

2 3

sw

" swA s 1 sA

ks kw " ssA 1

2 3

gsA

s sA

gw

#

2 3

s

2 3

swA s sA

2 # 3

swA sA

" sw swA 1

2 3

gw swA

s sA

2 # 3

k sA kw swA

To find the initial value of the Kubelka-Munk function, one stets s ? sA : 2 2 3 3 ssA 1 g sA sw swA 1 gw swA 1 FA k sA kw swA With qD = s/sA, dividing by the first equation and neglecting higher-order terms gives the Kubelka-Munk function for black pigment/white paste mixtures prepared by the dilution method: Fb;d FA

1 1

ub

2

ub qD3

ub 1

1

2 3

qD

(first approximation)

(4.41)

where qD = s/sA is the dilution ratio by volume and FA is the initial value before dilution. This formula has just one coefficient: 5

5

3 2 g ssA3 gw sw swA 3 gw swA ub ssA sw swA

(4.42)

The simplification at right is obtained because we always have swswA 4 ssA (see also Table 4-5). * Here it must be noted that Fb,c and Fb,a are nonetheless two distinct functions; Fb,c is still the KubelkaMunk function of the constant volume method, even when s is replaced by s = c/ (1 + c), and similarly for Fb,a. Likewise, FW and FWP are not the same quantities.

156

4 How Light Scattering and Absorption Depend on the Content ¼

Equation (4.41) is a ª2/3º approximation implied by the second approximation. The zero-th approximation is obtained for s ? 0, that is, infinite dilution: Fb;d ? 1 FA

ub

and is of little interest.

4.5.3 White Pigments Mixed with Black Paste By equations (4.20) and (4.23), the following hold for white pigments*: 2 KW k s ; SW ss 1 g s 3

(4.43)

where g = gs. The Kubelka-Munk functions for the standard mixing methods are once more found by imposing the conservation laws. Constant volume method. The conservation law sb = const now implies Kb = const and Sb = const. For the Kubelka-Munk function Fw,c , equation (4.32) then yields 2 3 s s 1 g s Sb 1 k s Kb Fw;c (where it is advantageous to use the reciprocal). The procedure is now similar to that in Section 4.5.2: Extraction of the Kubelka-Munk function of the black paste (after addition of medium to restore constant volume), Kb/Sb = FB ; division by the denominator; truncation after the second-order term. The result is: 1 2

Fw;c

1 cw1 s 1 FB

cw 5 s

2 3

3

cw2 s

(second approximation)

(4.44)

the PVC-dependent Kubelka-Munk function for white pigment/black paste mixtures prepared by the constant volume method. As in the preceding section, the first approximation is obtained by dropping the higher powers and the 1/FB term: 1 1 Fw;c

cw1 s

s s Kb

(first approximation)

* Quantities relating to the white pigment have no subscripts here.

(4.45)

4.5 Kubelka-Munk Functions of Pigment/Paste Mixture

157

The coefficients now have the following meanings: 1 s k s cw1 Fb Sb Kb Kb cw 5 g 3

cw2

Fb

Fb g Fw;PU

k Kb

(4.46)

where Fb = Kb /Sb and Fw,PU = k / s = (K / S) | s?0 (the Kubelka-Munk functions of, respectively, the black paste and the white pigment full shade in the Beer's law range). Equation (4.45), the first approximation of the Kubelka-Munk function for white pigment/black paste mixtures, expressed as a function of concentration, is ± like equation (4.36) ± one of the most frequently used formulas. Adding pigment method. With the conservation law sBP + s = 1 and the PVC equation for the black pigment, (4.47) sb sBP s0b where s0b is the PVC of the black pigment in the black paste, the derivation of the approximations is similar to the development in Section 4.5.2. The Kubelka-Munk function for white pigment/black paste mixtures prepared by the adding pigment method is 1 2

Fw;z

1 zw1 c 1 FBP

zw 5 c 3

2 3

zw2 c

(second approximation)

(4.48)

or, after dropping higher powers and the 1/FBP term, 1 1 Fw;z

zw1 c

s c KBP

(first approximation)

(4.49)

where the coefficients (approximate values) are s 2 s 53 s 1 gb b s0b zw1 s KBP 3 KBP zw 5 g 3

zw2

k 5 s 53 k gb b s0b s KBP 9 KBP

(4.50)

158

4 How Light Scattering and Absorption Depend on the Content ¼

(approximations for black paste pigments with low light-scattering power, such as carbon black; KBP is the absorption coefficient of the black paste). Dilution method. The conservation law for this method is sb /s = const = sbA /sA (subscript A referring to initial mixture before dilution), so a derivation similar to that in Section 4.5.2 yields the Kubelka-Munk function for white pigments in black paste: Fw;d 1 FA

2 3

uw 1

(4.51)

qD

where FA is the initial value and qD = s/sA is the dilution ratio by volume; the coefficient is 5

5

3 2 gssA3 gb sb sbA g sA3 uw ssA sb sbA

(4.52)

The simplified form at the extreme right holds because we always have ssA 4 sb sbA .

4.5.4 Colored Pigments Mixed with White Paste The l dependence of absorption and scattering has to be considered for colored pigments. The formulas can be found in Section 4.5.2, where the l-dependent quantities are identified as such. Constant volume method. From equations (4.32) to (4.36), the spectral KubelkaMunk function for colored pigments is 2

Fc l

2

FW c1 l s 1 c 5 l s 3 3

c2 l s

(second approximation)

Fc(1) (l) c1 (l) s

(first approximation)

where the coefficients (higher-order terms being dropped) are

(4.53)

(4.54)

4.5 Kubelka-Munk Functions of Pigment/Paste Mixture

c1 l

k l SW

c 5 l g l 3

c2 l

159

s l SW

FW FPU l (4.55)

With regard to the Kubelka-Munk function of colored pigments, however, there is a second aspect of great interest; the question whether Kubelka-Munk functions can be written for the CIE tristimulus values X, Y, Z. If so, there will be a appreciable benefit, for these ªbroad-bandº quantities* could be directly represented as functions of the pigment concentration. This would be wholly similar to what was done for the spectral Kubelka-Munk functions. That this can indeed be done will now be demonstrated for the CIE tristimulus value Y. We start with the l-dependent quantities of equations (4.53) to (4.55): 2 FW 3 c2 ls . . . (4.56) c1 l s 1 c 5 l s Fc l FW Fc l 1 Fc l 3 For an experimental determination of the Kubelka-Munk function to the required accuracy, the spectral reflectance R (l) of the colored pigment/white paste mixture (see Section 3.3.2 and Fig. 3-9) must lie in the range of 0.20 ^ R (l) ^ 0.75. With this restriction and except for the upper part of the range (0.55 ^ Rin ^ 0.75), equation (3.118) implies that ln F = A ± BR . Further, the additive term FW /Fc (l) is small enough compared to 1 that Fc (l) in the formula can be replaced by the first approximation F(1) c (l) = c1 (l) s. Taking logarithms on both sides of the equation leads to 2 FW ln c1 l ln s c 5 l s 3 c2 l s . . . (4.57) A BR l c1 l s 3 On both the left-hand and right-hand sides, the approximate rule ln (1 + e) & e (for small quantities) has Rbeen used. In order to get to the CIE tristimulus value Y, the colorimetric integral yN (l) ¼ dl is applied on both sides of the equation (where yN (l) denotes the CIE color matching function y (l) normalized to the CIE standard illuminant N, that is, already divided by 100). Upon integration, quantities indepenR dent of l remain constant, since yN (l) dl = 1.

* The CIE tristimulus values X, Y, Z (or the reflectometer values R'x, R'y, R'z) are not spectral values now, as required by the Kubelka-Munk theory; instead, each corresponds to a broad band of wavelengths from which it was derived.

160

4 How Light Scattering and Absorption Depend on the Content ¼

Z FW yN l dl A s c1 l R R 2 R y N l ln c1 l dl ln s s 3 y N l c 5 l dl s yN l c2 l dl . . . Y B 100

3

Here Y is the CIE tristimulus value in the interior of the paste (actually Y , but this notation has already been claimed by the value function in the CIELAB system). The three integrals onR the right-hand side are now written by turns as ln c1, c5/3, c2. Now 1/c1 = exp (± yN (l) 7 ln c1 (l) dl); because exp (±ln x) = 1/x, an obvious substitution for the remaining integral on the left is Z y N l 1 dl e c1 l c1 where e is a perturbation term. If this expression is substituted in the equation, the resulting term eFw /s will certainly be small of higher order than the already very small term Fw /(c1 s) and thus can be neglected. Then A

B

Y 100

FW 2 ln c1 ln s c 53 s 3 c1 s

c2 s

A comparison with equation (4.57) reveals full agreement if the following substitutions are made: R (l) by Y /100, c1 (l) by c1, c5/3 (l) by c5/3, and c2 (l) by c2. It is thus possible to go back through the steps from equation (4.57) to (4.56) in reverse order. An equation like (4.56) with the above substitution is obtained. Now the same arguments can be repeated for the other two CIE tristimulus values X and Z in order to obtain similar formulas. Listing all three equations together, we then have the Kubelka-Munk functions of the CIE tristimulus values for colored pigment/white paste mixtures prepared by the constant volume method: 2 FXc 2 FYc 2 FZc

2 FW cX1 s 1 cX 5 s 3 3 2 FW cY1 s 1 cY 5 s 3 3 2 FW cZ1 s 1 cZ 5 s 3 3

cX2 s cY2 s cZ2 s

(4.58)

(second approximation) and 1 FXc cX1 s ;

1 FYc cY1 s ;

(first approximation)

1 FZc cZ1 s

(4.59)

4.5 Kubelka-Munk Functions of Pigment/Paste Mixture

161

where the coefficients are cX1 e cY1 e

R R

x N lln c1 l dl y N lln c1 l dl

R cZ1 e zN lln c1 l dl R cX 5 x N l c 5 l dl 3 3 R cY 5 y N l c 5 l dl 3 3 R cZ 5 zN l c 5 l dl 3 3 R cX2 x N l c2 l dl R cY2 y N l c2 l dl R cZ2 zN l c2 l dl

(4.60)

xN (l), yN (l), and zN (l) being the CIE color matching functions normalized to CIE standard illuminant N. The Kubelka-Munk functions described by equations (4.58) and (4.59) are not identical to the colorimetric integral Rover F (l); in accordance with equations (4.57) ff. they are defined as F X = exp ( xN (l) 7 ln F (l) dl), etc. These are related in the following way to the CIE tristimulus values from the corrected reflectance:

F Xc

F Yc

F Zc

1

2

1

2

1

2

X Xn X 2 Xn

Y 100 Y 2 100

Z Zn Z 2 Zn

(4.61)

162

4 How Light Scattering and Absorption Depend on the Content ¼

where Xn and Zn are the CIE tristimulus values for the standard illuminant and X R x N l R l dl Xn Y R yN l R l dl 100 Z R zN l R l dl Zn

(4.62)

These results complete the proof that the concentration-dependent Kubelka-Munk functions of the CIE tristimulus values can be described by the same formulas commonly used for the spectral values or black pigments (see the above argument and Section 4.5.2), provided the restriction 0.1 5 Rin(l) 5 0.55 is imposed. But this is not an onerous restriction, since in striving for accuracy one will always make certain to take quantities of paste and pigment such that Rin(l) will lie in this range. Adding pigment method. First, the spectral Kubelka-Munk function for colored pigments is 2 Fa l

FWP

2 z1 l c 1 z 5 l c 3

z2 l c

(4.63)

(first approximation)

(4.64)

3

(second approximation)

1

Fa l z1 l c

k l c SW

where the coefficients (without higher-order terms) are z1 l

k l SWP

z 5 l g l 3

FWP FPU l

s l 2 sw 53 s l s0w 1 gw z2 l s l SWP 3 SWP (approximation for colored pigments with high light-scattering power).

(4.65)

4.5 Kubelka-Munk Functions of Pigment/Paste Mixture

163

With regard to the Kubelka-Munk functions of the CIE tristimulus values for the adding pigment method, the same arguments as cited above for the constant volume method lead to similar results, the Kubelka-Munk functions of the CIE tristimulus values of colored pigment/white paste mixtures prepared by the adding pigment method: 2

F Xa 2

F Ya 2

F Za

2 FWP zX1 c 1 zX 5 c 3 3 2 FWP zY1 c 1 zY 5 c 3 3 2 FWP zZ1 c 1 zZ 5 c 3

(second approximation)

zX2 c zY2 c zZ2 c

3

(4.66)

und 1

1

F Xa zX1 c ; F Ya zY1 c ;

1

F Za zZ1 c

(4.67)

(first approximation) where the coefficients are zX1 e zY1 e

R R

x N lln z1 l dl y N lln z1 l dl

R

zZ1 e zN lln z1 l dl R zX 5 x N l z 5 l dl 3 3 R zY 5 y N l z 5 l dl 3 3 R zZ 5 zN l z 5 l dl 3 3 R zX2 x N l z2 l dl R zY2 y N l z2 l dl R zZ2 zN l z2 l dl

(4.68)

Equations (4.61) and (4.62) with appropriate substitutions hold for F Xa, FYa, and F Za.

164

4 How Light Scattering and Absorption Depend on the Content ¼

Dilution method. The spectral Kubelka-Munk function of colored pigment/white paste mixtures, similarly to equation (4.41), are u l 1

Fd l 1 FA l

2 3

qD

(4.69)

where qD = s/sA, FA (l) being the initial value before dilution, and the coefficient is 5

5

3 5 g l s l sA3 gw sw swA 3 gw swA u l s l sA sw swA

(4.70)

Now the Kubelka-Munk functions of the CIE tristimulus values will again be derived. Starting with equation (4.69), we proceed as we did before, taking logarithms to get to the proven equality ln F = A ± BR*, we once more apply the approximations for small quantities on the right-hand side: 2 3 (4.71) B R l RA l 1 qD u l R

Application of the colorimetric integral B Y 100

YA

yN (l) ¼ dl leads immediately to

1

2 3

Z

qD

y N l u l dl

and formal identity with equation (4.71). From here, the steps are repeated in reverse order, yielding the Kubelka-Munk functions of the CIE tristimulus values for colored pigment/white paste mixtures prepared by the dilution method: F Xd 1 F A;Xd F Yd 1 F A;Yd

u X 1 u Y 1

F Zd 1 u Z 1 F A;Zd (qD s/sA)

2

qD3 2 3

qD 2 3

qD

(4.72)

where F A,Xd, F A,Yd, and F A,Zd are the Kubelka-Munk functions of the initial CIE tristimulus values and the coefficients are given by

4.6 Tinting Strength

u X u Y u Z

R R R

165

2

3 x N l u l dl gw swA 2

3 y N l u l dl gw swA 2

3 zN l u l dl gw swA

(4.73)

Equations (4.61) and (4.62), suitable modified, holdF Xd ,FYd , andF Zd . Thus the concentration dependence of the Kubelka-Munk functions of CIE tristimulus values for colored pigments by the dilution method is described by the same law as for black pigments.

4.6

Tinting Strength

4.6.1 Significance and Definition Tinting strength is a fundamental characteristic of coloring materials. It describes one of the most important optical qualities of dyes and pigments in the form of an ªeffectivenessº criterion and is continually used for optical performance comparisons of pigments and dyes. The assessment of the optical performance of pigments is commonly based on the tinting strength and hiding power in a stated medium. When the price is then taken into consideration along with the optical performance, conclusions can be drawn about the economics of a pigment (ªmoney valueº; see Section 7.4.4). As a rule, however, the determination of hiding power involves appreciable experimental effort. It appears much easier to determine the tinting strength, and a first examination reveals no problems in doing so; this approach is normally preferred, even if tinting strength and hiding power do not necessarily lead to the same economic results. Tinting strength is defined as ªa measure of the ability of a coloring matter to impart color, through its absorbing power, to other substancesº*. If one understands a definition as simultaneously being an instruction, telling how to carry out a determination implied by the definition, one comes to a surprising conclusion here: current testing specifications, without exception, define (i. e., tell how to determine) only a ªrelative tinting strengthº relative to a reference coloring matter. The justified question of absolute tinting strength remains largely unanswered, and existing standards say little about it. We can only return to this interesting question further on and seek an answer to it then.

* For standards see ªTinting Strength, Relativeº in Appendix 1.

166

4 How Light Scattering and Absorption Depend on the Content ¼

The concept and definition of relative tinting strength are worded differently for dyes and pigments and at first glance they do not seem to be identical. For dyes, the relative tinting strength is the ratio of the extinction coefficients for the test and reference dyes measured at the absorption maxima of the solutions: Pd

k00b

k00b;R

(4.74)

(Because there is no scattering, the extinction coefficients are equal to the absorption coefficients per unit concentration by mass k@b .) The absorption curves for both dyes should be quite similar. In the pigment field, tinting strength applies only to black and colored pigments, and accordingly there has to exist an analog for white pigments: the ªlightening powerº. The procedural instruction (the ªstandard experimentº) based on the definition of tinting strength or lightening power runs as follows: each of the pigments to be compared is mixed into a white paste (into a black or blue paste for lightening power), and the portion of one of the two pigments is varied until the two drawdowns match, i. e., look the same to an observer. The tinting strength or lightening power is the weight ratio of reference pigments (mass mR) and test pigment (mass m) needed to achieve the same color quality in a white system or the same lightening in a colored system. Thus the defining equation for tinting strength and lightening power is P

mR m

DQ0

mFPconst

(4.75)

where DQ = 0 denotes a match and mFP is the constant portion of white or black paste. Tinting strength and lightening power describe true effectiveness properties, since a tinting strength a factor of two greater signifies that only half as much of this pigment is needed to achieve the same optical effect as with the reference pigment. It is common to supplement the notion of tinting strength with that of ªtinting equivalentº. This is the reciprocal of the tinting strength and thus tells how many parts of a test pigment will have a color-imparting effect equivalent to that of 1 part by weight of the reference pigment. Another way to explain this property is to say that the tinting equivalent is lower for more strongly coloring pigments and higher for less strongly coloring ones, corresponding to the smaller and larger portions of these pigments required. In a formulation calculation context, the tinting strength of a pigment is sometimes linked with its coloristic properties in a arbitrary pigment mixture. Thus one attempts to interpret the tinting strength as the fundamental pigment property for

4.6 Tinting Strength

167

formulation, namely as the substitution ratio when a formula is to be converted. A definition of tinting strength in this sense would not, however, be possible unless the system itself or some general principle of formulation systems were included in the definition. Even if it were, results under this definition would necessarily differ from those under the classical definition. In practice, this means that substitution ratios in general formulas need not be identical with the relative tinting strength (substitution ratio in white). It is essential to keep this point in mind when tinting strength measurements are used to answer questions in formulation calculations. Equation (4.75) provides a basis for a test specification. The standards here have retained the decades-old interpretation of the tinting strength concept as well as its definition, both of which are far older than the standards themselves. As a consequence of the definition, the test is performed in a light-scattering substrate, but for each substrate the vehicle as well as the white pigment must be specified. Today, nondrying vehicles containing a titanium dioxide pigment are common use. A method of tinting strength determination usable in practice must, of course, cover some further points, for example the test pigment concentration, because the relative tinting strength depends not only on the white pigment used and its concentration, but also on the concentration of the colored pigment in the test. The procedure ultimately used may differ in a variety of ways from the standard experiment described above. This fact may well conceal the latent presence of defining equation (4.75) and the system of the standard experiment. This holds, in particular, for photometric techniques derived from the standard experiment. In these methods, a rationalization profit is achieved because only one mixture of white paste with the test pigment need be prepared. As in the case of the hiding power, this economy is the great motivation for using colorimetric methods to determine tinting strength; but the problem of a colorimetric matching criterion arises ± the problem to be discussed now in Section 4.6.2.

4.6.2 Coloristic Matching Criteria for Pigments As has been shown, methods of determining the tinting strength for pigments specify that the reference and test mixtures with white paste are to be ªmatchedº through variation of the pigment portions; when the match is completed, they should appear alike to the colorist. Matching does not present any difficulties to the colorist when the pigments involved have very similar spectra, that is, when the differences in hue and saturation are small. When these differences are greater, criteria based on coloristic experience are applied; the uncertainty of the assessment unavoidably grows larger as the color difference increases. On the other hand, as the spectral curves become less and less similar, a point is soon reached where the determination of relative tinting strength ceases to be meaningful, because the test pigment is no longer such that it can replace the reference in a color formulation. It is thus reasonable to restrict tinting strength determinations and studies to small color differences.

168

4 How Light Scattering and Absorption Depend on the Content ¼

The question of a matching criterion to be used becomes acute (if indeed it has not done so already) when visual matching is abandoned in favor of a colorimetric method. The only way for the colorimeter, and the computer fed by it, to draw on experience comparable to that of the colorist is to render objective the criterion used by colorists. Not until the color quality that the colorist utilizes has been identified and quantified can instructions for the computer be embodied in program form. The problematic aspect of tinting strength determination can be expressed in the question: What colorimetric or physiological criterion governs the optimal replacement of reference by test pigment? There are cases in which the pigment being assessed is fully capable of replacing the reference pigment at a certain concentration; i.g., the color difference between the mixtures of the two pigments with white paste vanishes. With inorganic colored pigments and some organic pigments, however, this is the exception, because in most such cases the differences in tinting strength can mostly be attributed to differences in particle size and particle-size distribution, with the inevitable result of shifts in hue. Because these color differences between test and reference pigments do not result from differences in concentration or unequal tinting strengths, there is no concentration at which the color difference between the two will vanish. The question then arises: What criterion can be applied in order to find the mass ratio at which the reference pigment can be optimally replaced? Is the matching of absorption coefficients (of reflectances) at the absorption maximum (that is the reflection minimum) the proper criterion, as older methods suggest? Or, in the case of pigments differing in color nuance, is it better to seek the concentration such that the color difference between reference and test pigments is a minimum? The applicability test for these criteria is the agreement on the visual match among many colorists. If a working technique is specified and the portion of the test pigment is progressively increased, the resulting colors describe a three-dimensional curve in color space. This curve is called the ªtinting characteristicº of the pigment. If the method is to add a colored pigment to a white paste, say by the constant volume method, then as expected the three-dimensional curve begins near the white locus (color locus of white paste; PVC of colored pigment s = 0) and ends close to the colored pigment full shade (s 4 sw). The nature of the curve between these two points may vary greatly from one pigment to another and from one color range to another. For the CIELAB color space, the tinting characteristic for mixtures with a white preparation (ªreducing whiteº) can even be formulated analytically (though not explicitly). From the PVC-dependent reflection spectra R (l, s) of reducing whites, the CIE tristimulus values X (s), Y (s), Z (s) can be obtained, and from these the CIELAB color locus V (s) = {a (s), b (s), L (s)} can be determined. If the components of a vector depend exclusively on a single variable (s), a three-dimensional curve always exists. Figure 4-8 presents one example of a tinting characteristic for reducing whites. In Equation (4.75), the match is signified by DQ = 0. The quantity Q, the color difference between test and reference pigments, which is to be made equal to zero,

4.6 Tinting Strength

169

Fig. 4-8. Tinting characteristic of a copper phthalocyanine pigment, after a model due to Keifer. (The highest color locus corresponds to the white paste; the negative b axis points toward the observer.)

is called the ªtinting strength criterionº. The selected tinting strength criterion can usually be represented by equipotential surfaces in corlor space (see Fig. 4-9 for L* as tinting strength criterion). One of the pigments to be compared (constant portion by weight) fixes a certain equipotential surface, and the tinting characteristic of the other pigment (variable portion by weight) intersects this surface at a point. The point is the location of the match, and the pigment concentration at this point of the three-dimensional curve is the desired concentration at the match. It should be clear that the value of the tinting strength is more-or-less strongly influenced by what tinting strength criterion is chosen. Accordingly, one can no longer speak of just the ªtinting strengthº; there are as many values of tinting strength as there are tinting strength criteria in use. What follows is a survey of criteria.

170

4 How Light Scattering and Absorption Depend on the Content ¼

Fig. 4-9. Equipotential surfaces of lightness (tinting strength criterion L ) with tinting characteristic of a colored pigment in CIELAB color space.

Tinting Strength Criteria 1) Criteria definable in physiological and simultaneously colorimetric terms ± Lightness L (or CIE tristimulus value Y). This criterion does not require any further explanation. Both quantities, L and Y, lead to the identical match, since DL = 0 and DY = 0 have the same meaning. Figure 4-9 shows the CIELAB color space with equi-lightness surfaces drawn in (planes in this instance). The figure also indicates how the tinting characteristic of a colored pigment intersects the plane of the reference. ± Color depth T . The color depth is a measure of the ªcolorednessº (intensity) of a color perception.* It increases with increasing saturation, but decreases with increasing lightness. Accordingly, in the CIELAB color space, it can be approximately represented as the distance from the white locus (Lw = 100): q q 2 100 L 2 (4.76) T a2 b2 100 L 2 Cab Surfaces of constant color depth are thus spherical shells centered on the white locus, as shown in Figure 4-10. The above formula is, however, too rough for practical use. ± The smallest of the CIE tristimulus values X, Y, Z. This is the CIE tristimulus value that is most strongly governed by the absorption. ± The smallest of the reflectometer values R'x, R'y, R'z . this measure provides a simplification when measurement is done by the tristimulus method. ± Smallest possible color difference DE ab . This tinting strength criterion is already a difference, but it is to be minimized instead of made equal to zero. In the CIELAB color space, the mixture of the reference pigment with white represents a * The term originated in textile dyeing and was coined for use in fastness comparisons, which are to be done not at an equal dye concentration but at an equal ªdepthº of coloration.

4.6 Tinting Strength

171

Fig. 4-10. Equipotential surfaces for color depth (tinting strength criterion T ) with tinting characteristic of a colored pigment, plotted in the CIELAB color space.

point (color locus). On the tinting characteristic of the test pigment, the point is sought that is nearest to the reference color locus. ± Chroma difference DC ab . This criterion is of little importance but is included here to complete the systematic order. 2) Criteria derived from the Kubelka-Munk function F ± Maximum of the spectral Kubelka-Munk function Fmax (l) or minimum of the reflection spectrum Rmin (l). This is a variant of the ªsmallest CIE tristimulus valueº criterion. DFmax (l) = 0 and DRmin (l) = 0 lead to the same match; DRmin (l) is also the tinting strength criterion for dyes in solution.* ± Sum of the colorimetrically evaluated Kubelka-Munk functionsF x,y,z . This criterion is formulated as R F x;y;z x l y l z l F l dl

(4.77)

The sum of the CIE color matching functions, which is multiplied by F (l) has the form of a double-peaked curve (see Fig. 2-4) with a deep notch at 500 nm. It is not immediately obvious why the wavelengths around 500 nm are thus discriminated against in the summation. The criterion originated in the textile field and is used there for tests of dye strength (on the fiber). Recently if has been applied to the determination of the tinting strength of organic pigments (see Section 8.2.3). * Thus the definitions of tinting strength for dyes, equation (4.74), and for pigments, equation (4.75), are identical for this tinting strength criterion.

172

4 How Light Scattering and Absorption Depend on the Content ¼

± Averaged spectral Kubelka-Munk functionF. This is given by R F F l dl

(4.78)

and should take care of the objections raised in connection with the criterion F x,y,z. The integral must be formed by summation; the magnitude of dl is not crucial provided the mixtures with the test and reference pigments are formulated with the same dl. ± Smallest possible variance sum of the spectral Kubelka-Munk functions DF 2 (min), calculated as R R DF 2 min DF 2 l dl F l FR l2 dl ! min: (4.79)

4.6.3 Color Matching Studies One may naturally ask which, among these tinting strength criteria, is the ªrightº one ± or which comes closest to the coloristic match. Two studies have been published that shed some light on this problem; their results will appreciably aid in the selection of a suitable tinting strength criterion. Keifer and the author pursed the question of what criteria colorists apply to assess the tinting strength of inorganic pigments. Six pairs of inorganic pigments corresponding to the principal color directions red, yellow, blue, green, and in addition orange and black were chosen. In each pair, mixtures of the two pigments in reduction displayed a hue difference |DH ab | < 3 after matching. This procedure insured the ªreplaceabilityº of one pigment by the other in a coloration. Mixtures of the pigments with a white paint were prepared; the quantity of one pigment (ªtest pigmentº) was incremented 10 mg at a time, while the quantity of the other (ªreference pigmentº) was held constant. From each test pigment mixture and the reference pigment mixture (the same every time), side-by-side drawdowns were made with a Bird applicator; after these had dried, matching trials and color measurement were performed. Half of the evaluators were experienced colorists skilled in the determination of tinting strength of inorganic pigments; the other half were person who did not meet this qualification but who had done visual color matching before. One result can be stated immediately: The difference between the two groups was non significant. The overall result is therefore not influenced just by coloristic learning processes; it holds some universal significance. The color matchers were given the following question to answer: ªWhich drawndown seems to you to be the best match between reference and test pigments?º For the colorimetric evaluation, the following tinting strength criteria were tested in the study: L , DE ab and Rmin (l). Two forms of the color depth were used, T (eq. 4.75) and Ts according to Gall's improved color depth formula (Section 4.6.5). Figures 4-11 to 4-16 present the results in graphical form, with the various tinting strength criteria identified as in Section 4.6.2. From these graphs it is quite

4.6 Tinting Strength

173

Fig. 4-11. Comparison of tinting strength criteria with visual assessment (heavy arrow) for two red iron oxide pigments.

Fig. 4-12. Same as Figure 4-11, for two cadmium orange pigments.

Fig. 4-13. Same as Figure 4-11, for two yellow iron oxide pigments.

Fig. 4-14. Same as Figure 4-11, for two chromium oxide green pigments (both minima labeled Rmin (l)).

174

4 How Light Scattering and Absorption Depend on the Content ¼

Fig. 4-15. Same as Figure 4-11, for two ultramarine blue pigments.

Fig. 4-16. Same as Figure 4-11, for two black iron oxide pigments.

Fig. 4-17. Statistical analysis of the visual matching of chromium oxide pigments.

Fig. 4-18. Statistical analysis of the visual matching of cadmium orange pigments.

4.6 Tinting Strength

175

clear that the criterion DL = 0 gives the best agreement with the visual assessment (heavy arrow) for each of the six hues tested. The plots also show how much the tinting strength value obtained under the other criteria, which is proportional to the quantity of pigment, can diverge from the visual match. The larger deviations include those of the tinting strength criteria Rmin (l), T , and Ts. Even DE ab comes off poorly with regard to both the positions of the minima and the uncertainty (due to the weakly marked minima). To find out about the reliability of coloristic judgment, the frequency distributions for test pigment selection in color matching trials were calculated and plotted. Two of the resulting curves are presented here. For chromium oxide green (Fig. 4-17), the distribution is relatively narrow (under +1% of the tinting strength); for the more highly saturated cadmium pigment (Fig. 4-18), it is markedly broader (over +2 %). According to these results, coloristic judgment appears to be more reliable for unsaturated color in reduction. The other color matching study that needs to be discussed here is that carried out and reported by GALL, an investigation performed with great care and based on profound knowledge. It differs in several points from the Uerdingen study just described: ± Organic pigments were studied. ± Color depth was taken as the typical tinting strength criterion for the pigments in the study. ± In accordance with the objective, reducing whites were ordered by the specified levels of color depth. ± The color matchers were practiced in working with organic pigments (i. e., pigments commonly having higher color saturation). The samples comprised 18 resp. 22 pigments covering roughly the entire color circle. For every hue, there was a selection from a series of gradations in the concentration of colored pigment in reduction. A mixture (standard) made with a copper phthalocyanine pigment in reduction, adjusted to the specified textile color depth standard, was to be rematched in color depth with the other pigments. The task was as follows: ªFrom each concentration series, select a reducing white that best agrees in color depth ± with the blue standard and ± with the samples already color-matched to the standard.º The textile standards were identified, in the traditional way, with fractions of the ªstandard depth of shadeº (R. T.). the levels studied were 1/1, 1/3, 1/25, and 1/200 R. T. Mixtures with white at 1/3 R. T. made with a further 18 pigments (five red, four yellow, four green, five blue) and lying on ªhue profilesº (i. e., each having the same hue but different saturation) were also prepared and matched. The purpose of doing this was to determine the extent to which the colorist rates a decrease in saturation as an increase in tinting strength.

176

4 How Light Scattering and Absorption Depend on the Content ¼

Table 4-6 presents the matching results. The last column gives the frequency of the assessments falling in a concentration range of +10 % about the average value. It can be seen that the reliability of coloristic judgment is appreciably higher for saturated samples (i. e., the ones with higher CIE tristimulus values) than for unsaturated samles*. The table also shows that the luminance (tristimulus value Y) differs significantly between these samples, which were selected to have equal color depth; the differences are particularly marked in the case of yellow. Table 4-6. Color matching results along the 1/3 R. T. hue profile, after Gall. Color

X

Y

Z

H

Red, standard A B C D E

48.18 41.83 36.96 32.49 28.07 25.26

32.38 29.38 26.28 23.36 21.00 19.12

9.89 9.76 9.48 9.40 9.49 9.66

80 % 67 % 69 % 58 % 59 %

Green, standard A B C D

15.81 15.89 16.04 15.84 15.69

29.23 29.01 28.85 27.90 27.25

24.46 24.03 24.24 23.88 23.53

94 % 98 % 98 % 91%

Blue, standard A B C D E

17.38 16.63 16.41 15.83 15.26 13.94

20.70 19.86 19.78 19.04 18.88 18.72

63.82 60.59 57.72 55.93 50.98 45.76

98 % 96 % 92 % 86 % 78 %

Yellow, standard A B C D

62.05 58.25 56.43 54.75 50.84

64.76 61.39 59.74 57.92 53.97

15.35 15.97 15.83 15.75 15.78

88 % 85 % 78 % 64 %

These studies also included matching of the same samples by ªuneducatedº observers, who arrived at virtually the same results as experienced colorists. The goal of this investigation was the colorimetric establishment of the various color-depth levels. From the color coordinates of the experimentally determined color depths corresponding to the same level, improved formulas for color depth were obtained. The results of these two painstaking color matching studies of tinting strength may at first appear contradictory. How is it possible that one group of colorists uses * The terms ªbrilliantº, ªpureº, and ªhazyº have purposely not been applied to pigments here because they are ambiguous. Further, they appear to contain hidden value judgments.

4.6 Tinting Strength

177

lightness as the tinting strength criterion over a wide range of color depths, while the other group adjudges samples differing greatly in lightness to have the same color depth in the context of a tinting strength determination? The clear up the apparent contradiction, it is necessary to return to the assumptions and constraints in the two studies and the differences that result from them. Table 4-7 briefly sums up the key points for both studies. Different pigments were used: in one case, inorganic pigments, relatively unsaturated, mostly dark in full shade; in the other, organic pigments, relatively saturated in reduction. The inorganic pigments had smaller color differences between test and reference than did the organic pigments. Of the latter, Gall's colorists gave more reliable matches of the more saturated reductions than of the less saturated ones; it was just the other way around with the Uerdingen colorists, and in addition their judgment (because of the smaller color differences) was on the whole more reliable than that of the other group. Table 4-7. Summary of differences between the color matching studies. Study Aspect

Gall

Keifer/Vælz

Tested pigments

Organic pigments

Inorganic pigments

Generally 4 3

Generally 5 3

DE ab

test/reference in reduction after matching Colorists

Experienced in matching organic pigments inorganic pigments

Task

ªEqual color depthº

ªBest matchº

Objective

To improve color depth formulas

To identify best tinting strength criterion

Result

Improved formulas

Lightness

Reliability of judgment

Better on saturated samples than unsaturated

Better on unsaturated samples than saturated; generally much higher than in Gall's study

There would appear to be no arguing with the view that pigments in reduction giving higher saturations are well represented by the color depth as tinting strength criterion, while pigments in reduction giving lower saturations are better evaluated by the lightness as the tinting strength criterion. Another point in favor of this conclusion is that ªuneducatedº matchers in both studies came to almost the same results as experienced colorists ± which appears to prove that the assessment criteria used by the colorists cannot be purely learned ones. It must be kept in mind that the matching in Gall's study was done by colorists whose special experience, not just with organic pigments but also with the problems of formula conversion and rematching, was greater than that of the Uerdingen colorists. Accordingly, it cannot be ruled out that formulation experience influenced the formation of a ªcolor

178

4 How Light Scattering and Absorption Depend on the Content ¼

depthº judgment. This would mean that too much weight was placed on color nuance because it is commonly a serious problem in formula conversions. In turn, this leads too far in the substitution ratio direction in formulas and can lead away from the tinting strength, as was already stated in Section 4.6.1. One important point must not be neglected here: The more unsaturated the color of a pigment in reduction, in other words the nearer its color locus is to the lightness axis in color space, the closer are the two equipotential surfaces of lightness (horizontal plane) and color depth (spherical shell), which ultimately become identical on the lightness axis. Thus it has become usual to use lightness as the tinting strength criterion in evaluating inorganic pigments and color depth as the criterion for organic pigments. In the case of highly saturated yellow pigments, which scatter strongly, both criteria appear to fail; the reason may, however, be an expectation of the tester, who ordinarily uses inorganic yellow pigments less for coloring than for lightening, a function that is of course not regarded in the tinting strength evaluation. Finally, it should be asked why DE ab showed such poor performance in the Uerdingen study* when, as the smallest color difference, it should in face be the decisive criterion. It may again be that this expectation failed because of inadequacies in the CIELAB system. It has already been established that CIELAB regularly understates the lightness and overstates the saturation. A glance at any of Figures 4-11 to 4-16 will reveal what changes come about if DL is multiplied by a quite resonable factor of 4. The DL curve becomes far steeper, so that the DE ab curve is much more strongly dominated by DL ; as a consequence, the minimum of DE ab moves closer to the zero crossing of DL and also becomes more strongly marked. Thus tinting strength criterion min(DE ab ) practically coincides with DL = 0.

4.6.4 Lightness Matching In a rational method for tinting strength determination, a desirable feature would be that the value can be obtained by a simple calculation based on a single reducing white. Because measurements by the tristimulus method directly yield the measurement R'y = Y, the tinting strength criterion DL = DY = 0 indeed satisfies this wish. This section begins by deriving the equation of the relative tinting strength for the criterion Y as a function of the mass of the pigment. The fundamental equation (4.75) requires a relation between m and mR after matching to DY = 0. The Kubelka-Munk function expressed in terms of the PMV c is a suitable way to get mR as a function of m. This approach is particularly convenient, since the tinting strength criterion DY = 0 can obviously be replaced by the corrected values DY = 0 and finally by the Kubelka-Munk functions DF = 0, that is, by setting F = FR (test and reference). Unfortunately, this chain, which looks so plausible, has * According to a communication from Gall, no other known DE formula makes a suitable tinting strength criterion either.

4.6 Tinting Strength

179

a blemish in the form of a weak link. The problem lies in the step from Y = YR to Y = Y R , for R R DY Y YR y l R l RR l dl y l DR l dl 0 (4.80) does not necessarily imply that R DY Y YR y l R l RR l dl Z Z dR DR l dl y l y l DR l dl dR

(4.81)

vanishes. This becomes clear if substitution (3.11) is made for R , RR . The integral on the right would vanish identically with DY = 0 if the derivative dR /dR were constant. This also is nearly given: the factor lies between 0.4 and 2.6, and so there are contributions to the integral, but the crucial point is that these contributions, because of the Y matching performed, must have different signs in different regions of the spectrum, so that they practically cancel out. Figure 8±4 shows the spectra of two red iron oxide pigments in reduction after Y matching. The DR are positive for l = 420 to 540 nm but negative for l = 580 to 700 nm. A quantitative analysis of this example shows that DY 5 0.03 %, which is sufficiently close to zero. Though selected on purpose, this example is typical enough for reflection spectra if mixtures with white after Y matching that it can be generalized: DY** must always be small of higher order than Y and Y R as DY goes to zero. Thus, at a practical level of accuracy, there is justification for setting the two quantities equal, and there is no further obstacle to using the criterion DF = 0. The equations for the Kubelka-Munk functions in Sections 4.5.2 (black pigments) and 4.5.4 (colored pigments) have the same form and can therefore be handled together. The CIE tristimulus value Y for the adding pigment method is described by 2 (4.82) F FWP z1 c 1 z 5 c 3 z2 c 3

Here c = m/m is the volume ratio of pigment to white paste, in accordance with equation (4.6), with m given by equation (4.4): R (4.83) m m WP RWP where mWP and RWP are the mass and density of the white paste and R is the density of the test pigment. The notations F for the Kubelka-Munk function and zi for the coefficients appear in the following forms: F (2) b,a , zbi

for black pigments

F (2) Ya , zYi

for colored pigments

180

4 How Light Scattering and Absorption Depend on the Content ¼

A similar equation then describes the reduced reference pigment: FR

2

FWP zR1 cR 1 zR 5 cR3 3

where cR = mR /mR, mR mWP

zR2 cR

RR RWP

(4.84) (4.85)

and RR is the density of the reference pigment. For easily discerned reasons, the desired function mR (m), or in its place cR (c), must have a structure like that of F (c): 2 cR p0 c 1 p 2 c 3 p1 c DF0

3

After this expression is substituted in equation (4.84), coefficients can be compared with equation (4.82), since F is supposed to be equal to FR. The following are therefore obtained for the coefficients p i : z1 p0 zR1 2

p2 z5

p03 zR 5

p1 z2

p0 zR2

3

3

3

(4.86)

The fundamental equation for the tinting strength can now be written down. By equation (4.83) and (4.85), the requirement mWP = const implies that mR/m = RR /R, so that P 1

mR m

DF0 mWPconst

mR m

mWPconst

cR c

DF=0

" # 2 s 2 RR m 3 m R s 3 p0 1 p 2 p1 p1 R p0 1 p 2 R R m m s 1 s 3 3 1 (first approximation) (4.87) This is the desired equation for the relative tinting strength as a function of the quantity m or the PVC s of the test pigment. The zero-th approximation is obtained by setting higher-order terms equal to zero: P 0

RR p0 R

(zero-th approximation)

(4.88)

4.6 Tinting Strength

181

The coefficients are described again by equations (4.86). They can be experimentally determined by mixing three suitable quantities of pigment with equal quantities of white paste and matching the reference pastes or, more simply, from the Kubelka-Munk functions (4.82) and (4.84) of the test and reference pigments. In testing practice, they are always determined empirically rather than by the laborious calculation from the zi (l). Nonetheless, for the sake of completeness and to identify their source, they must be written out exactly. By equations (4.68) in Section 4.5.4 and (4.86), zY1 z e po 1 zRY1 zR1

R

y N lln zz1 l dl l R1

Z

2 3

p2 z5

p0 zR 5 FWP

p1 z2

p0 zR2

3

3

3

1 SW

Z

y N l

g l y N l FPU l

k l dl kR l

gR l p0 dl FPU;R l 2 3

Z y N l s l

p0 sR l dl

(4.89)

Here k (l), kR (l), and s (l), sR (l) are the absorption and scattering coefficients per unit PVC; g (l) and gR (l) are the attenuation coefficients of the scattering interaction. The first of each pair is for the test pigment, the second for the reference. The formulas for black pigments simplify because the l dependences and thus the integral vanish; p0 & k/kR and so forth. Equation (4.87), however, is not yet well-suited to the rational determination of tinting strength, for it requires a new determination of the pi for every new test pigment, or at least of p0 if one is working with the zero-th approximation. An approach to further rationalization is offered by the use and direct analysis of the Kubelka-Munk functions, which are quickly derived from Y measurements. For this purpose, the functions F^ (test pigment) and F^ R (reference) for equal masses m = mR = m^ are found from equations (4.82) and (4.84), and the quotient of the functions is taken. With the approximations for small quantities, neglecting higherorder terms, one then obtains 2 3 0 1 z z 5 5 ^ 2 R z z R z2 F FWP R2 3A 3 m^ 5 (4.90) 1 R 41 @ 32 f^ m^ 2 ^ z R m m FR FWP R1 R 3 m3 mR Now one forms the ratio to the tinting strength in equation (4.87) for the same ^ so that quantity m, P 1 1 f^

"

R RR

2 3

2 3

#

2 m^ 3 R m 3 RR

p0 zR 5

m^ p0 zR2 m

(4.91)

182

4 How Light Scattering and Absorption Depend on the Content ¼

It is useful to consider the effects of the two perturbation terms on the righthand side. Equation (4.65) shows that the second perturbation term (containing zR2 ) is influenced by the scattering power of the colored pigment while the first (containing zR5/3 ) is influenced only by its much slighter scattering interaction. Accordingly, the first perturbation term can be neglected; the second, on the other hand, may be appreciable in the case of strongly scattering colored pigments. What is more, it must be taken into account that the reference pigment (thus zR2 ) and the mass of pigment m^ are fixed in the practical determination of relative tinting strength, and further that p0 can be replaced by f^7R / RR when higher-order terms are neglected. Finally, then P 1 f^ 1 a f^ Here

F^ f^ F^R

1

(first approximation)

(4.92)

m^ RWP mWP RR

(4.93)

(zero-th approximation)

(4.94)

FWP FWP

;

a zR2

and P 0

F^ F^R

The coefficient a is a constant and need to be determined just once as long as the masses and the reference pigment are not changed. In addition, F^R does not have to be determined anew for every tinting strength test. The effect of the bracketed expression in equation (4.92) is that high tinting strength values are further increased while low ones are reduced. Another important point should be added. When the Kubelka-Munk functions are calculated in order to determine the relative tinting strength with equations (4.92) to (4.94), the surface-corrected CIE tristimulus values Y and Y R are to be obtained from equation (4.62). In tristimulus measurements, however, the spectral reflectances needed are not available. The Y values with the Saunderson corrections applied directly must therefore be used:

Y 100

Y 100

0:04

Y 0:36 0:6 100

(4.95)

(To distinguish these from the exact values, we use the notation Y ++.) But this direct correction has no further consequences, for in this case the chain of equalities DY = DY ++ = DF = 0 always holds rigorously.

4.6 Tinting Strength

183

The zero-th approximation in equation (4.94) is often sufficient for determining the relative tinting strength. Even for pigments with strong intrinsic scattering, it can always be employed for relative tinting strengths in the range of 80 % ^ P ^ 120 %; the difference between P(0) and fÃ due to dropping FWP is less than 0.2 %. For this reason, the zero-th approximation is suitable especially for production control, where only small departures from 100 % relative tinting strength are seen. Because of its continual use all over the world, this is the most commonly employed equation in colorimetric pigment testing. Finally, the use of lightness matching DY = DL = 0 as the tinting strength criterion makes it possible to answer the question of Section 4.6 as to the absolute tinting strength: The coloring power F introduced in Section 3.5.2 can serve this function. The coloring power was defined for the white substrate as the rate of increase in DE ab with film thickness h, beginning at h = 0, that is, at the intrinsic lightness L0w of the substrate. Because of the lightness criterion for the tinting strength, only DL matters, and so DE ab can be replaced by DL ; now, with equations (3.140), (3.155), and (3.157), the Y analog of equation (3.159), and the PVCdependent absorption coefficient K (l = s k (l) of the pigment, one gets F

uDL uh

h?0

116 116Y k Yk 3 100

R 116 4:8 R y N l K l dl 1:856 s y N l k l dl 3 100

A pigmented medium is used for the determination of coloring power, a pigment mixture with white for the determination of relative tinting strength. For the two results to be comparable, the pigment concentration must be the same in both cases. If one takes the same quantity mÃ of test pigment as in the tinting strength test, then since V 5 VM s

V V m^ VM V VM RVM

VM=VWP

In other words, the volume VM if the medium used in determining F should be equal to the volume of white paste in the tinting strength test. Then Z m^ y N l k l dl F 1:856 RVM VM=VWP (4.96) For F to be accepted as the absolute tinting strength, it must be shown that the ratio of two absolute tinting strengths (F relative to FR) gives the same relative tinting strength P obtained from equation (4.88). Since m^ and VM are fixed, R y l k l dl F RR R N (4.97) R FR y N l kR l dl

184

4 How Light Scattering and Absorption Depend on the Content ¼

On the other hand, the relative tinting strength is given to a good approximation by equations (4.88) and (4.89): Z RR RR k l 0 P p0 yN l dl (4.98) R R kR l In general, the quotient of integrals in equation (4.97) is not exactly equal to the integral of the quotient in equation (4.98). But under the assumptions taken in tinting strength determination (only small hue differences allowed, hence similar reference and sample spectra), the two expressions are always so similar that they are nearly equal up to a numerical factor close to 1. Thus if k (l) = const 7 kR (l), F / FR and P (0) come out to the same value; the same is true if k (l) and kR (l) are independent of l (black pigments). Now the coloring power defined by equation (4.96) can indeed be regarded as the absolute tinting strength, provided the quantity mM is such that VM = mM/RM = mWP /RWP = VWP . It should be noted that the absolute tinting strength has as its units not 1 but mm±1 = m2/L (see Section 3.5.2) and, as a consequence, presents itself as yet another effectiveness measure.

4.6.5 Color Depth Matching On the basis of results obtained in the color depth study that was described in Section 4.6.3, Gall was able to work out new formulas for the color depth. The T formula (eq. 4.76) had proved quite inadequate for practical use, but the color depth formulas initially taken over from the textile field also failed to reproduce the results of color matching tests. Typically, the formulas used today* span three discrete surfaces of constant color depth; if a color locus x, y, Y is specified, they give the deviation DTs from these color depth level surfaces. Once again, the surfaces are labeled with fractions, this time of the standard color depth SDS (= standard depth of shade) instead of the older standard depth R. T. Thus the standard gives formulas for DTS,1/3 , DTS,1/9 , and DTS,1/25 (using the notation B1/3 , B1/9 , and B1/25). The reference is always adjusted to the selected SDS, and the quantity mR of the reference is recorded. The test pigment mass m is varied in order to achieve a match (i. e., to make DTS = 0). The formula p (4.99) DTS;i Bi Y s ai j 10 bi gives DTS values for the several color depth levels. Here i Y

denotes the color depth level (1/3, 1/9, or 1/25 times SDS) is the CIE tristimulus value Y

* For standards see ªColor Depthº in Appendix 1.

4.6 Tinting Strength

S

185

is a measure of the saturation, equal to ten times the linear distance between the CIE color locus x, y of the test pigment and the equi-energy stimulus q (4.100) s 10 x xn 2 y yn 2

ai (j) is a factor used in evaluating the saturation measure; it depend on the hue angle j = Arctan [( y ± y0)/(x ± xo)] and, to a slight degree, on the SDS are constants: b1/3 = 29, b1/9 = 41, b1/25 = 56 bi The ai (j) are tabulated in DIN 53235 part 1 (enter the tables with i and j). The convenient formulas (third-degree polynomials) presented in Chapter 8 are preferred for computer calculation. The levels defined by these formulas are again surfaces in color space resembling spherical shells or goblets (Fig. 4-19). To gain some idea of the situation, one can calculate from the bi where these surfaces intersect the lightness axis in CIELAB color space. For DTS = s = 0, equation (4.99), gives ! b1 2 3 Y0; 1 2:92 8:41 10 3 Y0; 1 16:81 9

Y0; 1 31:36 25

Fig. 4-19. Surface of constant color depth Ts (Ts = (1/3) SDS) in the CIE system, after Gall.

The respective lightness value are L0;1=3 = 34.8, L0;1=9 = 48.0, and L0;1=25 = 62.8; thus the lightness range of interest is well spanned. For the sake of rationalization, it is desirable if the test can be performed with a single weighed quantity of pigment. Bringing DTS to zero requires an iteration. The new quantity of pigment mass to add is mi1 mi 0:9DTS

(4.101)

186

4 How Light Scattering and Absorption Depend on the Content ¼

while the m dependence of the CIE tristimulus values Y used in equation (4.99) can be obtained from equation (4.66) or (4.67); the coefficients are determined by appropriate pigment mass additions. It is still better to apply the principle of spectral evaluation immediately. The function F (l) can be obtained from equation (4.63) for individual l values; the needed coefficients zRi for the reference can then be found with one to two pigment quantities. On the other hand, the tristimulus method can also be employed. The basis for this approach comprises equations (4.66) and (4.67) for the Kubelka-Munk functions of the CIE tristimulus values X, Y, Z, or the corresponding equations for the reflectometer values R'x , R'y, R'z. The coefficients here are easily determined with two pigment quantities.

4.7

Special Problems

4.7.1 Lightening Power As defined by standards, lightening power is ªthe ability of a pigment to increase the lightness of a colored, gray, or black mediumº. The lightening power is the relative tinting strength of white pigments, and the definition accords with that of the general relative tinting strength of pigments, equation (4.75). The problem, once again, is to derive a simple relation suitable for rationalizing the procedure; the tool used, once more, is the Kubelka-Munk function. Dispersions of white pigments in black pastes yield reflection spectra virtually independent of l, so that R (l) can be treated as equal to Y/100. Thus DY = DY++ = DF = 0 rigorously. Similarly to the development in Section 4.6.4, the Kubelka-Munk functions of the test and reference pigments are written out in accordance with equation (4.48). Next, an expression is sought for the function cR (c) at matching, which leads in the end to the lightening power equation: P 1 w

" RR 1 p R w0 RR 1 p R w0

2 m 3 pw 2 m 3

pw1

s 2 3 pw 2 s 3 1

m m

pw1

#

s 1

s

(4.102)

(first approximation)

P 0 w

RR R s pw0 R R R sR

(zero-th approximation)

(4.103)

4.7 Special Problems

187

Here, similarly to equation (4.50), pwo

zw1 s zwR1 sR 2

pw 2 zw 5

3 pw0 zwR 5 g

pw1 zw2

pw0 zwR2

3

3

2

3 pw0 gR

3

1 k Kb

pw0 kR

(4.104)

Equation (4.102) has the new feature that both the second and the third terms in brackets are negative (not just the third as in eq. 4.87). Next, the Kubelka-Munk functions for the test and reference pigments are writ^ and the ratio f^w of the two is formed. In contrast ten for equal pigment quantities m, to the previous derivation, an examination of the two perturbation terms shows that the pw2/3 term must be kept because it relates to the attenuation coefficient for the scattering interaction of the white pigment. On the other hand, the intrinsic absorp^ tion of the white pigment (pw1) can be neglected. Division of P(1) w by f w leads, finally, to the equations 1 Pw

h 2 ^ fw 1 aw f^w3

where

aw zwR 5 3

i 1

R m^ BP mBP RR

(first approximation)

2 3

gR

F^wR FBP f^w F^w FBP P 0 w

F^wR F^w

R m^ BP mBP RR

(4.105)

2 3

F^w F^wR

(zero-th approximation)

(4.106)

Equation (4.106) is another formula employed very frequently in pigment testing. It should be noted that the equation for the lightening power has the reference Kubelka-Munk function in the numerator and the test function in the denominator, in other words inverted to the relative tinting strength. The zero-th approximation gives the lightening power in the Beer's law region; outside this region, the first approximation has to be used. The reason has to do with the relatively strong effect on the lightening power due to the scattering interaction. An example is shown in Figure 4-20. Equation (4.106) implies that the

188

4 How Light Scattering and Absorption Depend on the Content ¼

Fig. 4-20. Significance of lightening power.

zero-th approximation is the ratio of the scattering coefficients per unit PMV for the test pigment and reference: P 0 w

mR m

DY=0

sR s

DY=0

s sR

s=sR

s sR

m=mR

(4.107)

No account is taken of the scattering interaction. The lightening power is thus correctly represented by the ratio of scattering coefficients only in the Beer's law range, not at higher PVC. For this reason, the lightening power and the relative scattering power are identical only in the lower range; the difference between them grows larger and larger outside this range. The first approximation requires a determination of gR. An appropriate technique is the dilution method, since g can be obtained directly with equation (4.52). Chapter 8 will describe a method by which the lightening power of white pigments can be determined in a rational manner combining the adding pigment and dilution methods.

4.7.2 Color Differences after Matching The ªcolor difference after color reductionº is the color difference still present after tinting strength matching; its analog after lightening power matching is called the ªshade difference after lightening power matchingº. These are obtained by colorimetry using the CIELAB system; they can be broken down into lightness difference, chroma difference, and hue difference components in the first case, into shade strength and nature of shade in the second (see Section 2.3.3). The color difference between the reduced test and reference pigment are calculated from the CIE tristimulus values of both. The X, Y, Z of the reduced test pigment are measured directly when the tinting strength and lightening power are de-

4.7 Special Problems

189

termined (or the reflectometer values R'x , R'y, R'z , when the tristimulus method is employed); XR, YR, ZR for the reference pigment at matching, on the other hand, have to be calculated. The PMV-dependent Kubelka-Munk functions of the CIE tristimulus values, equations (4.82) and (4.48), are available for this purpose; all that is necessary is to substitute the PMV of the reference at matching, cR = mR/mR, ^ because the mass mR of reference pigment at matchin the formulas, and mR = mP ing is very easily found with fundamental equation (4.75). In the equations that follow, the needed relations will be listed for direct use in tinting strength/lightening power programs. The term with subscript 5/3 is dropped in the case of tinting strength, the term with subscript 2 in that of lightening power, because they are negligible. Thus the color difference after color reduction (tinting strength) is given by FXa;R

2

FWP zXR1 cR 1

zXR2 cR

FYa;R

2

FWP zYR1 cR 1

zYR2 cR

2

FWP zZR1 cR 1

zZR2 cR

FZa;R

(4.108)

while the shade difference after color reduction (lightening power) is 1 2

Fw;Xa;R 1 2

Fw;Ya;R 1 2

Fw;Za;R

1 zw;XR1 cR 1 FBP 1 zw;YR1 cR 1 FBP 1 zw;ZR1 cR 1 FBP

Here cR with

m^ mR P mR mR

mR mWP

2 3

zw;XR 5 cR 3

2 3

zw;YR 5 cR 3

2 3

zw;ZR 5 cR 3

(4.109)

(4.110)

RWP RR

(and also Pw in place of P). When the determination is done by the tristimulus method, the needed coefficients zRi for the reduced reference pigment are deter-

190

4 How Light Scattering and Absorption Depend on the Content ¼

mined once for all with the help of two mixtures containing different quantities of pigment. If the first approximation for the Kubelka-Munk functions is sufficient, one can set FWP = 1/FBP = 0 in the above equation and set the brackets on the right equal to 1. The Kubelka-Munk functions of the CIE tristimulus values immediately imply the (simply) corrected CIE tristimulus values of the reduced reference, in accordance with equation (3.116) or (4.61) (the subscript R is dropped in the equations that follow): X 1 FX Xn

p FX FX 2

Y 1 FY 100

p FY FY 2

Z 1 FZ Zn

p FZ FZ 2

(4.111)

and hence the uncorrected CIE tristimulus values of the reduced reference pigment, in accordance with equation (3.10):

X 0:04 Xn

Y 0:04 100

Z 0:04 Zn

X Xn X 0:6 Xn

0:384 1

Y 100 Y 0:6 100

0:384 1

Z Zn Z 0:6 Zn

0:384 1

(4.112)

Now the CIE tristimulus values X, Y, Z of the reduced test and reference pigment are known, and with the scheme of Section 2.3.3 one can calculate DE ab along with the breakdowns of color or shade difference after matching. Both quantities are strongly affected by particle size, especially in pigments with high light-scattering power. The reason for this behavior will be explained in

4.7 Special Problems

191

Chapter 5. By virtue of this relationship, the color and shade differences after matching can well be used in production control, where they serve as sensitive indicators of any departure from constancy of particle size. Because the only concern is with deviations, simplified results are also adequate here; for example, the difference between the CIE tristimulus values X and Z can be cited, or this difference related to the CIE tristimulus value Y, (Z ± X)/Y.

4.7.3 Change in Tinting Strength Section 4.1.3 treated the steps in the dispersing of pigments: wetting, disintegration, and stabilization. Now the disintegration process need to be examined more closely, since it is directly related to the final tinting strength of the pigment. When pigments are dispersed in binders, it can be observed as a general rule that the relative tinting strength increases as the dispersing effort continues. Therefore the relative tinting strength is an excellent test instrument for describing the dispersing process (ªtinting strength developmentº) and the final dispersed condition. The mathematical instrumentarium of reaction kinetics, well-known from physical chemistry, can be employed for the quantitative description of dispersing over time, since dispersing is a transformation of substances ± of larger particles to smaller ones. For the sake of simplicity, just two classes of particles are considered, the particles to be dispersed (larger) and the particles already dispersed (smaller). It is still amazing that the process of dispersing can be handled by such a simple model and that the results are in such good agreement with observation. First, some conventions: s ? is the total PVC of particles in the mill base; this does not vary during the dispersing process, s is the PVC of fine particles at time t, so that s ? ± s is the PVC of coarse particles. If the PVC is referred to the total PVC, the relative fraction of fine particles is given by n = s/s ? and that of coarse particles by 1 ± n. We now investigate the following cases: ± Size reduction of the coarse particles is due to the grinding action of the large particles themselves ± It results from grinding on the grinding medium and the walls of the grinding vessel ± It is the consequence of grinding by already dispersed (small) particles Case 1: Size reduction by large particles themselves The increase in the fraction of small particles dn over time must be proportional to the squared fraction of coarse particles (1 ± n)2. For a selected coarse particle is reduced in size faster the more coarse particles it encounters (simple proportionality); because the same thing happens with all the coarse particles, however, there must be another proportionality to the fraction of coarse particles (double proportionality): dn kg (1 ± n)2 d t

(4.113)

192

4 How Light Scattering and Absorption Depend on the Content ¼

where kg is the rate of size reduction of coarse particles by coarse particles (units min±1 or h±1). With the initial condition that the initial concentration (at t = 0) of small particles is zero (n (0) = 0), the integral of the differential equations yields 1 1 1 n kg t

(4.114)

as in the case of a second-order reaction. The rate of dispersion kg can also be expressed in terms of the half-time t 0.5 : t0:5

1 kg

(units: min or h)

(4.115)

Now the relative tinting strength can be written in accordance with equations (4.97) and (4.98), with k for the colorimetric y (l) integrals of the absorption coefficients per unit PVC. The absorption coefficient k? (corresponding to the ªfinal tinting strengthº) is taken for the reduced reference pigment. In this way, the pigment is compared with its own final dispersion; as a consequence, there is a single pigment density R = RR. If P0 = k0 / k? is the initial tinting strength, then P

s1 k k1

s k0 s k1 P0 n 1 s1 k1

P0

(4.116)

Rewriting and substitution of equation (4.114) leads to 1 P

P0

1 1

P0

1

1 1 P0 kg t

(4.117)

^ F^ ? in accordance with equation (4.94), in other words makIf now one sets P = F/ ing the relative tinting strength equal to the ratio of the Kubelka-Munk functions for equal pigments masses mÃ, and if one further neglects the (usually very small) initial tinting strength P0, one gets 1 1 1 1 ^ ^ ^ F F1 F1 kg t

(4.118)

This is the well-known Pigenot equation, which states that a straight line results if the reciprocals of the Kubelka-Munk functions for the reduced pigments are plotted versus reciprocal time over the dispersion process. As equation (4.117) shows, the linearity can be improved if the initial function F^ 0 is subtracted from F^ and F^? at the outset. The Pigenot equation holds more-or-less well for many dispersing operations, indicating that the disintegration of coarse particles on themselves is the dominant

4.7 Special Problems

193

Fig. 4-21. Dispersing curves for the size reduction of coarse particles on themselves (1) and on the grinding medium and grinding vessel walls (2). The half-time is the same for both curves, t 0.5 = 1 h.

process in dispersion. The prerequisites for this are satisfied especially in mixtures for dispersion where the pigment concentration is high or the degree of filling of the grinding vessel is high. Curve 1 in Figure 4-21 presents one dispersing curve for this form of size reduction. In the final phase, the last little bit of reduction comes about very slowly because of the declining quantity of coarse particles. Case 2: Size reduction by grinding medium and vessel walls This process corresponds to a first-order reaction, so that the increment of fine particles is simply proportional to the fractional concentration of coarse particles: dn kw (1 ± n) dt

(4.119)

where kw is the rate of size reduction of coarse particles by grinding medium and wall, with units of min±1 or h±1. With the same initial condition as above, the integral comes out to n 1 ± e±kw t The half-time is t0:5

ln 2 0:693 kw kw

(4.120)

(4.121)

with units min or h. If n (t ) is substituted in tinting strength equation (4.116), the result after simplifying and taking logarithms is ln (1 ± P) ln (1 ± P0) ± kw t

(4.122)

Thus a plot on semilog paper, with 1 ± P on the logarithmic scale versus t on the linear scale, will give a straight line.

194

4 How Light Scattering and Absorption Depend on the Content ¼

This disintegration mode dominates when the mill base has a low pigment concentration (and thus also in the final phase) or the filling of grinding medium is high. Figure 4-21 also shows a dispersion curve for this type of disintegration (curve 2). The rate constant was selected so that the same half-time t 0.5 applies to curves 1 and 2. Obviously, this disintegration process is markedly more efficient than size reduction on the particles themselves, at least in the final phase. Case 3: All forms of disintegration In addition to the two modes with which we have already become acquainted, another disintegration process is possible: size reduction of coarse particles on fine ones. While this form will play a rather minor role, it must be allowed for in the global formula. It is not worthwhile, however, to examine it in isolation as we did the other two modes, for it contributes slightly to only the middle portion of the dispersion process. The reason is that there are no small particles at the beginning of the process, while there are no large ones at the end, so that conditions for t = 0 and t = ? cannot be introduced. The increase in the content of small particles for this type of disintegration must be expressed as an interaction term between small and large particles, which is thus proportional to n (1 ± n). The differential equation for all disintegration processes is now dn [kg (1 ± n)2 + kw (1 ± n) + kk n (1 ± n)] dt

(4.123)

where kk is the rate of size reduction of coarse particles by small particles (units min±1 or h±1). With the usual initial condition, the integral is 1 A 1 Bt 1 n e

(4.124)

where A = (kw + kk)/(kg + kw), B = kw + kk, and the half-time is t0:5

1 A ln 1 A 1 B B

A 2

1 3 1 kg kw kk 2 2

(4.125)

The approximation being obtained with A 5 1. the constants A and B can be determined by iteration based on two measurements. A plot versus time does not directly give a straight line as in the previous cases, but for the initial values of n or F^ (i. e., t 5 t 0.5) the smallness of the exponent in equation (4.124) means that the Pigenot equation (4.118) holds to a good approximation. Figure 4-22 shows how n varies with t for rate constants kg = 1, kw = 0.1, and kk = 0.01 h±1.

4.7 Special Problems

195

Fig. 4-22. A dispersing curve for all types of disintegration.

In order to evaluate eq. (4.124), first the quantity n from the Kubelka-Munk functions F of the colored pigment/white paste mixtures is calculated (from eq. 4.116):

n

F F0 F1 F0

(4.126)

where F0 is the initial value and F ? is the final value. When more than two pairs of measurements are being analyzed, the problem is overdetermined, since just two parameters A and B are to be calculated. Curve fitting is done by linearizing eq. (4.124). Writing y = n/(1 ± n) and a = 1/A yields y a (eBt ± 1) The sum of squared errors to be minimized is then P

f2

P

a eBt

1

y2 ! min

Accordingly, the partial derivatives with respect to a and B must vanish. Elimination of a leads to an equation for B: Z

EE 2 E n EY Y

EET ET !0 ETY

(4.127)

where E = exp (Bti), T = ti , Y = yi , n is the number of pairs of measurements, and [ ] is the Gaussian summation symbol. The first derivative

196

4 How Light Scattering and Absorption Depend on the Content ¼

EET EY

Z0 2

ET Y

EE

2 E n ETY EY Y2

2 EETT ETT EET ET ETTY ETY ETY2

(4.128)

is also used for the iterative solution by Newton's method. Because of the danger of an overrun in the numerical memory, a starting value of about B0 = (80 ± 3 ln tn)/3tn is recommended, where tn is the largest t value occurring. The value of A is then A

EET ET ETY

(4.129)

If B becomes very small, the iteration does not converge; if the values oscillate in a very narrow range about zero, we then set B = 0. In this case, A likewise becomes very small, so that B/A = [TY]/[TT ]. For the determination of the three rate constants kg , kk , kw, eq. (4.124) offers only two quantities A, B. A third equation is found by writing eq. (4.123) with the real PVC values instead of the relative values and comparing coefficients with the original equation. The result is kg k0g s1 ;

kw k0w ;

kk k0k s1

(4.130)

that is, kg and kk are proportional to the total concentration s ? , while kw is constant. A second mill base must therefore be made with a different concentration but other conditions the same. The parameters B = kk + kw and B/A = kg + kw are determined from each of the mill bases; we then have four parameters containing the three desired quantities kg , kk , kw . Linear regressions are used (naturally, these are also recommended when there are more than two mill bases). Now (with x = s?) the following equations are formed: y1 B=A B kg kk 2 kw k0g k0k s1 2 kw ax b y2 B=A

B kg

kk k0g

k0k s1 cx

(4.131)

From each pair (or more) of equations of the y1 and y2 types, a, b, and c are obtained directly (or through linear regression), and hence k0g a c=2 ;

k0k a

c=2 ;

kw b=2

Thus the three rate constants are known for any arbitrary PVC.

(4.132)

4.8 List of Symbols Used in Formulas

4.8

List of Symbols Used in Formulas

A, B A, B, a, b, c, a a , b , L Bi = DTSi b c

c D DC ab DE ab DH ab DL DTSi E e Z Z f^ F = K/S

197

constants Variables in the change of strength CIELAB coordinates deviations from surfaces of constant standard color depth with i = 1/3, 1/9, 1/25 pigment mass concentration, PMC (g cm±3) coefficients of the PVC-dependent Kubelka-Munk function for constant volume method with subscripts: b black pigment w white pigment 1 linear term 5/3 term in 5/3 power 2 quadratic term c for colored pigments with same subscripts as c, F particle diameter, mm chroma difference (CIELAB) color difference CIELAB) hue difference CIELAB) lightness difference (CIELAB) see Bi Variable in the change of strength small quantity (e 5 1) attenuation factor of scattering interaction Function in the NEWTON iteration quantity formed from Kubelka-Munk functions with subscript: w white pigment Kubelka-Munk function without subscript: test (sample) with subscripts: a adding pigment method A initial value b black pigment in white paste B black system (constant volume method) BP black paste (adding pigment method) c constant volume method d dilution method PU full shade R reference

198

4 How Light Scattering and Absorption Depend on the Content ¼

F

F^

F (1), F (2) g = gs g h K

k kb k' k b@ k

m

m m n n = s/s ?

W white system (constant volume method) w white pigment in mixture with black paste WP white paste (adding pigment method) Kubelka-Munk function of CIE tristimulus values of colored pigments with subscripts: X,Y, Z CIE tristimulus values see also F Kubelka-Munk function for constant pigment mass m^ with subscripts: 0 initial ? final see also F first and second approximations to Kubelka-Munk function with same subscripts as F attenuation term of scattering interaction coefficient in attenuation term, mm film thickness, mm absorption coefficient for diffuse irradiation, mm±1 with subscripts: F colored or black pigment see also c absorption coefficient referred to PVC, mm±1 absorption coefficient of dye for diffuse irradiation, referred to mass concentration, m2 g±1 absorption coefficient for directional irradiation, mm±1 absorption coefficient of dye for directional irradiation, referred to mass concentration, m2 g±1 reaction rate constant, min±1 or h±1 with subscripts: g size reduction on coarse particles k size reduction on fine particles w size reduction on wall and grinding body mass, g with subscripts: M medium see also F pigment mass equivalent to the medium volume (PVM), g with same subscripts as F pigment mass equivalent to the medium volume of the mass portion (PMM) Number of measurements relative volume fraction of fine particles during dispersing process

4.8 List of Symbols Used in Formulas

P

P (0), P (1) p pi

F j j c Q qD = s/sA R R' R

R (l) R (l) S s s s

relative tinting strength with subscripts: d dye w lightening power 0 initial zero-th and first approximations to relative tinting strength with same subscripts as P are fraction of individual particle (for scattering interaction) coefficients of relative tinting strength (i = 0, 2/3, 1) with subscripts: 0 absolute term 2/3 term in 2/3 power 1 linear term ^ c see also F, F, coloring power, mm±1 = m2 L±1 with same subscripts as F pigment volume portion hue angle in CIE chromaticity diagram pigment/medium volume ratio (PMV) with same subscripts as F any color quality dilution ratio by volume diameter of closest-packed spheres, mm reflectometer value with subscripts x, y, z for the tristimulus method density, g cm±3 with subscripts: D dispersion see also F, m spectral reflectance with same subscripts as F spectral reflectance after Saunderson correction with same subscripts as F scattering coefficient, mm±1 with same subscripts as K scattering coefficient referred to PVC, mm±1 with same subscripts as c measure of saturation in the CIE system pigment volume concentration (PVC) with subscripts: 0b black pigment in black paste 0w white pigment in white paste U achromatic pigment in mixture UA achromatic pigment in mixture, initial value

199

200

4 How Light Scattering and Absorption Depend on the Content ¼

UP achromatic paste in mixture U0 achromatic pigment in achromatic paste T Variable in the change of strength transmission factor T color depth T t time, min or h with subscript: 0.5 half-time V volume, cm3 or L with same subscripts, as F, m V CIELAB color locus u coefficient of PVC-dependent Kubelka-Munk function for dilution method with same subscripts as c u u for colored pigments F with same subscripts as c, w pigment mass portion (PMP) X,Y, Z CIE tristimulus values with subscripts: n for CIE standard illuminant n see also F X ,Y , Z CIE tristimulus value of Saunderson corrected reflection spectrum with same subscripts as F X ++,Y ++, Z ++ CIE tristimulus values after Saunderson correction with same subscripts as F x, y CIE chromaticity coordinates with subscript: n CIE standard illuminant n x (l), y (l), z (l) CIE color matching functions with subscript: N normalized to CIE standard illuminant N Variables in the change of strength Y, y, y1, y2 coefficients of PMV-dependent Kubelka-Munk function for adding zi pigment method with the same subscripts as c z z for colored pigments F with same subscripts as c,

4.9 Summary

4.9

201

Summary

Particle size is one of the most important parameters of a pigment; there is no application-related property that is not affected by it. This chapter reports on the needed definitions (primary particle, agglomerate, aggregate) and the particle-size parameters. The colorimetric properties of pigments are, in practice, always tested after incorporation into a vehicle system. The preparation of the dispersion (the dispersing process) must be done with particular care. Quantitative description of concentration-related phenomena demands clear definitions of measures for the dye and pigment concentrations. The following quantities are derived from the relationships in mixed-phase systems: pigment mass portion (PMP), pigment mass concentration (PMC), pigment volume concentration (PVC), pigment mass equivalent to the medium volume (PVM), pigment mass equivalent to the medium volume of the mass portion (PMM), and pigment/medium volume ratio (PMV). The absorption and scattering coefficients of Chapter 3 are not true constants of a material, since they also depend on the concentration of coloring material. The absorption of dyes and pigments is a linear function of concentration (Beer's law). There remains a real material constant, the ªabsorption coefficient referred to concentrationº (or per unit concentration). If several coloring materials are present, the individual coefficients can generally be summed. In the case of scattering, the relationship is linear only in the initial region (up to a PVC of ca. 10 %). At higher concentrations, the scattering falls increasingly behind the linear function because of the scattering interaction between particles as they come closer and closer together. This effect is included in an earlier published equation having a term in the 2/3 power of the concentration. Experimental tests of this formula have shown good agreement with the actual behavior of the scattering curves for white pigments. The laws for mixtures of pigments with achromatic pastes are systematized by the method used to prepare the mixture. The three most important methods in practice are ± Constant volume method. The PVC of the achromatic pigment in the paste is held constant. It is used chiefly in determining scattering and absorption coefficients ± Adding pigment method. The pigment is added, in measured quantities by weight, to a constant weight of paste. This is the most important of the three methods because it forms the basis for determining the tinting strength of pigments ± Dilution method. After a mixture is prepared, it is diluted by adding more vehicle. This method plays some role in the rationalization of test procedures Each of the preparation methods is characterized by its own conservation law. The concentration-dependent Kubelka-Munk functions for pigment/achromatic paste mixtures are obtained in the following way: the equations for the three stan-

202

4 How Light Scattering and Absorption Depend on the Content ¼

dard mixing methods are derived from a generally valid formula. Application of the proper conservation law in each case yields the equations for black pigments in white paste and white pigments in black paste; separate equations are obtained for the constant volume, adding pigment, and dilution methods. The pigment/medium volume ratio is the appropriate concentration measure for the adding pigment method. The procedure is also used for colored pigment whose spectral KubelkaMunk functions are to be derived. Then it is shown that similar approximate formulas can also be obtained for broad-band spectral distributions, and thus for the CIE tristimulus values. These are of great practical importance when tristimulus instruments are employed. In summary, the equations are all similar except for having different coefficients. Typical for these relations is that the Kubelka-Munk functions are linear in the concentration to a first approximation, while in the second approximation there are perturbation terms in the 5/3 and 2 powers respectively. The tinting strength describes one of the most important optical qualities of coloring materials. It is a measure of the ability to impart color to other substances through absorption. All testing methods give the relative tinting strength, that is, the absorbing power relative to another pigment or dye. In the case of dyes, the relative tinting strength is also logically defined as a relative absorption; for pigments, on the other hand, the definition is plainly a measure of effectiveness, stating the mass ratio of test and reference pigments such that mixtures of the pigments with white paste appear alike. The lightening power (the tinting strength of white pigments) is based on scattering and is determined in black pastes. ± The ªstandard experimentº of tinting strength determination thus consists in matching one pigment to the other in reduction by varying the mass of one pigment added. In matching, which means causing the mixtures to look alike or have the same color, the matching criterion plays a key role. An indispensable step in rationalizing computer-aided methods is to establish the tinting strength criterion. Any such criterion can be thought of as a set of equipotential surfaces in color space, which are intersected by the ªtinting characteristicº (a curve connecting the color loci of mixtures obtained by adding larger and larger amounts of colored pigment to a white paste). Among the tinting strength criteria in use, two are of special significance: the lightness L (or CIE tristimulus value Y) and the color depth. Two color matching studies reported in the literature are consulted in order to establish what tinting strength criteria are preferred by colorists. In one of the studies (on inorganic pigments only), the question to be answered was this: which of the added pigment quantities produces the best match? A comparison with colorimetric data gave the unambiguous answer that the CIELAB lightness L (or CIE tristimulus value Y) is the crucial tinting strength criterion. In the second study (primarily on organic pigments), the one sample was to be chosen that best agreed in color depth with the reference pigment and, simultaneously, with the other samples already selected, right around the color circle. This study resulted in improved formulas for calculating color depth values. Because the inorganic pigments in the first case were nearly all of a dark and not highly saturated full shade, while in the second case the pigments used were more highly saturated,

4.9 Summary

203

current practice is as follows: the lightness criterion is used for inorganic pigments, the color depth criterion for organic ones. There follows a complete derivation of the tinting strength equation expressed as a dependence on pigment concentration for the lightness matching case. As a result of the development, it is found that Y matching is virtually identical with matching based on the Saunderson-corrected Y values, and that this correction can be applied directly to the CIE tristimulus values. Finally, it is shown that the coloring power defined in Chapter 3 can be regarded as an absolute tinting strength. Because the color depth formulas taken over from the textile field were not accurate enough, the studies were utilized in improving these formulas as applied to pigments. To rationalize the determination of tinting strength based on color depth matching, the required mass of the test pigment must be determined by an iterative method; the principle of spectral evaluation is well-suited to this purpose. In the case of lightening power, the white-pigment analog of the relative tinting strength, the Kubelka-Munk function again serves as a tool for rationalization. the needed equations for the lightening power as a function of PVC are derived in a similar way to the tinting strength equations. The zero-th approximation of this equation provides a good description of the behavior in the Beer's law region; at higher pigment concentrations, the first approximation with the perturbation term must be employed. The color difference that remains after matching is called the ªcolor difference after color reductionº in the case of tinting strength and the ªshade difference after lightening power matchingº in the case of lightening power. The CIELAB coordinates are accessible from the CIE tristimulus values (calculated for the pigment mass at matching), and from these in turn the color differences between sample and reference can be obtained. For white pigments, the shade difference after lightening power matching is a particularly suitable tool for the quantitative characterization of the pigment particle size. In the dispersing process, the disintegration of pigment agglomerates is crucial to the quality of the resulting dispersion. It is shown how a quantitative description of the dispersing process can be arrived at with the equations of reaction kinetics. For example: ± The size reduction of large particles on large particles is a second-order reaction and can immediately be described by the well-known PIGENOT equation, which is suitable for linearizing the measured values. ± Size reduction on the vessel wall and grinding medium is described by a first-order reaction equation. ± Size reduction by all mechanisms includes disintegration on small particles already produced. In all three cases, the half-time can be used to characterize the rate of dispersion.

204

4 How Light Scattering and Absorption Depend on the Content ¼

4.10 Historical and Bibliographical Notes Even before Kåmpf's thorough work in 1965 [1], there was a large specialist literature dealing with the effect of particle size on pigment properties (see the bibliography in [1]). The particle-size concepts defined in Section 4.1.1 correspond to the classification of pigment proposed in 1963 by Honigmann and Stabenow [2], which has gained international adoption and has been set forth in standards. As the existence of several ªmean diametersº and other size measures shows, special care is needed when using the term ªparticle sizeº [1±4]. Keifer [5] and Kaluza [6] have worked on problems of flocculation. Next to the production of the individual components, the most important operation in the manufacture of lacquers and paints is the dispersing process, and numerous publications have dealt with this topic (see bibliography in Kaluza [7]). work by von Pigenot [8] on the tinting strength development as a second-order reaction dates from the early 1960s; This line has been followed up by many other authors [9±13], who also considered the first-order reaction. The linear dependence of absorption on dye concentration was discovered by Beer (1825±63) [14], whose work came long after Lambert's law was derived (see Section 3.7). The application of Beer's law to light scattering by pigments did not happen until our century; it was contained, for example, in the first edition of Judd's well-known book [15]. Perturbation terms for the intrinsic scattering of the white or colored pigment being tested, in the form of quadratic terms [16], were initially used for formulation and rematching problems [17]; the first publication of the s2/3 perturbation term was in 1967 [18]. The quasilinear concentration dependence of the Kubelka-Munk function (Chapter 4) is valid over a much broader concentration range than is a logarithmic dependence as suggested by von Pigenot [8]. It is no longer possible to tell when the consensus was reached that the relative tinting strength of pigments should be determined as the ratio of portions by weight added to a white substrate. An early indication is found in a 1932 paper [19]. For the Kubelka-Munk function of reduced black pigments, the famous work of the discoverers (see Section 3.9) already gives a linear dependence on the black pigment concentration (first approximation; see Section 4.5.2). The ratio of the test and reference Kubelka-Munk functions for equal pigment masses, which is easily derived from their remark, is identical to the zero-th approximation for the tinting strength of black pigments, derived in Chapter 4. For colored pigments, the tinting strength criterion is important. The color matching studies discussed in Chapter 4 were performed by Gall [20] and Keifer/Vælz [21]. Gall's publication derives the new color depth equations based on Raabe and Koch's earlier equations for dyed textiles [22]. A table of a (j) factors, needed for computer calculations of color depth shades, appeared later [23]. A rational determination of the tinting strength of colored pigments, based on the principle of spectral evaluation (Section 3.6) and thus suitable for any arbitrary tinting strength criterion, was also developed by Gall [24]. Schmelzer and co-workers have also proposed doing the matching for B = 0 [25].

4.10 Historical and Bibliographical Notes

205

The methods formerly used for lightening power have today been largely forgotten, for the most part with good reason (e. g., the Reynolds method [26]). This does not apply to the procedure of Grassmann and Clausen [27], which uses the fact that the functions log F (R) and F (1/m) have linear shapes over wide range (see Section 3.3.1 and 4.5.3 respectively), so that a straight calibration line is possible. This means that a graphical technique [28] can be used; despite being restricted to the Beer's law region, this technique produced good results in many laboratories before the introduction of computers. Another advance is Keifer's graphical method [29], in which the level of pigmentation is varied and the relative scattering power and shade can be determined simultaneously with the lightening power; this method has been incorporated into standards. A rationalized method for determining the lightening power, suitable for use in present-day laboratories, is described in Chapter 8 [30]. It is based on the equations of Section 4.7.1 for Pw as a function of m. A comprehensive summary of solved and unsolved problems from Chapter 1±4 should also be mentioned [31]. On the determination of dye concentrations, see [32]. For the change in strength, a method was proposed [33, 34] by which the three governing rate constants can be determined by a reaction-kinetic method; disintegration of large particles by grinding action on ± The large particles themselves ± Grinding bodies and the walls of the grinding vessel ± Already dispersed small particles An Example is described in Chapter 8.

References [1] G. Kåmpf, farbe + lack 7 (1965) 353. [2] B. Honigmann, J. Stabenow,VI. Fatipec-Congress Wiesbaden 1962, Congress-B., 89,Verlag Chemie Weinheim. [3] K. Leschonski, Particle Size Analysis and Characterization of a Classification Process, in Ullmann's Encyclopedia of Industrial Chemistry, Vol. B2, 5th edit. 1988, VCH Verlagsgesellschaft Weinheim. [4] T. Allen, Particle Size measurement, 3. Ed. 1981, Chapman & Hall, London/New York. [5] S. Keifer, farbe + lack 79 (1973) 1161. [6] U. Kaluza, farbe + lack 80 (1974) 404. [7] U. Kaluza, Physikalische Grundlagen der Pigmentverarbeitung fçr Lacke und Druckfarben, Edition Lack und Chemie E. Moeller, Filderstadt 1980. [8] D. v. Pigenot,VII. Fatipec-Congress Vichy 1964, Congress B. 249,Verlag Chemie Weinheim. [9] O. J. Schmitz, R. Kroker, P. Pluhar, farbe + lack 79 (1973) 733. [10] U. Zorll, farbe + lack 80 (1974) 17. [11] A. Klaeren, H. G. Vælz, farbe + lack 81 (1975) 709. [12] L. Gall, U. Kaluza, defazet 29 (1975) 102. [13] U. Kaluza, XII. Fatipec-Congress G.-Partenkirchen 1974, Congress B. 233, Verlag Chemie Weinheim.

206 [14] [15] [16] [19] [18] [19] [20] [21] [22] [23] [24] [25] [26] [27] [28] [29] [30] [31] [32] [33] [34]

4 How Light Scattering and Absorption Depend on the Content ¼ A. Beer, Grundriû des photometrischen Kalkçls, Braunschweig 1854. D. B. Judd, Color in business, science and industry, 1952, J. Wiley & Sons, New York. F. Vial, XII. Fatipec-Congr. G.-Partenkirchen 1974, Congr. B. 159. L. Gall, II. AIC-Congress York 1973, Congr. B. 153, A. Hilger, London. H. G. Vælz, Ber. Bunsen-Ges. phys. Chem. 71 (1967) 326. Anonym, Off. Digest Fed. Paint & Varnish Prod. Clubs (1932) 1029. L. Gall, I. AIC-Congress Stockholm 1969, Congr. B. Vol. I, F 6. S. Keifer, H. G. Vælz, farbe + lack 83 (1977) 180 und 278. P. Rabe, O. Koch, Melliand Textilber. 38 (1957) 173. L. Gall, K. Friedrichsen, Defazet 28 (1974) 158. L. Gall, IX. Fatipec-Congress Brçssel 1969, Congr. B. Sec. I, S. 34,Verlag Chim. d. peintures. G. Geiûler, H. Schmelzer, W. Mçller-Kaul, farbe + lack 84 (1978) 139. H. A. Gardner, G. G. Sward, Paint testing manual, 12. Ed., 1962, S. 53, Gardner Lab. Inc., Bethseda (Maryland). W. Graûmann, H. Clausen, Deutsche Farben-Z. 7 (1953) 211. W. Jaenicke, Z. Elektrochem. 60 (1956) 163. S. Keifer, farbe + lack 82 (1976) 811. H. G. Vælz, farbe + lack 88 (1982) 356. H. G. Vælz, Die Farbe 25 (1976) 147. G. Booth, H. Zollinger, K. McLaren, W. G. Sharples, Alan Westwell, Dyes, General Survey, in Ullmann's Encyclopedia of Industrial Chemistry,Vol. 9, 5th edit., 1987,VCH Verlagsgesellschaft Weinheim, p. 73. H. G. Vælz, Prog. Org. Coat. 18 (1990), 289. H. G. Vælz, Prog. Org. Coat. 33 (1998), 101.

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

5

How Light Scattering and Absorption Depend on the Physics of the Pigment Particle (Corpuscular Theory)

5.1

Introduction

5.1.1 Description and Significance of the Corpuscular Theory The term ªcorpuscular theoryº refers to model concepts that form a bridge between the Kubelka-Munk coefficients and two physical optical constants of the pigment particle, the refractive index and the absorption index. The development is centered on the theory of Mie, which links the physical constants, including particle size, with the scattering and absorption properties of the particle. With this theory, we complete the progression discussed in Chapter 1, finally getting from color back to the physics. Chapter 3 briefly outlined what differentiates the Mie theory from the phenomenological theory, which also makes statements about scattering and absorption. Following up what was stated there, one can say in simple language that while the phenomenological theory knows about material properties but not about particles, the Mie theory knows about the particle ± but just one particle. The step from here to ensemble and on to the material constants will involve other models of corpuscular theory. It is obvious why the corpuscular theory is of no importance for dye testing, since there are no discrete particles in dye solutions. In fact, however, it is possible to get along without this theory in pigment testing too, at least as far as direct application is concerned. If it is used here anyway ± if it must be used ± the reason lies in the unique insights permitted by Mie calculations of pigments. These are important for understanding circumstances, properties, and processes having to do with the optics of pigments. Only with its help can we understand why white pigments scatter differently or why otherwise identical colored pigments can exhibit different hues if they differ in particle size. This causal link between color properties and particle size means that methods utilizing the Mie theory are also interesting for the determination of particle sizes and particle-size distributions. Such methods, however, are not colorimetric but purely spectroscopic; they are based on the spectrum alone and therefore were not supposed to be discussed in this book. On the other hand, the scope of these meth-

208

5 How Light Scattering and Absorption Depend on the Physics

ods has grown so broad that a description of them could easily fill another book. All the same, the context of this chapter demands a short exposition of particle-size distributions, since the distributions are needed in order to establish the link between the Mie theory and the scattering and absorption coefficients. We will limit ourselves to explaining the basic terms, also leaving out the methods of determination, which can be found discussed in the extensive specialist literature. Similarly, determination methods for the physical-optical constants can be dealt with only in a cursory and decidedly nonexhaustive way ± so that there will be an opportunity to take up the proper subject, colorimetric test methods for coloring materials, and handle it comprehensively.

5.1.2 Particle-Size Distribution The discussion in this section bears a direct relationship to the descriptions and definitions of Section 4.1.1; we will continue to use the standardized terminology*. The particle-size distribution comes from the statistical analysis of the particle sizes in an ensemble (population). Pigments are manufactured on an industrial high-tonnage basis and thus are never monodisperse. The distribution of a particlesize parameter (chiefly the equivalent diameter) can be described in terms of a particle-size distribution curve. These curves generally depend strongly on the type of dispersing medium, the degree of dispersing, and the method of determination. The wetting power and polarity of the medium, the dispersing work done to disintegrate agglomerates, the tendency to reagglomeration, and other factors play significant roles. For these reasons, the particlesize distribution in most cases must be determined in a different way for each application. Statistical frequencies of the particle-size parameters defined in Section 4.1.1 (particle diameter, equivalent diameter, particle surface area, particle volume, particle mass and also the number of particles) are plotted versus the parameter of interest or some other one. A preferred type of plot for pigments is the ªvolume/diameter distributionº, the function u (D) obtained when the volume frequency is plotted against the diameter. The reason therefore has already been discussed: the fact that optical pigment properties such as scattering and absorption are functions of the volume. The following definitions can be stated: ± Density of distribution: the relative frequency of the particle-size parameter in the particle ensemble as a function of this or some other parameter. Especially prominent among particle-size parameters is the equivalent diameter D, but any other measure can be used in its place. Distribution density functions must always be normalized; that is, the total population must yield 100 % ± Cumulative distribution: the normalized frequency (i. e., the frequency referred to the whole ensemble) summed up to a stated value of the particle-size parameter * See ªParticle-Size Analysisº in Appendix 1.

5.1 Introduction

209

± Size fraction and class: the size fraction is the particle ensemble between two fixed values of the selected particle-size parameter that bound the class ± Mean: of the many possible central measures for the particle-size parameter, some are preferred in practice, such as the arithmetic mean, the mode, and the median of the distribution ± Breadth of distribution: a measure characterizing the dispersivity of the particle size in polydisperse populations Empirical particle-size distributions can be represented by the following means used in practice: ± Tables ± Diagrams, such as histograms (bar charts) or closed curves ± Analytic functions obtained by approximation techniques As a rule, a diagrammatic representation is recommended as the way to gain an overview and to make a quick comparison between pigments. The frequencies can be plotted by class and represented as areas in a histogram or bar chart, as shown in Figures 5-1 (distribution density) and 5-2 (cumulative distribution). The horizontal axis for the plot of distributions is the particle-size parameter, commonly the equivalent diameter. Because the parameter can be chosen freely, however, the frequencies for the number of particles, particle surface area, or particle volume (mass) can also be graphed versus a different particle-size parameter selected as the independent variable. In general, these curves are not identical for a given pigment. Special distributions are defined in special standards*: ± Logarithmic normal (lognormal) distribution ± Power-law distribution ± RRSB distribution

Fig. 5-1. Histogram for volume distribution density of a TiO2 pigment. * See ªParticle-Size Analysisº in Appendix 1.

210

5 How Light Scattering and Absorption Depend on the Physics

Fig. 5-2. Cumulative curve for the volume distribution of a TiO2 pigment.

The lognormal distribution is particularly important for pigments, at least when it can be generated by a nucleation and grain growth process. While nuclei ordinarily have a normal distribution on creation, the growth rate of a particle is usually proportional to its surface area. Integration of this growth rule gives a linear time dependence for the log of the particle diameter; substitution in the normal distribution automatically results in the lognormal distribution. A distribution states the probability of a particle being found between values x and x + dx of the particle-size parameter. The equations needed are therefore completely identical to those derived in Section 2.4.1 for the statistical analysis of color coordinates. For example, the series of equations beginning with (2.25) yield the following for the volume/diameter distribution: u D A e

1 2

ds2

mit ds

x

x s

(5.1)

where now x = ln D. The arithmetic mean is x = ln Dz , which is the logarithm of the median of the distribution. Because the sum of the logarithms between 0 and 1 is exactly as great as the sum between 1 and ?, this value divides the area under the distribution function exactly in half. The normalization factor in front of the exponential function changes to A' = A/D because d (ln D) = dD/D. A German standard (DIN 66 144) gives a lognormal coordinate grid. If the particle-size distribution function obeys the lognormal law, the cumulative frequency curve graphed on this grid yields a straight line. For details of the mathematical treatment, reference must be made to the specialist literature. As examples of the form of logarithmic normal distribution functions, which (for the reasons cited) can often be used with success to describe pigment distributions, Figure 5-3 shows several curves for various median diametersDzv1 ; the breadth of the distribution is the same in each case. The type of central measure, as defined in the standards, will be selected case by case in accordance with the test method used or the type of central measure most pertinent to the pigment property of interest. Depending on the breadth of the distribution, a given ensemble or population can show markedly different values of these central measures.

5.1 Introduction

211

Fig. 5-3. Lognormal distributions. Dzv1 is the median of the lognormal distribution; s is a parameter characterizing the breadth of the distribution (s = const = 1.6).

In particle-size analysis (granulometry), ªshape factorsº are sometimes used. With these, equivalent diameters obtained by one determination method should be converted to ªtrueº particle-size parameters. But the determination and use of shape factors is problematic; a better way to do the same thing is to use the statistical tool for the distribution of anisometric particles. While the frequency for isometric particles can be represented by a one-dimensional distribution curve, for anisometric particles it depends on at least two size parameters (e. g., the length L and the breadth B). Because of the dependence on two variables, a frequency surface w = w (x, y) was shown in Figure 5-4 is obtained. To describe the distribution of, say, acicular pigments, the whole shape of the ªhillº must be known, because only in this way is it possible to handle the correlation between L and B. If the logarithms of L and B are denoted by x respectively, the applicable equations are those beginning with equation (2.32). For the same reasons as in the onedimensional normal distribution case, the means are equal to the logarithms of the medians: x = ln Lz and y = ln Bz ; the normalization factor is then B' = B/(Lz 7Bz). Now equation (2.35) with the quadratic form ds2 = 1 represents the ªstandard-deviation ellipseº, which governs the exponents of the lognormal distribution. The family of such ellipses is the adequate form of visualizing the two-dimensional lognormal distribution; their coefficients yield the lengths of the ellipse axes, their slopes, and the eccentricity. At the same time, the coefficients determine the posi-

Fig. 5-4. Two-dimensional normal distribution.

212

5 How Light Scattering and Absorption Depend on the Physics

tion of the median about which the ellipses of equal cumulative probability are grouped, as well as the maximum value of the probability density, which lies at the center of the constant-height ellipses (loci of equal probability density). One way to represent such distribution graphically is the column chart (Fig. 5-5), here shown for the example of a yellow iron oxide pigment. The lognormal distribution is characterized by the concentric ellipses obtained when cumulative frequency is plotted to a logarithmic scale (Fig. 5-6); the constant probabilities on the curves increase from 10 % to 90 % in 10 % steps. The relative eccentricity of the ellipses is a measure of the correlation between the length L and breadth B of the particles. If the eccentricity is 1, there is a rigorous dependence between L and B and the ellipses degenerate to straight lines. If, on the other hand, the eccentricity goes to 0, L and B are independent of one another and the ellipses become circles. The slope of the ellipse axes indicates how rapidly B increases with increasing L. This type of mathematical analysis also prepares the way for cases involving more parameters, in which case higher-dimensional normal distributions are obtained.

Fig. 5-5. Two-dimensional volume distribution density plotted as log L versus log B (acicular yellow iron oxide pigment).

Fig. 5-6. Family of standard deviation ellipses for the two-dimensional lognormal distribution (yellow iron oxide pigment).

5.1 Introduction

213

The methods of determination* (dispersoid analysis) can be discussed only briefly here. The following are applicable to pigments: ± ± ± ±

Particle counting in electron micrographs Sedimentation analysis Light-scattering analysis Analytical techniques based on other physical volume effects such as electrical conductivity.

Particle counting is the most suitable of these methods for pigments. There are several reasons, a few of which are that counting can be done in the vehicle of interest; it can take place in the degree of dispersing that is under study; and concentration problems arise far less often than in other methods, some of which involve extremely high dilutions. The main advantages of counting are that particle shape is determined directly and that primary particles, agglomerates, and aggregates can be distinguished. Once again, further information can be found in the copious specialist literature.

5.1.3 The Optical Constants: Refractive Index and Absorption Index In all the developments up to this point, light could be treated in a geometrical-optical fashion: as propagating continuously in rays. This model was even adequate for the phenomenological theory. The corpuscular theory, however, involves the interaction of light with matter and the constants of that matter, and so it is necessary to come back to the wave nature of light. Light is electromagnetic radiation, and electromagnetic theory (electrodynamics) is governed by Maxwell's well-known equations, which we need not write down here because they can be found in any textbook. There are two differential equations for the electric and magnetic field vectors; their combination gives the universal wave equation for the electric field vector E (x, y, z, t): DE with D

1 u2 E u2 ut2

u2 u2 u2 ux2 uy2 uz2

(5.2)

is the Laplacian and u is the propagation velocity, cm/s. An enormous variety of phenomena are described by this differential equation; for example, every radio and television program in the world is a solution! Here, one of the simplest cases is * See ªParticle size analysisº in Appendix 1.

214

5 How Light Scattering and Absorption Depend on the Physics

to be examined: that of a homogeneous plane wave in a dielectric, with the oscillation in the x, y plane and propagation in the z direction. The solution for the components of E is Ex A eio t

n z c

Ey A eio t

n zid c

Ez 0

(5.3)

where o = 2 pn is the angular frequency, s±1 ; n is the frequency, s±1 ; c is the velocity of light in vacuum, cm/s; A and B are amplitude factors; d is a phase constant (if there is a phase shift between Ex and Ey); and n = c / u is the refractive index. These equations mark the first appearance in electromagnetic theory of a material constant, the refractive index , that links the propagation velocity u in the dielectric and the propagation velocity c in vacuum. If damped waves are also allowed, n has to be replaced by the complex refractive index n n (1 ± ik)

(5.4)

where k is the absorption index. This damping constant, like the refractive index itself, is dimensionless. How n and k can be further related to physical and molecular constants is not of interest here. In connection with absorption and scattering problems involving pigments, however, the experimental determination of these quantities is important. It is necessary to look back at the wave equation in order to explain this point briefly. Suppose one writes this equation for a wavefront incident on the plane surface of a dielectric (x, y plane) at angles j, W. Elementary wave arguments lead to the following conditions that must be satisfied by the electric and magnetic field vectors at the interface: for the reflected wave (i = incident, r = reflected) Wr Wi

(reflection law)

(5.5)

and for the transmitted wave (media 1 and 2) sin W1 n2 sin W2 n1

refraction law (Snell's law)

(5.6)

A boundary condition is needed if one is to answer the question what fraction of the incident radiation is reflected. The condition of continuous amplitudes at the interface is therefore imposed. As a result, the four famous Fresnel equations are obtained; here we use only the two that concern reflection:

5.1 Introduction

rk

sin W1 W2 sin W1 W2

2

tan W1 W2 and rk tan W1 W2

2

215 (5.7)

The reflection coefficient has been analyzed into a component in the place of incidence (r|| and a component perpendicular to that plane (r\). The angles W1 and W2 are linked by Snell's refraction law, equation (5.6). These equations were used earlier in Section 3.1.3. Thus, for normal incidence (W1 = 0), r0 is found very easily (with the approximation sin e & e for small angles; n1 = 1, n2 = n): r0

W1 W2 W1 W2

2

0

12 W1 2 B W2 1 C n 1 C B @ W1 A n1 1 W2

The other coefficients are found by integrating over the half-space. If the complex refractive indices are introduced for n1 and n2 in equation (5.6), two appropriate measurements have been done in equations (5.7), and n1 and k1 are known, then two equations are obtained from which the unknown optical constants n2 (l) and K2 (l) can be determined. This calculation used to be rather time-consuming, but in the computer age it has lost some of its terror. The reflection measurement should not be done at the air/specimen interface; instead, the specimen should be placed in contact with a material having a higher refractive index. The interfaces for this reflection measurement must be highly planar (i. e., as smooth as possible) and polished surfaces. These brief remarks have pointed up all the difficulties that stand in the way of the direct determination of n and k for pigments. The bounding surfaces of pigment particles are in the submicroscopic range, far too small for a reflection measurement ± to say nothing of the fact that ªgoodº surfaces (chemically homogeneous and identical with the pigment material) often cannot be obtained at all. For these reasons, the n (l) and k (l) values used for pigments often have to be the values measured on single crystals of the same material. This substitution is not without its own problems, since it has been shown for many pigments that the particle surfaces can differ chemically from the compact material. For example, TiO2 particles in their normal state have their surfaces covered with OH groups, and the same holds for other inorganic pigments. Organic pigments may also display chemical surface alterations resulting from the production process. As the particle size decreases, the area/volume ratio increases in inverse proportion to the diameter, so that the relative area of a particle measuring 0.1 mm is already a factor of 10 greater than that of a 1 mm particle. The chemical nature of the surface thus becomes rapidly more significant as the particle size decreases, with obvious impact on the optical constants. Thus no one up to now has been able to judge the extent to which constants measured on single crystals are also valid for

216

5 How Light Scattering and Absorption Depend on the Physics

Table 5-1. Refractive indices and optimal particle sizes for some white pigments and fillers at a wavelength of l = 550 nm. Compound, structure

Mean refractive index in contact with Vacuum Vehicle

TiO2, rutile TiO2, anatase a-ZnS, sphalerite ZrO2, baddeleyite ZnO2, zincite Basic lead carbonate Basic lead sulfate BaSO4, barite

2.80 2.55 2.37 2.17 2.01 2.01 1.93 1.64

1.89 1.72 1.60 1.47 1.36 1.36 1.30 1.11

Optimal particle size (in contact with vehicle) Dopt, mm 0.19 0.24 0.29 0.37 0.48 0.48 0.57 1.60

pigments. One would do well to take a skeptical stance toward them and treat results obtained by them (e. g., in Mie calculations) as rough approximations at first. Another source of trouble is that many pigments are optically anisotropic; that is, their n and k values depend on direction. The optical constants referred to the crystal axes can differ widely, as Table 5-2 shows. Averaged constants may be characteristic of pigment populations, depending on the directional distribution of the crystallites. Table 5-2. Refractive indices of important inorganic colored pigments (after Landolt-Bærnstein). Mineral

Chemical formula

Eskolaite Greenockite Goethite Hematite

a-Cr2O3 CdS a-FeOOH a-Fe2O3

Cobalt blue

CoAl2O4

Carbon (Note 2) Crocoite Magnetite Minium Ultramarine

C PbCrO4 Fe3O4 Pb3O4 (Note 3)

l nm 671 589 589 686 blue red 578 671 589 671

Note 1. Mean refractive index. Note 2. Arc carbon. Note 3. Chemical formula [AlSiO4]6(SO4)(S, Cl)2(Na, Ca)8

n no na

ne nb

ng

2.5 (Note 1) 2.506 2.275 2.988 1.74 > 1.78 1.97 2.31 2.42 2.42 1.50

± 2.529 2.409 2.759 ± ± ± 2.37 ± ± ±

± ± 2.415 ± ± ± ± 2.66 ± ± ±

5.2 Mie Theory

217

Another technique for direct determinations on fairly compressible pigments is to press the powder into a compact tablet. Because of residual air included in the compact, mixing rules for the refractive index must be employed in evaluating the data. The surface chemical effects are thus included, at least as an average, and any anisotropy present is at least partly smoothed out. Finally, the immersion method should be mentioned. When larger pigment particles are examined under the microscope, at least the real refractive index n can be determined from the point at which the bounding lines of the crystal vanish. Because of optical anisometry, even this method yields only rough approximations. In the case of the more strongly refracting pigments, there is also a lack of suitable highly refractive liquids or low-melting solids. A further hindrance is that the procedures are laborious and costly and, as a rule, give only the refractive index at a random wavelength or an average over the visible range of wavelengths. In conclusion, it must be stated that exact values for the optical constants of pigments are hardly ever known, even though a knowledge of these values is essential for the development of new products and all analyses of optical performance require them.

5.2

Mie Theory

5.2.1 Integration of the Wave Equation Our theoretical knowledge about the dependence of scattering and absorption on particle size and pigment refractive index is largely based on results derived from Mie theory. The complex of mathematical and physical knowledge that has been gained with this theory would occupy a whole book of its own. If an attempt is made here to trace the essential lines of thought in the theory, it will be done in quite brief form and under restrictive assumptions. For simplicity, the treatment is done with an eye to one objective, understanding the results of the theory as they apply to pigments. The model is a dielectric sphere on which a plane wavefront is incident. Application of the wave equation reveals that the sphere is excited into oscillation; as a oscillating multipole, it then acts as the center from which new waves are emitted. These waves are superposed on one another. First, in wave equation (5.2) ± including the Laplacian ± one must separate the time function and rewrite the equation as a harmonic oscillation for the polar coordinates r, j, W suitable to the problem. The result is called the Helmholtz equation. Its solutions can be found in textbook of theoretical physics. Any such solution can be written as a sum over products of three complex-valued functions; for example, the radial component of the electric field vector E is given by

218

5 How Light Scattering and Absorption Depend on the Physics

Er

1 P j1

Aj n; a Yj W Fj j

Along with the refractive index n, this includes the typical dimensionless parameter a

D p n0 l

(5.8)

where D is the particle diameter and n0 is the refractive index (relative to vacuum) of the medium surrounding the particle. The complex-valued functions have the following meanings: A (n, a): spherical Bessel function (n is the refractive index of the particle relative to the surrounding medium) Y (W): spherical functions (spherical Legendre polynomials) F (j): exponential function The summation takes care of the superposition of excited partial vibrations. In order to get to intensities, one must form the absolute squares of E. Two expressions are obtained: I|| for the ray parallel to the incidence/observation plane and I\ for the ray perpendicular to that plane. These are enough to describe unpolarized light. For specified sphere parameters n, a, these functions depend only on W (by the axial symmetry of the system); they can also be taken from tables (see Section 5.3). If the complex refractive index n* = n (1 ± ik) is formally introduced, the formulas once again include absorption. The solutions of the Mie theory for small particles show that the entire particle oscillates symmetrically as a dipole, along and opposite to the propagation direction of the incident wave. In the case of larger particles, multipole oscillations also occur; what is more, the secondary waves do not oscillate in phase. Figure 5-7 shows the first three partial oscillations as field lines on the surface of the sphere. The vibration place of the light ray generating the waves is in the plane of the drawing, so that the direction of propagation is perpendicular to the drawing plane. This is a symmetry plane of the process, and so the front hemispheres shown must be complemented by the back hemispheres, on which the curves fall into congruent patterns. Secondary waves outside the sphere are generated by the incident plane wave. For very small particles, the whole particle oscillates as a dipole; the excitation is symmetric, in and opposite to the propagation direction of the incident wave. Larger particles experience multipole oscillations; the secondary waves oscillate in unequal phases, and the superposition of the partial waves yields an increasingly complicated spatial distribution with a growing number of maxima and minima. There is also a decrease in the fraction scattered into the back half-space relative to the front half-space (see Fig. 5-8 for an example).

5.2 Mie Theory

219

Fig. 5-7. The first three partial oscillation modes of a dielectric sphere after Mie.

Fig. 5-8. Polar diagram for the emission distribution of a scattering sphere having n = 1.7 and a = 4.3, after J. Thiemann. (The center of the scattering particle is to be imagined at the cross+).

Similar calculations have been done for cubical, cylindrical, and ellipsoidal particles. These calculations are exceedingly complex, so that approximations are only used in practice. For the anisometric particles under consideration, one obtains a simplified scheme of two absorption and two scattering functions, one each perpendicular and parallel to the longitudinal axis of the particle.

5.2.2 Absorption and Scattering of the Particle Ensemble The solutions I || and I\ of the Mie theory will now be related to the Kubelka-Munk scattering and absorption coefficients. For it, with I || and I\, the fractions scattered into the space surrounding the sphere and absorbed in the sphere must be summed. This is done by integrating over the area 4p of the unit sphere* and dividing by the particle cross section D2p/4. the integral over j can be written out immendiately (I || and I\ do not depend on j):

* In the case of scattering, integration over the back hemisphere, i. e., 0 5 W 5 p /2, is also recommended.

220

5 How Light Scattering and Absorption Depend on the Physics

Z2p Zp 1 1 Q 2 dj f W Ik Ik sin W dW D p 4p j0 W0 4 2 2 D p

Zp

f W Ik n ; a; W Ik n ; a; W sin W dW

0

In this way, expressions not containing j and W are obtained: the scattering cross section QS (n, a) (real part) and the absorption cross section QA (n*, a) (imaginary part). The function f (W) takes care of the fact that the Mie theory (directional incidence of light) is not based on the same geometry as the Kubelka-Munk theory (diffuse incidence, plane-parallel layer). For absorption, fA = 2 in agreement with Kubelka's assumption in Section 3.2.2; for scattering, according to Mudgett and Richards, fS = (3/8) (1 ± cos W). The quantities QA and QS are dimensionless; they represent the ratios of the optically effective cross sections to the geometrical cross section: qopt qA 2 qgeo Dp 4 qS QS n; a 2 Dp 4

QA n ; a

i. e. qA l; n; k; D qS l; n; D

D2 p QA n ; a 4

D2 p QS n; a 4

For practical use, the quantitative reference must be made to the pigment particle, for knowing how much one pigment particle scatters or absorbs is less important than knowing how much 1 L or 1 kg of pigment does. The single-particle quantities k1, s1 referred to volume are obtained by dividing by the particle volume V = D3p/6 and using equation (5.8): k1 l; n; k; D s1 l; n; D

qA 3 3 p n0 QA l; n ; a QA l; n ; a V 2l 2D a qS 3 3 p n0 QS l; n; a QS l; n; a V 2l 2D a

(5.9)

5.2 Mie Theory

221

In the case of monodisperse particles, the quotient Q / a is thus proportional to the Kubelka-Munk coefficients. The spectral Kubelka-Munk coefficients referred to PVC, on the other hand, are generally constants of the material for ensembles of polydisperse distributions. They are thus obtained by summing the contributions over the particle-size distribution u (D): k l; n; k s l; n

R1 0

R1 0

u D k1 l; n; k; D dD u D s1 l; n; D dD

(5.10)

In the case of distributions of anisometric particles u (L, B),the angular distributions must also be known if one wishes to use a sum formula on the above pattern. If a random distribution (i. e., no preferred direction) is assumed, u (L, B) can be written, similarly to the above case, provided the scattering and absorption cross sections parallel and perpendicular to the axis of the acicular or platy particle are known (see Section 5.2.1). Two important special cases should be examined: those where the particles are very small and very large relative to the wavelength. Approximations will be obtained in both cases. For absorption, a fairly simple summary can be given: Thus, for particles smaller than a certain limiting size, absorption is independent of D; for large particles, absorption falls off as 1/D. An explanation of this behavior will follow in Section 5.2.3. The effect of particle size is somewhat more complicated for scattering. For large particles, scattering also decreases as 1/D (Fresnel reflection), since the sphere acts as a reflecting mirror. We have 3 n 1 2 QS where QS r0 s1 2D n1 In the small-particle case, Rayleigh scattering is obtained. The small sphere is excited only to dipole oscillations. The result is QS

8 4 2 aM 3

where

M

n2 1 n2 2

Here we are in the realm of molocular scattering, where the scattering cross section decreases as* a4*1/l4. This relation explains, say, why the sky is blue: The molecules of the atmosphere scatter violet light (l = 400 nm) more strongly than red * In this text, * denotes proportionality.

222

5 How Light Scattering and Absorption Depend on the Physics

(l = 700 nm) by a factor of (700/400)4 & 10. The sky is blue, rather than violet, because the solar spectrum contains far less violet than blue and because the sensitivity of the human eye rapidly falls off toward zero as the wavelength becomes shorter. Rayleigh scattering ceases to be important in the particle-size range of pigments, because Mie scattering dominates it by some orders of magnitude.

5.2.3 Scattering Behavior of Pigments Using the behavioral rules outlined above, van de HULST gave an equation for nonabsorbing spheres and for n = 1 + e: 4 4 sin b 2 1 b b where b 2a |n ± 1|

Qext 2

cos b (5.11)

where the extinction cross section ± the flux scattered away into all of space related to the geometrical cross section ± is described as a function of a and n. This is one of the most important formulas in the whole field of Mie theory, for it describes the essential features of scattering. It is valid not just for n close to 1 but even for n = 2. This can be seen from the curves of Figure 5-9, which shows scattering curves for refractive indices 0.8 5 n 5 1.5. The b scale at bottom applies to all five curves; there is a different a scale for each n.

Fig. 5-9. Total scattering cross section Qext calculated by Mie theory for n = 1.5, 1.33, 0.93, and 0.8.

5.2 Mie Theory

223

The most striking fact is the succession of maxima and minima. These extreme values result from interference between the refracted and transmitted light; maxima occur where the superposed waves reinforce, minima where they cancel. For small particles, the curves ought to begin as a4 (Rayleigh scattering), but equation (5.11) does not properly reflect this fact. The ordinates Qext increase systematically for larger n because of grazing reflection. From the van de Hulst calculated values, linear regression analysis yields the relation Qmax 2.716 n + 0.3235

(5.12)

The first minimum (ªfirst Mie minimumº) can still be clearly measured for isodisperse populations (e. g., latexes). The existence of the principal maximum immediately implies that an optimal value a must exist. Hence it follow that ± There must be a particle size optimal with respect to lightening power ± For a given particle size, there exists a wavelength at which the scattering takes on maximal values Because what is wanted is a proportionality to the Kubelka-Munk PVC-referred coefficients s1 (eq. 5.9), only scattering into the back half-space is to be counted. Semiquantitatively, this fraction can be set roughly proportional to Qext for a constant refractive index. Then, from the maximal value bopt & 4, Figure 5-9, immediately gives D p n0 n 1 4 (5.13) bopt 2 a n 1 2 l If the refractive index is given, an expression can be obtained for the optimal aopt ; if l is given, the optimal particle size can thus be found. In the case of TiO2 in rutile form (n = nTiO2 /nmedium = 2.8/1.5 & 1.9), for l = 550 nm we obtain Dopt

bopt l 4 0:55 0:26 mm 2 p 1:5 0:9 2 p n0 n 1

(5.14)

which is fairly close to the experimental value (see Table 5-1). Improved values are obtained if bopt is taken not at the maximum of Qext but at the maximum of Qext/a as suggested by equation (5.9). The division shifts the optimum to somewhat smaller values, giving bopt = 2.93, resulting in a Dopt of 0.19 mm for rutile. Figure 5-10 presents scattering curves of Qext /a for well-known white pigments, calculated with van de Hulst formula (5.11). As the refractive index decreases, the optimal particle size, typically, grows larger and less scattering takes place. Finally, when the refractive index approaches that of the vehicle, Qext/a decreases as 1/a, the behavior seen for Fresnel reflection, and vanishes. The optimal particle sizes for bopt = 2.93 were calculated with equation(5.13) and are listed in Table 5-1.

224

5 How Light Scattering and Absorption Depend on the Physics

Fig. 5-10. Scattering curves (plots of Qext /a versus particle size) for some white pigments and fillers.

The wavelength dependence of scattering can be determined with equation (5.11); the curve for n = 1 + e (Fig. 5-9) can also be used in a semiquantitative analysis. The plot in terms of a * 1/l must be read from right to left in order to trace what happens as the wavelength increases. The presence of the maximum indicates that particles smaller than Dopt preferentially scatter short-wavelength light while those larger than Dopt preferentially scatter long-wavelength light. This situation explains how white pigments in gray pastes can produce a colored shade through selective scattering: Finely-divided white pigments give bluish hues while larger ones give brownish hues.

5.2.4 Absorption Behavior of Pigments Van de Hulst also gives an equation for the absorption, but we need not discuss this because, fortunately, BROCKES has done systematic Mie calculations for fixed n and k. His curves (Fig. 5-11) are log-log plots of QA /a versus a for a range of n and nk. They imply the following: ± For very small particles, absorption is independent of a and thus of particle size. In other words, absorption will not increase on further size reduction. As the absorption index grows larger, absorption increases ± For very large particles, absorption is approximately the same for all refractive indices and absorption indices, falling off hyperbolically. The particle absorbs and reflects in accordance with its cross section, so that QA /a decreases as 1/D ± The uppermost curve in Figure 5-11 is for pigments with high absorption index k but low refractive index n, such as carbon black pigments. It shows that the optimal particle size is less than an identifiable limit ± The lowermost curve is for pigments with small absorption index k but high refractive index n, such as most inorganic pigments. This curve has distinct maxima, which should be thought of as higher and steeper than the log-log plot shows

5.2 Mie Theory

225

Fig. 5-11. Absorption curves of QA /a (log-log plot), after Brockes.

One other important point should be mentioned because it is overlooked many times. At the positions k (l0) of absorptions in the spectrum, the refractive index behaves in a anomalous way as described by the well-known dispersion formula n

1

k l0 2 l0 1 l

Figure 5-12 presents an example of the refractive index discontinuity for real pigments that exhibit absorption peaks of finite breath. Because the scattering shows a direct dependence on n, it also has a discontinuity. The rule is that the refractive index drops abruptly on the rising edge of the absorption and rises abruptly on the falling edge. This behavior of the scattering characteristic may well lead to remarkable color effects. There are cases of pigments in which absorption and scattering are antagonistic and others in which they vary in the same sense. The red iron oxide pigments can serve as an example of the second type. For particles smaller than Dopt, equation (5.13) says that lmax must also become shorter, if one would hold the maximum. this means that the position of maximal scattering shifts toward shorter wave-

Fig. 5-12. Absorption and anomalous refractive index.

226

5 How Light Scattering and Absorption Depend on the Physics

lengths: The red takes on a yellow cast. The absorption maximum shifts at the same time, also to shorter wavelengths, and this effect strengthens the yellow cast. For particles larger than Dopt , yellow is taken away in both ways, and the pigment becomes redder. In pigment reduction with TiO2, such coarse pigments are actually seen to take on a marked blue cast. Two factors can account for this effect: First, the absorption of the red pigment moves toward longer wavelengths, thus setting blue light free; second, the scattering increases suddenly because of the anomalous dispersion of the TiO2 pigment, whose strong absorption ends near 400 nm. The Mie theory has made it possible to predict the reflection spectrum of a pigment, and thus its color properties, given the complex refractive index, the concentration, and the particle-size distribution. We have now reached the goal stated in Chapter 1 by tracing the amazing range of optical qualities seen in coloring materials ± their technical color properties ± back to measurable physical quantities.

5.3

List of Symbols used in Formulas

a = Dpn0 /l A, B A (n, a) b = 2a | n ± 1| B B Bz c d ds2 D Dz E I k k1 k l L Lz M n

parameter in the Mie theory amplitude factors spherical Bessel function parameter in the van de Hulst equation normalization factor for two-dimensional normal distribution breadth of anisometric particle, mm median particle breadth, mm velocity of light in vacuum, cm/s phase constant quadratic form of normal distributions particle diameter, mm median particle diameter, mm electric field vector radiance factor, W cm±2 absorption coefficient per unit PVC, mm±1 single-particle absorption coefficient per unit PVC, mm±1 absorption index wavelength, nm length of anisometric particle, mm median particle length, mm abbreviated notation: M = (n2 ± 1)/(n2 + 2) (real) refractive index with subscript: 0 of the medium

5.4 Summary

n* = n (1 ± ik) n = c/u o = 2pn j F (j) q

Q r r s s1 s W Y (W) u u (D) x

5.4

227

complex refractive index frequency, s±1 angular frequency, s±1 meridian angle in spherical coordinates exponential function optically effective cross section, cm2 with subscripts: A absorption cross section ext total scattering cross section (nonabsorbing sphere) S scattering cross section effective cross section with same superscripts as q reflection coefficient distance from origin in spherical coordinates scattering coefficient per unit PVC, mm±1 single-particle scattering coefficient per unit PVC, mm±1 standard deviation, a parameter of distribution breadth polar angle in spherical coordinates spherical function propagation velocity, cm/s volume distribution of diameter general particle-size parameter

Summary

The corpuscular theory finally relates the material constants for absorption and scattering to the individual particle and its physical properties. At the center of the analysis is the Mie theory, which derives scattering and absorption properties from a few fundamental physical quantities. It is therefore important only for pigments, not for dyes, although even for pigments it yields insights that could not be received in any other way. The basic physical quantities are particle size, refractive index, and absorption index. Because a pigment ensemble comprises fractions differing in particle size, the statistics ± the particle-size distribution ± must here be treated. The optical scattering and absorption properties are volume-dependent, so that the preferred way of representing these data is the distribution density of volume versus diameter: u (D). The following concepts are discussed: distribution density, cumulative distribution, size fraction and class, measures of central tendency, and measures of distribution breadth. Representations include tables, diagrams, and analytic functions. When unlike pigments are to be compared, plots of distribution density and cumulative distribution are particularly useful. When distributions are to be described by analytic functions, the logarithmic normal (lognormal), power-law, and RRSB distribu-

228

5 How Light Scattering and Absorption Depend on the Physics

tions can be used; of these, the lognormal is especially well-suited to pigment distributions. In this distribution, the central measure is the median. For describing anisometric (e. g., acicular or platy) particles, the tools of mathematical statistics are also available. The two-dimensional lognormal distribution of particle length L and breadth B also yields a graphical representation and makes it possible to calculate the parameters and central measures. The eccentricity of the calculated standarddeviation ellipse is a measure of the correlation between length and breadth. The principle can be extended when more than two particle-size parameters are needed. This chapter gave only a brief discussion of methods used to determine the particle-size distribution. The phenomena treated here require for the first time that the wave nature of light must be considered. From the differential equation that describes oscillation processes (wave equation), the homogeneous plane-wave solution is derived; it contains the refractive index n as a constant. For absorption, there is also a damping constant k; the complex refractive index n* is formed by k together with n. Reflection and refraction laws are effortlessly derived from the wave equation by postulating continuity at the interface between two media. An attempt to obtain the fraction reflected and transmitted leads to the Fresnel equations, with whose aid n and k can be determined from reflection measurements. Because of the small size of pigment particles, unfortunately, such direct measurements are exceedingly difficult. In practice, it is necessary to employ physical constants measured on large single crystals instead, and ultimately this substitution is not satisfactory. What is more, the optical anisotropy of most pigments makes it hard to determine and use the constants. Reflection measurements to obtain the constants can be done on pressed pigment powders if the material is sufficiently compressible. The immersion method has sometimes been used to determine n. At present, there are just a few values of the optical constants directly measured on the pigment. The Mie theory, which uses a model of a plane wave incident on a dielectric sphere, is discussed as it aids in understanding pigment phenomena. The theory of differential equations gives solutions containing a = Dpn0 /l as a typical parameter. These are also functions of the angles j and W in the three-dimensional coordinate system. After introducing the complex refractive index, one can split the solutions into scattering and absorption parts. The results show that the spherical particle acts as an emission center for new waves that interfere with one another. Even anisometric particles have been calculated with the Mie theory. The procedure for linking the radiance factors in Mie theory to the KubelkaMunk coefficients involves first integrating over the solid angle (giving scattering cross section and absorption cross section). The result is divided by the sphere volume and then summed over the particle-size distribution. The same technique can be used with anisometric particles if the angle-dependent cross section values are known. Rayleigh scattering on very small particles (not important for pigments) and Fresnel reflection on very large particles are discussed. A formula stated by van de Hulst is examined as a way of describing how the scattering cross section depends on the refractive index and the parameter a. The

5.5 Historical and Bibliographical Notes

229

result displays maxima and minima, which can be attributed to interference between the partial oscillations. The principal maximum shows that there must be optimal particle sizes, or optimal wavelengths, for scattering. From the position of the principal maximum, the optimal particle sizes for well-known white pigments and fillers are derived along with the scattering curves. This procedure provides an explanation for the shade of white pigments in gray pastes. The laws describing the absorption of inorganic and organic pigments are obtained from Mie calculations performed by Brockes. Once again, maxima appear. Anomalous dispersion, seen at absorption edges, also has some effect. The results also account for the hue shift in iron oxide pigments when the particle size changes. The Mie theory makes it possible to calculate in advance the color properties of pigments.

5.5

Historical and Bibliographical Notes

The significance of particle size to the pigment properties has already been referred to, as have the various particle-size parameters; see [1±4] in Section 4.10. These prior publications also deal with the parameters and representations suitable for particle-size distributions. A special analysis of the logarithmic normal distribution appears in [1]. The mathematical treatment and representation of distributions of anisometric particles was first published just a few years ago [2]. The MIE theory [3], dating from 1908, is based on the principles of classical electrodynamics, which has been covered in textbooks [4], [5]. MIE derived this theory as a physical explanation of the color displayed by gold sols having various particle sizes; it was a complete success. The application to very small particles is due to Raleigh [6]. Manual Mie calculations used to be very tedious because of the summations that had to be done, but later workers [7±9] have performed calculations for a range of refractive indices; one much-used set of tables is due to Lowan [10]. Nonspherical particles such as cubes and ellipsoids have also been calculated [11]. Although there were no calculations for refractive indices in the range of 1.6 5 n 51.9, the very range of interest for pigments, an attempt was made at an early point to generalize the results into a single universal scattering function, with the object of predicting optimal particle sizes for the most important pigments. One such procedure is described by Jaenicke ([26] in Chapter 4). the approach taken in this book to determining the optimal particle size with respect to scattering was devised by van de Hulst, whose monograph Light Scattering by Small Particles [12] is the best treatment of this area. Kerker's book on scattering [13] should also be cited, as should the book by Kortçm ([19] in Chapter 3). Computers have greatly simplified the process of doing Mie calculations; this capability has been heavily used, for example by Dettmar [14] for higher refractive indices. Dettmar also performed the calculations for iron oxide pigments ci-

230

5 How Light Scattering and Absorption Depend on the Physics

ted by Brossmann [15] and those for the absorption of pigment particles, which were used by Brockes [16] in the publication discussed in Section 5.2.4. The application of Mie calculations to practical problems has been reported by Maikowski [17], Hauser and Honigmann [18], and Hediger and Pauli [19]. An interesting test is the one carried out by Felder [20]: spherical pigment particles made of a soft material (dyed PVA) were deformed into ellipsoidal particles by stretching the medium in which they were embedded. The results revealed how absorption changes on the transition from spheres to ellipsoids. The literature on methods for finding the optical constants of pigments by the immersion method is rather sparse; the same can be said for measurements done on colored pigments (see, e. g., [21]). In methods based on pressed powder measurements, the presence of residual air in the compact means that refractive index mixing rules must be employed [22]. Given two reflection measurements, the Fresnel equations simultaneously yield n and k, as Nassenstein has shown [23]. Unfortunately, this technique applies only to easily compressible pigments, a class that does not include inorganic pigments. Some work remains to be done in this direction.

References [1] J. Aitchinson, J. A. C. Brown, The Lognormal Distribution, Cambridge University Press, London, 5. Repring 1973. [2] H. .Vælz, farbe + lacke 90 (1984) 642 und 752. [3] G. Mie, Ann. Physik 25 (1908) 377. [4] G. Joos, Leerbuch der Theoretischen Physik, Geest & Portig, 7. edit., Leipzig 1950. [5] J. Honerkamp, H. Ræmer, Grundlagen der klassischen Theoretischen Physik, Springer, New York 1986. [6] J. W. Rayleigh, Proc. Roy. Soc., Ser. A, 90 (1914) 219. [7] H. Blumer, Z. Physik 32 (1925); 38 (1926) 920; 39 (1926) 195. [8] E. J. Meehan, H. Beattle, J. Optc. Soc. Am. 49 (1959) 735. [9] R. D. Murley, J. Phys. Chem. 64 (1960) 161. [10] A. N. Lowan, Tables of scattering functions for spherical particles, in Nat. Bur. Stand., Appl. Math. Ser. 4 (1949), US Gov. Print. Off. Washington 1948. [11] R. Gans, Ann. Physik 37 (1912) 881. [12] H. C. van de Hulst, Light scattering by small particles, J. Wiley & Sons, London 1957. [13] M. Kerker, The scattering of light, Academic Press, New York etc. 1969. [14] H. J. Metz, H.-K. Dettmar, Kolloid-Z. 192 (1963) 107. [15] R. Broûmann, AIC Color 69 Stockholm, Congr. B. Vol. 2, 15. [16] A. Brockes, Optik 21 (1964) 550. [17] M. A. Maikowski, Z. Elektrochem. 71 (1967) 313. [18] P. Hauser, B. Honigmann, farbe + lack 81 (1975) 1005. [19] H. Hediger, H. Pauli, XIX. Fatipec Congress Aachen 1988, Congr. B. II, 503. [20] B. Felder, Helv. Chim. Act. 49 (1966) 440. [21] V. Koutnik, Chem. Prumysl (Chem. Ind. CSSR) 11 (1964) 604. [22] W. Heller, Gov. Res. Rep. US Opt. Commerce, Nr. AD 608 337 (1964). [23] H. Nassenstein, AIC Color 65, Luzern, Congr. B 12.

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

Part II Test Methods

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

6

Measurement and Evaluation of Object Colors

6.1

Reflection and Transmission Measurement

6.1.1 Gloss Measurement and Assessment When light falls on a body, part of it is generally reflected at the surface of the body, even before the absorption and scattering processes described in Chapter 1 can take place in the interior of the layer (Fig. 1-1). The fraction reflected at the surface, as described by the Fresnel equation, is a function of the refractive index n and the angle of incidence. For perpendicular irradiation, the reflected fraction is given by r0 = (n ± 1)2/(n + 1)2 ; for paint and lacquer films with refractive indices of n & 1.5, this formula gives r0 & 0.04. The fraction increases very slowly with increasing angle of incidence and attains high values only at grazing incidence, that is, at incidence angles just below 908 (Fig. 6-1).

Fig. 6-1. Fresnel reflection at some surfaces.

234

6 Measurement and Evaluation of Object Colors

If the fraction reflected at the surface is plotted as an indicatrix, that is, as a function of the observation angle e2 in polar coordinates, two extreme cases can be identified: ± Directional reflection only (Fig. 6-2) ± Diffuse reflection only (Fig. 6-3)

Fig. 6-2. Specular (directional) reflection.

Fig. 6-3. Diffuse reflection.

The first case corresponds to regular specular reflection; in the second case, numerous microscopically small irregularities at the surface give rise to backscattering independent of the angle. The indicatrix here obeys the Lambert cosine law: r = cos W. Real paint and lacquer coatings commonly exhibit a mixture of the two extreme behaviors. It should be emphasized that this reflected light is no longer available to take part in absorption and scattering processes in the coating. As a consequence, the effect of surface reflection must be properly considered in color evaluation. We will hear more on this point in Section 6.1.2. Here, what is of interest about surface reflection is whether it is directional or contains directional components. One speaks of the ªglossº of a surface and distinguishes between ªhigh glossº and ªmat glossº (Fig. 6-4). These terms do not only refer to the purely physical phenomenon of surface reflection but rather to a visual experience. It follows that gloss has a physiological component plus a psychological one.

6.1 Reflection and Transmission Measurement

235

Fig. 6-4. Indicatrices for a nearly mat surface (1) and a high-gloss surface (2).

Studies of the way in which observers evaluate gloss have identified at least two types of observers: ± The ªanalyzingº observer, who considers the sharpness with which reflected objects (e. g., window cross) are imaged ± The ªintegratingº observer, who considers intensity contrasts of the reflected light; for example, the ªGolden Helmetº (formerly attributed to Rembrandt) gives the illusion of gloss without reflective surfaces, simply through the juxtaposition of light and dark. In visual gloss evaluation, as a rule, the evaluator includes varying proportions of both observers. It is immediately clear that the observer behavior just described can scarcely be imitated by any gloss measurement technique with a purely physical basis. The situation is similar to that in colorimetry, though in that instance the dilemma could be resolved by postulating a standard observer and basing definitions on matching judgments. It is not entirely out of the question that a similar approach might work in gloss evaluation; it is, however, made difficult by the two modes of visual assessment and the accidental mixing of these modes. In view of these circumstances, the gloss has to be determined as a function of observation angle in the great majority of cases. The preferred type of plot is the polar gloss indicatrix, as shown in Figure 6-4, but a bell-shaped curve in Cartesian coordinates is quite usual. Such a distribution curve is analogous to the spectral distribution in colorimetry (Chapter 2); the fact that no ªstandard gloss observerº exists here stands in the way of a more physiologically-oriented treatment of the measured values. The complete gloss curve is measured with a gonioreflectometer (goniophotometer), a instrument in which the angle of incidence can be set to any value and a probe (photocell) is placed on the observation side (Fig. 6-5). The probe is traversed across the cone of scattered light as the intensity distribution is measured and plotted. The resulting curve (indicatrix) can often be described in terms of a few parameters, chiefly the maximum value and half-value width. The proper functioning of a goniophotometer imposes certain requirements on construction, chiefly relating to the parallelism of the ray path and the aperture

236

6 Measurement and Evaluation of Object Colors

Fig. 6-5. Diagram of the reflectometer with ray paths.

angle on the observing side. These essential detail can be found in standards*. The same standards also describe simplified glossmeters in which definite aperture angles are set for three distinct incidence angles (208, 608, 858). The viewing angle should be equal to the angle of incidence and must not differ from it by more than +0.18. The incidence angles are recommended as follows for best differentiation in various applications: ± 208 for high-gloss specimens ± 608 for specimens with moderate gloss ± 858 for mat specimens Suitable primary standards are plane, polished plates of black glass having a refractive index of 1.567 for a wavelength of 589 nm. For each of the three incidence angles, the reflectometer reading for this standard is set equal to 100. If the refractive index differs from the stated value, the reflectometer reading for each of the three angles can be calculated with the Fresnel equations (which are stated in DIN 67530). Two gloss-related effects due to pigmentation should be mentioned here. First, it is often observed that the gloss initially decreases as the pigment concentration increases; at higher concentrations, particularly just before the critical pigment volume concentration is reached, the gloss may increase again. The cause of this phenomenon lies in the fact that the pigment particles become more and more ordered as the critical condition is approached; at the critical concentration they take on a close-packed configuration with binder filling the voids. This change is accompanied by smoothing of the surface, which was irregular at low concentrations because of individual pigment particles protruding from it. Second, when the mirror * See ªGloss, Measurementº in Appendix 1.

6.1 Reflection and Transmission Measurement

237

image of a very bright, small source of light in such a paint film is examined, a halo is seen around the image of the source (ªgloss hazeº). An incandescent filament thus appears as if viewed through a thin veil; that is, diffuse reflection is more intense in directions near the specular angle than far from it. Gloss haze is due to microscopic irregularities in the outermost layers of the surface, which may be present because, for example, inadequate pigment dispersing has left pigment agglomerates behind. The effect is easily measured with the goniophotometer by making the aperture angle as small as possible and traversing the measuring probe over a few degrees about the specular angle. Gloss effects with metal-effect paints are also caused by pigments (metaleffect pigments). Because the optical phenomena on such coatings have to be characterized by color measurement, they will not be described until later (Section 6.2.4). The term ªgloss developmentº denotes the variation of the degree of gloss as a function of the dispersing time. As a rule, gloss development is a way of gaining information about the progress of the dispersion process (Section 4.1.2). The measure used, as set forth in ISO 8781-3, is the dispersing work required to attain a given reflectometer value. Alkyd resin system* and alkyl/melamine resin systems** can be used as test media. These test methods, similarly to those for tinting strength development (Section 4.7.3 and 8.2.4), makes it possible to compare pigments, mill base compositions dispersing equipment, or dispersing processes. Preparation method: The test and reference pigments are dispersed in a suitable vehicle in accordance with suitable conditions (vehicle and conditions are to be agreed on). As the dispersing process continues, samples are taken from the batch and applied to a substrate; after drying or stoving, reflectometer values are measured.** Evaluation method: A diagram is prepared showing the reflectometer value (ordinate) versus the dispersing work (abscissa), that is, the dispersing time or stage. A curve is fitted to the point and, from the curve, the dispersing work required to attain a pre-estabilshed reflectometer value is read off.

6.1.2 Measurement and Evaluation Conditions We now turn back to the discussion in Section 2.1.2, where it was shown what geometrical configurations are used in the measurement of reflectance, reflection factor, transmittance, and transmission factor. Now we will explain how these geometries can be realized in instruments; it will be seen that the geometrical conditions of irradiation and observation, the ªmeasuring conditionsº, play a vital part***. * See ªEase of Dispersionº in Appendix 1. ** See ªGloss Measurementº in Appendix 1. *** See ªColorimetryº in Appendix 1.

238

6 Measurement and Evaluation of Object Colors

Fig. 6-6. The 45/0 geometry.

We begin with the 45/0 geometry, as illustrated in Figure 6-6. The source aperture angle should be no larger than 208, the receptor aperture angle no larger than 108. For specimens with surface texture, the reflection factor Rc depends on the orientation of the specimen relative to the direction of incidence; the predominant texture direction should be parallel to the plane of incidence. The figure also shows that the rays are not directional but conical (quasiparallel). In geometries with diffuse irradiation or diffuse observation, an integrating sphere is used to create a hemispherical distribution of flux. Figure 6-7, for example, shows the use of the integrating sphere for the 8/d geometry (reflectance Rc). If incidence on the specimen is diffuse (hemispherical), the setup of Figure 6-8 is em-

Fig. 6-7. Integrating sphere used in measurement of Rc (8/d geometry).

6.1 Reflection and Transmission Measurement

239

Fig. 6-8. Intregrating sphere used to create diffuse irradiation (a and b show alternative configurations).

ployed, giving the d/8 geometry (reflection factor Rdif ). Here the specimen and standard are measured in a comparative method; they are placed at the respective ports in the sphere either simultaneously or one at a time. Geometries involving the integrating sphere have this peculiarity: If the directionally reflected fraction of the radiation is absorbed or allowed to escape from the sphere (ªgloss exclusionº by a ªgloss trapº), what is measured is solely the scattered reflection without directional components (Fig. 6-7). Geometries with gloss exclusion therefore give values similar to those for the 45/0 geometry, in which, similarly, the directional components on the observing side are not measured. Whenever necessary to maintain this distinction, the subscript letters ªinº (inclusive, with surface reflection) or ªexº (exclusive, without surface reflection) will be added to the symbols for the reflection values. The decision whether or not to measure the directional components of the reflected radiation is extremely important for the measurement of nonluminous perceived colors. As a consequence, the geometries just described can also be classified by whether the surface reflection is included or excluded*: ± Method A: Geometry 8/d (reflectance Rin,c) or d/8 (reflection factor Rin,dif ), with no gloss trap in either case. The surface reflection is included in the measurement. Evaluation: Before calculating the color difference in accordance with * For standards see ªColor Differencesº in Appendix 1.

240

6 Measurement and Evaluation of Object Colors

ISO 7724/3, a correction for the surface reflection (r0 = 0.04; see preceding section) must be subtracted from the measured values. ± Method B: Geometry 45/0 (reflection factor Rc), resp. 8/d or 0/d both with gloss exclusion (reflectance Rex,c), and their inverses. The surface reflection is not measured. Evaluation: The color difference is calculated in accordance with ISO 7724/3, directly from the measured values (i. e., without the subtractive correction for surface reflection). In Method A, the color differences determined between test and reference specimen are those having to do with differences in coloring materials. The results are generally not affected by differences in specimen surface quality. Accordingly, Method A is particularly suitable for pigment testing. The only exception is in the fullshade determination of black pigments (see Section 6.2.2). If the gloss changes, the total surface reflection, which consists of a directional and a diffuse component, remains constant when Method A is employed for the measurement. Because the total surface reflection is included in the measurement and a correction must be made by subtracting the surface reflection from the measured value, color differences obtained in this way are strictly due to differences or changes in the interior of the system. If the measured values were used directly (i. e., without subtracting the surface reflection) for calculating color differences, the results would be too small because of the convexity of the cube-root curves for X ,Y , and Z (see Chapter 2). This holds particularly for color-saturated or dark specimens. Essentially, the effect of calculating out the surface reflection is that color differences are roughly the same as seen by an observer looking in a ªgloss-freeº manner at high-gloss specimens, that is, if the surface reflection were ªreflected outº at the time of observation. In the case of mat specimens, the color differences are equal to what an observer would see if diffuse surface reflection were eliminated, that is, if a coat of lacquer binding medium were applied to the specimen to render it glossy and the specimen were then examined in a gloss-free manner. Colorimetric evaluation by this method, then, has a direct visual analog only for highgloss specimens. In Method B, the color differences found between test and reference specimen are those that stem from the coloring materials as well as differences in surface quality. Accordingly, specimen color differences come out approximately the same as in visual color matching with gloss exclusion. If a specimen loses its gloss, as in the course of a durability test, the diffuse fraction in the surface reflection becomes larger, so that Method B yields a larger measured value. The method therefore gives integral color differences that include differences in coloring materials together with surface gloss differences. The method is therefore not well-suited to routine pigment testing, because comparisons between pigments must be free of coating surface effects. On the other hand, in the case of durability tests, a change in gloss is to be determined by a separate gloss measurement. nonetheless, Method B can yield marked departures from visual assessment, frequently because of the heavy angular dependence of the surface reflection for semi-mat specimens of because of the gloss haze for gloss specimens. These deviations are especially ap-

6.1 Reflection and Transmission Measurement

241

parent when the 45/0 geometry is not exactly observed for visual matching of specimens with gloss haze; often, the illumination employed for matching is not directional or the angle of incidence deviates from 458. Following this discussion, it should be emphasized that similar to identical results can be obtained with these two methods only on high-gloss specimens. In all other cases, the measuring method must be selected on the basis of what information is desired: Is the difference in the interior of two specimens (difference due chiefly to pigments or dyes) wanted, or the total difference (including surface effects)? Differences in gloss will thus result in unequal color differences, not just unequal between Methods A and B but from one instrument to another (depending on the accuracy of the measuring geometry in the instruments). Special problems in colorimetry arise when coloring materials must be examined in media whose surfaces are not smooth or homogeneous but display more-orless regular textures and variable degrees of gloss. Again, Method A or B can be Table 6-1. Criteria for selection of measurement geometry given the type of sample and the measurement objective I

Bulk properties of sample

Suitable measurement geometries

1

Isotropically scattering, covering (covering lacquer, plastic)

d/8, 45/0

2

Anisotropically scattering

Goniospectrometer (45/0 and d/8; reliability of test is limited)

3

Transparent (sheet materials, films)

d/8 or d/0 in transmission; d/8 or 45/0 or goniospectrometer if applied on scattering substrate

4

Slightly scattering (sheet materials, blow-molded products)

Errors due to edge losses with thick samples; smaller measuring spot and larger illuminated spot recommended, or sample can be placed in the sphere, d/8, 45/0. For transmission measurements, d/8 or d/0. It is necessary to state clearly whether total transmission or directional transmission is at issue and to agree on method.

5

Inhomogeneous, cloudy, spotted

d/8, 45/0; large measurement port and multiple measurements. For constraints see I, 1 to I, 3.

6

Fluorescing

Use CIE standard illuminant D65; 45/0 or (if applicable) d/8.

7

Thermochromic

Monochromatic illumination, d/8, 45/0. Use flash illumination or, if using continuous illumination, wait for temperature equilibrium. For constraints see I, 1 to I, 3.

8

Phototropic

Monochromatic illumination, d/8, 45/0. For constraints see I, 1 to I, 3.

9

Slightly reflective

Polychromatic illumination, 45/0 (d/8 with gloss trap if applied behind glass and measured through glass). Computational removal of gloss contribution from surface reflection is problematic.

242

6 Measurement and Evaluation of Object Colors

Table 6-1. (continued) II Surface characteristics

Suitable measurement geometries Measurement objective: overall assessment (final inspection)

Measurement objective: bulk assessment of sample (inspection of coloring matter)

1

Glossy and smooth (lacquer)

d/8 with computational removal of surface reflection; 45/0

d/8 with computational removal of surface reflection; 45/0

2

Ideally matte

d/8, d/0, 45/0

d/8, d/0, 45/0 with computational removal of surface reflection

3

Matte, silkily reflective, textured (embossing sheets)

All instruments if surface d/8 with computational removal is identical; otherwise, go- of surface reflection only with niospectrometer or, if jus- closed surfaces (lacquers, etc.) tified, 45/0

4

With gloss haze

45/0

45/0 or d/8 with computational removal of surface reflection

5

After chalking

45/0, geniospectrometer

d/8 after polishing or lacquer application; computational removal of surface reflection

employed, but the 08 geometries should be preferred so that the azimuthal dependence will be minimized in the measurement. It is desirable to use circularly symmetrical irradiation, for example circular/0 or d/0 (see Table 6-1). Agreements between the interested parties must always take account of the following points: ± Whenever possible, the same model of instrument should be used, but in any case the same measuring geometry. If possible, a check should be made in order to verify that the selected geometry yields color coordinates that are compatible with visual evaluation. ± An attempt should be made to create color reference standards whose surfaces match as closely as possible the surfaces of the color specimens to be tested. ± Acceptability can be determined only on the basis of color sample collections that have been visually evaluated by experienced colorists. The collection of color samples must be large enough that measurements lead to statistically reliable limits on the acceptable color differences (see Section 6.5).

6.2 Practical Evaluation of Color Differences

6.2

243

Practical Evaluation of Color Differences

6.2.1 Preparation of Specimens Preparation of the dispersion must be preceded by proper sampling. This is done with a suitable sampling device such as a scoop or thief for solids and appropriate equipment for liquids of high and low viscosity*. Good dispersion is essential for testing pigments in vehicles. Various standards** afford guidance in the selection of test media and dispersing methods. The standards describe media and techniques suitable for testing the dispersion properties of pigments, but these are also valid for colorimetric testing. There are problems in the testing of pigments in latex vehicles, because reproducible measurements are virtually impossible in these media. If such tests are unavoidable, special care must be taken in the choice of vehicle and the preparation of specimens. A second group of standards covers the testing of pigments in plastics. These include a detailed description of how to prepare basic mixtures and specimens. In solvent-based systems containing more than one pigment (and frequently also in full-shade systems), flocculation can give rise to color changes (ªrub-out effectº), especially when mechanical force is employed during application and drying. This behavior can be utilized to indicate a tendency to unwanted flocculation in the Rub-out test: Apply liquid system to cardboard or sheet metal; after stated time under exhaust hood, rub part of surface with a finger until the color difference between rubbed and unrubbed surfaces has reached largest possible value and remains constant, as indicated by resistance to rubbing. From color measurements on rubbed and unrubbed surfaces, determine color difference*** (see Section 6.2.3). In the remainder of Part II, specimen preparation techniques used with a number of test methods are described in more detail.

6.2.2 Color Measuring All color measurements start with the reflection values for the color sample. In principle, any instrument used for color measurement includes the following main components: ± Illumination device ± Monochromator (or wide-band filter) * For standards see ªSamplingº in Appendix 1. ** See ªEase of Dispersionº in Appendix 1. *** See ªColor Differencesº in Appendix 1.

244

6 Measurement and Evaluation of Object Colors

± Sample holder ± Radiation-measuring device A common arrangement has the monochromator and sample holder interchangeable to give two distinct configurations (Fig. 6-9). In the chain lamp-specimenchromator-detector, the specimen is irradiated with polychromatic light; in the other case, irradiation is monochromatic. The light source may be a halogen lamp, a xenon arc lamp, or a xenon flash lamp. Heating of the specimen and resulting changes of color coordinates must be anticipated with the xenon arc lamp.

Fig. 6-9. Paths followed by light in colorimeters with (1) monochromatic and (2) polychromatic irradiation.

The instrument is calibrated with a black standard (hollow light trap) for the zero and a BaSO4 white standard* (see Section 2.1.2). For practical tests, working standards calibrated to BaSO4 (secondary standard) are usually employed as white standards for the ideal matte white surface. In Chapter 2, it was shown that color measurement can be reduced to determining x, y, and Y; this means, according to the equations presented there, the measurement of the CIE tristimulus values* X, Y, Z. The product R 7 S or R 7 S for reflection measurements, resp. t 7 S or T 7 S for transmission measurements, must be multi y, z (see Table 7-4) in order to obtain plied by the CIE color matching functions x, the three curves shown in the last row of Figure 6-10; X, Y, and Z are given by the areas under these curves. The areas, in turn, are equal to the integrals in equation (2.3), and because these admit of two different interpretations, there are two distinct types of measuring instruments: ± Tristimulus method (tristimulus colorimeters) The transmission curves of optical filters together with the lamp spectrum and etc., so that the measured intensithe detector sensitivity correspond to the S 7 x, ties yield the CIE tristimulus values after a simple calculation * See ªColorimetryº in Appendix 1.

245

6.2 Practical Evaluation of Color Differences

Fig. 6-10. Schematic representation of color measurement.

± Spectral method (spectrophotometers) The reflection curve is measured with a spectrograph. Built-in analog computers S 7 y, S 7 z, then inor internal or external digital computers multiply by the S 7 x, tegrate. Both types are used in colorimetry; the manufacturers have developed photometers, and recent years have seen improvements in them. A tristimulus colorimeter has, instead of the monochromator, three wide-band filters whose transmission curves combine with the source spectrum and the photometer characteristic to give the reflectometer values** R'x, R'y, R'z . The CIE tristimulus values are obtained directly from these values as R0 R0 X=Xn 0:798 x 0:202 z 100 100 0 Y Ry Z=Zn R0z =100

(6.1)

where Xn and Zn are the CIE tristimulus values of the CIE standard illuminant. (Because x has two maxima, X is made up of R'x and R'z ). In spectrophotometers, the monochromator uses optics (entrance and exit slits, prisms, interference filters, optical gratings) to split up the visible spectrum into bands 10±20 nm wide. Gratings and filters have completely displaced prisms in modern instruments, because of their higher transparency, constancy of optical dispersion, and lower manufacturing cost. Interference filters take two distinct forms: a single filter with fixed wavelength and a graded filter continuously traversing the ** According to the standards, reflectometer values are symbolized by R' (to distinguish them from reflection factors R); see ¹Photometric Properties of Materialsª in Apendix 1.

246

6 Measurement and Evaluation of Object Colors

spectrum. The bell-shaped transmission curves of interference filters, however, exhibit relatively large half-value widths (ca. 20 nm), so that deviations relative to gratings can occur in spectra having steep slopes. The sample holder is matched to the desired geometry, usually 0/d, 8/d, or 45/0. The light-measuring device, finally, can be either a photomultiplier (for low irradiation intensities) or a silicon cell (for higher intensities). Silicon elements process the input signals in quasi-parallel fashion, so that instruments so equipped can offer measuring cycles shorter than 3 s. In the past ± usually on grounds of cost and short cycle times ± tristimulus instruments dominated in the fields of production control and other applications as well. The situation has been changing since new technologies have made it possible Table 6-2. Sample computation based on color measurement. (Figures in italics represent handwritten entries.) CIE color notation a) Spectral method Wave- Refleclength tance

Pigment: test

b) Tristimulus method

CIE color matching functions

Reflectometer values (C/28)

l (nm)

R (l)

x C/2 (l)

R 7 x

y C/2 (l)

R 7 y

zC/2 (l)

R 7 z

400 420 440 460 480 500 520 540 560 580 600 620 640 660 680 700

0.0126 0.0125 0.0119 0.0119 0.0122 0.0125 0.0137 0.0176 0.0357 0.0967 0.1726 0.2072 0.2226 0.2403 0.2675 0.3010

0.044 2.926 7.680 6.633 2.345 0.069 1.193 5.588 11.751 16.801 17.896 14.031 7.437 2.728 0.749 0.175

0.0006 0.0366 0.0914 0.0789 0.0286 0.0009 0.0163 0.0983 0.4195 1.6247 3.0888 2.9072 1.6555 0.6555 0.2004 0.0527

0 0.085 0.513 1.383 3.210 6.884 12.882 18.268 19.606 15.989 10.684 6.264 2.897 1.003 0.271 0.063

0 0.0011 0.0061 0.0165 0.0392 0.0861 0.1765 0.3215 0.6999 1.5461 1.8441 1.2979 0.6449 0.2410 0.0725 0.0190

0.187 14.064 38.643 38.087 19.464 5.725 1.450 0.365 0.074 0.026 0.012 0.003 0 0 0 0

0.0024 0.1758 0.4599 0.4532 0.2375 0.0716 0.0199 0.0064 0.0026 0.0025 0.0021 0.0006 0 0 0 0

P CIE tristimulus values CIE chromaticity coordinates

:

10.96

7.01

1.44

F X

F Y

F Z

F x

X X Y Z 0.5649

y F

Y X Y Z 0.3613

R'x = 13.71 R'y = 7.01 R'z = 1.22

F X =0.7827R'x +0.1987R'x 10.721 + 0.242 = 10.96

F Y = R'y 7.01

F Z = 1.182 7 R'z 1.44 CIE tristimulus values

6.2 Practical Evaluation of Color Differences

247

Table 6-3. Sample computation of color differences. (Figures in italics represent handwritten entries.) CIELAB color coordinates p X 3 X=98:07

Pigment: test

0.4817

L = 116 7 Y ± 16

31.83

Y

p 3 Y=100

0.4123

a = 500 7 (X ± Y )

34.70

Z

p 3 Z=118:22

0.2296

b = 200 7 (Y ± Z )

36.54

Note: If radicand r ^0.008856 then: X = 7.787 7 r + 0.138 (similarly for Y and Z ) CIELAB color differences Reference (R):

Test (T):

D = T± R

L

30.71

31.38

DL

1.12

a

35.45

34.70

Da

± 0.75

b

35.62

36.54 p a2 b2

Db

0.92

DCab

0.14

Chroma difference

1.63

Color difference

C ab C ab

50.25

50.39

p DL2 Da2 Db2 q 2 2 jDHab j DEab DL2 DCab DE ab

aR bT

aT bR

DHab Sign jDHab j

1.18 +59.33 +1.18

Lightness difference

) Sign(60) = +1 + Sign ( < 0) = ±1 Hue difference

to build fast spectral instruments at competitive prices. Another factor here is that tristimulus photometers cannot tell metameric color samples apart, because these instruments do not recognize metamerism. After color measurements have been performed on the test and reference specimens, the X, Y, Z are transformed into the CIELAB system so that the color differences can be calculated for the full-shade determination. Practical (manual, so to speak) evaluations of colorimetric data for both tristimulus and spectral methods are illustrated in Tables 6-2 and 6-3. The values of the CIE

248

6 Measurement and Evaluation of Object Colors

color matching functions used here, are those from Stearns' 20 nm table* (see Chapter 3). The example shows very clearly the burden of computation that used to be necessary and has now been taken off the colorimetrist's back by the computer age.

6.2.3 Full Shade A standardized test of dry pigment powder is possible for white pigments**. In the procedure, the CIE tristimulus value Y can be determined as a way of characterizing the lightness of white pigment and filler powders in pressed form. A suitable powder press has to be used to prepare the tablets. The measured Y value depends on a number of factors (rate of pressing, degree of compaction, surface texture, etc.), so that specimen preparation conditions must be clearly agreed on. Naturally, the CIE tristimulus value Yof the powder has no power to indicate the lightness of the pigment in media; it is suitable ± at most ± as a supplementary receiving inspection method for pigments. Thus the colorimetric values obtained on such tablets are not in any way typical, for the color of colored, white, and black pigments must be evaluated in suitable media (binders, vehicles). This means that final paint and lacquer coatings as well as plastics can be evaluated by the methods. Full-shade testing is described in separate standards*** for black, white, and colored pigments. These also define the terms ªfull shadeº and ªmass toneº, which were formerly used inconsistently. A full-shade system is a pigment/vehicle dispersion with a single pigment, and the color of such a system in a optically hiding layer is called the full shade. In contrast, the mass tone is a full-shade system in a non-hiding layer. Thus no mass tone is unambiguously defined unless information is provided on the preparation, composition, application, and substrate; many mass tones can be made with the same fullshade system, differing in film thickness and substrate properties. A special role in pigment testing is played by the test media**** used, first because of their actual effect and second because the use of suitable media makes it possible not only to avoid certain problems (inadequate dispersion, flocculation, etc.; see Section 4.1.2) but also to achieve certain economies. Chief among the latter are time savings in the testing procedure; one time-saving step is the use of nondrying pastes as vehicles. In addition to the time saving, the measured values also gain in significance, because full-shade measurements on pigmented pastes exhibit much smaller preparation errors than those on dried vehicles. Other proposals for test systems and their preparation can be found in Section 6.2.1. A good vehicle for nondrying pastes (DIN 55983) is an alkyd resin, Alkydal L 64 (Bayer AG). This binder combines the advantages of easy dispersion with the suppression of any tendency for the pigment to flocculate. * ** *** ****

See ªColor matching functions in steps of 20 nmº in Appendix 1. See ªLightnessº and ªReflection Factorº in Appendix 1. See ªColor in Full-Shade Systemsº in Appendix 1. See ªCoating materialsº in Appendix 1.

6.2 Practical Evaluation of Color Differences

249

Preparation method: Mix 97 % by weight Alkydal with 3 % by weight Aerosil 200 (Degussa), taking steps to prevent dust losses. Pass the mixture through a triple-roll mill twice. Weigh out 3 g of this mixture and a quantity of pigment such as to give a PVC of 10±20 %. Put the Aerosil paste in the middle of the lower plate of an automatic muller, scatter the pigment on the test medium; work together with a spatula without applying pressure. Next, distribute the paste in dots or a circle about 35 mm away from the center of the lower plate. A useful marking technique is to place beneath the lower glass plate a ring-shaped paper pattern with an inside diameter of 40 mm and an outside diameter of ca. 100 mm. Add a 25 kg weight to the upper plate. Wipe as much as possible of the paste from the spatula onto the upper plate. Mull the paste in two stages of 25 revolutions each. Transfer the finished pigmented paste to a special paste film holder made of metal or polyamide (see Fig. 6-11) and draw down with the doctor blade included. Among drying systems (DIN 55 983), air-drying systems are preferred to stove-drying ones because the preparation errors are smaller in the first case. Espectially

Fig. 6-11. Paste film holder with doctor blade, corresponding to DIN 55 983 (dimensions in mm).

250

6 Measurement and Evaluation of Object Colors

good choices are Alkydal F 48 (Bayer AG) and URALAC 6008 (Scado GmbH), both in 50 % solution. URALAC does not require and additional dryer and dries in 1±2 h (see also DIN 53 238 Part 30); Alkydal has to have a dryer added. Preparation method: Weigh out 5 g of the test medium and the quantity of pigment to give a PVC of 10±20 %. Using an automatic muller, proceed as before. Apply hiding coats of the finished reference and test pigment mixtures to a suitable substrate (glass plate, metal sheet, contrast card, lacquered or aluminiumlined cardboard), employing the same procedure in each case; the use of a Bird applicator is desirable. Coatings are hiding if a coating applied on a black/white contrast substrate exhibits a color difference DE ab after drying. Measurement method: Using a suitable colorimeter, measure test and reference preparations in such a way that the measurement conditions for Method A (i. e., use of integrating sphere with no gloss trap, correction by subtracting surface reflection; see Section 6.1.2 are fulfilled. Depending on the configuration of the measuring apparatus, either the reflectance R or the reflection factor R is obtained (in tristimulus instruments, the reflectometer values R'x , R'y, R'z are obtained). The corrections for surface reflection must be subtracted from each such quantity. Evaluation is done with the CIELAB formulas, equations (2.5) to (2.14). Figure 6-12 shows a computer printout illustrating the calculations for a fullshade measurement on yellow iron oxide pigments. Special aspects in the evaluation for white pigments have already been discussed (Section 2.3.3). In this instance, it is preferable to state as the color designation the Program ªFULL SHADE COLOREDº Full shade of colored pigments, according to ISO 787-25 *************** Date: ..-..-.. Pigment: Iron oxide yellow Reference is A Test is B Binder: Alkydal L 64 PVC: 20 % Colorimeter, Standard observer: N.N., C/28 Measuring conditions: d/8 (incl.) Input: ******************************************************** R'(x) R'(y) R'(z) Reference 17.00 10.57 4.95 Test 15.96 10.39 5.26 Output:******************************************************* a* b* L* C*(ab) h(ab) Reference 34.6 38.3 30.8 51.7 47.98 Test 30.6 33.4 30.4 45.3 47.58 Color differences Delta Delta E*(ab) a* 6.4 ±4.0

Delta b* ±4.9

Delta L* ±.4

Delta C*(ab) ±6.3

Delta H*(ab) ±.3

Delta h(ab) ±.48

Fig. 6-12. Full shade, colored, yellow iron oxide (computer output).

6.2 Practical Evaluation of Color Differences

251

ªhue of near-white specimensº* and its strength Ds (eq. 2.15). Figure 6-13 presents an example for titanium dioxide pigments. Similar considerations apply for black pigments and gray coatings: The recommended statement of the result is ªhue of near-black (or gray) specimensº instead of color differences (Section 2.3.3). Another special point is the more stringent requirements on the colorimeter for the full-shade measurement of black pigments. These conditions, which are met by few instruments today, relate to the display (five decimal places for reflection measurements, three for CIE tristimulus values), zero adjustment (calibration with a hollow light trap as special black standard), and reproducibility (standard deviation of CIE tristimulus values less than 0.001). An example, based on a full-shade measurement of black iron oxide pigments, appears in Figure 6-14. Program ªFULL SHADE WHITEº Full shade of white pigments, according to ISO 787-25 **************** Relative hue of near white specimens ****************************** Date: ..-..-.. Pigment: Titanium dioxide Reference is A Test is B Binder: Alkydal L 64 PVC: 20 % Colorimeter, Standard observer: N.N., C/28 Measuring Conditions: d/8 (incl.) Input: ******************************************************* R'(x) R'(y) R'(z) Reference 94.52 93.91 91.48 Test 94.54 94.18 92.55 Output: ****************************************************** Color difference Hue Delta (E*(ab)) Delta (L*) Type Magnitude Delta (s) .6 .1 blue .6 Fig. 6-13. Full shade, white (relative hue of near-white specimens), titanium dioxide (computer output). Program ªFULL SHADE BLACKº Full shade of black pigments, according to ISO 787-25 *************** Relative hue of near black specimens Date: ..-..-.. Pigment: Iron oxide black Reference is A Test is B Binder: Alkydal L 64 PVC: 20 % Colorimeter, Standard observer: N.N., C/28 Measuring Conditions: d/8 (excl.) Input: ****************************************************** R'(x) R'(y) R'(z) Reference .491 .442 .471 Test .369 .348 .429 Output:***************************************************** Color difference Hue Delta (E*(ab)) Delta (L*) Type Magnitude Delta (s) 1.3 ±.8 blue green .9 Fig. 6-14. Full shade, black, black iron oxide (computer output). * See ªHue of Near-White Specimensº in Appendix 1.

252

6 Measurement and Evaluation of Object Colors

The full-shade determination of dyes in solution is accomplished with colorimeters capable of transmission measurements. The CIELAB evaluation is similar to that for nonluminous perceived colors. Determinations of CIELAB color differences are described, as secondary procedures, in a number of other standards, for example under methods for determining the thermostability of plastics*.

6.2.4 Special Problems Metamerism (see Section 2.2.2) is commonly of secondary significance for pigment testing, though in practice it is much more important and can therefore become a factor in special testing situations. In formulation (as also in the pigmenting of lacquers and paints), one often cannot simulate the reflection spectrum of a given color, because (among other reasons) to do so would require having an unlimited number of pigments on hand. Instead, one has to be satisfied with reproducing the three CIE tristimulus values, even though this means that the new color will match only for the precise illuminant used. Such ªmetamericallyº matched colors will therefore show differences between the ªdaylightº color (under CIE standard illuminant C or D65) and the ªincandescent light colorº (under CIE standard illuminant A). In order to describe how much the color equality of two objects under a certain illuminant changes on a change of illuminant, the metamerism index** is employed. The color difference between the originally matching colors under the new illuminant is expressed in the perceptually-based CIELAB system. Figure 6-15 shows reflectance curves for two metameric specimens.

Fig. 6-15. Spectral reflectance for two yellow specimens having the same appearance in CIE standard illuminant D65 for the 108 observer. * See ªPVCº, and ªThermosplasticsº in Appendix 1. ** See ªMetamerism Indexº in Appendix 1.

6.2 Practical Evaluation of Color Differences

253

Even more important in pigment testing is the variety of metamerism called ªgeometricº. While normal metamerism involves a change in color when the illuminant is changed, in geometric metamerism a color change is brought about when the irradiation or viewing geometry relative to the specimen is altered. A special form of geometric metamerism is encountered in the Silking effect, where the reflectance changes when the specimen is rotated about the surface normal. Several conditions must hold for the Silking effect to occur. The first condition is a anisometric pigment, one made up of acicular, bladed, or rod-shaped particles, whose scattering and absorption coefficients are different in the principal axis direction and perpendicular to this axis. What is more, the pigmented medium must be applied in such a way that the particles are oriented, that is, in a quasi-parallel arrangement. The Silking effect can be measured only in geometries involving directional fluxes (e. g., 45/0). In practice, the Silking effect can be rather a problem, for example producing the ªpicture-frame effectº when a painting job has been finished up by painting once more around the edge of a large area in order to equalize the coat. Thermochromism is the property of coloring materials that show changes in reflection with changes in temperature. When performing colorimetric measurements on thermochromic specimens, it is necessary to wait for temperature equalization or, better, to use an irradiation source that does not heat up the specimen (monochromatic source or flash lamps). The following method is a suitable way of testing for the effect: Measure specimen a number of times in succession without removing it from the measuring port. Determine color differences relative to first measurement and note the time up to which differences remain constant. It should be noted that thermochromism can also be pretended by a change in the moisture content of the specimen. Fluorescence occurs when absorbed radiation is reflected after a very short time (ca. 10±6 s) in the longer-wavelength visible. If the reflection is delayed for a longer time, the behavior is called phosphorescence. Both these phenomena come under the general heading of luminescence. Fluorescent coloring materials can be used in molecularly dissolved form or as fluorescent pigments. Often, fluorescent coloring materials in low concentrations are added to paints or inks to enhance their brilliance (ªoptical brightenersº); the attenuated fluorescence is not perceived as luminosity but as greater brightness or saturation. The exciting radiation can lie in a more-or-less wide range of wavelengths, between 350 and 550 nm, depending on the chemical nature of the colorant; similarly, the fluorescent radiation is generally not monochromatic. Media and coatings that contain fluorescent coloring materials are, in fact, self-luminous, at least to the degree that the reflection is caused by them. Nonetheless, they are treated as nonluminous perceived colors, that is, referred to a mat white surface, so that reflectances R 4 1 can occur. Fluorescent object colors also differ from ordinary nonluminous perceived colors in that the reflectance and color stimulus depend

254

6 Measurement and Evaluation of Object Colors

on whether the incident light contains sufficient exciting radiation. For this reason, fluorescent specimens must be irradiated with the illuminant to which the measured values will be referred, that is, under which they will be visually matched. The content of fluorescent radiation is proportional to the intensity of the exciting radiation, and so if the incident radiation is deficient in the exciting range then there will be little fluorescent light; as a consequence, the measured color will no longer match with the visual results. This means that specimens must not be monochromatically irradiated for the spectral method; hence the only candidate configuration is number 2 in Figure 6-9. Figure 6-16 presents curves for a ªrightº and a ªwrongº measurement; the absorptions can be seen clearly in the ªrightº curve.

Fig. 6-16. Spectral reflectance for a fluorescent red color, measured in a ªwrongº configuration (number 1 in Figure 6-9) and a ªrightº one (number 2 in Figure 6-9).

Furthermore, mirrors and lenses in the instrument, and particularly the integrating sphere, will more-or-less strongly alter the spectral makeup of the incident radiation and, as implied by the discussion just presented, can again lead to changes in the color loci. It is therefore recommended that Method B of Section 6.1.2 be employed for these measurements, but only in the 45/0 geometry. Lamps with a daylight-like spectrum can be used to irradiate the specimen, because daylight contains sufficient radiation in the ultraviolet near 400 nm. This is why high-pressure xenon lamps or xenon flash tubes are used in instruments. CIE standard illuminant C is not appropriate because it is deficient in this radiation; at present, illuminant D65 lacks a technical implementation that can be used for routine measurements. Metal-effect paints, also called simply ªmetallicsº, are made with metal-effect pigments (Section 1.2). Their color properties are governed mainly by specular reflection on blade-shaped pigment particles, which are relatively large in diameter (up to 20 mm) and are predominantly oriented parallel to the paint surface. The fundamental physical processes of absorption and scattering observed on pigmented coatings are here joined by specular reflection. The interplay and interaction of these three processes give rise to the attractive aspect of a metal-effect paint. The directional distribution of the returned radiation depends heavily on the irradiation

6.3 Test Errors

255

angle and the viewing angle, so that significant and abrupt changes of lightness and hue can occur (lightness flop, hue flop). There are major difficulties associated with unsolved problems in color measurement on metallics. To determine the overall behavior, goniometric methods would have to be applied on both the irradiation and viewing sides of the system; this would lead to a multitude of plotted curves or measured values. Rationalization will not be possible until the colorimetric characterization of such paints can be acomplished with a limited number of angle settings, but no theoretical general approach has yet been devised to this problem. The situation is not much better with regard to instruments, plainly because of the lack of theoretical initiatives. One goniometric instrument that used to be available has now disappeared from the market, and devices that can be set to at least certain predetermined angles are slow in coming out. The present state of the art comprises instruments with conventional features, but these permit only the study of special aspects. Given these circumstances, for example, the only way to acquire new information about the conditions for hue and lightness flop is to analyze the scattered and reflected components separately to whatever extent this is possible. Problems with nacreous pigments stem from the need to measure interference colors. This again involves an angle-dependent indicatrix, so that conventional colorimeters fall down. Only the beginnings of a approach to measurement exist now; development into routine lab methods will have to wait. Generally accepted techniques for measurements on metal-effect and nacreous pigments are not yet in prospect. The methods gap is due to a lack of both theory and apparatus. Unfortunately, there is an intimate interaction between theory and hardware. This example shows that even colorimetric problems cannot be solved until the right instrument is available.

6.3

Test Errors

6.3.1 Calculation of the Standard Deviation Ellipsoid A number of computer programs are needed for the calculations demonstrated in Section 2.4. These can be classified into four groups: ± ± ± ±

Calculation of the coefficients of the ellipsoid Visualization of the resulting ellipsoid Calculation of test errors and significance Calculation of acceptability

It is desirable to program these calculations for a suitable computer. The calculation of ellipsoid coefficients is preceded by measurements performed in a ªreproducibility seriesº of a least 20 color samples. This term refers to

256

6 Measurement and Evaluation of Object Colors

a series of preparations made in the same way with the same pigments. The program takes the CIELAB coordinates (two decimal places) as input and calculates the means and the standard deviation ellipsoid. First, the arithmetic means of the color coordinates a , b , and L are calculated. By substituting these means into the successive formulas, it calculates the barred values of the polar coordinates C ab and hab (to two decimal places) with equations (2.8) and (2.9).

Program ªSTANDARD DEV. ELL.º Standard deviation ellipsoid, according to DIN 55600 ********************** Date: ..-..-.. Pigment: Chromium oxide green Binder: Alkydal F 48 PVC: 10 % Dispersing equipment: Automatic Muller, 2*100 Rev. Colorimeter (Measuring conditions, Standard observer): N.N., d/88, C/28 Input: ************************************************************ Pigment is A No. a* b* L* 1 ±19.09 16.08 45.48 2 ±19.10 16.12 45.37 3 ±19.10 16.01 45.39 4 ±19.09 16.10 45.36 5 ±19.02 16.06 45.36 6 ±19.06 16.12 45.47 7 ±19.12 16.16 45.36 8 ±19.11 16.06 45.41 9 ±19.10 16.09 45.47 10 ±19.15 16.10 45.43 11 ±19.08 16.15 45.43 12 ±19.08 16.03 45.46 13 ±19.13 16.20 45.36 14 ±19.09 16.07 45.46 15 ±19.09 16.14 45.40 16 ±19.13 16.16 45.46 17 ±19.11 16.12 45.47 18 ±19.14 16.17 45.44 19 ±19.10 16.12 45.37 20 ±19.14 16.11 45.39 Output:*********************************************************** Means: a*= ±19.10 b*=16.11 L*= 45.42 C*(ab) = 24.99 h(ab) = 139.858 Ellipsoid (70 %): g(1,1) = 424.7 g(2,2) = 152.3 g(3,3) = 139.5 g(1,2) = 137.5 g(2,3) = 21.64 g(1,3) = 22.62 Fig. 6-17. Means and calculated standard deviation ellipsoid for 20 preparations of a chromium oxide pigment (computer output).

6.3 Test Errors

257

Next, the variances and covariances are calculated (equations 2.78 and 2.79) and arrayed to form the covariance matrix V (equation 2.80). The program now inverts the matrix (equation 2.81) to get G. Appropriate software is often available for matrix inversion on the computer; an individual sample calculation is presented here. The formula is gik = u^ ik =det V, where det V denotes the determinant of matrix V, u^ ik is the cofactor of element uik, obtained from matrix V by deleting the i-th row and the k-th column and taking the determinant of the matrix that remains, with the sign (±1)i+k. The program requests the desired probability, divides the coefficients by the appropriate significance level ds2cum (Table 2-4), and rounds the gik to four significant figures. It outputs the means and the coefficients of the standard deviation ellipsoid for the desired probability. The programming is not very complicated and can well be done on a mediumsized desktop computer. Figure 6-17 presents a typical printout. With the aid of such a program, the CIELAB coordinates for 20 preparations of a chromium oxide pigment have been transformed to the means and the coefficients gik of the standard deviation ellipsoid for a 70 % confidence interval. A (very detailed) sample computation is contained in DIN 55600-2. In this instance, the 70 % confidence interval means that 70 % of all measured values lie inside the ellipsoid, or that there is a 70 % probability of an individual measurement lying in the interior (see also Section 2.4.1).

6.3.2 Visualization of the Ellipsoid It has proved useful in practice to visualize the ellipsoid in the CIELAB color space. When comparing two series of color measurements, it is often not enough to state just the standard deviations associated with the measurements; detailed conclusions about a measurement or preparation method can be arrived at only when the location and orientation of the error ellipsoid in color space are accessible for comparison. Two programs are needed for this purpose: ± Calculation of principal axes ± Projection of the ellipsoid onto the principal planes of the CIELAB color space (plot program) For the calculation of principal axes, the gik of the ellipsoid become the inputs. The program first verifies that the coefficients do pertain to a ellipsoid (and not to a different second-order surface); this is done with equation (2.47). If the result is affirmative, the secular equation (2.51) is then solved, for example by the trigonometric method. From its roots la, lb, lc, the three principal axes of the ellipsoid are then obtained as vectors a, b, c, each expressed in terms of its Cartesian coordinates a , b , L (equations 2.45±2.48) and its three-dimensional polar coordinates r, j, W (equation 2.49). An example in the form of a computer printout is given in Figure 6-18. The calculation relates to the total error ellipsoid, which will be described more fully in

258

6 Measurement and Evaluation of Object Colors

Section 6.3.3. The three principal axes are expressed as vectors a, b, c, each with its components. Listed next are the three-dimensional polar coordinates (one length plus polar angles; see Fig. 2-14). A quick comparison of the lengths of the three principal axes shows that one is very long ( | a | = 0.1606) and two are shorter. One of the short axes ( | b | = 0.0762) is roughly 3.5 times as long as the other ( | c | = 0.02 133). The ellipsoid is thus shaped like a surfboard or a somewhat flattened cigar with an elliptical cross section; the long axis of the cigar is some eight times as long as the short axis and twice as long as the longer axis of the cross-sectional ellipse. The polar angles give the spatial orientation of the figure: The long axis (a) lies in the positive quadrant (a and b positive, j positive) of the color plane and also in the positive octant of the CIELAB color space (L and W also positive). It is nearer to be b axis than to the a axis of the three-dimensional coordinate system (j = 74.18 closer to 908 than to 08), and also somewhat nearer to the color plane than to the L axis of the coordinate system (W = 66.18 closer to 908 than to 08). Program ªSEMIAXESº Ellipsoid semiaxes, according to VÚLZ, Industrial Color Testing ********* Input: Ellipsoid coefficients*************************************** g(1,1) = 228,5 g(2,2) = 345,9 g(3,3) = 1835 g(1,2) = 104,7 g(2,3) = ±730 g(1,3) = ±344,1 Output: Semiaxes *********************************************** Vector a* b* L* Långe Phi Theta a b c

.0402 .0725 ±.00382

.1412 ±.02294 ±.00788

.0652 .00493 .01945

.1606 .0762 .02133

74.108 ±17.558 ± 115.838

66.088 86.298 24.258

Fig. 6-18. Calculation of principal axes of a total error ellipsoid (computer output).

Next we come to the plot program for the ellipsoid projections. After the gik are input, the coefficients of the three projected ellipses (in the a, b, a, L, and b, L planes, equation 2.60) are calculated along with the axes (equation 2.61) and the paired section lines (equation 2.65), and these results are output by the plotter*. Figure 6-19 presents an example, a plot of the total error ellipsoid from Section 6.3.3 and Figure 6-18. With some practice, one can gain an idea of the position and orientation in three-dimensional color space by examining the plot. Fig. 6-19 (left-hand side) shows the three projections, i. e. a vertical and two horizontal projections; these are superimposed to simplify the display (Fig. 6-19, right-hand side). The outermost points of the projections are connected in pairs by section lines (dotted). If a color plotter is available, each of the three projections can be drawn in a different color. * In all plots, the horizontal axis is named first and the vertical axis second; thus the phrase ªa*,b* planeº denotes the plane with coordinates a* (abscissa) and b* (ordinate).

6.3 Test Errors

259

Fig. 6-19. Total error ellipsoid represented by projections in the principal planes of the CIELAB color space (from 20 preparations).

As has already been shown, the ellipsoid represented here has the shape of a flattened cigar. The projections bear out the description just obtained: The b, L projection clearly shows the lengthwise orientation, and it together with the two others shows the flattening of the figure. It should be noted that the ellipse axes drawn are not identical with the principal axes of the ellipsoid but are merely their projections. In order to get a still better idea of the three-dimensional shape of the figure, the ellipsoid can also be represented in its own principal-axis system. As equation (2.53) suggests, the three axis lengths, in the form of their reciprocal squares, are simply substituted in equation (2.52) and g12, g23, and g13 are simultaneously set equal to zero. The plot for the total error ellipsoid transformed in this way is illustrated in Figure 6-20. It confirms what has been said about the shape of the figure.

6.3.3 Total Error and Its Components The total error of a colorimetric pigment test is made up of the error of preparation and the error of measurement. Because the error of measurement is commonly very small, preparation methods are crucial for the size and location of the total error ellipsoid. If the preparation error is too large, an attempt must be made to split it into several contributions so that error sources can be identified and eliminated.

260

6 Measurement and Evaluation of Object Colors

Fig. 6-20. Total error ellipsoid of Figure 6-19, each projection into its own principal-axis plane.

In the example under discussion, the color dispersions for the measurement of the total error are prepared by the paste method of Section 6.2.2. The measurement of the tristimulus reflectometer values R'x , R'y, R'z was carried out by Method A of Section 6.1.2 (88/d) as follows: Measure R'x , R'y, R'z on one preparation in quick succession. Measure the next preparation after about 2 min, and so forth. After every five preparations, measure preparation No. 1 in order to recalibrate colorimeter to the values acquired on this preparation at the outset. The differences between actual and nominal values in recalibration were always less than 0.05 reflectometer units. The reproducibility series (dispersions of a pigment) used to define the total error ellipsoid was independent of random variations after 20 preparations. Confirmation of this claim is obtained by comparing Figure 6-19, the ellipsoid containing all 20 preparations, with the ellipsoids based on groups of 10 from the 20 preparations (Figure 6-21 and 6-22). These total error ellipsoids were determined for pastes (binder Alkydal L 64) pigmented with a red iron oxide pigment (10 % PVC). In contrast to the total error, the error of measurement is supposed to show how much the measured values will differ when repeated measurements are done on one and the same preparation within a series; the cause of this error lies in short-term instabilities of the instrument. Place on the instrument, 20 times, exactly the same portion of a selected preparation (e. g., No. 1 of the pastes prepared for the total error ellipsoid of Figure 6-19). After each placement (at time intervals of 3 min), measure the reflectometer values R'x , R'y, R'z without recalibrating the instrument. Figure 6-23 presents an ellipsoid for the error of measurement derived in this way. It has a somewhat different appearance from the total error ellipsoid of Figure 6-19,

6.3 Test Errors

261

Fig. 6-21. Total error ellipsoid of the first 10 preparations from Figure 6-19.

Fig. 6-22. Total error ellipsoid of the last 10 preparations from Figure 6-19.

being more discus-shaped, flattened in the direction of the a , L diagonals. To reduce or eliminate the scatter of the measured values due to long-term instabilities of the instrument, the same procedure as described for the total error must be employed: Maintain a time interval of 2 min between every two measurements; recalibrate colorimeter after every five measurements. In addition, perform each of the 20 measurements for this measurement error ellipsoid in the two minute pause between every two of the 20 measurements for the total error ellipsoid. This methodology insures that the measurement error ellipsoid is contained inside the total error ellipsoid. The measurement error ellipsoid acquired in this way is shown in Figure 6-24. It is much smaller than the ellipsoid in Figure 6-23 and also differs in shape and orientation.

262

6 Measurement and Evaluation of Object Colors

Fig. 6-23. Ellipsoid of measurement error, with no recalibration of instrument (measurement interval 3 min).

Fig. 6-24. Measurement error ellipsoid contained in the total error ellipsoid of Figure 6-19. (Measurement interval 2 min, instrument recalibrated after every five measurements.)

Certain fluctuations in the values resulting from specimen preparation can be eliminated or at least reduced if they are caused by ± ± ± ± ± ±

Weighing errors Lack of constancy in dispersing Inhomogeneities due to flocculation or floating of pigments Surface defects produced when drawing down the pastes Temperature effects Moisture effects

A reduction in the preparation error can be achieved if the error components can be identified and the larger error contributions minimized through changes in the preparation process.

6.4 Significance

263

Fig. 6-25. Ellipsoid of preparation error, contained in the total error ellipsoid of Figure 6-19.

The gik values characterizing the preparation error are formed, as stated in equation (6.2), by writing the covariance matrices (total error minus measurement error) and inverting the resulting difference matrix. The relative contributions of preparation and measurement error to the total error can be determined by comparing the ellipsoids for the total error (Figure 6-19), the preparation error (Figure 6-25), and the measurement error (Figure 6-24). Note the differences in size, shape, and (in part) orientation of the ellipsoids in figures 6-24 and 6-25. The preparation error ellipsoid is nearly as large as, and also quite similar in appearance to, the total error ellipsoid of Figure 6-19 (surfboard); thus it can be said that the preparation error is the dominant constituent of the total error in this example. The preparation error can be splitted up further (eq. 2.84).

6.4

Significance

6.4.1 Calculation of Standard Deviations Now, with the equations in Section 2.4.3, there is no further difficulty in calculating standard deviations. The standard deviations of the color coordinates will be calculated on the basis of a test error ellipsoid gik associated with these standard deviations. It is advisable once again to write a program using equations (2.68) to (2.75). A printout appears in Figure 6-26; the program was tested on the reference from the color difference test with red iron oxide pigments (see below). When comparing standard deviations in order to evaluate errors, it should be kept in mind that the confidence intervals of the three dimensional normal distribution here are systematically different from the confidence intervals of the ordinary

264

6 Measurement and Evaluation of Object Colors

Program ªST. DEV. COORD.º Standard deviations of CIELAB coordinates, according to DIN 55600 Input: *************************************************** Pigment is Red iron oxide A Medium: Alkydal L 64 Dispersing: Automatic muller Colorimeter: Tristimulus Nr. 2 Means: a* = 27.02 b* = 19.76 L* = 39.40 C*(ab) = 33.47 (h(ab)) = 36.188 Ellipsoid: g(1,1) = 146.7 g(2,2) = 137.60 g(3,3) = 192.0 g(1,2) = ±50.49 g(2,3) = ±134.0 g(1,3) = ±30.52 Output: ************************************************** Sigma(a*) = .08 Sigma(b*) = .09 Sigma(L*) = .07 Sigma(C*(ab)) = .10 Sigma(h(ab)) = .188 Fig. 6-26. Standard deviations of color coordinates (computer output).

one-dimensional distribution. In the 3D case, we consider the 70 % ellipsoid, assuming the associated standard deviation equal to s, by analogy with the onedimensional case. In the 1D case, ca. 95 % of the measured values fall between twice the positive standard deviation and twice the negative standard deviation (+2s), but the situation with the 3D distribution is different: As Table 2-4 shows, replacing the 70 % with the 95 % confidence interval changes the value obtained to (7.81/3.665)1/2 s &+1.5 7 s. The other values of interest are found in a similar way; Table 6-4 offers a comparison. Table 6-4. Comparison of confidence intervals for one- and three-dimensional normal distributions. Confidence interval

1D

3 D (s = s (70 %))

70 % 90 % 95 % 99 % 99.5 % 99.9 %

+1.04 s & +s +1.64 s +1.96 s & +2 s +2.58 s +2.81 s +3.09 s & +3 s

+1 s = +s +1.31 s +1.46 s &+1.5 s +1.76 s +1.87 s +2.11 s &+2 s

The procedure for standard deviations of color differences is exactly the same. Another computer printout is given in Figure 6-27 (reference and test of a red iron oxide pigment). In the case of color differences, it is commonly not enough to state the standard deviations alone, especially when these are of the same order of magnitude as the measured values. It is important to ask whether a color difference is significant, in other words, to perform a test of significance. This will take account of the number of measurements from which the mean color differences were obtained.

6.4 Significance

265

Program ªST. DEV. DIFF.º Standard deviations of CIELAB color differences, according to DIN 55600 Input: ******************************************************* Standard is Red iron oxide A Test is Red iron oxide B Medium: Alkydal L 64 Dispersing: Automatic muller Colorimeter: Spectral Nr. 3 Means: Delta(a*) = ± .03 Delta(b*) = ±1.20 Delta(L*) = ± .71 Delta(h(ab)) = ±1.678 Delta(H*(ab)) = ± .96 Delta(C*(ab)) = ± .71 Delta(E*(ab)) = 1.39 Ellipsoid: g(1,1) = 135.7 g(2,2) = 99.50 g(3,3) = 484.7 g(1,2) = 36.37 g(2,3) = ±165.1 g(1,3) = ±190.0 Output: ***************************************************** Sigma(Delta(a*)) = .09 Sigma(Delta(b*)) = .10 Sigma(Delta(L*)) = .05 Sigma(Delta(h(ab)) = .148 Sigma(Delta(H*(ab) = .08 Sigma(Delta(C*(ab)) = .15 Sigma(Delta(E*(ab)) = .14 Fig. 6-27. Standard deviations of color differences (computer output).

6.4.2 Test of Significance In Section 6.3.3 is was shown that 20 preparations are ordinarily both necessary and sufficient for the calculation of standard deviations. The same applies to the test of significance. Once again, it is useful to write a computer program based on the information and formulas in Section 2.4.4. Such a program can be generated by combining our sample programs STANDARD DEV.ELL. for color differences (Figure 6-17) and ST.DEV.DIFF. (Figure 6-27). The procedure begins with values evaluated by the CIELAB method (Section 2.3.3), that is, test and reference are measured one right after the other. The covariances to be formed will depend on the sequence of measurements, since they are supposed to describe relationships between two distinct measured quantities. Thus the results will include not only colorimetric relationships (e. g., a and b are calculated from the same CIE tristimulus value Y, and in addition the CIE color matching functions from which the X,Y, Z and ultimately the a , b are formed may overlap considerably) but also common differences in the method of preparing the color samples as well as short-term fluctuations of the colorimeters. It is therefore necessary to leave the measurements in the order in which they were acquired, forming the differences between two successive measurements of test and reference. If, on the other hand, an earlier ellipsoid is used again for the reference and it is desired to dispense with the separate determination of the gik for the color-differ-

266

6 Measurement and Evaluation of Object Colors

ence ellipsoid, equation (2.72) can be employed again because there is no correlation between the measurements on the reference and on the test. First, as in Section 6.3.1, the means of the color measures aR ; bR ; LR ; aT ; bT ; LT ; and of the differences Da ; Db ; DL are formed. Because it is always the case that Da aT aR and so on, it is enough to obtain two of each triplet of means (of aR ; aT ; Da , etc.) by averaging, then simply use these relations to find the third. In series measurements against the same reference, the quantities aR ; bR ; LR are already in hand and all that is necessary is to form the means of the Da , Db , DL . This can be done when the covariance matrix is calculated, since the same sums are used in both cases. It should be pointed out again that only statistical fluctuations, in the sense of stochastically independent events, may enter into the variance and covariance calculation in the determination of standard deviations or significances. As a result, systematic errors, which lie outside the bounds of probability theory, must be carefully eliminated by appropriate means. Systematic errors include heating of the speProgram ªSIGNIº, Page 3 Significance of CIELAB color differences, according to DIN 55600 **** Output: Significance test*************************************** Number of measurements: n = 20 Conf. int. Color differences (abs.) Crit. value Color difference is 70 % 95 % 99 %

Delta(a*) Delta(a*) Delta(a*)

= .03 = .03 = .03

> .02 ^.03 ^.03

significant non-signif. non-signif.

70 % 95 % 99 %

Delta(b*) Delta(b*) Delta(b*)

= 1.20 = 1.20 = 1.20

> .02 > .03 > .04

significant significant significant

70 % 95 % 99 %

Delta(L*) Delta(L*) Delta(L*)

= .71 = .71 = .71

> .01 > .01 > .02

significant significant significant

70 % 95 % 99 %

Delta(C*(ab)) = .71 Delta(C*(ab)) = .71 Delta(C*(ab)) = .71

> .03 > .05 > .06

significant significant significant

70 % 95 % 99 %

Delta(h(ab)) = 1.678 Delta(h(ab)) = 1.678 Delta(h(ab)) = 1.678

> .038 > .058 > .068

significant significant significant

70 % 95 % 99 %

Delta(H*(ab)) = .96 Delta(H*(ab)) = .96 Delta(H*(ab)) = .96

> .03 > .04 > .05

significant significant significant

70 % 95 % 99 %

Delta(E*(ab)) = 1.39 Delta(E*(ab)) = 1.39 Delta(E*(ab)) = 1.39

> .03 > .05 > .05

significant significant significant

Fig. 6-28. Test of significance (n = 20; computer output).

6.4 Significance

267

cimen in the instrument during the measurement, miscalibration of the instrument, and other such constant and regular deviations. The standard deviation ellipsoid generated in the test of significance described here is valid for ± A given reference pigment with color locus aR , bR , LR ± A given binder ± A given dispersing method ± A given type of colorimeter All these items must therefore be noted every time a dispersion ellipsoid is calculated. If such an ellipsoid already exists, the procedure for determining the significance can also be applied to other color differences under the same conditions (i. e., same reference, same vehicle, same dispersing method, same instrument type). Figure 6-28 is a significance test listing for a red iron oxide pigment, based on measurements of 20 specimens (n = 20). It is worth mentioning here that Da* is so Program ªSIGNIº, Page 3 Significance of CIELAB color differences, according to DIN 55600***** Output: Significance test *************************************** Number of measurements: n = 1 Conf. int. Color differences (abs.) Crit. value Color difference is 70 % 95 % 99 %

Delta(a*) Delta(a*) Delta(a*)

= .05 = .05 = .05

^.09 ^.13 ^.15

non-signif. non-signif. non-signif.

70 % 95 % 99 %

Delta(b*) Delta(b*) Delta(b*)

= 1.12 = 1.12 = 1.12

> .10 > .15 > .18

significant significant significant

70 % 95 % 99 %

Delta(L*) Delta(L*) Delta(L*)

= .66 = .66 = .66

> .05 > .07 > .08

significant significant significant

70 % 95 % 99 %

Delta(C*(ab)) = .60 Delta(C*(ab)) = .60 Delta(C*(ab)) = .60

> .15 > .22 > .26

significant significant significant

70 % 95 % 99 %

Delta(h(ab)) = 1.648 Delta(h(ab)) = 1.648 Delta(h(ab)) = 1.648

> .148 > .218 > .258

significant significant significant

70 % 95 % 99 %

Delta(H*(ab)) = .95 Delta(H*(ab)) = .95 Delta(H*(ab)) = .95

> .08 > .12 > .15

significant significant significant

70 % 95 % 99 %

Delta(E*(ab)) = 1.30 Delta(E*(ab)) = 1.30 Delta(E*(ab)) = 1.30

> .14 > .20 > .24

significant significant significant

Fig. 6-29. Test of significance (n = 1, computer output).

268

6 Measurement and Evaluation of Object Colors

small for the higher confidence levels (95 % and higher) that it is no longer significant, while all the other color differences are still significant. Another example, this one for a single color measurement (n = 1) with an already existing dispersion ellipsoid, appears in Figure 6-29. The analysis is based on one measurement of the 20 in the same example. It should be noted that the critical values are higher, but the only additional rejection is for Da and confidence level 70 %.

6.5

Acceptability

6.5.1 Specimen Preparation Growing interest in colorimetric production control, not just for pigment but also for textile dyes, has slowed down the process of creating test methods based on proposals made in the literature. In any such method, two aspects must be given special attention: ± The preparation of color samples needed for matching ± The clear statement of task for colorists who take part in matching The determination of acceptability calls for a collection of samples. When testing the acceptability of pigments, full-shade systems (air drying systems) as discussed in Section 6.2.3, with side-by-side drawdowns of test and reference, can be prepared. It is recommended that color samples be created with systematic departures all around the color locus of the reference pigment. Such a group of samples might be prepared by adding to the reference small amounts of suitable pigments in the directions of the four color red, yellow, green, and blue, while seeking to remain in the a , b plane, that is maintaining DL = 0 (see Figure 6-30). This requirement comes about because lightness differences are weighted much more heavily in visual evaluation than are CIELAB chroma or hue differences of equal magnitude. Experience in matching tests shows that a lightness difference as small as | DL | 4 0.3 between reference and test will cause the color differences ± even if chroma and hue are equal ± to be deemed unacceptable. This point again calls attention to a weakness of the CIELAB system: Lightness differences are underestimated. In addition to the samples with pure hue-direction deviations, further samples with deviations in the lighter/darker direction should also be manufactured. The available set of samples must, of course, be sufficiently large. The number of samples to be matched can grow quite large if every one is laid next to every other one in the form of side-by-side drawdowns (like test and reference). An example: Suppose there are three difference steps in the four color directions and in each light/dark direction; then the total number of color samples including the reference is 3 7 6 + 1 = 19 (see Figure 6-30). If every sample is laid next to every other (19 7 18)/2 = 171 side-by-side drawdowns must be matched. The number of

6.5 Acceptability

269

Fig. 6-30. Color samples deviating systematically from a gray reference (the spacing between samples is greatly exaggerated for clarity).

ªdoubleº drawdowns increases rapidly with the number of deviating steps away from the reference. Adding just one more step in each of the six directions raises the total number of double drawdowns to (25 7 24)/2 = 300. Numbers of this order are also required because the orientation of the acceptability ellipsoid is initially unknown. It is therefore useful to do preliminary matches by colorists of a few typical drawdowns in order to determine rough acceptability limits. The difference steps selected on the basis of these preliminary trials should then extend out to twice the acceptability limits, so that the desired ellipsoid will definitely lie inside the region spanned by the samples. The trick of laying every color sample next to every other one not only increases the number of double drawdowns to be matched, but also permits a closer approach to the desired normal distribution. In any case, not too much importance should be attached to departures from the normal distribution that result from this procedure. If the requirement of normally distributed measurements were taken too strictly, there would be virtually no possibility of applying statistical methods to practical problems, for intact normal distributions are quite rare in practice. Textbooks state that it is sufficient for the random sample to have a single-peaked distribution, and this will always be the case here because the reference color locus lies at the center of the ellipsoid.

270

6 Measurement and Evaluation of Object Colors

6.5.2 Matching and Color Measurement Well-defined conditions for color matching have already been implied by the requirement of a clear task statement for the colorists. Where the resultant acceptability ellipsoid is intended for later use in production control, say of pigments or paints, the colorists should be selected from those who are daily involved in batch inspection, so that they can take advantage of their experience in this form of matching. The difference between acceptability* and perceptibility of a color difference is that perceptibility characterizes the visual threshold for small color differences, while acceptability represents the range of color differences that manufacturer, purchaser, user, and consumer are prepared to accept. Acceptability must, further, be in accord with the variations resulting from the methods used to produce the coloring materials and media. If acceptability limits are set so narrow that they are smaller than the fluctuations due to process variations, it is no longer possible to make a product in conformity with the standard. If, on the other hand, they are set too wide, there is a danger that they will be rejected by consumers as excessive. All these relationships and insights become part of the experienced colorist's background ± and thus the task in hand is to embody this experience in the acceptability ellipsoid, so that the computer can be supplied with the information needed for colorimetric production control. The following points are crucial for color matching proper, and must be treated with special care**: ± The illuminant under which colors are matched ± The geometric conditions of color matching ± The physiological conditions of color matching The illuminant should be chosen from among the well-known CIE standard illuminants (Section 6.1.1). For artificial average daylight, corresponding to illuminant D65, the standard gives a method for determining the quality of the lamp spectrum with the help of test color pairs. A factor working against the use of illuminant D65, however, is that no satisfactory technical implementation has yet been devised; CIE standard illuminant C is better realizable. The lamp service time must be monitored (elapsed time indicator). The geometric conditions have to do with the direction of incidence and the viewing direction (e. g., 08 incidence and 458 viewing), the aperture angle of the irradiation, and the position and size of the specimen. Physiological conditions include the visual capabilities of the viewer (ability to distinguish color, color-normality), the luminance level, the state of adaptation of the eye, the surroundings (e. g., gray, CIE tristimulus value Y = 25), and the field of view. * The use of the term ªtoleranceº in place of ªacceptabilityº is sometimes noted. This usage is not recommended, because tolerances correspond just as well to perceptibility. ** See ªColor Matchingº in Appendix 1.

6.5 Acceptability

271

The conditions listed here must be fixed exactly; they should correspond to the situation previously existing in coloristic-visual production control. It is helpful to have a suitable matching room (light box) painted gray on the inside, in which appropriate light sources and a pivoting specimen stage with angular scale are mounted. In matching, all the double drawdowns are shuffled at random like a deck of cards, then matched in a single pass. The color samples are arranged by the colorist in two groups: ± Conforming with the standard (ªYesº), that is, accepted ± Not conforming with the standard (ªNoº), that is, not accepted In reports of matching trials of this type, it is sometimes stated that even experienced colorists suffer from a ªtestº psychosis and feel themselves in a stress situation as a result. The consequence is usually an excessively strict set of decisions, that is, too many rejections. To counter this effect, it may be useful to allow two passes for matching the samples. In the first pass, the task is to classify as ªcolor difference perceptibleº or ªnot perceptibleº. In the second pass, the actual task is set: to classify as ªcolor difference acceptableº or ªnot acceptableº. In this way, the colorist is enabled to differentiate better between color differences that he can just see (though this question is not asked) and color differences that he does perceive but just regards as conforming. These two passes can be combined into one if the colorist is asked to form three groups: ± No difference perceptible: accepted ± Conforming with the standard despite difference: accepted ± Not conforming with the standard, difference too great: not accepted The first and second groups together form the ªYesº group; the third is the ªNoº group. The number j of ªYesº evaluations is tabulated for each of the numbered samples. Naturally, special care is necessary in color measurement as well, because any error made in this operation can lead to incorrect decisions later on in colorimetric production control. The requirement must be that the color measurements take place within a short time of matching by the colorist, because samples may be subject to color changes due to aging phenomena. It is desirable to sandwich the matching task between two color measurements, whose results should be averaged. Every individual measurement is tabulated under the same sample number as in matching.

6.5.3 Evaluation and Example Calculation of the ellipsoid coefficients with the likelihood function of equation (2.87) requires an appropriate computer program. Finding the maximum amounts to determining the zeroes of the partial derivatives of ln M. All methods for finding parameters by iteration, such as Newton's method (there is no difficulty in forming

272

6 Measurement and Evaluation of Object Colors

the second derivative), as well as other numerical methods, are candidates for this operation. Once the initial values for the gik and p are specified, the Da , Db , DL associated with specimen number i are input to equation (2.42) together with the number ji of ªYesº judgments: ds2 g11 Da2 g22 Db2 g33 DL2 2 g12 Da Db 2 g23 Db DL 2 g13 Da DL Aside from p = 0 the initial values for the iterative procedure should be as close to the expected values as possible given the approximate knowledge of the acceptability ellipsoid. This will prevent convergence problems. If little is known about the expected ellipsoid, it is also possible to begin with values g11 = g22 = g33 = 1 and g12 = g23 = g13 = 0. A calculation can take some minutes, depending on the number of double drawdowns, the number of colorists, the type of computer, and the iterative method chosen. As discussed in Section 2.4.5, this procedure yields the coefficients gik of the acceptability ellipsoid plus a ªfalse alarm rateº p = 1 ± q. This rate points to the reproducibility of the color-matching experiment; if one works carefully, it can be held as small as desired. If there are problems with convergence, different initial values for the gik should be tried. The resulting acceptability ellipsoid can, for example, form the basis for computer-aided colorimetric production control. The following approach seems practicable: The 50 % and 75 % ellipsoids are calculated by dividing the gik by the ds2den factors from Table 2-4. Two concentric ellipsoids result; these divide the color space into three regions. If a color locus is inside the inner ellipsoid, it is ªconforming to the referenceº; if it is outside the outer ellipsoid, it is ªnot conformingº. But if the color locus is in the region between the two ellipsoids, it can be identified as ªtentatively conformingº. The confidence limits of an acceptability test must not be confused with the confidence limits of the tolerances for mass-produced articles in production control (e. g., length of nails, cross-sectional area of thermometer capillaries). The 50 % confidence level here means that half of colorists will accept this specimen; the 75 % level means that three-fourths of colorists will accept the specimen. Accordingly, 50 % can be viewed as the limit of acceptability, since here there are equal numbers of ªYesº and ªNoº judgments. A specimen that more than half of colorists reject is thus rightly deemed ªnot acceptedº. What is more, the ellipsoids represent the result of psychophysical experiments (color matching by colorists), and so human shortcomings (errors, blunders, and prejudices) enter into them and ªblurº the acceptability limits. Ultimately, the uncertainty due to the significance, that is, the effect of the (much smaller) test error ellipsoid, must also be taken into account. These are the reasons for the recommended confidence limits; the ªtentativeº region defined by them provided a good buffer between the two effects (see also Section 6.5.4).

273

6.5 Acceptability

Fig. 6-31. Acceptability ellipsoids (projections).

Figure 6-31 presents an example of two such ellipsoids. The drawing was produced by a plot program as discussed in Section 2.4.2. Table 6-5 lists the ellipsoid coefficients. The use of a computer to determine conformity or nonconformity can then be implemented roughly as illustrated in the following examples. Suppose there are three specimens, with are to be tested for conformity to the standard. Their color differences relative to a reference are given in Table 6-6. Using the gik, the program calculates the squared distances from the reference ds250 % and ds275 %. These are entered in the right-hand columns of Table 6-6. The values indicate that Specimen 1 is conforming because ds275 % < 1 Specimen 2 is tentatively conforming because ds250 % < 1 and ds275 % > 1 Specimen 3 is not conforming because ds250 % > 1 Table 6-5. 50 % and 75 % acceptability ellipsoids for a pigment. Ellipsoid

g11

g22

g33

g12

g23

g13

50 % 75 %

2.063 4.97

0.520 1.253

9.83 23.69

0.558 1.345

0.0845 0.2037

2.069 4.99

Table 6-6. Inspection of three specimens for conformity to the standard. Specimen

Da

Db

DL

ds250 %

ds275 %

Judgment

1 2 3

0.2 0.2 0.3

0.3 0.3 0.4

0.1 0.2 0.2

0.38 0.76 1.05

0.92 1.84 2.54

Yes Tentative No

274

6 Measurement and Evaluation of Object Colors

In this way, the acceptability can be calculated by the computer and output as a ªYesº, ªNoº, or ªTentativeº on the printer. The form of the ellipsoids in Figure 6-31 once again makes it clear how much the lightness differences are underestimated by the CIELAB system. Strictly speaking, such a statement can be arrived at only with perceptibility ellipsoids, but in fact there is little doubt in specialist circles that acceptability is not entirely independent of perceptibility. Perceptibility ellipsoids in an intact color-difference system would have to be spheres in the color space; acceptability ellipsoids should be expected to display a greater similarity to a sphere. Practical trials have shown again and again that this is not the case. Accordingly, in no case known up to the present can the acceptability be characterized by citing a DE ab value alone (corresponding to the radius of this sphere). Often the agreed-on limits include not only DE ab but also the components DC ab and DH ab . One must, however, keep in mind that this expedient is nothing more than that, because such limits do not exactly divide acceptable from non-acceptable color differences. Figure 6-32 illustrates this statement clearly. If limits [DC ab ] and [DH ab ] were taken, the color locus P would be wrongly accepted; in reality, it should be rejected because it lies outside the ellipsoid. Thus it has to be stressed that a statistically correct division into acceptable and unacceptable can be accomplished only with the acceptability ellipsoid. In the field of standards development*, the first efforts are now being made to deal with the acceptability problem. In theses, however, on should perhaps see nothing more than preliminary attempts to establish the first solid methods. In a further step, the ªColorº subcommittee of the German Standards Committee (DIN) has repared a report titled ªMethods of Agreement on Color Tolerancesº (see [38] and [39] in Section 2.7). Its report should help remedy the information gap that now exists among manufacturers and users in this field. A trend that should not be emulated is the practice of some software vendors who deal with the acceptability of textile dyes but do not disclose the color-difference formulas or the test criteria used. One might well ask whether this secrecy is a attempt to mask the inadequate scientific basis for the algorithms! Even if it is not,

Fig. 6-32. Acceptability ellipsoid. [DC ab ] and [DH ab ] are agreedon limits. The color locus P is wrongly judged conforming to the standard. * See ªColor tolerances for automative paintsº in Appendix 1.

6.5 Acceptability

275

the result is very negative because it prevents discussion of the systems, possible recommendations for improving the color-difference formulas, and ± ultimately ± advances in what is today the most important specialty area of our field.

6.5.4 Acceptability and Test Errors It has been shown that the acceptability ellipsoid is a useful criterion for the approval of color formulations, since it decides what color differences are tolerated. The test error ellipsoid (total error ellipsoid, See Section 6.3.3), in contrast, tells only how well a color laboratory can perform the tests. Nonetheless, test errors are of some importance in acceptability testing, because from what has been said it should be clear that the acceptability ellipsoid can be meaningfully applied only when it is much larger than the total test error ellipsoid. The term ªtest error ellipsoidº here denotes the 2 s ellipsoid, whose confidence interval roughly corresponds to the 3 s interval in the one-dimensional case (see Table 6-4). If one uses the method described in Section 6.5.3, with 50 % and 75 % acceptability ellipsoids, this problem does not arise. The reason is that the color measurements used in finding the acceptability ellipsoids already contained errors. It is true that the errors average out on the whole, but they do contribute to increasing the standard deviation, and thus the colorist's uncertainty. If, accordingly, the region between the 50 % and 75 % ellipsoids is regarded as a ªtentativeº region, this ªgray areaº takes care of the test error in the great majority of cases. As a quantitative treatment shows, the error ellipsoid in this case can have linear dimensions as large as 1/5 of those of the 50 % acceptability ellipsoid. If this is so, then the exact size and shape of the total error ellipsoid no longer play any decisive role, because the figure vanishes in the ªtentativeº region. This 1 : 5 requirement is more than satisfied in many practical cases because test errors are commonly much smaller. The question now arises what has to happen if the linear dimensions of the error ellipsoid are larger than 20 % of the acceptability ellipsoid. First, the color lab must make an effort to reduce the total error below this threshold. The measures by which this can be accomplished are described in Section 6.3.3. It is desirable to state the 1 : 5 limit in terms of the coefficients of the two ellipsoids. There is a linear factor of five between the two ellipsoids if the traces of the two ellipsoid matrices differ by a factor of 52 = 25: tr (GT) > 25 tr (GA) or, written out in full: A A gT11 gT22 gT33 > 25 gA 11 g22 g33

where GA is the acceptability ellipsoid, and GT is the test error ellipsoid. If this limit cannot be maintained, it will be necessary to combine the test error ellipsoid with the acceptability ellipsoid. Two cases must be distinguished:

276

6 Measurement and Evaluation of Object Colors

± A color difference that is just acceptable can be rejected as a result of test error, because it appears to be shifted outside the acceptability ellipsoid ± A color difference that is just unacceptable can be accepted as a result of test error, because it appears to be shifted inside the acceptability ellipsoid Only the second of these cases is dangerous, since it gives the appearance of acceptability when there is none. For this reason, the best way to deal with excessively large test error is to diminish the acceptability ellipsoid by the test error ellipsoid. This must be done through the covariance matrices, as shown i Section 6.3.3. We then have GA 1 VA

1 GT 1 GA corr ;

that is

VT VA corr :

This relation is illustrated in a obvious way by Figure 6-33. After subtraction, the matrices must be re-inverted so that the corrected acceptability ellipsoid. GA(corr) can be obtained. The correction must be carried our with both the 50 % and 75 % acceptability ellipsoid, using the same error ellipsoid.

Fig. 6-33. Schematic representation of the integration of the test error ellipsoid into the acceptability ellipsoid.

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

7

Determination of Hiding Power and Transparency

7.1

Measurement of Film Thickness

7.1.1 Selection of Method Any determination of hiding power, transparency, or color strength requires a knowledge of the spectral scattering and absorption coefficients; in other words, these must generally be determined first. For this purpose, paint or plastic layers are prepared and used in reflection measurements with suitable photometers. This information is enough for the calculation of the relative scattering and absorption coefficients (relative to a reference pigment). For the absolute quantities, which are needed for the determination of hiding power and transparency, reflection measurements alone are not sufficient: the thickness of the layer must also be determined, as the equations in Section 3.3.3 show. The significance of film-thickness measurement in the determination of scattering, absorbing, and hiding power and transparency is immediately evident from an error analysis: If one form the differential of ln S in equation (3.124), one sees that the percent error of the scattering coefficient dS/S = ±dh/h is absolutely equal to the percent error of the film thickness. Films used in such determinations often have to be so thin that the substrate has a marked effect on the reflectance; with highly pigmented media, films only 25±35 mm thick may well occur. If the error in the thickness measurement is 3 mm (a level that is not attained by all methods), the relative error will be ca. 10 %, and this will propagate in linear fashion to the scattering or absorption coefficient. The fact that the film-thickness measurement alone has such a heavy influence on the final result is not tolerable, however, because smaller errors would be necessary even if the only requirement imposed were that of conformity to a standard. What follows is a survey of methods commonly used to termine film thickness. These are also listed in standards*, along with brief descriptions and error ranges. We follow this classification, adding the pneumatic method and also creating higher-level groupings.

* See ªFilm Thicknessº in Appendix 1.

278

7 Determination of Hiding Power and Transparency

± Mechanical methods Dial-gauge or micrometer methods Pneumatic method ± Optical methods Wedge cut method Profile measuring method (only for transparent films with known refractive index; not nondestructive) Microscopic measurement of film thickness by cross section method (not nondestructive) ± Chemical methods Gravimetric method Titrimetric method (not nondestructive) ± Electrical and magnetic methods (require metallic substrates) Coulometric method Capacitive method Eddy-current method Magnetic method ± Methods based on absorption of scattering (not applicable to all pigments or all substrates) Beta-ray backscatter method X-ray fluorescence method The selection of methods suitable for the determination of the absorbing, scattering, and hiding power must be based on the following considerations: ± ± ± ± ± ± ± ± ± ±

Range: 0±2000 mm Accuracy: +0.5 mm (better still, +0.2 mm) Noncontact measurement (no contact with the film) Nondestructive measurement Measurement on small areas, under 4 mm2 Measurement in same film areas where photometric measurements are performed Measurement independent of vehicle and pigment, pigment volume concentration, and film surface quality Method suitable for opaque black/white glass plates between 2 and 8 mm thick as substrates Measurement of mean film thickness (i. e., for films with no smooth surface) possible if necessary partly or fully automated measurement with printout of results

These requirements imply right away that most of the methods listed above are not candidates. A short list includes just four methods: dial-gauge/micrometer, wedgecut, gravimetric, and pneumatic. All other techniques are unsuitable, chiefly because they are not nondestructive or do not permit the use of glass plates as substrates. Nor do the other methods satisfy the accuracy requirements. The first three

7.1 Measurement of Film Thickness

279

of the short list methods, indeed, do not entirely fulfill some of the requirements (in particular, errors of measurement are too large; what is more, the dial-gauge/micrometer and wedge cut methods also require the destruction of the film, if only in small areas), as will be discussed in depth.

7.1.2 Gravimetric,Wedge Cut, and Dial-Gauge/Micrometer Methods The basic procedure in the gravimetric methods is to determine the mass of the film per unit area by weighing, in a analytical balance, a known area of the substrate with and without the film and taking the mass difference. Since the density of the coating material at the time of weighing is known, the mean film thickness can then be calculated. The overall uncertainty of the method is around +5 %; film ranging from under 1 mm up to 1 mm in thickness can be measured. These methods have some drawbacks that make them more difficult to use and, in terms of accuracy and speed, severely limit their application in determining the scattering coefficient, absorption coefficient, and hiding power. They are integral methods yielding only a mean film thickness over a large known surface area: Thickness variations cannot be detected and characterized; in other words, these methods do not meet the test that the thickness should be measured where the reflection measurement is done. What is more, the limited relative sensitivity of commercial analytical balances means that the accuracy is strongly dependent on the weight of the substrate. For example, the balance must have a relative sensitivity better than 2 7 105 (e. g., 1 mg in 200 g) if 1 mm variations are to be determined to 10 % accuracy on glass substrates. Another problem with these methods is that the coating density must be exactly determined or calculated; in pigmented coatings, this usually means that the PVC, the density of the pigment, and the density of the medium must be known. In the wedge cut method, a sharp cutting tool is used to make a scratch in the film, creating a wedge-shaped cut with a certain inclination angle. The specimen is placed under a measuring microscope or profile measuring microscope and the horizontal dimension of the cut is measured. From this measurement and the known section angle, the film thickness is calculated. The uncertainty is around +10 %, and films from 10 mm to 2 mm thick can be measured. In coating systems, it is also possible to measure the thickness layer by layer, provided the layers can be distinguished by color or structure. Of-the-self instruments ± a cutting device and a measuring microscope ± can be employed. The cutter has a hard-metal blade (usually replaceable) having a known edge angle and a guidance system that positions the blade in a consistent way relative to the film surface. A suitable measuring microscope will have a magnification of 506 and a scale with 100 divisions. Commercial profile measuring microscopes have 200±4006 magnification. When a measuring microscope is used to deter-

280

7 Determination of Hiding Power and Transparency

mine the projection b of the section flank, the film thickness h is calculated from b and the section angle a (see Fig. 7-1). The film thickness h is read directly off the profile cut under the profile measuring microscope. A number of factors can falsify the results given by these methods: ± Surface roughness requires more individual measurements if a representative average is to be obtained. The rougher the surface, the more uncertain the measurement ± Deformation of the coating occurs frequently when none-too-strong coatings are cut; as a result, the method cannot be used for such films ± Errors can also result from breaking of the cut edges, especially with extrabrittle paint coatings

Fig. 7-1. Wedge cut (schematic).

Even though the cut requires only a relatively small area, this method cannot really be classed as nondestructive, because the cut has to be made quite near the place where the reflection measurement is to be carried out. The dial-gauge/micrometer method involves measuring the height of the coating surface relative to a fixed datum plane and then measuring the height of the substrate after removal of the film. The difference in height gives the film thickness. This method has been reported to have +20 % uncertainty. Below 20 mm, it has a absolute uncertainty of at least +3.6 mm. Coatings from 3 mm up to several mm thick can be measured. A commercial standard instrument comprises a measuring table, a fixture for the specimen, and a dial gauge mounted so that it can be moved over the table. Any mechanically contacting instruments or suitable micrometers can be employed, regardless of whether measured values are acquired mechanically, optically, or electronically. The measuring area of the dial gauge is a sphere or spherical cap whose radius, for metrological reasons, should be as large as possible (at least 1.5 mm); the force applied must not exceed a maximum value (1.5 N). The requirements are even more stringent for the measurement of organic coatings, such as the ones of concern here: The radius must be ca. 30 mm, the force between

7.1 Measurement of Film Thickness

281

0.1 and 0.5 N. Ordinary varnish solvents or paint removers are used to remove the coating from the measurement area. Aside from not being nondestructive, this method has the drawback that the measuring device exerts a mechanical reaction on the object being measured, and the pressure is great enough to produce errors through local deformation of the coating even when the force applied is relatively slight. There are limits on how much the measuring sphere of the dial gauge can be enlarged, because otherwise a sphere with too large a diameter will measure only maximum values on rough surfaces, not the desired mean values over small specimen areas. In order to extrapolate to zero applied force, extensive series of measurements and costly calculations would have to be done.

7.1.3 Pneumatic Method The pneumatic method is really a variety of the dial-gauge method and almost ideally satisfies all the requirements of Section 7.1.1. It permits the nondestructive, non-contact, and also very accurate point-by-point determination of film thickness at locations where the film reflectances are also measured. The method is independent of the binder and pigment content and, in the case of rough surfaces, permits the measurement of the mean coating thickness in small regions, which is the quantity of interest in practice. Pneumatic distance measurement techniques are based on the fact that the volume of an air stream is governed by the narrowest cross section of the flow channel. Any change in the smallest cross section will alter the quantity of air flowing through the channel per unit time. In the pneumatic method of measuring film thickness, the air stream from a measuring nozzle is directed against the surface of the test film in such a way that the spacing between the film and the nozzle outlet is the most constricted part of the channel. With the substrate fixed in place, differences in coating thickness alter the smallest flow cross section. Two kinds of measurement are made on this principle, volume and pressure. The method described here employs the pressure principle, because the components available on the market for this method are more resistant to wear and less susceptible to malfunction, over a wider linear range, than the ones available for the volume method. In the pressure method, the pressure drop is measured within the air stream ahead of the exit from the nozzle. The pressure drop is a function of the flow rate and thus of the slit size, that is, the clearance between the nozzle and the coating surface (Fig. 7-2). Off-the-shelf instruments (for other purposes) offer transformation ratios of up to 2 7 104 ; that is, a difference of 1 mm results in a 20 mm shift in the manometer water level. Special models have accuracies down to 0.025 mm. Figure 7-3 is a diagram of a pneumatic instrument for measurements of film thickness. The names of the part are indicative of their functions. The ball-bearing posts (2) insure plane-parallel movement of the nozzle guide plate (3) over the

282

7 Determination of Hiding Power and Transparency

Fig. 7-2. Pneumatic measurement of film thickness (schematic diagram of pressure method).

Fig. 7-3. Apparatus for pneumatic measurement of film thickness. 1, baseplate; 2, ball-bearing guides; 3, adjustable nozzle guide plate; 4, top plate; 5, handwheel (or servomotor); 6, glass flat held in place by point supports and edge stops; 7, four measuring nozzles; 8, precision inductive dial gauge.

baseplate (1), exact to +1 mm. The column assembly and the measuring nozzles are available commercially (see [26] in Section 3.7); the apparatus as a whole must be shop-fabricated. To determine the scattering and absorption coefficients or the hiding power and transparency of paint films, black or white plane-parallel glass plates (100 mm 6 100 mm 6 5 mm) are used. The reflectance of the applied coating is measured on each of four circular regions; the thickness of the paint film is then measured at four fixed points in the same regions, with the four nozzles of the

7.2 Scattering and Absorption Coefficients

283

pneumatic apparatus. The glass plate rests on three points in the apparatus and is fixed in place by three edge stops. Because the linear range of the nozzles (Fig. 7-2) is not wide enough to give the needed high sensitivity at the coating thicknesses encountered in practice, the pneumatic nozzles are used solely as null indicators. The nozzle guide plate is lowered to a constant, specified distance away from the coating surface. The actual clearance measurement is done separately, with a precision inductive dial gauge to the side of the glass plate; over a linear range of up to 2 mm, this guarantees a maximum error no greater than 0.02 mm. When the measurement is performed semiautomatically, the nozzle guide plate is lowered by hand and the value for the uncoated glass flat is recorded. In the subsequent measurement on the coated plate, this value is input by means of a digital setpoint adjuster. In the fully automatic device, the plate is raised and lowered by a servomotor controlled by the nozzles. The absolute film thickness is output in analog or digital form(with the aid of an analog-digital converter). High accuracies can be achieved with the pneumatic method. The absolute error of measurement can be held under 0.3 mm, which corresponds to coefficients of variation smaller than 1% for a film 30 mm thick. The accuracy is higher than that of the dial gauge method because no mechanical pressure is exerted on the specimen.

7.2

Scattering and Absorption Coefficients

7.2.1 Kubelka-Munk Coefficients S and K of White Pigments Methods for determining the scattering coefficient S are set forth in standards*. What these methods yield is not the absolute S but a relative (i. e., referred to a reference pigment) scattering coefficient per unit mass. Such results can be meaningfully compared only if the measurements are performed with equal masses of pigment or equal PVC values. Therefore, the S values obtained (m2/L) of the pigment/binder mixtures are then referred to the pigment mass concentration PMC, i. e., to the mass of pigment (m2/g). The exclusive use of relative values has to do with results from round-robin tests performed by DIN, which showed that absolute scattering coefficients could be reproduced comparatively well in the same laboratory but no adequate agreement was possible from one laboratory to another. In contrast, relative scattering powers showed quite satisfactory agreement. Those results are no longer consid* See ªScattering Power, Relativeº in Appendix 1.

284

7 Determination of Hiding Power and Transparency

ered entirely representative for present-day conditions, because essential technical elements of specimen preparation (such as dispersing equipment and methods) and color measurement (such as the calibration of instruments) have been substantially improved since they were reported. There are, accordingly, virtually no objections to absolute measurement today, even when the same techniques are employed. The standards distinguish between ± Black-ground method ± Gray-paste method (Because of its intimate link to the determination of lightening power in the Beer's law region, the gray-paste method will be described in Section 8.3.2) Black-ground method The black-ground method* is based on evaluating the Kubelka-Munk equations over a black substrate, as described in Section 3.3.3. The German standard initially leaves preparation methods (medium used, pigment concentration, dispersing conditions, coating application conditions) open ± these are to be agreed on between testing laboratories ± and limits itself to specifying the measurement and evaluation procedure. The pigment for test and the reference pigment are dispersed in the agreed-on medium. From the resulting pigmented media, a non-hiding coat over black and an optically infinitely thick coating are prepared. Instead of the reflectances in the middle of the visible spectrum, the CIE tristimulus value Y is measured for each coating. The calculation employs this Y value, plus either the pigment mass concentration (b) and film thickness (h) or the pigment mass per unit area (mF) of the non-hiding coat**; in either case, the methods of determination must be agreed on. This point shows a second reason that relative coefficients are attractive: the possibility of doing away with the little-loved measurement of film thickness. (In other words, if the pigment mass per unit area mF can be obtained without it, e. g., from the formulation, then the film thickness does not have to be measured.) An example of this procedure will be described further on. The colorimeter should be set up to measure the CIE tristimulus value Y. The parties must agree as to whether method A or B will be used for the measurement. Black glass plates having a plane surface and CIE tristimulus values Y 5 5 are to be used as substrates; these are available commercially. The test cannot be done with pastes (no well-defined film thickness), only with solid films or plastic films or plastic wafers. In the last two of these cases, a contact liquid (e. g., immersion oil) must be used to establish optical contact between the specimen and the substrate. * See ªScattering Power, Relative, Black-ground Methodº in Appendix 1. ** Not to be confused with the pigment surface concentration (see Section 4.1.4).

7.2 Scattering and Absorption Coefficients

285

Measurement method: Measure CIE tristimulus values Y for the coatings under standard illuminant D65 or C at several points of the coating. The number of points to be measured should be dictated by the size of the sample port and the size of the surface regions on which the film thickness and pigment mass per unit area are determined. Determine Y values to four decimal places and average the measured values on each coating to obtain Y1 (hiding coat) and Yb (non-hiding coat). Select the thickness of the non-hiding coat such that the difference between Y1 and Yb is a least two units. Evaluation method: Apply surface correction (eq. 3.11) to measured CIE tristimulus values Y, setting Y /100 = R (or R, depending on configuration) in each case. When measuring high-gloss specimens by method B of Section 6.1.2, add 0.04 to the R values before applying the correction. From the corrected reflectances R , calculate auxiliary variables a and b with equations (3.118) and (3.119). From a, b, and the corrected reflectance Rb , calculate to found decimal places the product Sh from equation (3.124): Sh

1 1 x1 Arcoth x ln b 2b x 1 where x

1

(7.1)

a Rb b Rb

Here Rb is the corrected reflectance over black, and a and b are the auxiliary variables in the Kubelka-Munk theory. Now, with Sh, b, and h or from Sh and mF first calculate the scattering coefficient per unit PMC b, SP = S/b: SP

S Sh Sh b bh mF

(7.2)

Here b is the pigment mass concentration (PMC) and mF is the pigment mass per unit area, g/cm2. The formula to be used from (7.2) will depend on whether b and h or mF is determined experimentally. The test and reference values of b or mF should be as nearly equal as possible. From the values SP,T (test pigment) and SP,R (reference pigment), calculate the relative scattering power per unit pigment mass as Sr

SP;T SP;R

(7.3)

Annexes of the German standard give very detailed examples of preparation, measurement, and calculation procedures. Annex 1 cites as test medium a longoil alkyd resin modified with linseed oil; as dispersing equipment, high-speed impeller mills and single-roll and triple-roll mills. The method used to determine pigment mass per unit area in this example is to detach 100 cm2 of the film with the help of a solvent, then combust and ignite the film.

286

7 Determination of Hiding Power and Transparency

Annex 2 contains another example with PVC-P (plasticized polyvinyl chloride) plasticizer containing materials. The dispersing equipment is a mixing roll; the film is brought into contact with the black glass plates by an immersion oil used as contact liquid. The pigment mass per unit area is determined gravimetrically, with the aid of the pigment mass portion known from the preparation. The following description of a test is based on this example and also relates to PVC-P materials. Preparation method: Test medium: PVC-P materials (basic mixture A*) Dispersing equipment: mixing roll with heating; speed 30 min±1, roll width 350 mm, roll diameter 150 mm Film preparation device: multi-platen press with heating Colorimeter for method A Substrate: black glass plate with CIE tristimulus value Y ^ 4 Contact liquid: immersion oil, refractive index 1.515 Formula: 1 g TiO2 pigment + 99 g basic mixture A for test and reference In double-roll mill, premix quantity of basic mixture at 1308C until plastic. Uniformly add pigment and mix (friction 1 : 1.2, total mixing time 8 min). Prepare two mixtures each from reference and test. Using spacers (1 mm thick) in the multi-platen press, press films of the pigmented media at 140 8C (pressing time 5 min, pressure 1500 N/cm2). Cut films into pieces 500 mm 6 40 mm. The CIE tristimulus values Y are measured in the way already described. The condition 2 ^ Y1 ± Yb ^ 6 is virtually fulfilled. For the layer of infinite thickness, pieces (at least four) were stacked on the black glass plate together with immersion oil until the CIE tristimulus value Y remained constant. The pigment mass per unit area was determined as mF = mf w/F, where w is the pigment mass portion, w = m / (m + mM), F is the area, m is the weight of pigment, mM the weight of basic mixture A, and mf the weight of the film. By way of example, Figure 7-4 shows a printout of the results from one such test. Note that the quantity determined according to the standard and in the above examples is the relative scattering coefficient per unit pigment mass. Theoretically, this is identical to the zero-th approximation of the lightening power P(0) W (Section 4.7.1). In comparing two pigments, it is often more informative to compare the relative scattering coefficient SV per unit pigment volume, which is obtained by multiplying the mass coefficient by the density ratio: SV = (RT /RR) Sr (see Section 8.3.2 for more detail). Thus, for pigments of equal density SV = Sr. As has been shown, the method described can be used without change for determining the absolute S and K values as well. Of course, the film thickness h must be measured, but once this is done, the scattering coefficient S is obtained by simply * See ªPVC, Plasticized, Basic Mixturesº in Appendix 1.

7.2 Scattering and Absorption Coefficients

287

Program ªS(Rel)º Relative scattering power of white pigments (Black ground method), according to ISO 787-24 *********************************** Date: ..± ..± .. Binder: PVC-P Apparatus: Double-roll mill Colorimeter: N.N., d/8, C/2 Multi-platen press Manufacturing method: Black glass plates Method C1.1.5, recipe X, Contact liquid Dispersing method: C Input: ************************************************** |Reference is TiO2-1 |Test is TiO2-2 | PVC: .312 % | PVC: .328 % | PMP: 1.00 % | PMP: 1.00 % Film |Area No |cm2

Mass g

Y(inf) Y(b) |Area | cm2

Mass g

Y(inf) Y(b)

1 2 3 4

3.606 3.671 3.443 3.447

82.7 83.2 82.6 82.8

4.461 4.173 3.825 3.673

86.5 86.5 85.9 86.0

|20.44 |19.71 |19.33 |19.03

80.8 81.3 80.5 80.9

|21.22 |21.32 |20.71 |20.28

83.1 83.2 82.6 82.8

Output: ************************************************* |Reference |Test Film |Pigment mass Scatt. coeff. |Pigment mass Scatt. coeff. Nr. |per area per unit mass |per area per unit mass |kg/m2 m2/kg |kg/m2 m2/kg 1 2 3 4

|.01764 |.01957 |.01781 |.01811

897.4 938.3 844.5 890.7

Means: 892.7 Relative scattering power: 91.5 %

|.02102 |.01957 |.01847 |.01811

765.5 833.9 814.8 852.6 816.7

Fig. 7-4. Relative scattering powers of white pigments (computer output).

dividing the experimental product Sh (eq. 7.1) by h. The absorption coefficient is then given by equation (3.121): K = S (a ± 1). If h is measured in mm, S and K will have units mm±1 = m2/L. Finally, it should be recalled that the scattering coefficient is a nonlinear function of the pigment concentration. The product Sh is then also a nonlinear function of pigment concentration, so that doubling the pigment mass per unit area and simultaneously halving the film thickness will not necessarily preserve the same value for Sh. The product will, however, be constant if both the concentration and the doubled concentration lie in the Beer's law region. The standard takes this point into account by prescribing that the PVC be reported. Outside the Beer's law range, it is not possible to calculate the lightening power (the mass ratio at which the scattering power of the test is equal to that of the reference; see Chapter 4) from the relative scattering power, because of the nonlinear relationship between scattering

288

7 Determination of Hiding Power and Transparency

power and pigment content. In general, then, there is non expectation that relative scattering powers will be in agreement with lightening powers for given test and reference pigments.

7.2.2 Kubelka-Munk Coefficients S and K of Black and Colored Pigments In principle, the method described in the preceding section is also applicable to determining the Kubelka-Munk coefficients of black and colored pigments. All that changes is that white glass plates can be used instead of black ones with dark pigments. It is still better to use commercially available black/white glass plates right from the outset. These measure 10 cm 6 10 cm and consist of a black part and a white part cemented together. The crucial point for a consistent film thickness over the black and white parts is that there must be no step at the transition. The CIE tristimulus value Y of the white part should be 80 +2, while that of the black part should be < 5. It is also desirable to use these black/white plates for the hiding coat; reflection measurements will quickly tell whether the Y difference between the coat over black and the coat over white is less than a significance threshold (e. g., 0.002). A point to remember is that the determination of the coefficients from a non-hiding coat over black or white, together with a hiding coat, is generally more accurate than the determination based on a film of equal thickness over black and white (see Section 3.7). The reason for this gain in accuracy is that the determination of the auxiliary variable a requires just one measurement in the first case (R1 , eq. 3.120) but four in the second case (Rb , Rw, R0b , R0w, eq. 3.122), so that the error of the reflection measurement acts on the error of a four times. The measurement of R1 should be dispensed with only when special difficulties are encountered in applying the hiding coat, for example with poorly hiding pigments. For a program, it is advantageous to ask first whether a measurement of R1 is available; if it is, a is calculated from R1 . A further gain in accuracy comes about because either Rb, R0b, or Rw, R0w can be substituted in equation (3.120) for S, provided that all four measurements have been done. It is desirable to take the pair that gives the smaller error in S, as was shown in Section 3.6.2 (eqs. 3.145 to 3.149). With this improvement, the program automatically looks for the best way to calculate S and K. As an aid to programming, the calculations are listed in full in Table 7-1. Accuracy problems in the determination of S and K can arise if the pigment has a very high absorption. In order to differentiate R and R0, the films must then be made very thin or the pigment concentration must be greatly reduced. There are, however, limits to how far either change can be carried: Usable films less than 30 mm thick are difficult to make, while excessive dilution of the pigment means that not all incident photons hit a pigment particle (ªsieve effectº; see Section 3.7), so that the premises of the Kubelka-Munk theory may not be fulfilled. In such

7.2 Scattering and Absorption Coefficients

289

Table 7-1. Formulas for calculating the error of S. Primed symbols denote partial derivatives (u / ux) with respect to the variable x identified by the subscript. y S

a R R0 R R0 b R R0

1

1 Arcoth y bh 1 b2 h y2

z

(3.121) (same as eq. (3.124))

1

(3.148, 3.149)

where 1) s sb R Rb R0 R0b y yb z zb 2) sw Rw R0w yw zw sR

z

sR0 z

1

1

2 a R0 R2 0 R R0 2

2 a R R2 R R0 2

(3.147)

where 1) R Rb R0 R0b z zb sR sRb sR0 sR0b 2) Rw R0w zw sRw sR0w R

dR 1 1 1 r2 R 2 dR R dR 1 r0 1 r2 dR

(3.146)

(derivative of Saunderson correction) where 1) R R 0b R R0b 2) R 0w R0w 3) R b Rb 4) R w Rw dS 2 s2R R 2 s2R R 2 0 0

where 1) dS dSb sR sRb sR0 sR0b R R b R 0 R 0b 2) dSw sRw sR0w R w R 0w If dS2b < dS2w then it is preferable to calculate S from R0b, Rb ; otherwise, from R0w, Rw.

(3.145)

Fig. 7-5. Flowchart for calculation of S (l) and K (l).

290 7 Determination of Hiding Power and Transparency

7.2 Scattering and Absorption Coefficients

291

cases, there is nothing to do but use other methods to determine S (e. g., in white or black pastes; see Chapter 8). If S and K are used in determining the hiding power or transparency, the strongly absorbing regions of the spectrum can be neglected entirely in the evaluation in certain cases since the hiding layer practically depends upon the weakly absorbing regions (see example below). Figure 7-5 presents a flowchart for the determination of S and K. In a long loop, the wavelength-dependent reflectances are input and checked for logic (e. g., R must always lie between R0 and R1 regardless of the substrate) and accuracy (the difference between R and R0 or between R and R1 must be at least 0.02), and the Saunderson correction is applied to all values. Next comes a conditional jump based on whether R1 is present or not. If all the other four reflectances are present (regardless of whether R1 is), the error calculation is done by two methods: over black substrate and over white substrate. The S (and K) values with the smallest error are output. An example will illustrate the method. Consider the determination of S and K for a paint containing a yellow iron oxide pigment. The paint was prepared in accordance with the ªdrying systemº method (see Section 6.2.3); the vehicle was Alkydal F48 and the PVC was equal to 1%. The measured reflection spectra Rb, Rw, R0b , R0w are shown in Figure 7-6. A printout of the results appears in Figure 7-7, while Figure 7-8 is a plot of the spectral S and K values. This is a highly instructive example, showing that the required accuracy makes it impossible to determine S and K at short wavelengths, at least for the selected concentration and coating thickness. The program has generated a message (ªPigment mass per unit area too largeº) that implies a suggestion to reduce the coating thickness and/or the pigment concentration. Where S is calculable, the last column in Figure 7-7 states whether the calculation was based on Rb or Rw . As in Section 7.2.1, the gray-paste method of ISO 787-24 should also be mentioned. Absolute scattering and absorption coefficients can also be determined by this method. Because of the close interrelationship with the relative tinting strength or lightening power, this method is discussed in Chapter 8.

Fig. 7-6. Reflection spectra of a yellow iron oxide pigment in a alkyd resin paint (reflectances are Rb over black, Rw over white, Rob for black substrate, R0w for white substrate).

292

7 Determination of Hiding Power and Transparency

Program ªS AND Kº Scattering and absorption coefficients (Black ground method), according to DIN 53164 ****************************************** Date: ..-..-.. Pigment: Yellow iron oxide A Binder: Alkydal F 48 PVC: 1% Preparation: Instruction 00 Film thickness measurement: gravimetric Colorimeter, Standard observer: N.N., d/8(incl) Input:********************************************************* Film thickness h: .0476 mm Lambda Rho(inf) Rho(b) Rho(w) Rho/0,b) Rho(0,w) nm 400 --.053 .053 .048 .671 420 --.056 .056 .048 .721 440 --.063 .063 .048 .760 460 --.068 .068 .048 .784 480 --.073 .073 .048 .801 500 --.092 .092 .048 .817 520 --.129 .154 .048 .838 540 --.192 .300 .048 .848 560 --.258 .504 .048 .857 580 --.260 .579 .048 .864 600 --.250 .583 .048 .872 620 --.236 .568 .048 .883 640 --.229 .568 .048 .893 660 --.219 .579 .048 .901 680 --.217 .608 .048 .905 700 --.218 .643 .048 .914 Output: ******************************************************* KUBELKA-MUNK Coefficients Lambda a b S K Calculated nm 1/mm 1/mm from: 400 420 440 460 480 500 520 540 560 580 600 620 640 660 680 700

Pigment mass per unit area too large Pigment mass per unit area too large Pigment mass per unit area too large Pigment mass per unit area too large Pigment mass per unit area too large Pigment mass per unit area too large 2.462 2.250 14.23 20.81 1.538 1.169 16.48 8.87 1.184 0.633 19.49 3.580 1.137 0.540 18.25 2.492 1.144 0.556 17.07 2.461 1.170 0.607 15.77 2.680 1.180 0.627 15.05 2.715 1.187 0.640 13.88 2.598 1.170 0.607 13.38 2.276 1.148 0.564 13.19 1.952

Rho(w) Rho(w) Rho(w) Rho(w) Rho(w) Rho(w) Rho(w) Rho(w) Rho(w) Rho(w)

Fig. 7-7. Determination of spectral S and K values (computer output).

7.2 Scattering and Absorption Coefficients

293

Fig. 7-8. Scattering coefficient S and absorption coefficient K for a yellow iron oxide pigment.

7.2.3 Four-Flux Coefficients s+, s±, k' The computational method described in Chapter 3 fully cover the region of technical interest with regard to accuracy and complexity. The two-flux (Kubelka-Munk) and four-flux calculations in ªexplicitº form (Section 3.2 and 3.3) are simple enough that they can be performed on a desktop computer (beyond fundamental operations, only exponential and log functions are required). There is, however, a mild constraint on reliability. On the other hand, ªimplicitº many-flux calculations, that is, based on numerical integration of the differential equations, are best carried out on a medium-sized or large digital computer; the results are as reliable as the best experimental data. Even if many-flux calculations are mathematically rather complicated and tedious, they have taken on a standard form since the renowned publications of Mudgett and Richards, so that most of the work can now be done with readily available subroutines. If is therefore most remarkable that only a few publications have dealt with even the experimental aspects of many-flux theories and the four-flux theory in particular. Our first example is taken directly from Mudgett and Richards ([17] in Section 3.9). The authors report how values of the coefficients s+, s± and k ' can be obtained from S and K with the calculable coefficients of the Legendre polynomials. This means that values for these coefficients can be derived from the KubelkaMunk coefficients with the aid of approximation formulas. What is more, however, the authors cite experimental data based on measurements on plastic wafers. The specimens in the first series were colored with a TiO2 (rutile) pigment; those in the second series, with a red dye. As a consequence, the scattering and absorption coefficients were measurable separately.

294

7 Determination of Hiding Power and Transparency

The measured transmittances and reflectances were compared with the values obtained by the authors from scattering and absorption coefficients that had been calculated by the method just mentioned, that is, from series of Legendre polynomials. The agreement was excellent. The coefficients for the surface reflection were also found close to the known values r0 = 0.04 and r2 = 0.6. The coefficients referred to S and K had the following values: s+/S 2.306, s±/S = 0.464, k'/K = 0.5 These figures provide strong confirmation of Kubelka's conjecture that the absorption coefficient in the parallel flux (k ') would be half as large as in the diffuse flux (K) (see Section 3.2.2). This hypothesis also holds to a good approximation for the backscattering coefficients (s±, S). As expected, the coefficient s+ is much larger than S ± more than twice as large. With these results, equation (3.19) can now be used to calculate m/S s+/S + s±/S + k'/S 2.306 + 0.464 + (a ± 1)/2 2.270 + a/2 which will be needed for the calculation of p and q with equations (3.30) and (3.31). Equation (3.90) with the specified values of Rdif,1 (or Rdif,1 after the Saunderson correction) then yields the reflectance Rg,1 for directional irradiation. We have used these data in calculating, for the first time, the (uncorrected) reflectances Rg,1 over the reflectance range of 0.05 to 1. There is no problem with expanding the scope in this way, because mixtures of TiO2 and the red dye can be prepared experimentally for any K/S. The results appear in Table 7-2, which shows the actually expected values (i. e., after Saunderson back-correction); as expected, only small differences (50.05) are seen between the reflectances for the directional and diffuse cases, with the latter values being somewhat higher throughout the series. This is also in agreement with expectations, for there is less scattering per unit path length for the directionally incident flux than for the diffuse one. The transfer of a photon from the forward to the backward direction thus requires, on average, a longer path length than in the diffuse case. What is more, experiment has not yet provided sufficiently sure confirmation for these differences between diffuse and directional irradiation; they are too large to be excused as ªuncertainty of measurementº or ªpoor linearity at moderate reflectancesº. The reason cannot be identified with exactness; undoubtedly it is a fact that the conditions ªdirectionalº and ªdiffuseº cannot be realized precisely enough. Conventional instruments allow measurements only with conical, quasi-parallel, or diffuse irradiation, and the d/d geometry cannot be implemented neatly. Other implications of the Mudgett and Richards work include the following: The phase function for a scattering medium can be obtained from Mie equations if the scattering is due to approximately spherical particles, or from pure scattering experiments if optically thin layers can be fabricated. Similar methods can be used for determining the absorption coefficient, insuring that the scattering and absorb-

7.2 Scattering and Absorption Coefficients

295

Table 7-2. Reflectances for diffuse and directional irradiation, calculated from data of Mudgett and Richards. Rdif,?

Rg,?

0.05 0.10 0.15 0.20 0.25 0.30 0.35 0.40 0.45 0.50 0.55 0.60 0.65 0.70 0.75 0.80 0.85 0.90 0.95 1.00

0.046 0.083 0.125 0.168 0.213 0.259 0.306 0.354 0.403 0.452 0.503 0.554 0.607 0.660 0.714 0.769 0.826 0.883 0.941 1.000

ing characteristics of the medium are described adequately for use in many-flux methods. For a simpler but less accurate calculation, the two-flux or four-flux method can be employed along with the empirical relations stated above for the effective scattering and absorption coefficients. Two problems that must be allowed for in two-and four-flux calculations relate to the angular distribution of the radiant flux in the interior of the medium. The internal surface reflection coefficients react directly to changes in this angular distribution, as do the effective scattering and absorption coefficients. What causes the errors in the two-flux calculation is that the radiant flux departs more from the approximate diffuse distribution as the K / S ratio increases. Such deviations occur in layers with low pigment concentration (e. g., translucent plastics) or very thin layers (e. g., printing inks). It might be possible to counter these effects with relatively simple empirical algorithms in many practical cases, for example in order to achieve better and faster convergence for color formulations. The second application example appears in a publication of Atkins and Billmeyer (see [23] in Section 3.9). The authors compared the results of four-flux calculations with experimental results on TiO2 specimens. They find a value of s+/(s+ + s±) = 0.84 for the forward scattering as a fraction of total scattering of a directional radiant flux. In the Mudgett and Richards example, the fraction was

296

7 Determination of Hiding Power and Transparency

2.306/(2.306 + 0.464) = 0.832; this represents a good result, although it must be kept in mind that the two results are not for the same TiO2 pigment. Finally, the literature does not report any test to determine s+, s±, and k ' using the formulas of Section 3.2.5. The computational derivation of these coefficients would greatly simplify the problems that arise with translucent specimens and in color formulations. Once coefficients were determined, the laborious procedure involving implicit many-flux theories could be rendered superfluous.

7.3

Transparency

7.3.1 Single-Point and Multi-Point Methods Transparency is significant for a wide variety of applications (transparent lacquers, printing inks, etc.). That uniform testing standards* have nonetheless been devised can be attributed to the fact that such applications have in common one physical phenomenon, transparence. What is more, in view of the broad range of applications, no preparation method has been prescribed, so this point must be covered by an agreement between the parties. It should be noted that transparent pigments have to be dispersed with special care, because their small particle size means that they exhibit extremely strong adhesion forces. A preparation method will be set forth in Section 7.3.2. The standards therefore stop with general provisions that must always be considered (geometry used in measurements, corrections to be applied, calculation of results). What is determined is the transparency number of a medium, which can be unpigmented or pigmented. If the specimen preparation conditions (vehicle system, application method, film thickness, pigment concentration) are held constant, transparent pigments can also be subjected to comparative evaluation by this method. The definition of the transparency number T is expanded somewhat from the definition stated in Section 3.5.1. In Figure 3-10, the film thickness (abscissa) could be replaced by the mass of the coating (at constant pigment concentration) of by the pigment concentration (at constant film thickness) without changing the nature of the curves. The h in equation (3.139) could then be replaced by the mass of the system per unit area (e. g., the ªink loadº in the testing of printing inks) or the pigment concentration. It goes without saying that the units of the transparency number T will vary from case to case. If, for example, the pigment mass per unit area (unit g/m2, especially suitable for testing of transparent pigments) is taken as the pigment portion, the transparency number will have units of g/m2 too, and Tm then tells how much pigment is required to coat 1 m2 of substrate so that the color difference is DE ab = 1. * See ªTransparencyº in Appendix 1.

7.3 Transparency

297

The test is performed by coating a black/white substrate and using a colorimeter to measure the color differences over the black substrate relative to ideal black. As a rule, the measured values have to be corrected before the color difference is calculated, because the coating filters the light incident on the substrate and reflected from it. This correction, which should take care of the departure of the real substrate from an ideally black substrate, is applied by preparing a drawdown of the same thickness on the white substrate. The transparency number is obtained from the color difference at one or more film thicknesses (if the pigment concentrations are equal) or at one or more concentrations (if the film thicknesses are equal). The black/white glass plates must fulfill the same requirements as in Section 7.2.2. With regard to the geometry of the colorimeter, care must be taken to minimize the effect of specimen surface characteristics on the measured value. On principle, method A of Section 6.1.2 can be used if the value of surface reflection is subtracted. In the case of high-gloss plane specimens, however, the measurement can be carried out by method B of Section 6.1.2 (45/0 or 8/d(ex)). For non-highgloss specimens, overlacquering is recommended; this step is essential in the case of bronzing specimens, particularly such as occur with printing inks. The needed correction of the measured values to eliminate the effect of the real black substrate is based on the filter action of the coating, mentioned above. This is found as the ratio of the reflectometer value R' (R' = R or R' = R) of the coating over white (R'w) to the value of the white substrate (R'0w). The reflectometer value for the black substrate (R'0b) is multiplied by this ratio and the product is subtracted from the specimen reflectometer value R'b : R0corr R0b

R00b

R0w R00w

(7.4)

If the measurement is done by the tristimulus method, the same computational scheme is applied to the reflectometer values R'x , R'y, R'z or the CIE tristimulus values X, Y, Z. The CIELAB color differences are calculated by the method of Section 6.2.2. Because the transparency number so defined is a function of h, its determination requires at least two specimens differing in film thickness (multi-point method); the transparency number obtained in this way is valid in the range between the two thicknesses h1 and h2, which should differ by at least ten times the standard deviation of the h measurement. With the color differences DE1 and DE2 measured on the two films, the transparency number becomes T

h h2

h1 DE2 h1

h DE1 DE1

(7.5)

where h is an arbitrary film thickness or pigment mass per unit area lying between h1 and h2.

298

7 Determination of Hiding Power and Transparency

If the two specimens differing in film thickness have roughly equal transparency numbers, that is, when the increase in color difference is approximately linear for small film thicknesses or pigment concentrations, the transparency number can be determined in a simpler way: The multi-point method reduces to the single-point method. The formula then simplifies to a form identical to equation (3.139): T

h

(7.6)

h DEab

These methods of determination have the drawback that the coloring power or tinting strength cannot be taken into the evaluation of two transparent pigments without more details. The standards therefore suggest determining transparency numbers after tinting strength matching for the respective film thicknesses or pigment concentrations. This problem will be treated more fully in the method (see the next section) based on the principle of spectral evaluation and using the transparencycoloring power and transparency-coloring degree defined in Section 3.5. An example of the two-point method follows. The test system is a transparent yellow iron oxide pigment in an alkyd resin, 1% PVC. The following were measured: Film thicknesses h1 = 0.035 mm h2 = 0.052 mm

Color differences relative to ideal black DE1 = 12.83 DE2 = 18.87

Now the two-point formula gives T

h

h 0:035 18:87 0:052 0:035

12:83 12:83

h 355:3 h 0:39

This implies, for a film thickness of, say, h = 0.045 mm, a transparency number of T = 0.002748 L/m2 = 2.748 mL/m2. If the only measured values available were those for the first point, h1 and DE1, the single-point formula (eq. 7.6) would yield T = 0.002727 L/m2 = 2.727 mL/m2. Multiplying this value by the PVC of s = 0.01 and the pigment density of R = 4.08 g/mL yields a transparency number related to the pigment mass of Tm = 0.1113 g/m2. This value is also obtained if the pigment mass per unit area is determined instead of the film thickness and substituted for h.

7.3.2 Method Based on Principle of Spectral Evaluation The calculation employs the equations of Section 3.6.3. To make the programming easier, a flowchart is presented in Figure 7-9 and the required formulas in closed form are summarized in Table 7-3. In addition to the equations needed for calculat-

7.3 Transparency

299

Fig. 7-9. Flowchart for determination of transparency by the principle of spectral evaluation.

Table 7-3. Calculation of transparency number, coloring power, transparency-coloring power, and transparency-coloring degree. Primes denote application of the operator (u/uh)h?0 to the respective unprimed quantities. R R s rl 1 r0 1 r2 Sl dl R k 2

Z rl

1 1

r0 Kl dl r2

(3.158) (3.159)

where 1) R s X s R k X k rl x l (CIE color matching functions) 2) Y s Y k y l Z k 3) Z s z l R s R s 7:787 Rn

(3.156)

1 R k R k 3 Rn

(3.157)

where 1) R s X s R k X k R s X s R k X k Rn Xn 2) Y s Y k Y s Y k Yn Z k Z s Z k 3) Zs Zn a 500 X

Y ; b 200 Y

where 1) a a s b bs 2) a k bk DE ab

(CIE stristimulus values of standard illuminant)

Z ; L 116 Y

(3.155)

L L s X X s Y Y s Z Z s L k X k Y k Z k

q a 2 b2 L 2

where 1) DE ab DE ab;s a a s b bs L L s L k 2) DEab;k bk a k

Transparency number: Coloring power:

T = 1000/DE ab;s

F=

DE ab;k /1000

Transparency-coloring power: L = T 7 F p Transparency-coloring degree: G = L L 2

mL 7 m±2 2

m 7 mL

(3.160)

±1

(3.141) L

(3.142)

300

7 Determination of Hiding Power and Transparency

ing the transparency number, those for the coloring power F, the transparency-coloring power L, and the transparency-coloring degree G are also listed. The determination of transparency will now be demonstrated for an example. A transparent red iron oxide pigment is prepared in an alkyd resin vehicle, and the preparations are applied in ± a non-hiding coat over white ± an opaque coat The reflection spectra are then measured. After the film thickness has been determined for the non-hiding coat, the Kubelka-Munk coefficients S and K can be determined from it and the two spectra (calculation outlined in Section 7.2.2). then, by using a program running on a desktop computer, the transparency number, coloring power, transparency-coloring power, and transparency-coloring degree are calculated. Preparation method: Precondition the test pigment at 1058; determine density* and loss on ignition** (needed for analytical determination of PVC of finished paint). Use Alkydal F481 in the following preparation: 87.5 g Alkydal, 52 % in white spirit 0.57 g Ca octoate, 4 % 10.3 g white spirit 0.9 g Ascinine R55 0.74 g Bayer OL silicone oil, 5 % in xylene Add dryer (to 95 g clear paint): 0.36 g Co octoate, 6 % in xylene 0.91 g Pb octoate, 24 % in xylene Calculate PVC from pigment density and loss on ignition for pigment and paint (both by titrimetric determination of iron content). At 7.5 % PVC, disperse in agate vessels on planetary mill. Terminate dispersion operation only when coarseness 510 mm***. To prepare non-hiding coatings, dilute paint to 1% PVC and apply by a spinning film spreader on(black/)white glass plates according to Section 7.2.2. After 24 h drying, coatings should have thicknesses between 30 and 70 mm. Measure film thicknessses with pneumatic device (method of Section 7.1.3). For hiding coat, dilute starting paint to 5 % PVC (because hiding is difficult to achieve with 1% PVC); apply in several coats, allowing to dry between coats (ca. 15 min required). Place in fresh-air cabinet dryer for at least 72 h dry completely.

* See ªDensity of Pigmentsº in Appendix 1. ** See ªLoss on Ignitionº in Appendix 1. *** See ªFineness of Grindº in Appendix 1.

7.3 Transparency

301

Measurement and evaluation method: Measure reflection spectra with spectrophotometer (method A of Section 6.1.2). Determine scattering and absorption coefficients in 20 nm intervals as in Section 7.2.2. Use CIE color matching functions from Stearns' tables* (Table 7-4 and 7.4 a; see also Section 3.6.7 and [32] in Section 3.9). Next, the S and K values obtained are input to the calculation of the transparency number and the other transparency quantities. Figure 7-10 is a printout of such a calculation. Program ªTRANSPº Transparency number, Coloring Power, Transparency, Degree of Transparency, according to VÚLZ, Industrial Color Testing ****************************** Date: ..-..-.. Pigment: Red iron oxide (transp.) B Binder: Alkydal F 481 Preparation: Instruction N.N. S and K evaluation: PVC 1%, gravimetr. film thickness measurement: .0473 mm Meûgeråt u. Lichtart/Beobachter: N.N., d/8(in): C/28 Input: ************************************************************* Lambda S K nm 1/mm 1/mm 400 2.187 133.9 420 2.474 146.7 440 2.268 126.5 460 2.057 102.5 480 1.557 84.3 500 1.556 71.8 520 1.311 59.0 540 1.357 46.4 560 1.193 28.54 580 1.038 15.62 600 1.003 8.77 620 0.963 5.91 640 0.921 4.38 660 0.887 3.424 680 0.869 2.747 700 0.840 2.160 Output: ************************************************************ TRANSPARENCY NUMBER T: 1.518 ml/qm COLORING POWER Phi: 24.86 qm/ml TRANSPARENCY-COLORING POWER L: 37.74 TRANSPARENCY-COLORING DEGREE G: 98.7 % Abb. 7-10. Determination of transparency number, coloring power, transparency, transparency-coloring power, and transparency-coloring degree of a transparent red iron oxide pigment based on the principle of spectral evaluation (computer output). * See ªColor matching functions in steps of 20 nmº in Appendix 1.

302

7 Determination of Hiding Power and Transparency

Table 7-4. CIE color matching functions in 20 nm intervals after Stearns (28 standard observer). C/28 y (l)

x (l)

400 420 440 460 480 500 520 540 560 580 600 620 640 660 680 700

0.044 2.926 7.680 6.633 2.345 0.069 1.193 5.588 11.751 16.801 17.896 14.031 7.437 2.728 0.749 0.175

±0.001 0.085 0.513 1.383 3.210 6.884 12.882 18.268 19.606 15.989 10.684 6.264 2.897 1.003 0.271 0.063

0.187 14.064 38.643 38.087 19.464 5.725 1.450 0.365 0.074 0.026 0.012 0.003 0 0 0 0

0.136 2.548 6.680 6.364 2.190 0.051 1.342 5.778 11.290 16.260 17.922 14.047 7.029 2.507 0.707 0.166

0.002 0.070 0.455 1.322 2.939 6.822 14.121 19.013 18.861 15.462 10.673 6.288 2.734 0.922 0.256 0.060

0.628 12.221 33.666 36.507 18.157 5.515 1.621 0.389 0.069 0.025 0.012 0.003 0 0 0 0

98.044

100.000

118.102

95.017

100.000

108.813

P

z (l)

x (l)

D65/28 y (l)

l (nm)

z (l)

Tab. 7-4 a. CIE color matching functions in 20 nm intervals after Stearns (108 standard observer). C/108 y (l)

x (l)

400 420 440 460 480 500 520 540 560 580 600 620 640 660 680 700

0.143 3.593 7.663 6.330 1.837 0.061 1.958 6.555 12.618 16.960 17.157 12.833 6.566 2.291 0.604 0.127

0.011 0.373 1.252 2.732 5.344 8.752 12.591 16.615 17.777 14.582 10.079 5.979 2.731 0.898 0.234 0.049

0.581 17.172 39.355 36.753 16.979 4.151 0.924 0.221 0.004 ±0.002 0 0 0 0 0 0

0.251 3.232 6.679 6.096 1.721 0.059 2.184 6.810 12.165 16.467 17.233 12.894 6.226 2.111 0.573 0.120

0.023 0.330 1.106 2.620 4.938 8.668 13.846 17.355 17.157 14.148 10.105 6.020 2.587 0.827 0.222 0.047

1.090 15.383 34.376 35.355 15.897 3.997 1.046 0.237 0.002 ±0.002 0 0 0 0 0 0

97.296

100.000

116.137

94.825

100.000

107.381

P

z (l)

x (l)

D65/108 y (l)

l (nm)

z (l)

7.4 Hiding Power

7.4

303

Hiding Power

7.4.1 General (Graphical Method) According to an ISO standard*, a ªhiding power valueº is used to characterize the hiding power of pigmented media such as paints and plastic films. The standard does not contain instructions for preparation, and it leaves open such questions as the method used to measure the film thickness. It is general in application (i. e., for both chromatic and achromatic coatings) and even offers a way of obtaining hiding power values on arbitrary contrast substrates**. The hiding power value is defined (consistently with Section 3.4.1) as the area of a well-defined contrast substrate such that a hiding layer can be created with a unit volume or unit mass of the pigmented medium. ªHiding layerº means that a stated hiding criterion ± here, an agreed-on color difference between the two fields of the contrast substrate supporting the layer ± is satisfied. In comparison with the definition in Section 3.4, however, the present definition of hiding power value is extended in the same way that we treated the transparency number (Section 7.3.1). There are, accordingly, two hiding power values: ± Dv in m2/L, the area such that a hiding layer can be created with 1 L of the pigmented medium ± Dm in m2/kg, the area such that a hiding layer can be created with 1 kg of the pigmented medium If the pigmented concentration is held constant, the hiding power values of pigments can be compared. Up to ca. 10 % PVC, the hiding power value can actually be corrected for the nominal concentration by linear interpolation (see Chapter 4, ªBeer's Lawº). In order to determine the hiding power value, coatings made of the pigmented medium and having various thicknesses are applied to the contrast substrate. After the films have dried, the color differences between the two contrasting fields are determined. A plot of color difference (ordinate) versus the reciprocal of the film thickness or of the mass per unit area (absciassa) is prepared. The hiding power value is obtained by going to the ordinate value of the agreed-on hiding power criterion and reading off the corresponding abscissa. The reason for using the reciprocals is that a quasilinear plot results; what is more, the abscissa, found as just described, gives the hiding power value directly with no further calculation. As a rule, the contrast substrates are the black/white glass plates described in Section 7.2.2, with nominal Y values of Y 5 5 for the black and Y = 80 + 2 for the white parts. The standard also permits the use of black/white contrast cards, but these can no longer be recommended because they amplify the errors of measure* See ªHiding Power, Pigmented Mediaº in Appendix 1. ** For other standards see ªHiding Powerº in Appendix 1.

304

7 Determination of Hiding Power and Transparency

ment to an unacceptable degree and also because pneumatic measurement of the film thickness is not possible with cards. A gray/brown contrast substrate is also permitted; the CIE tristimulus value are specified as ± Gray field: X = 30 + 2, Y = 32 + 2, Z = 33 + 2 ± Brown field: X = 9 + 1, Y = 9 + 1, Z = 8.5 + 1 If a hiding power value is to be determined on a free film, that is, a film that has no optical contact to a substrate, a hollow light trap is to be used for the black substrate (special black standard, see Section 6.2.2) and a BaSO4 white standard for the white (see Section 2.1.2). The mass per unit area of a free film can be determined very accurately by weighing a piece whose area has been measured. Most commonly, however, it is possible to produce an optical contact with the substrates described above. The film together with a suitable contact liquid (having approximately the same refractive index as the specimen) is placed on the contrast substrate, and a rubber roller is used to press it against the substrate and expel any included air. Just as described in Section 6.2.2 for full-shade determinations on colored media, the colorimetric measurement on the contrasting fields is done by method A of Section 6.1.2. The DE ab values are determined on at least four distinct films. One of the methods of Section 7.1 is used to measure the film thickness. If Dm is desired, the mass of the medium per unit area must be determined; if no free film is available for a direct determination, the formula mF = RM h makes it possible to calculate mF from the density RM of the medium. Now DE ab is plotted versus the reciprocal of h or mF, and a curve is fitted to the points. From the hiding power criterion (DE ab = 1 is preferred), a vertical is dropped to the horizontal axis and the hiding power value is read off. Figure 7-11 presents an example of the evaluation method (yellow iron oxide pigment, 5 % PVC in alkyd resin paint). The hiding power value obtained is 17.9 m2/L.

Fig. 7-11. Graphical determination of hiding power value Dv for a yellow iron oxide pigment.

7.4 Hiding Power

305

The hiding power value is strongly influenced by the substrate contrast, increasing with decreasing contrast. On the other hand, the final result is also affected by what hiding criterion is selected; as the critical DE ab decreases, the hiding power value also falls off. For this reason, the commonly used criterion DE ab = 1 represents a good compromise between the weaker contrast substrates often found in practice and the need for a lower critical color difference due to the lower perceptual threshold of the human eye.

7.4.2 Achromatic Case Another German standard* also defines a hiding power value as in the preceding section. As before, the pigment concentration, test medium, and dispersing must be agreed on between the parties. The hiding criterion is now the lightness difference DL = 1, because the small color difference between the coating over white and black can be set equal to the lightness difference in the ideal case (i. e., if the coating really is achromatic). Hiding and non-hiding coats of the pigmented medium for test are applied and the CIE tristimulus value Y are measured. From these results and the film thickness or the mass of medium per unit area (measured on the nonhiding coat), the hiding power value Dv or Dm is determined from tables, with formulas, or by a iterative calculation. The following method is an extension of the one found in the standard, specifically in two points (see Section 3.4.2): ± Inclusion of gloss in the computer-simulated matching ± Calculation of scattering and absorption components of the hiding power value. The discussion of the preceding section can be adapted to cover the preparation of the pigmented layers and the measurement of the CIE tristimulus values Y and film thickness or mass per unit area. The calculation of hiding power values was described fully in Section 3.4.2; R is now replaced by Y /100 as it was there. After application of the Saunderson correction to the measured values and calculation of the auxiliary variables a and b, the scattering coefficient and the factor a are calculated. The three approaches mentioned above can now be used: 1) The a table (see [24] in Section 3.7). Because a depends only on the CIE tristimulus value Y1 of the hiding coat and its degree of gloss g, the table is entered with two parameters R1 and g, and a is either read off directly or found by linear interpolation. The table is restricted to the range 0.7 5 R1 5 1, corresponding to 50 5 Y1 5 100. The standard also gives a table starting directly from the measured Y1 (i. e., bypassing the Saunderson correction), but this leaves g out of account; the a table in the standard has only the values for the g = 1 column. The table need not be reproduced here, because the second approach now to be described will be more convenient and offer sufficient accuracy. * See ªHiding Power, White and Light Gray Mediaº in Appendix 1.

306

7 Determination of Hiding Power and Transparency

2) Nonlinear regression equations. They are y0 a02 R1 a01 R1 a00

(7.7)

y1 a12 R1 a11 R1 a10

(7.8)

Once y0 and y1 are known, a is calculated from their values and g: a y0 + g ( y1 ± y0)

(7.9)

It has proved useful to split the region of interest (0.7 5 R1 5 1) into three parts: Region I: 0.7 ^ R1 5 0.9 Region II: 0.9 ^ R1 5 0.97 Region III: 0.97 ^ R1 5 1 The coefficients aik needed for the calculation are listed in Table 7-5. The formulas are quite accurate, with error less than 0.2 % in all cases. Tab. 7-5. Coefficients for the calculation of a (R1 , g) with the regression formulas.

a00 a01 a02 a10 a11 a12

Region I 0.7 ^ R1 < 0.9

Region II 0.9 ^ R1 < 0.97

Region III 0.97 ^ R1 ^ 1

0.88869 ±1.32952 0.47622 0.86519 ±1.28370 0.45315

1.30598 ±2.23071 0.96232 1.27680 ±2.17282 0.93288

5.53410 ±10.96049 5.46863 5.53121 ±10.95552 5.46579

3) Direct (iterative) calculation. The equations of Section 3.4.2 are used. Figure 7-12 gives a flowchart of the calculation along with all needed equations. In principle, the hiding power values can also be calculated for black and dark gray coatings; the algorithm must then include tests for the selection of the value function (R ± gr0 5 0.008856?) as well as formulas valid for the lower range. If, however, a method based on the principle of spectral evaluation is available (see the next section), there is no need for these modifications because the method is applicable generally to chromatic and achromatic layers. Finally, the hiding power values are calculated with equation (3.133). In the iterative procedure (3) with the equations of Section 3.4.3, there is no difficulty in calculating the scattering and absorption components of the hiding power. When the a table (1) or the regression formulas (2) are employed, computational aids are called for. The tabular solutions use equations (3.133) and (3.136): Dsca aS S ;

Dabs bK K bK (a ± 1) S

7.4 Hiding Power

307

Fig. 7-12. Flowchart for iterative determination of hiding power value of white and light gray coatings.

308

7 Determination of Hiding Power and Transparency

Table 7-6. The functions aS (g) (ªhiding power due to scattering aloneº) and bK (g) (ªhiding power due to absorption aloneº). g

aS

bK

0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9 1

0.042298 0.042222 0.042146 0.042070 0.041993 0.041917 0.041840 0.041763 0.041686 0.041608 0.041531

0.42342 0.41732 0.41071 0.40347 0.39542 0.38630 0.37571 0.36290 0.34841 0.34779 0.34779

Here aS and bK depend only on the degree of gloss g; Table 7-6 gives their values. If formulas are preferred, the two values are given by aS 0.042298 ± 0.000767 g

(7.10)

For bK, two cases are distinguished: g < 0.8063: bK ± (0.05986g + 0.04386) g + 0.42263 g60.8063: bK 0.34779 (independent of g)

(7.11)

The values from these equations differ by less than 0.3 % from the tabulated values. Parts 2 and 3 of the German standard give two very thoroughly worked-out examples of the determination of hiding power values for white specimens. The pigmented medium in Part 2 is an air-drying alkyd resin paint with a TiO2 pigment; in Part 3, a plasticized polyvinyl chloride (PVC-P) also with a TiO2 pigment. What follows here is a earlier example (TiO2 pigment in alkyd resin paint) with film thickness measurement by the gravimetric method; the computer printout appears in Figure 7-13. The hiding power value and its components are obtained with an iterative routine based on the flowchart of Figure 7-12. The calculation gives a = 0.05 861, the same result as found in the a table. Equation (7.9) for 0.9 ^ R? 5 0.97 (Region II) yields a = 0.05 864, which differs by 0.05 % from the calculated value. The hiding power value is then Dv = 14.17 m2/L in both cases. For the scattering and absorption components, equations (3.133), (3.136), and (3.137) give the same results as the iterative calculation: dsca = 71.2 % and dabs = 1.1%. One point in favor of using this method for white pigments is that the result is easily derived from tables or simple formulas. There is, however, another point

7.4 Hiding Power

309

Program ªHIDING WHITEº Hiding power of white and light gray media, according to DIN 55984 (extended method) *************************************************** Date: ..-..-.. Pigment: TiO2-Z Binder: Alkydal F 48 PVC: 27.23 % Preparation: Instruction PP Film thickness measurement: gravimetr. Colorimeter, Standard Observer: N.N., d/0 (incl.), C/2 degr Input: ************************************************************* Film thickness h: .0473 mm Gloss degree g (of Rho(b)): .764 Reflectances: Rho(b): .8030 Rho(inf): .8688 Output:************************************************************ Auxiliary quantities: a = 1.0018854 b = 0.061435 Scattering coefficient: S(v) = 241.73 l/mm Hiding power value: D(v) = 14.17 m2/l Scattering component: Delta(sca) = 71.2 % Absorption component: Delta(abs) = 1.1% Interaction component: Delta(int) = 27.7 % Fig. 7-13. Deterimination of hiding power value for a white paint containing a titanium dioxide pigment (computer output).

grounded in the hiding power criterion. The hiding power value obtained by this method will be the same as in Section 7.4.1 only with extrapolation to DL = 1 (instead of DE ab ) in the graphical evaluation. For a nearly white or nearly gray specimen, the chroma and hue differences between white and black should be of a higher order than the lightness difference, but this condition is not always adequately fulfilled. The effect is exaggerated because the CIELAB system underestimates lightness differences and overestimates chroma differences. As a result, the undertone in many cases becomes an effect of less than second order. This difference between the hiding power criteria manifests itself in the following way: Two specimens equal in lightness, one being a neutral white and the other exhibiting a slight yellow undertone, would have the same hiding power value over a black/ white contrast substrate if the evaluation were based on DL = 1, but if it were based on DE ab then the yellow-toned specimen would have a higher DE ab between black and white than the neutral specimen, since it would have a chroma difference DC ab contributing to the color difference DE ab . To make DE ab equal to 1, as specified by the criterion, the layer would have to be made thicker, and this would lead to a lower hiding power value. Accordingly, when comparing white pigments, it may sometimes be useful to determine the hiding power in accordance with the criterion DL = 1. In the evaluation with DE ab = 1, a yellow-toned specimen will therefore have a lower hiding power than a color-neutral specimen of the same lightness. The next section will show how this effect can show up in the scattering and absorption components of the hiding power.

310

7 Determination of Hiding Power and Transparency

A determination of the contrast ratio of white latex paints* is mentioned only peripherally. Such determinations tell nothing beyond whether a stated contrast over black and white is or is not attained at a given film thickness. They do not provide unambiguous information about what hiding power can be achieved or about the effectiveness of the paint.

7.4.3 Based of Principle of Spectral Evaluation The basis for determining the hiding power with the principle of spectral evaluation was treated in great depth in Section 3.6.2, which also presents the equations (repeated here in Table 7-7 as a programming aid). Figure 7-14 is a flowchart for the procedure including determinations of S and K (see Section 7.2.2). After the required data and the film thickness have been input, the program requests the needed reflectances as a function of wavelength in 20 nm steps. The CIE color matching functions are taken from Stearns' table (Table 7-4; see Section 3.6.2 and [32] in Section 3.9). In each pass through this first loos, the scattering and absorption coefficients associated with this wavelength are calculated and output. When the loop terminates, the second loop is performed; it iterates h up to the hiding coat. A suitable iterative method must be used; that is, the change in film thickness must be derived from the residual difference between the actual color difference and the nominal value 1. When a color difference of 1 has been reached (to the required accuracy), the reciprocal of the hiding film thickness is output as the hiding power value. In Section 3.6.2, Newton's method was also recommended for this calculation and the equations for the method were written out. Table 7-8 again lists these formulas as a programming aid; here the prime denotes a partial derivative with respect to h. The flowchart in Figure 7-15 shows, in the nested loop, the iterative calculation of the hiding power and its components in accordance with Table 7-8. An example (chromium oxide green) is given Figure 7-16; the reflectances of the substrates, of the non-hiding coat over black and white, and of the hiding coat are shown. Figure 7-17 is a printout generated by the program for the same pigment; the calculations of transparency, coloring power, and so forth have now been included. The program yields basically the same hiding power values as the procedure of Section 7.4.1. If, however, the procedure of Section 7.4.2 (achromatic layer) is used, departures may show up because of the DL = 1 hiding power criterion. The effect of the hiding power criterion on the final result was discussed in the preceding section, where it was stated that white specimens showing an undertone may have lower hiding power values than neutral white specimens of equal lightness if DE ab = 1 is selected as the hiding power criterion. A further consequence of this behavior is that the ªhiding power due to scattering aloneº, as calculated with the * See ªEmulsion Paintsº in Appendix 1.

7.4 Hiding Power

311

Table 7-7. Formulas needed for determination of the hiding power. Specified as measured values: (I) R1 Reflectance of hiding coat R Reflectance of non-hiding coat R0 Reflectance of substrate OR (II) R0b R0w Rb Rw R

Reflectance of black substrate Reflectance of white substrate Reflectance over black Reflectance over white R

1

r0

r0 r2 1

(3.8)

R

(Saunderson-correction r0 = 0.04; r2 = 0.6; or r0 (l), r2 (l) as inputs) 1) R R1 R R1 2) R0b R0b 3) R0w R0w 4) Rb Rb 5) Rw Rw

where

(I) a

1 R1 R1

(3.120)

or (II) a

1 Rw R0w Rb R0b 1 Rb R0b R0w 2 Rb R0w Rw R0b

b

p a2 1

S

1 1 Arcoth bh

Rw

(3.122) (3.120)

a R R0 R R0 (Scattering coefficient; R, R0 from I or II) b R R0

(3.121)

K (a ± 1) S (absorption coefficient) Begin iteration loop: With h = h0 as initial value R

1

where

R

1

R0 a b coth bSh a b coth bSh R0

(3.111)

1) R Rb R0 R0b 0 2) Rw R0w 0.9048 (from R0w = 0.8) r0 1

r2 R r0 r2 R

g r0

(3.150)

312

7 Determination of Hiding Power and Transparency

Table 7-7. Continuation (Saunderson back-correction with allowance for gloss) 1) R Rb R Rb 2) Rw Rw

where Rb

R

rl Sl Rb;l dl ;

Rw

R

rl Sl Rw;l dl

(Sl = S (l), standard illuminant) where

(3.151)

1) Rb Xb Rw Xw rl x l (CIE color matching functions) 2) Yb Yw y (l) 3) Zb Zw z (l) Branch in program: A) R/Rn >p0.008856 B) R/Rn ^ 0.008856 R 3 R=Rn R 7.787 7 R/Rn + 0.138 where

(2.5) (2.6)

1) R Xb R X b Rn X n (CIE tristimulus values of standard illuminant) 2) Y b Yb Yn 3) Z b Zb Zn 4) X w Xw Xn 5) Y w Yw Yn 6) Z w Zw Zn

End of branch a 500 (X ± Y*) b 200 (Y ± Z ) L 116 7 Y ± 16 where

1) a ab b bb L Lb X Xb Y Yb Z Zb 2) aw bw Lw Xw Yw Zw

Dr rw where

DEab

(2.7)

rb

(2.11)

1) Dr Da rw aw rb ab 2) Db bw bb 3) DL Lw Lb p Da2 Db2 DL2

Return to beginning of loop (eq. 3.111) after applying correction to h; continue until DE ab = 1.

(2.10)

7.4 Hiding Power

Fig. 7-14. Flowchart for determination of hiding power with the principle of spectral evaluation.

313

314

7 Determination of Hiding Power and Transparency

Table 7-8. Formulas for h iteration (Newton's method). Prime denotes partial derivative u/uh of the unprimed quantity. See Table 7-7 for specified inputs. After equation (3.111) of Table 7-7, insert: R

a

bS 2 1 R0 2 a R0 R0 sinh bSh b cosh bSh2

(3.153)

1) R R b R0 R0b 0 2) R w R0w 0.9048 (from R0w = 0.8)

where

On grounds of computational economy, it is desirable to calculate the three hyperbolic functions in equations (3.111) and (3.153) as follows: E = exp (bSh), sinh bSh = x = (E ± 1/E)/2; cosh bSh = y = (E + 1/E)/2; coth bSh = y/x. After equation (3.150) of Table 7-7, insert: R

1

where

1

r0 1 r2 R r2 R 2 1) R R b R Rb R R b 2) R w Rw R w

After equation (3.151) of Table 7-7, append: where

4) Rb X b Rw X w Rs;l R b l Rw;l R w l 5) Y b Y w R w (l) R b (l) 6) Z b Z w R w (l) R b (l)

After equations (2.5) and (2.6) of Table 7-7, insert: R R b R R w A) R b b ; R w w ; 3 Rb 3 Rw where

R b R w B R b 7:787 ; R w 7:787 Rn Rn

1) R b X b R w X w Rb Xb Rw Xw R b X b R w X w Y w Y b Y w 2) Y b Yb Yw Z w Z b Z w 3) Z b Zb Zw

After equation (2.7) of Table 7-7, insert: a 500 X where

Y ;

b 200 Y

L 116 Y

1) a a b b bb L L b X X b Y Y b Z Z b L w X w Y w Z w 2) a w bw

After equation (2.11) of Table 7-7, append: where

Z ;

4) Dr Da rw a w r a b 5) Db bw bb Lw L b 6) DL

7.4 Hiding Power

315

Table 7-8. Continuation After equation (2.10) of Table 7-7, insert: Z = ln DEab

Z

(ln x converges to 0 faster than x ± 1)

1 2 DEab

Da Da Db Db DL DL Z Z

hn1 hn

(new value h = hn+1)

(3.152)

If jhn1 hn j 1 < 10 6 ; then h hD and D hn hD Special cases 1. ªDue to scattering aloneº Delete equation (3.111) of Table 7-7 and equation (3.153) of Table 7-8 and replace with: 1 R0 S h R0 1 R0 S h 1 2 1 R0 R S 1 R0 S h 1

R

(3.113) (3.154)

as equation (3.133) with h hD;sca ;

Dsca

1 ; hD;sca

dsca

Dsca D

(scattering component)

2. ªDue to absorption aloneº Delete equation (3.111) of Table 7-7 and equation (3.153) of Table 7-8 and replace with: R R0 e

2Kh

R

;

2 K R

(3.112), (3.154)

as equation (3.133) with h hD;abs ;

Dabs

1 ; hD;abs

dabs

Dabs D

(absorption component)

For each of cases 1 and 2, the same iteration loop can be used as in Table 7-7, supplemented by equations (3.153), (3.152), (1.133) (see above) dint 1 ± dsca ± dabs

(interaction component)

(3.137), (3.138)

316

7 Determination of Hiding Power and Transparency

Fig. 7-15. Flowchart for determination of hiding power in accordance with the principle of spectral evaluation (Newton's method).

Fig. 7-16. Reflection spectra of a chromium oxide pigment in alkyd resin paint (reflectances: Rb over black, Rw over white; R1 , hiding coat; R0b , black substrate; R0w, white substrate.

7.4 Hiding Power Program ªHIDING COLOREDº Hiding power and Transparency of Colored Pigments, according to the Principle of Spectral Evaluation (VÚLZ, Industrial Color testing) ******************************************************* Date: ..-..-.. Pigment: Chrome oxide green Binder: Alkydal F 48 r0,r2: Standard values Gloss degree: 94% PVC: .98 % Film thickness: .05796 mm Measuring conditions: d/8 (incl) Rho(inf): measured Rho(b): Input from keyboard Rho/0b): Input from keyboard Rho(w): Input from keyboard Rho(0w): Input from keyboard Input: ***************************************************************************** Lambda Rho(inf) Rho(0b) Rho(0w) Rho(b) Rho(w) 400 nm .1328 .0446 .5145 .1214 .1641 420 .1155 .0453 .5650 .1104 .1415 440 .0783 .0452 .6231 .0766 .0928 460 .0687 .0452 .6866 .0677 .0803 480 .0749 .0445 .7442 .0737 .0894 500 .0963 .0443 .7753 .0931 .1209 520 .1678 .0440 .7968 .1467 .2360 540 .2088 .0439 .8071 .1699 .3052 560 .1476 .0439 .8229 .1287 .2079 580 .1022 .0438 .8249 .0948 .1367 600 .0912 .0436 .8246 .0864 .1203 620 .0977 .0436 .8270 .0917 .1313 640 .1130 .0434 .8252 .1038 .1574 660 .1407 .0434 .8258 .1232 .2051 680 .1751 .0431 .8243 .1431 .2650 700 .2086 .0430 .8192 .1587 .3234 Output:**************************************************************************** KUBELKA-MUNK-Coefficients, related to PVC 1% Lambda a b K (1/mm) S (1/mm) Calculated from 400 nm 2.474 2.263 12.77 8.661 Rho(w) 420 2.931 2.755 15.42 7.984 Rho(w) 440 5.360 5.266 22.77 5.221 Rho(w) 460 7.026 6.954 25.88 4.295 Rho(w) 480 5.845 5.758 23.94 4.941 Rho(w) 500 3.778 3.643 18.62 6.704 Rho(w) 520 1.9411 1.664 9.371 9.958 Rho(w) 540 1.6114 1.264 6.722 10.99 Rho(w) 560 2.204 1.964 10.86 9.014 Rho(w) 580 3.461 3.313 16.31 6.630 Rho(w) 600 4.112 3.988 18.15 5.831 Rho(w) 620 3.696 3.559 16.78 6.222 Rho(w) 640 3.015 2.845 14.15 7.019 Rho(w) 660 2.320 2.093 10.80 8.182 Rho(w) 680 1.8664 1.576 8.004 9.238 Rho(w) 700 1.6125 1.265 6.089 9.940 Rho(w) TRANSPARENCY Standard Illuminant/Standard Observer: C/2 degr Transparency number T .2602 ml/m2 Coloring power Phi 4.607 m2/ml Transparency-coloring power L 1.199 Transparency-coloring degree G 75.9% HIDING POWER Hiding power value D 6.171 m2/l Scattering component p(sca) 3.04% Absorption component p(Abs) 40.18% Interaction component p(Ww) 56.78% **********************************************************************************

Fig. 7-17. Determination of hiding power, including transparency (computer output).

317

318

7 Determination of Hiding Power and Transparency

scheme described above, may be larger than the hiding power itself; in other words, the scattering component of the hiding power may be more than 100 %. The unavoidable conclusion is that the interaction component is negative. In such a case, absorption makes only a small positive direct contribution; on the other hand, the interaction makes a clearly larger negative contribution to the hiding power, since the undertone that reduces the hiding power comes about only through the interaction of scattering and absorption. This statement is illustrated by the example in Figure 7-18, where a white pigment with a slight yellow undertone was used.

Fig. 7-18. Hiding power of a white pigment in alkyd resin paint (example of negative interaction component of hiding power).

The program described here seems to be a sort of final step in the determination of hiding power for arbitrary paints. The hiding power can be determined with a computer program that leaves virtually nothing to be desired. As has been shown, the determination of transparency (and the transparency quantities) has also been integrated into the program. At the same time, this program illustrates the universal applicability of the principle of spectral evaluation.

7.4.4 Economic Aspects Any statement about hiding power, regardless of whether it is expressed as Dv in m2/L or as Dm in m2/kg, is a statement about effectiveness. This becomes particularly obvious if hiding power values are plotted versus the pigment volume concentration. The flowchart of Figure 7-19 makes clear what steps are required in order to plot the D versus s curve (curve of hiding power value versus PVC). Figure 7-20 shows Dv versus s curves for two TiO2 pigments (one anatase and one rutile). The plot demonstrates not only the well-known superiority of rutile pigments, but also the existence of a maximum in the D curves for both pigments,

7.4 Hiding Power

319

Fig. 7-19. Flowchart for determination of hiding power of white pigments as a function of PVC.

Fig. 7-20. Hiding power value Dv, versus PVC (TiO2 pigments in alkyd resin paint).

each maximum lying at a PVC value of around 30 %. Further, the curves show the relationships between rutile and anatase with regard to a hiding coat (run a horizontal from one curve to the other). The maximum hiding power value of 21 m2/L for anatase, at 29 % PVC, is already reached by the rutile pigment at a PVC of 13 %. In other word, substantial amounts of pigment can be saved. On the other hand, more binder must be used; the actual saving is not seen until the costs of pigment and binder for the hiding coats are added up. A cost analysis based on the Dv versus s plot is quite possible, as KEIFER has shown (see [27] in Section 3.9). The reciprocals of the ordinate values 1/Dv = hD give the dry film thicknesses; the abscissa values s and the densities of the pigment and medium give the mass fractions; and these are multiplied by the respective prices. The sum of the cost contributions for pigment and medium yields the desired total cost fL of the hiding coat of paint. The formulas are

320

7 Determination of Hiding Power and Transparency

f hD sRP fM hD (1 ± s) RM PM

(7.12)

fL f + fM hD [(RP ± RM PM) s + RM PM] where f is the cost per unit area, US$/m2 ; R is the density, g/cm3( = kg/L); s is the PVC; P is the price per unit weight, US$/kg; hD is the hiding film thickness, mm( = L/m2); and the subscripts have the following meanings: no subscript, pigment; M, medium (unpigmented); L, pigmented paint. Figure 7-21 presents cost curves obtained in this way. The total cost (fL) curves show the expected distinct minima. From this plot it can be deduced that a hiding coat made with anatase pigment has a much higher total cost than one made with rutile pigment; the difference ranges from 25 % to 30 %, depending on the PVC. The component curves (f and fM) show that not only the cost of the pigment but also the cost of the medium used to create a hiding coat are higher for anatase.

Fig. 7-21. Costs of hiding coats versus PVC.

The explanation of this result is that, when an optically less capable pigment is used at a given PVC, hiding requires a thicker film. This thicker coat, however, contains not just more pigment but also more of the medium. Hence it is easy to see that even small differences in the optical properties of pigments have major effects on the cost calculation. The minimum in the cost curve of Figure 7-21 shows how much pigment must be used in order to obtain the least expensive hiding coat. The position of the cost minimum depends on the shape of the Dv versus s curve, as has been shown. If the prices per unit volume for pigment and vehicle were equal (RP = RMPM), the price minimum in Figure 7-21 would coincide with the hiding power maximum in Figure 7-20, as can be inferred from equation (7.12). If the prices change, the minimum shifts and a new curve has to be plotted. For example, suppose the price

7.4 Hiding Power

321

of the pigment goes up; then the cost minimum moves toward lower PVC. This means that it has become more economical to use less pigment, even though the new pigmented medium hides less well and so must be applied in a thicker coat to hide. The method described here makes it possible to arrive at correct assessments of pigments ± with respect to optical performance and economics ± on the basis of the hiding power versus PVC curve. Such results cannot be achieved through simple estimation.

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

8

Determination of Tinting Strength and Lightening Power

8.1

Content of Coloring Material

8.1.1 Dyes Organic dyes can be quantitatively determined by methods based on physical optics or by chemical analysis. The recommended way to determine dye concentrations in solutions is through the concentration-dependent Kubelka-Munk function, which is discussed in Section 8.2 in connection with tinting-strength determination of dyes. For the test methods described here, the determination of concentration is not so important, because tests are commonly performed on preparations (paint, resin, aqueous solution) made up with a known quantity of dye in the first place. This survey will be a brief one making no claim of completeness. When determination problems occur in relation to dyes, the extensive specialist literature must be consulted (see [3] in Section 1.4 and [32] in Section 4.10). Chemical methods for determining the concentration of dyes can be employed only when the constitution of the dye, or at least its molecular weight, is known. The first technique to mention is elemental analysis, but only when the dye contains an element that the medium does not. Other methods are applicable to a dye dissolved in a liquid. The most important of such methods ± because they are valid for nearly all groups of dyes ± are reduction methods. Titanium(III) sulfate or titanium trichloride is used as reducing agent. Azo dyes in (acidic) aqueous solution can be titrated directly or indirectly; the same holds for a number of heterocyclic dyes. Azo and anthraquinone dyes can also be determined by oxidizing with chromic acid and measuring the volume of nitrogen evolved. Other basic dyes can also be determined by oxidimetric titration with cerium(IV) sulfate. Precipitation methods are sometimes used for the quantitative determination of anionic dyes (e. g., with cetyl triammonium bromide in chloroform). In the case of basic dyes, anion-active compounds such as alkylsulfonates are suitable for precipitation titrimetry. Some of the techniques listed are also appropriate when several dissolved dyes must be determined at the same time (dye mixtures).

324

8 Determination of Tinting Strength and Lightening Power

8.1.2 Pigments Again, in most test methods the quantity and hence the concentration of pigment are known from the outset. Even so, concentration determination may be useful, as for example in the determination of S by the black-ground method, already discussed. Procedures for the determination of pigment contents are set forth in standards*: ± Centrifuge methods, chiefly for production control by the producer and incoming inspection by the consumer (not suitable for separation of carbon black or finely divided SiO2) ± Incineration methods (not suitable for determination of organic pigments) ± Filtration methods (also suitable for the separation of carbon black and finely divided SiO2) Of these groups, centrifuge and filtration methods are applicable chiefly to liquid paints; incineration, on the other hand, is also appropriate for determinations on surface coating finishes and other coatings as well as plastics. The residue generally contains all the non-combustible particles, that is, pigments, fillers, and other solid additives. Any of the three methods will require an analytical balance, a desiccator, and an oven. Centrifuge Methods The quantity determined is the mass fraction of solid particles insoluble in the selected solvent. A sample is diluted with a solvent or mixture of solvents, and the solid particles are separated by centrifugation. The solid material is dried and weighed, and the pigment content is calculated as a fraction. The following apparatus is required in addition to those listed above: a laboratory centrifuge with cups and taring device, and a ball-type stirrer. A low-boiling solvent should be chosen if possible. Incineration Methods The solvent is first evaporated off from the sample; the residue is then ashed at 450 8C if carbonates are present, at 700±900 8C otherwise. The pigment content is determined from the mass of the residue, either directly of after an analysis. Additional apparatus required includes porcelain crucible, crucible tongs, muffle furnace, or fast ashing device. Filtration Methods The sample is mixed with a suitable organic solvent or mixture of solvents, then with a solution of KOH in methanol. The mixture is filtered through a glass filter crucible with filter aid. The solid matter recovered is dried and then weighed. The * See ªPigment Contentº in Appendix 1.

8.2 Relative Tinting Strength

325

pigment content is calculated from the mass of the solid component. The following additional equipment will be needed: glass filter crucible, safety pipet, filter aid, KOH solution in methanol (1 mol/L), analytical-grade methanol. With many pigments and pigment mixtures, a simple determination of the residue is not enough; the residue must be subjected to analysis and examination. The analytical methods for inorganic pigments are contained in standards*.

8.2

Relative Tinting Strength

8.2.1 Dyes A method for determining the relative tinting strength of dyes in solution is described in standards**; the procedure is a spectrophotometric one. On the basis of the relative tinting strength as defined for dyes (Section 4.6.1), the absorption coefficients (or extinction coefficients) are determined at the absorption maximum and the ratio is taken. The dye solutions must not scatter light, and the absorption curves must be highly similar in nature; that is, only dyes similar in hue may be compared. This kind of test applies to dyes such as are used in paints, inks, and so forth. The solution media (solvents but also binders) employed in preparing the solutions must satisfy the following requirements: The dyes must be completely soluble in the medium, the resulting solutions must be stable, and the results of the measurement must be such that they can be extended to lab practice. Solutions of the test dye and reference are prepared; these should have concentrations as nearly equal as possible. In addition to the usual laboratory apparatus (pipets, volumetric flasks, analytical balance), a spectrophotometer or filter photometer with the proper glass cuvettes is necessary. No particular solution medium is specified, but the following are especially suitable: ± N-Methyl-2-pyrrolidone (particularly good for basic, oil-soluble, and metal complex dyes) ± Dimethylformamide ± Dimethylsulfoxide When concentrated dye solutions must be further diluted, the above list can be supplemented with ± ± ± ±

Toluene 2-Ethoxyethanol Ethanol Water

* For a Listing, see [1] in Section 1.4. ** See ªTinting Strength, relative, Dyes in Solutionº in Appendix 1.

326

8 Determination of Tinting Strength and Lightening Power

Binders and other additives (acids, bases, complexing agents, surfactants, antioxidants, etc.) can also be used as part of the medium. Preparation method: Weigh out suitable amounts of solid dyes (e. g., 0.1 or 1 g) or dye solutions, with accuracy to 0.0001 g. Quantitatively transfer weighed samples to volumetric flasks (100 or 250 mL) and completely dissolve in solution medium. In the case of solid dyes, it is useful to predissolve the material (stirrer, heating). Fill volumetric flasks, homogenize contents, and dilute in one or more steps to a concentration for measurement such that the transmittance is 10±30 % (corresponds to concentrations of 2 to 40 mg/L). Measurement method: Within one hour after preparation (protect from light until measurement), measure transmission/extinction at the absorption maximum of the solutions; in the same cuvette, measure blank value (solution medium used).Take difference in extinction between measurement and blank (unless using a two-beam instrument).From it, calculate absorption coefficients k@ b per unit mass concentration (specific extinction coefficients), using the formula k@ b = E/(h 7 b), where E is extinction, h is length of path of the cuvette, and b is mass concentration of dye. The relative tinting strength is then found as the ratio of k@ b values between test and reference dyes. Figure 8-1 is a computer printout from a determination of relative tinting strength for dyes. Standard deviations obtained in round-robin tests between laboratories were less than 2 %; in repetitions by the same laboratory, ca. 1%. Program ºP(REL), DYEº Relative Tinting Strength of dyes in solution, according to DIN 55978 ********* Date: ..-..-.. Colorimeter: Spectral ABC Cuvette: 10 mm Input:************************************************************* Test: Red dye T Reference: Red dye R Measured solution: Instruction Dye/3 Measured wavelength: 505 nm Mass concentration: Test: 19 mg/l Standard: 20 mg/l Extinctions; Test: 1.6094 Standard: 1.6607 Output: *********************************************************** Relative Tinting Strength: 102 % ****************************************************************** Fig. 8-1. Determination of relative tinting strength of dyes in solution (computer output).

8.2 Relative Tinting Strength

327

8.2.2 Inorganic Black and Colored Pigments (Lightness Matching) Effective methods for determining the relative tinting strength and color difference after color reduction on inorganic black and colored pigments can be found in standards*, which set forth the conditions that must always be fulfilled if erroneous results are to be avoided. The ISO standard is concerned with some of the tinting strength criteria discussed in Section 4.6.2. The following criteria are permitted: ± Minimum (X,Y, Z) ± the smallest of the CIE tristimulus values ± CIE tristimulus value Y (or lightness L ) ± Color depth TS What is more, instructions for determining the color difference after color reduction are given. The ISO standard includes the use of the zero-th approximation (see Section 4.6.4) to rationalize the determination of tinting strength with the aid of the Kubelka-Munk function. It describes an alkyd resin paste method with which the spectral absorption coefficients per unit mass and the relative tinting strength can be determined. The tinting strength criterion is Rmin (l), the reflectance at the absorption maximum (or else min (R'x , R'y, R'z ), i. e., the smallest of the reflectometer values). Thus the prerequisites exist for an effective method in the case of inorganic pigments; the tinting strength criterion is the CIE tristimulus value Y (i. e., the lightness L ); see Section 4.6.3. The following equipment is needed: ± ± ± ±

Triple-roll mill Automatic muller Paste film holder (see Section 6.2.3) or other suitable paste support Colorimeter (spectrophotometer or tristimulus instrument) Preparation method: White pigment paste with the following composition (by mass): ± 40 parts TiO2 (type R2 of ISO 591; e. g., Bayertitan R-KB2) ± 56 parts Alkydal L 64 (Bayer AG) ± 4 parts Ca stearate Thoroughly mix ingredients on order to wet the solids. Pass through triple-roll mill until grindometer test** yields a value 55 mm. Store paste in airtight container. Place 3 g of white pigment paste on lower plate of muller; spread 0.12 g of inorganic pigment (test or reference) on it and mix with spatula. Distribute mixture

* See ªTinting Strength, Relativeº in Appendix 1. ** See ªFineness of Grindº in Appendix 1.

328

8 Determination of Tinting Strength and Lightening Power

in form of a circular ring. Mull in four stages of 25 revolutions each with a weight (1 kN) applied; after each stage, collect paste and redistribute. Measurement method: Measure CIE tristimulus value Y (also X and Z for color difference after color reduction) or reflectometer value R'y (also R'x and R'z if necessary) of the reducing white on the paste film holder. Preferred procedure is method A of Section 6.1.2 (i. e., with surface reflection included). Evaluation: Apply Saunderson corrections to all CIE tristimulus values (eq. 4.95). use equation (4.61) to calculate Kubelka-Munk functions F, FR ; use equation (4.94) to calculate tinting strength. The tinting strength obtained in this way is identical to the relative absorption coefficient per unit mass, so the F values must first be divided by the pigment mass concentrations unless precisely 0.12 g of test and reference pigments was taken. To determine the color difference after color reduction, convert CIE tristimulus values X and Z of reference to matching concentration (with help of Kubelka-Munk functions and the relative tinting strength P just determined). From the CIE tristimulus values after Saunderson back-correction, calculate CIELAB coordinates by known method, and thence color differences. In the case of black pigments, it may be desirable to report the relative hue* as specified in Section 2.3.3 instead of the hue and chroma differences. The flowchart for this determination appears in Figure 8-2; Table 8-1 lists the needed computational steps as an aid to programming. Here the reference is matched to the test pigment; this is recommended because the test is performed at ^ If the test were matched to the reference, a fixed PVC value corresponding to m. the pigment concentration would vary with the relative tinting strength of the test pigment. The summary of computational steps also shows how the measured CIE tristimulus values of the reference are converted to the CIE tristimulus values at matching. An example in the form of spectral reflection curves for reducing whites is presented in Figures 8-3 and 8-4. In the first case, the curves are for equal masses of test and reference; in the second, the curves are plotted after lightness matching. Finally, Figure 8-5 is a printout of a tinting strength determination. For most purposes, the use of the zero-th approximation to obtain the tinting strength as described here is entirely adequate ± for example, for production control. If there should be a need for a comparison between inorganic pigments with high light scattering power or a very great difference in tinting strength, so that more that +20 % departures from 100 % relative tinting strength occur, then the first approximation is recommended (Section 4.6.4, eq. 4.92). The factor a in equation (4.93) depends on the reference alone and can easily be determined once for all. * See ªHue, Relative, of Near White Specimensº in Appendix 1.

8.2 Relative Tinting Strength

329

Fig. 8-2. Flowchart for determination of relative tinting strength of black and inorganic colored pigments.

330

8 Determination of Tinting Strength and Lightening Power

Table 8-1. Formulas needed for calculating relative tinting strength and color difference after color reduction for inorganic colored and black pigments. ^ Y; ^ Z; ^ X^ R ; Y^ R ; Z^ R or R^ 0 ; R^ 0 ; R^ 0 ; R^ 0 ; R^ 0 ; R^ 0 Given: X; x y z x;R y;R z;R R^

R^

0:04

1 F^

;

0:36 0:6 R^

^ n where 1) R^ X=X ^ 2) Y=100 ^ 3) Z=Zn 4) X^ R =Xn 5) Y^ R =100 6) Z^ R =Zn P 0

F^Y F^Y;R

R^ 2 2 R^

eqs. (4.95), (4.61)

R^ X^ =Xn F^ F^X 0:782R^ 0x 0:198R^ 0z =98 R^ y =100 Y^ =100 F^Y ^ ^ F^Z Rz =100 Z =Zn F^X;R 0:782R^ 0x;R 0:198R^ z;R =98 X^ B =Xn R^ y;R =100 Y^ R =100 F^Y;R F^Z;R R^ 0z;R =100 Z^ R =Zn

or P 1 f^ 1 a f^

F^Y FWP with f^ F^Y;R FWP

1

(a is determined experimentally) q ^ R F^R P F^B P 2 ; R 1 FR P

eqs. (4.92, 4.93, 4.94)

0:384 R R 1 0:6 R R

RR 0:04

eqs. (4.111), (4.112)

where 1) F^R F^X;R R RR XR =Xn R XR =Xn 2) F^Y;R YR =100 YR =100 3) F^Z;R ZR =Zn ZR =Zn

Two cases: A) R ^ 0.008856

B) R > 0.008856 p R 3 R

R 7.787 R + 0.138 where 1) 2) 3) 4) 5) 6)

a 500 X where 1) X 2) Da aT DEab

eq. (2.5)

^ n R X R X=X T ^ Y=100 YT ^ n Z=Z ZT XR =Xn XR YR =100 YR ZR =Zn ZR

Y ; XT XR

aR ;

b 200 Y Y

YT YR

Db bT

Z bR ;

Z ; ZT ZR

a

L 116 Y aT aR

DL LT

b

LR ;

p Da2 Db2 DL2

DCab

q 2 a2 T bT

L

eq. (2.7)

LT LR eq. (2.11)

eq. (2.12)

Dhab Arctan DHab

16

eq. (2.10)

q 2 a2 R bR

bT b Arctan R aT aR q 2 2 2 DEab DL DCab

bT bR

eq. (2.14) (same sign as Dhab)

eq. (2.13)

8.2 Relative Tinting Strength

331

Fig. 8-3. Spectral reflectance of two red iron oxide pigments in reducing white (equal added pigment masses).

Fig. 8-4. Example from Fig. 8-3 after Y matching.

332

8 Determination of Tinting Strength and Lightening Power

Program ªP(REL)º Relative Tinting Strength by means of lightness matching, according to ISO 787-24 (modified) ******************************************************************* Date: ..-..-.. Standard is A Test is B Medium and white paste: according to ISO 787-24 Colorimeter, Standard Observer: N.N., C/28 Measuring conditions: d/8 (incl) Input: ************************************************************** Masses: White paste: 3 g Pigment: .12 g Reflectometer values: Reference: Test: R'(x) 47.74 47.02 R'(y) 41.03 39.93 R'(z) 39.68 38.18 Output: ************************************************************* Relative Tinting Strength: P = 108 % Tinting Equivalent: 1/P = 93% CIELAB Coordinates after matching: Reference: Test: a* = 15.0 15.7 b* = 1.7 2.2 L* = 69.4 69.4 Color difference after reduction: Delta(E*(ab)) = .9 Delta(L*) = .0 Delta(C*(ab)) = .8 Delta(H*(ab)) = .4 Delta(h(ab)) = 1.58 Fig. 8-5. Relative tinting strength of a red iron oxide pigment by lightness matching.

The accuracy with which tinting strength and color difference after color reduction are determined for inorganic pigments can be improved somewhat with a recent method (DIN 55 603). the method is again based on Y-matching, but now the principle of spectral evaluation is employed.

8.2.3 Organic Pigments (ªFIAFº Method Based on Principle of Spectral Evaluation) The principles of this section were established by Gall (see [19], [23] in Section 4.10), whose work has become the basis for standards*. The German standard defines ªstandard color depthsº and gives a procedure for the preparation of color depth standards (i. e., color samples of known standard color depth); these are used * See ªTinting Strength, Relativeº and ªColor Depthº in Appendix 1.

8.2 Relative Tinting Strength

333

as controls in both visual and colorimetric matching. The same standard provides instructions for bringing about the standard color depth in color samples. We follow the standards in determining the relative tinting strength of organic colored pigments and in describing Gall's ªFIAFº method, a computer-aided method of colorimetric tinting strength determination by iterative color depth matching based on the principle of spectral evaluation*. The color depth standards are available commercially; they should be calibrated, that is, they should indicate the CIE tristimulus values and the color depth parameter B = DTS (deviation from the color depth level), measured in the prescribed way. The visual adjustment of color samples to a given color depth level is of secondary importance in practice, so only the colorimetric technique needs explanation here. The color depth standards are necessary when results from different instruments or different laboratories are to be compared. Corrections to the measured CIE tristimulus values with respect to the nominal values of the calibrated standards take the form of ratios: Xcorr = (XS /XM) 7 X, where XS is the nominal value for calibration and XM is the value measured on the standard (and similarly for Y and Z). Ordinary paint bases (white enamels) are used as test media (see Section 8.2.4 for examples); naturally, pastes can also be used as in Section 8.2.2. Gall's method is contrasted to the method based on Y matching described in Section 8.2.2, where on Y value was specified and the second was adjusted; in the color depth matching method, both reducing whites (test and reference) must be adjusted to the specified color depth level**. The ratio of the masses of pigment required are input to the fundamental equation (4.75), which gives the relative tinting strength. The formulas needed for this procedure were already introduced in Section 4.5.6. The method results in the value DTS = B of a selected standard color depth being made equal to zero for test and reference through variation of the amounts of pigment added to the white paste. Now it is possible to describe Gall's FIAF method, which functions on the principle of spectral evaluation. A flowchart is shown in Figure 8-6. From the input reflection spectrum R (l) at 16 chosen wavelengths (20 nm intervals), the computer calculates the CIE tristimulus values X, Y, Z, the CIE chromaticity coordinates x, y, and thence DTS . A check is then made in order to see whether DTS = 0 to a sufficiently good approximation. If not, the mass-referred spectral Kubelka-Munk function F/m are calculated from the Saunderson-corrected reflection spectrum, then multiplied by a appropriately modified mass of pigment. From the result, the new CIE tristimulus values and DTS are calculated. This loop is repeated until DTS = 0. As a rule, two to four times around the loop will be required; five may be needed in quite rare cases. Once the target match for test and reference has been found, the * The letters FIAF stand for the German phrase ªFarbstårke durch iterativen Angleich der Farbtiefenº, with the meaning stated above. ** Schmelzer and co-workers propose the following departure from the standard: Test and reference are adjusted to the same (nonzero) value of B. Drawback: It is not possible to report the standard color depth level (SDS).

334 8 Determination of Tinting Strength and Lightening Power

Fig. 8-6. Flowchart of FIAF program for calculating relative tinting strength and color difference after color reduction by Galls method.

8.2 Relative Tinting Strength

335

tinting strength is output as the ratio of the two masses (along with the tinting strength equivalent if appropriate); in addition, the color difference after color reduction and the lightness, chroma, and hue differences are included in the output. Table 8-2 lists the needed equations as an aid to programming. A problem is presented by the a (j) factors (see Section 4.6.5): The standard includes long tables for ªmanualº searching and calculating. Gall and Friedrichsen have written convenient formulas for computer calculations based on third-degree polynominals; these are excerpted here for 1/1, 1/3, 1/9, 1/25, and 1/200 SDS and for illuminant/observer combinations C/28 and D65/108 (Tables 8-3 and 8-4), so that there is no need to reproduce the full tables. The formula for calculation is a(j) a(j0) + K1 W + K2 W 2 + K3 W 3 where W = (j ± j0)/100. A flowchart for the computer calculation is shown in Figure 8-7; the coefficients of the polynomials (tabulated values) must be stored in the computer memory. Figure 8-8 gives a printout by way of example. Two blue pigments were tested; the resulting value of the relative tinting strength is around 126 %. The example is instructive in that a relative tinting strength based on lightness matching can also be determined from these data. It is only 117 %; thus, less of the reference pigment would have to be added for matching. But this also means that the color difference after color reduction will change. It is found that DE ab is smaller than in the color depth matching method. The difference can be attributed primarily to a smaller chroma difference (saturation); the hue difference, on the other hand, is larger. These results imply that a greater difference in nuance is accepted when lightness matching is employed, even though in the case of color depth matching this larger difference would be perceived as interfering. This may indicate that questions of color formulation must be accorded more weight in color depth matching, while lightness differences are more significant in the case of Y matching. As Table 8-2 and equation 4.64 show, the zero-th approximation is employed in calculating the relative tinting strength. This is justified even for higher pigment concentrations, since organic pigments commonly have a lower refractive index (in the neighborhood of 1) and thus only slight light-scattering power. Thus the use of the zero-th approximation is proper even outside the Beer's law range, and therefore even at high relative tinting strength values differing by more than +20 % from 100 % ± as in the example. For organic black pigments, it is desirable to employ Y matching; the procedure of Section 8.2.2 can thus be used. Another method (ISO 787-26) has gained acceptance for organic pigments along with the FIAF method. The tinting strength is quantified as the sum of the colorimetrically evaluated Kubelka-Munk function F x,y,z (see eq. 4.77). This quantity is matched in a similar way to the Y value as described in Section 4.6.4. The formulas of Figure 8-2 and Table 8-1 can be used provided the tinting strength criterion just identified is employed.

336

8 Determination of Tinting Strength and Lightening Power

Table 8-2. Formulas needed for calculating relative tinting strength and color difference after color reduction for organic colored pigments. Given: R (l), RR (l) with 16 chosen wavelengths spaced 20 nm apart X Y Z x

R

x l R l dl

R R

y l R l dl z l R l dl

(2.3)

X ; X Y Z

y

Y X Y Z

(2.4)

q s 10 x xn 2 y yn 2 j Arctan

y x

yn xn

(4.100)

a(j) from subroutine, Fig. 8-7, Tables 8-3 and 8-4 DTS

p Y s a j

b 1 19 ; 1

R l F l f l

10 bi

b 1 29 ; 3

b 1 41 ; 9

(4.99) b 1 56 ; 25

b

1 200

73

R l 0:04 0:36 0:6 R l 1

(3.11)

R l2 2 R l

(3.117)

F l m

(4.64)

m i1 m i 0:9DTS

(4.101)

f l m i1 F l

(4.64)

R l 1 F l R l

p F l F l 2

(3.116)

0:384 R l 0:04 1 0:6 R l

(3.10)

Iteration yields mend ; hence mend ! Fend l ! Rend l ! Rend l ! X; Y; Z : Hence a , b , L and aR , BR , LR and hence DE ab , DC ab , Dhab, DH ab

) as in Tab. 8-1

For black pigments: shade difference after color reduction as in Table 8-7.

8.2 Relative Tinting Strength

337

Table 8-3. Polynomial coefficients for calculating the a (j) factors in the determination of DTS, standard illuminant C,28 observer. Range

j8

a (j)

K1

K2

K3

1/1 SDS

1 2 3 4 5 6 7 8

0 56 88 200 228 244 328 344

2.1620 3.7730 3.8850 2.6205 1.7110 1.1170 2.1700 2.0510

2.1146 2.2982 ±1.4047 ±0.71265 ±2.5648 3.6796 ±1.0190 ±1.4617

5.6685 ±11.750 0.86005 ±7.2510 ±57.746 ±4.1844 4.7036 15.468

±7.6914 17.685 ±0.54797 ±6.4238 316.03 1.5426 ±18.645 ±12.263

1/3 SDS

1 2 3 4 5 6 7 8 9

0 52 156 188 216 252 276 308 344

1.9710 3.5230 3.4910 2.8560 2.1300 0.7710 2.1770 2.4000 2.2240

1.8854 0.56964 ±0.36932 ±2.8126 ±2.7444 ±0.42114 2.7983 ±0.49271 ±2.9558

7.2139 ±0.97366 ±5.5142 ±2.3760 ±25.405 70.0632 ±12.018 3.1561 ±5.1289

±9.8081 0.38087 1.4815 11.254 62.615 ±182.87 17.020 ±8.7220 85.152

1/9 SDS

1 2 3 4 5 6 7 8

0 48 92 188 224 244 288 344

2.3380 3.5020 4.0690 3.0610 1.7010 1.0100 2.5250 2.7690

±0.89972 5.2484 ±0.36496 ±1.7819 ±5.8311 4.6563 1.5168 ±0.85358

11.961 ±17.432 0.64710 ±3.7832 14.461 ±0.21240 ±1.5772 ±31.714

±10.490 19.165 ±1.4171 4.8936 ±12.941 5.7842 ±0.63062 125.77

1/25 SDS

1 2 3 4 5 6 7 8 9 10

0 24 44 72 104 144 196 220 236 296

2.3990 2.4540 3.7250 4.1260 4.7880 4.6710 3.2310 1.9640 1.2040 2.9080

±3.0667 6.0507 6.8347 ±0.30389 3.5030 ±1.6006 ±3.9918 ±8.6798 3.0071 0.41689

16.380 19.039 ±38.741 5.6079 ±17.579 ±3.7578 ±3.5840 27.377 4.0166 ±1.0629

±10.999 ±87.763 69.481 5.6553 20.218 2.9038 ±7.4141 ±17.633 ±7.1562 ±1.2985

1/200 SDS

1 2 3 4 5 6 7 8 9 10 11 12 13

0 20 56 88 104 140 196 216 232 248 264 304 344

5.7810 4.0900 4.0750 6.2600 6.9570 6.8870 5.0030 3.5420 3.4160 5.3360 6.8390 7.5100 7.0040

±8.2288 ±6.2950 3.9274 6.7537 2.3532 ±2.5572 ±4.1350 ±4.1230 0.28516 19.078 4.3458 ±1.0073 ±5.1011

±7.5625 27.716 13.590 ±11.422 ±12.454 4.1401 ±31.582 16.913 121.20 ±110.38 ±12.814 1.2544 ±17.707

32.188 ±28.732 ±14.148 ±22.258 14.924 ±9.9624 78.570 24.602 ±299.69 311.44 15.352 ±4.7446 10.250

338

8 Determination of Tinting Strength and Lightening Power

Table 8-4. Polynomial coefficients for calculating the a (j) factors in the determination of DTS, standard illuminant D65, 108 observer. Range

j8

a (j)

K1

K2

K3

1/1 SDS

1 2 3 4 5 6 7

0 60 156 224 240 268 340

2.250 3.973 3.127 1.987 1.285 2.185 2.142

1.85034 1.51213 ±1.21851 ±4.00696 7.42688 0.822426 ±1.032

8.68115 ±6.23596 5.39038 ±47.8125 ±17.5547 0.741241 8.05627

±11.6328 3.89874 ±8.91809 284.023 8.95508 ±2.73209 ±0.828125

1/3 SDS

1 2 3 4 5 6 7 8

0 52 140 196 236 252 276 340

2.040 3.669 3.524 2.710 1.101 1.351 2.504 2.319

1.8064 1.4459 1.21893 ±0.562195 ±4.18735 7.98462 1.54935 ±2.57889

9.15625 ±3.59046 ±8.80359 ±9.45264 16.9717 ±9.83203 ±3.91061 ±4.03809

±12.6865 2.00006 7.20239 1.99219 118.672 ±14.2773 1.62125 50.0312

1/9 SDS

1 2 3 4 5 6 7

0 52 148 224 244 280 336

2.345 3.94 3.864 1.756 1.438 2.785 2.932

±0.634155 2.40570 ±1.28906 ±4.93951 5.80115 1.67851 ±1.5271

11.2192 ±4.96634 1.00537 ±20.8896 ±1.04980 ±3.35052 ±15.6045

±7.88379 2.47712 ±3.8938 188.117 ±12.9629 1.46381 49.1836

1/25 SDS

1 2 3 4 5 6 7 8

0 28 56 96 148 224 244 292

2.36 3.035 4.1268 4.7271 4.636 1.6873 1.8945 3.1622

±3.05167 8.93835 ±0.28082 2.57528 ±2.0782 ±5.801 6.0961 0.66899

11.0864 ±15.2949 5.0835 ±6.64651 0.12793 28.7262 ±8.30859 ±3.24585

1/200 SDS

1 2 3 4 5 6 7 8

0 28 80 120 208 232 248 280

5.68 3.646 6.203 7.464 4.17 3.555 6.779 7.935

±9.19458 ±0.990845 14.1318 ±1.57855 ±8.99036 4.26904 10.6932 ±0.109528

±19.9785 12.063 ±49.8843 1.25879 23.0088 215.078 ±40.9404 0.637939

30.0801 ±9.64844 ±1.5747 2.61005 ±3.27197 27.2941 2.31348 0.796387 95.9844 ±1.34961 56.0981 ±4.22656 15.7344 ±723.844 58.8066 ±5.00452

8.2 Relative Tinting Strength

339

Fig. 8-7. Flowchart for computer calculation of DTS (after Gall and Friedrichsen).

340

8 Determination of Tinting Strength and Lightening Power

Program ªFIAFº Relative Tinting Strength by means of Color Depth matching, according to DIN 53235 and 55986 ******************** Date: ..-..-.. Color Depth level: 1/3 ST Standard is A Test is B Medium and white paste according to ISO 787-24 Colorimeter, Standard Observer: N.N., C/28 Measurement Conditions: d/8 (incl) Input: ******************************************* Masses: White paste: 3 g Pigment: .3 g Spectral Reflectances: on-line colorimeter Output:****************************************** Relative Tinting Strength: P = 126 % Tinting Equivalent: 1/P = 80 % CIELAB Coordinates of 1/3 ST: Reference: Test: a* = ±10.5 ±11.2 b* = ±27.8 ±28.2 L* = 72.4 73.0 Color Difference after reduction: Delta(E*(ab)) = 1.1 Delta(L*) = .6 Delta(C*(ab)) = .7 Delta(H*(ab)) = ±.6 Delta(h(ab)) = ±1.18 Fig. 8-8. Relative tinting strength of a blue pigment by color depth matching (FIAF method) (computer output).

8.2.4 Change in Tinting Strength Test methods are set forth in the standard* for lacquer binding media and plastics. Test and reference pigments are dispersed in agreed-on vehicles in accordance with agreed-on conditions. Methods and vehicles listed in Section 6.2.1 are recommended. From the mill base, samples are taken after specified dispersion stages and mixed with a white paint (same vehicle) or with a specified white paste. The reflectances are then measured, and the Kubelka-Munk function F of the test and reference mixtures are calculated from the results. The standard still prescribes R (l) (min) as the tinting strength criterion; that is, the F value is to be determined at the reflection minimum (i. e., the absorption maximum). It goes without saying that different criteria (in particular the CIE tristimulus value Y) can be employed as agreed on. Along with an analytical balance and porcelain dishes, the method requires the following:

* See ªChange in Tinting Strengthº in Appendix 1.

8.2 Relative Tinting Strength

341

± Bird applicator or paint spray gun ± Substrate material (glass plates, sheet metal, cardboard; also paste film holders as discussed in Section 6.2.3) ± Perforated cardboard template (for covering in measurements on pastes) ± Spatula ± Automatic muller ± Colorimeter (spectral or tristimulus) ± Oven ± White paint (20 % TiO2) or white paste (40 % TiO2) made up with same vehicle as used in mill base The standard distinguishes between: ± Low-viscous mill bases ± High-viscous, pastelike mill bases Preparation method 1 for low-viscous mill bases Dispersing: generally with oscillatory shaking machine. Withdraw samples after fixed time intervals (initial sample after shortest dispersion time or stage, final sample after longest reasonable dispersion time or stage; tinting strength must reach at least 90 % of potential final value). Reducing white: Mix 3 g of ground mill base with such a quantity of white paint (generally 30 g) that a certain color quality as agreed on (an agreed-on color depth, according to the standard) is achieved. Application: Apply reducing whites to substrates with Bird applicator or spray gun. Check hiding of the coat with contrast cards and rub-out test (see Section 6.2.1). Preparation method 2 for high-viscous, pastelike mill bases Dispersing: generally with automatic muller, otherwise same as method 1. Reducing white: Mix 5 g of white paste with such a quantity of colored pigment paste (generally 0.1 to 0.5 g) that a certain color quality as agreed on (an agreed-on color depth according to the standard) is achieved. Disperse mixture in four stages of 25 revolutions in the automatic muller. After every stage, homogenize with spatula and collect toward center of plate. Application: Apply reducing whites to substrates with Bird applicator. Check hiding with contrast cards and rub-out test (see Section 6.2.1). Measurement and evaluation method Measure CIE tristimulus values Y (in the standard, reflectance at the absorption maximum), apply Saunderson correction, and calculate Kubelka-Munk functions F. use perforated template when measuring pastelike specimens. When rub-out effect is marked (i. e., DE ab > 10), measure the rubbed area. Plot F versus rubbing time or stages also plot the reciprocals 1/F versus 1/t in a Pigenot diagram.

342

8 Determination of Tinting Strength and Lightening Power

A practical example will now be described for the change in strength evaluated by the method of Section 4.7.3. A semitransparent iron oxide pigment was chosen. A planetary ball mill was used for dispersing; the method was that of ISO 8780-4 appropriately modified. Alkydal F 48 (Bayer AG) was selected as the vehicle, and formulation was carried out in accordance with DIN 53238-30. Mill bases with PVC values of 5 %, 7.5 % and 10 % were prepared, and samples were taken from these after, 5, 10, 20, 60, 120, and 240 min. The change in strength was determined experimentally as set forth in ISO 8781-1; the tinting strength determinations were done in accordance with ISO 787-24. For this purpose the samples taken from the mill base were incorporated into a stabilized white paste of Alkydal L 64 (Bayer AG), and the pastes were measured colorimetrically on the paste film holder (DIN 55893). The CIE tristimulus values Y were used in determining the Kubelka-Munk functions F and in the subsequent calculations. The initial and final values F0 and F1 were employed for the determination of the relative PVC values n (eq. 4.126). The 5 minute value was taken for F0 ; for F1, a value obtained from a nonlinear regression of 1/F over all measured values at t = 0 was employed (the Pigenot line yields an unusable value). The use of F0 as initial value shifts the time scale: the new 0 minute value is the old 5 minute value, so that the sampling times must now be associated with times t' = t ± 5, that is, 0 (= F0), 5, 15, 55, 115, and 235 min. Figure 8-9 shows the measured points for B and B / A obtained with eqs. (4.127) to (4.130); these define the lines (determined by curve fitting) that are also re-

Fig. 8-9. Parameters as a function of PVC.

8.2 Relative Tinting Strength

343

Fig. 8-10. Dispersion rate constants as a function of PVC.

Fig. 8-11. Dispersion curves: KUBELKA-MUNK functions (measure of the tinting strength) as a function of the dispersion time.

344

8 Determination of Tinting Strength and Lightening Power

quired by eq. (4.130). Next, eqs. (4.130) to (4.132) were used to calculate the variations of the three rate constants; Figure 8-10 presents the results. With the calculated constants, the F (t) curves representing the change of strength for the three mill bases were calculated with eqs. (4.124) and (4.126); the results are plotted in Figure 8-11. The calculated curves are in remarkably good agreement with the experimental points. To make the calculation traceable, at least in the second half, Table 8-5 lists the most important intermediate results. The end results in Table 8-6 are the rate constants and the half-value times. It should be noted that the dispersing resistance of a pigment is correctly described by the half-value time, while the increase in tinting strength IS (ISO 8781-1) is not appropriate for this purpose. These results yield new information about the dispersing resistance of pigments, which could not be acquired in any other way. First it should be stated that the halfvalue times, and thus the dispersing resistances, decrease with increasing PVC. But the most striking fact is that kk is negative. This can only mean that no size reduction of large particles on small ones occurs: the small particles are reagglomerating and thus becoming large particles again. The constant kg overrides the negative effect of kk , however, so that disintegration on the large particles themseleves is the dominant process. At low PVC, on the other hand, disintegration on the vessel wall and grinding bodies goes faster than disintegration on coarse particles; this result holds up to about 3 % PVC (Figure 8-10). The F (t) curves in Figure 8-11 show a steeper rise and a flatter final phase at higher PVC values, thus expressing the fact that the disintegration of large particles on other such particles, that is, the secondorder reaction, is intensified (as expected) and the other processes become less important as the PVC rises. The increase in strength IS as defined in ISO 8781-1 is not informative as to the dispersing process, and it is not worthwhile listing it as well. Table 8-5. Intermediate values. PVC

B/A

B

y1

y2

a, b, c

k'

5.0 % 7.5 % 10.0 %

0.0532 0.0779 0.0870

0.00817 0.00518 0.00073

0.0614 0.0830 0.0878

0.0450 0.0727 0.0863

a = 0.527 b = 0.03738 c = 0.901

k'g = 0.714 k'k = ±0.1868 k'w = 0.01892

Table 8-6. Final values PVC

kg [min±1]

kk [min±1]

kw [min±1]

t0,5 [min]

5.0 % 7.5 % 10.0 %

0.03571 0.0536 0.0714

±0.00934 ±0.01401 ±0.01868

0.01892 0.01892 0.01892

16.7 13.3 11.1

8.3 Lightening Power

8.3

345

Lightening Power

8.3.1 Graphical Method Instructions for the graphical method are provided in standards*. The determination is based on the lightening power as defined in equation (4.75): It is the mass of reference white pigment that, when added to a colored paste of stated composition, yields the same lightness as with the reference pigment. A calibration curve, showing the CIE tristimulus value Y for the reference colored paste as a function of PVC, is used in the evaluation. In order to determine the lightening power, one disperses the test pigment, at an agreed-on concentration, in a certain quantity of the agreed-on colored paste. In this way, what is measured is the CIE tristimulus value Y for the mixture with colored or black base. From the calibration curve (measured Y values versus white pigment PVC of reference), the nominal PVC is read off; this is the value that would give the same CIE tristimulus value Y. The lightening power is then obtained as the ratio of masses calculated from the two PVC values. It is useful to plot, over the calibration curve, the associated curve from which the lightening power can be read off directly. The method can be further simplified by plotting Y directly against the pigment mass (instead of the PVC). The lightening power curve then becomes a straight line. The standards present examples of lightening power determination by a gray paste method and a blue paste method. The composition of the black paste is chosen such that the concentration of the black pigment in the gray pastes remains constant for all PVC values; this corresponds to the constant volume method. Here we go through the example, but using the adding pigment method for simplicity; in this technique, the Y values are plotted directly against the added masses of white pigment, so that only one black paste has to be prepared. Aside from the analytical balance, spatula, doctor blade, and so forth, the following apparatus will be needed: ± ± ± ±

Triple-roll mill Automatic muller Colorimeter Measuring setup for measurements on pastes, such as the paste film holder of Section 6.2.3 Preparation method: First prepare master carbon black paste: Carefully stir by hand 18.7 g Flammruss 101 (Degussa) 81.3 g Alkydal L64 (Bayer)

* See ªLightening Power of White Pigmentsº and ªScattering Power, Gray Paste methodº in Appendix 1.

346

8 Determination of Tinting Strength and Lightening Power

and pass through the triple-roll mill six times. Composition of the black paste for, say, a PVC of 15 % of the reference (density R = 4.1 g/cm3): ± 91.72 g Alkydal L64 ± 5.11 g Aerosil 200 (Degussa) ± 3.17 g master carbon black paste (see above) For other black paste compositions for other test PVC values or other pigment densities, see Table 8-7. Table 8-7. Compositions of black pastes. Pigment volume concentration (PVC)

Composition of black paste, g Alkydal Aerosil L 64 200 g g

Carbon black paste (Section 8.3.1)

Volume of white pigment per 2.50 g black paste (cm3)

5% 6% 7% 8% 9% 10 % 11% 12 % 13 % 14 % 15 % 16 % 17 % 18 % 19 % 20 % 21% 22 % 23 % 24 % 25 %

92.04 92.02 91.98 91.95 91.92 91.89 91.86 91.82 91.79 91.75 91.72 91.68 91.64 91.60 91.56 91.52 91.48 91.43 91.39 91.34 91.30

2.84 2.87 2.90 2.93 2.96 2.99 3.03 3.06 3.10 3.13 3.17 3.21 3.25 3.29 3.33 3.37 3.41 3.45 3.50 3.54 3.59

0.123 0.149 0.176 0.203 0.251 0.259 0.288 0.318 0.349 0.380 0.412 0.444 0.478 0.512 0.547 0.583 0.620 0.658 0.697 0.737 0.777

5.12 5.12 5.12 5.12 5.12 5.12 5.12 5.12 5.12 5.11 5.11 5.11 5.11 5.11 5.11 5.11 5.11 5.11 5.11 5.11 5.11

In order to generate the calibration curve of the reference, add increasing masses of white pigment to equal masses of black paste and place on the lower plate of the automatic muller. After mixing, distribute in the form of a circular ring. Mull in four stages of 25 revolutions each, under pressure of 1.5 N/cm2. After each stage, rehomogenize and redistribute. Prepare and measure each calibration paste twice.

8.3 Lightening Power

347

Testing method: Mix together 2.5 g of black paste and 1.684 g of test pigment, using the method described above. Measure the CIE tristimulus value Y of the resulting gray paste. From the calibration curve, read off the mass to be added such that the reference will exhibit the same Y value as the test. The calibration diagram for the example is shown in Figure 8-12 along with the lightening power line. From the curve it can be inferred that a reference quantity of 1.250 g corresponds to the Y value of the test, so that the lightening power is Pw = 1.250/1.684 = 74%. This value is also read directly off on the upper line. Figure 8-12 further contains the CIE tristimulus value X and Z of the reference, measured at the same time. With their help, the X and Z values of the reference at matching can be read off; these can be further analyzed together with the measured test tristimulus value in order to obtain the shade difference after color reduction (see Section 2.3.3). If the calibration curve were plotted as Y versus the logarithm of the added mass (instead of versus the mass itself), a straight line would again be obtained in the Beer's law range of PVC, according to equations (3.118) and (4.49). Such a calibration line is the basis for Grassmann and Clausen's method of determining the lightening power (see Section 4.8). It has been shown that the increase in the scattering interaction outside the Beer's law range (see Fig. 4-20) means no linear variation of lightening power with PVC can be expected. The advantage of the standard method is that it permits light-

Fig. 8-12. (Bottom) Calibration curve for Y with CIE tristimulus values X and Z. (Top) Lightening power versus added pigment mass of reference.

348

8 Determination of Tinting Strength and Lightening Power

ening power (and shade difference after color reduction) to be determined as a function of the PVC of the reference pigment. For this purpose, a special black paste as characterized in Table 8-7 must be prepared from the master carbon black paste for every new PVC. The procedure described above ± recording of a calibration curve, etc. ± must then be repeated for every PVC. It is clear that the method of determination needs a good deal of rationalization. This is the subject of the sections that follow.

8.3.2 Rationalized Method The method is described in the standards*. The Kubelka-Munk function is used for rationalization. As in Section 8.2.1, gray pastes with equal added masses of white pigment are prepared and their CIE tristimulus values Y are measured. After Saunderson correction of the Y values (eq. 4.112), the Kubelka-Munk functions F (eq. 3.117) are calculated for the reference and test. The ratio of scattering coefficients per unit pigment mass concentration then gives the relative scattering coefficient of the test pigment per unit mass (eq. 4.106). This is identical with lightening power, but only in the Beer's law range. The relative scattering coefficient itself is usually better stated in terms of volume; the conversion from the mass-referred quantity is easily given by the reference/test density ratio (eq. 4.103). When relative scattering coefficients obtained by this method are compared with those from the black-ground method of Section 7.2.1, the unlike nature of the methods means that complete agreement cannot always be expected. The apparatus and materials for this test are as listed in Section 8.3.1, and the same master carbon black paste is again prepared. The ISO standard describes the analysis at a fixed test PVC of 17 %; the German standard allows other PVC values, and it includes a table giving the required paste compositions for PVC values in 1% steps from 5 % to 25 % (see Table 8-7). In parallel to the lightening power, the shade difference after lightening power matching can also be calculated from the pigment mass added to match. The formulas for this calculation are collected in Table 8-8 as a programming aid. A printout of results appears in Figure 8-13. This method can be employed only in the Beer's law range; at higher pigment concentrations, the values contain errors, that is, they no longer agree with the values obtained by the Y matching method of Section 8.3.1. In such cases, it is necessary to use the first approximation of the lightening power, equation (4.105). This means that aw must be determined; it contains pigment data for the reference alone. The coefficient gR of the scattering interaction of the reference white pigment occurs in it. This is expediently determined by using the dilution method (see section 4.4.1), or simply from two gray mixtures containing quantities of the reference * See ªLightening Power of White Pigmentsº and ªScattering Power, Relative, Gray Paste Methodº in Appendix 1.

8.3 Lightening Power

349

Table 8-8. Formulas needed to calculate lightening power and shade difference after lightening power matching in the Beer's law range. ^ Y; ^ Z^ and X^ R ; Y^ R ; Z^ R for equal added pigment masses m^ Given: X; R^ 1 F^

R^

0:04

(4.112)

0:36 0:6 R^ R^ 2 2 R^

(3.117)

^ where 1) R^ Y=100 2) X^ R =Xn 3) Y^ R =100 4) Z^ R =Zn Pw

R^ Y^ =100 X^ R =Xn Y^ R =100 Z^ R =Zn

F^ F^Y F^X;R F^Y;R F^Z;R

F^Y;R F^Y

(4.106)

FX;R F^X;R Pw ;

FZ;R F^Z;R Pw

(4.67)

Then continue as in Table 8-1 (eqs. 4.111ff.). The CIELAB coordinates are substituted in the formulas for shade difference after color lightening power matching: Ds

p Da2 Db2 ;

Dj Arctan

Db Da

(2.16)

From Table 2-3, Dj ? nature of undertone.

that differ as widely as possible; in this case, two expressions are obtained from equation (4.48) (we now drop the subscript R): 2 1 1 3 (8.3) z1 c1 1 z 5 c1 j1 F1 FBP 3 2 1 1 3 j2 z1 c2 1 z 5 c2 F2 FBP 3 and thence g z5 3

j1 c2

j2 c1

j1 c2

j2 c1

5 3

(8.4)

5 3

The desired factor aw is calculated with equation (4.105): 2

aw g c^ 3

where

m^ c^ m

and m mBP

R RBP

350

8 Determination of Tinting Strength and Lightening Power

Program ªLPº Lightening Power, according to ISO 787-24 ********** Date: ..-..-.. Reference is A Test is B Medium and black paste: according to ISO 787-24 Colorimeter/Standard Observer: N.N., C/28 Measuring Conditions: d/8 (incl) Input:**************************************** Masses: Black paste: 2.5 g Pigment: 2.0 g Reflectometer values: Reference: Test: R'(x) 46.88 46.81 R'(y) 48.08 48.79 R'(z) 52.50 55.84 Output:************************************** Lightening Power: 105 % Lightness: 74.9 Color Difference after matching Type: Magnitude: blue Delta(s) = 2.8 Fig. 8-13. Lightening power and shade difference after lightening power matching for a white pigment, obtained by the rationalized method (computer output).

As a computational example, the values from Annex 1 of the German standard can be used again: m1 = 0.520 g, m6 = 2.062 g, Y1 = 32.6, Y6 = 50.4. The transformations made are, first the Saunderson correction (Y ? Y ++) and, second, the calculation of the Kubelka-Munk functions (Y ++ ? F); see Table 8-8 for the formulas: Y1++/100 (32.6/100 ± 0.04)/(0.36 + 0.6 7 32.6/100) = 0.515 Y++ 6 /100 0.700 1/F1 2 7 0.515/(1 ± 0.515)2 4.372 1/F6 15.61. Now, with 1/FBP = 0.027, equation (8.3) gives j1 = 4.372 ± 0.027 = 4.35 and j2 = 15.59. Given mBP = 3 g, RBP = 1.285 g/cm3, R = 4.1 g/cm3, and m = 3 7 4.1/ 1.285 = 9.57 g, the PMV values are found to be c1 = 0.520/9.57 = 0.0543 and c6 = 0.2155. By equation (8.4), then, g = (4.35 7 0.2155 ± 15.59 7 0.0543)/ (4.35 7 0.21555/3 ± 15.59 7 0.05435/3) = 0.422. Finally, with m^ = 1.689 g, equation (4.105) yields aw = 0.422(11.689/9.57)2/3 = 0.1328. In the DIN example (see Fig. 8-12), the mixture of the test gray paste has a CIE tristimulus value Y = 44.0. If the associated F value is substituted in equation (4.105) together with the value just calculated for aw, the result is a lightening power of P(1) w = 74 % ± in extremely good agreement with the graphical solution (whereas the zero-th approximation

8.3 Lightening Power

351

would have given P(0) w = 76 %). Thus the example shows that the first approximation still supplies correct values far away from 100 % lightening power. If X and Z (or R'x and R'z ) are measured at the same time, then from any pair of values (X1, X6 and Z1, Z6) the coefficients zX1, zX5/3 and zZ1, zZ5/3 of the KubelkaMunk functions FX and FZ of the reference can be caluclated with equation (4.109). Thus the CIE tristimulus values XR and ZR of the reference at matching are accessible, and from these together with X, Z of the test, the shade difference after lightening power matching can be determined. Even with this new method, a black paste must be mixed for every new PVC, and new gray mixtures must be prepared. Section 8.3.3 will show how the entire curve of lightening power versus PVC can be obtained from a single gray mixture.

8.3.3 PVC Dependence from One Gray Mixture This method requires only a single mixture of pigment with black paste but yields values for the lightening power throughout the PVC range of interest. The key to the method is a rather simple relation with which the dilution method (Section 4.4.1) can be used to obtain the coefficient zw5/3 = g (eq. 4.52). Accordingly, one need only dilute the initial gray paste in a known ratio with additional vehicle ± i. e., the black paste without black pigment ± in order to calculate g from the two Kubelka-Munk functions. This test can be performed much more quickly than any of the determinations that have been discussed, because the pacing step is mixing in the automatic muller. All that is required for dilution is more stirring. One of the preparation methods set forth above can be employed for the preparation of the starting mixture. The algorithm uses equations (4.51) and (4.52) to calculate g, then equation (4.48) to calculate the other coefficient z1. If both coefficients are known for both test and reference, equation (4.102) can be used with pw1 = 0 to draw or plot the full curve of lightening power versus PVC. Table 8-9 lists out the formulas needed for programming, and Figure 8-14 shows a flowchart for the procedure. The data needed for the dilution require some separate calculations; these are also described in Table 8-9. First, the volumetric dilution factor qD = s/ sA is fixed. The volume ratio of white pigment/black paste mixture (ªgray pasteº, subscript GP) VGP to medium VM to be added is then derived from sA = V/VGP and s = V/(VGP + VM), where V is the volume of white pigment: VM 1 VGP qD and mM mGP

RM RGP

1

1 qD

1

(8.5)

352

8 Determination of Tinting Strength and Lightening Power

Table 8-9. Formulas needed for calculation of lightening power and shade difference after lightening power matching as functions of PVC. Given: c^ A ; X^ A ; Y^ A ; Z^ A ^ X; ^ Y; ^ Z^ c;

before dilution

of test and reference (subscript R)

after dilution

Saunderson correction and calculation of Kubelka-Munk functions of all values with equations (4.112) and (3.117), (see Table 8-8): gY

1

F^Y;A

F^Y;A 2

sA3

F^Y 2

s3

where s

c 1c

(4.51), (4.52)

similarly gX, gZ of test and reference: jA

1 FY;A

1 ; FBP

zY1

jA cA 1

(4.48)

2

gY cA3

similarly zX1 , zZ1 of test and reference: pwo

zY1 ; zY1;R

P 1 w

RR pw0 1 R

1 FX;A 1 FZ;A

pw 2 gY 3

2

3 pwo gY;R

pw1 0

(4.104)

s 2 3 1 s 3 1 s s 23 1 1 g zX1 P 1 P X w w FBP 1 s 1 s 1 s s 23 1 1 g zZ1 P 1 P Z w w FBP 1 s 1 s pw 2

(4.102) (4.109) (4.66)

Then continue as in Table 8-1 (eqs. 4.111 ff.). The CIELAB coordinates are analyzed to give shade difference after lightening power matching, as in Table 8-8 (eq. 2.16 and Table 2-3). Lightening power and shade difference after lightening power matching can be plotted (manually or by computer) versus s. Dilution data: If sA is to be lowered to s by dilution, the volumetric dilution factor is qV = s/sA. The following must then be calculated: m mSP w

R 4:4 ; RBP

m 4:1 ; m mBP

c

m 4:6 ; m

RGP

s

Rs 4:17 ; w

c 1c mM mGP

(4.15) RM RGP

1 qD

1

(8.5)

8.3 Lightening Power

353

Fig. 8-14. Flowchart for determining lightening power and shade difference after lightening power matching as functions of PVC from a single gray mixture.

354

8 Determination of Tinting Strength and Lightening Power

To convert columes to masses, the density of the gray paste must be known. It can be found in the following way: First, the PVM m (eq. 4.4) and thence, with the PMV c (eq. 4.6), the PVC s in the gray paste are calculated (eq. 4.15). Together with the PMP w, equation (4.1), the density RGP of the gray paste is then obtained with equation (4.17). The prodecure can be illustrated by an example. The starting values are as follows: m = 5 g, mBP = 6.5 g, R = 3.957 g/cm3, RBP = 1.286 g/cm3. Then m = 6.5 7 3.957/1.286 = 20.00 g, c = 5/20 = 0.2500, s = 0.25/(1 + 0.25) = 0.200, w = 5/(5 + 6.5) = 0.435, RGP = 3.957 7 0.2/0.435 = 1.819 g/cm3. If the PVC is to be reduced from 20 % to 0.5 % by dilution, qD = 0.005/0.2 = 0.025. The mass of med-

Fig. 8-15. Lightening power versus PVC for three rutile pigments (series 1).

Fig. 8-16. Lightening power versus PVC for three rutile pigments (series 2).

8.3 Lightening Power

355

ium required for 0.5 g of gray paste is then obtained from equation (8.5): mM = (0.5 7 1.231/1.839) 7 (1/0.025 ± 1) = 13.05 g. Figures 8-15 and 8-16 give plotted curves of lightening power versus PVC for a total of six white pigments, all against the same reference. The curves show that pigments initally having a better relative lightening power may well become worse at higher PVC, and vice versa. It should be kept in mind that lightening power values for PVC s 4 30 % do not necessarily represent reality, because of the possibility of a pigment concentration exceeding the critical PVC. In calculating the shade difference after lightening power matching, one proceeds in an analogous way. Again, equations (4.52) and (4.109) are used to calculate g and z1 from the Kubelka-Munk functions of the CIE tristimulus values X and ^ w is substituted in the equations. Similarly to Z, and the mass added at matching mP what was done in Table 8-1 and 8-7, the strength and nature of the undertone are then inferred; they can also be plotted in suitable form as functions of the PVC. This test can be performed in less than 20 minutes (up to plotting of the curves). At our current level of knowledge, an interim goal ± a more rational test for lightening power has thus been attained with the method just described.

Appendix 1 Listing of Standards Key words Change in tinting strength (see Dispersion and PVC) Coating materials, terms and definitions

ISO

ASTM

BS

NF

JIS

DIN

4618-1 to 4

D 16

2015

T 36-001 T 36-005

K 5500

Color depth Color differences: CIELAB

55945 EN ISO 4618-2 to -4 EN 971-1 53235-1 to 2

7724-3

D 1729 D 2244 E 308

3900-D10

T 36-004-3

K 5600-4-6

6174

T 36-004-2

K 5600-4-5

6176 53236 55600

CIE94 CMC DIN99 Conditions/evaluation of measurement Significance Color in full-shade systems: Black pigments Colored pigments White pigments Color matching Color matching functions in steps of 20 nm Color measurement (see also Color differences) Color tolerances for automotive paints Colorimetry Coloring materials: Classification

7724-6 7724-4

6923

7724-2 787-25 787-25 787-25 3668 7724-2 7724-1 to 6 7724-2

3900-D9 D 3022 D 3022 D 2805

3900-D1

T 30-061

K 5400

E 308 E 259 E 308

4764 3900-D8 3900-D9

T 36-004-1 T 36-004-2

K 5600-4-4 K 5600-4-5

55985-2 55985 55983 6173-1 ISO 3668 53218 6175-1 to 2 5033-1 to 9 55944

Automatic muller Bead mill Change in gloss Change in tinting strength Fineness of grind (see below) High speed impeller mill Introduction Oscillatroy shaking machine Triple roll mill Emulsion paints Film thickness

8780-5 8780-4 8781-3 8781-1

Fineness of grind Gloss, measurement Hiding power: Color difference method Contrast ratio (opacity): of light-colored paints General introduction Pigmented media Wedge-shaped layer

787-23 787-10

ASTM

D 153

D 387

8780-3 8780-1 8780-2 8780-6

BS 2015

NF

JIS

EN ISO 787-23 EN ISO 787-23

T 31-201 T 31-202

K 5101

EN ISO 8780-5 EN ISO 8780-4 EN ISO 8781-3 EN ISO 8781-1

T 31-210-5 T 31-210-4 T 31-220-3 T 31-220-1

EN ISO 8780-3 EN ISO 8780-1 EN ISO 8780-2 EN ISO 8780-6

T 31-210-3 T 31-210-1 T 31-210-2 T 31-210-6

2808 1524 8781-2 2813 6504-4 6504-3 6504-0 6504-5

D 1210 D 523 D 5307

3900-C6 EN ISO 8781-2 3900-D5 EN ISO 2813

T 30-120 to 125 EN 21524 T 31-220-1 T 30-064

K 5101

K 5101 K 5400 K 5101 K 5400 K 5600-4-7

DIN 55943 EN ISO 787-10 EN ISO 787-1 6164-1 to 3 53238-30 53238-33 53238-31 53238-32 EN ISO 8780-5 EN ISO 8780-4 EN ISO 8781-3 EN ISO 8781-1 EN ISO 8780-3 EN ISO 8780-1 EN ISO 8780-2 EN ISO 8780-6 53778-3 EN ISO 2064 EN ISO 2808 EN 21524 EN ISO 8781-2 67530 EN ISO 2813

3900-D11 D 2805

3900-D7

55987 55601

Appendix 1

ISO 4618-1

358

Key words Terms and definitions Density of pigments: Centrifuge method Pyknometer method DIN Color System Dispersion, ease of: Alkyd resin and alkyd melamine system: Drying by oxidation: Stoving type

Key words White and light-colored paints White and light gray media Hue of near white specimens Hue relative of near white specimens Lightening power of white pigments Lightness: Emulsion paints (see above) White pigment powders Loss on ignition (Red iron oxide pigments) Metamerism index Mixtures, Composition Particle-size analysis Basic terms:

ASTM D 2805

BS 3900-D7

NF

7724-5 787-24

D 2745

3483-A5 EN ISO 787-24

T 30-023 T 31-228

1248

D 3721

3981

T 31-002

JIS

5775-6 13320-1 13319 13322 13321 9276-1 9276-2 9276-4

13318-1 to 3 13317-1 to 3 13323-1

ISO 13320-1 3406-1 to 9 ISO 13319 D 1366

D 3360

DIN 55984 55980 55981 53165 55982 53163 55913-1 6172 1310

3406-8

X 11-666-1 X 11-671 X 11-696 X 11-672

ISO 9276-1

X 11-632-1

66141 66144 66143 66145

Z 8820 T 30-044 Z 8822 X 11-685-1 to 3 X 11-680-1 to 3 Z 8821

66160 66111 66115

359

5036-1, 3 to 4 55678-1 to 3

Appendix 1

Electrical sensing zone Image analysis method Photon correlation spectroscopy Representation: Basic terms Logarith. normal diagram Power function grid RRSB grid Sedimentation methods: Balance method Basic standards Centrifugal liquid Gravitational liquid Pipette method Single particle light interaction method Photometric properties of materials Pigment content

ISO 6504-1

Thermoplastics Tinting strength, relative: Carbon black Change in (see Dispersion and PVC) Colorimetric method Dyes in solution FIAF method (see Color depth) Inorganic pigments

ASTM

BS

NF

JIS

DIN 53773-1 53773-2 53775-1 53775-7 53775-3 53774-1 53774-2

15528

D 3925

EN ISO 15528

T 30-048

787-24 6504-1

3483-A6

EN ISO 787-24

31

5775

X 02-001

K 4001 K 5101 K 5400

EN ISO 15528

ISO 787-24 53164 Z 8202

1301-1 to -3 1303 1304 EN 12877-1 to 2

D 3349 55986 55978 55603

Appendix 1

Scattering power, relative: Gray paste method Black ground method Significances (see Color differences) Symbols for use in formulas

ISO

360

Key words PVC, paste: Basic mixture Test specimen preparation PVC, plasticized: Basic mixture Change in tinting strength Test specimen preparation PVC, unplasticized: Basic mixture Test specimen preparation Radiometric properties of materials (see Photometric properties of materials) Reflectometer (see Gloss) Residual color difference (see Tinting strength) Sampling

Key words Lightness method Organic pigments (see Color depth) Photometric methods Visual Weighted K/S value method Transmission of optical radiation Transparency (Pigmented/unpigmented systems)

ISO

ASTM

BS

NF

787-24

D 387 D 3022 D 4838

EN 787-24

T 30-031 T 31-228

55978 EN ISO 787-24

EN ISO 787-1

T 30-027 T 31-227

EN ISO 787-16 1349

787-16 787-26

JIS

DIN 55603

1349-1 to 2 55988

Appendix 1

361

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

Subject Index

A absorbing power 3±9, 71±130, 131±196, 207±226 ± test method 233±235, 254, 255, 325±327 absorption coefficient 11, 71±130, 137±141, 207±226 ± four-flux theory 78±83, 138±141, 291±296 ± Kubelka-Munk theory 78±81, 138±141, 282±296 ± ± determination 283±296 ± ± ± error 287±293 ± ± per unit mass 138, 327, 328 ± ± ± relative, determination 327 ± ± per unit volume 150±152, 191, 192, 219±226 ± many-flux theory 72±75 ± test methods 252, 253, 282±296, 327±333 absorption cross-section 11, 219±222, 224±226 absorption index 11, 213±217, 224±226 absorption maximum 140, 141, 167, 168, 325, 327, 340 acceptability 16, 59±62, 241, 242, 277; see also ellipsoid, acceptability adding-pigment method 146±149, 327, 328 agglomerate 132, 208, 236, 237 aggregate 132 anisotropy, optical 215, 216 application error 58 B basic conditions (CIE94) 36, 37 Beer's law 138±140 ± region 140±144, 284, 335±338 black standard see colorimeters black value 251, 252 brightness see lightness C characteristic equation 47, 74, 257, 258 chi-square distribution 45, 57

chroma 29, 105, 169±171 ± test methods 247±252, 308, 329 chroma difference, principles 32±34, 105, 169±171 ± test methods 247±252, 308, 329 CIE chromaticity coordinates 23±26, 246, 333 CIE chromaticity diagram 25, 274, 275 Cie color matching functions 23±26, 118, 119, 160±161, 243±248, 299 CIE color notation system 20±26, 116, 184, 185, 247, 248 CIE standard colorimetric system see CIE color notation system CIE standard illuminants 17, 119, 160±163, 246, 255 CIE standard observer See CIE color notation system CIE tristimulus values 23±26, 119, 159±165 ± test methods 243±248, 284, 327±329 CIELAB color space 31, 36, 168±171, 257±259, 273, 274 CIELAB coordinates 28±36, 115±117, 168, 249, 250±252, 329 CIELAB system 28±36, 116, 118, 188±191, 246±248, 308, 309 CIE94 system 36±38 CMC system 38±39 coating materials 3 ± thickness see film thickness colloid chemistry 131, 133±138 color depth 169±171, 327, 332, 333 ± criteria 184±186, 332, 333 ± level see standard depth of shade ± matching 184±186, 328±333, 335±337 ± standards 328±333 color difference 15, 104, 105, 167±171 ± after color reduction 188±191, 327±333; see also shade difference ± test methods 239±242, 296, 329

364

Subject Index

color formulation 15, 167±169, 177, 178, 294±295, 335±337 color identification code 15 Color Index 41 color matching 172±187, 267±276 ± trichromatic, theory 23 color measurement 10, 15±17, 278 ± errors 54±57, 100, 101, 259±263 ± ± ellipsoid 257±260 ± ± preparation 249, 259±263 ± ± ± ellipsoid 260±263 ± test errors 255±263 ± ± ellipsoid 255±263 color mixing 20 color, object see object color color order systems 39±41 color plane 29, 33±35 color rendering 15 color sample 39, 241±243, 332, 333 color saturation see saturation color space, absolute 27, 40 ± CIELAB see CIELAB color space ± euklidean 37, 39 color stimulus 9±12, 15, 27, 115, 253, 254, 267, 268 color systems 15, 26 ± perceptual 26±36 ± physiologically equidistant 7, 28 color tolerances see acceptability colorimeters 17±19, 76±78, 237±242, 285, 327, 328 ± black standard 243, 244, 251, 252, 303, 304 ± calibration 243, 244, 284, 332, 333 ± light sources 242±244, 269, 270 ± measuring conditions 19, 76±78, 237±242, 253, 254, 285, 286, 287, 327, 328 ± sample illumination 253, 254 ± spectrophotometer see spectral method ± three-filter see tristimulus method ± trichromatic matching 23, 27 ± white standard 19, 244, 303±304 colorimetry 10±12, 15±50, 178, 179, 234, 235, 332, 333 coloring material 3±9, 208, 240±242; see also dyes; pigments coloring power 111±113, 121±123, 182±184, 277, 297, 298 ± condition (measurement) see colorimeter ± determination 299

confidence interval, level 57, 247, 248, 255±257, 264, 271, 272 conformity (with standard) see acceptability constant-volume method 146±149, 345 contrast ratio 104, 105, 308, 309 contrast substrate 104±110, 144, 145, 249, 287, 288 corpuscular theory 71, 207±226 cosine distribution, Lambert's 76, 234, 235 covariance 54±56, 58, 255, 256, 264, 265 ± matrix 55, 56, 255, 256 critical value see confidence interval D daylight color 252, 253 dilution method 146±149, 348 DIN Color system 41 dispersing (dispersion) of pigments see pigments, dispersing dispersing resistance 344 dispersion (colloid chemistry) 131±138, 241±243 ± density 137, 138 dispersion, anomalous (optics) 225, 226 distribution ± cumulative 218, 219 ± density 217, 218 ± width 218, 219 see also normal distribution; lognormal distribution dye 71, 131±138, 323±325 ± content 71, 131±206, 254, 255, 323±325 ± test methods 240, 241, 252±255, 267, 268, 323±325 E effectiveness 104, 183, 184, 318±321 ellipse ± axes 212 ± coefficients 43 ± eccentricity 212 ± standard deviation 43, 212, 213 ellipsoid ± acceptability 59, 267±276 ± coefficients 52±55, 255±263 ± conditions 46, 51±55, 257, 258 ± normal form 46, 47, 50, 57 ± principal axes 46±49, 257±260 ± ± system 47, 259, 260 ± projections 49, 257±260

Subject Index ± radius 51 ± standard deviation 44±51, 55, 56, 255±257 see also color measurement, errors equi-energy stimulus 25 equivalent diameter 133 Eurocolor system 41 F FIAF method 184±187, 228±240 fillers (extenders) 3, 133, 134, 215, 216, 249, 324 film thickness 11, 78±81, 138, 139 ± test methods 249, 277±287, 315, 316 ± measurement 277±283 ± ± chemical, electrical, magnetic, optical methods 278 ± ± dial-gauge micrometer methods 280±282 ± ± errors 277 ± ± gravimetric methods 279, 303, 304 ± ± pneumatic methods 281±283, 300, 301, 303, 304, 318, 319 ± ± wedge cut method 279, 280 floating 134, 262, 263 flocculation 132, 134, 242, 243 fluorescence 253, 254 four-flux theory 71, 72, 74, 78±96, 291±293 Fresnel equations 233, 236, 237 Fresnel reflection 221±224, 233 full shade 134, 239±241 ± black 231, 240, 247±252 ± chromatic 247±252 ± ± determination 303, 304 ± white 247±252 full-shade system 242, 243, 247, 248, 267, 268 G gloss 105, 134, 234, 296 ± degree of 108, 236, 237, 240, 241, 305±308, 315, 316 ± high 234, 240, 241, 285, 296, 297 ± mat 234, 240, 241 ± measurement 233±238 gloss angle 236, 237 gloss exclusion (trap) 239±241 gloss haze 134, 336±341 gloss indicatrix 234, 235, 255, 256 glossmeters 234, 235, 254±256 goniophotometers see glossmeters Grassmann's laws 20 gray scale 29

365

H Helmholtz equation 217, 218 hiding criterion 104, 105, 301±303, 311, 312 hiding power 104±110, 115±121, 164±166, 277±321 ± economic aspects 318±321 hiding power value 104, 106±110, 277, 301±321 ± absorption component 108, 109, 306±308, 315, 316 ± achromatic, determination 304±309 ± graphical determination 301±308, 311, 312 ± interaction component 109, 110, 308, 309, 311, 312, 315, 316 ± scattering component 108, 109, 306±308, 315 histogram 209, 212 homogeneity error 58 hue 26, 27, 53, 54, 105, 167, 168 ± test methods 249, 250, 308, 325 hue angle 29, 250, 251 ± difference 32, 33, 250, 251 hue difference 32±34, 53, 54, 105, 172 ± test methods 249, 250, 308, 329 hue (shade, undertone) 33±35, 188±191, 249±252, 327, 328 ± near-black specimens 249±252 ± near-gray specimens 105, 249±252, 308 ± near-white specimens 105, 249±252, 308 I immersion method 216, 217 incandescent light color 252, 253 infinitely thick layer 92, 93, 284 integrating sphere 237±240, 249, 253, 254 K Kubelka-Munk ± function 97±101, 139, 140, 195, 323, 327±329 ± ± error of determination 100, 101 ± theory 11, 72, 145, 146, 149±165, 219, 220, 283±293 L Lambert's law 72, 78, 79, 85, 86, 138, 139 light absorption power see absorbing power light scattering power see scattering power

366

Subject Index

lightening power 131, 148, 149, 165, 166, 186±188 ± determination 345±355 ± ± graphical 345±348 ± ± per unit PVC 350±355 ± ± rationalized method 347±351 ± test methods 284, 287±291, 345±355 ± ± Reynolds 149, 150 lightness 26, 27, 168, 169, 247±252, 310, 311, 327, 329 ± difference 32±34, 104, 105, 247±250, 304, 305 ± matching 178±187, 327±333 likelihood see maximum likelihood method lognormal distribution 209, 211±213 ± two-dimensional 211±213 M many-flux theory 71±75, 291±293, 294±296 mass tone 247, 248 matching criteria see tinting strength criteria matrix inversion 255±257, 262, 263 maximum likelihood method 59, 272 measurement error 58 metallics 4, 254, 255 metamerism 23, 246, 251±253 ± geometrical see Silking effect ± index 252, 253 Mie minimum 222, 223 Mie theory 11, 74, 207, 217±226, 294, 295 Munsell system 28, 36, 40 N nacreous pigments 4, 255 Natural Color System 40 Newton's method (approximation) 107, 120, 121, 196, 272, 314±316 nonluminous perceived color see object color non-self-radiating medium 17 normal distribution ± logarithmic see lognormal distribution ± one-dimensional 42, 209±211, 259, 260 ± three-dimensional 42±45, 259, 260, 264, 269, 270 ± two-dimensional 43 O object color 17, 19, 23, 233±276 one-flux theory see Lambert's law optical brighteners 253, 254

optical contact 285±287, 303, 304 OSA-UCS (color order system) 41 Ostwald color system 41 P parametric factors (CIE94) 36±38 partial oscillations 217±222 particle size ± fractions 218, 219 ± optimal 222±224, 225, 226 ± parameters 133, 208±213 particle-size 11, 71, 131±133, 207±223, 296, 297 ± analysis 212, 213 ± distribution 133, 167, 168, 208±213, 220, 221, 225, 226 ± ± analysis based on volume effects 213 ± ± class 209±211 ± ± light scattering analysis 213 particles 11, 71, 131±138, 207±226 ± anisometric 211, 219, 220, 252, 253 ± counting 213 ± diameter 133, 208, 215, 216 ± form 131±133, 220, 221 ± mass 133, 208 ± number 208 ± ± analysis see particle-size analysis ± ± distribution see particle-size distribution ± surface area 133, 208, 215±217 ± test methods 236, 237, 252, 253, 296, 297 ± volume 133, 209±211, 215, 216, 220, 221 paste film holder 249, 250, 346, 347 perceptibility 16, 269, 270, 273, 274 phenomenological theory 71±130, 207 Pigenot equation 191±193 pigment content 11, 71, 131±138, 213 ± determination, centrifuge method 324 ± ± filtration method 324, 325 ± ± incineration method 324 ± test methods 236, 237, 324, 325 pigment distribution see particle-size distribution pigment mass 135 ± concentration (PMC) 135±137, 283±285, 327, 328, 347, 348 ± equivalent to the medium volume (PVM) 136, 137, 179, 180, 351, 354 ± equivalent to the medium volume of the mass portion (PMM) 136, 137 ± per unit area 284 ± portion (PMP) 135±137, 283

Subject Index pigment/medium volume ratio (PMV) 136, 137, 347, 348 pigment particle see particle pigment/paste mixing 146±165 pigment surface area see particles, surface area pigment surface concentration 137, 138 pigment volume see particles, volume ± concentration (PVC) 116, 135±138, 236, 237, 279 ± ± critical 134, 140, 141, 354, 355 ± portion (PVP) 137, 138 pigments 3±9, 131±138, 207±226 ± black 4, 5, 146, 147, 151±156, 239±241, 287±293, 327±333 ± colored 4, 6±8, 108, 146, 147, 157±165, 207±226 ± ± test methods 247±252, 256±258, 287±293, 327±333 ± density 136, 137, 279, 346 ± dispersing (dispersion) 132±135, 208±213, 236, 237, 284, 340, 341 ± ± equipment 241, 242, 284, 327, 328, 341, 345±347 ± ± rate of 191±196, 342±344 ± ± resistance 196, 344 ± fluorescent 4±5, 253, 254 ± interference 4, 255, 256 ± luminescent 4±5, 253±255 ± luster 4 ± metal-effect 4, 236, 237, 254, 255 ± nacreous 4, 255, 256 ± phosphorescent 5, 253±255 ± test methods 236, 237, 283, 324, 325 ± transparent 325±329 ± visual 23 ± white 4±5, 108, 109, 146, 147, 156±158, 207±226 ± ± test methods 247±252, 283±288 PMC see pigment mass concentration PMM see pigment mass equivalent to the medium volume of the mass portion PMP see pigment mass portion PMV see pigment/medium volume ratio polarized light 214, 215, 217±219 power-law distribution 209 preparation error 58 primary particle 132, 143 primary stimulus 20, 21, 24, 27 probability, cumulative 44, 212

367

probability density 44, 212 production monitoring (control) 15±17, 182, 183, 249, 327, 328 PVC see pigment volume concentration PVM see pigment mass equivalent to the medium volume PVP see pigment volume portion R radiance factor 18 radiative transfer 66, 67 RAL Color Register 40, 41 RAL-Design-System 41 rate constants (dispersing) 191±196, 342±344 Rayleigh scattering 221, 222 reaction kinetics 191±196 reference stimulus see primary stimulus reflectance 10±12, 17±19, 71±130, 150±152, 225, 226 ± errors of measurement 100, 101, 277, 287±293 ± test methods 233±242, 277 reflection see also reflectance ± coefficients 75±76, 122, 214, 215, 233±242, 293, 294 ± factor 17±19, 75±78, 233±242, 277, 327 ± law 224, 225 ± specular 86±91, 234, 254, 255 reflectometer values 169±171, 236, 296, 297, 327, 328 refractive index 11, 71, 213±217, 233 ± complex 213, 214, 218, 219 ± mixing rules 216, 217 retina 31 rhodopsins 23 RRSB distribution 209 rub-out test ± determination 341 ± method 242, 243 Ryde theory 71, 84 S sampling 241, 242 ± error 58 saturation 26±27, 40, 167, 168, 175±177, 253, 254 Saunderson correction 75, 151, 152, 285, 327±329 ± dependent (multiple) see scattering interaction

368

Subject Index

scattering coefficient 11, 71±130, 138, 139±146, 207±226 ± four-flux theory 78±83, 137, 138, 291±296 ± Kubelka-Munk theory 78±81, 143, 144, 277, 282±296 ± ± error of determination 117, 118, 277, 287±293 ± ± per unit mass 283±293, 347±351 ± ± per unit volume 143, 150, 151, 220, 221, 286, 287, 347, 348 ± ± ± relative see scattering power, relative ± many-flux theory 71±75 ± test methods 252, 253, 283±296 scattering cross-section 11, 219±225 scattering interaction 11, 140±144, 348±351 scattering power 4, 9, 10, 71±130, 131±196, 207±226 ± relative 277, 283, 284 ± ± black-ground method 284±288, 347, 348 ± ± determination, paste methods 347±351 ± test methods 233±242, 277, 340, 341 SDS see standard depth of shade secular equation see characteristic equation sedimentation analysis 213 shade difference after color reduction 188±191, 332, 333, 336±348; see also hue (shade, undertone) shape factor 212 sieve effect (Kubelka-Munk theory) 288 significance 16, 57, 58, 247±249, 255±257, 262±268 ± level see confidence interval ± test 264±268 Silking effect 252, 253 size reduction see pigments, dispersing (dispersion) Snell's law 214, 215 special color differences 27±28, 119, 239±242, 304, 305, 329 spectral colors 20±21 spectral evaluation, principle of 115±118, 298±301, 328±340 spectral locus 21, 26 spectral luminosity curve (spectral luminous efficiency function) 26 spectral method 121, 122, 243, 244, 298±300, 325±327 stabilization see pigments, dispersing (dispersion) standard depth of shade 175, 328±334

standard deviation 42, 43, 51±55, 257, 258, 327 standard deviation ellipse see ellipse, standard deviation standard deviation ellipsoid see ellipsoid, standard deviation standard illuminants 23, 24, 37 standard observer see SIE color notation system surface chemistry 215±217 surface correction see Saunderson correction surface reflection 75±78, 97, 233±242, 279, 327, 328 T thermochromism 253 tinting characteristic 168±171 tinting strength 164±187 ± absolute 166, 167, 182, 183 ± change in (increase in strength) 191±196, 236, 237, 340±344 ± criteria 167±172, 327 ± matching 297, 298, 329±333 ± relative 115, 131, 236, 237, 283, 284, 323±355 ± ± of coloring maerials, determination 325±341 ± ± of pigments, inorganic, determination 327±333 ± ± of pigments, organic, determination 328±340 tinting strength equivalent 166, 167, 332, 333 total error 58 transmission see transmission factor; transmittance transmission factor 19, 82±86, 138, 139 ± test method 233±242, 291±295, 325, 326 transmittance 19, 74 ± test methods 233±242, 291±293, 325, 326 transparency 110±114, 121±123, 277±321 ± number 110±114, 122, 123, 277, 296±299 ± ± single-point method determination 297±300 ± ± two-point method 296±300 transparency-coloring degree 113, 122 ± determination 297, 298, 317 ± transparency-coloring power 112, 122 trichromatic principle 21±23 tristimulus method 169±171, 243±248, 297, 298, 327±333 two-flux theory see Kubelka-Munk theory

Subject Index V van de Hulst formula 221±225 van der Waals forces 133 vision, color 23 ± cones 23, 31 see also pigments, visual volume distribution 209, 213

W wave equation 213, 214, 217, 218 wavelength 11, 115, 140, 141, 213±217 ± test methods 222±226, 288±291 Weber-Fechner law 28 wetting 133 white locus see equi-energy stimulus white standard see colorimeters

369

Industrial Color Testing: Fundamentals and Techniques, 2nd Edition. Hans G. Vælz Copyright # 2002 Wiley-VCH Verlag GmbH & Co. KGaA ISBNs: 3-527-30436-3 (Hardback); 3-527-60048-5 (Electronic)

Name Index

A Abramowitz, W. 69 Adams, E. Q. 67, 68 Aitchinson, J. 230 Allen, T. 205 Atkins, J. T. 128, 129, 295 B Beasley, J. K. 129 Beattle, H. 230 Beer, A. 131, 139±141, 143, 149, 152, 154, 157, 187, 188, 204, 205, 284, 287, 303, 335, 347±348, 349 Berger, A. 68 Berger-Schunn see Berger Bessel, F. W. 218 Billmeyer, F. W., Jr. 68, 69, 128, 129, 295 Blumer, H. 230 Booth, G. 13, 206 Born, M. 68 Bouguer, P. 72, 127 Brockes, A. 68, 69, 128, 129, 230 Brossmann, R. 230 Brown, J. A. C. see Aitchinson Brown, W. R. J. 67, 68 Bçchel, K. H. 13 Bçchner, W. see Bçchel Buxbaum, G. 13 C Chandrasekhar, S. 128, 129 Channon, H. J. 129 Clausen, H. 205, 206, 347 Cremer, M. 130 D Descartes, R. 235, 257 Dettmar, H.-K. 229, 230 Duntley, S. Q. 127±129

E Eitle, D. 128, 129 Euclid 40 F Fechner, G. T. 28 Felder, B. 230 Fisher, R. A. 67 Fresnel, A. J. 75, 76, 214, 215, 221, 223, 230, 233, 236, 243 Friedrichsen, K. 206, 335, 337±339 Fritzsche, E. 13 Fukshanski, L. 127, 129 G Gall, L. 67, 68, 128, 130, 172, 175±178, 184± 186, 204±206, 328±339 Gans, R. 230 Gardner, H. A. 206 Gauss, F. K. (C. F.) 16, 45, 67 Geissler, G. 206 Grassmann, H. 20, 66, 68, 205, 206, 347 Grassmann, W. see Clausen Guild, H. 66, 68 Gurevic, M. 127, 129 H Hauser, P. 230 Hediger, H. 230 Heine, H. 13 Heller, W. 230 Helmholtz, H. von 23, 66, 68, 217 Hengstenberg, J. 69 Herbst, W. 13 Honerkamp, J. 230 Honigmann, B. 132, 205, 230 Howe,W. G. 69 Hubel, D. H. 68 Hunger, K. see Herbst Hunt, R. W. G. 68

372

Name Index

J Jaenicke,W. 206, 229 Joos, G. 230 Judd, D. B. 128, 129, 204, 206 K Kaluza, U. 204, 205 Kåmpf, G. 128, 130, 204, 205 Keifer, S. 128, 130, 134, 169, 172, 177, 204± 206, 319 Kerker, M. 229, 230 Klaeren, A. 205 Koch, O. 204, 206 Kæhler, P. see Buxbaum Kortçm, G. 128, 129, 229 Koutnik,V. 230 Kreyszig, E. 69 Kroker, R. 205 Kronecker, L. 73 Kubelka, P. 294 and see Munk L Lambert, J. H. 72, 75, 79, 85, 86, 126, 139, 204, 234 Laplace, P. S. 213, 217 Legendre, A. M. 74, 293, 294 Leschonski, K. 205 Lowan, A. N. 229, 230 M MacAdam, D. L. 67, 68 Madelung, E. 143 Maikowski, M. A. 230 Maxwell, J. C. 213 McLaren, K. see Booth Meehan, E. J. see Beattle Metz, H. J. 230 Mie, G. 11, 74, 207, 208, 217±226, 229, 230, 294 Mudgett, P. S. 128, 129, 220, 293, 295 Mçller-Kaul, W. see Geissler Munk, F. 11, 72, 84, 86, 88, 92, 93, 96±103, 105±109, 113±122, 127±129, 139, 146±165, 171, 178±184, 204, 219, 220, 223, 283±293, 300, 317, 323, 327±329, 333, 335, 340, 342, 343, 348, 350±353, 355 Munsell, A. H. 28, 35, 40, 65, 67, 68 Murley, R. D. 230

N Nassenstein, H. 230 Newton, I. 66, 68, 107, 119, 120, 129, 271, 314 Nickerson, D. see Adams O Ostwald, W. 23, 41 P Paffhausen, W. 69 Panek, P. see Buxbaum Pauli, H. 128, 129, 230 Pigenot, D. von 192, 194, 204, 205, 342 Pluhar, P. see Kroker R Rabe, P. see Koch Rayleigh, J. W. 221, 222, 229, 230 Rembrandt van Rijn, H. 235 Renwick, F. F. 127, 129 Reynolds, C. E. 149, 150, 205 Rich, R. M. see Howe Richards, L. W. see Mudgett Richter, M. 67, 68 Robertson, A. R. 67±69 Ræmer, H. see Honerkamp Ryde, J. W. 71, 83, 86, 91, 92, 127±129 S Saunderson, J. L. 75, 83, 97, 102, 117, 118, 128, 129, 182, 289±291, 294, 305, 311±313, 328, 329, 333, 334, 348, 350, 352, 353 Schliebs, R. see Bçchel Schmelzer, H. 69, 204, 206, 333 Schmitt, K.-H. see Hengstenberg Schmitz, O. J. see Kroker Schrædinger, E. 68 Schuster, A. 127, 129 Sharples, W. G. see Booth Silberstein, L. 68, 127, 129 Snell (Snellius van Roijen), W. S. 214 Stabenow, J. 132, 204, 205 Stange, K. 69 Stearns, E. I. 119, 129, 130, 247, 302 Stegun, I. see Abramowitz Steinbuch, K. 68 Stiles, W. 68 Stokes, G. G. 127, 129 Storr, B. V. see Channon

Name Index Strocka, D. 69, 129, 130 Stultz, K. F. 68 Sturm, B. see Hengstenberg Suzuki, S. see Okuda Sward, G. G. see Gardner T Thiemann, J.

219

V van de Hulst, H. C. 222, 223, 229, 230 van der Waals, J. D. 134 Vial, F. 206 Vælz, H. G. 13, 65, 66, 68, 129, 130, 177, 204±206, 230

W Wald, G. 68 Walraven, J. 68 Weber, E. H. see Fechner Westwell, A. see Booth Winkler, O. see Hengstenberg Winter, G. see Bçchel Woditsch, P. see Buxbaum Wright, W. D. 66, 68 Wyszecki, G. 68 Y Young, T.

23, 66, 68

Z Zollinger, H. see Booth Zorll, U. 205

373

Thank you for interesting in our services. We are a non-profit group that run this website to share documents. We need your help to maintenance this website.